*420*
*105*
*30MB*

*English*
*Pages XXXVI, 621
[628]*
*Year 2020*

Table of contents :

Front Matter ....Pages i-xxxvi

Front Matter ....Pages 1-1

Influence of Composition and Structure of Pt-Based Electrocatalysts on Their Durability in Different Conditions of Stress-Test (Elizaveta Moguchikh, Kirill Paperj, Angelina Pavlets, Anastasia Alekseenko, Maria Danilenko, Aleksey Nikulin)....Pages 3-20

Investigation of the Effect of Different Organic Additives on Morphology and Electrocatalytic Activity of Platinum Nanomaterials Towards Oxygen Reduction Reactions (Sergey V. Belenov, Weldegebriel G. Yohannes, Nikolay V. Lyanguzov, Vadim A. Volochaev)....Pages 21-32

X-ray Spectroscopy Study of the Atomic and Electronic Structure of Polyacrylonitrile-Based Nanocomposites at Different Stages of Formation (M. A. Kremennaya, V. A. Shmatko, T. A. Mikhailova, E. V. Pronina, K. D. Kosolapova, G. E. Yalovega)....Pages 33-39

Morphology and Structure of Carbon Nanoparticles Generated from Graphite Nitrate Co-intercalation Compound. Effect of Sonication Regime (E. V. Raksha, A. A. Davydova, Yu. V. Berestneva, M. V. Savoskin, V. A. Glazunova, A. N. Vdovichenko et al.)....Pages 41-47

Formation of Surface Micro and Nanostructures When Exposed to Laser UV and VUV Radiation of Nanosecond Duration (Vladislav Khomich, Vladimir Yamshchikov, Sergey Mikolutskiy)....Pages 49-60

The Effect of Preliminary Laser Surface Treatment on the Mechanical Properties of a Solid-Phase Compound of an Iron-Nickel Alloy in Diffusion Welding (Yury Khomich, Vladimir Yamshchikov)....Pages 61-71

The Nucleation and Development of Wear in Nanocomposite Coatings Under the Action of a Discrete Vapor-Droplet Flow (Valery N. Varavka, Oleg V. Kudryakov, Igor Yu. Zabiyaka, Natalia I. Bronnikova)....Pages 73-83

Mechanical Properties Derived by Spherical Indentation of TiN Coating Deposited by a Method Combining Magnetron Sputtering and Arc Evaporation (Evgeniy Sadyrin, Roman Karotkiyan, Nikolay Sushentsov, Sergey Stepanov, Igor Zabiyaka, Evgeniy Kislyakov et al.)....Pages 85-95

Studies on Predicting Spring-Back and Verifying the Effects of Temperature, Sheet Thickness and Punch Speed on Forming Force of V-Bending for SS400 Steel Plate (Gia-Hai Vuong, Thi-Hong-Minh Nguyen, Duc-Toan Nguyen)....Pages 97-108

Buckling Analysis of Folded Composite Plate Subjected to In-Plane Loading Condition (Bui Van Binh, Le Thuong Hien)....Pages 109-121

The Effect of Strain Rate on Chip Formation and Cutting Process During High-Speed Cutting of A6061 Aluminum Alloy (Pham Thi Hoa, Banh Tien Long, Nguyen Duc Toan, Doan Thi Huong, Pham Duc Thanh)....Pages 123-130

Prediction of Temperature Distribution in PCBN Cutting Tools in Orthogonal Turning 9XC Hardened Alloy Steels (Dung Thi Quoc Nguyen)....Pages 131-139

Study on the Optimal Sealing Technological Regime for Making Sport Wears from Waterproof Fabric (Tran Thuy Trang, Phan Thanh Thao)....Pages 141-156

Front Matter ....Pages 157-157

Equation for Density Matrix Systems of Identical Particles (Boris V. Bondarev)....Pages 159-172

Crystal Structure and Dielectric Properties of Layered Perovskite-Like Solid Solutions Bi3−xLuxTiNbO9 (x = 0, 0.05, 0.1) with High Curie Temperature (S. V. Zubkov, S. I. Shevtsova)....Pages 173-182

Fabrication and Investigation of InSb Thin Films for IR SAW Photodetectors (M. E. Kutepov, T. A. Minasyan, D. A. Zhilin, V. E. Kaydashev, G. Y. Karapetyan, K. G. Abdulvakhidov et al.)....Pages 183-190

The Investigation of Optical and Dielectric Properties of Ferroelectric BSN Ceramics Doped with Rare-Earth Elements (L. V. Grigoryev, A. A. Semenov, P. Yu Belyavskiy)....Pages 191-201

Universal Technique to Determine the Intensity of the Optical Fields, Generated by Laser Interference Meter of Displacements (I. P. Miroshnichenko, I. A. Parinov, V. P. Sizov)....Pages 203-226

Strength of Interatomic Bonds at High-Angle Grain Boundaries in Iron (Yuri F. Migal)....Pages 227-234

Digital Microscopy Image Enhancement Technique for Microstructure Image Analysis of Bottom Ash Particle Polymer Composites (F. A. Hermawati, I. M. Kastiawan, Muhyin)....Pages 235-244

Analysis of Effect of Oil Viscosity and Temperature on Dynamic Pressure Distribution in Internal Gear Motor and Pump (Pham Trong Hoa)....Pages 245-253

Experimental Investigation of Effect of Process Parameters on Surface Roughness in Electrochemical Machining (Loc P. Ngo, Tai P. Nguyen, Thanh T. Tran)....Pages 255-270

Optimization of Surface Roughness and Vibration During Thermal—Assisted Milling SKD11 Steel Using Taguchi Method (Thi-Bich Mac, Banh Tien Long, Duc-Toan Nguyen)....Pages 271-282

Assessment of the Surface Roughness of Metal Mechanical Parts by Microsoft Kinect V2 (Bui Van-Bien, Banh Tien Long, Nguyen Duc-Toan)....Pages 283-292

New Materials for Road Construction (N. I. Buravchuk, O. V. Guryanova, M. A. Jani, E. P. Putri)....Pages 293-307

Front Matter ....Pages 309-309

Finite Element Modelling of Active Composite Materials in ACELAN-COMPOS Package (Andrey Nasedkin)....Pages 311-323

Finite Element Investigation of Effective Moduli of Transversely Isotropic Thermoelastic Materials with Nanoscale Porosity (Andrey Nasedkin, Anna Nasedkina, Amirtham Rajagopal)....Pages 325-337

Investigation of Initial Stresses’ Influence on Surface Wave Field in Bulk Metallic Glass Layer (T. I. Belyankova, E. I. Vorovich, V. V. Kalinchuk, O. M. Tukodova)....Pages 339-352

Comparison of Two Numerical Inverse Laplace Transform Methods with Application for Problem of Surface Waves Propagation in an Anisotropic Elastic Half-Space (Ivan Markov, Leonid Igumnov)....Pages 353-368

Twofold Re-reflections of Ultrasonic Waves from Obstacles in a Two-Dimensional Elastic Material, Taking into Account Any Laws of Their Reflections and Transformations (Nikolay V. Boyev)....Pages 369-381

On the Use of Models of the Tymoshenko Type in the Analysis of Wave Processes in Wedge-Shaped Waveguides (Aleksandr Vatulyan, Lyubov Parinova)....Pages 383-389

Construction of the Mechanical Model of Keratoprosthesis of the Ocular Cornea (Arkadiy Soloviev, Nadegda Glushko, Alexander Epikhin, Michael Swain)....Pages 391-403

Simulation of the Stress-Strain State of the Spline Joint of the Helicopter Tail Transmission (M. I. Chebakov, S. A. Danilchenko, E. M. Kolosova)....Pages 405-413

Shell with Auxetic Properties in the Model Taking into Account the Transverse Shear (Anatoly S. Yudin)....Pages 415-428

Coupled Problem of Thermoviscoelasticity for Composite Polymer Shell of Revolution (V. G. Safronenko)....Pages 429-438

The Study of Stratification of Multilayer Structures Based on Finite Element Modeling and Neural Network Technologies (A. V. Cherpakov, P. V. Vasiliev, A. N. Soloviev, I. A. Parinov, B. V. Sobol)....Pages 439-447

The Structural Correlation and Mechanical Properties in Amorphous Hafnium Oxide Under Pressure (Nguyen-Hoang Thoan, Nguyen-Trung Do, Nguyen-Ngoc Trung, Le-Van Vinh)....Pages 449-459

A Comparison Study of a DIC and Extensometer on Stress-Strain Curve for AL5052 Aluminum Sheets and Its FEM Applications (Ngoc-Duc Do, Van-Thuong Nguyen, Duc-Toan Nguyen)....Pages 461-474

Front Matter ....Pages 475-475

An Analytical Model for AlGaN/GaN MOS-HEMT for High Power Applications (Nguyen-Trung Do, Nguyen-Hoang Thoan, Tran Minh Quang, Dao Anh Tuan, Nguyen-Ngoc Trung)....Pages 477-485

Structural Scheme of Electroelastic Actuator for Nanomechatronics (Sergey M. Afonin)....Pages 487-502

On Extraction of Energy from Rotating Objects (Tejkaran Narolia, Vijay K. Gupta, Ivan A. Parinov)....Pages 503-511

Computer Modeling and Experimental Research of Component Processing Procedure in the Centrifugal-Rotary Equipment (Nguyen Van Tho, A. N. Soloviev, M. A. Tamarkin, I. A. Panfilov)....Pages 513-528

Optimization Design of a 2-DOF Compliant Parallel Mechanism Using NSGA-II Algorithm for Vibration-Assisted Milling (Huy-Tuan Pham, Van-Khien Nguyen, Khac-Huy Nguyen, Quang-Khoa Dang, Trung-Kien Hoang, Son-Minh Pham)....Pages 529-539

Design and Analysis of a Compliant Constant-Torque Mechanism for Rehabilitation Devices (Thanh-Vu Phan, Huy-Tuan Pham, Cong-Nam Truong)....Pages 541-549

Improve the Loading Capacity and Stiffness of Hydrostatic Spindle Medium Sized Circular Grinding Machines Based on Simulation and Geometric Parameters of the Bearing (Van-Hung Pham, Manh-Toan Nguyen, Tuan-Anh Bui)....Pages 551-558

Inverse Method for Estimating the Convection Coefficient at Gap Inside Bearing Rig Test (Thi-Thao Ngo, Jin H. Huang, Van-The Than)....Pages 559-570

Combining the Kalman Filter and Particle Filter in Object Tracking to Avoid Occlusion Problems (Jen-Hong Lan, Ssu-Wei Chen, Chih-Hsueh Lin, Chin-Shiuh Shieh, Shyh-An Yeh, I-Hsing Tsai et al.)....Pages 571-586

Generative Artificial Neural Network Model for Visualization of Internal Defects of Structural Elements (Arcady Soloviev, Boris Sobol, Pavel Vasiliev, Alexander Senichev)....Pages 587-595

Direct Mapping Based FBMC-LDPC Advanced Underwater Acoustic Transmission Scheme for Data Signals (Chin-Feng Lin, Tsung-Jen Su, Shun-Hsyung Chang, Ivan A. Parinov, Sergey N. Shevtsov)....Pages 597-603

Acquisition and Analysis of Endodontic Handpiece Vibration Signals (Ankit Nayak, P. K. Kankar, Prashant K. Jain, Niharika Jain)....Pages 605-613

Back Matter ....Pages 615-621

Front Matter ....Pages i-xxxvi

Front Matter ....Pages 1-1

Influence of Composition and Structure of Pt-Based Electrocatalysts on Their Durability in Different Conditions of Stress-Test (Elizaveta Moguchikh, Kirill Paperj, Angelina Pavlets, Anastasia Alekseenko, Maria Danilenko, Aleksey Nikulin)....Pages 3-20

Investigation of the Effect of Different Organic Additives on Morphology and Electrocatalytic Activity of Platinum Nanomaterials Towards Oxygen Reduction Reactions (Sergey V. Belenov, Weldegebriel G. Yohannes, Nikolay V. Lyanguzov, Vadim A. Volochaev)....Pages 21-32

X-ray Spectroscopy Study of the Atomic and Electronic Structure of Polyacrylonitrile-Based Nanocomposites at Different Stages of Formation (M. A. Kremennaya, V. A. Shmatko, T. A. Mikhailova, E. V. Pronina, K. D. Kosolapova, G. E. Yalovega)....Pages 33-39

Morphology and Structure of Carbon Nanoparticles Generated from Graphite Nitrate Co-intercalation Compound. Effect of Sonication Regime (E. V. Raksha, A. A. Davydova, Yu. V. Berestneva, M. V. Savoskin, V. A. Glazunova, A. N. Vdovichenko et al.)....Pages 41-47

Formation of Surface Micro and Nanostructures When Exposed to Laser UV and VUV Radiation of Nanosecond Duration (Vladislav Khomich, Vladimir Yamshchikov, Sergey Mikolutskiy)....Pages 49-60

The Effect of Preliminary Laser Surface Treatment on the Mechanical Properties of a Solid-Phase Compound of an Iron-Nickel Alloy in Diffusion Welding (Yury Khomich, Vladimir Yamshchikov)....Pages 61-71

The Nucleation and Development of Wear in Nanocomposite Coatings Under the Action of a Discrete Vapor-Droplet Flow (Valery N. Varavka, Oleg V. Kudryakov, Igor Yu. Zabiyaka, Natalia I. Bronnikova)....Pages 73-83

Mechanical Properties Derived by Spherical Indentation of TiN Coating Deposited by a Method Combining Magnetron Sputtering and Arc Evaporation (Evgeniy Sadyrin, Roman Karotkiyan, Nikolay Sushentsov, Sergey Stepanov, Igor Zabiyaka, Evgeniy Kislyakov et al.)....Pages 85-95

Studies on Predicting Spring-Back and Verifying the Effects of Temperature, Sheet Thickness and Punch Speed on Forming Force of V-Bending for SS400 Steel Plate (Gia-Hai Vuong, Thi-Hong-Minh Nguyen, Duc-Toan Nguyen)....Pages 97-108

Buckling Analysis of Folded Composite Plate Subjected to In-Plane Loading Condition (Bui Van Binh, Le Thuong Hien)....Pages 109-121

The Effect of Strain Rate on Chip Formation and Cutting Process During High-Speed Cutting of A6061 Aluminum Alloy (Pham Thi Hoa, Banh Tien Long, Nguyen Duc Toan, Doan Thi Huong, Pham Duc Thanh)....Pages 123-130

Prediction of Temperature Distribution in PCBN Cutting Tools in Orthogonal Turning 9XC Hardened Alloy Steels (Dung Thi Quoc Nguyen)....Pages 131-139

Study on the Optimal Sealing Technological Regime for Making Sport Wears from Waterproof Fabric (Tran Thuy Trang, Phan Thanh Thao)....Pages 141-156

Front Matter ....Pages 157-157

Equation for Density Matrix Systems of Identical Particles (Boris V. Bondarev)....Pages 159-172

Crystal Structure and Dielectric Properties of Layered Perovskite-Like Solid Solutions Bi3−xLuxTiNbO9 (x = 0, 0.05, 0.1) with High Curie Temperature (S. V. Zubkov, S. I. Shevtsova)....Pages 173-182

Fabrication and Investigation of InSb Thin Films for IR SAW Photodetectors (M. E. Kutepov, T. A. Minasyan, D. A. Zhilin, V. E. Kaydashev, G. Y. Karapetyan, K. G. Abdulvakhidov et al.)....Pages 183-190

The Investigation of Optical and Dielectric Properties of Ferroelectric BSN Ceramics Doped with Rare-Earth Elements (L. V. Grigoryev, A. A. Semenov, P. Yu Belyavskiy)....Pages 191-201

Universal Technique to Determine the Intensity of the Optical Fields, Generated by Laser Interference Meter of Displacements (I. P. Miroshnichenko, I. A. Parinov, V. P. Sizov)....Pages 203-226

Strength of Interatomic Bonds at High-Angle Grain Boundaries in Iron (Yuri F. Migal)....Pages 227-234

Digital Microscopy Image Enhancement Technique for Microstructure Image Analysis of Bottom Ash Particle Polymer Composites (F. A. Hermawati, I. M. Kastiawan, Muhyin)....Pages 235-244

Analysis of Effect of Oil Viscosity and Temperature on Dynamic Pressure Distribution in Internal Gear Motor and Pump (Pham Trong Hoa)....Pages 245-253

Experimental Investigation of Effect of Process Parameters on Surface Roughness in Electrochemical Machining (Loc P. Ngo, Tai P. Nguyen, Thanh T. Tran)....Pages 255-270

Optimization of Surface Roughness and Vibration During Thermal—Assisted Milling SKD11 Steel Using Taguchi Method (Thi-Bich Mac, Banh Tien Long, Duc-Toan Nguyen)....Pages 271-282

Assessment of the Surface Roughness of Metal Mechanical Parts by Microsoft Kinect V2 (Bui Van-Bien, Banh Tien Long, Nguyen Duc-Toan)....Pages 283-292

New Materials for Road Construction (N. I. Buravchuk, O. V. Guryanova, M. A. Jani, E. P. Putri)....Pages 293-307

Front Matter ....Pages 309-309

Finite Element Modelling of Active Composite Materials in ACELAN-COMPOS Package (Andrey Nasedkin)....Pages 311-323

Finite Element Investigation of Effective Moduli of Transversely Isotropic Thermoelastic Materials with Nanoscale Porosity (Andrey Nasedkin, Anna Nasedkina, Amirtham Rajagopal)....Pages 325-337

Investigation of Initial Stresses’ Influence on Surface Wave Field in Bulk Metallic Glass Layer (T. I. Belyankova, E. I. Vorovich, V. V. Kalinchuk, O. M. Tukodova)....Pages 339-352

Comparison of Two Numerical Inverse Laplace Transform Methods with Application for Problem of Surface Waves Propagation in an Anisotropic Elastic Half-Space (Ivan Markov, Leonid Igumnov)....Pages 353-368

Twofold Re-reflections of Ultrasonic Waves from Obstacles in a Two-Dimensional Elastic Material, Taking into Account Any Laws of Their Reflections and Transformations (Nikolay V. Boyev)....Pages 369-381

On the Use of Models of the Tymoshenko Type in the Analysis of Wave Processes in Wedge-Shaped Waveguides (Aleksandr Vatulyan, Lyubov Parinova)....Pages 383-389

Construction of the Mechanical Model of Keratoprosthesis of the Ocular Cornea (Arkadiy Soloviev, Nadegda Glushko, Alexander Epikhin, Michael Swain)....Pages 391-403

Simulation of the Stress-Strain State of the Spline Joint of the Helicopter Tail Transmission (M. I. Chebakov, S. A. Danilchenko, E. M. Kolosova)....Pages 405-413

Shell with Auxetic Properties in the Model Taking into Account the Transverse Shear (Anatoly S. Yudin)....Pages 415-428

Coupled Problem of Thermoviscoelasticity for Composite Polymer Shell of Revolution (V. G. Safronenko)....Pages 429-438

The Study of Stratification of Multilayer Structures Based on Finite Element Modeling and Neural Network Technologies (A. V. Cherpakov, P. V. Vasiliev, A. N. Soloviev, I. A. Parinov, B. V. Sobol)....Pages 439-447

The Structural Correlation and Mechanical Properties in Amorphous Hafnium Oxide Under Pressure (Nguyen-Hoang Thoan, Nguyen-Trung Do, Nguyen-Ngoc Trung, Le-Van Vinh)....Pages 449-459

A Comparison Study of a DIC and Extensometer on Stress-Strain Curve for AL5052 Aluminum Sheets and Its FEM Applications (Ngoc-Duc Do, Van-Thuong Nguyen, Duc-Toan Nguyen)....Pages 461-474

Front Matter ....Pages 475-475

An Analytical Model for AlGaN/GaN MOS-HEMT for High Power Applications (Nguyen-Trung Do, Nguyen-Hoang Thoan, Tran Minh Quang, Dao Anh Tuan, Nguyen-Ngoc Trung)....Pages 477-485

Structural Scheme of Electroelastic Actuator for Nanomechatronics (Sergey M. Afonin)....Pages 487-502

On Extraction of Energy from Rotating Objects (Tejkaran Narolia, Vijay K. Gupta, Ivan A. Parinov)....Pages 503-511

Computer Modeling and Experimental Research of Component Processing Procedure in the Centrifugal-Rotary Equipment (Nguyen Van Tho, A. N. Soloviev, M. A. Tamarkin, I. A. Panfilov)....Pages 513-528

Optimization Design of a 2-DOF Compliant Parallel Mechanism Using NSGA-II Algorithm for Vibration-Assisted Milling (Huy-Tuan Pham, Van-Khien Nguyen, Khac-Huy Nguyen, Quang-Khoa Dang, Trung-Kien Hoang, Son-Minh Pham)....Pages 529-539

Design and Analysis of a Compliant Constant-Torque Mechanism for Rehabilitation Devices (Thanh-Vu Phan, Huy-Tuan Pham, Cong-Nam Truong)....Pages 541-549

Improve the Loading Capacity and Stiffness of Hydrostatic Spindle Medium Sized Circular Grinding Machines Based on Simulation and Geometric Parameters of the Bearing (Van-Hung Pham, Manh-Toan Nguyen, Tuan-Anh Bui)....Pages 551-558

Inverse Method for Estimating the Convection Coefficient at Gap Inside Bearing Rig Test (Thi-Thao Ngo, Jin H. Huang, Van-The Than)....Pages 559-570

Combining the Kalman Filter and Particle Filter in Object Tracking to Avoid Occlusion Problems (Jen-Hong Lan, Ssu-Wei Chen, Chih-Hsueh Lin, Chin-Shiuh Shieh, Shyh-An Yeh, I-Hsing Tsai et al.)....Pages 571-586

Generative Artificial Neural Network Model for Visualization of Internal Defects of Structural Elements (Arcady Soloviev, Boris Sobol, Pavel Vasiliev, Alexander Senichev)....Pages 587-595

Direct Mapping Based FBMC-LDPC Advanced Underwater Acoustic Transmission Scheme for Data Signals (Chin-Feng Lin, Tsung-Jen Su, Shun-Hsyung Chang, Ivan A. Parinov, Sergey N. Shevtsov)....Pages 597-603

Acquisition and Analysis of Endodontic Handpiece Vibration Signals (Ankit Nayak, P. K. Kankar, Prashant K. Jain, Niharika Jain)....Pages 605-613

Back Matter ....Pages 615-621

- Author / Uploaded
- Ivan A. Parinov
- Shun-Hsyung Chang
- Banh Tien Long

Springer Proceedings in Materials

Ivan A. Parinov Shun-Hsyung Chang Banh Tien Long Editors

Advanced Materials Proceedings of the International Conference on “Physics and Mechanics of New Materials and Their Applications”, PHENMA 2019

Springer Proceedings in Materials Volume 6

Series Editors Arindam Ghosh, Department of Physics, Indian Institute of Science, Bangalore, India Daniel Chua, Department of Materials Science and Engineering, National University of Singapore, Singapore, Singapore Flavio Leandro de Souza, Universidade Federal do ABC, Sao Paulo, São Paulo, Brazil Oral Cenk Aktas, Institute of Material Science, Christian-Albrechts-Universität zu Kiel, Kiel, Schleswig-Holstein, Germany Yafang Han, Beijing Institute of Aeronautical Materials, Beijing, Beijing, China Jianghong Gong, School of Materials Science and Engineering, Tsinghua University, Beijing, Beijing, China Mohammad Jawaid, Laboratory of Biocomposite Tech., INTROP, Universiti Putra Malaysia, Serdang, Selangor, Malaysia

Springer Proceedings in Materials publishes the latest research in Materials Science and Engineering presented at high standard academic conferences and scientiﬁc meetings. It provides a platform for researchers, professionals and students to present their scientiﬁc ﬁndings and stay up-to-date with the development in Materials Science and Engineering. The scope is multidisciplinary and ranges from fundamental to applied research, including, but not limited to: • • • • • • • • •

Structural Materials Metallic Materials Magnetic, Optical and Electronic Materials Ceramics, Glass, Composites, Natural Materials Biomaterials Nanotechnology Characterization and Evaluation of Materials Energy Materials Materials Processing

To submit a proposal or request further information, please contact one of our Springer Publishing Editors according to your afﬁliation: European countries: Mayra Castro ([email protected]) India, South Asia and Middle East: Priya Vyas ([email protected]) South Korea: Smith Chae ([email protected]) Southeast Asia, Australia and New Zealand: Ramesh Nath Premnat (ramesh. [email protected]) The Americas: Michael Luby ([email protected]) China and all the other countries or regions: Mengchu Huang (mengchu. [email protected])

More information about this series at http://www.springer.com/series/16157

Ivan A. Parinov Shun-Hsyung Chang Banh Tien Long •

•

Editors

Advanced Materials Proceedings of the International Conference on “Physics and Mechanics of New Materials and Their Applications”, PHENMA 2019

123

Editors Ivan A. Parinov I. I. Vorovich Mathematics, Mechanics and Computer Sciences Institute Southern Federal University Rostov-on-Don, Russia

Shun-Hsyung Chang Department of Microelectronics Engineering National Kaohsiung University of Science and Technology Kaohsiung, Taiwan

Banh Tien Long School of Mechanical Engineering Hanoi University of Science and Technology Hanoi, Vietnam

ISSN 2662-3161 ISSN 2662-317X (electronic) Springer Proceedings in Materials ISBN 978-3-030-45119-6 ISBN 978-3-030-45120-2 (eBook) https://doi.org/10.1007/978-3-030-45120-2 © Springer Nature Switzerland AG 2020 This work is subject to copyright. All rights are reserved by the Publisher, whether the whole or part of the material is concerned, speciﬁcally the rights of translation, reprinting, reuse of illustrations, recitation, broadcasting, reproduction on microﬁlms or in any other physical way, and transmission or information storage and retrieval, electronic adaptation, computer software, or by similar or dissimilar methodology now known or hereafter developed. The use of general descriptive names, registered names, trademarks, service marks, etc. in this publication does not imply, even in the absence of a speciﬁc statement, that such names are exempt from the relevant protective laws and regulations and therefore free for general use. The publisher, the authors and the editors are safe to assume that the advice and information in this book are believed to be true and accurate at the date of publication. Neither the publisher nor the authors or the editors give a warranty, expressed or implied, with respect to the material contained herein or for any errors or omissions that may have been made. The publisher remains neutral with regard to jurisdictional claims in published maps and institutional afﬁliations. This Springer imprint is published by the registered company Springer Nature Switzerland AG The registered company address is: Gewerbestrasse 11, 6330 Cham, Switzerland

Preface

Materials science is a very quickly developing area of modern science, techniques and technologies. It requires corresponding development of theoretical, experimental and numerical methods, directed on researching and designing numerous advanced materials, composites and structures. Industrial needs are aimed on the manufacture of devices, demonstrating very high accuracy of measurement, reliability and durability. These goods must operate under temperatures and pressures changing into broad limits, as well as in aggressive media. Besides pure scientiﬁc and technical problems, they should decide sharp social tasks of modern life (ecology, medicine, rehabilitation, etc.). At the same time, the quality of these devices and technologies is directly caused by the structure-sensitive properties, physical and mechanical characteristics of used materials. The investigation of modern physical, technical and technological processes also requires the manufacture of materials and devices demonstrating optimal and outstanding properties. This collection of 50 chapters presents selected reports of the 2019 International Conference on “Physics, Mechanics of New Materials and Their Applications” (PHENMA-2019), which has been taken place in Hanoi, Vietnam, November 7–10, 2019 (http://phenma2019.math.sfedu.ru). The conference was sponsored by the National Foundation for Science and Technology Development (Vietnam), Vietnam Union of Science and Technology Associations (VUSTA), Ministry of Education and Science of Russian Federation, Russian Foundation for Basic Research, South Scientiﬁc Center of Russian Academy of Science, Ministry of Science and Technology of Taiwan, The Korean Society of Ocean Engineering (South Korea), New Century Education Foundation (Taiwan), Ocean and Underwater Technology Association (Taiwan), Unity Opto Technology Co. (Taiwan), Fair Well Fishery Co. (Taiwan), Woen Jinn Harbor Engineering Co. (Taiwan), Lorom Group (Taiwan), Longwell Co. (Taiwan), Vietnam Maritime University (Vietnam), Vinh Long University of Technology Education (Vietnam), Hanoi University of Industry (Vietnam), Vietnamese-German University (Vietnam), Ho Chi Minh City University of Agriculture and Forestry (Vietnam), Research Institute of Agriculture Machinery (Vietnam), Don State Technical University (Russia), University of 17 Agustus 1945 Surabaya (Indonesia), v

vi

Preface

University of 45, Surabaya (Indonesia), University of Islam Kadiri (Indonesia), University of Darul Ulum, Jombang (Indonesia), University of Maarif Hasyim Latif, Sidoarjo (Indonesia), PDPM Indian Institute of Information Technology, Design and Manufacturing (India), Korea Maritime and Ocean University (South Korea) and South Russian Regional Centre for Preparation and Implementation of International Projects. The thematic of the PHENMA-2019 continued ideas of previous international symposia and conferences: PMNM-2012 (http://pmnm.math.rsu.ru), PHENMA2013 (http://phenma.math.sfedu.ru), PHENMA-2014 (http://phenma2014.math. sfedu.ru), PHENMA-2015 (http://phenma2015.math.sfedu.ru), PHENMA-2016 (http://phenma2016.math.sfedu.ru), PHENMA-2017 (http://phenma2017.math. sfedu.ru) and PHENMA-2018 (http://phenma2018.math.sfedu.ru), whose results have been published in the following edited books Physics and Mechanics of New Materials and Their Applications, Ivan A. Parinov, Shun-Hsyung Chang (Eds.), Nova Science Publishers, New York, 2013, 444 p. ISBN: 978-1-626-18535-7; Advanced Materials—Physics, Mechanics and Applications, Springer Proceedings in Physics. Vol. 152. Shun-Hsyung Chang, Ivan A. Parinov, Vitaly Yu. Topolov (Eds.), Springer, Heidelberg, New York, Dordrecht, London, 2014, 380 p. ISBN: 978-3-319-03748-6; Advanced Materials—Studies and Applications, Ivan A. Parinov, Shun-Hsyung Chang, Somnuk Theerakulpisut (Eds.), Nova Science Publishers, New York, 2015, 527 p. ISBN: 978-1-634-63749-7; Advanced Materials—Manufacturing, Physics, Mechanics and Applications, Springer Proceedings in Physics, Vol. 175, Ivan A. Parinov, Shun-Hsyung Chang, Vitaly Yu. Topolov (Eds.). Heidelberg, New York, Dordrecht, London: Springer Cham. 2016, 707 p. ISBN: 978-3-319-26322-9; Advanced Materials—Techniques, Physics, Mechanics and Applications, Springer Proceedings in Physics, Vol. 193, Ivan A. Parinov, Shun-Hsyung Chang, Muaffaq A. Jani (Eds.). Springer Nature, Cham, Switzerland. 2017, 627 p. ISBN: 978-3-319-56062-5; Advanced Materials— Proceedings of the International Conference on “Physics and Mechanics of New Materials and Their Applications,” PHENMA-2017, Springer Proceedings in Physics, V. 207, Ivan A. Parinov, Shun-Hsyung Chang, Vijay K. Gupta (Eds.). Springer Nature, Cham, Switzerland. 2018, 640 p. ISBN: 978-3-319-78918-7; Advanced Materials—Proceedings of the International Conference on “Physics and Mechanics of New Materials and Their Applications,” PHENMA-2018, Springer Proceedings in Physics, V. 224, Ivan A. Parinov, Shun-Hsyung Chang, Yun-Hae Kim (Eds.). Springer Nature, Cham, Switzerland. 2019, 666 p. ISBN: 978-3-030-19893-0, respectively. The papers of the PHENMA-2019 are divided into four scientiﬁc directions: (i) Processing Techniques of Advanced Materials, (ii) Physics of Advanced Materials, (iii) Mechanics of Advanced Materials and (iv) Applications of Advanced Materials. Into the framework of the ﬁrst direction, it is considered the influence of composition and structure of Pt-based electrocatalysts on their durability. Then, there are investigations of the effect of organic additives on morphology and electrocatalytic activity of platinum nanomaterials and X-ray spectroscopy study of the

Preface

vii

atomic and electronic structures of polyacrylonitrile-based nanocomposites. Moreover, morphology and structure of carbon nanoparticles, generated from graphite nitrate, are studied also as the formation of surface micro-, nanostructures and wear in nanocomposite coatings with passing to TiN coating deposited by a method combining magnetron sputtering and arc evaporation. Buckling folded composite plate subjected to in-plane loading condition with the cutting process in metallic alloys continues the studies of this part. The ﬁrst part is ﬁnished by considering the optimal technology for processing sport wears from waterproof fabric. The physical topic is opened by the theoretical investigation of the equation for density matrix systems of identical particles. Then, crystal structure and dielectric properties of solid solutions Bi3–xLuxTiNbO9 with high Curie temperature are studied also as an investigation of InSb thin ﬁlms for IR SAW photodetectors. Experimental investigations of optical and dielectric properties of ferroelectric BSN ceramics doped with rare-earth elements and the developed universal technique to determine the intensity of the optical ﬁelds are present in the next chapters. Moreover, the strength of interatomic high-angular bonds in iron and properties of bottom ash particle polymer composites are studied by modern physical methods. Effects of process parameters on surface roughness and methods of its optimization in metallic samples are studied by different theoretical and experimental approaches. Finally, the investigation of technogenic materials, applied for road constructions, ﬁnishes the physical part. In the part of mechanics are present new mathematical and ﬁnite element modeling of active composite materials in original ACELAN-COMPOS package and FEM investigation of effective moduli of transversely isotropic thermoelastic materials with nanoscale porosity. Surface waves in the metallic glass layer with initial stresses and surface wave propagation in anisotropic elastic half-space are investigated in the next chapters also as the problem of re-reflections of ultrasonic waves from obstacles in 2D elastic material. Timoshenko model is used to analyze wave processes in wedge-shaped waveguides, and the mechanical model of a keratoprosthesis of the ocular cornea is developed. Then, the shell with auxetic properties in the model of transverse shear is studied also as the coupled problem of thermoviscoelasticity for composite polymer shell of revolution. The FEM study of the stratiﬁcation of multilayer structures is developed based on neural network technologies. Finally, the structural correlation and mechanical properties in amorphous hafnium oxide under pressure are stated. An analytical model for AlGaN/GaN MOS-HEMT for high-power applications opens the fourth part. The structural scheme of electroelastic actuator for nanomechatronics and the process of extraction of energy from rotating objects are studied. Computer modeling and experimental research of the centrifugal-rotary equipment and also compliant parallel mechanism for vibration-assisted milling are developed. Then, the design and analysis of a compliant constant-torque mechanism for rehabilitation devices are present. Moreover, some actual experimental and theoretical problems are decided on machines with bearings. Combining the Kalman ﬁlter and particle ﬁlter in object tracking is considered, and the artiﬁcial neural network model for visualization of internal defects in structural elements is

viii

Preface

developed. Finally, some approaches and methods for processing the vibration signals in underwater applications and stomatology are discussed. The book will be very useful for students of different levels of education, scientists and engineers, whose research interests are devoted to the development and manufacture of nanomaterials, nanostructures, piezoelectrics and other promising materials and composites with special properties. The book also discusses theoretical and experimental problems, directed to R&D of modern devices based on advanced materials, which are available for a broad spectrum of scientiﬁc and technical applications. The book includes new research results in the ﬁelds of materials science, condensed matter physics, chemistry, mechanics, computational and physical modeling and experiment, manufacture of advanced materials and composites, mathematical processing test results, computational methods and various applications. This edited book was partially supported by Southern Federal University, grant No. VnGr/2020-04-IM (Ministry of Science and Higher Education of the Russian Federation). Rostov-on-Don, Russia Kaohsiung, Taiwan Hanoi, Vietnam February 2020

Ivan A. Parinov Shun-Hsyung Chang Banh Tien Long

Contents

Part I 1

2

Processing Techniques of Advanced Materials

Inﬂuence of Composition and Structure of Pt-Based Electrocatalysts on Their Durability in Different Conditions of Stress-Test . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Elizaveta Moguchikh, Kirill Paperj, Angelina Pavlets, Anastasia Alekseenko, Maria Danilenko, and Aleksey Nikulin 1.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.2 Experimental Part . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.2.1 Preparation of Pt/C Catalysts . . . . . . . . . . . . . . 1.2.2 Preparation of PtCu/C Catalysts . . . . . . . . . . . . 1.2.3 Characterization of the Catalysts Structure . . . . 1.2.4 Electrochemical Measurements . . . . . . . . . . . . 1.3 Results and Discussion . . . . . . . . . . . . . . . . . . . . . . . . . 1.3.1 The Effect of the Size of Pt NPs on the Degree of Degradation of Pt/C Electrocatalysts . . . . . . 1.3.2 The Effect of the Spatial Distribution of Pt NPs on the Degree of Degradation of Pt/C Electrocatalysts . . . . . . . . . . . . . . . . . . . . . . . . 1.3.3 The Effect of the Structure of Bimetallic Nanoparticles on the Stability of Catalysts with Stress Testing . . . . . . . . . . . . . . . . . . . . . 1.4 Conclusions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

....

3

. . . . . . .

. . . . . . .

3 5 6 6 7 7 8

....

8

....

13

.... .... ....

15 19 19

Investigation of the Effect of Different Organic Additives on Morphology and Electrocatalytic Activity of Platinum Nanomaterials Towards Oxygen Reduction Reactions . . . . . . . . . . Sergey V. Belenov, Weldegebriel G. Yohannes, Nikolay V. Lyanguzov, and Vadim A. Volochaev

21

. . . . . . .

. . . . . . .

ix

x

Contents

2.1

Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.1.1 Research Purpose . . . . . . . . . . . . . . . . . . . . 2.2 Experimental . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.2.1 Preparation of Electrode . . . . . . . . . . . . . . . 2.2.2 Electrodeposition of Platinum . . . . . . . . . . . 2.2.3 Characterization of Pt/C . . . . . . . . . . . . . . . 2.3 Results and Discussion . . . . . . . . . . . . . . . . . . . . . . . 2.3.1 Platinum Electrodeposition on Carbon Supported . . . . . . . . . . . . . . . . . . . . . . . . . . 2.3.2 Activity of Platinum Nanomaterials Towards Oxygen Reduction Reactions . . . . . . . . . . . . 2.4 Conclusions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

3

4

5

. . . . . . .

22 23 24 24 24 24 26

......

26

...... ...... ......

29 31 31

. . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

X-ray Spectroscopy Study of the Atomic and Electronic Structure of Polyacrylonitrile-Based Nanocomposites at Different Stages of Formation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . M. A. Kremennaya, V. A. Shmatko, T. A. Mikhailova, E. V. Pronina, K. D. Kosolapova, and G. E. Yalovega 3.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.2 Experiment and Methods . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.3 Results and Discussion . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.4 Conclusion . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Morphology and Structure of Carbon Nanoparticles Generated from Graphite Nitrate Co-intercalation Compound. Effect of Sonication Regime . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . E. V. Raksha, A. A. Davydova, Yu. V. Berestneva, M. V. Savoskin, V. A. Glazunova, A. N. Vdovichenko, O. N. Oskolkova, P. V. Sukhov, V. V. Gnatovskaya, I. A. Verbenko, and Yu. I. Yurasov 4.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.2 Experimental . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.3 Results and Discussion . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.4 Conclusion . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Formation of Surface Micro and Nanostructures When Exposed to Laser UV and VUV Radiation of Nanosecond Duration . . . . . . Vladislav Khomich, Vladimir Yamshchikov, and Sergey Mikolutskiy 5.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.1.1 Research Purpose . . . . . . . . . . . . . . . . . . . . . . . . . 5.1.2 Research Scope . . . . . . . . . . . . . . . . . . . . . . . . . . 5.2 Research Method . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.2.1 Experimental Setup for Direct Laser Micro- and Nanostructuring . . . . . . . . . . . . . . . . . .

.

33

. . . . .

33 34 34 37 38

.

41

. . . . .

42 42 43 46 46

.

49

. . . .

49 50 50 50

.

50

Contents

xi

5.2.2

Theoretical Model of Nanostructure Formation on the Solid Surface Melted by Nanosecond Laser Pulse . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.2.3 Nanostructure Formation Without Melting . . . . . . 5.3 Results and Discussion . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.3.1 Processing by a F2-Laser with Wavelength of 157 Nm . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.3.2 Processing by ArF-Laser with Wavelength of 193 Nm . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.3.3 Processing by a Nd:YaG-Laser with Wavelength of 355 Nm . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.4 Conclusion . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6

7

.. .. ..

52 54 56

..

56

..

57

.. .. ..

58 59 60

..

61

. . . .

. . . .

61 62 62 62

..

62

.. .. ..

64 65 66

..

66

.. .. ..

68 70 70

....

73

....

73

.... .... ....

74 75 78

The Effect of Preliminary Laser Surface Treatment on the Mechanical Properties of a Solid-Phase Compound of an Iron-Nickel Alloy in Diffusion Welding . . . . . . . . . . . . . . . Yury Khomich and Vladimir Yamshchikov 6.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.1.1 Research Purpose . . . . . . . . . . . . . . . . . . . . . . . . 6.1.2 Research Scope . . . . . . . . . . . . . . . . . . . . . . . . . 6.2 Research Method . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.2.1 Experimental Setup for Direct Laser Micro- and Nanostructuring . . . . . . . . . . . . . . . . . 6.2.2 Nano- and Microstructure Formation Under the Action of Laser Pulse . . . . . . . . . . . . . . . . . . 6.2.3 Diffusion Welding . . . . . . . . . . . . . . . . . . . . . . . 6.3 Results and Discussion . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.3.1 Processing by a Scanning Beam of Nd:YAG Laser . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.3.2 Tensile Tests After Diffusion Welding of Samples Treated by Laser . . . . . . . . . . . . . . . . . . . . . . . . . 6.4 Conclusion . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . The Nucleation and Development of Wear in Nanocomposite Coatings Under the Action of a Discrete Vapor-Droplet Flow Valery N. Varavka, Oleg V. Kudryakov, Igor Yu. Zabiyaka, and Natalia I. Bronnikova 7.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7.2 Theoretical Foundations of the Calculate-Analytical Model . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7.3 Estimation of the Model Parameters . . . . . . . . . . . . . . . . 7.4 Research Results and Discussion . . . . . . . . . . . . . . . . . .

xii

Contents

7.5 Conclusion . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 8

9

Mechanical Properties Derived by Spherical Indentation of TiN Coating Deposited by a Method Combining Magnetron Sputtering and Arc Evaporation . . . . . . . . . . . . . . . . . . . . . . . . . Evgeniy Sadyrin, Roman Karotkiyan, Nikolay Sushentsov, Sergey Stepanov, Igor Zabiyaka, Evgeniy Kislyakov, and Alexander Litvinenko 8.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 8.1.1 Research Purpose . . . . . . . . . . . . . . . . . . . . . . . . 8.1.2 Research Scope . . . . . . . . . . . . . . . . . . . . . . . . . 8.2 Research Method . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 8.2.1 Sample Preparation . . . . . . . . . . . . . . . . . . . . . . . 8.2.2 Scanning Electron Microscopy . . . . . . . . . . . . . . 8.2.3 Atomic Force Microscopy . . . . . . . . . . . . . . . . . . 8.2.4 Nanoindentation Test . . . . . . . . . . . . . . . . . . . . . 8.3 Results and Discussion . . . . . . . . . . . . . . . . . . . . . . . . . . . 8.3.1 Coating Thickness and Chemical Composition . . . 8.3.2 Microgeometrical Characteristics . . . . . . . . . . . . . 8.3.3 Mechanical Properties . . . . . . . . . . . . . . . . . . . . . 8.4 Conclusion . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Studies on Predicting Spring-Back and Verifying the Effects of Temperature, Sheet Thickness and Punch Speed on Forming Force of V-Bending for SS400 Steel Plate . . . . . . . . . . . . . . . . . . Gia-Hai Vuong, Thi-Hong-Minh Nguyen, and Duc-Toan Nguyen 9.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.2 Material and Hardening Model . . . . . . . . . . . . . . . . . . . . . 9.2.1 Materials . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.2.2 Hardening Models . . . . . . . . . . . . . . . . . . . . . . . 9.3 Experimental and Finite Element Method of V-Bending . . . 9.3.1 Finite Element Model of V-Bending . . . . . . . . . . 9.3.2 Taguchi Orthogonal Array . . . . . . . . . . . . . . . . . . 9.4 Conclusion . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

10 Buckling Analysis of Folded Composite Plate Subjected to In-Plane Loading Condition . . . . . . . . . . . . . . . . . . . . Bui Van Binh and Le Thuong Hien 10.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 10.2 Theoretical Formulation . . . . . . . . . . . . . . . . . . . . . 10.2.1 Displacement, Strain and Stress Fields . . . 10.2.2 Finite Element Formulations . . . . . . . . . .

82 82

..

85

. . . . . . . . . . . . . .

. . . . . . . . . . . . . .

85 86 86 86 86 87 87 87 89 89 89 91 93 94

..

97

. . . . . . . . .

. . . . . . . . .

98 98 98 101 103 103 105 108 108

. . . . . . . . 109 . . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

109 110 110 111

Contents

10.3

Numerical Results . . . . . . . . . . . . . . . . . . . . . . . . . . . . 10.3.1 Validation Example . . . . . . . . . . . . . . . . . . . 10.3.2 Buckling Analysis of Folded Laminated Plate 10.4 Numerical Results . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

xiii

. . . . .

. . . . .

. . . . .

11 The Effect of Strain Rate on Chip Formation and Cutting Process During High-Speed Cutting of A6061 Aluminum Alloy . . . . . . . Pham Thi Hoa, Banh Tien Long, Nguyen Duc Toan, Doan Thi Huong, and Pham Duc Thanh 11.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 11.2 Mechanical Properties of A6061 Aluminum Alloy . . . . . . . 11.3 Inﬂuence of Strain Rate on Stress in High-Speed Cutting . . 11.4 Simulation Model . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 11.5 Results and Discussion . . . . . . . . . . . . . . . . . . . . . . . . . . . 11.5.1 Inﬂuence of Strain Rate on Stress and Strain During Chip Formation . . . . . . . . . . . . . . . . . . . . . . . . . 11.5.2 Effect of Strain Rate on Cutting Force . . . . . . . . . 11.6 Conclusion . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 12 Prediction of Temperature Distribution in PCBN Cutting Tools in Orthogonal Turning 9XC Hardened Alloy Steels . . . . . . . . . . Dung Thi Quoc Nguyen 12.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 12.2 Temperature Calculation . . . . . . . . . . . . . . . . . . . . . . . . . . 12.2.1 Thermal Model . . . . . . . . . . . . . . . . . . . . . . . . . . 12.2.2 Heat Generation Rate in the Primary Deformation Zone q1 . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 12.2.3 Heat Generation Rate in the Secondary Plastic Zone q2 . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 12.2.4 Heat-Generation Rate at the Tool Flank-Work Interface qw . . . . . . . . . . . . . . . . . . . . . . . . . . . . 12.2.5 Experimental Parameters . . . . . . . . . . . . . . . . . . . 12.2.6 Finite Element Model . . . . . . . . . . . . . . . . . . . . . 12.3 Results and Discussion . . . . . . . . . . . . . . . . . . . . . . . . . . . 12.4 Conclusion . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 13 Study on the Optimal Sealing Technological Regime for Making Sport Wears from Waterproof Fabric . . . . . . . . . . . . . . . . . . . . Tran Thuy Trang and Phan Thanh Thao 13.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 13.2 Experimental Research . . . . . . . . . . . . . . . . . . . . . . . . . . . 13.2.1 Object of Researching . . . . . . . . . . . . . . . . . . . . .

. . . . .

. . . . .

113 113 113 119 120

. . 123

. . . . .

. . . . .

123 124 125 126 127

. . . .

. . . .

127 128 130 130

. . 131 . . 131 . . 132 . . 132 . . 132 . . 133 . . . . . .

. . . . . .

135 135 137 138 138 139

. . 141 . . 141 . . 142 . . 142

xiv

Contents

13.2.2 Research Methodology . . . . . . . . . . . . . . . . . . . Research Results . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 13.3.1 The Results of Each Factors Affect the Adhesion Strength of the Sealing Seam . . . . . . . . . . . . . . . 13.3.2 Effect of Air Temperature on Adhesive Strength of the Sealing Seam . . . . . . . . . . . . . . . . . . . . . 13.4 Conclusion . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 13.3

Part II

. . . 144 . . . 145 . . . 145 . . . 145 . . . 155 . . . 156

Physics of Advanced Materials

14 Equation for Density Matrix Systems of Identical Particles Boris V. Bondarev 14.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 14.2 Equation for the Density Matrix of One Particle . . . . . 14.3 The Hierarchy for the Statistical Operators . . . . . . . . . 14.4 The Equation for the Statistical Operators . . . . . . . . . . 14.5 The Equation for the Density Matrix . . . . . . . . . . . . . 14.6 Kinetic Equation . . . . . . . . . . . . . . . . . . . . . . . . . . . . 14.7 The Energy of the System of Identical Particles Unitary Matrix . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 14.8 Variational Principle . . . . . . . . . . . . . . . . . . . . . . . . . 14.9 Correlation Function . . . . . . . . . . . . . . . . . . . . . . . . . 14.10 The Probability of Transition of a Particle . . . . . . . . . 14.11 Conclusion . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . 159 . . . . . .

. . . . . .

. . . . . .

. . . . . .

. . . . . .

. . . . . .

159 160 162 163 165 167

. . . . . .

. . . . . .

. . . . . .

. . . . . .

. . . . . .

. . . . . .

168 169 170 170 171 171

15 Crystal Structure and Dielectric Properties of Layered Perovskite-Like Solid Solutions Bi3−xLuxTiNbO9 (x = 0, 0.05, 0.1) with High Curie Temperature . . . . . . . . . . . . . . . . . . . . . . . . . . . S. V. Zubkov and S. I. Shevtsova 15.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 15.2 Experimental . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 15.3 Results and Discussion . . . . . . . . . . . . . . . . . . . . . . . . . . . 15.4 Conclusion . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 16 Fabrication and Investigation of InSb Thin Films for IR SAW Photodetectors . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . M. E. Kutepov, T. A. Minasyan, D. A. Zhilin, V. E. Kaydashev, G. Y. Karapetyan, K. G. Abdulvakhidov, S. I. Shevtsova, and E. M. Kaidashev 16.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 16.2 Experimental . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 16.2.1 Synthesis . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . 173 . . . . .

. . . . .

173 174 175 181 182

. . . 183

. . . 183 . . . 184 . . . 184

Contents

xv

16.2.2 16.2.3

Study of InSb Thin Films Structure . . . . . . . . . . Investigation of the Electrical Properties of Thin InSb Films on LiNbO3 and (111) Si Substrates . 16.2.4 Optical Properties of Thin InSb Films . . . . . . . . 16.3 Conclusion . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 17 The Investigation of Optical and Dielectric Properties of Ferroelectric BSN Ceramics Doped with Rare-Earth Elements . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . L. V. Grigoryev, A. A. Semenov, and P. Yu Belyavskiy 17.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . 17.2 Sample Preparation . . . . . . . . . . . . . . . . . . . . . . . 17.3 Structural Properties . . . . . . . . . . . . . . . . . . . . . . 17.4 Dielectric Properties . . . . . . . . . . . . . . . . . . . . . . 17.5 Optical Properties at THz . . . . . . . . . . . . . . . . . . 17.6 Conclusions . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . 185 . . . .

. . . .

. . . .

186 187 189 190

. . . . . . . . . 191 . . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

18 Universal Technique to Determine the Intensity of the Optical Fields, Generated by Laser Interference Meter of Displacements . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . I. P. Miroshnichenko, I. A. Parinov, and V. P. Sizov 18.1 Introduction, Problem Statement, Initial Relations and Assumptions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 18.2 Relations for Determining the Strength and Intensity of the Electromagnetic Field at Observation Points . . . . . . . 18.3 Relations for Determining the Field Falling on the Beam-Splitter Surface . . . . . . . . . . . . . . . . . . . . . . . 18.4 Relations for Determining the Total Field on Beam-Splitter Surface . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 18.5 Relations for Determining the Field and Intensity in the Location Area of Photodetectors in the Case of Using Sinusoidal Diffraction Grating as Beam-Splitter . . 18.6 Conclusion . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 19 Strength of Interatomic Bonds at High-Angle Grain Boundaries in Iron . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Yuri F. Migal 19.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 19.2 High-Angle Grain Boundary Model . . . . . . . . . . . . . . . . . . 19.3 Results of Calculations and Discussion . . . . . . . . . . . . . . . . 19.4 Conclusions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . .

. . . . . . .

191 192 192 194 197 199 200

. . 203

. . 203 . . 205 . . 211 . . 216

. . 221 . . 225 . . 225 . . 227 . . . . .

. . . . .

227 229 232 233 234

xvi

20 Digital Microscopy Image Enhancement Technique for Microstructure Image Analysis of Bottom Ash Particle Polymer Composites . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . F. A. Hermawati, I. M. Kastiawan, and Muhyin 20.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 20.2 Material and Method . . . . . . . . . . . . . . . . . . . . . . . . . 20.2.1 Material Preparation . . . . . . . . . . . . . . . . . . 20.2.2 Proposed Method . . . . . . . . . . . . . . . . . . . . 20.3 Results and Discussion . . . . . . . . . . . . . . . . . . . . . . . 20.4 Conclusion . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

Contents

. . . . . . 235 . . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

21 Analysis of Effect of Oil Viscosity and Temperature on Dynamic Pressure Distribution in Internal Gear Motor and Pump . . . . . . Pham Trong Hoa 21.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 21.2 Formation of the Equation . . . . . . . . . . . . . . . . . . . . . . . . . 21.2.1 Hydrodynamic Pressure Distribution . . . . . . . . . . 21.3 Simulation Results and Discussion . . . . . . . . . . . . . . . . . . . 21.3.1 Effect of Oil Temperature . . . . . . . . . . . . . . . . . . 21.3.2 Effect of Oil Viscosity . . . . . . . . . . . . . . . . . . . . 21.4 Conclusion . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . .

22 Experimental Investigation of Effect of Process Parameters on Surface Roughness in Electrochemical Machining . . . . . . . . Loc P. Ngo, Tai P. Nguyen, and Thanh T. Tran 22.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 22.2 Experimental Study . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 22.2.1 Experimental Preparation and Setup . . . . . . . . . . 22.2.2 Selection of Work Piece and Tool Materials . . . . 22.2.3 Design of Experiments . . . . . . . . . . . . . . . . . . . 22.2.4 Experiments and Data Collection . . . . . . . . . . . . 22.3 Optimal Selection of Process Parameters in ECM Process . 22.3.1 Weka Software for Regression Model . . . . . . . . 22.3.2 Optimal Selection of Process Parameters . . . . . . 22.3.3 Analysis and Validation of Experimental Results 22.4 Conclusion . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . .

. . . . . . .

235 237 237 237 240 244 244

. . 245 . . . . . . . .

245 246 247 248 249 250 252 253

. . . 255 . . . . . . . . . . . .

. . . . . . . . . . . .

255 257 257 259 261 264 265 265 267 267 268 270

23 Optimization of Surface Roughness and Vibration During Thermal—Assisted Milling SKD11 Steel Using Taguchi Method . . . 271 Thi-Bich Mac, Banh Tien Long, and Duc-Toan Nguyen 23.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 271 23.2 Experimental Work . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 272

Contents

23.2.1 Material . . . . . . . . . . . . . . . 23.2.2 Experimental Design . . . . . . 23.3 Control Parameters and Levels . . . . . . 23.4 Results and Discussion . . . . . . . . . . . 23.4.1 Surface Roughness . . . . . . . 23.4.2 Vibration . . . . . . . . . . . . . . 23.4.3 Multi-response Optimization 23.5 Conclusions . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . .

xvii

. . . . . . . . .

. . . . . . . . .

. . . . . . . . .

. . . . . . . . .

. . . . . . . . .

. . . . . . . . .

. . . . . . . . .

. . . . . . . . .

. . . . . . . . .

. . . . . . . . .

. . . . . . . . .

. . . . . . . . .

. . . . . . . . .

. . . . . . . . .

. . . . . . . . .

. . . . . . . . .

24 Assessment of the Surface Roughness of Metal Mechanical Parts by Microsoft Kinect V2 . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Bui Van-Bien, Banh Tien Long, and Nguyen Duc-Toan 24.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 24.2 Related Works . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 24.3 Methodology . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 24.3.1 Measuring of Surface Roughness . . . . . . . . . . . . . 24.3.2 Data Acquisition Using Microsoft Kinect V2 . . . . 24.3.3 PCA Plane Fitting . . . . . . . . . . . . . . . . . . . . . . . . 24.4 Results and Discussion . . . . . . . . . . . . . . . . . . . . . . . . . . . 24.4.1 Experimental Setup . . . . . . . . . . . . . . . . . . . . . . . 24.4.2 Assessment of Surface Roughness . . . . . . . . . . . . 24.5 Conclusion . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 25 New Materials for Road Construction . . . . . . . . . . . . . . . . . . . N. I. Buravchuk, O. V. Guryanova, M. A. Jani, and E. P. Putri 25.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 25.1.1 Purpose of Research . . . . . . . . . . . . . . . . . . . . . 25.1.2 Field of Study . . . . . . . . . . . . . . . . . . . . . . . . . 25.2 Research Method . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 25.3 Results and Discussion . . . . . . . . . . . . . . . . . . . . . . . . . . 25.3.1 Characteristics of Burnt Rocks . . . . . . . . . . . . . . 25.3.2 Burnt Mine Rocks for Subgrade Construction . . . 25.3.3 Physico-Mechanical Properties of Burnt Crushed Stone from Mine Dumps . . . . . . . . . . . . . . . . . . 25.3.4 Materials from Burnt Rocks of Mine Dumps in Structural Layers of Pavements . . . . . . . . . . . 25.4 Discussion . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . .

. . . . . . . . .

272 273 274 276 276 277 277 281 281

. . 283 . . . . . . . . . . .

. . . . . . . . . . .

283 284 285 285 286 287 288 288 290 291 292

. . . 293 . . . . . . .

. . . . . . .

. . . . . . .

293 294 294 295 295 295 299

. . . 301 . . . 302 . . . 305 . . . 306

xviii

Part III

Contents

Mechanics of Advanced Materials

26 Finite Element Modelling of Active Composite Materials in ACELAN-COMPOS Package . . . . . . . . . . . . . . . . . . . . . Andrey Nasedkin 26.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 26.2 Setting of Homogenization Problems . . . . . . . . . . . . . 26.3 Finite Element Approximations . . . . . . . . . . . . . . . . . 26.4 Models of Representative Volumes and Some Results . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . 311 . . . . .

. . . . .

. . . . .

. . . . .

27 Finite Element Investigation of Effective Moduli of Transversely Isotropic Thermoelastic Materials with Nanoscale Porosity . . . . Andrey Nasedkin, Anna Nasedkina, and Amirtham Rajagopal 27.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 27.2 Homogenization Problems . . . . . . . . . . . . . . . . . . . . . . . . . 27.3 Finite Element Approaches and Models of Representative Volumes . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 27.4 Numerical Results . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 28 Investigation of Initial Stresses’ Inﬂuence on Surface Wave Field in Bulk Metallic Glass Layer . . . . . . . . . . . . . . . . . . . . . . . . . . . T. I. Belyankova, E. I. Vorovich, V. V. Kalinchuk, and O. M. Tukodova 28.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 28.2 Formulation of the Problem . . . . . . . . . . . . . . . . . . . . . . . . 28.3 Solution of the Problem . . . . . . . . . . . . . . . . . . . . . . . . . . . 28.3.1 Shear Layer Vibrations . . . . . . . . . . . . . . . . . . . . 28.4 Determination of Initial Stress State . . . . . . . . . . . . . . . . . . 28.5 Numerical Analysis . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 28.5.1 Inﬂuence of Initial Stresses on Dispersion Properties of Layer . . . . . . . . . . . . . . . . . . . . . . . 28.5.2 Inﬂuence of Initial Stresses Magnitude on Surface Waves Velocity . . . . . . . . . . . . . . . . . . . . . . . . . 28.6 Conclusions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 29 Comparison of Two Numerical Inverse Laplace Transform Methods with Application for Problem of Surface Waves Propagation in an Anisotropic Elastic Half-Space . . . . . . . . Ivan Markov and Leonid Igumnov 29.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 29.2 Preliminary Considerations and Test Functions . . . . . . 29.3 Durbin’s Method . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . .

. . . . .

311 313 315 317 322

. . 325 . . 325 . . 327 . . 331 . . 334 . . 337 . . 339

. . . . . .

. . . . . .

339 341 343 344 345 346

. . 347 . . 348 . . 350 . . 352

. . . . . . 353 . . . . . . 353 . . . . . . 354 . . . . . . 357

Contents

xix

29.4 Convolution Quadrature Method . . . . . . . . . . . . . . . . . . . . . . 363 29.5 Conclusions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 367 References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 367 30 Twofold Re-reﬂections of Ultrasonic Waves from Obstacles in a Two-Dimensional Elastic Material, Taking into Account Any Laws of Their Reﬂections and Transformations . . . . . . . Nikolay V. Boyev 30.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 30.2 Problem Statement . . . . . . . . . . . . . . . . . . . . . . . . . . . . 30.3 Solution Method . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 30.4 Study of the Problem in a Local Formulation . . . . . . . . . 30.5 Double Re-reﬂection of Elastic Waves from the Plane Contours of Obstacles, Taking into Account Possible Transformations . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 30.5.1 Case of p-p-p Transformation . . . . . . . . . . . . . 30.5.2 Case of p-p-s Transformation . . . . . . . . . . . . . 30.5.3 Case of p-s-p Transformation . . . . . . . . . . . . . 30.5.4 Case of p-s-s Transformation . . . . . . . . . . . . . . 30.5.5 Case of s-s-s Transformation . . . . . . . . . . . . . . 30.5.6 Case of s-s-p Transformation . . . . . . . . . . . . . . 30.5.7 Case of s-p-s Transformation . . . . . . . . . . . . . . 30.5.8 Case of s-p-p Transformation . . . . . . . . . . . . . 30.6 Conclusion . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . .

. . . .

. . . .

. . . .

369 370 370 371

. . . . . . . . . . .

. . . . . . . . . . .

. . . . . . . . . . .

. . . . . . . . . . .

372 377 377 377 378 378 379 379 380 380 380

31 On the Use of Models of the Tymoshenko Type in of Wave Processes in Wedge-Shaped Waveguides . Aleksandr Vatulyan and Lyubov Parinova 31.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . 31.2 Formulation of Problem . . . . . . . . . . . . . . . . 31.3 The Model of the Timoshenko Type Plate . . 31.4 Computational Experiments . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . .

. . . . 369

the Analysis . . . . . . . . . . . . . 383 . . . . .

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

32 Construction of the Mechanical Model of Keratoprosthesis of the Ocular Cornea . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Arkadiy Soloviev, Nadegda Glushko, Alexander Epikhin, and Michael Swain 32.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 32.1.1 Research Purpose . . . . . . . . . . . . . . . . . . . . 32.1.2 Research Scope . . . . . . . . . . . . . . . . . . . . . 32.2 Research Method . . . . . . . . . . . . . . . . . . . . . . . . . . . 32.2.1 Continuous Formulation of the Problem . . . .

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

383 384 385 387 389

. . . . . . 391

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

391 396 396 396 396

xx

Contents

32.3 Results and Discussion . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 398 32.4 Conclusion . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 400 References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 403 33 Simulation of the Stress-Strain State of the Spline Joint of the Helicopter Tail Transmission . . . . . . . . . . . . . . . . . . . . M. I. Chebakov, S. A. Danilchenko, and E. M. Kolosova 33.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 33.2 Formulation of the Transmission Spline Junction Contact Interaction Problem . . . . . . . . . . . . . . . . . . . . . . . . . . . . 33.3 Finite-Element Simulation of Contact Interaction in Transmission Spline Junction . . . . . . . . . . . . . . . . . . . 33.4 Results . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 33.5 Conclusions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . 405 . . . . 405 . . . . 406 . . . .

. . . .

. . . .

34 Shell with Auxetic Properties in the Model Taking into Account the Transverse Shear . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Anatoly S. Yudin 34.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 34.2 Basic Equations . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 34.3 Method of Solution . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 34.4 Calculations and Analysis . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . .

35 Coupled Problem of Thermoviscoelasticity for Composite Polymer Shell of Revolution . . . . . . . . . . . . . . . . . . . . . . . V. G. Safronenko 35.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 35.2 Methods . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 35.3 Numerical Experiment . . . . . . . . . . . . . . . . . . . . . . . 35.4 Conclusion . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . .

. . . .

408 408 411 413

. . 415 . . . . .

415 416 420 425 428

. . . . . . . 429 . . . . .

. . . . .

. . . . .

. . . . .

36 The Study of Stratiﬁcation of Multilayer Structures Based on Finite Element Modeling and Neural Network Technologies A. V. Cherpakov, P. V. Vasiliev, A. N. Soloviev, I. A. Parinov, and B. V. Sobol 36.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 36.2 Statement of the Problem . . . . . . . . . . . . . . . . . . . . . . . . 36.3 FE Modeling . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 36.4 Application of Neural Network Technologies in the Task of Identifying the Thickness of Hidden Layer of Structure . 36.5 Conclusion . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . .

. . . . .

429 430 433 436 438

. . . 439

. . . 439 . . . 441 . . . 442 . . . 445 . . . 445 . . . 447

Contents

xxi

37 The Structural Correlation and Mechanical Properties in Amorphous Hafnium Oxide Under Pressure . . . . . . . . . . . . Nguyen-Hoang Thoan, Nguyen-Trung Do, Nguyen-Ngoc Trung, and Le-Van Vinh 37.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 37.2 Computational Procedures . . . . . . . . . . . . . . . . . . . . . . . 37.3 Results and Discussion . . . . . . . . . . . . . . . . . . . . . . . . . 37.4 Conclusion . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . 449

. . . . .

. . . . .

38 A Comparison Study of a DIC and Extensometer on Stress-Strain Curve for AL5052 Aluminum Sheets and Its FEM Applications . Ngoc-Duc Do, Van-Thuong Nguyen, and Duc-Toan Nguyen 38.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 38.2 Development of 2D-DIC System and Its Application . . . . . 38.2.1 The 2D-DIC System in House [10] . . . . . . . . . . . 38.2.2 Experiment System . . . . . . . . . . . . . . . . . . . . . . . 38.3 Experiment and Simulation of Tensile Test . . . . . . . . . . . . . 38.3.1 Flow Curve . . . . . . . . . . . . . . . . . . . . . . . . . . . . 38.3.2 FEM Model . . . . . . . . . . . . . . . . . . . . . . . . . . . . 38.3.3 Ductile Damage Model . . . . . . . . . . . . . . . . . . . . 38.3.4 Relationship Between Ductile Damage Parameters for Kim-Tuan Hardening Model . . . . . . . . . . . . . 38.4 Comparison Results . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 38.5 Conclusion . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Part IV

. . . . .

. . . . .

449 450 451 458 459

. . 461 . . . . . . . .

. . . . . . . .

461 462 462 466 467 467 468 469

. . . .

. . . .

471 472 474 474

Applications of Advanced Materials

39 An Analytical Model for AlGaN/GaN MOS-HEMT for High Power Applications . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Nguyen-Trung Do, Nguyen-Hoang Thoan, Tran Minh Quang, Dao Anh Tuan, and Nguyen-Ngoc Trung 39.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 39.2 Simulation Procedure and Experimental . . . . . . . . . . . . . 39.2.1 Simulation Model . . . . . . . . . . . . . . . . . . . . . . 39.2.2 Fabrication Procedure . . . . . . . . . . . . . . . . . . . 39.3 Results and Discussion . . . . . . . . . . . . . . . . . . . . . . . . . 39.3.1 Comparing Simulation and Experiment Results of Conventional HEMT . . . . . . . . . . . . . . . . . . 39.3.2 Comparing Simulation and Experiment Results of MOS-HEMT with Long Channel . . . . . . . . . 39.3.3 Comparing Simulation and Experiment Results of HEMT with Short Channel . . . . . . . . . . . . .

. . . . 477

. . . . .

. . . . .

. . . . .

. . . . .

477 478 479 481 482

. . . . 482 . . . . 483 . . . . 484

xxii

Contents

39.4 Conclusion . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 485 References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 485 40 Structural Scheme of Electroelastic Actuator for Nanomechatronics . . . . . . . . . . . . . . . . . . Sergey M. Afonin 40.1 Introduction . . . . . . . . . . . . . . . . . . . . 40.1.1 Research Purpose . . . . . . . . . 40.1.2 Research Scope . . . . . . . . . . 40.2 Research Method . . . . . . . . . . . . . . . . 40.3 Results and Discussion . . . . . . . . . . . . 40.4 Conclusion . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . 487 . . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

41 On Extraction of Energy from Rotating Objects . . . . Tejkaran Narolia, Vijay K. Gupta, and Ivan A. Parinov 41.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . 41.2 Conﬁguration of Piezoelectric Energy Harvester with Parallel Coaxial Plates . . . . . . . . . . . . . . . 41.3 Results and Discussion . . . . . . . . . . . . . . . . . . 41.4 Conclusion . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

488 489 489 489 498 501 502

. . . . . . . . . . . 503 . . . . . . . . . . . 503 . . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

42 Computer Modeling and Experimental Research of Component Processing Procedure in the Centrifugal-Rotary Equipment . . . . . Nguyen Van Tho, A. N. Soloviev, M. A. Tamarkin, and I. A. Panﬁlov 42.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 42.2 Problem Formulation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 42.2.1 Problem Formulation of Abrasive Particle Movement Taking into Account Friction and Heat Release . . . . . . . . . . . . . . . . . . . . . . . . . 42.2.2 Problem Formulation of Material Removal . . . . . . . 42.3 Finite Element Modeling . . . . . . . . . . . . . . . . . . . . . . . . . . . 42.3.1 Distribution of Stress-Strain State and Temperature Characteristics . . . . . . . . . . . . . . . . . . . . . . . . . . . 42.3.2 Value of Removed Metal from Workpiece Surface . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 42.4 Numerical Results . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 42.4.1 Calculation of Stress-Strain State and Temperature . . . . . . . . . . . . . . . . . . . . . . . . . . 42.4.2 Calculation of Removed Metal from Workpiece Surface . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 42.5 Experiments . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 42.5.1 Technology Equipment . . . . . . . . . . . . . . . . . . . . . 42.5.2 Experimental Research on the CROS-7 . . . . . . . . .

. . . .

504 507 510 511

. 513 . 513 . 514

. 515 . 517 . 518 . 518 . 518 . 520 . 520 . . . .

522 525 525 526

Contents

xxiii

42.6 Conclusion . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 526 References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 527 43 Optimization Design of a 2-DOF Compliant Parallel Mechanism Using NSGA-II Algorithm for Vibration-Assisted Milling . . . . . . Huy-Tuan Pham, Van-Khien Nguyen, Khac-Huy Nguyen, Quang-Khoa Dang, Trung-Kien Hoang, and Son-Minh Pham 43.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 43.2 Problem Formulation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 43.2.1 Design Concept . . . . . . . . . . . . . . . . . . . . . . . . . 43.2.2 Design Concept . . . . . . . . . . . . . . . . . . . . . . . . . 43.3 Results and Discussion . . . . . . . . . . . . . . . . . . . . . . . . . . . 43.4 Conclusion . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . .

44 Design and Analysis of a Compliant Constant-Torque Mechanism for Rehabilitation Devices . . . . . . . . . . . . . . Thanh-Vu Phan, Huy-Tuan Pham, and Cong-Nam Truong 44.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 44.2 Design . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 44.2.1 Operational Principle and Design Concept 44.2.2 Optimization Design of the CFM . . . . . . . 44.3 Results and Discussion . . . . . . . . . . . . . . . . . . . . . 44.4 Conclusions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . .

. . 529

. . . . . . .

529 531 531 532 536 538 539

. . . . . . . . 541 . . . . . . .

. . . . . . .

45 Improve the Loading Capacity and Stiffness of Hydrostatic Spindle Medium Sized Circular Grinding Machines Based on Simulation and Geometric Parameters of the Bearing . . Van-Hung Pham, Manh-Toan Nguyen, and Tuan-Anh Bui 45.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 45.2 Loading Capacity and Stiffness Simulation . . . . . . . . . 45.3 Experimental Setup . . . . . . . . . . . . . . . . . . . . . . . . . . 45.4 Results and Discussion . . . . . . . . . . . . . . . . . . . . . . . 45.5 Conclusion . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

541 542 542 543 545 548 548

. . . . . . 551 . . . . . .

. . . . . .

. . . . . .

. . . . . .

46 Inverse Method for Estimating the Convection Coefﬁcient at Gap Inside Bearing Rig Test . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Thi-Thao Ngo, Jin H. Huang, and Van-The Than 46.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 46.2 Inverse Algorithm . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 46.3 Results and Discussion . . . . . . . . . . . . . . . . . . . . . . . . . . . 46.3.1 Testing Results . . . . . . . . . . . . . . . . . . . . . . . . . . 46.3.2 Inverse Value of h . . . . . . . . . . . . . . . . . . . . . . .

. . . . . .

. . . . . .

551 552 555 556 558 558

. . 559 . . . . .

. . . . .

559 560 566 566 566

xxiv

Contents

46.3.3 Comparison of the Temperature Results . . . . . . . . . . 569 46.4 Conclusion . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 570 References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 570 47 Combining the Kalman Filter and Particle Filter in Object Tracking to Avoid Occlusion Problems . . . . . . . . . . . . . . . . . . . . Jen-Hong Lan, Ssu-Wei Chen, Chih-Hsueh Lin, Chin-Shiuh Shieh, Shyh-An Yeh, I-Hsing Tsai, Chao-Hong Liu, Chin-Dar Tseng, Hung-Yu Wang, Jia-Ming Wu, and Tsair-Fwu Lee 47.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 47.2 Methods . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 47.2.1 KF . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 47.2.2 PF . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 47.2.3 KF and PF Flowchart . . . . . . . . . . . . . . . . . . . . . 47.2.4 KF System . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 47.2.5 PF System . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 47.2.6 Combination of KF and PF . . . . . . . . . . . . . . . . . 47.2.7 Performance Evaluation . . . . . . . . . . . . . . . . . . . . 47.3 Experimental Results . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 47.4 Discussion . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . .

48 Generative Artiﬁcial Neural Network Model for Visualization of Internal Defects of Structural Elements . . . . . . . . . . . . . . . Arcady Soloviev, Boris Sobol, Pavel Vasiliev, and Alexander Senichev 48.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 48.2 Related Work . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 48.3 Proposed Method . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 48.4 Network Architecture . . . . . . . . . . . . . . . . . . . . . . . . . . 48.5 Training Set Preparation . . . . . . . . . . . . . . . . . . . . . . . . 48.6 Neural Network Training . . . . . . . . . . . . . . . . . . . . . . . . 48.7 Results . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 48.8 Conclusion . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . .

. . 571

. . . . . . . . . . . .

572 573 573 574 575 575 578 580 581 582 584 585

. . . . 587

. . . . . . . . .

. . . . . . . . .

49 Direct Mapping Based FBMC-LDPC Advanced Underwater Acoustic Transmission Scheme for Data Signals . . . . . . . . . . . . . . Chin-Feng Lin, Tsung-Jen Su, Shun-Hsyung Chang, Ivan A. Parinov, and Sergey N. Shevtsov 49.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 49.2 Research Method . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 49.3 Simulation Results . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 49.4 Conclusion . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . .

587 588 589 589 590 591 591 592 594

. 597

. . . . .

598 598 599 602 603

Contents

50 Acquisition and Analysis of Endodontic Handpiece Vibration Signals . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Ankit Nayak, P. K. Kankar, Prashant K. Jain, and Niharika Jain 50.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 50.2 Material and Method . . . . . . . . . . . . . . . . . . . . . . . . . . . 50.2.1 Endodontic Handpiece . . . . . . . . . . . . . . . . . . 50.2.2 Experimental Setup and Signal Analysis . . . . . 50.3 Results and Discussion . . . . . . . . . . . . . . . . . . . . . . . . . 50.4 Conclusion . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

xxv

. . . . 605 . . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

606 608 608 609 610 610 612

Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 615

Contributors

K. G. Abdulvakhidov Southern Federal University, Rostov-on-Don, Russia Sergey M. Afonin Institute of Microdevices and Control Systems, National Research University of Electronic Technology (MIET), Moscow, Russia Anastasia Alekseenko Chemistry Department, Southern Federal University, Rostov-on-Don, Russia Sergey V. Belenov Chemistry Faculty, Southern Federal University, Rostov-onDon, Russia T. I. Belyankova Southern Scientiﬁc Center of Russian Academy of Sciences, Rostov-on-Don, Russia; I. I. Vorovich Institute of Mathematics, Mechanics and Computer Science, Southern Federal University, Rostov-on-Don, Russia P. Yu Belyavskiy ETU “LETI”, St. Petersburg, Russia Yu. V. Berestneva Biotechnology Laboratory, Federal State Budget Scientiﬁc Institution “Federal Scientiﬁc Centre of Agroecology, Complex Melioration and Protective Afforestation of the Russian Academy of Sciences”, Volgograd, Russia Bui Van Binh University of Power Electric, Hanoi, Viet Nam Boris V. Bondarev Moscow Aviation Institute, Moscow, Russia Nikolay V. Boyev Southern Federal University, Rostov-on-Don, Russia Natalia I. Bronnikova Material Science Department, Don State Technical University, Rostov-on-Don, Russia Tuan-Anh Bui School of Mechanical Engineering, Hanoi University of Science and Technology, Hanoi, Vietnam N. I. Buravchuk I. I. Vorovich Mathematics, Mechanics and Computer Sciences Institute, Southern Federal University, Rostov-on-Don, Russia

xxvii

xxviii

Contributors

Shun-Hsyung Chang Department of Microelectronic Engineering, National Kaohsiung University of Science and Technology, Kaohsiung, Taiwan, ROC M. I. Chebakov Southern Federal University, Rostov-on-Don, Russia; Rostov State Transport University, Rostov-on-Don, Russia Ssu-Wei Chen Department of Electrical Engineering, National Kaohsiung University of Science and Technology, Kaohsiung, Taiwan, ROC A. V. Cherpakov Department of Theoretical and Applied Mechanics, Don State Technical University, Rostov-on-Don, Russia; Institute of Mathematics, Mechanics and Computer Sciences, Southern Federal University, Rostov-on-Don, Russia Quang-Khoa Dang Faculty of Mechanical Engineering, Ho Chi Minh City University of Technology and Education, Ho Chi Minh City, Vietnam S. A. Danilchenko Southern Federal University, Rostov-on-Don, Russia; Rostov State Transport University, Rostov-on-Don, Russia Maria Danilenko Chemistry Rostov-on-Don, Russia

Department,

Southern

Federal

University,

A. A. Davydova Supramolecular Chemistry Department, L.M. Litvinenko Institute of Physical-Organic and Coal Chemistry, Donetsk, Ukraine Ngoc-Duc Do School of Mechanical Engineering, Hanoi University of Science and Technology, Hai Ba Trung District, Hanoi City, Vietnam Nguyen-Trung Do School of Engineering Physics, Hanoi University of Science and Technology, Hanoi, Vietnam Nguyen Duc-Toan School of Mechanical Engineering, Hanoi University of Technology and Science, Hanoi, Vietnam Alexander Epikhin Don State Medical University, Rostov-on-Don, Russia V. A. Glazunova Department of High-Pressure Physics and Advanced Technologies, Donetsk Institute for Physics and Engineering named after A.A. Galkin, Donetsk, Ukraine Nadegda Glushko Department of Theoretical and Applied Mechanics, Don State Technical University, Rostov-on-Don, Russia V. V. Gnatovskaya Supramolecular Chemistry Department, L.M. Litvinenko Institute of Physical-Organic and Coal Chemistry, Donetsk, Ukraine L. V. Grigoryev ITMO University, St. Petersburg, Russia; ETU “LETI”, St. Petersburg, Russia Vijay K. Gupta PDPM IIITDM Jabalpur, Jabalpur, India

Contributors

xxix

O. V. Guryanova I. I. Vorovich Mathematics, Mechanics and Computer Sciences Institute, Southern Federal University, Rostov-on-Don, Russia F. A. Hermawati Department of Informatics, Universitas 17 Agustus 1945, Surabaya, Indonesia Le Thuong Hien University of Power Electric, Hanoi, Viet Nam Pham Thi Hoa Hung Yen University of Technology and Education, Hung Yen, Viet Nam Pham Trong Hoa University of Transport and Communications (UTC), Hanoi, Vietnam Trung-Kien Hoang Faculty of Mechanical Engineering, Ho Chi Minh City University of Technology and Education, Ho Chi Minh City, Vietnam Jin H. Huang Department of Mechanical and Computer-Aided Engineering, Feng Chia University, Taichung, Taiwan, ROC Doan Thi Huong Hung Yen University of Technology and Education, Hung Yen, Viet Nam Leonid Igumnov Research Institute for Mechanics, National Research Lobachevsky State University of Nizhny Novgorod, Nizhny Novgorod, Russia Niharika Jain Department of Conservative Dentistry and Endodontics, Triveni Institute of Dental Science, Hospital and Research Centre, Bilaspur, Chhattisgarh, India Prashant K. Jain CAD/CAM Lab, Mechanical Engineering Discipline, PDPM, Indian Institute of Information Technology, Design and Manufacturing Jabalpur, Jabalpur, Madhya Pradesh, India M. A. Jani University of 17 Agustus 1945, Surabaya, Indonesia E. M. Kaidashev Southern Federal University, Rostov-on-Don, Russia V. V. Kalinchuk Southern Scientiﬁc Center of Russian Academy of Sciences, Rostov-on-Don, Russia; I. I. Vorovich Institute of Mathematics, Mechanics and Computer Science, Southern Federal University, Rostov-on-Don, Russia P. K. Kankar Discipline of Mechanical Engineering, Indian Institute of Technology Indore, Indore, Madhya Pradesh, India G. Y. Karapetyan Southern Federal University, Rostov-on-Don, Russia Roman Karotkiyan Research and Education Center “Materials”, Don State Technical University, Rostov-on-Don, Russia

xxx

Contributors

I. M. Kastiawan Department of Mechanical Engineering, Universitas 17 Agustus 1945, Surabaya, Indonesia V. E. Kaydashev Southern Federal University, Rostov-on-Don, Russia; Moscow Institute of Physics and Technology, Dolgoprudny, Russia Vladislav Khomich Institute for Electrophysics and Electric Power RAS, Saint-Petersburg, Russia Yury Khomich Institute for Electrophysics and Electric Power RAS, Saint Petersburg, Russia Evgeniy Kislyakov Research and Education Center “Materials”, Don State Technical University, Rostov-on-Don, Russia E. M. Kolosova Southern Federal University, Rostov-on-Don, Russia K. D. Kosolapova Faculty Rostov-on-Don, Russia

of

Physics,

Southern

Federal

University,

M. A. Kremennaya Faculty of Physics, Southern Federal University, Rostov-on-Don, Russia Oleg V. Kudryakov Material Science Department, Don State Technical University, Rostov-on-Don, Russia M. E. Kutepov Southern Federal University, Rostov-on-Don, Russia Jen-Hong Lan Medical Physics & Informatics Lab., Department of Electronics Engineering, National Kaohsiung University of Science and Technology, Kaohsiung, Taiwan, ROC; Medical Physics and Research Department, Hong Kong Sanatorium & Hospital, Hong Kong, China Tsair-Fwu Lee Medical Physics & Informatics Lab., Department of Electronics Engineering, Department of Electrical Engineering, National Kaohsiung University of Science and Technology, Kaohsiung, Taiwan, ROC; Biomedical Engineering, Kaohsiung Medical University, Kaohsiung, Taiwan, ROC Chih-Hsueh Lin Medical Physics & Informatics Lab., Department of Electronics Engineering, National Kaohsiung University of Science and Technology, Kaohsiung, Taiwan, ROC; Biomedical Engineering, Kaohsiung Medical University, Kaohsiung, Taiwan, ROC Chin-Feng Lin Department of Electrical Engineering, National Taiwan Ocean University, Kaohsiung, Taiwan, ROC Alexander Litvinenko Research and Education Center “Materials”, Don State Technical University, Rostov-on-Don, Russia

Contributors

xxxi

Chao-Hong Liu Medical Physics & Informatics Lab., Department of Electronics Engineering, National Kaohsiung University of Science and Technology, Kaohsiung, Taiwan, ROC Banh Tien Long School of Mechanical Engineering, Hanoi University of Science and Technology, Hanoi, Viet Nam Nikolay V. Lyanguzov Physical Faculty, Southern Rostov-on-Don, Russia; Southern Research Center RAS, Rostov-on-Don, Russia

Federal

University,

Thi-Bich Mac Department of Mechanical Engineering, Hung Yen University of Technology and Education, Hung Yen, Vietnam Ivan Markov Research Institute for Mechanics, National Research Lobachevsky State University of Nizhny Novgorod, Nizhny Novgorod, Russia Yuri F. Migal Southern Scientiﬁc Center of Russian Academy of Sciences, Rostov-on-Don, Russian Federation T. A. Mikhailova Faculty Rostov-on-Don, Russia

of

Physics,

Southern

Federal

University,

Sergey Mikolutskiy Institute for Electrophysics and Electric Power RAS, Saint-Petersburg, Russia T. A. Minasyan Southern Federal University, Rostov-on-Don, Russia I. P. Miroshnichenko Don State Technical University, Rostov-on-Don, Russia Elizaveta Moguchikh Chemistry Department, Southern Federal University, Rostov-on-Don, Russia Muhyin Department of Mechanical Engineering, Universitas 17 Agustus 1945, Surabaya, Indonesia Tejkaran Narolia PDPM IIITDM Jabalpur, Jabalpur, India Andrey Nasedkin Institute of Mathematics, Mechanics and Computer Science, Southern Federal University, Rostov-on-Don, Russia Anna Nasedkina Institute of Mathematics, Mechanics and Computer Science, Southern Federal University, Rostov-on-Don, Russia Ankit Nayak CAD/CAM Lab, Mechanical Engineering Discipline, PDPM, Indian Institute of Information Technology, Design and Manufacturing Jabalpur, Jabalpur, Madhya Pradesh, India Loc P. Ngo Department of Global Production Engineering and Management, Vietnamese-German University, Thu Dau Mot City, Binh Duong, Vietnam

xxxii

Contributors

Thi-Thao Ngo Faculty of Mechanical Engineering, Hung Yen University of Technology and Education, Khoai Chau, Hung Yen, Vietnam Duc-Toan Nguyen School of Mechanical Engineering, Hanoi University of Science and Technology, Hai Ba Trung District, Hanoi City, Vietnam Dung Thi Quoc Nguyen Faculty International Training, Thai Nguyen University of Technology, Thai Nguyen, Viet Nam Khac-Huy Nguyen Faculty of Mechanical Engineering, Ho Chi Minh City University of Technology and Education, Ho Chi Minh City, Vietnam Manh-Toan Nguyen School of Mechanical Engineering, Hanoi University of Science and Technology, Hanoi, Vietnam Tai P. Nguyen Department of Global Production Engineering and Management, Vietnamese-German University, Thu Dau Mot City, Binh Duong, Vietnam Thi-Hong-Minh Nguyen School of Mechanical Engineering, Hanoi University of Science and Technology, Hanoi City, Viet Nam Van-Khien Nguyen Faculty of Mechanical Engineering, Ho Chi Minh City University of Technology and Education, Ho Chi Minh City, Vietnam Van-Thuong Nguyen School of Mechanical Engineering, Hanoi University of Science and Technology, Hai Ba Trung District, Hanoi City, Vietnam Aleksey Nikulin Chemistry Department, Southern Federal University, Rostov-onDon, Russia O. N. Oskolkova Supramolecular Chemistry Department, L.M. Litvinenko Institute of Physical-Organic and Coal Chemistry, Donetsk, Ukraine I. A. Panﬁlov Department of Theoretical and Applied Mechanics, Don State Technical University, Rostov-on-Don, Russia Kirill Paperj Chemistry Department, Southern Federal University, Rostov-onDon, Russia I. A. Parinov Institute of Mathematics, Mechanics and Computer Sciences, Southern Federal University, Rostov-on-Don, Russia Ivan A. Parinov I. I. Vorovich Mathematics, Mechanics, and Computer Science Institute, Southern Federal University, Rostov-on-Don, Russia Lyubov Parinova I. I. Vorovich Mathematics, Mechanics and Computer Sciences Institute, Southern Federal University, Rostov-on-Don, Russia Angelina Pavlets Chemistry Rostov-on-Don, Russia

Department,

Southern

Federal

University,

Contributors

xxxiii

Huy-Tuan Pham Faculty of Mechanical Engineering, Ho Chi Minh City University of Technology and Education, Ho Chi Minh City, Vietnam Son-Minh Pham Faculty of Mechanical Engineering, Ho Chi Minh City University of Technology and Education, Ho Chi Minh City, Vietnam Van-Hung Pham School of Mechanical Engineering, Hanoi University of Science and Technology, Hanoi, Vietnam Thanh-Vu Phan Faculty of Mechanical Engineering, HCMC University of Technology and Education, Ho Chi Minh City, Vietnam E. V. Pronina Faculty of Physics, Southern Federal University, Rostov-on-Don, Russia E. P. Putri University of 17 Agustus 1945, Surabaya, Indonesia Tran Minh Quang School of Engineering Physics, Hanoi University of Science and Technology, Hanoi, Vietnam Amirtham Rajagopal Department of Civil Engineering, Indian Institute of Technology, Hyderabad, India E. V. Raksha Supramolecular Chemistry Department, L.M. Litvinenko Institute of Physical-Organic and Coal Chemistry, Donetsk, Ukraine Evgeniy Sadyrin Research and Education Center “Materials”, Don State Technical University, Rostov-on-Don, Russia V. G. Safronenko I. I. Vorovich Mathematics, Mechanics and Computer Sciences Institute, Southern Federal University, Rostov-on-Don, Russia M. V. Savoskin Supramolecular Chemistry Department, L.M. Litvinenko Institute of Physical-Organic and Coal Chemistry, Donetsk, Ukraine A. A. Semenov ETU “LETI”, St. Petersburg, Russia Alexander Senichev Department of Information Technologies, Don State Technical University, Rostov-on-Don, Russia Sergey N. Shevtsov South Center of Russian Academy of Science, Rostov-onDon, Russia S. I. Shevtsova Institute of Earth Science, Southern Federal University, Rostov-on-Don, Russia Chin-Shiuh Shieh Medical Physics & Informatics Lab., Department of Electronics Engineering, National Kaohsiung University of Science and Technology, Kaohsiung, Taiwan, ROC; Biomedical Engineering, Kaohsiung Medical University, Kaohsiung, Taiwan, ROC

xxxiv

Contributors

V. A. Shmatko Faculty of Physics, Southern Federal University, Rostov-on-Don, Russia V. P. Sizov Southern Federal University, Rostov-on-Don, Russia B. V. Sobol Department of Information Technologies, Don State Technical University, Rostov-on-Don, Russia Boris Sobol Department of Information Technologies, Don State Technical University, Rostov-on-Don, Russia Arcady Soloviev Department of Theoretical and Applied Mechanics, Don State Technical University, Rostov-on-Don, Russia; Institute of Mathematics, Mechanics and Computer Sciences, Southern Federal University, Rostov-on-Don, Russia Arkadiy Soloviev Department of Theoretical and Applied Mechanics, Don State Technical University, Rostov-on-Don, Russia A. N. Soloviev Department of Theoretical and Applied Mechanics, Don State Technical University, Rostov-on-Don, Russia; Institute of Mathematics, Mechanics and Computer Sciences, Southern Federal University, Rostov-on-Don, Russia Sergey Stepanov Volga State University of Technology, Yoshkar-Ola, Russia Tsung-Jen Su Department of Electrical Engineering, National Taiwan Ocean University, Kaohsiung, Taiwan, ROC P. V. Sukhov Supramolecular Chemistry Department, L.M. Litvinenko Institute of Physical-Organic and Coal Chemistry, Donetsk, Ukraine Nikolay Sushentsov Volga State University of Technology, Yoshkar-Ola, Russia Michael Swain Sydney University, Sydney, Australia M. A. Tamarkin Department of Mechanical Engineering, Don State Technical University, Rostov-on-Don, Russia Van-The Than Faculty of Mechanical Engineering, Hung Yen University of Technology and Education, Khoai Chau, Hung Yen, Vietnam Pham Duc Thanh Hanoi University of Transport and Communications, Hanoi, Viet Nam Phan Thanh Thao Hanoi University of Science and Technology, Hanoi, Vietnam Nguyen Van Tho Department of Theoretical and Applied Mechanics, Department of Mechanical Engineering, Don State Technical University, Rostov-on-Don, Russia; Faculty of Mechanical Engineering, Hai Phong University, Hai Phong City, Vietnam

Contributors

xxxv

Nguyen-Hoang Thoan School of Engineering Physics, Hanoi University of Science and Technology, Hanoi, Vietnam Nguyen Duc Toan School of Mechanical Engineering, Hanoi University of Science and Technology, Hanoi, Viet Nam Thanh T. Tran Department of Global Production Engineering and Management, Vietnamese-German University, Thu Dau Mot City, Binh Duong, Vietnam Tran Thuy Trang Hanoi University of Science and Technology, Hanoi, Vietnam Nguyen-Ngoc Trung School of Engineering Physics, Hanoi University of Science and Technology, Hanoi, Vietnam Cong-Nam Truong Faculty of Mechanical Engineering, HCMC University of Technology and Education, Ho Chi Minh City, Vietnam I-Hsing Tsai Medical Physics & Informatics Lab., Department of Electronics Engineering, National Kaohsiung University of Science and Technology, Kaohsiung, Taiwan, ROC Chin-Dar Tseng Medical Physics & Informatics Lab., Department of Electronics Engineering, National Kaohsiung University of Science and Technology, Kaohsiung, Taiwan, ROC Dao Anh Tuan School of Engineering Physics, Hanoi University of Science and Technology, Hanoi, Vietnam O. M. Tukodova Don State Technical University, Rostov-on-Don, Russia Bui Van-Bien Department of Mechanical Engineering, Haiphong University, Haiphong, Vietnam Valery N. Varavka Material Science Department, Don State Technical University, Rostov-on-Don, Russia P. V. Vasiliev Department of Information Technologies, Don State Technical University, Rostov-on-Don, Russia Pavel Vasiliev Department of Information Technologies, Don State Technical University, Rostov-on-Don, Russia Aleksandr Vatulyan I. I. Vorovich Mathematics, Mechanics and Computer Sciences Institute, Southern Federal University, Rostov-on-Don, Russia A. N. Vdovichenko Supramolecular Chemistry Department, L.M. Litvinenko Institute of Physical-Organic and Coal Chemistry, Donetsk, Ukraine I. A. Verbenko Research Institute of Physics, Southern Federal University, Rostov-on-Don, Russia Le-Van Vinh Phenikaa University, Hanoi, Vietnam

xxxvi

Contributors

Vadim A. Volochaev Chemistry Faculty, Southern Federal University, Rostovon-Don, Russia E. I. Vorovich Don State Technical University, Rostov-on-Don, Russia Gia-Hai Vuong School of Mechanical Engineering, Hanoi University of Science and Technology, Hanoi City, Viet Nam; Hai Phong University, Hai Phong, Viet Nam Hung-Yu Wang Medical Physics & Informatics Lab., Department of Electronics Engineering, National Kaohsiung University of Science and Technology, Kaohsiung, Taiwan, ROC; Biomedical Engineering, Kaohsiung Medical University, Kaohsiung, Taiwan, ROC Jia-Ming Wu Department of Biomedicine Engineering, Department of Medical Physics, Chengde Medical University, Chengde, Hebei, China; Department of Radiation Oncology, Yee-Zen Hospital, Tao Yuan City, Taiwan, ROC G. E. Yalovega Faculty of Physics, Southern Federal University, Rostov-on-Don, Russia Vladimir Yamshchikov Institute for Electrophysics and Electric Power RAS, Saint-Petersburg, Russia Shyh-An Yeh Medical Physics & Informatics Lab., Department of Electronics Engineering, National Kaohsiung University of Science and Technology, Kaohsiung, Taiwan, ROC Weldegebriel G. Yohannes Department of Chemistry, College of Natural and Computational Sciences, Addis Ababa University, Addis Ababa, Ethiopia Anatoly S. Yudin I. I. Vorovich Institute of Mathematics, Mechanics and Computer Sciences, Southern Federal University, Rostov-on-Don, Russia Yu. I. Yurasov Research Institute of Physics, Southern Federal University, Rostov-on-Don, Russia; Southern Scientiﬁc Centre RAS, Rostov-on-Don, Russia Igor Zabiyaka Research and Education Center “Materials”, Don State Technical University, Rostov-on-Don, Russia Igor Yu. Zabiyaka Material Science Department, Don State Technical University, Rostov-on-Don, Russia D. A. Zhilin Southern Federal University, Rostov-on-Don, Russia S. V. Zubkov Research Institute of Physics, Southern Federal University, Rostov-on-Don, Russia

Part I

Processing Techniques of Advanced Materials

Chapter 1

Influence of Composition and Structure of Pt-Based Electrocatalysts on Their Durability in Different Conditions of Stress-Test Elizaveta Moguchikh, Kirill Paperj, Angelina Pavlets, Anastasia Alekseenko, Maria Danilenko, and Aleksey Nikulin Abstract Stability in the course of exploitation and catalytic activity in reactions, taking place on the electrodes, are the most important characteristics of electrocatalysts that determine their application in fuel cells. Relationship of the electrochemical behavior of Pt/C and PtCu/C catalysts with their morphology is studied in this chapter. In according with results of our study, Pt(Cu)/C materials with core-shell architecture of two-component nanoparticles can be a promising direction in electrocatalysis. Such materials can exhibit high specific characteristics, while being characterized by a reduced content of platinum and a low percentage of d-metal dissolution. The resulting Pt/C catalysts are characterized by surface area values from 11 to 80 m2 /g(Pt), average crystallite size from 1.1 to 5.7 nm, mass fraction of platinum from 18 to 39% and relative stability during long-term stress testing of more than 70%, which is comparable to or exceeds this value for the commercial catalyst JM20.

1.1 Introduction In recent years, research in the development of low temperature fuel cells (LT PEMFC) has become important due to the growing environmental problems in the world. LT PEMFC are devices that are promising alternative energy sources [1–3]. One of the most important parts of low-temperature fuel cells is a membrane coated with catalytic layers [1–5]. It is the component part of the device that makes it possible to increase the efficiency of current-forming reactions: electrooxidation of methanol and hydrogen, electroreduction of oxygen (ORR) [6, 7]. The nanoparticles (NPs) of platinum and its alloys deposited and evenly distributed over the surface of the carbon support are considered promising materials used as catalysts in the membrane-electrode block of fuel cells (FCs) [1–7]. Unfortunately, the high cost of platinum is one of the factors that impede the widespread use of devices based on low-temperature FCs [6–8]. The stability of the catalyst is its ability E. Moguchikh · K. Paperj · A. Pavlets · A. Alekseenko (B) · M. Danilenko · A. Nikulin Chemistry Department, Southern Federal University, Rostov-on-Don, Russia e-mail: [email protected] © Springer Nature Switzerland AG 2020 I. A. Parinov et al. (eds.), Advanced Materials, Springer Proceedings in Materials 6, https://doi.org/10.1007/978-3-030-45120-2_1

3

4

E. Moguchikh et al.

to maintain high functional characteristics during the operation of the LT PEMFC [1–8]. Thus, one of the urgent tasks is the development of Pt-containing catalysts with a low percentage of precious metal and, at the same time, with high specific characteristics, in particular high stability [8–11]. Methods of studying the structural and electrochemical characteristics of catalysts are of great importance in the field of research of alternative energy sources [1, 5–8]. The study of the relationship between the conditions of electrochemical measurements and the degradation mechanisms of platinum-containing materials plays a special role. Stability is the ability of materials to maintain their functional characteristics during prolonged electrochemical testing [12–15]. As we know, in the process of a stress test, a deterioration of the initial characteristics of the material is observed, which is associated with its degradation. The degradation of platinum-containing catalysts in a fuel cell depends on several parameters related to the operating conditions of the membrane-electrode block and to the structure and composition of the electrocatalyst, for example the size of the NPs, their distribution over the surface of the substrate, and the type of support. Various studies of the degradation process have shown what changes can occur with the catalysts (Fig. 1.1). Most studies present two major degradation processes associated with the oxidation of a carbon support (Corrosion of Carbon Support) and the degradation of platinum NPs (Dissolution of Pt NPs and Alloy d-Metal) [16]. During the degradation of the carbon support, the detachment of carbon parts with deposited metal particles occurs. This process leads to a loss of electronic contact and a subsequent decrease in the qualitative characteristics of the samples [17–19]. It is known that the larger the average size of NPs and the mass fraction of platinum in the catalyst, the higher is the stability of Pt/C electrocatalysts [17–20]. An electrocatalyst containing large NPs degrades to a lesser extent during the operation of a fuel cell. This occurs due to the almost complete absence of processes associated

Fig. 1.1 Degradation processes Pt/C and PtM/C electrocatalysts during operation in the membraneelectrode assembly

1 Influence of Composition and Structure …

5

with the movement of NPs on the surface of the support, the aggregation and dissolution of small platinum NPs due to their strong fixation on a carbon support and greater thermodynamic stability of large particles. However, such materials are also characterized by a small electrochemically active surface area [12, 16, 17, 20, 21]. Catalysts containing platinum NPs smaller than 2 nm are more susceptible to degradation due to the greater contribution of the oxidation of the carbon support. The increased rate of this oxidation can be associated with the catalytic activity of platinum NPs, which accelerate the process of carbon oxidation [18–21]. The transition to bimetallic NPs made it possible to reduce the degree of degradation of the obtained electrocatalysts [12, 22]. Apparently, the d-metal stabilizes the system due to the fact that a certain fraction of platinum NPs, which is located on the surface of the alloying component, does not have a direct contact with the carbon substrate. This reduces the catalytic effect of the noble metal on the oxidation of the carbon support [12, 23]. Testing in the membrane-electrode block is the best way to measure the stability of the materials, but they are rather laborious, expensive and energy intensive. Therefore, many studies are aimed at the rapid assessment in laboratory conditions, which is closest to real conditions [12, 22–24]. The most common method of studying the stability of electrocatalysts in laboratory conditions is the repetition of a cyclic potential sweep, accompanied by periodic measurement of ESA and specific activity of the catalyst [12]. For stress-tests carried out in laboratory conditions, an important role is played by the range of potentials, sweep speed, electrolyte composition, medium, and temperature [12, 16–18, 20]. Many authors argue that the contribution of each of the above degradation processes is unequal and depends on the range of stress test potentials [10, 11, 14]. There are two main areas of potentials for studying the degradation of platinumcontaining electrocatalysts [17, 18, 20, 24]. In the range 0.4–1.0 V, degradation processes mainly occur associated with the conversion of metal NPs distributed over the surface of the support. At potentials above 1.1 V, processes leading to material degradation due to oxidation of the carbon support make a greater contribution [18, 22, 24, 25]. The purpose of this study is to identify the relationship between structural characteristics and corrosion-morphological stability during stress testing of platinum electrocatalysts for low-temperature fuel cells.

1.2 Experimental Part As the materials under study, various methods of liquid-phase synthesis were used to obtain a number of Pt/C electrocatalysts that differ in the mass fraction of platinum and the crystallite size and a series of PtCu/C materials obtained by the liquid-phase synthesis method with the assumed structure of the shell-core NPs and an alloy

6 Table 1.1 Catalyst names and reducing agents used

E. Moguchikh et al. Sample

Reducing agents

S-1, S-2

Hydrazine hydrate

S-3, S-4, S-10

Sodium borohydride

S-5

Formic acid

S-6, S-11

Ethylene glycol

S-7, S-8, S-9, S-12, S-13, S-14, S2-1, S2-2, S2-3, S2-4, S2-5

Formaldehyde

with different architecture of the NPs. The obtained samples were compared with each other, as well as with the behavior of the commercial Pt/C electrocatalyst JM (Johnson Matthey, 20% Pt).

1.2.1 Preparation of Pt/C Catalysts The synthesis of platinum-carbon catalysts was carried out by chemical reduction of the Pt (IV) precursor (H2 PtCl6 · 6H2 O) in the liquid phase. Vulcan XC-72 brand carbon black was used as a support. The synthesis of each of the samples was repeated at least three times, which made it possible to evaluate the reproducibility of the structural and electrochemical characteristics of the obtained materials. Platinum-carbon catalysts were obtained by chemical reduction in the liquid phase using various reducing agents according to Table 1.1. More synthesis methods are described previously in [26].

1.2.2 Preparation of PtCu/C Catalysts Platinum-copper electrocatalysts were obtained by sequential reduction of metals in several stages, with a gradual decrease in the concentration of the copper precursor and an increase in the concentration of the platinum precursor to create a uniform shell. The molar ratio in the obtained samples was Pt:Cu = 1:1 and the loading of metals 30% (20% Pt). Electrocatalysts were obtained by liquid phase synthesis with carbon black Vulcan XC-72 used as a carbon support, and sodium borohydride as a reducing agent. The preparation of PtCu/C catalysts is described in more detail in the article [27].

1 Influence of Composition and Structure …

7

1.2.3 Characterization of the Catalysts Structure The mass loading of metals in the samples was determined by the mass of the residue, which consisted of Pt and copper (II) oxide, remaining unburned after heating to 800 °C. The ratio of copper and platinum in the samples was determined by Xray fluorescence analysis on spectrometer with complete external reflection of Xray radiation RFS-001 (Research Institute of Physics, Southern Federal University). Control over the metal component composition of the catalysts was carried out before and after the stress testing. To determine the average crystallite size, the X-ray phase analysis (XRD) was used. The X-ray diffractograms of Pt/C materials were recorded in the angle range 2θ = 15°–55° on an ARL X’TRA diffractometer (Thermo Fisher Scientific, Switzerland) using filtered CuKα radiation (λ = 0.154056 nm) at room temperature. The calculation of Dav was carried out for a characteristic reflection of 111 by the Scherrer formula [26]. The microstructure of the samples was studied by transmission electron microscopy (TEM). Photographs were taken with a JEM-2100 microscope (JEOL, Japan) at a voltage of 200 kV and a resolution of 0.2 nm.

1.2.4 Electrochemical Measurements Electrochemical measurements were carried out in a standard three-electrode cell at a temperature of 25 °C. 0.1 M HClO4 saturated with argon was used as the electrolyte. All potentials in the work are given relative to a reversible hydrogen electrode. The studied catalyst was deposited on the end face of a rotating disk electrode in the form of catalytic “inks”, as described in [28]. Before measuring the electrochemically active surface area (ESA) of the catalyst, the electrolyte was saturated with argon for 40 min. 100 cycles are recorded in the potential range from −0.23 to 1.26 V relative to the silver chloride electrode. The sweep rate is 200 mV/s. Calculation of ESA was carried out by the amount of electricity spent on the electrochemical adsorption and desorption of atomic hydrogen, taking into account the contribution of the charging currents of the double electric layer, as described in [28]. As methods for assessing the degree of degradation electrocatalysts, were selected the cyclic voltammetry methods in the potential range 0.6–1.0 V (RHE) with a sweep rate of 100 mV/s and 0.6–1.4 V (RHE) with a sweep rate of 100 mV/s. The cycling was carried out in a 0.1 M solution of HClO4 saturated with argon at 25 °C; the number of cycles that were recorded—5000 and 500 respectively. After every 500 or 100 cycles, two CV were recorded at a potential sweep rate of 20 mV/s in the potential range from −0.23 to 1.26 V relative to the silver chloride electrode. According to the second CV, ESA was calculated as described previously.

8

E. Moguchikh et al.

The stability was assessed by the relative change in the ESA of platinum before j (S0ESA ) and after (SESA ) stress test according to Formula (1.1). j Stability = SESA /S0ESA × 100%,

(1.1)

where j is the number of potential sweep cycles carried out before a specific SESA measurement, S0ESA is the initial area measured after standardization. The degree of degradation was calculated using Formula (1.2): j Degree of degradation = 1 − SESA /S0ESA × 100%.

(1.2)

1.3 Results and Discussion 1.3.1 The Effect of the Size of Pt NPs on the Degree of Degradation of Pt/C Electrocatalysts In the course of the research work, 8 Pt/C catalyst were synthesized with various NP sizes from 1.1 to 5.7 nm and a close platinum mass fraction of 20% (Table 1.2). Figure 1.2 schematically depicts the arrangement of platinum NPs on the surface of a carbon support for catalysts characterized by a close metal mass fraction and different average NP sizes. X-ray diffraction patterns of the studied catalysts have the form characteristic of the deposited Pt/C materials (Fig. 1.3). The presence of nanosized crystallites of platinum causes a broadening of the characteristic platinum maxima, and with a decrease in the average crystallite size Table 1.2 Structural and electrochemical characteristics of the synthesized Pt/C catalysts Sample

ω(Pt), %

Dav , nm

ESA0 , m2 /g(Pt)

Sgeom , m2 /g(Pt)

Degree of aggregation

S-1

19 ± 0.6

5.7

12 ± 1

48

0.75

S-2

21.8 ± 0.7

5.2

13 ± 1

54

0.76

S-3

20.2 ± 0.6

3.7

20 ± 2

75

0.73

S-4

20.7 ± 0.6

3.5

49 ± 5

79

0.38

S-5

18 ± 0.5

2.6

54 ± 5

106

0.49

S-6

23.5 ± 0.7

2.1

59 ± 6

135

0.56

20 ± 0.6

2.0

86 ± 9

140

0.39

S-7

19.5 ± 0.6

1.3

78 ± 8

214

0.63

S-8

19 ± 0.6

1.1

111 ± 11

248

0.55

JM20

1 Influence of Composition and Structure …

9

Fig. 1.2 Schematic representation of the location of NP platinum of various sizes on the surface of the carbon support of catalysts with a close mass fraction of metal

Fig. 1.3 XRD patterns of the Pt/C materials

(Dav ), this broadening increases. The results of calculating the Dav according to the Scherrer equation are shown in Table 1.2. The smallest platinum crystallites 1.1 and 1.3 nm are characterized by samples S-8 and S-7, respectively, obtained by the liquid-phase synthesis method using formaldehyde as a reducing agent. Samples S-1 and S-2 obtained using hydrazine as a reducing agent contain platinum crystallites of the largest size of all synthesized samples—more than 5 nm. In order to assess the degree of aggregation of NPs (the fraction of platinum particles “stuck together” during the synthesis), we compared the electrochemical (experimentally determined) and geometric (calculated value) surface areas. For each of the samples, the degree of aggregation was calculated using (1.3): Degree of aggregation = 1 −

ESA Sgeom

(1.3)

where ESA is the electrochemically active surface area determined according to the CV data; Sgeom is the geometric area calculated as Sgeom =

6 ∗ 1000 DNP ∗ ρ(Pt)

(1.4)

10

E. Moguchikh et al.

where ρ(Pt) is the platinum density equal to 21.4 g/cm3 ; DNP was calculated using the Scherrer equation using X-ray analysis data. The higher the difference between the values of the electrochemical and geometric areas, the higher the parameter—the degree of aggregation, and the investigator, the higher the proportion of large NPs. So, for samples S-1, S-2, S-3, S-6 and S-7, the highest degree of aggregation of platinum particles was determined. On the CV obtained during standardization of the electrodes, a change in the currents in the hydrogen region is observed for all Pt/C materials (Fig. 1.4). This may be due to the cleaning of the surface of the catalysts from organic compounds remaining after synthesis. Thus, in the process of standardization, a significant change in the parameters of the hydrogen, and often oxygen, regions of the CV occur, followed by stabilization of the electrode characteristics of the material (Fig. 1.4). The largest number of development cycles is observed for catalysts S-6, S-8 and commercial JM20. The electrochemically active surface area was determined after the standardization stage by the method of cyclic voltammetry (Fig. 1.5). During prolonged stress testing, two CVs were recorded every 500 cycles to calculate the intermediate ESA values. Figure 1.5 shows the initial and final (after stress testing) CV Pt/C catalysts. Voltammograms of all investigated electrocatalysts have a characteristic form for nanosized platinum (Fig. 1.5). The currents in the hydrogen region are maximum for sample S-8 (Fig. 1.5). Accordingly, this material is also characterized by the highest active surface area among the obtained Pt/C catalysts (Table 1.2). For samples S-1, S-2, and S-3, the currents in the hydrogen region are noticeably lower in comparison with other Pt/C catalysts presented.

Fig. 1.4 Cyclic voltammograms of the metal-carbon catalysts in the process of standardizing cycling. Samples: 1—S-1, 2—S-2, 3—S-3, 4—S-4, 5—S-5, 6—S-6, 7—JM20, 8—S-7, 9—S8100 cycles. The sweep rate of the potential is 200 mV/s. 0.1 M HClO4 solution saturated by Ar at room temperature

1 Influence of Composition and Structure …

11

Fig. 1.5 Cyclic voltammograms of commercial Pt/C electrodes after surface standardization. Sample: 1—S-1, 2—S-2, 3—S-3, 4—S-4, 5—S-5, 6—S-6, 7—JM20, 8—S-7, 9—S-8. Electrolyte is 0.1 M HClO4 saturated by Ar at room temperature. The sweep rate is 20 mV/s

The experiment showed that for the majority of the studied samples the ratio is satisfied: the smaller the average diameter of the platinum crystallites contained in the Pt/C catalyst, the higher the active surface area is characterized by the sample (Table 1.2). It is worth noting that sample S-7 falls out of this dependence, containing relatively small platinum crystallites of about 1.3 nm and, at the same time, characterized by a smaller surface area compared to the commercial analogue of JM20 (Table 1.2). Sample S-7 apparently contains larger platinum NPs consisting of small crystallites, as indicated by the high degree of aggregation. It is important to note that when comparing the initial CV and CV after stress testing, a decrease in currents in the hydrogen region is observed for samples S-5, S-6, JM20, S-7, S-8, which leads to a more pronounced decrease in surface area (Fig. 1.5; Table 1.2). The degree of degradation of Pt/C catalysts during repeated (5000 cycles) voltammetric cycling in the potential range 0.6–1.0 V was estimated by the change in the electrochemically active surface area (Fig. 1.6). It is believed that this potential range corresponds to the “soft mode” of stress testing, in which processes associated with platinum NPs (separation of particles from the surface, agglomeration, dissolution of platinum) make a significant contribution to the degradation of the electrocatalyst [17]. The highest stability is demonstrated by samples S-1, S-2, S-3 and S-4, more than 90%, characterized by the largest platinum crystallite size (Table 1.3; Fig. 1.6). Larger particles are better attached to the carbon support and, therefore, to a lesser

12

E. Moguchikh et al.

Fig. 1.6 Dependence of the relative degree of degradation (a) and ESA (b) on the number of cycles during cycling in the potential range 0.6–1.0 V

Table 1.3 Sample characteristics calculated after stress testing

Sample

ESA5000 , m2 /g(Pt)

Relative stability, %

S-1

11 ± 1

92

S-2

12 ± 1

92

S-3

18 ± 2

90

S-4

47 ± 5

96

S-5

47 ± 5

87

S-6

45 ± 5

76

JM20

61 ± 6

71

S-7

58 ± 6

74

S-8

80 ± 8

72

extent detach and aggregate. These samples were obtained using reducing agents of hydrazine and sodium borohydride. Samples S-6, S-7, S-8 and the JM20 catalyst are characterized by the lowest stability during prolonged stress testing—about 70% and the lowest average crystallite size from 1.1 to 2.1 nm. The rapid degradation of these materials is associated with the small size of the NPs, which are irreversibly detached from the surface of the support, agglomerate during cycling, dissolve and reprecipitate to form larger particles. It should be noted that sample S-4 shows high relative stability throughout the stress test, despite the relatively large crystallite size of 3.5 nm and a moderate surface area of 49 m2 /g(Pt). On the one hand, this high stability can be explained by the equal distance of platinum NPs from each other on the surface of the support and, therefore, they tend to aggregate to a lesser extent, as well as crystallites of more than 3 nm are better attached to the carbon support. It is important to note that all samples are characterized by a monotonous decrease in ESA during stress testing (Fig. 1.6b). Despite the high degree of degradation, the highest residual surface area is characterized by sample S-8, the value of which exceeds the ESA of the commercial analogue—JM20. Thus, we can conclude that with an increase in the particle size of platinum, the relative stability of Pt/C catalysts increases with prolonged cyclicity.

1 Influence of Composition and Structure …

13

1.3.2 The Effect of the Spatial Distribution of Pt NPs on the Degree of Degradation of Pt/C Electrocatalysts To study the effect of the spatial distribution of Pt NPs, 5 materials were obtained with different mass fractions of platinum, but with a close average crystallite size of about 2.0 nm (Table 1.4; Fig. 1.7). It was based on the idea that in these materials, with a close degree of aggregation, platinum NPs are located at different distances from each other. The larger the mass fraction, the smaller the distance between the NPs. The obtained samples are characterized by a mass fraction of platinum from 23 to 39% and an average crystallite size of about 2.1 nm (Table 1.4). It should be noted that with an increase in the mass fraction of platinum in the samples, there is a slight increase in the average crystallite size, as well as a decrease in ESA (Table 1.4). The calculated values of the distance between the NPs show that the larger the mass fraction of platinum in the sample, the smaller the distance between the particles due to their larger number (Table 1.4). For all the studied Pt/C catalysts, an increase in the currents in the hydrogen region from cycle to cycle is observed. Figure 1.8 shows the intermediate and final CV stress tests for clarity. The most pronounced decrease in currents in the hydrogen region is characteristic of catalyst S2-1 and the commercial analogue of JM20, which is characterized by low relative stability of 71% (Fig. 1.8; Table 1.5). The relative stability of the catalysts increases with an increase in the mass fraction of platinum in the samples (Table 1.5; Fig. 1.9a). The highest stability during prolonged stress testing is characterized by sample S2-5 88%, which also shows the Table 1.4 Structural and electrochemical characteristics of Pt/C samples Dav (nm)

ESA0 , m2 /g(Pt)

Sgeom , m2 /g(Pt)

Degree of aggregation

λ, nm

20 ± 0.6

2.0

86 ± 9

140

0.39

9.3

S2-1

23.5 ± 0.7

2.1

59 ± 6

135

0.56

8.7

S2-2

32 ± 1.0

2.1

73 ± 7

134

0.45

6.8

S2-3

33.6 ± 1.0

2.3

68 ± 7

122

0.44

7.5

S2-4

35 ± 1.1

2.3

59 ± 6

120

0.51

7.4

S2-5

39 ± 1.2

2.3

48 ± 5

124

0.61

6.4

Sample JM20

ω(Pt) (%)

Fig. 1.7 Schematic representation of the spatial distribution of platinum NPs on the surface of a carbon support with a close average crystallite size

14

E. Moguchikh et al.

Fig. 1.8 Initial cyclic voltammograms, 500, 2000 and 5000 cycles (1, 2, 3 and 4 respectively). The sweep rate of the potential is 20 mV/s. 0.1 M HClO4 solution saturated by Ar at room temperature. Samples: 1—JM20, 2—S2-1, 3—S2-2, 4—S2-3, 5—S2-4, 6—S2-5

Table 1.5 Characteristics of Pt/C samples calculated after stress testing

Sample

ESA5000 , m2 /g(Pt)

Relative stability, %

JM20

61 ± 6

71

S2-1

45 ± 5

76

S2-2

59 ± 6

81

S2-3

57 ± 6

84

S2-4

51 ± 5

86

S2-5

42 ± 4

88

Fig. 1.9 Dependence of the relative degree of degradation (a) and ESA (b) on the number of cycles during cycling in the potential range 0.6–1.0 V

lowest surface area throughout the entire cycle (Table 1.5; Fig. 1.9). The calculated value of the degree of particle aggregation for this sample is the highest among all studied, and this fact indicates that platinum NPs S2-5 consist of several crystallites, which is confirmed by the low initial ESA. For the remaining Pt/C catalysts, the values of the degree of aggregation are close, and, therefore, it is possible to compare the effect of the average distance between platinum particles on stability (Table 1.5). Relative stability increases in the series

1 Influence of Composition and Structure …

15

JM20 > S2-1 > S2-2 > S2-3 > S2-4. As previously indicated, the irreversible processes of changes in the catalysts during stress testing are associated with the aggregation of Pt particles and the complete separation of NPs from the surface of the carbon support. When considering these samples, we can conclude that for catalysts with a small mass fraction of platinum, the most characteristic method of degradation may be the separation of platinum NPs, and, as a consequence, a decrease in ESA. The contribution of the aggregation of platinum NPs to the degradation of samples with a low loading of platinum (about 20%) is less evident. For samples with a higher metal content, the separation of NPs is apparently less characteristic, and aggregation processes are difficult, since the particles are equidistant from each other. All these factors lead to increased stability in prolonged stress testing. Samples S2-2, S2-3 and commercial JM20 are characterized by the highest residual surface area (Fig. 1.9b). All studied materials confirmed a straightforward relationship: with an increase in the mass fraction of platinum in the catalyst, relative stability increases (the degree of degradation decreases). Additionally, the inverse proportional dependence of the stability of the catalysts on the distance between the particles is determined. The higher the mass fraction of platinum in the sample, and, correspondingly, the lower the λ value (at a close degree of aggregation and the average crystallite size of platinum), the higher the relative stability of the catalyst during prolonged stress testing in the “soft” range of potentials. It is possible that the detachment of NPs makes a greater contribution to the degradation of catalysts, since for Pt/C with a small mass fraction of platinum, the loss of a part leads to a significant decrease in surface area. Sample S2-2 is distinguished from the general dependence, which is characterized by an average distance between particles and at this low stability.

1.3.3 The Effect of the Structure of Bimetallic Nanoparticles on the Stability of Catalysts with Stress Testing To study the stability of the catalysts in the “hard” mode of stress testing, PtCu/C catalysts with the “solid solution” and “shell-core” structures were obtained. The actual composition of the obtained samples turned out to be close to the calculated one: the mass fraction of metals in PtCu/C and Pt(Cu)/C samples is 28% and 29%, with a pure platinum content of 21% and 20%, respectively (Table 1.6). The results obtained by X-ray fluorescence method confirmed that the ratio of metals in the samples is close to the calculated 1:1. Photographs of platinum-copper catalysts obtained by TEM (Fig. 1.10) show a large number of small-sized (2–4 nm) Ns. The Pt(Cu)/C sample is characterized by the presence of large NPs or aggregates of NPs, 10–15 nm in size. Taking into account the multistage procedure for producing the Pt(Cu)/C catalyst, as well as the presence of NPs of various sizes in this material, it can be assumed that part of the precursors

16

E. Moguchikh et al.

Table 1.6 Structural and electrochemical characteristics of the studied catalysts Sample

Pt(Cu)/C

The composition of the metal component Initial

After standart. CV

Pt0.8 Cu

Pt1.5 Cu

ω(Pt + Cu), %

ω(Pt), %

Dav , nm

ESA0 , m2 /g(Pt)

29

20

3.9

96 ± 10

PtCu/C

Pt1.0 Cu

Pt2.1 Cu

28

21

3.2

75 ± 8

HiSPEC

Pt

Pt

20

20

2.0

98 ± 10

Fig. 1.10 Transmission electron microscopy photographs (a, b, c, d) and diagrams (i, f) of the nanoparticles size distribution for “core-shell” Pt(Cu)/C (a, b, i) and “Solid Solution” PtCu/C (c, d, f) samples

at each subsequent synthesis stage is spent not only on the growth of particles formed at the previous stage, but also on the formation of new platinum NPs. Note that for a certain number of large particles in the Pt(Cu)/C sample, the shell-core architecture is clearly distinguishable, however, for NPs with a size of 2–3 nm, the determination of the platinum shell by TEM data is impossible. For a commercial Pt/C sample, the average NP size is 2.0 nm according to TEM. Based on the histograms of the size distribution of NPs (Fig. 1.10c, f), we can conclude that there is a wider size distribution and a larger average NP size for the Pt(Cu)/C sample in comparison with the PtCu/C material, which was obtained by the simultaneous reduction of precursors. The development and cleaning of the surface of NPs, occurring on all the studied catalysts in the process of their electrochemical standardization, leads to the growth and subsequent stabilization of the current strength (Fig. 1.11).

1 Influence of Composition and Structure …

17

Fig. 1.11 Cyclic voltammograms of the metal-carbon catalysts in the process of standardizing cycling. The sweep rate of the potential is 200 mV/s. 0.1 M HClO4 solution saturated by Ar at room temperature

The nature of the change in the type of CV is similar for both bimetallic catalysts, the establishment of stationary current values occurs rather quickly, after 10–20 cycles. The presence of shallow maximums of the anode current in the potential region of about 0.8 V in the first cycles of the potential sweep can be due to the selective dissolution of copper atoms from the Pt–Cu solid solution [29]. We should like to note that the type of standardizing CV for Pt/C and PtCu/C electrocatalysts are different. This is due to the presence of an alloying component in the bimetallic system. Initially, the stability of PtCu/C catalysts was studied in the “soft” test mode: 5000 cycles in the potential range 0.6–1.0 V (Fig. 1.12). The structure of platinumcopper catalysts also affects the change in the composition of the metal component as a result of standardization and stress testing. The NPs in the Pt(Cu)/C catalyst obtained by successive multi-stage reduction of precursors seem to acquire a uniform protective platinum shell faster. Therefore, for the Pt(Cu)/C catalyst, the selective dissolution of copper during standardization and the subsequent stress test in the potential range 0.6–1.0 V is much less pronounced than for the PtCu/C sample (Table 1.7). At the same time, both bimetallic electrocatalysts show higher stability than the commercially available Pt/C sample (Fig. 1.12a). We believe that bimetallic NPs are more firmly attached to the surface of the carbon support and their tendency to peel and agglomerate is less than that of Pt NPs. Note that in the “soft” multiple cycling mode, even less resistant to Pt/C degradation material retains about 60% of its ESA (Table 1.7; Fig. 1.12b).

Fig. 1.12 Dependence of the relative stability (a) and ESA (b) on the number of cycles during cycling in the potential range 0.6–1.0 V

18

E. Moguchikh et al.

Table 1.7 Summary table of the results of stress testing of platinum-copper and Pt/C materials Stress testing conditions

Sample

Stability, %

Composition after stress testing

After stress-test 0.6–1.0 B (5000 cycles)

Pt(Cu)/C

82

PtCu0.6

PtCu/C

70

PtCu0.4

HiSPEC

64

Pt(Cu)/C

79

PtCu0.5

PtCu/C

79

PtCu0.3

HiSPEC

15

After stress-test 0.6–1.4 B (500 cycles)

Fig. 1.13 Dependence of the relative stability (a) and ESA (b) on the number of cycles during cycling in the potential range 0.6–1.4 V, 500 cycles

As a result, the minimum decrease in the active surface of platinum according to the results of the stress test was demonstrated by the Pt(Cu)/C sample. Expanding the range of stress testing potentials to 0.6–1.4 V, as expected, led to an increase in the rate of catalyst degradation. Moreover, the differences in the behavior between Pt/C and platinum-copper samples intensified: after 500 cycles, the stability of the Pt(Cu)/C and Pt/C catalysts was 82 and 72%, while for JM it was 20% (Fig. 1.13a). After the stress test, ESA and the relative stability of platinum-copper catalysts are 4–8 times higher than for Pt/C (Table 1.7; Fig. 1.13b). It has already been noted that at high potentials, platinum catalyzes the oxidation of a carbon support in the direct contact zone, which facilitates the separation of NPs. Apparently, the presence of copper atoms at the NP/support interface decreases the catalytic activity of the metal with respect to the carbon oxidation reaction. A comparative study of platinum-carbon materials with different mass fractions of metal showed that in almost all cases there is a direct relationship between the loading of platinum in the electrocatalyst and the increase in its resistance to degradation during stress testing in the potential range 0.6–1.0 V.

1 Influence of Composition and Structure …

19

1.4 Conclusions A number of new Pt/C catalysts with a mass fraction of 18 to 39% and an average crystallite size from 1.1 to 5.7 nm were obtained by liquid-phase synthesis methods using various reducing agents. It was determined that a decrease in the average crystallite size of platinum leads to an increase in the area of the electrochemically active surface of the electrocatalyst, but at the same time, its resistance to degradation during prolonged cycling in the “soft” range of potentials decreases. It is shown that materials with the smallest diameters of platinum crystallites are characterized by reduced relative stability, but they have the largest residual areas after stress testing, which makes them promising for use in low-temperature fuel cells. A comparative study of the electrochemical behavior of platinum-copper and commercial Pt/C catalysts with a 20% loading of platinum under different voltammetric stress testing modes showed that bimetallic systems exhibit higher stability, especially under severe cycling conditions, when the potential variation range is 0.6– 1.4 V. The positive effect of the doping component on stability can be due to a more solid nanoparticles fixation on the surface of the support and a lower rate of carbon oxidation at the interface with nanoparticles compared to Pt/C. The thermodynamic stability of the metal nanoparticles themselves in platinum-copper catalysts can also be higher than in Pt/C, due to the larger average size of the NPs. An important role in the behavior of the catalysts is played not only by the qualitative composition of NPs (alloying with copper), but also by their structural features. A Pt(Cu)/C sample obtained by multistage metal deposition is characterized by a lower degree of degradation in comparison with a catalyst based on Pt-Cu NPs with a solid solution structure. The reason for the established differences may be a higher concentration of platinum in the surface layers of Pt(Cu)/C NPs in the “as obtained” state, which leads to the rapid formation of a protective platinum shell during subsequent selective dissolution of copper. Most of the obtained Pt/C and PtCu/C catalysts are characterized by comparable or superior electrochemical characteristics to the commercial analog of JM20. Acknowledgements This research was supported by the Ministry of Education and Science of the Russian Federation (project No. 13.3005.2017/4.6).

References 1. R. O’Hayre, S.-W. Cha, W. Colella, F.B. Prinz, Fuel Cell Fundamentals, 2nd edn. (Wiley Inc., New York, 2009), p. 576 2. N.V. Korovin, Int. Sci. J. 10, 8 (2004) 3. V.S. Bagotskiy, N.V. Osetrova, A.M. Skudin, Electrochemistry 39, 1027 (2003) 4. G. Crawley, Fuel Cell Today, vol. 1 (2006)

20

E. Moguchikh et al.

5. D. Thompsett, Handbook of Fuel Cells. Fundamentals, Technology and Applications (2003), vol. 3, p. 6 6. A.B. Yaroslavtsev, Y.A. Dobrovolsky, N.S. Shaglaeva, L.A. Frolova, E.V. Gerasimova, E.A. Sanginov, Russ. Chem. Rev. 81, 191 (2012) 7. S. Litster, G. McLean, Power Sources 130, 61 (2004) 8. H. Lv, D. Li, D. Strmcnik, A.P. Paulikas, N.M. Markovic, V.R. Stamenkovic, Nano Energy 29, 149 (2016) 9. O.T. Holton, J.W. Stevenson, Platin. Metals Rev. 57, 259 (2013) 10. E.H. Yu, U. Krewer, K. Scott, Energies 3, 1499 (2010) 11. J. Chen, D.S. Jiang, G.A. Cameron, B. Hards, R.J. Potter, Platin. Metals Rev. 31, 173 (1987) 12. S.V. Belenov, AYu. Pakharev, NYu. Tabachkova, E.B. Mikheykina, L.L. Vysochina, T.A. Lastovina, Int. J. Hydrogen Energy 41, 1609 (2016) 13. I.N. Leontyev, S.V. Belenov, V.E. Guterman, P. Haghi-Ashtiani, A.P. Shaganov, B. Dkhil, J. Phys. Chem. 115, 5429 (2011) 14. H. Zhu, X. Li, F. Wang, Int. J. Hydrogen Energy 36, 9151 (2011) 15. A.A. Alekseenko, V.E. Guterman, V.A. Volochaev, Springer Proc. Phys. 175, 37 (2016) 16. N.V. Smirnova, A.B. Kuriganova, D.V. Leontyeva, I.N. Leontyev, A.S. Mikheykin, Kinet. Catal. 54, 262 (2013) 17. C. Chunhua, G. Lin, L. Hui-Hui, Yu. Shu-Hong, Nano Lett. 12, 5885 (2012) 18. U.A. Paulus, A. Wokaun, G.G. Scherer, T.J. Schmidt, V. Stamenkovic, N.M. Markovic, P.N. Ross, Electrochim. Acta 47, 3787 (2002) 19. M. Oezaslan, F. Hasche, P. Strasser, J. Phys. Chem. Lett. 4, 3273 (2013) 20. M. Ji, J. Liu, J. Zhang, H. Zhu, Nano Res. 8, 271 (2015) 21. R. Awasthi, C.S. Sharma, Int. J. Electrochem. Sci. 9, 5607 (2014) 22. D.A. Cantane, F.E.R. Oliveira, S.F. Santos, F.H.B. Lima, Appl. Catal. 136, 351 (2013) 23. V.E. Guterman, A.A. Alekseenko, V.A. Volochaev, NYu. Tabachkova, Inorg. Mater. 52, 23 (2016) 24. D. Wang, H.L. Xin, R. Hovden, H. Wang, Y. Yu, D.A. Muller, F.J. DiSalvo, H.D. Abruña, Nat. Mater. 12, 81 (2013) 25. M.R. Tarasevich, V.A. Bogdanovskaya, V.N. Andreev, Catal. Ind. 6, 159 (2014) 26. A.A. Alekseenko, V.E. Guterman, V.A. Volochaev, S.V. Belenov, Inorg. Mater. 51, 1258 (2015) 27. A.A. Alekseenko, E.A. Moguchikh, O.I. Safronenko, V.E. Guterman, Int. J. Hydrogen Energy 43, 22885 (2018) 28. A.A. Alekseenko, V.E. Guterman, S.V. Belenov, V.S. Menshikov, NYu. Tabachkova, O.I. Safronenko, E.A. Moguchikh, Int. J. Hydrogen Energy 43, 3676 (2018) 29. L. Dubau, M. Lopez-Haro, J. Durst, F. Maillard, Catal. Today 262, 146 (2016)

Chapter 2

Investigation of the Effect of Different Organic Additives on Morphology and Electrocatalytic Activity of Platinum Nanomaterials Towards Oxygen Reduction Reactions Sergey V. Belenov, Weldegebriel G. Yohannes, Nikolay V. Lyanguzov, and Vadim A. Volochaev Abstract In the present study, different carbon-supported platinum nanomaterials were prepared using electrodeposition method and the influences of some organic additives, such as potassium citrate, Nafion and polyvinylidene fluoride (PVDF) on the morphology, electrochemically active surface area (ESA) and electrocatalytic activity of platinum nanomaterials (Pt/Vulcan XC-72) were evaluated. The materials were electrodeposited on a rotating disk electrode (RDE) from the electrolyte hexachloroplatinic acid (H2 PtCl6 ) and H2 SO4 in the absence and presence of the organic additives. The materials obtained were characterized using powder X-ray diffraction, scanning electron microscopy, electrochemical methods. In addition, the electrocatalytic activity of the materials towards oxygen reduction reactions was evaluated by employing linear sweep voltammetry on RDE at 1000 rpm. The presence of the organic additives increased the overpotential at the growth stage of the particles, leading to a decrease in the particle size and hence an increase in the ESA of platinum nanoparticles from 19 to 43 m2 /g(Pt) The electrocatalysts prepared using the different organic additives have the following increasing order of electrochemical activities towards the ORR in an aqueous solution of HClO4 : citrate < without the organic additives < Nafion < PVDF in the potential range of ca. 0.7–0.9 V. This electrochemical behavior can be attributed to the differences in the particle size, ESA, and the morphology of the synthesized carbon-supported platinum nanomaterials.

S. V. Belenov (B) · V. A. Volochaev Chemistry Faculty, Southern Federal University, Zorge St. 7, Rostov-on-Don, Russia 344090 e-mail: [email protected] W. G. Yohannes Department of Chemistry, College of Natural and Computational Sciences, Addis Ababa University, Addis Ababa, Ethiopia N. V. Lyanguzov Physical Faculty, Southern Federal University, Zorge St. 5, Rostov-on-Don, Russia 344090 Southern Research Center RAS, Rostov-on-Don, Russia 344006 © Springer Nature Switzerland AG 2020 I. A. Parinov et al. (eds.), Advanced Materials, Springer Proceedings in Materials 6, https://doi.org/10.1007/978-3-030-45120-2_2

21

22

S. V. Belenov et al.

2.1 Introduction Controlling the morphology, microstructure, and electrochemical properties of platinum electrodeposits with a developed surface is a key factor to enhance catalytic activity of electrode materials. This can be possibly achieved by varying electrodeposition parameters and incorporating different organic additives into the electrolyte used [1, 2]. One of the main reasons for the degradation of Pt-based electrocatalysts is the loss of the electrochemically active surface area by agglomeration of catalyst particles. Metal nanoparticles, because of their small size and high surface energy, have an inherent tendency toward the formation of agglomerates (bigger particles) to minimize their high surface energy and hence to be stabilized. Organic additives (stabilizing agents), usually surface active substances or polymers, are often used to prevent the metal particles against agglomeration, to control the size and shape by adsorbing to the particle surfaces or by separating the metal nanoparticles from each other via electrostatic or steric stabilization [3–6]. Thus, employing organic additives can effectively influence the structure of the prepared Pt nanoparticles to attain improved electrocatalytic activity, to obtain smaller size, uniform dispersion and highly dispersed Pt nanoparticles over the supporting carbon materials by limitation of the growth of metal nanoparticles. In our previous study [7], the use of the organic compound ethylene glycol in the electrodeposition of platinum over the carbon support Vulcan XC-72 resulted in a significant decrease in the Pt nanoparticles size and an enhanced catalytic activity towards oxygen reduction reaction. To remove the organic additives from the obtained catalysts, it usually necessary thermal and/or oxidative post-treatment. Harsh conditions of post-treatment may lead to agglomeration of metal nanoparticles, whereas soft conditions may result in an incomplete removal of organic additives, causing subsequent reduction in the catalytic activity of the resulting material [8]. Nevertheless, a number of publications [9–11] have shown that certain types of post-treatment of Pt/C catalysts, such as washing with different alcohol, centrifugation, heat treatment in inert atmosphere etc. can lead to a complete removal of additives and highly effective catalysts towards oxygen reduction reaction that are comparable or can have even higher activity than that of commercial electrocatalysts. Citric acid and its salts are often used as organic additives in the formation of platinum nanoparticles in the chemical reduction of platinum precursor [12–15]. Citrates are characterized by low cost, high efficiency as a stabilizing agent and the simplicity to remove residual of the additive from the prepared material. Chou et al. [12] using different aqueous solutions containing citric acid prepared enhanced catalytic activity of Pt/C and Pt–Ru/C electrocatalysts by a factor of about 1.5 and 2.8, respectively compared to those prepared without involving the additives. The authors attributed the increased electroactivities to the citric acid playing dual roles as both a stabilizing agent and particle size reducing agent in the aqueous solutions. In other studies, it was shown that some additives such as polyvinylpyrrolidone (PVP) affected not only the average size but also the shape of the platinum nanoparticles [4, 16, 17]. Tang et al. [16] reported that when the ratio of PVP/Pt varies, it allows

2 Investigation of the Effect of Different Organic Additives …

23

changing not only the average size of nanoparticles but also their shape. Ye et al. [4] studied the effect of PVP on the surface area and catalytic activity of Pt catalyst and demonstrated that PVP being adsorbed onto some of the surface of growing platinum crystals, complicates further deposition of platinum atoms on these surfaces, resulting in a significant change in the morphology of the obtained Pt deposits. This leads to an increase in the value of ESA and catalytic activity in the methanol oxidation reaction as compared to a Pt catalyst synthesized without the addition of PVP. Sharma et al. [17] synthesized platinum nanoparticles via electrodeposition method using CNT coated carbon fiber and reported an enrichment of the catalytic active Pt surfaces such as Pt (100) upon increasing PVP concentration. The proton conductive polymer Nafion is commonly used as a binding material when the porous dispersed Pt/C catalyst layer is applied onto the surface of electrodes and also in the formation of catalytic active layer in the membrane electrode assemblies (MEAs) of fuel cells. Moreover, in some cases the polymer Nafion is used as a stabilizer in the wet chemical synthesis of platinum nanoparticles. Liu et al. [18] reported that using a small amount of Nafion resulted in higher activity towards ORR as compared to platinum black and commercial Pt/C material while the activity of these catalysts in MOR was found to be very low. The analysis of literature data indicates that the introduction of organic additives into platinized electrolyte and variation of their concentration affects the microstructure and the catalytic activity of the platinum materials. However, there are limited studies on the effects of organic additives of different natures on platinum crystallite size, particle size, ESA, morphology and electrochemical behavior of the synthesized catalysts. Therefore, the objective of the present work was to prepare carbon-supported platinum nanomaterials by electrodeposition from the electrolyte hexachloroplatinic acid (H2 PtCl6 ) and H2 SO4 in the absence and presence of different organic additives such as potassium citrate, Nafion and PVDF and to investigate their influence on platinum crystallite size, particle size, morphology and electrocatalytic activity of the prepared platinum nanomaterials towards oxygen reduction reactions.

2.1.1 Research Purpose It is investigated the effect of different organic additives during electrochemical deposition of Pt on carbon supported on morphology and electrocatalytic activity of obtained platinum nanomaterials towards oxygen reduction reactions.

24

S. V. Belenov et al.

2.2 Experimental 2.2.1 Preparation of Electrode Carbon black Vulcan XC-72 (Cabot Corporation, with surface area of 270 m2 g−1 ) was used as carbon support. The carbon support for the platinum nanoparticles turns out to be critically important to provide high surface area for their dispersion, stability and electrical conductivity. Hence, a homogeneous suspension was prepared by mixing Vulcan XC-72 carbon, isopropanol and Nafion by ultrasonication and magnetic stirring. Then, the resulting suspension was pipetted onto a previously dried polished and cleaned surface of glassy carbon disc electrode to form a thin porous carbon layer (ca. 4 μm). Further details for the method of preparation of the carbon layer and the electrodes is described in [7].

2.2.2 Electrodeposition of Platinum Electrochemical experiments were carried out using a common three-electrode cell at room temperature, glassy carbon electrode is coated with a layer of Vulcan XC-72 carbon-Nafion as working electrode, a platinum wire as a counter electrode and a saturated KCl/AgCl electrode as reference electrode. However, all the potentials in this work are given relative to standard hydrogen electrode (SHE) unless otherwise noted. Electrodeposition of platinum was conducted using a rotating disc glassy carbon electrode at a speed of 1000 rpm, as described in [19]. Electrochemical measurements were performed with potentiostat-galvanostat and rotator (Pine Research Instrumentation, USA). Galvanostatic electrodeposition technique was conducted in 1 M H2 SO4 , 5 mM chloroplatinic acid (H2 PtCl6 ) aqueous solution in the presence and absence of the organic additives such as potassium citrate, Nafion and PVDF.

2.2.3 Characterization of Pt/C 2.2.3.1

Characterization of Structure

The morphology of prepared Pt/C electrodes and average size of the electrodeposited Pt particles were investigated by scanning electron microscopy (Zeiss Supra 25, 20 keV). In order to analyze morphology of prepared Pt/C electrodes and Pt particles size and distribution of carbon-supported using image analysis software called ImageJ.

2 Investigation of the Effect of Different Organic Additives …

25

The X-ray powder diffraction data were obtained using ARL X’TRA diffractometer, CuKα radiation (λ = 1.54056 Å). Measurements were carried out in the range of 2θ angles 35°–50° with scan rate—0.5°/s. A zero-background holder and polymer tissues were used in order to mount the samples. The crystallite size for all the prepared Pt/C electrodes is calculated from the width of (111) diffraction peak using Scherer equation (2.1). D=

0.95xλ β2θ cos θ

(2.1)

where D is the average crystallite size in (nm), λ is the wave length (λ = 1.54056 Å), β 2θ and θ are the full width at half maximum (FWHM) and a diffraction angle of (111) reflection in radians, respectively.

2.2.3.2

Electrochemical Measurements

After electrodeposition of Pt on carbon, the electrode was rinsed thoroughly with bi-distilled water and the obtained catalyst electrode was examined in a freshly prepared 100 mL of 0.1 M HClO4 solution. HClO4 was used as an electrolyte in all electrochemical measurements because it is considered as a non-adsorbing or a weakly adsorbing electrolyte unlike H2 SO4 and H3 PO4 . Prior to each electrochemical experiment, pure argon was purged through the electrolyte for 30 min to remove oxygen dissolved in the solution. Then, the electrode was CV scanned with 100 cycles at a scan rate of 200 mV s−1 in the potential range between −0.04 and 1.2 V versus SHE. Then, cyclic voltammograms (2 cycles) with a scan rate of 20 mV s−1 were used to determine the ESA of the Pt catalysts. The ESA was estimated by measuring the charge associated with the hydrogen adsorption/desorption at the potential region about −0.03 to 0.3 V as detailed in [20]. Briefly, determination of the electrochemically active surface area was carried out by measuring the quantity of electricity consumed according to Formula (2.2). ESA =

Q m × 210

(2.2)

where, Q is the average charge for the hydrogen adsorption and desorption (μC) which is obtained after double-layer correction; m is the mass of platinum loading (μg) and the numerical value 210 (μC cm–2 ) represents the charge required to oxidize a monolayer of hydrogen on Pt surface. Linear sweep voltammograms (LSVs) on a rotating disk electrode (RDE) were measured to evaluate the electrocatalytic activity of the obtained Pt/C materials towards oxygen reduction reactions (ORR). In this case, after the ESA measurements, a 0.1 M HClO4 electrolyte solution was saturated with oxygen at atmospheric pressure for about 1 h. Then, while continuing to purge oxygen gas, the potential of the working electrode was changed from 1.196 to 0.020 V with a sweep rate of

26

S. V. Belenov et al.

20 mV s−1 . The different disk electrode rotation rates were the following: 400, 600, 1000, 1400, 1800 and 2400 rpm. To compare the activity of the catalysts, measured currents were normalized by the mass of platinum (A/g of Pt) and/or by the ESA of the catalyst (mA/cm2 of Pt) [21].

2.3 Results and Discussion 2.3.1 Platinum Electrodeposition on Carbon Supported In order to obtain deposits of platinum with the highest value of ESA, cathodic current corresponding to platinum electrodeposition was optimized according to the results given in a previous study [7] and was found to be ca. 1.42 mA. The addition of the organic additives increases the deposition overpotential of platinum (Fig. 2.1) possibly due to their adsorption on the surface of the carbon support and on the growing platinum particles. However, there is no such a significant difference observed in the effect of the studied organic additives at the growth stage of the Pt particles above 2 s (t > 2 s) as shown in Fig. 2.1. Figure 2.2 shows diffractogram patterns for the prepared catalysts in the presence and absence of the organic additives. The diffractogram patterns exhibit reflections that are characteristic for pure platinum phase for the prepared catalysts.

Fig. 2.1 Chronopotentiograms for the electrodeposition of platinum on the surface of the carbon support Vulcan XC-72, cathodic current = 1.42 mA, rotation rate—1000 rpm. The electrolyte is an aqueous solution of 5 mM H2 PtCl6 , 1MH2 SO4 in the presence and absence of the various organic additives: 0.01 M potassium citrate, 0.01% polyvinylidene fluoride (PVDF), 0.01% Nafion

2 Investigation of the Effect of Different Organic Additives …

27

Fig. 2.2 Diffractograms for Pt/C materials. The electrolyte is an aqueous solution of 5 mM H2 PtCl6 , 1M H2 SO4 in the presence of various additives: 1—0.01% Nafion, 2—0.01% PVDF, 3—0.01 M potassium citrate, 4—without additives

All the synthesized materials exhibit clear characteristic diffraction peaks to the corresponding Pt (111) and the Pt (200) crystal planes emerged at 2θ values about 40 and 46, respectively. However, the ‘full width at half maximum reflection’ (FWHM) for the platinum materials formed under various conditions are considerably different. The most pronounced broadened reflection is noticed in the case of the organic additive potassium citrate. In fact, this is consistent with the result from Scherrer’s equation (see, Sect. 2.2). The incorporation of potassium citrate into the electrolyte resulted in the reduction of the average platinum crystallite size from 10 to 7 nm (Table 2.1). The organic additives Nafion and PVDF also reduce the average size of platinum crystallites, but to a lesser extent relative to that of potassium citrate. The decrease in the crystallites size can be attributed to the adsorption of additives on the growing platinum particles which in turn leads to the inhibition of further growth of the particles. The result found using the organic additives is consistent with the findings of Table 2.1 Characteristics of platinum electrodeposits obtained in aqueous electrolytes with different organic additives, deposition time—15 s, cathodic current—1.42 mA, Q ≈ 21 μC, weight of electrodeposited platinum ≈ 10.78 μg

Additives

D (XRD) (nm)

ESA (m2 g−1 Pt)

D (SEM) (nm)

Without additives

10 ± 0.5

19 ± 1

150

Potassium citrate

7 ± 0.5

34 ± 2

85

Nafion

8 ± 0.5

35 ± 2

115

PVDF

9 ± 0.5

43 ± 2

135

28

S. V. Belenov et al.

Fig. 2.3 SEM images at different magnifications for Pt particles obtained by electrodeposition on a carbon support in an aqueous electrolyte: a without any additives, b 0.01 M potassium citrate, c 0.01% of polyvinylidene fluoride (PVDF), d 0.01% Nafion

previous reports from [4, 5, 12, 17, 18]. The obtained platinum particles on Vulcan XC-72 (Fig. 2.3) are large aggregates with a wide range of size distribution (predominantly from 85 to 150 nm) consisting of fused crystallites with size ranging from 7 to 10 nm. Based on the results of SEM analysis, the introduction of the organic additives into the electrolyte resulted in a reduction of the average size of the deposited platinum particles (Table 2.1; Fig. 2.3). Most notably, this effect is pronounced in the presence of potassium citrate. The average particle size of the deposits decreased approximately from 150 nm to 85 nm. The average particle size of platinum for the materials determined using the SEM corresponds well with the average size of the crystallites of platinum calculated from XRD. Thus, for the electrocatalyst prepared in the electrolyte containing the organic additive, according to the SEM (Fig. 2.3a) is characterized by spherical platinum deposits with the size dispersion of ca. 50– 250 nm and with an average platinum crystallite size of about 10 nm (Table 2.1). When considering the SEM images at a higher magnification (the inset of Fig. 2.3a), it is noticeable that platinum deposits consist of small size of Pt nanoparticles with a high degree of roughness. Incorporation of the investigated organic additives not only reduces the size of the platinum particles formed during electrodeposition, but also has demonstrated a significant impact on the microstructure of the deposits.

2 Investigation of the Effect of Different Organic Additives …

29

Figure 2.3d exhibits the preferential formation of cubic shape of platinum nanoparticles [Pt (100)] in the presence of the organic additive PVDF, while the particles obtained using potassium citrate have characteristic sharp edges (Fig. 2.3b) and such changes in the microstructure of the deposits should in turn affect the electrochemically active surface area and electrocatalytic activity towards oxygen reduction reaction.

2.3.2 Activity of Platinum Nanomaterials Towards Oxygen Reduction Reactions Therefore, evaluation of the ESA and activities of the catalysts towards ORR were carried out. When the organic additives are introduced into the platinized electrolyte, the ESA value increased 1.5–2 times compared to that synthesized in the electrolyte without any additives (Table 2.1). It is noticeable that the cyclic voltammograms (Fig. 2.4) of the Pt/C materials obtained in the presence of the various organic additives have not significant differences and have the overall features of a typical cyclic voltammogram for Pt/C catalyst, showing that there is no considerable difference in the Pt/C loading among the formed materials. Moreover, the current values in the double layer region are considerably increased for the materials prepared in the presence of the organic additives

Fig. 2.4 Cyclic voltammograms for the obtained Pt/C electrodes by electrodeposition in the presence of various additives: 0.01 M potassium citrate, 0.01% PVDF, 0.01% Nafion. Electrolyte— 0.1 M HClO4 with saturated argon at atmospheric pressure, sweep rate—0.02 V/s

30

S. V. Belenov et al.

Fig. 2.5 LSV curves in the potential range from 0.6 to 0.9 V for Pt/C electrodes obtained by electrodeposition in the presence of various additives: 0.01 M potassium citrate, 0.01% PVDF, 0.01% Nafion. Electrolyte—0.1 M HClO4 oxygen saturated at atmospheric pressure, sweep rate—0.02 V/s

with the exception of the catalyst obtained using Nafion. From the investigated additives, PVDF is found to be the most effective organic additive from the point of view of achieving high ESA [43 m2 /g (Pt)] (Table 2.1). It has to be noted that direct correlation between the average platinum particle size and the ESA of platinum is not observed. The smallest size of platinum particle is obtained in the case of using potassium citrate, while the ESA of this material [34 m2 /g (Pt)] is lower than that of the electrocatalyst obtained using PVDF [43 m2 /g (Pt)]. This is possibly due to the influence of the additives not only on the size of the particles but also on the surface roughness of the particles. The obtained Pt/C catalysts by electrodeposition method are of great interest from the point of view of clarifying the relationship between the different levels of microstructural characteristics and catalytic activity of the carbon-supported platinum materials. The catalytic activity of the prepared platinum catalysts towards ORR varies significantly (Fig. 2.5). The organic additive PVDF notably increases the catalytic activity of Pt/C material as compared to a similar catalyst prepared without using the additives and this may be possibly associated with a higher ESA and with a greater proportion of active platinum crystal faces such as Pt (100), which have higher catalytic activity. Similar results were reported by Housmans et al. [22], indicating higher catalytic activity on the Pt(100) facets for methanol electrooxidation. On the other hand, despite the addition of potassium citrate increases the value of the ESA, catalytic activity of the resulting Pt/C catalyst for the ORR is somewhat reduced and the catalyst prepared in the presence of Nafion shows a slight increase in the cathodic current in the potential range of 0.7–0.8 V (Fig. 2.5), compared to the material produced without the addition of the additives. However, at potentials E < 0.7 V, the catalytic activity of Pt/C obtained in the presence of Nafion is significantly lower than the material obtained in the absence of the additives. Thus, the addition of additives into platinized electrolyte, depending on the nature of the organic additives, may positively or negatively affect the catalytic activity of the resulting

2 Investigation of the Effect of Different Organic Additives …

31

Pt/C catalyst. The highest catalyst activity is obtained in the presence of PVDF, apparently not only due to high ESA, but also attributed to the shape of the obtained carbon-supported platinum nanoparticles. PVDF has resulted greater proportion of the preferential catalytically active platinum nanocubes with Pt(100) facets, which is in a good agreement with the literature results from [2, 17, 20, 23, 24].

2.4 Conclusions The study showed that the different organic additives used adsorbed on the platinum surface in different ways and hence affected the morphology, ESA and catalytic activity of Pt/C materials to different extents. The usage of the organic additives such as potassium citrate, Nafion and PVDF increases the overpotential of the electrodeposition process, resulting in a decrease in particle size and an increase in the ESA of the Pt catalysts. In particular, the addition of potassium citrate has resulted in the reduction of the average size of the platinum particles more than 1.5 times. On the other hand, electrochemical measurements indicated that PVDF has resulted more than 2-fold enlargement in the ESA and an enhanced electrocatalytic activity of the material towards ORR. The ESA of platinum was found to be much more dependent on the surface roughness of the metal particles than on their size. The activity of Pt/C catalysts in the ORR is determined not only by the corresponding ESA but also by the predominant type of active crystal surfaces constituting the Pt nanoparticles. Acknowledgements This work was performed in the framework of the state task of the Russian Federation No 13.3005.2017/4.6.

References 1. Y.D. Gamburg, Z. Giovanni, Theory and Practice of Metal Electrodeposition (Springer, Science & Business Media, 2011) 2. R.M. Antoniassi, J.C.M. Silva, T. Lopes, N.A. Oliveira, E.V. Spinacé, Int. J. Hydrogen Energy 42(48), 28786 (2017) 3. Y.W. Jun, J.H. Lee, J.S. Choi, J. Cheon, J. Phys. Chem. B. 109, 14795 (2005) 4. F. Ye, W. Hu, T. Zhang, J. Yang, Y. Ding. Electrochim. Acta 383, 386 (2012) 5. F. Ye, L. Chen, J. Li, J. Li, X. Wang. Electrochem. Commun. 10, 476 (2008) 6. A. Quintanilla, V.C.L. Butselaar-Orthlieb, C. Kwakernaak, W.G. Sloof, M.T. Kreutzer, F. Kapteijn, J. Catal. 271(1), 104 (2010) 7. W. Yohannes, S.V. Belenov, V.E. Guterman, L.M. Skibina, V.A. Volotchaev, N.V. Lyanguzov, J. Appl. Electrochem. 45, 623 (2015) 8. P. Serp, J.L. Figueiredo, Carbon Materials for Catalysis (Wiley, Hoboken, 2009) 9. J.M. Sieben, M.M. Duarte, C.E. Mayer, J. Alloys Compd. 509, 4002 (2011) 10. P.L. Kuo, W.F. Chen, H.Y. Huang, I.C. Chang, S.A. Dai, J. Phys. Chem. B. 110, 3071 (2006) 11. C.L. Hui, X.G. Li, I.M. Hsing, Electrochim. Acta 51, 711 (2005) 12. H.Y. Chou, C.K. Hsieh, M.C. Tsai, Y.H. Wei, T.K. Yeh, C.H. Tsai, Thin Solid Films 584, 98 (2015)

32

S. V. Belenov et al.

13. G.A. Attard, J.Y. Ye, P. Jenkins, F.J. Vidal-Iglesias, E. Herrero, S.G. Sun, J. Electroanal. Chem. 688, 249 (2013) 14. I. Ojea-Jiménez, V. Puntes, J. Am. Chem. Soc. 131(37), 13320 (2009) 15. L. Pei, K. Mori, M. Adachi, Langmuir 20(18), 7837 (2004) 16. Z. Tang, D. Geng, G. Lu, J. Colloid Interface Sci. 287, 159 (2005) 17. R. Sharma, K.K. Kar, Electrochim. Acta 156, 199 (2015) 18. Z. Liu, Z.Q. Tian, S.P. Jiang, Electrochim. Acta 52, 1213 (2006) 19. A.J. Bard, L.R. Faulkner, J. Leddy, C.G. Zoski, Electrochemical Methods: Fundamentals and Applications (Wiley, New York, 1980) 20. V.E. Guterman, A.Y. Pakharev, N.Y. Tabachkova, Appl. Catal. A: Gen. 453, 113 (2013) 21. V.E. Guterman, S.V. Belenov, A.A. Alekseenko, N.Y. Tabachkova, V.A. Volochaev, Russ. J. Electrochem. 53(5), 531 (2017) 22. T.H. Housmans, A.H. Wonders, M.T. Koper, J. Phys. Chem. B. 110(20), 10021 (2006) 23. C. Wang, H. Daimon, T. Onodera, T. Koda, S. Sun, Angew. Chem. Int. Ed. 47(19), 3588 (2008) 24. I.N. Leontyev, S.V. Belenov, V.E. Guterman, P. Haghi-Ashtiani, A.P. Shaganov, B. Dkhil, J. Phys. Chem. C. 115(13), 5429 (2011)

Chapter 3

X-ray Spectroscopy Study of the Atomic and Electronic Structure of Polyacrylonitrile-Based Nanocomposites at Different Stages of Formation M. A. Kremennaya, V. A. Shmatko, T. A. Mikhailova, E. V. Pronina, K. D. Kosolapova, and G. E. Yalovega Abstract Study the atomic and electronic structure of polyacrylonitrile (PAN) during IR-annealing and the formation of Co/PAN nanocomposite based on a combination of computer simulation methods and X-ray absorption spectroscopy was carried out. Using the Density Functional Theory method, structural models of pure PAN and Co/PAN nanocomposite were obtained and electronic density of states was calculated. X-ray absorption spectra for the obtained structural models were calculated and showed good agreement with the experiment. The densities of states demonstrated that polymer form changes from non-conducting to conducting during annealing process.

3.1 Introduction Conductive polymers with poly conjugated systems are great interest due to their unique physicochemical properties, which allow their use in various fields of chemistry, physics and materials science [1]. Among these materials, polyacrylonitrile (PAN) occupies a special place. PAN is able to change the electronic structure during heat treatment, in particular during IR pyrolysis. PAN pyrolysis makes it possible to obtain a structures with various electrical properties controlled conductivity, as well as low cost and simple material manufacturing technology [2]. Adding of metal salts (Ni, Co, Cu, Ag, Fe) into the PAN also allows one to change the electrical conductivity of nanocomposites films [3]. Moreover, PAN exhibits excellent catalytic properties [4], and can be used as an adsorbent [5]. It can be used in tribology or microelectronics as thin films deposited on the surface [4]. The study of the atomic and electronic structures of such materials and their dependence on the synthesis M. A. Kremennaya (B) · V. A. Shmatko · T. A. Mikhailova · E. V. Pronina · K. D. Kosolapova · G. E. Yalovega Faculty of Physics, Southern Federal University, Zorge str. 5, Rostov-on-Don, Russia 344090 e-mail: [email protected] © Springer Nature Switzerland AG 2020 I. A. Parinov et al. (eds.), Advanced Materials, Springer Proceedings in Materials 6, https://doi.org/10.1007/978-3-030-45120-2_3

33

34

M. A. Kremennaya et al.

parameters is an important task, the solution of which opens up possibilities for creating nanocomposites with desired properties. A study of the electronic structure of various materials is usually carried out using a combination of photoelectron spectroscopy and X-ray absorption spectroscopy. Photoelectron spectroscopy allows studying occupied electronic states, as well as the valence band. X-ray absorption spectroscopy allows the study of free electronic states. In addition, the use of the density functional theory for studying the atomic and electronic structure of various carbon materials is widespread [6–10]. As well as an approach that includes a combination of density functional theory to obtain model structures and calculation of X-ray absorption spectra to verify these models [11–13]. X-ray absorption spectra are sensitive to changes in the charge, to small changes in bond lengths (up to 0.01 Å) and angles, which allows an accurate simulation of the atomic and electronic structure of the studied objects. In this chapter, we present the results of study the atomic and electronic structure of polyacrylonitrile during IR-annealing and the formation of Co/PAN nanocomposite based on a combination of computer simulation methods and X-ray absorption spectroscopy.

3.2 Experiment and Methods Density functional theory (DFT) calculations were performed in ADF code [14]. The atomic and electronic structures were simulated for the initial structure of polyacrylonitrile, during IR pyrolysis and formation of Co/PAN nanocomposite. Geometry optimization was carried out using the BPE [15] exchange-correlation potential with TZP basic set. Theoretical X-ray absorption spectra were calculated with the FDMNES code [16]. Near edge X-ray absorption fine structure (NEXAFS) spectra for C K-edge and Co L2,3 -edge were calculated by the finite difference method at the full potential. The radius of the calculated cluster was 5.5 Å. The obtained spectra were convoluted by Lorentzian to remove occupied states. A detailed description of the Co/PAN nanocomposite preparation is given in [17]. Experimental NEXAFS spectra for Co L2,3 -edge were recorded at the Elettra Sincrotrone Trieste (Italy), Materials Science Beamline. Spectra were obtained in the partial KVV Auger electron yield detection mode.

3.3 Results and Discussion A structure reorganization of PAN is observed at various temperatures during IRannealing (Fig. 3.1) [18–21]. The initial structure is a polymer consisting of chains with conjugated triple bonds C≡N (Stage 1). Stage 2: cyclization (100–200 °C), the interaction of nitrile groups with the formation of a regular linear network.

3 X-ray Spectroscopy Study of the Atomic and Electronic …

35

Fig. 3.1 Structural models of PAN: 1—initial structure, 2—stage of cyclization at 200–300 °C, 3—stage of carbonization at 250–450 °C, 4—stage of intermolecular carbonization at 450–1300 °C

Stage 3: carbonization (250–450 °C), polymerization by nitrile groups and dehydrogenation of the hydrocarbon chain occur. Stage 4: intermolecular carbonization (400 °C and higher), crosslinking of linear polymer chains with the formation of a spatially cross-linked polymer. Further heating (up to 1300 °C) leads to the formation of a graphite-like structure with a small content of nitrogen atoms. Theoretical X-ray absorption spectra were calculated for four cases of the structure evolution before and after PAN IR-annealing. The theoretical NEXAFS spectrum for the initial structure of PAN (1) is shown in Fig. 3.2. The shape and energy position of the spectral features coincides with the experimental spectra given in [22–24]. Theoretical spectrum 1 has an intense peak A at an energy of 286.8 eV, which refers to C1s (C≡N) → π*C≡N transitions, peak B at 288.5 eV refers to C1s (C-H) → Fig. 3.2 Comparison of experimental and theoretical PAN C K-edge NEXAFS spectra; experimental spectra taken from [22]

36

M. A. Kremennaya et al.

Fig. 3.3 Comparison of experimental C K-edge NEXAFS spectra for pure PAN film annealed at 260–440 °C [25] and theoretical NEXAFS spectra of PAN during IR-annealing (Models 2–4)

2π*C–C transitions and peak C at 293.3 eV corresponding to C1s (C-H) → σ*C=C transitions [23]. The next block of comparisons is carried out with the experimental spectrum for pure PAN film annealed at 260–440 °C, obtained in [25] (Fig. 3.3). Peak A at 285.1 eV for presented spectrum can be characterized as C1s(C–H) → π*C=C transitions, peak B at 287.8 eV as C1s(C–H) → σ*C-H transitions, peak C as 288.5 eV is C1s(C–H) → 2π*C–C transitions, peak D as 292.3 to C1s(C–H) → σ*C–H transitions [23]. The theoretical spectrum 2 corresponds to the structure of PAN at the stage of cyclization. There are three intense peaks at energies of 285.1, 290.6 and 296.8 eV, as well as a shoulder at 287.8 eV. The energy positions of peak A and shoulder B coincide with the experimental spectrum. In spectrum 3 for PAN at the carbonization stage, the energy position coincides for the spectral feature of A with the experimental spectrum. However, the peak D is doubled and shifted along the energy to the right, and double peaks B and C are also not observed. In the theoretical spectrum 4 for PAN at intermolecular carbonization stage, the energy position of the singularity A coincides with the experimental position and its intensity is higher, the peaks B and C are present. The spectral feature D is narrower than the experiment. It can be seen from the figure, the theoretical spectrum for the structure of a spatially cross-linked polymer (4) reproduces the main spectral features of the experimental spectrum. However, the intensities of the spectral features for all theoretical spectra are overestimated because in the calculation models, only one polymer layer is taken into account and there is no consideration for interaction with oxygen.

3 X-ray Spectroscopy Study of the Atomic and Electronic …

37

Fig. 3.4 Density of states in PAN at various stages of IR-annealing

The densities of states were calculated for the initial PAN structure and PAN during IR-annealing (Fig. 3.4). As can be seen, the band gap decreases and the state of the substance changes from non-conducting to conducting in the IR-annealing process [26]. The asterisk indicates the highest occupied states and point indicates the lowest unoccupied states. In [25] was found that cobalt binds to nitrogen atoms in the pyridine rings and is in the oxidic form. Based on these data, the Co/PAN nanocomposites structure 5 was simulated (Fig. 3.5b) and X-ray absorption spectra for Co L2,3 -edge were calculated. Figure 3.5a shows a comparison with the experimental spectrum. The theoretical spectrum shows good agreement with the experimental one. Diffuse spectral features of the experimental spectrum are associated with energy resolution. Peak A in the presented spectra corresponds to L3 , and peak B to L2 . Splitting at L3 peak indicates that cobalt is in a 2+ state [27]. Thus, the applied research technique allows us to consider the electronic structure not only from the side of the polymer matrix, but also from the side of the inject metal into the structure.

3.4 Conclusion The atomic and electronic structures for the initial structure of polyacrylonitrile, during IR pyrolysis and formation of Co/PAN nanocomposite were simulated using the density functional theory. Theoretical C K and Co L2,3 -edges absorption spectra were calculated for all obtained models. Theoretical NEXAFS spectra showed good agreement with experimental spectra. However, the intensities of spectral features for theoretical spectra are overestimated, what can be reduced by adding additional layers of polymer and oxygen molecules. The densities of states calculations for the initial PAN and PAN during IR-annealing structures showed that polymer form changes

38

M. A. Kremennaya et al.

Fig. 3.5 Comparison of experimental and theoretical Co L2,3 -edge spectra for Co/PAN (a) and structural model 5 of Co/PAN nanocomposites (b)

from non-conducting to conducting during annealing process. The analysis showed that cobalt is in 2+ oxidation state. Thus, the applied technique, which includes computer simulation and X-ray absorption spectroscopy, allowed us to analyze the electronic structure both from the side of the polymer matrix and from the side of the metal added into the structure. Acknowledgements This work was supported by the Southern Federal University (Project no. VN_GR_07_2017-30).

References 1. D.G. Muratova, E.V. Yakushko, L.V. Kozhitov, A.V. Popkova, M.A. Pushkarev. Mod. Electron. Mater. 2, 70 (2016) 2. T.A. Bednaya, S.P. Konovalenko, Russ. Microelectron. 47, 112 (2018) 3. E.A. Stefanescu, C. Daranga, C. Stefanescu, Materials 2, 2095 (2009) 4. G. Tourillon, D. Guay, A. Fontaine. Faraday Discuss. Chem. Soc. 89, 275 (1990) 5. Z. Jiang, Y. Liu, G. Zeng, W. Xu, B. Zheng, X. Tana, S. Wang. RSC Adv. 5, 25389 (2015) 6. C. Ehlert, W.E.S. Unger, P. Saalfrank, C. Phys. Chem. Chem. Phys. 16, 14083 (2014) 7. S.G. Minasian, J.M. Keith, E.R. Batista, K.S. Boland, S.A. Kozimor, R.L. Martin, D.K. Shuh, T. Tyliszczak, L.J. Vernon. J. Am. Chem. Soc. 135, 14731 (2013)

3 X-ray Spectroscopy Study of the Atomic and Electronic … 8. 9. 10. 11. 12. 13. 14. 15. 16. 17. 18. 19. 20. 21. 22. 23. 24. 25. 26. 27.

39

D.R. Nascimento, A.E. DePrince, J. Phys. Chem. Lett. 8, 2951 (2017) P.A. Denis, F. Iribarne, J. Mol. Struc-Theochem. 907, 93 (2009) G. Bertoni, L. Calmels, Micron 37, 486 (2006) J.P. Rueff, Y. Joly, F. Bartolome, M. Krisch, J. L. Hodeau, L. Marques, M. Mezouar, A. Kaprolat, M. Lorenzen, F. Sette. J. Phys.: Condens. Matter. 14, 11635 (2002) M. Brzhezinskaya, V. Shmatko, G. Yalovega, A. Krestinin, I. Bushkin, E. Bogoslavskaya, J. Electr. Spectr. Rel. Phen. 196, 99 (2014) A. Nikitin, L.-Å. Näslund, Z. Zhang, A. Nilsson, Surf. Sci. 602, 2575 (2008) G. te Velde, E.J. Baerends. Phys. Rev. B. 44, 7888 (1991) J.P. Perdew, K. Burke, M. Ernzerhof. Phys. Rev. Lett. 77, 3865 (1996) O. Bunau, Y. Joly. J. Phys.: Condens. Matter. 21, 345501 (2009) G. Yalovega, T. Semenistaya. Solid State Phenom. 257, 175 (2017) R. Janus, P. Natka´nski, A. Wach et al. J. Therm. Anal. Calorim. 110, 119 (2012) C.R. Wu, W.R. Salaneck. Synth. Met. 16, 147 (1986) S.Y. Jin, M.H. Kima, Y.G. Jeong, Y.I. Yoon, W.H. Park. Mater. Des. 124, 69 (2017) Q. Luo, X. Yang, X. Zhao, D. Wang, R. Yin, X. Li. J. An. Appl. Catal. B-Environ. 204, 304 (2017) J. Wang, H.D.H. Stöver, A.P. Hitchcock, T. Tyliszczak. J. Synchrotron Rad. 14, 181 (2007) O. Dhez, H. Ade, S.G. Urquhart, J. Electron Spectrosc. Relat. Phenom. 128, 85 (2003) H. Ade, X. Zhang, S. Cameron, C. Costello, J. Kirz, S. Williams. Science. 258, 972 (1992) G. Yalovega, T. Semenistaya, V. Shmatko, M. Kremennaya, N. Tsud, Radiat. Phys. Chem. (2019). https://doi.org/10.1016/j.radphyschem.2019.04.006 S.K. Nataraj, K.S. Yang, T.M. Aminabhavi. Prog. Polym. Sci. 37, 487 (2012) F.M.F. de Groot, M. Abbate, J. van Elp, G.A. Sawatzky, Y.J. Ma, C.T. Chen, F. Sette, J. Phys.: Condens. Matter 5, 2277 (1993)

Chapter 4

Morphology and Structure of Carbon Nanoparticles Generated from Graphite Nitrate Co-intercalation Compound. Effect of Sonication Regime E. V. Raksha, A. A. Davydova, Yu. V. Berestneva, M. V. Savoskin, V. A. Glazunova, A. N. Vdovichenko, O. N. Oskolkova, P. V. Sukhov, V. V. Gnatovskaya, I. A. Verbenko, and Yu. I. Yurasov Abstract Few-layer graphenes and nanoscrolls have been prepared by exfoliation of the triple graphite nitrate co-intercalation compound (GNCC) as well as pre-thermally expanded GNCC in liquid media. Graphite nitrate sequentially cointercalated with ethyl formate and acetic acid and thermally expanded graphite (TEG) obtained from it were used as precursors of carbon nanoparticles. Ethanol, acetonitrile and a mixture of DMFA:H2 O (9:1 by volume) were used as solvents for liquid phase exfoliation of GNCC and TEG assisted with sonication. The microstructure and morphology of obtained few-layer graphenes and nanoscrolls were investigated by transmission electron microscopy (TEM). Planar sizes of the as-prepared few-layer graphenes reached several tens of µm and their thickness was within 1– 10 atomic layers according to TEM data. Sonication regime effect on the resulting carbon nanoparticles morphology was studied. It was shown that sonication with a power of 70 W (42 kHz) provided obtaining of the few-layer graphene suspensions containing also single-layered graphene particles. The sonication with 315–630 W E. V. Raksha (B) · A. A. Davydova · M. V. Savoskin · A. N. Vdovichenko · O. N. Oskolkova · P. V. Sukhov · V. V. Gnatovskaya Supramolecular Chemistry Department, L.M. Litvinenko Institute of Physical-Organic and Coal Chemistry, 70, R. Luxemburg Street, Donetsk 83114, Ukraine e-mail: [email protected] Yu. V. Berestneva Biotechnology Laboratory, Federal State Budget Scientific Institution “Federal Scientific Centre of Agroecology, Complex Melioration and Protective Afforestation of the Russian Academy of Sciences”, 97, Universitetsky Avenue, Volgograd, Russia 400062 V. A. Glazunova Department of High-Pressure Physics and Advanced Technologies, Donetsk Institute for Physics and Engineering named after A.A. Galkin, 72, R. Luxemburg Street, Donetsk 83114, Ukraine I. A. Verbenko · Yu. I. Yurasov Research Institute of Physics, Southern Federal University, 194, Stachki Avenue, Rostov-on-Don 344090, Russia Yu. I. Yurasov Southern Scientific Centre RAS, 41, Chehova Sreet, Rostov-on-Don 344006, Russia © Springer Nature Switzerland AG 2020 I. A. Parinov et al. (eds.), Advanced Materials, Springer Proceedings in Materials 6, https://doi.org/10.1007/978-3-030-45120-2_4

41

42

E. V. Raksha et al.

(22 kHz) leads to the formation of carbon nanoscrolls. It was found that ethanol is more preferable medium for carbon nanoparticles generation as compared to acetonitrile. Liquid phase exfoliation of GNCC and pre-thermally expanded GNCC allows obtaining dispersions of carbon nanoparticles with various morphology—single- and few-layer graphenes, nanoscrolls as well as small graphene particles.

4.1 Introduction There are three promising routes for graphene production from natural graphite: reduction of graphene oxide, electrochemical exfoliation of graphite, and liquidphase exfoliation of graphite, graphite co-intercalation compounds or thermally expanded graphite. Both anions and cations, including their solvated forms, can intercalate between graphene sheets via oxidation or reduction reactions, respectively, forming graphite intercalation compounds. A variety of applications for graphite intercalation compounds have been proposed or realized, including use as thermally expansion and liquid phase exfoliation precursors [1–7]. The synthesis, composition and properties of a broad range of binary and triple graphite nitrate co-intercalation compounds containing different organic co-intercalant species have been studied [4, 5]. They have pre-organized structure for graphene particles generation due to enlarged distance between the nearest graphene layers filled with intercalant species. Such structural reorganization of graphite matrix is responsible for graphite nitrate intercalation compounds application as precursors of carbon nanoparticles generation in mild conditions. This chapter presents the results on the production of nanoscrolls and fewlayer graphenes by sonication of graphite nitrate co-intercalated with ethyl formate and acetic acid (GNCC) prepared by natural graphite chemical treatment and prethermally expanded GNCC in different solvents. Sonication regime effect on the resulting carbon nanoparticles morphology was also studied.

4.2 Experimental At the first step graphite nitrate co-intercalation compound was prepared as a starting material for the thermally expanded graphite production and generation of carbon nanoparticles dispersions. GNCC was synthesized in a thermostatic reactor at 20 °C. Nitric acid with a density of 1.502 g cm–3 (98%) was added to the sample of natural flake graphite GT-1 (Zavalie Graphite Works, Kirovograd region, Ukraine). The mixture was stirred for 10 min. Then co-intercalants (ethyl formate and acetic acid) were sequentially added in equal amounts to the reaction mixture and the system was stirred again for 10 min. The consumptions of nitric acid and each co-intercalant were 0.6 and 6 cm3 per 1 g of graphite, respectively. Resulted GNCC was separated by filtration and dried at 20 °C until the sample mass became constant. Thermally

4 Morphology and Structure of Carbon Nanoparticles …

43

expanded graphite was obtained from GNCC by the thermal shock mode of heating (900 °C). Dispersions of carbon nanoparticles were obtained by liquid phase exfoliation of the GNCC as well as TEG at different sonication regimes (42 kHz and 70 W; 22 kHz and 315–630 W). Ethanol, acetonitrile and mixture of DMFA and H2 O (9:1 by volume) were used as media for liquid phase exfoliation of GNCC and TEG. Carbon nanoparticles dispersions were prepared by adding of GNCC (0.5 g dm−3 ) or (0.3 g dm−3 ) to examined solvents and sonication of mixtures for 1 h. Dispersions were sprayed on TEM grid and investigated using JEOL JEM-200 transmission electronic microscope. Absorption spectra were recorded on a UV-VIS spectrometer (Helios Gamma, Thermo Electron Corporation, USA). The dispersions of carbon nanoparticles in ethanol and acetonitrile were used as the samples, and the pure ethanol and acetonitrile were used as a reference.

4.3 Results and Discussion The structure of acceptor-type graphite intercalation compounds is very specific. Their quasi-two-dimensional layers of intercalants are quite labile, being not connected to a rigid graphite matrix by covalent bonds. These negatively charged layers alternate with positively charged graphene layers. Organic co-intercalants additionally stabilize the graphite nitrate through the formation of hydrogen bonds network. Interplanar space filled with co-intercalants species increases up to 7.8 Å for such compounds [1]. This structural reorganization of graphite matrix may be considered as a pre-organization process for few-layer and single-layer graphene formation. Thus, GNCCs are prospective compounds for the liquid phase exfoliation and graphene-like particles generation. However, GNCCs possess ability of thermal expansion [1, 5]. Thermally expanded graphite, obtained from GNCCs can also be used as a precursor for liquid phase exfoliation. Graphite nitrate sequentially co-intercalated with ethyl formate and acetic acid was used as source of carbon nanoparticles. Spontaneous bloating of particles for these compounds has been observed in its drying process at 20 °C. Thermally expanded graphite, obtained from this GNCC was also investigated as a precursor for carbon nanoparticles with different morphology. Dispersions of carbon nanoparticles were obtained by GNCC exfoliation in ethanol and acetonitrile induced by ultrasound (22 kHz, 315 and 470 W). The duration of the sonication was 1 h. Then, the samples were centrifuged (7 min, 3000 rpm). The dispersions obtained were investigated by UV spectroscopy and transmission electron microscopy (TEM). It should be noted that treatment of intercalated graphite compounds with alcohols is used as a method of graphite matrix exfoliation without additional temperature influence [2, 8]. Since our investigations were carried out mainly on the co-intercalated compounds of the IV and II intercalation stages, it was difficult to expect a complete graphite lattice exfoliation into monolayer graphene particles which formation was demonstrated earlier [2].

44

E. V. Raksha et al. 500 nm

1,5 μm

1,5 μm

a

b

c

1 μm

1 μm

d

e

500 nm

f

Fig. 4.1 TEM images of carbon nanoparticles obtained in ethyl alcohol (a–d) and acetonitrile (e, f) by sonication of the graphite nitrate co-intercalated with ethyl formate and acetic acid

An analysis of the dispersions obtained in ethyl alcohol and acetonitrile by the TEM method revealed that carbon nanoparticles of various morphologies can be generated by this technique. Most commonly, a mixture of particles is formed, which includes graphene-like particles of various sizes (both single-layer and few-layer), nanoscrolls, and small amorphous nanocarbon particles. Figure 4.1 shows typical TEM micrographs of carbon nanoparticles obtained by GNCC exfoliation in ethanol induced by ultrasound (22 kHz, 470 W). The planar sizes of obtained individual few-layer graphene particles reach several micrometers (Fig. 4.1a). A large number of small particles with planar sizes up to 200 nm is also formed in the system (Fig. 4.1b). Nanoscrolls with a length of 50–400 nm were present in the dispersions (Fig. 4.1c, d) in significant amount. The solvent effect on the graphite matrix exfoliation of the synthesized GNCC was also investigated. Acetonitrile was also used as a liquid medium for the GNCC exfoliation. TEM images of carbon nanoparticles obtained by GNCC sonication in this solvent are shown in Fig. 4.1e, f. By passing from ethyl alcohol to acetonitrile, an increase in the degree of structural deformation is observed for particles formed as a result of GNCC sonication. At the same time, a small number of few-layer graphene particles were present in the samples. However, most commonly a large number of amorphous small particles with sizes up to 1 nm was formed as a result of GNCC sonication in acetonitrile. Apparently, such intercalants as ethyl formate and acetic acid, which, when interacting with nitric acid, can generate free radical particles, as well as acetonitrile involved in chain transfer reactions, contribute to a significant increase in the number of defects and fragmentation of graphene planes formed upon GNCC exfoliation. Aggregates of small clusters have different morphologies and are characterized by the absence of a crystalline structure.

4 Morphology and Structure of Carbon Nanoparticles …

45

275 nm

A

280 nm

λ, nm Fig. 4.2 Representative UV absorption spectra of the dispersions obtained by exfoliation of GNCC in ethanol and acetonitrile (sonication: 1 h, 22 kHz, 470 W)

UV absorption spectra obtained for carbon nanoparticles dispersions show an absorption peaks at 275 nm for both ethanol and acetonitrile media (Fig. 4.2). Additional peaks were observed at near 280 nm for both ethanol and acetonitrile dispersions. Such character of absorption spectra can be due to the presence of nanoparticles with different types of morphology (graphenes and nanoscrolls as well as small clusters with different morphologies and a large number of structural defects) in the studied dispersions. Further investigations to detail the features of considered dispersions absorption spectra are required. Thus, carbon nanoparticles of various sizes and diverse morphologies can be obtained by exfoliation of triple GNCC in acetonitrile and ethanol. Acetonitrile contributes to the formation of a larger number of structural defects in graphene planes and to the generation of amorphous carbon particles with sizes less than 1 nm. Carbon nanoparticles (few-layer graphenes and nanoscrolls) were also obtained by sonication of thermally expanded graphite in the mixture of DMFA:H2 O = 9:1 by volume. Graphite nitrate sequentially co-intercalated with ethyl formate and acetic acid was used as a source of thermally expanded graphite. It was demonstrated that sonication with a power of 70 W and higher frequency (42 kHz) produced suspensions of few-layer graphene particles containing also single-layer graphenes. The sonication with 315–630 W (22 kHz) leads to the formation of carbon nanoscrolls (Fig. 4.3) with a diameter of about 30–80 nm and a length from 140 to 200 nm along with few-layer graphenes. Thus, it was shown that variation of the sonication conditions leads to obtaining of carbon nanoparticles with different morphology. Thus, in accordance with the TEM data, the formation of few-layer graphene particles and nanoscrolls as a result of the liquid phase exfoliation of TEG based on the graphite nitrate co-intercalation compound is established. It is shown that a change in the ultrasonic treatment regime leads to the production of carbon nanoparticles with different morphologies.

46 a)

1 µm

E. V. Raksha et al. c)

330 nm

b)

d)

330 nm

330 nm

Fig. 4.3 Representative TEM images and electron diffraction pattern of carbon nanoparticles obtained by sonication of thermally expanded graphite in the mixture of DMFA:H2 O = 9:1 by volume. Sonication power: 315 W (a, b), 470 W (c), 630 W (d); 22 kHz

4.4 Conclusion The presence of carbon nanoparticles (few-layer graphenes and nanoscrolls) in the exfoliation products of triple graphite nitrate co-intercalation compound in different media has been established by the transmission electron microscopy method. It was shown that varying the solvent nature makes it possible to obtain different types of carbon nanoparticles. Graphene-like particles with planar sizes up to several micrometers were formed from GNCC in ethyl alcohol. Acetonitrile contributes to a significant increase in the number of defects and fragmentation of graphene planes formed by GNCC exfoliation. TEG exfoliation in DMFA:H2 O mixture leads to the few-layer graphenes and nanoscrolls generation. The presented results revealed graphite nitrate co-intercalation compounds as well as thermally expanded graphite to be a promising source of carbon nanoparticles. Exfoliation of GNCC or TEG in liquid media by sonication can be simple and effective route for obtaining carbon nanoparticles under mild conditions at large scales.

References 1. M.V. Savoskin, A.P. Yaroshenko, G.E. Whyman, R.D. Mysyk, J. Phys. Chem. Sol. 67, 1127–1131 (2006) 2. M.V. Savoskin, V.N. Mochalin, A.P. Yaroshenko, N.I. Lazareva, T.E. Konstantinova, I.V. Barsukov, I.G. Prokofiev, Carbon 45, 2797–2800 (2007)

4 Morphology and Structure of Carbon Nanoparticles …

47

3. M.V. Savoskin, A.N. Vdovichenko, E.V. Raksha, Yu.V. Berestneva, V.Yu. Vishnevskij, O.M. Padun, I.A. Verbenko, Yu.I. Yurasov, in Proceedings of the 2016 International Conference on “Physics, Mechanics of New Materials and Their Applications”, ed. by I.A. Parinov, S.-H. Chang, M.A. Jani(Nova Science Publishers, New York), pp. 115–120 (2017) 4. M.V. Savoskin, A.N. Vdovichenko, E.V. Raksha, Yu.V. Berestneva, V.Yu. Vishnevskij, A.P. Prudchenko, V.A. Glazunova, K.P. Andryushin, Yu.I. Yurasov, in Proceedings of the 2017 International Conference on “Physics, Mechanics of New Materials and Their Applications”, ed. by I.A. Parinov, S.-H. Chang, V.K. Gupta (Nova Science Publishers, New York), pp. 7–13 (2018) 5. A.A. Voitash, V.Yu. Vishnevsky, Yu.V. Berestneva, E.V. Raksha, A.V. Muratov, A.B. Eresko, V.A. Glazunova, V.V. Burhovetskiy, G.K. Volkova, M.V. Savoskin, in Applied Aspects of NanoPhysics and Nano-Engineering, ed. by K. Levine, A.G. Syrkov (Nova Science Publishers, New York), pp. 25–28 (2019) 6. G. Bepete, E. Anglaret, L. Ortolani, V. Morandi, K. Huang, A. Penicaud, K. Drummond, Nat. Chem. 9, 347–352 (2017) 7. W. Sirisaksoontorn, A.A. Adenuga, V.T. Remcho, M.M. Lerner, J. Am. Chem. Soc. 133, 12436– 12438 (2011) 8. E.D. Grayfer, A.S. Nazarov, V.G. Makotchenko, S.J. Kim, V.E. Fedorov, J. Mater. Chem. 21, 3410–3414 (2011)

Chapter 5

Formation of Surface Micro and Nanostructures When Exposed to Laser UV and VUV Radiation of Nanosecond Duration Vladislav Khomich, Vladimir Yamshchikov, and Sergey Mikolutskiy Abstract Micro- and nanostructures improved different surface properties, which is used in various fields of science and technology. It is of a great interest to develop the physical foundations of new effective methods for creation of such structures. The paper proposes a method of direct laser micro- and nanostructuring based on nanosecond lasers with radiation of UV and VUV range. The method allows surface laser treatment of materials with different physical properties: metallic alloys, ceramics, diamond-like films, semiconductors. Formation of surface micro and nanostructures on the surfaces of diamond-like film, germanium, aluminum oxide and zirconium bronze is demonstrated. A theoretical model of nanostructure formation on solid surface melted by nanosecond laser pulse is considered. Moreover, a simple model for formation of conical structures at laser ablation without melting is described.

5.1 Introduction The formation of micro- and nanostructures on the material surface can improve its optical, tribological, adhesive, hydrophilic and other technical properties [1–5]. Also it enhance biocompatibility between living tissues and implants employed in dentistry and orthopedics. Due to that fact surface micro- and nanostructuring found its application in microelectronics, nanophotonics, selective nanocatalysis, spectroscopy, power optics, machine manufacturing, medicine, and so on. Therefore, it is of a great interest to develop new effective methods for obtaining surface structures with characteristic sizes less than 100 nm. It is generally known that there are a lot of methods and techniques for producing nanomaterials and surface nanostructures. They are laser irradiation with use of projection-masks; interference of two or more laser beams; combination of laser beam with the tip of atomic force microscope; direct laser nanostructuring by picoand femtosecond lasers [2, 6–8]. V. Khomich · V. Yamshchikov (B) · S. Mikolutskiy Institute for Electrophysics and Electric Power RAS, Saint-Petersburg, Russia e-mail: [email protected] © Springer Nature Switzerland AG 2020 I. A. Parinov et al. (eds.), Advanced Materials, Springer Proceedings in Materials 6, https://doi.org/10.1007/978-3-030-45120-2_5

49

50

V. Khomich et al.

In this paper we consider results on direct laser micro- and nanostructuring by nanosecond lasers with ultraviolet (UV) and vacuum ultraviolet (VUV) radiation of different wavelengths (157, 193 and 355 nm). Moreover, the chapter describes a mechanism of nanostructure formation on the solid surface by nanosecond laser radiation.

5.1.1 Research Purpose The formation of micro and nanostructures on solid surfaces exposed to laser UV and VUV radiation of nanosecond duration is investigated. A theoretical model of nanostructure formation on solid surface by nanosecond laser pulse melting the material is proposed.

5.1.2 Research Scope At this study, we consider the following frameworks of the problem: (i)

experimental setup for direct laser micro- and nanostructuring with nanosecond lasers; (ii) theoretical models of nanostructure formation on the solid surface under the action of nanosecond laser pulse; (iii) analysis of surface topography after laser treatment by UV and VUV radiation.

5.2 Research Method 5.2.1 Experimental Setup for Direct Laser Microand Nanostructuring In our experiments we use a simple method of so called “direct” laser nanostructuring [9, 10], which does not require the use of projection masks, the surface shielding with small micro- and nanoparticles, or the interference of two or more laser beams on the surface of material. This method is effective and affordable in implementation due to simple optical scheme. The method includes only one stage, which is laser irradiation of the surface with high intensity enough for melting or sublimation of the material. As sources of coherent light, we use nanosecond lasers generated UV and VUV radiation of different wavelengths (157, 193 and 355 nm). Nanosecond lasers are simpler and more reliable in operation at a relatively low cost. They have higher output energy and stability of radiation pulses than femtosecond lasers.

5 Formation of Surface Micro and Nanostructures …

51

Fig. 5.1 Scheme of experimental setup for direct laser micro- and nanostructuring. 1—ArF-laser; 2—NdYAG laser; 3—translucent mirror; 4—turning mirror; 5—laser radiation energy meter; 6— condenser; 7—diaphragm; 8—projection lens; 9, 11—fluorite windows; 10—irradiated sample; 12—gas chamber; 13—scanning table; 14, 15, 19, 20—gas valves; 16, 18—pressure regulators; 17—balloon with premix; 21—halogen filter; 22—the vacuum pump; 23—pump; 24—balloon with a gas mixture

Figure 5.1 shows a scheme of an experimental setup [11] consisting of two laser sources: an excimer ArF laser 1 and a pulsed solid-state NdYaG laser 2 operating at the third harmonic. The radiation from the selected laser with a system of dichroic mirrors 3, 3 and mirrors 4, 4 is directed to the forming optical system consisting of the condenser 6, the diaphragm 7 and the projection lens 8, and then through the fluorite window 9 of the gas chamber 12 on the sample 10. The gas chamber allows sample irradiation in gas media, if it is necessary. The gas chamber is mounted on a three-coordinate positioner 13 controlled by a PC to move the irradiation spot along the surface (scanning) of the sample fixed inside. The experimental setup allows laser treatment of material samples with laser pulses of 20 ns duration at wavelengths of 193 and 355 nm. The use of fluoride laser with wavelength of 157 nm allows surface modification of almost any material. The combination of a short pulse duration and a short wavelength radiation absorbed in the micrometer layer makes it possible to affect a thin (near several μm) surface layer, in which large temperature gradients are created, which contribute to the formation of new micro- and nanostructures. In a case of fluoride laser [12] the whole optical path and material sample are inserted in a gas chamber, because of intensive absorption of radiation with a wavelength of 157 nm in the atmosphere. A scheme of this chamber is shown in Fig. 5.2. The chamber can be pumped up with a nitrogen or other working gas. It comprises a window for laser beam entrance 1, a transparent window 8 from polymethyl methacrylate to observe the sample to be irradiated, and also a control mechanism 7 for sample displacement and a sample adjustment with the help of a sample holder 5. Focusing lens 4 and splitting plate 2 were also placed inside the chamber. The laser was connected with the chamber by flexible tube 1. A chamber flange 9 could

52

V. Khomich et al.

Fig. 5.2 Scheme of the gas chamber: 1—flexible tube for laser beam entrance; 2—fluorite plate; 3—energy meter; 4—focusing lens; 5—sample holder; 6—sample; 7—sample control mechanism; 8—transparent window; 9—removable flange

be easily removed allowing to change the sample 6 in the chamber and also to adjust a position of the mentioned optical elements 2, 4 and the laser energy meter 3. The investigation and obtaining of surface topography characteristics of irradiated samples were carried out using the NewView 7300 optical profilometer, the Alpha 300 atomic force microscope (AFM) and the Phenom Pro X table scanning electron microscope. The pulse energy density was estimated as the ratio of the measured laser radiation energy to the characteristic cross-sectional area of the focused laser beam.

5.2.2 Theoretical Model of Nanostructure Formation on the Solid Surface Melted by Nanosecond Laser Pulse There are many models of direct laser nanostructuring of a wide range of technological materials (metals, ceramics, diamond films, polymers) for a variety of surface modification processes [9, 12–14]: (i) (ii) (iii) (iv) (v) (vi)

laser-induced evaporation in the absence of melting, etching, deposition, the combined effect of melting and evaporation, laser pulse melting the surface of solids in the absence of intense evaporation, stress relaxation in the material in the form of nanostructures.

In this chapter we consider the mechanism for nanostructure formation on the solid surface melted by nanosecond laser pulse. Two parts can be mentioned by the solution of this task. In the first part, the process of material melting under the action of laser pulse and the Stefan problem with the corresponding boundary conditions is being solved. In the second part, the process of a melted layer cooling at the expense of heat conductivity into the solid phase together with a theory explaining

5 Formation of Surface Micro and Nanostructures …

53

the formation of crystalline seeds is being considered [9]. In the result, we obtain the expression for the characteristic size of nanostructures depending on the pulse duration and energy. So let us consider a semi-infinite one-dimensional plane of material at initial temperature T = T in for x ∈ [0, ∞]. The material is heated with heat flux of pulsed laser radiation. The flux causes the material to melt down leaving an interval [0, y(t)] occupied by material melt, where y(t) is moving boundary of two phases (liquid and solid). Using heat equations for each phase with corresponding boundary conditions we have ∂ 2 T1 1 ∂ T1 , 0 < x < y(t), = 2 ∂x a1 ∂t

(5.1)

∂ 2 T2 1 ∂ T2 = , 2 ∂x a2 ∂t

(5.2)

y(t) < x < ∞,

T2 (x, 0) = T2 (∞, t) = Tin , ∂ T1 ∂ Q(t) = −λ |x=0 , ∂t ∂x T1 x=y(t) = T2 x=y(t) = Tk ,

(5.3) (5.4) (5.5)

where a, λ, c are the thermal diffusivity, thermal conductivity, and specific heat capacity, respectively; ρ is the material density; Q(t) is the energy absorbed per unit area during t < τ , where τ is the pulse duration; T k is the melting temperature. Liquid phase is denoted by number 1, solid phase is denoted by number 2. Making certain simplifications [9] and solving this system of equations we get transcendental equation to define β: 2cρ(Tk − Tin )

√ a β = 2Hρβ exp β 2 /2a − 2 + Q(τ )/τ er f c √ π 2a

(5.6)

This parameter β allows us to calculate melting depth of different materials irradiating with laser pulses of various duration and energy. After laser pulse ends a phase transition process starts. Liquid phase transforms into solid one. The crystallization with nanostructure formation occurs if cooling rate of molten metal is high enough. To determine the cooling rate we need to solve the problem of molten layer cooling into solid phase [9]. Using variation principle in basic heat conduction law [15] and kinetic equation in nucleation theory [16] we obtain the size of nucleating center of solid phase in supercooled liquid:

54

V. Khomich et al.

h U εt εt (U + h) U kTk2 U − exp − 2 + exp − r (t) = ν0 d exp − kTk U ε U + h U +h kTk kTk2 .

U εt ≈ R 1 − exp − 2 , kTk

(5.7) R=

ν0 d exp(−U/kTk )kTk2 h . εU (U + h)

(5.8)

Here v0 is the Debye frequency of atom oscillation in supercooled liquid, d is the characteristic size per atom, U is the activation energy for atom transition, kT is the thermal energy, μ is the difference of atom chemical potentials in supercooled liquid at temperature T and phase change temperature of T k ( μ = h(T k − T )/T k ), where h is the heat of phase change per atom). For example, at cooling rates ε ≈ 107 °C/s average characteristic size is about 10 nm. By reducing the cooling rate to 106 °C/s and 105 °C/s distribution function shifts to larger sizes with a maximum at r ≈ 100 and ~500 nm, respectively.

5.2.3 Nanostructure Formation Without Melting For some materials such as diamond-like film the surface melting at nanosecond laser pulses is practically absent. A possible mechanism of surface structure formation is a non-homogeneous laser vaporization giving rise to a formation of cones having sub-micron lateral sizes. It is proposed that the growth of cones is initiated by material non-homogeneities represented by particles having a higher ablation threshold F’a then threshold F a of surrounding material. Particles can originally be available in the material or on its surface before irradiation, or can be created in a course of multipulse irradiation as a result of laser-induced chemical transformations. These submicron particles are situated in the peaks of cones. Laser fluence F for cones formation should be in a range F a < F < F’a , otherwise even these more resistant to ablation particles can be removed from the surface. Surface relief in a shape of cones represents an example of self-organizing surface structures at laser ablation. After many pulses the slope i of the lateral surface of cones (Fig. 5.3) changes and is self-adjusted to the incident laser beam in such a way that incident laser fluence F becomes exactly equal to a ablation threshold F a (i) for lateral surface of the cone [12]: F = Fa (i) =

A(i = 0)Fa (i = 0) . A(i) cos i

(5.9)

Here A is the local surface absorption factor depending on the angle of beam incidence i on the lateral surface of the cone. As follows from evident geometrical

5 Formation of Surface Micro and Nanostructures …

55

Fig. 5.3 Scheme of cone formation at laser irradiation; i is an angle of beam incidence on the lateral surface of the cone

i

i

consideration, i is simultaneously the angle at the cone base. The relation (5.9) means that laser ablation stops on cone surface with such angle at the cone base for the given laser fluence F, even at a continuation of irradiation with pulses with such laser fluence. Although the ablation continues to go on parts of the material surface with other slopes having another angle of radiation incidence, it can be a base plane of the material or surface of other cones with other slopes, for which the incidence angle i of incoming radiation is smaller: i < i. The relation (5.9) is valid when two following conditions are fulfilled: √ d λ and d > 2 χ · τ .

(5.10)

Here d is a lateral (along the surface) size of the cones, λ is a radiation wavelength, χ is the thermal diffusivity of the material, τ is a pulse duration. The first inequality is a condition of geometrical optics applicability, and the second inequality provides a difference in heating rates of lateral cone surface and of the base material plane around the cone. This difference provides the emergence and further growth of cone from the base plane. Thus, the minimal cone size can be evaluated from (5.10) as √ dmin > max(λ, 2 χ · τ ).

(5.11)

Thus, if we know the thermal diffusivity of the material and laser radiation parameters, we could estimate the minimal lateral size of structures forming without melting.

56

V. Khomich et al.

5.3 Results and Discussion 5.3.1 Processing by a F2-Laser with Wavelength of 157 Nm The radiation of fluoride laser with extremely short wavelength of 157 nm makes possible the treatment of superhard materials such as ceramics and diamond like films. In our experiments we study the formation of submicron structures on the surface of a diamond like film on a rough copper substrate. The samples were irradiated by fluoride laser with 100 laser pulses with an incident energy density of about 3 J/cm2 at still laser spot. The analysis of irradiated sample surface is carried out by an atomic-force microscope (AFM). AFM analysis shows that for diamond-like film the initial non-irradiated surface already contains nanograins with characteristic lateral sizes from 40 to 70 nm and a small enough aspect ratio about 0.1–0.15 (Fig. 5.4a). After irradiation with laser energy density of 3 J/cm2 conical structures with lateral size from 200 to 600 nm were formed (Fig. 5.4b). The aspect ratio of these structures was about 1. The formation of conical structures on diamond-like film surface can be explained by model of laser ablation without melting mentioned above. In our case for laser ablation of diamond-like film, which is accompanied with a material grafitisation, probable candidates for particles at the peaks of cones can be a material formations from a so-called “hard carbon”, which is intermediate phase between diamond and graphite. According to (5.11) and considering that the thermal diffusivity of material at high temperature stage is about 1 mm2 /s and the pulse duration is 20 ns, we obtain the minimal lateral size of surface structures is about 280 nm. Such simple estimation agrees well with cone sizes 200–600 nm observed in the experiment (Fig. 5.4).

Fig. 5.4 AFM images of non-irradiated diamond-like film (a) and diamond-like film after irradiation by 100 pulses of fluoride laser with energy density of 3 J/cm2 (b)

5 Formation of Surface Micro and Nanostructures …

57

5.3.2 Processing by ArF-Laser with Wavelength of 193 Nm Another source of coherent radiation, which is suitable for nanostructuring, is the excimer ArF-laser with a wavelength of 193 nm, since its radiation strongly absorbed by most materials [14, 17]. In this work the formation of nanoreliefs on germanium surface is carried out by one laser beam without any optional devices and masks. After the necessary preparatory procedures, germanium samples were irradiated by laser pulses with energy density from 2 to 4 J/cm2 and pulse duration of 20 ns. AFM-analysis shows the formation of various types of surface micro- and nanostructures in different parts of irradiation zone. In Fig. 5.5 one can see relief of nonirradiated germanium surface and nanostructures in peripheral low-intensity region of the irradiation spot. They have the form of bulbs with rounded peaks with characteristic dimensions along the surface of 40–120 nm and height of 40–70 nm. Considering the model for nanostructure formation on the solid surface melted by laser pulse (5.1–5.8) with material parameters for germanium and laser irradiation conditions for ArF-laser, we obtain the estimation for average diameter of nanostructures on germanium surface is about 20 nm after the action of 1 laser pulse. Moreover, on the germanium surface AFM-analysis shows the formation of another various types of micro- and nanostructures in different parts of irradiation zone [17]. In the region of shallow melt one can see the relief in the form of hexaand pentagonal cells with characteristic dimensions along the surface of 300–500 nm and the height of the edges between the cells of 20–25 nm. Near the center of the spot in the region of “deep” melt wavy relief arises with period of about 1500 nm and amplitude of about 700 nm. In the ablation zone of central part of the spot we can see wavelike relief with periods of 200–400 nm and amplitude of about 150 nm. Considering these experimental data, we propose five main types of surface reliefs formed by nanosecond laser pulses melting the solid surface [17].

Fig. 5.5 AFM images of non-irradiated germanium surface (a) and germanium after irradiation by 20 pulses of ArF-laser with energy density of 2–4 J/cm2 (b)

58

V. Khomich et al.

Fig. 5.6 AFM images of non-irradiated aluminum oxide surface (a) and aluminum oxide after irradiation by scanning beam of Nd:YaG-laser with scanning speed of 0.25 mm/s and energy density of 0.2 J/cm2 (b)

5.3.3 Processing by a Nd:YaG-Laser with Wavelength of 355 Nm Now we consider micro- and nanostructuring by solid-state Nd:YaG-laser working on third harmonic with wavelength of 355 nm. It is suitable for processing even ceramic materials such as aluminum oxide. Irradiation by scanning beam of solidstate laser at scanning speed of 0.25 mm/s, energy density of about 0.2 J/cm2 and frequency of 100 Hz leads to formation of surface round structures with lateral size from 5 to 15 μm and height of about 1–2 μm (Fig. 5.6). This result can be used for changing tribological or adhesive material properties [4, 18]. Interesting results were obtained in a case of processing the zirconium bronze surface by scanning beam of Nd:YaG-laser. Figure 5.7 shows the structures in the form of submicron spherical drops with diameter of 500 nm located on the tops of conical legs with lateral size of 300–400 nm at a characteristic distance between structures along the surface of 1.5–2 μm [4]. This type of structures is also known as microjets. The formation of such structures was observed at laser pulse energy densities from 0.6 to 1.2 J/cm2 , and the number of spherical structures per unit area increases with increasing laser pulse energy density. It was also found that the number of such structures per unit area increases with a decrease in the scanning speed of the laser beam over the surface [4]. The growth of structures in the form of submicron spherical droplets on the legs can be explained by the combined action of melting and evaporation in a certain range of energy densities above the melting threshold. For example, modulation of the surface topography in the form of capillary waves with micron periods for metals and alloys [19, 20] leads to the corresponding modulation of temperature and evaporative pressure along the surface in the form of a certain two-dimensional quasi-periodic lattice. The melt during such inhomogeneous evaporation is squeezed

5 Formation of Surface Micro and Nanostructures …

59

Fig. 5.7 Images of bronze surface irradiated by scanning beam of Nd:YaG-laser with energy density of 1.2 J/cm2 by means of AFM (a) and SEM (b)

along the surface to the places of the minimum evaporation pressure, where the liquid jets of the melt are released mainly in the direction transverse to the surface. In this case, the surface tension forces lead to the development of spherical droplets at the ends of these jets at the final stage of their development, when the action of pulsed evaporation pressure ends and solidification of the melt begins. Materials with surface processed in this way could be used in different fields of science and technology. For example, we use laser surface micro- and nanostructuring in diffusion welding, where heterogeneous materials such as metallic alloys connect to each other in special chamber at high temperature and pressure [4].

5.4 Conclusion A method of direct laser micro- and nanostructuring by nanosecond lasers with UV and VUV radiation of different wavelengths (157, 193 and 355 nm) is proposed. A theoretical model of nanostructure formation on solid surface melted by nanosecond laser pulse is considered. Moreover, a simple model for formation of conical structures at laser ablation without melting is described. Both models give consistent results according to experimental data for corresponding processes of laser treatment. Using the radiation of nanosecond F2-laser, ArF-laser and Nd:YaG-laser micron, submicron and nanostructures were obtained on the surfaces of diamond-like film, germanium, aluminum oxide and zirconium bronze. These types of structures can be used in nanophotonics, spectroscopy, microelectronics, machine manufacturing, nuclear industry, aviation, space technology, and many other fields of science and technology.

60

V. Khomich et al.

Acknowledgements This research was performed into framework of State assignment of IEE RAS.

References 1. F. Luo, W. Ong, Y. Guan, F. Li, Sh Sun, G.C. Lim, M. Hong, Appl. Surf. Sci. 328, 405 (2015) 2. T. Csizmadia, T. Smausz, C. Tapai, J. Kopniczky, X. Wang, M. Ehrhardt, P. Lorenz, K. Zimmer, L. Orosz, E. Varga, E. Oszko, B. Hopp, J. Laser Micro Nanoeng. 10(2), 110 (2015) 3. V.Yu. Fominskii, S.N. Grigor’ev, R.I. Romanov, V.N. Nevolin. Techn. Phys. 57(4), 516 (2012) 4. Yu.A. Vashukov, S.F. Demichev, V.D. Elenev, T.V. Malinskiy, S.I. Mikolutskiy, Yu.V. Khomich, V.A. Yamshchikov, Appl. Phys. 1, 82 (2019). (in Russian) 5. P.F. Rios, H. Dodiuk, S. Kenig, S. McCarthy, A. Dotan, J. Adhes. Sci. Technol. 20(6), 563 (2006) 6. K. Vestentoft, J.A. Olesen, B.H. Christensen, P. Balling, Appl. Phys. A 80, 493 (2005) 7. Y. Nakata, T. Okada, M. Maeda, Proc. SPIE Int. Soc. Opt. Eng. 5662, 749 (2004) 8. X. Wang, Y. Lu, J. Appl. Phys. 98, 114304 (2005) 9. S.I. Mikolutskiy, V.Yu. Khomich, V.A. Shmakov, V.A. Yamshchikov, Nanotechnol. Russ. 6(11– 12), 733 (2011) 10. V.N. Tokarev, V.A. Shmakov, R.R. Khasaya, S.I. Mikolutskiy, S.V. Nebogatkin, V.Yu. Khomich, V.A. Yamshchikov, in Proceedings of the 29th International Congress on Applications of Lasers and Electrooptics, Anaheim, USA, p. 1257 (2010) 11. Yu.A. Zheleznov, T.V. Malinskiy, S.I. Mikolutskiy, Yu.V. Khomich, V.N. Tokarev, R.R. Khasaya, V.A. Yamshchikov, Appl. Phys. 3, 83 (2014). (in Russian) 12. V.N. Tokarev, V.Yu. Khomich, V.A. Shmakov, V.A. Yamshchikov, Phys. Chem. Mater. Treat. 4, 18 (2008). (in Russian) 13. V.Yu. Khomich, V.A. Shmakov, Phys. Uspekhi 58, 455 (2015) 14. D.V. Ganin, S.I. Mikolutskiy, V.N. Tokarev, V.Yu. Khomich, V.A. Shmakov, V.A. Yamshchikov, Quantum Electron. 44(4), 317 (2014) 15. J. Christian, in The Theory of Transformations in Metals and Alloys. Pergamon, Oxford, 1200 p. (1975) 16. M.A. Biot, Variational Principles in Heat Transfer. Oxford University Press, Oxford, 185 p. (1970) 17. S.I. Mikolutskiy, R.R. Khasaya, Yu.V. Khomich, V.A. Yamshchikov, J. Phys: Conf. Ser. 987, 012007 (2018) 18. Yu.A. Zheleznov, T.V. Malinskiy, Yu.V. Khomich, V.A. Yamshchikov, Inorg. Mater.: Appl. Res. 9(3), 460 (2018) 19. S.A. Ahmanov, V.I. Emel’yanov, N.I. Koroteev, V.N. Seminogov. Phys. Uspekhi 147, 675 (1985) 20. V.N. Elkin, T.V. Malinskiy, S.I. Mikolutskiy, R.R. Khasaya, Yu.V. Khomich, V.A. Yamshchikov, Phys. Chem. Mater. Treat. 6, 5 (2016). (in Russian)

Chapter 6

The Effect of Preliminary Laser Surface Treatment on the Mechanical Properties of a Solid-Phase Compound of an Iron-Nickel Alloy in Diffusion Welding Yury Khomich and Vladimir Yamshchikov Abstract Laser micro- and nanostructuring is used in various fields of science and technology, because it can improve different surface properties. The chapter considers a method of direct laser micro- and nanostructuring of metallic surfaces and an effect of such preliminary laser surface treatment on the mechanical properties of solid-phase joints made by diffusion welding. For laser treatment it is proposed to use scanning beam of Nd:YAG laser with a wavelength of 355 nm. Analysis of surface topography of samples treated by nanosecond laser was performed by optical profilometer. After the diffusion welding tensile tests were performed on conjunction samples cut out from welded workpieces. These tests showed that preliminary laser processing of the surface of samples made of nickel alloy leads to an improvement in the mechanical properties of the conjunction obtained by diffusion welding. It leads to an increase in the tensile strength up to 29% and tensile strain up to 20%. The pulse energy density at laser surface treatment significantly affects the properties of welded joint. Also the preliminary laser treatment of surfaces allows one to reduce the temperature of diffusion welding.

6.1 Introduction Laser surface modification with the formation of micro and nanostructures is used in various fields of science and technology. Laser processing can improve electronemission, radiative, tribological, hydrophobic and hydrophilic surface properties of materials [1–5]. Also the formation of periodic micron and submicron structures with specified geometry parameters by means of laser irradiation of the surface can lead to an improvement in the adhesion properties of materials and, thereby, an increase in the quality of the joint at a diffusion welding of homogeneous and dissimilar metals and alloys [6, 7]. The diffusion welding is a junction method, in which the parts Y. Khomich · V. Yamshchikov (B) Institute for Electrophysics and Electric Power RAS, Saint Petersburg, Russia e-mail: [email protected] © Springer Nature Switzerland AG 2020 I. A. Parinov et al. (eds.), Advanced Materials, Springer Proceedings in Materials 6, https://doi.org/10.1007/978-3-030-45120-2_6

61

62

Y. Khomich and V. Yamshchikov

come into contact under the conditions of a defined continuous pressure and heat up in the contact area or in the entire volume at a given temperature for a certain time [8]. In diffusion welding the connection is achieved due to mutual diffusion at the atomic level of the surfaces of the parts to be welded. The advantages of diffusion welding include the possibility of welding parts of different thickness and surfaces with a large area. This method is widely used in the nuclear industry, aviation and space technology. In this paper we consider results on direct laser micro- and nanostructuring of the metallic surfaces and the effect of this preliminary laser surface treatment on the mechanical properties of solid-phase joints made by diffusion welding.

6.1.1 Research Purpose The effect of preliminary laser surface treatment on the mechanical properties of a solid-phase compound of a nickel alloy in diffusion welding is investigated. A method of direct laser micro- and nanostructuring is proposed for sample surface treatment.

6.1.2 Research Scope At this study, we consider the following frameworks of the problem: (i) direct laser micro- and nanostructuring with nanosecond lasers; (ii) theory of nanostructure formation on the solid surface under action of laser pulse; (iii) analysis of surface topography of samples treated by nanosecond laser; (iv) diffusion welding of irradiated samples and tensile tests for compounds obtained.

6.2 Research Method 6.2.1 Experimental Setup for Direct Laser Microand Nanostructuring Various methods are used, among them applying of projection masks, interference of two or more laser beams, combination of laser radiation with the tip of a scanning probe microscope, and direct laser nanostructuring using picosecond and femtosecond lasers.

6 The Effect of Preliminary Laser Surface Treatment …

Diaphragm

63

Forming diaphragm

Target material

Laser 355 nm

Condenser

Projection lens

Fig. 6.1 Scheme of projection-optical system for method of direct laser micro and nanostructuring

In our experiments, we use the method of direct laser micro and nanostructuring with nanosecond lasers. This method is very affordable and effective in implementation, because it has a simple projection-optical system shown in Fig. 6.1. The method includes only one stage. It is a laser irradiation of the surface with intensity sufficient for melting or sublimation of the material. Scanning the surface by laser beam with high repetition rate of radiation pulses opens up the possibility of nanostructuring sufficiently large extended surface areas. As sources of coherent light we use nanosecond lasers generated UV and VUV radiation. At a relatively low cost, such lasers are simpler and more reliable in operation; they have higher output energy and stability of radiation pulses than femtosecond lasers. Based on said above, an experimental setup for direct laser micro- and nanostructuring of the solid surface was created with use of ArF laser with a wavelength of 193 nm [9] and an Nd:YAG laser operating at the third harmonic with a wavelength of 355 nm [10]. When replacing the gas mixture and the optics, the ArF laser can work as an F2 laser and generate nanosecond radiation pulses with an extremely short wavelength of 157 nm. This allows one to perform surface modification of almost any material. The combination of the short wavelength absorbed in the micrometer layer and the short pulse duration makes it possible to influence a small (several micrometers) surface layer, in which large temperature gradients are created, which contribute to the formation of new micro- and nanostructures. The shape and size of these structures also depend on the energy density, wavelength, number of pulses in the laser spot, as well as on the pulse repetition rate and the scanning speed of the laser beam over the surface [11]. As mentioned above laser processing can also influence the surface properties of a material. This can be used in laser technologies for surface preparation in diffusion welding.

64

Y. Khomich and V. Yamshchikov

In this chapter we performed experimental studies on diffusion welding with preliminary laser processing of the welded surfaces of workpieces made of nickel alloy (ChS57). For the experiments we used cylindrical samples with a diameter of 22 mm and a height of 18 mm. In order to prevent the formation of oxides on the surface of the workpieces during laser processing, the samples were placed in a sealed chamber from which air was evacuated and an inert gas (argon) was injected under a pressure of 1.5 atm. The surfaces to be welded were pretreated with radiation of Nd:YAG laser pulses with a wavelength of 355 nm. The pulse duration was 10 ns, the pulse repetition rate was 100 Hz and the cross-section radius of the laser spot in the workpiece plane was 220 µm. The laser beam was moved along the surface of the workpieces along a raster path (snake) at a speed of 1 mm/s and a pitch of 10 µm along the x-axis and 30 µm along the y-axis. The main variable laser processing parameters were pulse energy density and number of laser pulses per unit area.

6.2.2 Nano- and Microstructure Formation Under the Action of Laser Pulse The duration of pulses of nanosecond laser radiation is much longer than the electronphonon relaxation time, which is several or tens of picoseconds for various materials. Therefore, thermal processes occur already during laser exposure to the material. The depth of the surface layer modified by laser radiation is determined by a thermal diffusion length during the duration of the laser pulse τ . √ LT = 2 χ · τ.

(6.1)

Here χ is the thermal diffusivity of the material. When irradiated with nanosecond pulses, L T turns out to be much larger than for femtosecond pulses. For metals the depth of the modified layer reaches several microns. This can be crucial for a number of practical applications, for example in the case diffusion welding. From the theoretical point of view there are many models of direct laser nanostructuring of a wide range of technological materials (metals, ceramics, diamond films, polymers) for a variety of surface modification processes: laser-induced evaporation in the absence of melting; etching; deposition; the combined effect of melting and evaporation; laser pulse melting the surface of solids in the absence of intense evaporation; stress relaxation in the material in the form of nanostructures [11–14]. In a case of heat-resistant nickel alloy, which consists of many different elements, defining the mechanism of surface structure formation is a very complicated task. However, for simple evaluation of sizes of surface structures formed by laser radiation one can use formula for lateral size of long roughness periods [14]: dmin > max(λ, L T ),

(6.2)

6 The Effect of Preliminary Laser Surface Treatment …

65

where λ is a radiation wavelength. We use a third harmonic of Nd:YAG laser with a wavelength of 355 nm. Considering that in our case the thermal diffusivity χ of nickel alloy is about 6 mm2 /s and the pulse duration is 10 ns, we obtain the thermal diffusion thickness L T near to 500 nm. Thus, for our case minimal lateral size of surface structures is about 500 nm.

6.2.3 Diffusion Welding Diffusion welding is widely used in many engineering industries. The implementation of welding in hot isostatic press extends the technological capabilities of this method. Improving the quality of the connection and expanding the allowable temperature range of welding remains to be a relevant task. Diffusion welding is pressure welding in which parts contact at a set continuous pressure and are heated in the contact area or in the entire volume at a given temperature for a specified time. We performed diffusion welding in gasostat (Abra, Switzerland) under hot isostatic pressing (ISP) conditions. The scheme of diffusion welding in gasostat is presented on Fig. 6.2a. Figure 6.2b shows cyclograms of temperature and pressure changes during diffusion welding. Welding of workpieces was carried out at temperature 1000 °C and at temperature 1160 °C. In both cases working continuous pressure was about 160 MPa. The welding time was about 3 h. We performed experimental investigation on diffusion welding with preliminary laser processing of the welded surfaces of workpieces made of nickel alloy (ChS57). Two modes with different energy density of laser radiation were used for sample (a)

(b)

Fig. 6.2 Scheme of diffusion welding (a) and cyclograms of temperature and pressure changes during diffusion welding (b)

66

Y. Khomich and V. Yamshchikov

Fig. 6.3 Vacuum container with three groups of samples: (1) laser treatment with the energy density 2 J/cm2 (mode 1); (2) laser treatment with the energy density 3 J/cm2 (mode 2); (3) samples with non-irradiated surface; (4) thin walled container; (5) container cover

surface treatment: mode 1 with the energy density 2 J/cm2 , mode 2 with the energy density 3 J/cm2 . After laser treatment the samples were placed in a container as shown on Fig. 6.3. The container was sealed by an electron beam in a vacuum and then it was placed in a gasostat.

6.3 Results and Discussion 6.3.1 Processing by a Scanning Beam of Nd:YAG Laser As mentioned above the sample surfaces were pretreated by scanning beam of Nd:YAG laser working on third harmonic with a wavelength of 355 nm. The pulse duration was 10 ns, the pulse repetition rate was 100 Hz and the cross section radius of the laser spot in the workpiece plane was about 200 µm. The laser beam was moved along the surface of the workpieces along a raster path (snake) at a speed of 1 mm/s. The profiles of the irradiated surface were analyzed with an optical profilometer (Zygo NewView 7300). Figure 6.4a shows surface profile of nickel alloy marked as ChS57 without laser treatment, where only mechanical treatment traces are visible in the form of furrows with a width of 10–40 µm and a height of 5 µm. Surface profile after laser treatment with a pulse energy density of 1 J/cm2 is shown in Fig. 6.4b and c presents an optical image of the same irradiated surface of ChS57. As can be seen, after laser irradiation the initial grooves begin to break into round hill-shaped islands with transverse dimensions from 5 to 10 µm and a height of approximately 500 nm.

6 The Effect of Preliminary Laser Surface Treatment …

67

Fig. 6.4 Profilometry data for non-irradiated ChS57 surface (a) and surface after laser treatment with energy density of 1 J/cm2 (b) with its optical image (c)

68

Y. Khomich and V. Yamshchikov

For further diffusion welding sample laser processing was performed in two modes with different energy density of laser radiation: mode 1 with the energy density 2 J/cm2 , mode 2 with the energy density 3 J/cm2 .

6.3.2 Tensile Tests After Diffusion Welding of Samples Treated by Laser After laser treatment, the nickel alloy samples were placed in a container, which was sealed by an electron beam in a vacuum. Then the diffusion welding in gasostat was carried out at certain conditions mentioned above (Fig. 6.2). After the diffusion welding tensile tests were performed at room temperature on conjunction samples cut out from welded workpieces. In the result of tensile tests for nickel alloy conjunctions we obtained average tensile strength and tensile strain for different welding temperatures and modes of laser treatment. Figure 6.5 shows tensile strength of welded joints of ChS57 samples without preliminary processing and after laser modification in modes 1 and 2. They are obtained at welding temperatures T = 1160 °C and T = 1000 °C. For temperature T = 1160 °C the tensile strength of the conjunctions with laser treatment reaches 630 MPa. There is an increase of the tensile in both modes by 12% compared to control non-irradiated samples. When the temperature of hot isostatic pressing is reduced to 1000 °C, the effect of laser treatment on the tensile strength in mode 1 becomes even more significant and reaches 29%. Thus, preliminary laser treatment with an energy density of 2 J/cm2 provides an increase in the tensile strength at the welding temperature of 1000 °C and at a temperature of 1160 °C. Similar results are observed for tensile strain also called an elongation at break (Fig. 6.6). At a temperature of 1160 °C the tensile strain of the laser treated conjunctions in both modes increased by 20% compared to the control non-irradiated Fig. 6.5 Tensile strength of welded joints of ChS57 samples without preliminary processing and after laser modification; welding temperature T = 1160 °C (orange column) and T = 1000 °C (blue column)

6 The Effect of Preliminary Laser Surface Treatment …

69

Fig. 6.6 Tensile strain (elongation at break) of welded joints of ChS57 samples without preliminary processing and after laser modification; welding temperature T = 1160 °C (orange column) and T = 1000 °C (blue column)

samples. However, at the temperature near 1000 °C these values differ significantly. For mode 1, the elongation increased by 2.6 times, and for mode 2 decreased by 20%. Thus, the pulse energy density during surface laser treatment of welded samples significantly affects the mechanical characteristics of the welded joint. Let us consider some possible reasons for the improvement of mechanical properties in welded joints with preliminary laser treatment of the surface. It is known that the diffusion coefficient along the grain boundaries can be some orders of magnitude higher than the values in the grain volume [15]. Therefore, the creation of ultra-fine-grained material on the surface under the action of a laser can significantly increase the density of the mesh along the grain boundaries and provide a more active diffusion in the material. The second reason for improving the mechanical properties of the welded joint may be a more uniform distribution of the degree of deformation in conjunctions with preliminary laser surface treatment. The creation of micro and nanostructures on the surfaces to be welded results in more efficient slamming of irregularities in the joint area [16]. In our results, the preliminary laser treatment of surfaces allows one to reduce the temperature of diffusion welding. At a reduced temperature, the phenomenon of low-temperature superplasticity can play a significant role in the character of the solid-phase conjunction. This phenomenon is observed in metals and alloys, which are characterized by a structure with an ultra-fine grain with a diameter of about 1 µm or less [17, 18]. Such average size of the grains can be formed during the preliminary laser treatment. Early by us it has been shown that the lower energy density of the laser pulses, the smaller characteristic size of the surface structures [13, 14]. This circumstance is consistent with the results of experiments in which a higher quality

70

Y. Khomich and V. Yamshchikov

conjunction was obtained in mode 1 with a lower energy density of irradiation pulses than in mode 2 at a welding temperature reduced to 1000 °C.

6.4 Conclusion Preliminary laser processing of the surface of samples made of nickel alloy leads to an improvement in the mechanical properties of the conjunction obtained by diffusion welding. In particular, it leads to an increase in the tensile strength up to 29% and tensile strain up to 20%. The pulse energy density at laser surface treatment significantly affects the properties of welded joint. Also the preliminary laser treatment of surfaces allows one to reduce the temperature of diffusion welding. Thus, the present method of preliminary surface laser treatment for welded samples can be used in nuclear industry, aviation and space technology to improve bonding quality of dissimilar materials. Acknowledgements This research was performed with the support of Presidium of the Russian Academy of Sciences, the Basic Research Program I.7. The authors thank Elkin V. N. and Malinsky T. V. for their assistance in conducting experiments and discussing the results of the work.

References 1. H.A. Quintana, E. Song, G.T. Wang, J.A. Martinez, Chem. Eng. Process Technol. 1, 1008 (2013) 2. C.-T. Hsieh, J.-M. Chen, H.-H. Lin, H.-C. Shih, Appl. Phys. Lett. 83, 3383 (2003) 3. V.Yu. Fominskii, S.N. Grigor’ev, R.I. Romanov, V.N. Nevolin. Tech. Phys. 57(4), 516 (2012) 4. C.H. Crouch, J.E. Carey, J.M. Warrender, M.J. Aziz, E. Mazur, Appl. Phys. Lett. 84(11), 1850 (2004) 5. M.C. Ferrara, L. Pilloni, S. Mazzarelli, L. Tapfer, J. Phys. D Appl. Phys. 43, 095301 (2010) 6. V.N. Elkin, V.P. Gordo, V.V. Melukov, Bull. PNRPU Mech. Eng. Mater. Sci. 183(7), 673 (2013) (in Russian) 7. Yu.A. Vashukov, S.F. Demichev, V.D. Elenev, T.V. Malinskiy, S.I. Mikolutskiy, Yu.V. Khomich, V.A. Yamshchikov, Appl. Phys. 1, 82 (2019) (in Russian) 8. N.F. Kazakov, Diffusion Welding of Materials (Mashinostroenie, Moscow, 1976), 312 p (in Russian) 9. S.I. Mikolutskiy, R.R. Khasaya, Yu.V. Khomich, V.A. Yamshchikov, J. Phys: Conf. Ser. 987, 012007 (2018) 10. S.I. Mikolutskiy, R.R. Khasaya, Yu.V. Khomich, in Proceedings of the 14th Sino-Russia Symposium on Advanced Materials and Technologies, November 2017 (Metallurgical Industry Press, Beijing, 2017), p. 319 11. V.Yu. Khomich, V.A. Shmakov, Physics Uspekhi 58, 455 (2015) 12. D.V. Ganin, S.I. Mikolutskiy, V.N. Tokarev, V.Yu. Khomich, V.A. Shmakov, V.A. Yamshchikov, Quantum Electron. 44(4), 317 (2014) 13. S.I. Mikolutskiy, V.Yu. Khomich, V.A. Shmakov, V.A. Yamshchikov, Nanotechnol. Russ. 6(11– 12), 733 (2011)

6 The Effect of Preliminary Laser Surface Treatment …

71

14. V.N. Tokarev, V.Yu. Khomich, V.A. Shmakov, V.A. Yamshchikov, Phys. Chem. Mater. Treat. 4, 18 (2008) (in Russian) 15. M.Kh. Mukhametrakhimov, Lett. Mater. 3, 276 (2013) (in Russian) 16. R.G. Khazgaliev, M.F. Imayev, R.R. Mulyukov, F.F. Safin. Lett. Mater. 5(2), 133 (2015) (in Russian) 17. M.W. Mahoney, Superplastic properties of alloy 718, in Superalloy 718—Metallurgy and Applications, ed. by E.A. Loria (The Minerals, Metals & Materials Society, 1989), p. 391 18. R.Ya. Lutfullin, O.A. Kaibyshev, O.R. Valiakhmetov, M.Kh. Mukhametrakhimov, R.V. Safiullin, R.R. Mulyukov, Perspect. Mater. 4, 21 (2003) (in Russian)

Chapter 7

The Nucleation and Development of Wear in Nanocomposite Coatings Under the Action of a Discrete Vapor-Droplet Flow Valery N. Varavka, Oleg V. Kudryakov, Igor Yu. Zabiyaka, and Natalia I. Bronnikova Abstract The analysis of the initial stage of wear initiation in crystalline materials with a heterogeneous structure under cyclic impact loading is conducted. Wear under these conditions begins with the formation of fatigue defects. Depending on the structure of the material and loading conditions, they are formed as cracks, pores or craters. A theoretical model is proposed for calculating the duration of their nucleation. The parameters of the model for its application in the conditions of droplet impingement erosion, in particular, under the influence of a discrete vapor-droplet flow, are considered and determined. The results of model calculations are presented in comparison with the experimental data of bench droplet tests for steel samples 20Cr13 with a sorbite structure and samples with a vacuum ion-plasma coating of the TiAlSi-system with a 3D-nanocomposite structure. It is shown that under conditions of contact cyclic loads, the wear resistance of materials and coatings is primarily determined by structural parameters. Based on the presented calculation results and experimental data, the use of the proposed model for the design of wear-resistant materials and coatings is recommended. Experimental data on the development of wear of the ion-plasma TiAlSi-coating upon droplet impingement action are also presented. Chipping of the coating occurs by the formation of fragmented porous cracks.

7.1 Introduction From the applied point of view, the most problematic field of knowledge in studying of the fatigue wear of various industrial materials is the stage of nucleation of fracture sites, which can be cracks, pores, microcraters. Thus, when studying crack nucleation due to difficulties in instrumental fixing of cracks at the early stages of its development, it is necessary to resort to the method of analogies or use empirical coefficients in calculation models. This approach leads to uncontrolled computational errors. V. N. Varavka · O. V. Kudryakov (B) · I. Yu. Zabiyaka · N. I. Bronnikova Material Science Department, Don State Technical University, Rostov-on-Don, Russia e-mail: [email protected] © Springer Nature Switzerland AG 2020 I. A. Parinov et al. (eds.), Advanced Materials, Springer Proceedings in Materials 6, https://doi.org/10.1007/978-3-030-45120-2_7

73

74

V. N. Varavka et al.

In this regard, the goal of the work was to develop a universal computational and analytical model that describes the stage of initiation of fatigue defects in order to increase the accuracy of estimates of the performance of materials under conditions of impact and fatigue loading. The universality of the model refers to its applicability to most industrial materials and coatings. As an applied use of such a model, the field of exploitation of materials and coatings in the conditions of droplet impingement erosion is determined, for example, when the blade turbine equipment is operating in an environment with vapor-droplet condensate. Based on these conditions, the analytical task of constructing a model is to establish expressions for calculating the number of impacts of droplets N 3 with a turbine blade, which are necessary for the formation of a fatigue defect of critical size in a material or coating.

7.2 Theoretical Foundations of the Calculate-Analytical Model The final equation for calculating N 3 should include mechanical, kinetic and structural components, each of them characterizes a separate side of the complex process of droplet impingement erosion [1–6]. Moreover, the action of all components of the total number of impacts N 3 on the process of formation of a fatigue defect occurs at each collision simultaneously. Moreover, the interaction of the mechanical, kinetic and structural components of the impact-droplet effect on the material or coating has a commutative character. The universality of the developed model and the commutative nature of the contributions of all its components can be ensured provided that all components of the model are connected by a single theoretical basis. When the object of the study is crystalline materials or coatings, such a unified basis for the components of the model can be the theory of defects in the crystal structure, namely, the theory of dislocations. We consider this thesis as applied one to each component of the droplet-impacts process. The mechanical component is associated with the density of mobile dislocations ρ m arising from a single drop impact. In the process of multiple impacts, the number of mobile dislocations increases, they move in the metal matrix along the slip planes under the action of shear stresses σ s until they form flat clusters (“pile-up” with a critical density ρ kr ) at the nearest insurmountable barriers. We take as ρ kr = 1016 m−2 the dislocation density, the excess of which leads to spontaneous breaking of interatomic bonds in the metal and the formation of a crack nucleus. Then the mechanical component of the number of impacts is expressed as N 3 = f (ρ kr /ρ m ). The kinetic component of the number of impacts N 3 takes into account the dependence of the dislocation energy on its velocity V d . Dislocation glide upon impact occurs at a high speed. It is known from the theory of dislocations that as the speed of a dislocation increases, its energy increases in accordance with an expression similar to Einstein’s expression for bodies moving with speeds close to the speed of light. For a dislocation velocity, the limit is the speed of sound in a crystal C 0 . When V d

7 The Nucleation and Development of Wear in Nanocomposite …

75

= C 0 , the dislocation energy becomes infinite. Therefore, under the conditions of droplet impacts, the kinetic component of the number of collisions is expressed as N 3 = f (V d /C 0 ). The structural component of the number of impacts N 3 must take into account two circumstances. First, upon impact, the movement of dislocations is limited by the size of the structural element of the metal matrix, within which the free path of the dislocations is possible. For polycrystalline materials, grain size D is usually considered as such an element. On the other hand, secondly, within the grain there can be various obstacles to the movement of dislocations: particles of secondary phases, small-angle boundaries, the dislocations fixed by atmospheres, and stacking faults. Even if there are no such obstacles in the structure of the material, there is lattice resistance—Peierls stress. Therefore, the structural component of the number of impacts must take into account both of these points and will be a function of two variables N 3 = f (D, G), where G is Gibbs free energy to activate the process of overcoming a moving dislocation of obstacles within the structural element D. The mechanism of overcoming the obstacle depends on the nature of the obstacle and can be different, which determines the value of G for each specific type of material structure. The dislocation concept of the model, the analysis of its components, and the commutative principle of their interaction lead to the following theoretical expression for the value of N 3 calculation [7]: ρkr N3 = · ρm

1−

Vd C0

2 ·

D − G · e kT l0

(7.1)

where l0 is the path traveled by moving dislocations in one loading cycle (single impact/collision); k is the Boltzmann constant; T is the thermodynamic temperature.

7.3 Estimation of the Model Parameters To use expression (7.1) as a calculation method for evaluating the wear resistance of materials and coatings under conditions of cyclic liquid-droplet impacts, it is necessary to express the quantities entering into it (such as ρ m , V d , l 0 , G) in terms of measured impact/collision parameters, such as droplet size R0 and collision velocity V 0 . Thus the value of ρ m at the established stage of plastic flow is exclusively a function of stress σ s and temperature. The simplest dependence, consistent with theory and experiment [8, p. 25]: ρm = α ·

σs μ·b

2 (7.2)

76

V. N. Varavka et al.

where μ is the shear modulus; b is the Burgers vector; α is the coefficient taken under normal conditions as α = const ≈ 1. The shear stress in the slip plane, under the action of which the sliding of dislocations occurs, is considered as the stress σ s in expression (7.2). Stress σ s can be expressed in terms of impact parameters. In some of our works (see, for example, [4]), the stress in the surface layer of the target metal in the center of the collision zone during a single loading cycle (droplet impact) is expressed in relative units of ρ 0 · c0 · V 0 , called the hydraulic impact approximation, where ρ 0 is the density of the unperturbed liquid, c0 is the speed of sound in a liquid under normal conditions (for water ρ 0 = 1000 kg/m3 , c0 = 1500 m/s). Under the conditions that the average level of acting stresses during a complete cycle of a single loading (collision) is determined by the value of σ m = 0.33 · ρ 0 · c0 · V 0 , and the dislocation glides over the entire time of this cycle with a length τ = 2 · R0 /V 0 , we can switch from the applied external stress σ m to the shear stress in the slip plane σ s . To do this, we use the Schmidt-Boas law for a polycrystal: σm = Mp × σs

(7.3)

where M p is the Taylor factor, component: M p = 2.9 for bcc-metals and M p = 3.06 for fcc-metals [8, p. 30]. Then, in accordance with formula (7.2), the stress σ s is expressed in terms of the impact parameters: σs =

0.33 · ρ0 · c0 · V0 Mp

(7.4)

Under impact loading, the strain rate can reach very large values (more than 102 s ). In this case, plastic deformation (hardening) is controlled by phonon and electronic braking of dislocations. The sliding velocity of dislocations for these conditions is determined by the braking coefficient B from the expression [8, p. 31]: −1

Vd = σs × b/B

(7.5)

where the values of the braking coefficient B are in a rather narrow range 10−5 …10−4 Ns/m2 , for further calculations we accept B = 10−4 Ns/m2 . Taking into account expressions (7.4) and (7.5) and assuming the linearity of the motion law, the mean free path of dislocations per loading cycle (one droplet impact) is defined as l0 = V d · τ and can be written as: l0 =

0.66 · R0 · ρ0 · c0 · b B · Mp

(7.6)

The determination of the energy of overcoming of structural obstacles by dislocations G requires a more detailed analysis. From classical works on the theory of dislocations (for example, [8–10]), it is known that the energy G is a function of stress σ s and depends on the shape and

7 The Nucleation and Development of Wear in Nanocomposite …

77

distribution of obstacles, as well as on the field of internal stresses between obstacles. In general terms, the value of G in (7.1) can be represented as: σs G(σs ) = F · 1 − στ

(7.7)

where F is the activation energy of the process of overcoming obstacles without applying external stress, value of F actually determines the strength of the obstacles with respect to the movement of dislocations; σ τ is the internal stress existing in the material and allowing the dislocation to pass through the obstacle at the minimum values of G; the flow stress of the solid at T = 0 K is taken as σ τ . Values σ τ and F are the properties of the material and, in the general case are expressed through its basic physical characteristics μ and b: σt = α1 · μ · b/l; F = α2 · μ · b3 .

(7.8)

The value l in the expression (7.8) represents the distance between the obstacles. Coefficients α 1 and α 2 characterize obstacles in their resistance to the motion of dislocations. In metal-physical terminology, α 1 and α 2 classify obstacles by strength. Between the parameters l, α 1 and α 2 there is a rather strict correlation. So, strong or large particles of secondary phase precipitates are determined by the coefficient α 2 = 2, and the linear average statistical distance between the precipitates is taken as l. Small particles cutting by dislocation, as well as the dislocation “forest”, formed, for example, during strain hardening, considered medium-strength obstacles. Such obstacles have a coefficient α 2 = (0.2–1.0), and as l is taken the distance between the √ dislocations, i.e. l = 1/ ρd . Low-strength obstacles include atoms of an element dissolved in the lattice (for example, during quenching) or Peierls resistance of the lattice (at a relatively low dislocation density ρ d ). In this case α 2 < 0.2, and the value l has a size commensurate with the Burgers vector b. This data indicates that a deterministic inverse relationship is observed between the values σ τ and F: as the strength of the obstacles increases, the stress in the lattice σ τ between the obstacles weakens, respectively, the energy of overcoming obstacles F increases. The physical meaning of coefficient α 1 is not completely clear. According to the results of our studies, including numerical experiments, we can say that for compact metal materials in which dislocation interactions are determined by the type of microstructure and the free path of dislocations is always greater than the distance √ between dislocations (D > 1/ ρm ), coefficient α 1 in expression (7.8) can not be used, i.e. α 1 = 1. Coefficient α 1 , different from 1, is relevant for nanomaterials and nanostructured coatings. For this category of materials, coefficient α 1 in expression (7.8) acts as a regulator of the Burgers vector value. This fact may indirectly indicate that plastic deformation in nanomaterials is carried out with the participation of partial or grain boundary dislocations. Thus, the presented calculation and analytical model is universal with respect to materials and coatings of various nature, for which the dislocation concept of the

78

V. N. Varavka et al.

considered processes is applicable. The obtained basic expression of model (7.1) is based on the principle of commutativity of components: the generation of mobile dislocations, their sliding speed and free path, the mechanism for overcoming structural obstacles. It determines the number of loading cycles N 3 necessary for the formation of a critical local dislocation density that initiates a fatigue defect formation. The morphology of the resulting defect (crack, pore, microcrater) depends on the properties of the material and was considered in some of our previous works [4–6]. The free path of dislocations is limited by the size of the structural element of the matrix. By default, this element is the grain size, for thin monolayers of coatings— their thickness. The model also includes such characteristics of the material as: the speed of sound in the crystal, its temperature, the activation energy of the process of overcoming obstacles by dislocations, the stress in the slip plane, the resistance of the lattice (Peierls stress), etc. The main feature of the model is that the calculations are based on either known reference material characteristics (μ, b, M p ), or measured process parameters (V 0 , R0 ). This makes the model practically feasible, in particular, in the conditions of droplet impingement erosion of materials and coatings.

7.4 Research Results and Discussion As an applied use of the calculation model (7.1), its numerical solutions were obtained for those materials for which experimental data of bench tests under the conditions of droplet cyclic impacts had been carried out. This made it possible to compare and evaluate the calculated and experimental results. Comparative data was obtained for two congruent materials with the heterogeneous structure of same type: (i) steel 20Cr13 after quenching and high tempering, the samples had a trivial sorbite structure, which is not shown in the illustrations; (ii) vacuum ion-plasma coating of the TiAlSi-system with the structure of a 3Dnanocomposite on a steel substrate, its structure is shown in Fig. 7.1. The materials under study are structurally congruent, since morphologically similar globular dispersed particles (obstacles for dislocations) are arranged in an orderly manner in their matrix determining the range of mobile dislocations. The fundamental difference between the presented materials is expressed in the different composition of the matrices and particles, as well as in the mean free path of the dislocations. The ion-plasma technology of magnetron deposition provided for the layered formation of a TiAlSi coating due to the alternate evaporation of elements from two cathodes of various compositions. However, self-organization processes taking place in systems with Al and Si, the mechanisms of which are still not well understood [11, 12], led to the formation of a modulated structure with a spatially ordered arrangement of phase components in the form of a 3D-composite. A phase analysis of the coating structure was not performed. The scatter of nanoparticle diameters in the coating was 10–77 nm with an average size of 38 nm (assuming equiaxial morphology). The average distance between particles in the composite matrix was

7 The Nucleation and Development of Wear in Nanocomposite …

79

Fig. 7.1 The structure of the coating of the TiAlSi-system in cross-section at various magnifications, scanning electron microscopy: a coating of 9.3 µm thickness with a Ti sublayer (0.23 µm), b modulated structure of a 3D-nanocomposite in the coating of the TiAlSi-system

~50 nm. In calculations, this value was taken as the value of l for the coating. Moreover, the mechanism of interaction of dislocations with reinforcing particles was not regulated. It can be assumed that the interaction of dislocations with obstacles in the TiAlSi coating is carried out according to the principle of “cutting” or “cutting with bending”. However, additional metal-physical studies are needed to refine the data on this issue. In the regard of such uncertainty, the value of coefficient α 1 in √ expression (7.8) for coating the TiAlSi-system was calculated as α1 = l · ρm . TiAlSi coating refers to systems with a mixed ion-metal bond in which dislocations have a fairly high degree of mobility [8]. This determines the appropriateness of applying the developed calculation and analytical model to similar systems and comparing the results of calculations with classical metal systems (such as steel 20Cr13 with a sorbite structure), for which the theory of dislocations is basic. Comparative calculated and experimental data obtained using the calculationanalytical model and testing of samples on a droplet impact stand are shown in Table 7.1. In Table 7.1, the value of m0 was obtained during bench tests and represents the number of droplet impacts required to start the loss of mass of the sample, that is, to start wear. For the impact droplets loads under consideration, the value of m0 characterizes the incubation period of droplet impingement erosion, which includes both the stage of the onset of the defect (cracks, pores, microcrater) and the stage of its development before the start process of mass loss by the sample: m 0 = N3 + Np ,

(7.9)

where N 3 is the number of impacts for the initiation of a crack, N p is the number of impacts for the development of a crack to a critical size and the beginning of chipping of wear particles; it is not possible to differentiate the experimental value of m0 on

80

V. N. Varavka et al.

Table 7.1 Summary data on the calculated and experimental characteristics of the samples Material

Characteristics of material ρ (kg/m3 )

E (GPa)

ν

μ (MPa)

b (10−10 m)

Lattice type

C0 (m/s)

20Cr13 (sorbite)

7670

218

0.30

79

2.5

bcc

1956

3D-composite of TiAlSi-system

3840

148

0.24

60

3.9

fcc

2131

Material

Impact parameters: V 0 = 250 m/s; R0 = 0.55 mm

Structure parameters Mp

α2

D (m−6 )

l (m−6 )

Calculations

20Cr13 (sorbite)

2.9

2.0

100

0.35–0.50

3D-composite of TiAlSi-system

3.06

2.0

9.3

0.05

Experiment

α0

m0

4655

0.280

16,630

16,730

0.445

37,650

N3

N 3 and N p by metal-physical methods; α 0 = N 3 /m0 is the coefficient characterizing the contribution of the nucleation stage to the total value m0 . Without going into details of the calculation algorithm, we note that the model also allows one to obtain the dependences of the number of impacts N 3 , necessary for the initiation of a fatigue defect in the coating, on the speed of impact (collision) V 0 for fixed values of the droplet size R0 . Such dependences for the studied materials (steel 20Cr13 and TiAlSi coating) are presented in Fig. 7.2. A comparison of the graphs in Fig. 7.2 shows that, at any collision velocity V 0 , the TiAlSi coating at the stage of initiation of a fatigue crack provides about a three times

Fig. 7.2 The calculated dependences of the number of impacts N 3 , necessary for the initiation of cracks, on the impact velocity V 0 at R0 = 0.55 mm: a sorbite of steel 20Cr13, b 3D-nanocomposite coating of the TiAlSi-system

7 The Nucleation and Development of Wear in Nanocomposite …

81

higher resistance to drop impact than steel 20Cr13. The experimental data of bench tests show the advantage of the coating by 2.26 times with respect to the parameter m0 (see Table 7.1 and sources [13, 14]). The calculations concern only the nucleation stage, while the experimental parameter m0 includes both the nucleation stage and the stage of development of fatigue defects. Hence, a preliminary conclusion can be made that the effectiveness of protecting the surface of metal products by applying a TiAlSi coating is determined, first of all, by an increase in the duration of the stage of initiation of fatigue defects. The preliminary conclusion is due to the fact that, because of the instrumental difficulties in studying this stage, one has to rely on the calculated data. Usage of TiAlSi-system coatings to increase wear resistance during droplet impact cyclic loading has features not only at the stage of nucleation of defects, but also at the stage of their sustainable development. In the performed study the behavior of the nanocomposite coating, an unusual fact that needs explanation is noteworthy. At the stage of sustainable development of fatigue cracks, they possess a discrete character of development and are presented as a chain of narrow pores (Fig. 7.3a, c). Each such structural element (narrow pore) of a crack in a TiAlSi coating is 0.6–0.8 µm in length. With a dislocation density that ensures material breakage (ρ kr ≈ 1016 m−2 ), the distance between dislocations in a flat pile-up of a crack fragment will be about 10 nm, i.e., a cluster should consist of 60-80 dislocations. A simple calculation shows that the stresses in the head dislocation zone of such an accumulation will exceed the

Fig. 7.3 Successive stages of TiAlSi-system coatings wear under contact cyclic loads, scanning electron microscopy: a, b beginning (a) and development (b) of the growth stage of fatigue cracks, c, d the beginning (c) and development (d) of the coating chipping stage

82

V. N. Varavka et al.

hardness of the coating (22–27 GPa, for functionally-graded or multilayer coatings the mathematical model [15, 16] can be applied). Therefore, chipping of the coating begins already at the stage of their discrete (with pores) development (Fig. 7.3a, c). After the pores merge and the crack faces are formed (Fig. 7.3b), the development of wear does not occur due to further chipping of the coating, but after the crack propagates into the base metal (Fig. 7.3d). Apparently, the main regulator of this process is the adhesion strength of the coating: with slow adhesion, the coating continues to chip, while with high adhesion, cracks deepen.

7.5 Conclusion The results obtained show that there are structural parameters that determine the wear resistance under conditions of contact cyclic loads. Therefore, the limitation of the mobility of dislocations is the main structural principle for the significant increase the wear resistance. The implementation of this principle in coatings allows, among other things, one to increase the contribution of the nucleation stage N 3 of fatigue defects (α 0 = 0.445 in Table 7.1) to the overall level of wear resistance m0 . Structural parameters are the basis for the developed analytical model. The correspondence of the calculation results and experimental data, presented in the article, allows us to recommend the proposed model for the targeted design of wear-resistant materials and coatings. The presented results are based on the concept of the dislocation nature of the considered processes, and they show a good correlation with experiment. It seems to us that they deserve attention, but also it requires a deeper critical analysis, taking into account the fact that, in the general opinion, dislocation interactions in nanostructured materials, which include the TiAlSi-system coating, are significantly limited or even impossible. Acknowledgements This research was performed into framework of financing RFBR grant number 18-08-00546.

References 1. 2. 3. 4. 5. 6.

H. Itoh, N. Okabe, Trans. JSME (A) 59, 2736 (1993) R.H. Richman, ASM Handb. ASM Int. 11, 1013 (2002) M. Ahmad, M. Casey, N. Sürken, Wear 267, 1605 (2009) V.N. Varavka, O.V. Kudryakov, J. Frict. Wear 36(1), 71 (2015) V.N. Varavka, O.V. Kudryakov, J. Frict. Wear 36(2), 153 (2015) O.V. Kudryakov, V.N. Varavka, J. Surf. Invest. X-ray Synchrotron Neutron Tech. 9(1), 203 (2015) 7. V.N. Varavka, O.V. Kudryakov, I.S. Morozkin, I.Yu. Zabiyaka, N.I. Bronnikova, J. Phys: Conf. Ser. 1281, 012085 (2019)

7 The Nucleation and Development of Wear in Nanocomposite …

83

8. H.J. Frost, M.F. Ashby, Deformation-Mechanism Maps. The Plasticity and Creep of Metals and Ceramics (Pergamon, Oxford, New York, Sydney, 1982), 166 p 9. B. de Meester, C. Yin, M. Doner, H. Conrad, in Rate Processes in Plastic Deformation, ed. by J.C.M. Li, A.K. Mukherjee (A.S.M., Metals Park, OH, 1975), 746 p 10. J.P. Hirth, J. Lothe, Theory of Dislocations (McGraw Hill, New York, London, 1968), 791 p 11. A. Cavaleiro, J.T. de Hosson (eds.), Nanostructured Coatings (Springer, New York, 2007), 752 p 12. V.N. Varavka, O.V. Kudryakov, I.Yu. Zabiyaka, N.I. Bronnikova, in Physics, Mechanics of New Materials and Their Applications, ed. by I.A. Parinov, S.-H. Chang, Y.-H. Kim (Nova Science Publishers, New York, 2019), pp. 1–12 13. V.N. Varavka, O.V. Kudryakov, A.V. Ryzhenkov, in Piezoelectrics and Nanomaterials: Fundamentals, Developments and Applications, ed. by I.A. Parinov (Nova Science Publishers, New York, 2015), 105 p 14. O.V. Kudryakov, V.N. Varavka, Inorg. Mater. 51(15), 1508 (2015) 15. A.S. Vasiliev, E.V. Sadyrin, B.I. Mitrin, S.M. Aizikovich, A.L. Nikolaev, Russ. Eng. Res. 38(9), 735 (2018) 16. S.S. Volkov, A.S. Vasiliev, E.V. Sadyrin, in MATEC Web of Conferences. EDP Sciences, vol. 226 (2018), p. 03018

Chapter 8

Mechanical Properties Derived by Spherical Indentation of TiN Coating Deposited by a Method Combining Magnetron Sputtering and Arc Evaporation Evgeniy Sadyrin, Roman Karotkiyan, Nikolay Sushentsov, Sergey Stepanov, Igor Zabiyaka, Evgeniy Kislyakov, and Alexander Litvinenko Abstract The chapter presents a comprehensive analysis of the nanoindentation derived mechanical characteristics (elastic modulus and indentation hardness) of the TiN coating deposited using the method combining magnetron sputtering and arc evaporation on a steel substrate. For the nanoindentation experiments, spherical indenter was used. The results of studies of microstructure, chemical composition, and also measurements of the coating thickness using a focused ion beam on a scanning electron microscope are presented.

8.1 Introduction Deposition of TiN coating has become a widespread solution for improving lifetime and performance of cutting tools [1–3], prosthesis replacements and fixation devices [4, 5], steam turbine blades and power equipment [6, 7], medical instruments [8], drills [9], diffusion barriers [10], and other technological applications. As conventional testing methods (tensile-compression tests and dynamic methods measuring frequency of elastic vibrations of a rod made of a test material) cannot be applied to such small objects as thin films, for the estimation of the mechanical properties of TiN coatings nanoindentation experiments using Berkovich indenter are often conducted [11–13], whereas Vikers [14, 15], cube corner [16] and spherical [17] indenters are not as much widespread. Nevertheless, indentation testing with spherical indenters is a promising technique because of the non-singular nature of the stress fields produced by such indenters, which makes the analysis and testing less E. Sadyrin (B) · R. Karotkiyan · I. Zabiyaka · E. Kislyakov · A. Litvinenko Research and Education Center “Materials”, Don State Technical University, Rostov-on-Don, Russia e-mail: [email protected] N. Sushentsov · S. Stepanov Volga State University of Technology, Yoshkar-Ola, Russia © Springer Nature Switzerland AG 2020 I. A. Parinov et al. (eds.), Advanced Materials, Springer Proceedings in Materials 6, https://doi.org/10.1007/978-3-030-45120-2_8

85

86

E. Sadyrin et al.

complex [18] and more suitable for the mathematical modelling of indentation of the thin films, functionally graded or multilayered coatings [19–26]. Moreover, the extent of damage and plasticity is minimized in the course of the experiment using the spherical indenter as compared to sharp and flat indenters [27–31].

8.1.1 Research Purpose In the present research, the behavior of the mechanical properties of the TiN coating deposited on steel substrate using a method combining magnetron sputtering and arc evaporation was studied using the spherical indentation. The investigation was supplemented by the measurement of the coating thickness, chemical composition and microgeometrical parameters.

8.1.2 Research Scope At this study, we consider the following frameworks of the problem: (i) mechanical properties estimation for the TiN coating; (ii) measurement of the coating thickness using scanning electron microscope (SEM) with the focused ion beam; (iii) evaluation of the chemical composition of the coating using energy by dispersive X-ray spectroscopy on SEM; (iv) determination of the microgeometrical characteristics of the surface using atomic-force microscopy (AFM).

8.2 Research Method 8.2.1 Sample Preparation The coating was deposited using an automated vacuum complex combining the methods of magnetron sputtering and arc evaporation based on the NNV-6 unit. An electric bias potential of 1.5 A was applied to the coating. TiN coating was applied at a total gas mixture pressure of 0.3 Pa. Coating deposition time was 10 min. Arc evaporator current was 100 A. The coating was deposited on a steel 12Cr18N10T substrate (analogue to steel AISI 321).

8 Mechanical Properties Derived by Spherical Indentation …

87

8.2.2 Scanning Electron Microscopy The research of the coating thickness was conducted using SEM Crossbeam 340 (Zeiss, Germany) equipped with the focused ion beam. For surface visualisation we used Everhart-Thornley secondary electron detector with an acceleration voltage of 2 kV, chemical analysis was made using an X-ray microanalyzer Oxford Instruments X-Max 80.

8.2.3 Atomic Force Microscopy The topography of the coating was studied using AFM Nanoeducator (NT-MDT, Russia) equipped with a tungsten probe. The non-contact mode was applied. Probe positioning was performed using the optical microscope integrated to the AFM. The scanning field was 36 × 36 µm2 .

8.2.4 Nanoindentation Test For the study of the mechanical properties of the coating, the nanoindentation device Nanotest 600 Platform 3 (Micro Materials, UK) was used. The series of experiments was conducted in a closed chamber at a constant temperature of 27 ± 0.2 °C. Values of the restored effective Young’s modulus E eff and indentation hardness H for the coating were obtained using the multi-point method, which uses the approach proposed by Oliver and Pharr [32]. During the indentation test, the displacement of spherical indenter h was recorded while the load P was applied. The maximum value of the displacement (attained at Pmax ) was denoted as hmax . Thus, the output of each experiment was a load-displacement curve. Thus, the unloading “branch” of this curve was approximated by the function: P = a(h − h r )m

(8.1)

where a and m were fitting parameters, h r was the residual depth of the imprint, i.e. the amount of displacement of the indenter at which the material ceased to resist during unloading (i.e., the force equals zero). Using this approximation, the derivative of P(h), called indentation stiffness S, was determined at hmax : S=

dP (h max ) dh

(8.2)

88

E. Sadyrin et al.

Then the depth of the deflection out of contact hs was calculated: hs =

Pmax S

(8.3)

where is geometrical constant, for the paraboloid of revolution [33]; = 0.75. After that the contact depth h s was calculated: h c = h max − h s

(8.4)

On the following step the radius of the contact circle was established: a=

2Rh c − h 2c

(8.5)

where R is the radius of the spherical indenter. The reduced Young’s modulus was determined according to the formula: √ S π Er = √ 2β Ac

(8.6)

where Ac was the projected contact area (the projection of the contact surface on a plane orthogonal to the axis of indentation), for the ideal sphere Ac = πa 2 . Indentation hardness was then calculated using the following formula: H=

Pmax Ac

(8.7)

Effective Young’s modulus of the coating was calculated as E eff

√ S π = √ 2 Ac

(8.8)

Finally, we calculated the restored effective Young’s modulus: r E eff = (1 − v 2 )

1 − vi2 1 − Er Ei

−1 (8.9)

The dependence of the restored effective Young’s modulus on the maximum penetration depth of a spherical indenter with a radius of curvature of 20 µm was established. The positions for the indentations were chosen using optical microscope integrated into the nanoindentation device. In each indentation series Pmax was the same, 12 identical indentations were performed with 70 µm column and row offset. However, Pmax increased from series to series, totally from 2.5 to 250 mN.

8 Mechanical Properties Derived by Spherical Indentation …

89

8.3 Results and Discussion 8.3.1 Coating Thickness and Chemical Composition The thickness of the TiN coating was obtained by etching of the surface of the sample with a focused ion beam. The thickness was 1.49 µm, standard deviation was 0.02 µm (the average of six measurements in Fig. 8.1). The energy-dispersive X-ray spectroscopy analysis revealed the chemical composition of the coating by measuring average data on the three specters on the three surface areas (Fig. 8.2). The summary on the data obtained is shown in Table 8.1, which demonstrates a high quality of deposition from the point of view of the chemical composition of the coating.

8.3.2 Microgeometrical Characteristics The average surface roughness Ra was measured by the obtained AFM image (Fig. 8.3) using software (Gwyddion, Czech Metrology Institute, Czech Republic). Due to the irregularities observed on the visualized surface (cavern-shaped artifacts of deposition) we considered measurement of the roughness based on a single profile as not being completely indicative. Thus, average roughness Ra was measured in three directions (horizontal, vertical and diagonal). For each of the directions we constructed five profiles. Following that the average value with the standard deviation was calculated. Maximum height of roughness was also calculated and denoted as Rt . Thus, average Ra by 15 profiles was 198.9 nm,

Fig. 8.1 Etched TiN coating with the focused ion beam

90

E. Sadyrin et al.

Fig. 8.2 Areas selected for the energy-dispersive X-ray spectroscopy

Table 8.1 Chemical composition of the TiN coating

Chemical element

Spectrum 1

Spectrum 2

Spectrum 3

N

47.07

42.73

46.22

O

–

5.42

–

Al

0.12

0.11

0.12

Si

0.10

0.10

0.09

Ti

50.04

49.11

51.08

Cr

0.65

0.54

0.53

Fe

1.78

1.62

1.60

Ni

0.24

0.22

0.26

Cu

–

0.14

0.10

Sum

100.00

100.00

100.00

standard deviation was 53.0 nm, Rt was 1.97 µm. Although the sample possessed a developed surface relief, its Ra value was significantly lower than those reported in literature for different types of steel substrate preparation, ranging from 0.03 to 7.0 µm in the investigation by Steinmann et al. [34]. At the same time, in our previous research [35] we obtained average roughness of 10.7 nm of TiN coating deposited on a mirror polished steel 40Cr (analogue to AISI 5135) using ion plasma deposition.

8 Mechanical Properties Derived by Spherical Indentation …

91

Fig. 8.3 AFM image of the TiN coating under research

8.3.3 Mechanical Properties Figure 8.4 demonstrates some of the load-displacement curves obtained in the nanoindentation series. Table 8.2 summarizes the analysed values for the restored effective Young’s modulus and indentation hardness for different Pmax . The following constants were used during the analysis: E i = 1141 GPa, vi = 0.07 [32] v = 0.3 [36].

Fig. 8.4 Load-displacement curves obtained for the series with Pmax of 20 mN (a), and 140 mN (b)

92

E. Sadyrin et al.

Table 8.2 Mechanical properties estimation for the TiN coating H (GPa)

±

9.53

0.22

0.08

45.52

14.49

0.20

0.10

229.67

60.44

17.19

0.29

0.10

291.51

15

75.60

14.88

0.38

0.12

346.67

20

75.42

12.16

0.37

0.07

433.26

30

87.03

19.53

0.46

0.13

591.43

40

102.66

12.59

0.62

0.09

531.00

50

106.99

13.70

0.68

0.16

616.21

60

118.70

18.21

0.78

0.15

652.25

70

126.25

15.55

0.87

0.17

681.65

80

134.54

21.13

0.95

0.17

706.18

90

132.88

11.97

0.94

0.14

793.84

100

134.77

14.06

0.94

0.15

885.76

120

137.68

11.44

0.99

0.09

999.14

140

146.30

8.86

1.13

0.12

1030.51

160

144.19

11.88

1.18

0.11

1128.78

180

161.14

22.47

1.09

0.25

1453.30

200

155.68

13.77

1.20

0.19

1407.51

250

158.38

19.22

1.39

0.22

1523.17

P (mN)

r (GPa) E eff

2.5

38.67

5 10

±

h max (nm) 101.95

The overall behavior of both restored effective Young’s modulus and indentation hardness demonstrate increase in its values with increase of indentation load and depth (Fig. 8.5). On the interval of maximum depth h max from 344 to 433, both mechanical properties demonstrate stable state and afterwards begin to increase rapidly, presumably because of huge amount of plastic deformation inside the coating and increasing of the influence of the substrate on the effective values. For both mechanical characteristics the next stable segment stretches from 706 to 999 nm on depth. After this segment, the growth of the properties is not pronounced, indicating dominance of the properties of the substrate over the those for the coating. The values obtained partially fit in the ranges obtained earlier for the TiN coating via bulge test in the research by Karimi et al. [37] (160–260 GPa) and are close to the indentation results in the same paper (160–280 GPa), where authors also remarked notable variation of mechanical properties with the increase of indentation depth. The values obtained are significantly lower than those for the reactively and non-reactively magnetron sputtered TiN coatings obtain in the paper of Mayrhofer et al. [38] using computer-controlled microhardness tester. Presumably accurate experimental examination of the mechanical properties of such complex systems as coating-substrate

8 Mechanical Properties Derived by Spherical Indentation …

93

Fig. 8.5 Dependencies of the mechanical characteristics on the maximum indentation depth: a restored effective Young’s modulus, b indentation hardness

(even for the case of a single layered coatings) should be supplemented by the mathematical modelling to obtain the elastic moduli of the coating to avoid influence of the substrate and surface roughness on the results.

8.4 Conclusion The behavior of the mechanical characteristics on the indentation depth was experimentally obtained for the TiN coating deposited on 12Cr18N10T steel substrate by a method combining magnetron sputtering and arc evaporation. The values of the coating thickness and microgeometrical characteristics of the coating were derived using SEM and AFM, respectively, as well as chemical composition of the coating by means of energy-dispersive X-ray spectroscopy. Results demonstrated high

94

E. Sadyrin et al.

dependence of the mechanical properties on the indentation depth. For their further clarification the mathematical modelling of the indentation process of the spherical indenter into inhomogeneous by depth coating is required. Acknowledgements This research was supported by RFBR grants Nos. 18-07-01397-a, 18-0701177-a, and 18-57-00015 Bel_a. Experiments on nanoindentation, SEM and AFM were conducted in the Nanocenter of the Research and Education Center “Materials” (http://nano.donstu.ru/). E. V. Sadyrin was supported by the scholarship of the President of the Russian Federation No. SP3672.2018.1.

References 1. H.E. Rebenne, D.G. Bhat, Surf. Coat. Technol. 63(1–2), 1–13 (1994) 2. H.Y. Li, H.B. He, W.Q. Han, J. Yang, T. Gu, Y.M. Li, S.K. Lyu, Int. J. Precis. Eng. Manuf. 16(4), 781–786 (2015) 3. P. Hedenqvist, M. Olsson, P. Wallén, Å. Kassman, S. Hogmark, S. Jacobson, Surf. Coat. Technol. 41(2), 243–256 (1990) 4. Q. Wang, F. Zhou, C. Wang, M.F. Yuen, M. Wang, T. Qian, M. Matsumoto, J. Yan, Mater. Chem. Phys. 158, 74–81 (2015) 5. A.P. Serro, C. Completo, R. Colaço, F. Dos Santos, C.L. Da Silva, J.M.C. Cabral, H. Araújo, E. Pires, B. Saramago, Surf. Coat. Technol. 203(24), 3701–3707 (2009) 6. M.K. Lee, W.W. Kim, C.K. Rhee, W.J. Lee, Metall. Mater. Trans. A 30(4), 961–968 (1999) 7. V.N. Varavka, O.V. Kudryakov, I.S. Morozkin, I.Y. Zabiyaka, N.I. Bronnikova, J. Phys.: Conf. Ser. 1281(1), 012085 (2019) 8. P.V. Kola, S. Daniels, D.C. Cameron, M.S.J. Hashmi, J. Mater. Process. Technol. 56(1–4), 422–430 (1996) 9. W.D. Sproul, R. Rothstein, Thin Solid Films 126(3–4), 257–263 (1985) 10. S.Q. Wang, I. Raaijmakers, B.J. Burrow, S. Suthar, S. Redkar, K.B. Kim, J. Appl. Phys. 68(10), 5176–5187 (1990) 11. H.C. Barshilia, K.S. Rajam, Bull. Mater. Sci. 27(1), 35–41 (2004) 12. S.J. Bull, Thin Solid Films 688, 137452 (2019) 13. L.W. Ma, J.M. Cairney, M.J. Hoffman, P.R. Munroe, Surf. Coat. Technol. 200(11), 3518–3526 (2006) 14. A.R. Franco Jr., G. Pintaúde, A. Sinatora, C.E. Pinedo, A.P. Tschiptschin, Mater. Res. 7(3), 483–491 (2004) 15. J. Richter, Surf. Coat. Technol. 162(2–3), 119–130 (2003) 16. J.J. Roa, E. Jiménez-Piqué, R. Martínez, G. Ramírez, J.M. Tarragó, R. Rodríguez, L. Llanes, Thin Solid Films 571, 308–315 (2014) 17. M. Kot, W. Rakowski, L. Major, J. Lackner, Mater. Des. 46, 751–757 (2013) 18. K.L. Johnson, Contact Mechanics (Cambridge University Press, Cambridge, 1985) 19. E.V. Sadyrin, A.S. Vasiliev, S.S. Volkov, B.I. Mitrin, S.M. Aizikovich, WIT Trans. Eng. Sci. 122, 209–221 (2019) 20. A.S. Vasiliev, Int. J. Eng. Sci. 142, 230–241 (2019) 21. L.I. Krenev, E.V. Sadyrin, S.M. Aizikovich, T.I. Zubar, in Advanced Materials—Techniques, Physics, Mechanics and Applications. Springer Proceedings in Physics, vol. 193, ed. by I.A. Parinov, S.-H. Chang, M.A. Jani (Springer, Cham, Switzerland, 2017), pp. 397–405 22. I.I. Argatov, F.J. Sabina, Int. J. Eng. Sci. 50(1), 132–143 (2012) 23. S.S. Volkov, A.S. Vasiliev, S.M. Aizikovich, N.M. Seleznev, A.V. Leontieva, PNRPU Mech. Bull. 4, 20–34 (2016)

8 Mechanical Properties Derived by Spherical Indentation …

95

24. T. Chudoba, N. Schwarzer, F. Richter, Surf. Coat. Technol. 127(1), 9–17 (2000) 25. L.I. Krenev, S.S. Volkov, E.V. Sadyrin, S.A. Chizhik, J. Eng. Phys. Thermophys. 91(3), 594–600 (2018) 26. I.I. Kudish, S.S. Volkov, A.S. Vasiliev, S.M. Aizikovich, Math. Mech. Solids 23(7), 1061–1080 (2018) 27. U. Ramamurty, S. Sridhar, A.E. Giannakopoulos, S. Suresh, Acta Mater. 47(8), 2417–2430 (1999) 28. A.S. Vasiliev, S.S. Volkov, A.A. Belov, S.Y. Litvinchuk, S.M. Aizikovich, Int. J. Eng. Sci. 112, 63–75 (2017) 29. A.S. Vasiliev, S.S. Volkov, S.M. Aizikovich, Mater. Phys. Mech. 35(1), 175–180 (2018) 30. A.S. Vasiliev, E.V. Sadyrin, S.S. Volkov, E.A. Kislyakov, I. Sevostianov, in AIP Conference Proceedings, vol. 2188(1) (AIP Publishing, 2019), p. 040017 31. A.S. Vasiliev, E.V. Sadyrin, B.I. Mitrin, S.M. Aizikovich, A.L. Nikolaev, Russ. Eng. Res. 38(9), 735–737 (2018) 32. W.C. Oliver, G.M. Pharr, J. Mater. Res. 7(6), 1564–1583 (1992) 33. I.N. Sneddon, Int. J. Eng. Sci. 3(1), 47–57 (1965) 34. P.A. Steinmann, Y. Tardy, H.E. Hintermann, Thin Solid Films 154(1–2), 333–349 (1987) 35. E.V. Sadyrin, B.I. Mitrin, L.I. Krenev, S.M. Aizikovich, Vestnik Don State Tech. Univ. 15(4), 37–45 (2015) (in Russian) 36. A.J. Perry, Thin Solid Films 193, 463–471 (1990) 37. A. Karimi, O.R. Shojaei, T. Kruml, J.L. Marti, Thin Solid Films 308, 334–339 (1997) 38. P.H. Mayrhofer, F. Kunc, J. Musil, C. Mitterer, Thin Solid Films 415(1–2), 151–159 (2002)

Chapter 9

Studies on Predicting Spring-Back and Verifying the Effects of Temperature, Sheet Thickness and Punch Speed on Forming Force of V-Bending for SS400 Steel Plate Gia-Hai Vuong, Thi-Hong-Minh Nguyen, and Duc-Toan Nguyen Abstract The sheet metal forming process is a basic deformation method in the mechanical field. In particular, bending deformation processing is a universal processing method that is widely used to form sheet metal parts such as the aviation industry, shipbuilding, automotive and so on. During the sheet metal bending process, the spring-back and forming force are very important output parameters that need to be determined to ensure the accuracy and load capacity of machining equipment. To predict the spring-back of V-bending process for SS400 sheet material, various hardening models have been imported into FEM simulation software in order to predict and compare with corresponding experimental results of SS400 sheet material. To simulate spring-back of V-bending, the deformed results of V-shape from the forming simulation in Abaqus/Explicit should be imported into Abaqus/Standard, and then a static analysis will calculate the spring-back of V-bending. The results showed both hardening laws were in good agreement with experimental results due to the thick sheet of material. Moreover, the forming force magnitude of V-bending will vary according to machining conditions, geometric shapes of products, sheet materials, etc. Then, this study verifies the effect of technological and geometric parameters such as elevated temperature, punch speed and sheet thickness to bending force when forming a V-shape of SS400 sheet material and selects the optimum parameters using Taguchi design and ANOVA method.

G.-H. Vuong · T.-H.-M. Nguyen · D.-T. Nguyen (B) School of Mechanical Engineering, Hanoi University of Science and Technology, 1A-Dai Co Viet Street, Hai Ba Trung District, Hanoi City, Viet Nam e-mail: [email protected] G.-H. Vuong Hai Phong University, Hai Phong, Viet Nam © Springer Nature Switzerland AG 2020 I. A. Parinov et al. (eds.), Advanced Materials, Springer Proceedings in Materials 6, https://doi.org/10.1007/978-3-030-45120-2_9

97

98

G.-H. Vuong et al.

9.1 Introduction Nowadays the steel sheet has been widely used in the processing of steel structures and shipbuilding. There are many different machining technologies applied in sheet processing such as cutting, welding, cyclone, bending and so on [1, 2]. Among of the products made from steel sheet, the parts machined by bending technology account for a large of proportion. The spring-back and the bending force of forming processes are often greatly influenced by technology parameters such as the thickness of the sheet, the velocity of bending punch, heating when bending, etc. Determining a suitable set of technology parameters is very necessary, it can help manufacturers save maximum production costs while still bringing high economic efficiency. To determine the influence of these technological parameters, many studies have now applied the Taguchi experimental method [1, 3] and have brought very good results. The Taguchi method experimental is based on empirical statistical analysis through minimizing the cost or experimental process while ensuring a reasonable set of design parameters. The advantage of this method is that many factors are considered at the same time, including confounding factors. The Taguchi method, when combined with other statistical tools, such as variance analysis (ANOVA), becomes a powerful tool for selecting suitable machining parameters. There are various studies have focused on spring-back and bending force calculation [4, 5], however, a universal solution has still not been found [6]. Plastic deformation of the steel sheets requires, at the design stage of manufacturing, taking into account specific properties of the sheet material, i.e., Young’s modulus, yield stress, ratio of yield stress to ultimate tensile stress, and microstructure of the material [7]. In this study, in order to verify the effects of the hardening model on springback prediction, the kinematic and isotropic hardening models were used to simulate corresponding V-bending shapes by using ABAQUS/explicit software. the Taguchi method experimental was used to examine the influence of technological parameters such as elevated temperature, punch velocity and sheet thickness on the force when V-bending of SS400 steel plate. With the main purpose of reducing the bending force, this study uses three levels for each element through the orthogonal array of Taguchi L9 (3 3) [8, 9]. The Minitab software also used to analyze the ANOVA (Analysis of Variance), evaluate the effects of each parameter on the spring-back prediction and select the optimal parameters set the corresponding experiment.

9.2 Material and Hardening Model 9.2.1 Materials The material used in this study is SS400 steel sheet, according to JISG 3101 [10] with a chemical composition as Table 9.1.

9 Studies on Predicting Spring-Back and Verifying the Effects …

99

Table 9.1 Chemical composition of SS400 steel sheet C

Si

Mn

P

S

Cr

0.19–0.21

0.05–0.17

0.4–0.6

0.04

0.05

≤0.3

The tensile test pieces are cut on a wire cutting CNC machine, the tensile specimens were cut from the sheet in parallel to the rolling direction in order to carry out uni-axial tensile tests. After that, the tensile specimens are honed smoothly with a armor paper. The shapes and dimensions of the specimens were prepared in accordance with TCVN 197-85 (197-2000) [11], as shown in Fig. 9.1. The experiment tensile test pieces are carried out at different temperature conditions (room temperature, 300 and 600 °C) on the Hung Ta H-200kN compressor as shown in Fig. 9.2. The system heated tensile test is set as shown in Fig. 9.3.

Fig. 9.1 Tensile test specimen: a dimensions, b wire cutting by CNC and c final shape

100

Fig. 9.2 Tensile and bending test machine

Fig. 9.3 Heat generation testing system

G.-H. Vuong et al.

9 Studies on Predicting Spring-Back and Verifying the Effects …

101

Fig. 9.4 Comparison of Voce’s laws with experimental data at room and elevated temperatures

The experimental results of tensile tests at different temperature conditions are shown in Fig. 9.4.

9.2.2 Hardening Models To identify the parameters of hardening model corresponding with the data after the tensile test by Voce’s hardening law [12], the stress-strain curves as (9.1) were used. By using Excel 2013 software with SOLVER tool based on the method of summing the smallest deviations is easy to find the coefficients of the equation as shown in Table 9.2. The obtained coefficients will be declared in the input material model when performing numerical simulations by Abaqus software: pl )) σ¯ = σY + A(1 − exp(−Bεeq

Table 9.2 Hardening parameters at elevated temperatures determined by fitting curves following Voce’s hardening law

(9.1)

Temperature (°C)

σY

A

B

32

348.7

188.86

28.3293

300

199.3

171.56

3.452

36.89

6.0145

600

72.43

102 Table 9.3 Material attribute parameters for numerical simulation

G.-H. Vuong et al. Parameters

Levels

Temperature (°C)

32; 300; 600

Bending speed (mm/s)

1

Thickness sheet (mm)

6

Poisson’s ratio

0.3

Young’s modulus (MPa)

213,000 (32 °C) 184,410 (300 °C) 107,640 (600 °C)

pl

where A and B are the plastic coefficients σ¯ , εeq , and σ Y are the equivalent stress, equivalent strain, and tension yield stress, respectively. Other material attribute parameters used to simulate the bending force prediction at different conditions are shown in Table 9.3. To describe the hardening model, the Von-Mises yield surfaces that both translates (kinematic) and expanding (isotropic) are defined as [5]: f (σ ) =

1 2 1 ξ j : ξ j = σ¯ iso 2 3

(9.2)

In the pure isotropic hardening case, there is only the size evolution of the yield locus then the back stress α in (9.3) is zero. When isotropic hardening law was used to simulate the uniaxial tension/compression tests then only parameters, σ Y , A, and B in (9.1) are adopted as input data. The corresponding values of σ Y , A, and B at room temperature can be used as 348 MPa, 188.86 MPa and 28.3293, respectively. α=

pl C (1 − e−γ εeq ) γ

(9.3)

To introduce the Bauschinger effect, a kinematic hardening model was implemented to simulate tension/compression test and predict stress-strain curves evolution. To determine the kinematic hardening parameters C and γ in (9.3), back-stress α curve was first obtained by offsetting tensile stress-strain curve data about yield stress value (σ Y ) then fitting method based on the back-stress evolution law (9.3) was utilized to calculate calibration yields C and γ . Based on the back-stress evolution law at room temperature, (9.3) was utilized to calculate calibration yields C as 5350.272 MPa and γ as 17.7.

9 Studies on Predicting Spring-Back and Verifying the Effects …

103

9.3 Experimental and Finite Element Method of V-Bending 9.3.1 Finite Element Model of V-Bending To simulate spring-back and predict forming force when V-bending SS400 plate, the data collected from the test results and the calculation are using Abaqus/Explicit and then imported the deformed results into Abaqus/Standard, 3D Experience® 2016 HF2 (2016 HF2, Dassault Systèmes Simulia Corp., Providence, RI, USA, 2016). The V-bending models have depicted in Fig. 9.5 corresponding to the experimental setup of Fig. 9.2. Specifically, reduced-integration eight-node linear brick elements (C3D8R) are utilized for the blank. The die/tool and clamping parts are assigned as the rigid body. The size of the element for all parts corresponds to approximately 6 × 55 × 160 mm (Thickness × width × length). The boundary conditions in the model are as follows: a die part—ENCASTRE condition; a punch part: vertical movement; a sheet part: symmetrical boundary condition with respect to the center of the sheet. In order to determine to bend forming force through simulation and experiment, the bending part deformation of V-shaped part is done by moving the punch down vertically Y = 18 mm. The corresponding experimental setup for the forming process of SS400 steel sheet bending is shown in Fig. 9.6. Figure 9.7 presents the simulation results after spring-back occurrence for the case bending angle of 90° at room temperature. The error (α) between simulation of isotropic and kinematic hardening law when compared with experimental result can be calculated as α = αSimulation − αExperimental . As shown in Fig. 9.7 with the thick sheet, the kinematic hardening model is in good agreement when comparing with an isotropic hardening model. Therefore, in this chapter, a kinematic hardening model was used to simulate the bending process of V-bending part at elevated temperature conditions. Figure 9.8 depicts the experiment results after V-bending at elevated temperatures. The comparison of the bending force between experiments and corresponding finite

Fig. 9.5 V-bending models

104

G.-H. Vuong et al.

Fig. 9.6 Setup for V-bending experiment at elevated temperatures

Fig. 9.7 V-bending test after spring-back (a) and simulation results spring-back based on isotropic (b) and kinematic (c) hardening models

element results are presented in Table 9.4. The error (P%) between simulation and experimental results can be calculated as PSimulation − PExperimental × 100% P% = PExperimental

(9.4)

From Table 9.4, it is shown that the error value of bending force P (%) between experiment and simulation has the highest value of 3.42%. Therefore it is possible to use numerical simulation methods to predict similar testing process.

9 Studies on Predicting Spring-Back and Verifying the Effects …

105

Fig. 9.8 The experimental result of V-bending tests at: 600 °C (a), 300 °C (b) and room temperature (c)

Table 9.4 Comparison of the bending force values between simulation and experiment

Temperature (°C)

PSim (N)

PEx (N)

P (%)

32

28,022.1

29,014

3.42

300

27,827.2

28,322

1.74

600

20,423.7

19,333

2.89

9.3.2 Taguchi Orthogonal Array The purpose of this study is to verify the effect of the input parameters on the desired output parameters. Therefore, the Taguchi method was chosen to allow the minimum of experiments needed to study the effect of parameters on an output characteristic and quickly adjust the input parameters to optimize the fastest output value. In order to verify the effect of parameters on the forming force prediction P (N) by experiment, three parameters such as the thickness of the sheet (S), temperature (T ) and bending speed (V ) were selected according to Taguchi method. Table 9.5 lists the levels of parameter selection. During the experiment, there are 3 selected levels of each parameter. The L9 orthogonal array will be then used to design the experimental statistical method. At least 9 experiments are needed to test the effect of changing parameters on simulation results. The use of the Taguchi orthogonal algorithm will reduce the number of experimental designs from 27 to 9 experiments. The results of the simulated Taguchi experiments are shown in Table 9.6. The S/N

106

G.-H. Vuong et al.

Table 9.5 Parameters and their level in experiment Factor

Level 1

2

3

Temperature (°C) (T )

Room temperature (32)

300

600

Bending speed (mm/s) (V )

1

1.5

2

Thickness (mm) (S)

6

8

7

Table 9.6 The results according to Taguchi method No.

T

V

S

PEx (N)

S/NEx

1

32

1

6

29,014

−89.252

2

32

1.5

8

66,000

−96.391

3

32

2

7

84,372

−98.524

4

300

1

8

61,619

−95.794

5

300

1.5

7

74,920

−97.492

6

300

2

6

37,970

−91.589

7

600

1

7

37,073

−91.381

8

600

1.5

8

19,333

−85.726

9

600

2

6

32,801

−90.318

noise ratio selected according to smaller is better conditions: S/N = −10log10 (MSD)2

(9.5)

where MSD =

(y12 + y22 + · · · + yn2 ) n

(9.6)

MSD is the mean squared deviation from the target value of the quality characteristic, and y1 , y2 , …, yn , n are the results of experiments and the corresponding number of experiments. The measurement results for 9 test samples according to Taguchi (Fig. 9.9) are given in Table 9.6. Effect of parameters of temperature (°C) (T ), bending speed (mm/s) (V ) and thickness (mm) (S) to forming force is calculated and analyzed for variance (ANOVA) as shown in Table 9.7. The F-ratio test is a statistic tool to verify, which design parameters affect significantly the quality characteristic. It is defined as the ratio of the mean squared deviations to the mean squared error. The analysis of the F-ratio values reveals that the thickness of the sheet (S) is the most significant parameter. The thickness of the plate contributed with 53.17%, followed up by the temperature (T ) contributed with 43.72% and the bending speed (V ) is only 1.95% contribution on forming force.

9 Studies on Predicting Spring-Back and Verifying the Effects …

107

Fig. 9.9 Results of experiments when using the orthogonal array method Taguchi

Table 9.7 ANOM and ANOVA table of data affecting the forming force Factor

Average by level

Sum of squares

Contribution (%)

1

2

3

T

−94.72

−94.96

−89.14*

65.034

43.72

V

−92.14*

−93.2

−93.48

2.908

1.95

S

−88.86*

−95.8

−94.17

79.089

53.17

Err.

–

–

–

1.672

1.16

Sum

–

–

–

148.731

100

* indicates Optimum level

As shown in Fig. 9.10, the optimal parameters for the best forming force are the temperature at level 3 of 600 °C, the thickness of the sheet (t) at level 1 of 6 mm and the bending speed at level 1 of 1 mm/s. Main Effects Plot for Means

Main Effects Plot for SN ratios

Data Means

T

Data Means

S

V

Mean of SN ratios

Mean of Means

70000 60000 50000 40000 30000

32 200 600 1.0

1.5

2.0

6

Fig. 9.10 Main effects plot for means

7

8

-88 -89 -90 -91 -92 -93 -94 -95 -96

T

32 200 600 1.0

S

V

1.5

2.0

Signal-to-noise: Smaller is better

6

7

8

108

G.-H. Vuong et al.

9.4 Conclusion This study has been carried out to set up a system of experimental heated tensile testing of the SS400 steel sheet at elevated temperature conditions. A stress-strain curves at elevated temperatures has been shown that the higher the temperature, the lower the yield strength of the tensile test. The experimental and simulation results are in good agreement so that ABAQUS software could be used in spring-back prediction for V-bending SS400 steel sheet. Taguchi orthogonal array method with technological parameters such as temperature, bending speed, the thickness of workpiece has been conducted to evaluate the influence of input parameters on forming force when Vshaped bending. Experimental results and data analysis (ANOVA) have shown that processing conditions: temperature of 600 °C, bending speed of 1 mm/s and thickness of 6 mm will give the smallest bending force value. Acknowledgements This research is funded by University Project at Hanoi University of Science and Technology under grant number “T2018-TÐ-204”.

References 1. 2. 3. 4. 5. 6. 7. 8. 9. 10. 11. 12.

D.-T. Nguyen, Y.-S. Kim, Proc. IMechE Part B: J. Eng. Manuf. 224(3), 435–445 (2009) T.H. Pham, T.B. Mac, V.C. Tong, T.L. Banh, D.T. Nguyen, Adv. Mech. Eng. 8, 1–11 (2016) Y. Kim, Y. Kwon, J. Nam et al., Metal. Mater. Trans. A 31(1), 93–98 (2000) P.A. Eggertsen, K. Mattiasson, Int. J. Mech. Sci. 51(7), 547–563 (2009) M.L. Garcia-Romeu, J. Ciurana, I. Ferrer, J. Mater. Process. Technol. 191(1–3), 174–177 (2007) R.H. Wagoner, M. Li, Int. J. Plast. 23(3), 345–360 (2007) T. Trzepiecinski, H. Lemu, Metals 7(9), 380 (2017) G. Taguchi, On-line Quality Control During Production (Japan Standard Association, Tokyo, 1981) B.T. Long, N.H. Phan, N. Cuong, N.D. Toan, Adv. Mech. Eng. 8(7) (2016). https://doi.org/10. 1177/1687814016657732 JIS G3101 SS400 Steel Plate Sheet for General Purpose Structural Steels, 86011881 M. M.-T. T. P. 1-2. TCVN 197:2002, ‘TCVN 197’ E. Voce, J. Inst. Met. 74, 537–562 (1948)

Chapter 10

Buckling Analysis of Folded Composite Plate Subjected to In-Plane Loading Condition Bui Van Binh and Le Thuong Hien

Abstract This paper presents some numerical results of buckling analysis of a folded laminate composite plate using finite element method. The effects of fiber orientations, folding angle on buckling loads, and the corresponding mode shapes under in-plane loading condition were considered. Matlab programming using nine nodded rectangular isoparametric plate element with five degree of freedom per node based on Mindlin plate theory was built to solve the problems. A good agreement is found between the results of this technique and other published results available in the literature.

10.1 Introduction Folded laminate composite plates are very useful in engineering. Applications for them have been found almost everywhere in various branches of engineering, such as roofs, sandwich plate cores, cooling towers, marine, aviation, and many other structures. Because of their high strength-to-weight ratio, easy to form, economical, and have much higher load carrying capacities than flat plates, which ensures their popularity and has attracted constant research interest since they were introduced. Bending, free vibration and time displacement response of isotropic folded plates, composite folded plates have been studied in many works [1–13]. In that, folded plates analyzed only the structural members made of isotropic materials or modeled as an equivalent orthotropic plate or special cases of onefold; twofold folded laminate composite plates, or used otherwise method. Buckling analysis is one of the most important studies for structures subjected to in-plane loads. These excellent information are buckling modes, buckling types, and critical buckling loads for the easy replacement with good load bearing capacity (which should be taken into the consideration at design process). In the previous B. Van Binh (B) · L. T. Hien University of Power Electric, Hanoi, Viet Nam e-mail: [email protected] L. T. Hien e-mail: [email protected] © Springer Nature Switzerland AG 2020 I. A. Parinov et al. (eds.), Advanced Materials, Springer Proceedings in Materials 6, https://doi.org/10.1007/978-3-030-45120-2_10

109

110

B. Van Binh and L. T. Hien

works, Singh et al. [12] presented some results of buckling analysis of three dimensional braided composite plates under uniaxial loading using Inverse Hyperbolic Shear Deformation Theory. Liang et al. [13] presented nonlinear buckling analysis of variable stiffness composite plates based on the Koiter-Newton method. In the paper, a four-node quadrilateral element is developed based on the classical laminated plate theory, considering both the symmetrical and unsymmetrical laminates for variable stiffness composite plates. Rasheed and Ahmadi [14] presented a lateral torsional buckling of anisotropic laminated thin-walled simply supported beams subjected to mid-span concentrated load. Barbero et al. [15] presented some results of static and buckling analysis of laminated folded plates by using a mixed isostatic 24 (d.o.f) element. By using finite strip analysis Ovesy et al. [16] presented buckling and free vibration of composite plates with cutout based on two different modeling approaches. In that, the formulations are based on Reddy type higher order plates theory in order to include the transverse shear stresses effect in case of moderately thick plates. In this chapter, we used the nine-nodded isoparametric rectangular flat plate element to build home-made Matlab computer code based on the first-order shear deformation theory to buckling analyze composite folded plates. The effects of geometrical parameters on critical buckling loads and buckling mode shapes under in-plane loading condition were considered.

10.2 Theoretical Formulation 10.2.1 Displacement, Strain and Stress Fields According to the Reissner-Mindlin plate theory, the displacements (u, v, w) are referred to those of the mid-plane (u0 , v0 , w0 ) as u(x, y, z, t) = u 0 (x, y, t) + zθx (x, y, t) v(x, y, z, t) = v0 (x, y, t) + zθ y (x, y, t) w(x, y, z, t) = w0 (x, y, t)

(10.1)

where t is the time; θx and θ y are the bending slopes in the xz- and yz-plane (rotations about the y- and x-axes), respectively. The z-axis is normal to the xy-plane that coincides with the mid-plane of the laminate positive downward and clockwise with x and y. The generalized displacement vector at the mid-plane can thus be defined as T {d} = u 0 , v0 , w0 , θx , θ y

(10.2)

10 Buckling Analysis of Folded Composite Plate Subjected …

111

The strain-displacement relations can be taken as ⎧ ⎫ ⎧ ⎪ ⎪ ⎪ ⎪ ε ⎪ ⎪ ⎪ xx ⎪ ⎪ ⎪ ⎪ ⎪ ⎪ ⎪ ⎪ ⎪ ⎪ ⎪ ⎪ ε yy ⎪ ⎪ ⎪ ⎨ ⎨ ⎬ εzz = ∂u 0 ⎪ ⎪ ∂y + ⎪ γx y ⎪ ⎪ ⎪ ⎪ ⎪ ⎪ ⎪ ⎪ ⎪ ⎪ ⎪ γ ⎪ ⎪ yz ⎪ ⎪ ⎪ ⎪ ⎪ ⎩ ⎭ ⎪ ⎩ γx z

x + z ∂θ ∂x ∂θ y + z ∂y 0

∂u 0 ∂x ∂v0 ∂y

∂v0 x + z ∂θ ∂x ∂y ∂w0 + θy ∂y ∂w0 + θx ∂x

+

∂θ y ∂x

⎫ ⎪ ⎪ ⎪ ⎪ ⎪ ⎪ ⎪ ⎪ ⎬ (10.3)

⎪ ⎪ ⎪ ⎪ ⎪ ⎪ ⎪ ⎪ ⎭

10.2.2 Finite Element Formulations The Hamilton variation principle is used here to derive the laminate equations of motion. The mathematical statement of the Hamilton principle in the absence of damping can be written as [17]

t2

⎛ 1 δ⎝ 2

t1

1 ρ{u} ˙ T {u}dV ˙ − 2

V

−

{ε}T {σ }dV − V

⎞ {u}T { f b }dV ⎠

V

⎞

{u}T { f s }dS + {u}T { f c }⎠dt = 0

(10.4)

S

In which: T =

1 2

ρ{u} ˙ T {u}dV ˙ ; U= V

{u}T { f b }dV +

W = V

1 2

{ε}T {σ }dV ;

(10.5)

V

{u}T { f s }dS + {u}T { f c }

(10.6)

S

where U , T are the potential energy, kinetic energy; W is the work done by externally applied forces. u = [u, v, w]T is the displacement of any generic point (x, y, z) in space. In laminated plate theories, the membrane {N }, bending moment {M} and shear stress {Q} resultants can be obtained by integration of stresses over the laminate thickness. The stress resultants-strain relations can be expressed in the form: ⎧ ⎫ ⎡ ⎨ {N } ⎬ Ai j {M} = ⎣ Bi j ⎩ ⎭ {Q} [0]

⎤⎧ 0 ⎫ Bi j [0] ⎨ ε ⎬ Di j [0] ⎦ {κ} ⎩ 0 ⎭ γ [0] Fi j

(10.7)

112

B. Van Binh and L. T. Hien

where

n Ai j , Bi j , Di j = k=1 h

Fi j =

n k=1

h k

Q i j

k

1, z, z 2 dz i, j = 1, 2, 6

(10.8)

f = 5/6; i, j = 4, 5

(10.9)

k−1

h k Ci j k dz; f h k−1

n is the number of layers, h k−1 , h k are the positions of the top and bottom faces of the kth layer. [Q i j ]k and [Ci j ]k are the reduced stiffness matrices of the kth layer (see [18]). In the present work, nine-nodded isoparametric quadrilateral element with five degrees of freedom per nodes is used. The displacement field of any point on the mid-plane given by: u0 =

9

Ni (ξ ,η) · u i ; v0 =

i=1

θx =

9 i=1

9

Ni (ξ ,η) · vi ; w0 =

i=1

Ni (ξ ,η) · θxi ; θ y =

9

9

Ni (ξ ,η) · wi ;

i=1

Ni (ξ ,η) · θ yi

(10.10)

i=1

where Ni (ξ, η) is the shape function associated with node i in terms of natural coordinates (ξ ,η). The free vibration analysis is used to determine natural frequencies by given equation: [M] − ω2 [K ] = {0}

(10.11)

The eigenvalue type of buckling equation can be expressed as in the following steps by dropping force terms and conceded to {[K ] + λCR [K G ]}{d} = {0}

(10.12)

where, [K G ] is the geometric stiffness matrix; {d} is the displacement increment vector and λCR is the critical mechanical load at which the structure buckles; [M], [K ] are the global mass matrix, stiffness matrix, respectively.

10 Buckling Analysis of Folded Composite Plate Subjected … Fig. 10.1 Two folded composite plate

113

z L/3

L/3

x

y α

L/3

L

Table 10.1 Comparison of first five natural frequencies (Hz) of two folded composite plates for different folding angle, [90°/90°/90°], thickness t = 3 cm Folding angle α 90° 120° 150°

Source

f1

f2

f3

f4

f5

Present

63.3(0.47%)

69.7(0.14%)

150.5(1.44%)

156.7(0.47%)

204.0(1.04%)

[9]

63.6

69.8

152.7

158.3

201.9

Present

59.5(0.34%)

63.1(0.47%)

150.3(1.44%)

153.9(0.71%)

193.5(1.36%)

[9]

59.3

63.4

152.5

155.0

190.9

Present

42.3(0%)

60.7(0.16%)

133.8(1.75%)

144.9(0.48%)

149.9(1.25%)

[9]

42.3

60.8

131.5

145.6

151.8

10.3 Numerical Results 10.3.1 Validation Example In this section, the first five natural frequencies of a cantilever twofolded composite plate studied by Guha Niyogi [9] are recalculated (Fig. 10.1). The layout of the plate is shown in Fig. 10.1 with the dimension L = 1.5 m, total thickness t = 0.03 m, physical and mechanical properties of material: E 1 = 60.7 GPa, E 2 = 24.8 GPa, G12 = G13 = 12.0 GPa, υ 12 = 0.23, ρ = 1300 kg/m3 . Three cases are considered for different folding angle α = 90°, 120°, 150° with fiber orientation [90°/90°/90°]. Comparison first five natural frequencies (Hz) of our results have been compared with published results given by Guha Niyogi [9] and presented in Table 10.1. It is shown that the five natural frequencies are in excellent agreement with the percentage difference of peak values less than 1.75% of each other.

10.3.2 Buckling Analysis of Folded Laminated Plate Consider a twofolds folded composite plate is shown in Fig. 10.2, the material properties shown in Table 10.2, the dimension L = 1.5 m, total thickness t = 0.005 m, folding

114

B. Van Binh and L. T. Hien

L/3

z

z

z x

x

y

L/3 L/3

x

y

L/3

(2)

(1)

L/3

(1)

L/6

(2)

(2)

b - Case 2

a - Case 1

y

L/3

L/6

(1)

L/3

c - Case 3

Fig. 10.2 Geometry of stiffened folded composite plate

Table 10.2 Boron-Epoxy material properties E 1 (GPa)

E 2 (GPa)

G12 (GPa)

G13 (GPa)

υ 12

υ 13

ρ (kg/m3 )

206.9

20.7

5.2

5.2

0.3

0.3

1724

angle α (α = 90°; α = 120°; α = 150°), Lamination schemes: symmetric in-axis configurations [0°/90°/0°/90°/0°]; and off-axis configurations [θ °/−θ °/θ °/−θ °/θ °] are constructed. Three following cases for different stiffener orientations are studied: Case 1. Unstiffened folded composite plate (Fig. 10.2a). Case 2. Three y-stiffeners are attached below the folded plate running along the length of the plates (width of stiffening plate taken equal to 0.1 m and thickness remaining same as the original folded plate) (Fig. 10.2b). Case 3. Two x-stiffeners are attached below the folded plate along transverse direction (Fig. 10.2c) (width of stiffening plate taken equal to 0.1 m and thickness remaining same as the original folded composite plate). The boundary conditions: • At edges y = 0: u = v = w = θ x = θ y = θ z = 0 (without the edges of stiffeners). • At edges (1) and (2): u = v = 0 (without the edges of stiffeners). Loading condition The plate subjected to a uniform knife-edge loading q = 5 N/m along its edge of y = L towards the negative direction of the y-axis while the bottom edge is constrained to move. In the sub-sections below, the eigenvalue buckling analysis calculates a scaling factor for the existing loads, if a unit load is applied, the scaling factor yields the buckling load. 2 The non-dimensional buckling load parameters is as follows: λ∗CR = λECR2 ta3 . 10.3.2.1

Effect of Stiffeners

To observe the effects of stiffener on critical load, the plates having laminate schemes [45°/−45°/45°/−45°/45°] and [0°/90°/0°/90°/0°] (cross-ply) are considered. The

10 Buckling Analysis of Folded Composite Plate Subjected …

115

results presented in Figs. 10.3 10.4, 10.5 and 10.6 have been compared for different cases. We denote cases of the plate with and without stiffeners as follow: (i) Case of the plate without stiffener is WOS (Case 1) (ii) Case of the plate with y-stiffeners is WYS (Case 2) (iii) Case of the plate with x-stiffeners is WXS (Case 3).

Fig. 10.3 Effects of stiffeners on buckling load of flat composite plate [45°/−45°/45°/−45°/45°]

Non-dimensional buckling load

For flat plate: folding angle α = 180° and laminate schemes [45°/−45°/45°/−45°/45°] (Fig. 10.3). For flat plate: folding angle α = 180° and laminate schemes [0°/90°/0°/90°/0°] (Fig. 10.4). For folded plate: folding angle α = 120° and laminate schemes [45°/−45°/45°/−45°/45°] (Fig. 10.5). 20

WOS

18 16

WYS

14

WXS

12 10 8 6 4 2 0

1

2

3

4

5

6

7

8

9

10

8

9

10

Fig. 10.4 Effects of stiffeners on buckling load of flat composite plate [90°/0°/90°/0°/90°]

Non-dimensional buckling load

Buckling mode

35

WOS

30

WYS

25

WXS

20 15 10 5 0

1

2

3

4

5

6

7

Buckling mode

B. Van Binh and L. T. Hien

Fig. 10.5 Effects of stiffeners on buckling load of folded composite plate [45°/−45°/45°/−45°/45°]

Non-dimensional buckling load

116 60

WOS

50

WYS WXS

40 30 20 10 0 1

2

3

4

5

6

7

8

9

10

8

9

10

Fig. 10.6 Effects of stiffeners on buckling load of folded composite plate [90°/0°/90°/0°/90°]

Non-dimensional buckling load

Buckling mode

90

WOS WYS WXS

80 70 60 50 40 30 20 10 0

1

2

3

4

5

6

7

Buckling mode

For folded plate: folding angle α = 120° and laminate schemes [0°/90°/0°/90°/0°] (Fig. 10.6). It is observed that case of WYS is the best process of reinforcement for buckling with the compressive loading and the case of WYS is the worst process of reinforcement. For both of laminate schemes: buckling load of the plate descended form case of WYS to case of WXS and case of WOS. Figures 10.7 and 10.8 plotted buckling modes of flat plate Case 1 and folded plate Case 3, respectively.

10.3.2.2

Effect of Fibre Orientations

In this subsection, we calculated the buckling load of the plates for various ply orientations of θ = 15°, 30°, 45°, 60°, 75° and [0°/90°/0°/90°/0°]. The lamination

10 Buckling Analysis of Folded Composite Plate Subjected …

1.5

1

1

1.5

0

1

1

0.5 0

0.5

0.6 0.4 0.2 0 -0.2 -0.4 -0.6

0.6 0.4 0.2 0 -0.2 -0.4 -0.6

0.6 0.4 0.2 0 -0.2 -0.4 -0.6

0.8 0.6 0.4 0.2 0 -0.2 -0.4

117

-0.5

0

Mode 1

1.5

1

1

0.5 0

0.5

1.5

-0.5

0

0.5 0

0.5

-0.5

0

Mode 3

Mode 2

1

1

0.5 0

0.5

-0.5

Mode 4

Fig. 10.7 Buckling mode of flat plate Case 1, folding angle α = 180°, [45°/−45°/45°/−45°/45°]

0.5

0.5

0.5

0.5

0

0

0

0

-0.5

-0.5

-0.5

-0.5

1.5

1

1

0.5 0

0.5 0

-0.5

Mode 1

1.5

1

1

0.5 0

0.5 0

-0.5

Mode 2

1.5

1

1

0.5 0.5

0 0

-0.5

Mode 3

1.5

1

1

0.5 0

0.5 0

-0.5

Mode 4

Fig. 10.8 Buckling mode of folded plate Case 3, folding angle α = 150°, [90°/0°/90°/0°/90°]

schemes are [θ °/−θ °/θ °/−θ °/θ °] and laminate scheme is [0°/90°/0°/90°/0°]. The buckling load, plotted in Fig. 10.3, shows the influence of ply orientation for different cases. We denote: θ =150

θ =450

θ =750

θ =300

θ =600

Cross-ply

For folded plate of Case 2: folding angle α = 90° and laminate schemes [0°/90°/0°/90°/0°] (cross-ply) (Fig. 10.9). For folded plate of Case 2: folding angle α = 120° and laminate schemes [0°/90°/0°/90°/0°] (cross-ply) (Fig. 10.10). For folded plate of Case 2: folding angle α = 150° and laminate schemes [0°/90°/0°/90°/0°] (cross-ply) (Fig. 10.11). In this numerical analysis, buckling loads of three cases (Case 1; Case 2 and Case 3) were determined but only the effects of stiffeners for Case 2 were plotted in Figs. 10.9, 10.10 and 10.11. From the results, we obtained that buckling load of cross-ply plate were significantly higher than others fibre orientational schemes. Four buckling mode of folding angle α = 150° of Case 2 (three y-stiffeners) were plotted in Fig. 10.12.

118

B. Van Binh and L. T. Hien 80

Non-dimensional buckling load

Fig. 10.9 Effects of stiffeners on buckling load for folding angle α = 90°

70 60 50 40 30 20

1

2

3

4

5

6

7

8

9

10

7

8

9

10

Buckling mode

80

Non-dimensional buckling load

Fig. 10.10 Effects of stiffeners on buckling load for folding angle α = 120°

70 60 50 40 30 20

1

2

3

4

5

6

Buckling mode

10.3.2.3

Effect of Folding Angles

In this subsection, the effects of folding angles on buckling load have been investigated. The plates having lamination schemes of [45°/−45°/45°/−45°/45°] and [90°/0°/90°/0°/90°] are taken to these analyses. The present results have been compared in Fig. 10.13a, b for four cases (with flat plate α = 180°). In this numerical analysis, buckling loads of three cases (Case 1, Case 2 and Case 3) were also determined but only the effects of folding angles for Case 2 were plotted in Fig. 10.13a, b. From the calculated results, we found that the buckling load of flat plates are significantly lower than the others cases of folding angles.

10 Buckling Analysis of Folded Composite Plate Subjected …

119

Non-dimentional buckling load

80 70 60 50 40 30 20

1

2

3

4

5

6

7

8

9

10

Buckling mode

Fig. 10.11 Effects of stiffeners on buckling load for folding angle α = 150°

a 0.5

0.5

0.5

0

0

-0.5

-0.5

1.5 1 0.5 0

-0.5

0

0.5

1

0.5

0

0

-0.5

-0.5

1.5

1.5 1 0.5 0

Mode 1

0

-0.5

0.5

1

1 0.5 0

-0.5

0

0.5

1

1.5 1 0.5 0

Mode 3

Mode 2

-0.5

0

0.5

1

Mode 4

b 0.5

0.5

0.5

0

0

0

0

-0.5

0.5

-0.5

-0.5

1.5 1 0.5 0

-0.5

0

Mode 1

0.5

1

1.5 1 0.5 0

-0.5

0

Mode 2

0.5

1

0.5

1.5 1 0.5 0

-0.5

0

Mode 3

0.5

1

1.5 1 0.5 0

-0.5

0

0.5

1

Mode 4

Fig. 10.12 a Buckling mode of case 2, folding angle α = 150°, [45°/−45°/45°/−45°/45°]. b Buckling mode of Case 2, folding angle α = 150°, [0°/90°/0°/90°/0°]

10.4 Numerical Results A finite element analysis was conducted to predict the buckling load of un-stiffened and stiffened folded composite plate for three types of stiffeners. The transverse shear deformation, the rotary inertia of plate and stiffeners are considered in the present method to see that is the more advanced in presented model. The model is used to obtain the buckling responses for folded laminate plates with different folding

B. Van Binh and L. T. Hien

Fig. 10.13 a Effects of folding angles on buckling load for case 2, [45°/−45°/45°/−45°/45°]. b Effects of folding angles on buckling load for Case 2, [0°/90°/0°/90°/0°]

a

60

Non-dimentional buckling load

120

50 40

α=900 α=1200 α=1500 α=1800 (flat plate)

30 20 10 0

1

2

3

4

5

6

7

8

9

10

7

8

9

10

b

80

Non-dimentinal buckling mode

Buckling mode

70 60

α=900 α=1200 α=1500 α=1800 (flat plate)

50 40 30 20 10

1

2

3

4

5

6

Buckling mode

angles, stiffeners orientations under compressive loading condition. The results of this study will serve as a benchmark for future research for designing folded composite structures and sandwich structures made of composite materials, as it was extremely quick and reliable in producing design results.

References 1. 2. 3. 4. 5. 6.

J.E. Goldberg, H.L. Leve, Int. Assoc. Bridg. Struct. Eng. 17, 58–86 (1957) D. Yitzhaki, M. Reiss, J. Struct. Div. ASCE 88, 107–142 (1962) Y.K. Cheung, Proc. ASCE 94, 1365–1378 (1968) Y.K. Cheung, J. Struct. Div. ASCE 12, 2963–2979 (1969) S. Maleki, Comput. Struct. 40, 527–538 (1991) Y. Lavy, P. Bar-Yoseph, G. Rosenhouse, Comput. Struct. 42, 433–446 (1992)

10 Buckling Analysis of Folded Composite Plate Subjected … 7. 8. 9. 10. 11. 12. 13. 14. 15. 16. 17. 18.

121

T. Irie, G. Yamada, Y. Kobayashi, J. Acoust. Soc. Am. 76(6), 1743–1748 (1984) B. Perry, P. Bar-Yoseph, G. Rosenhouse, Comput. Struct. 44, 177–183 (1992) S. Pal, A. Guha Niyogi, J. Reinf. Plast. Compos. 27, 692–710 (2008) S. Haldar, A.H. Sheikh, Finite Elem. Anal. Des. 42, 208–226 (2005) T.I. Thinh, B. Van Binh, T.M. Tu, Vietnam. J. Mech., VAST 34(3) (2012) D.B. Singh, B.N. Singh, Compos. Struct. 157, 360–365 (2016) K. Liang, Q. Sun, Y. Zhang, Compos. Struct. 206, 681–692 (2018) H. Ahmadi, H.A. Rasheed, Compos. Struct. 185, 348–361 (2018) E.J. Barbero, A. Madeo, G. Zagari, R. Zinno, G. Zucco, Compos. Struct. 116, 223–234 (2014) H.R. Ovesy, J. Fazilati, Compos. Struct. 94, 1250–1258 (2012) K.-J. Bathe, Finite Element Procedures (Prentice Hall, Upper Saddle River, NJ 1996) T.I. Thinh, Composite materials (Viet Nam Education Publishing House, Hanoi 1994) (in Vietnamese)

Chapter 11

The Effect of Strain Rate on Chip Formation and Cutting Process During High-Speed Cutting of A6061 Aluminum Alloy Pham Thi Hoa, Banh Tien Long, Nguyen Duc Toan, Doan Thi Huong, and Pham Duc Thanh Abstract Nowadays, increasing productivity and quality of machining become major challenges of the metal cutting process. Due to the complexity of the chip formation process at high cutting speeds, the finite element method (FEM) has been widely used as an approximate solution. In the metal cutting, the chip formation is essentially concerned with the large strains and the high strain rates. In this chapter, two numerical models with and without strain rate effects are proposed. An appropriate model is then verified by comparing the simulated cutting forces under varying cutting parameters. The simulation model with strain rate is consistent with the experimental value, whereas the model without strain rate underestimates the cutting forces. The strain rate also modifies the cutting forces owing to the stresses that occurred at cutting regions and significantly affected by the strain rate.

11.1 Introduction Nowadays, along with the development of machining industry, metal cutting is one of the key techniques. Research on chip formation problems during cutting helps to improve the surface quality of the workpiece and reduce machining time. Strain rate influences the chip formation and other factors during cutting. Therefore, research on strain rate of cutting has attracted significant attentions. Sun et al. [1] studied the strain rate in the primary shear zone. They showed that there is a distinct peak shift in the shear strain rate distribution during saw-tooth chip formation, while there is a stable peak position of the strain rate distribution during continuous chip formation. P. T. Hoa (B) · D. T. Huong Hung Yen University of Technology and Education, Hung Yen, Viet Nam e-mail: [email protected] B. T. Long · N. D. Toan School of Mechanical Engineering, Hanoi University of Science and Technology, Hanoi, Viet Nam P. D. Thanh Hanoi University of Transport and Communications, Hanoi, Viet Nam © Springer Nature Switzerland AG 2020 I. A. Parinov et al. (eds.), Advanced Materials, Springer Proceedings in Materials 6, https://doi.org/10.1007/978-3-030-45120-2_11

123

124

P. T. Hoa et al.

Moreover, the primary shear zone thickness during saw-tooth chip formation is more localized and smaller than that during continuous chip formation during cutting of AISI 1045 and AA6082-T6 alloys. Jaspers and Dautzenberg [2] studied the strain, strain rate, and temperature during chip generation. They proposed a method to determine the strain and strain rate from which to identify the chip stock. List et al. [3] determined the strain, strain rate in the high shear speed area. The authors compared the deformation and strain rate between experimental and simulation models, which showed a good correlation. Some studies highlighted the strain and the rate of strain occurring during shearing such as in [4, 5]. In this study, the effect of strain on the cutting process of aluminum alloy A6061 is simulated. Simulation results of stress and strain with strain rates and without strain rates effect are compared. From the simulated and measured shear forces, it is found that at high-speed, the strain rate significantly affects the performance of the cutting process.

11.2 Mechanical Properties of A6061 Aluminum Alloy In this study, the workpiece material of A6061 aluminum alloy is used. This material is widely used in industry because of its excellent properties regarding wear resistance, weldability, and strength. Major chemical compositions and physical properties of A6061 aluminum alloy are shown in Tables 11.1 and 11.2, respectively. Figure 11.1 shows the tensile stress-strain curve of A6061 aluminum alloy. Table 11.1 Chemical composition of A6061 aluminum alloy (%wt.) Si

Fe

Cu

Mn

Mg

Cr

Zn

Ti

Al

0.4–0.8

0.7

0.15–0.4

0.15

0.8–1.2

0.04–0.4

0.25

0.15

Remainder

Table 11.2 Physical properties of A6061 aluminum alloy Physical properties

Value

Physical properties

Value

Melt temperature (°C)

582–652

Elastic modulus (GPa)

68.9

Thermal conductivity coefficient (W/m K)

167

Resistance ( m)

3.99 × 10−6

Specific heat capacity (J/g °C)

0.896

Fracture strength (MPa)

96.5

Density

(kg/m3 )

Hardness (HB)

2.7

Tensile strength (MPa)

276

95

Poisson’s ratio

0.33

11 The Effect of Strain Rate on Chip Formation and Cutting Process …

125

Fig. 11.1 Tensile stress-strain curve of A6061 aluminum alloy

11.3 Influence of Strain Rate on Stress in High-Speed Cutting The strain rate can affect the chip formation and stress during cutting. During highspeed milling alloy aluminum, the yield stress decreases with the increase of strain rate. This is because the aluminum alloy is capable of average deformation speed. To accurately simulate the cutting process in high-speed milling of A6061 aluminum alloy, this study considers the effect of deformation speed and includes the properties of materials in the simulation model. When the strain rate is higher than 103 s−1 , the shear stress increases rapidly as shown in Fig. 11.2 [6–8]. Therefore, the stress will be increased quickly if the strain rate exceeds 103 s−1 . Fig. 11.2 Relationship between stress and strain rate for A6061 aluminum alloy [7, 8]

126

P. T. Hoa et al.

11.4 Simulation Model This study employs the Bao–Wierzbicki (B-W) material fracture model, which indicates that the fracture occurs when the accumulated plastic strain reaches a critical value. The accumulated equivalent plastic strain or damage parameter based on the B-W model is given by [6] ε f D= 0

σ σH H dε = εf σ σ av

(11.1)

where σσH av is the average stress triaxiality. The equivalent strain to fracture can be described by the curve-fit formulae given as follows [6] 1 −0.46 1 σH σH + =− ÷0 ε f = 0.1225 for σ 3 σ 3 2 σ σH σH H + 0.21 for = 0 ÷ 0.4 ε f = 0.19 − 0.18 σ σ σ σ H −1 σH = 0.4 ÷ 0.95 ε f = 0.15 for σ σ

(11.2) (11.3) (11.4)

The variation of the equivalent strain to fracture as a function of average stress triaxiality is shown in Fig. 11.3, which is determined by using (11.2)–(11.4) for A6061 aluminum alloy. The commercial software Abaqus/Explicit 6.14.1 is employed for simulation of chip formation and determination of cutting force for A6061 aluminum alloy. Fig. 11.3 Fracture curve of A6061 aluminum alloy based on the B-W model

11 The Effect of Strain Rate on Chip Formation and Cutting Process …

127

Fig. 11.4 Finite element model of cutting problem

Figure 11.4 shows a two-dimensional (2D) finite element (FE) model for the cutting problem. The model consists of four geometrical parts as shown in Fig. 11.4. The uncut chip portion is represented by part 1, which is coupled to the workpiece support (part 3) by the passage zone of tool tip (part 2). Part 3 plays the role of a sacrificial layer, which directly interacts with the cutting tool. This layer is modeled by a mesh of three elements with a total thickness larger than the cutting-edge radius. A major part of the chip is formulated from the elements in the uncut chip portion. Another part arises from the elements in the sacrificial layer if they are not completely damaged. The remaining elements in the damaged zone, which are completely damaged, will be removed.

11.5 Results and Discussion 11.5.1 Influence of Strain Rate on Stress and Strain During Chip Formation The effect of strain rate on stress and strain generated is simulated. Simulation was performed under the cutting speed of 1000 m/min, and the cutting depth of 1.5 mm. The stress-strain results for two cases: with and without strain rate, are shown in Fig. 11.5. The simulated stresses without and with strain rate are 565 and 838 MPa, respectively, as shown in Fig. 11.5. Hence, the stress with strain rate is about 33.9% higher than that without strain rate. The equivalent plastic strains (EPSs) with and without strain rate show the similar behavior as the stress. Specifically, EPSs determined in the absence of the influence of the strain rate is 1.87 MPa, compared to

128

P. T. Hoa et al.

Fig. 11.5 Simulated stress and strain during milling of A6061 aluminum alloy (V = 1256 m/min, t = 0.5 mm): a without strain rate; b with strain rate

1.94 MPa for the case with the influence of the strain rate. Thus, EPSs with strain rate increases by 3.7% compared to the case without strain rate. On the other hand, the shape of the chip also varies with each case as shown in Fig. 11.5. In the case with strain rate (see Fig. 11.5a), the formed chip has a higher level of curved shape than that of the chip formed in Fig. 11.5b.

11.5.2 Effect of Strain Rate on Cutting Force Figure 11.6 shows the progress of simulated cutting forces during milling at a cutting speed of 1256 m/min and a cutting depth of 1.5 mm. The cutting force by the model with strain rate is higher than that of the model without strain rate (see Fig. 11.6). To further assessing the effect of strain rate on the cutting force, experimental and simulated cutting forces at cutting speeds of 1000, 1256, 1512 m/min, and cutting

11 The Effect of Strain Rate on Chip Formation and Cutting Process …

129

Fig. 11.6 Simulated cutting forces during milling of A6061 aluminum with and without strain rate effect (V = 100 m/min, t = 1.5 mm)

Fig. 11.7 Measured and simulated cutting force with and without strain rate effect

Table 11.3 Comparison of cutting forces with and without strain rate F(N)

% F

V (m/min)

1000

1256

1512

Experiment (F E )

142.83

128.42

121.26

With strain rate (F S )

127.89

117.74

110.25

Without strain rate (F NS)

80.19

74.81

70.48

With strain rate (F S )

10.39

8.31

9.07

Without strain rate (F NS)

43.85

41.17

41.87

depth of 1.5 mm are compared as shown in Fig. 11.7. From Fig. 11.7, the deviations of simulated and measured cutting forces are summarized in Table 11.3. The results showed that at the cutting speed 1256 m/min, the maximum deviation of the measured (F E ) and the simulated forces with strain rate (F S ) is 10.39%; compared to a deviation

130

P. T. Hoa et al.

of about 43.85% without strain rate. The smallest error of cutting force with strain rate is 8.31% at the cutting speed of 1512 m/min; compared to about 41.17% without strain rate at the cutting speed of 1000 m/min.

11.6 Conclusion When cutting is performed at high speed, the strain rate significantly influences the chip formation and cutting force in milling of A6061 aluminum alloy. Following conclusions are obtained from this study: (i) the simulated stresses and EPSs during chip formation with strain rate are higher than those without strain rate; (ii) the comparisons of measured and simulated the cutting force with and without strain rate show that it is of significance importance to take into account the strain rate in the finite element model, especially for high-speed cutting condition.

References 1. C.Z. Duan, M.J. Wang, J.Z. Pang, G.H. Li, J. Mater. Process. Technol. 178, 274–277 (2006) 2. S.P.F.C. Jaspers, J.H. Dautzenberg, J. Mater. Process. Technol. 121(1), 123–135 (2002) 3. G. List, G. Sutter, X.F. Bi, A. Molinari, A. Bouthiche, J. Mater. Process. Technol. 213, 693–699 (2013) 4. B. Shi, J. Manuf. Sci. Eng. 132(5) (2013) 5. A. Hor, F. Morel, J.-L. Lebrun, Int. J. Mech. Sci. 67, 108–122 (2013) 6. Y. Bao, T. Wierzbicki, Int. J. Mech. Sci. 46(1), 81–98 (2004) 7. D.R. Lesuer, G.J. Kay, M.M. LeBlanc, in Third Biennial Tri-Laboratory Engineering Conference on Modeling and Simulation, pp. 3–5 (2001) 8. A. Manes, L. Peroni, M. Scapin, M. Giglio, Procedia Eng. 10, 3477–3482 (2011)

Chapter 12

Prediction of Temperature Distribution in PCBN Cutting Tools in Orthogonal Turning 9XC Hardened Alloy Steels Dung Thi Quoc Nguyen

Abstract In this research, a numerical model of temperature distribution in PCBN cutting tools in orthogonal turning 9XC hardened alloy steel was developed. The heat sources generated at cutting zones were determined by theoretical calculations. The temperature distribution in the cutting tool, chip, and workpiece was found by using the heat transfer equations combined with finite element analysis. The isotherms obtained from the numerical model are high compatible with those obtained from experimental measurements. The results indicate that the numerical model has satisfied the requirements and can be applied to similar machining conditions.

12.1 Introduction In metal cutting, cutting temperature plays an important role in determining machining efficiency. The cutting temperature influences the mechanical properties of the workpiece and cutting tool, thus affecting the cutting forces and the tool life, integrity, and quality of the machined surface. There are several methods for determining cutting temperature such as thermoelectricity, thermocouple, infrared radiation, mapping the change in structure and hardness of materials depended on temperature, determining the color of hardened steels, coating the materials working as the temperature indicators on the examined surface, etc., but all methods have not yielded accurate results since it is not directly accessible to the heat-generating area. The development of coating technology allowed the use of thermistor sensors to measure the temperature at the tool-chip interface. However, all the tested coating layers were peeled off at the beginning of the cutting process and after that, the sensor was damaged by chips [1]. Thus far, no simple method with high accuracy has been identified to measure temperatures in the cutting zone, even during orthogonal cutting. This is especially difficult for the PCBN cutting tool since the material has very high hardness and it does not D. T. Q. Nguyen (B) Faculty International Training, Thai Nguyen University of Technology, Thai Nguyen, Viet Nam e-mail: [email protected] © Springer Nature Switzerland AG 2020 I. A. Parinov et al. (eds.), Advanced Materials, Springer Proceedings in Materials 6, https://doi.org/10.1007/978-3-030-45120-2_12

131

132

D. T. Q. Nguyen

conduct electricity, so the use of the thermistor method and the machining the holes for placing thermocouple has encountered with difficulties. In fact, only a few studies have been accomplished to measure the temperature of the PCBN cutting tools using thermocouples or temperature indicators or measuring infrared radiation [2–4]. Therefore, the analytical models predicting the temperature in PCBN cutting tools received much interest from researchers [3, 5–7]. In this study, a numerical model for determing temperature distribution in the PCBN cutting tool when orthogonal turning 9XC hardened alloy steels has been developed based on the heat transfer model and finite element analysis.

12.2 Temperature Calculation 12.2.1 Thermal Model The steady, two-dimensional heat transfer equation during orthogonal cutting can be written as [8]

∂T ∂T ρc u x + uy ∂x ∂y

∂2T ∂2T −k + ∂x2 ∂ y2

+ q(x, y) = 0.

(1)

where ρ, c, k, T, q are the density, specific heat, thermal conductivity, temperature, and heat generation rate per unit volume, respectively; x, y are the coordinates, and ux and uy are the velocity components in the x and y directions. This equation must be solved in the region illustrated in Fig. 12.1 [9], which represents the boundary conditions that the equation must satisfy. Solving (1) can be done numerically using the finite element method [10]. The solution yields the temperature distribution over the solution region.

12.2.2 Heat Generation Rate in the Primary Deformation Zone q1 The rate of plastic deformation heat generated per unit area in the primary deformation zone q1 is calculated from the shear stress τAB and sliding velocity Vs in the shear plane [11]. For simplicity, assume that the velocity is constant over the length of the shear plane [12]. The equation of q1 can be written as q1 = τAB Vs =

(Fc cos φ − Ft sin φ) sin φ cos α V, wt cos(φ − α)

(2)

where Fc and Ft are the tangential and axial components of the cutting force, respectively; w and t are the width and thickness of the chip corresponding to the depth of

12 Prediction of Temperature Distribution in PCBN Cutting Tools …

133

Fig. 12.1 Boundary conditions for the thermal model [9]

cut a and the feed rate d; φ and α are the shear and the rake angles,V is the cutting speed.

12.2.3 Heat Generation Rate in the Secondary Plastic Zone q2 The heat generation rate on the secondary plastic region q2 includes two components: q2 = q f + q p where q f is the heat generated due to the friction between the chip and the rake face of the cutting tool and q p is the heat generated due to the plastic deformation of the chip in the secondary zone.

12.2.3.1

Heat Generation Rate Due to Friction Between the Chip and the Rake Face qf

The rate of frictional heat generated per unit area at the tool-chip interface q f is calculated from the shear stress τ(x) and sliding velocity V(x) of the chip. Both of them vary along the tool-chip interface as shown in Fig. 12.2 [12–14]. With τs is the average shear stress, l is the total contact length, l1 is the length of the adhesive part, over which the shear stress is constant, Vc is the chip velocity. Assume that l ≈ 2l1 and the shear stress varies linearly on the length of contact l1 , the equation of q f is given by [9]:

134

D. T. Q. Nguyen

Fig. 12.2 Variation of velocity, stress and friction heat on tool-chip interface [9]

qf =

12.2.3.2

1 + 4xl 0 ≤ x ≤ l/2 l/2 ≤ x ≤ l 2τs Vc 1 − xl τs Vc 3

(3)

Heat Generation Rate in the Secondary Plastic Zone qp

The rate of plastic heat generated per unit volume in the secondary zone is given by [15] q p = τsec γ˙sec =

(Fc sin α + Ft cos α)V sin φ . lwδt2 cos(φ − α)

(4)

where τsec is the shear stress at the tool-chip interface, which is assumed to be constant along the interface, γ˙sec is the strain rate in the secondary plastic area, which varies linearly from constant value along the tool-chip interface to zero along the boundary HM in Fig. 12.1; l and w are the contact length, and contact width of the tool-chip interface, respectively; δt2 is the maximum thickness of the secondary plastic zone: δt2 = 0.05 mm or 1/8 for the range of shear speeds considered (Fig. 12.1) [8, 15].

12.2.3.3

Equivalent Shear Stress in the Secondary Plastic Zone τs

For simplicity, consider the heat generated by plastic deformation and friction in the secondary zone is equivalent to the heat generated due to the equivalent friction in as the variable equivalent stress and τs is constant the tool-chip interface. Denote τ(x) equivalent stress, τs can be found by the law of conservation of energy as l/2 Q2 = 0

l 4x τs Vc x 1+ wdx + 2τs Vc 1 − wdx = FF Vc . 3 l l l/2

(5)

12 Prediction of Temperature Distribution in PCBN Cutting Tools …

τs =

135

12FF FF 1 1 = . 7wl wl 3 + 4

(6)

Substituting τ s into (3) to find the rate of heat generated in secondary zone q2 (x).

12.2.4 Heat-Generation Rate at the Tool Flank-Work Interface qw The flank wear land is considered flat and parallel to the finished surface. The stress distributions are assumed uniform along with the interface. The rate of heat generated over the flank wear land is constant and given by [13]: q3 = K c

V FC 1 = 0.0671V Fc , tw t1 w

(7)

where K c is the experimentally cutting force coefficient.

12.2.5 Experimental Parameters It is necessary to carry out the experiments to estimate the input parameters for solving (1). The experiments were conducted on HOWA STRONG 860 (Japan) lathe at the machining conditions: cutting speed of v = 119.3 m/min; depth of cut a = 3 mm, and the feed rate d = 0.06 mm/rev. The PCBN triangular inserts were used with the geometric parameters as shown in Table 12.1. The cutting forces were measured by a three-component force dynamometer (Kistler 9257BA) after machining the length of 50 mm which is equivalent to 2.19 s of cutting. The chip thickness t c and the contact length of the tool-chip interface l are measured on the SEM image of the chip root and tool rake face. The values of dimensions, cutting forces, and velocities are summarized in Table 12.2. The material properties include heat conductivity k, density ρ and specific heat c, where the density ρ is considered unchanged, while the heat conductivity k and specific heat c are the temperature dependent. For the 9XC workpiece and PCBN cutting tool, the material properties are given as [3]: PCBN cutting tool material: ρ = 3120 (kg/m3 ); k varies from k (20 °C) = 100 (W/mK) to k (900 °C) = 130 (W/mK); c varies from c(20 °C) = 1000 (J/kg K) to c(900°C) = 1966 (J/kg K). Workpiece material of 9XC steel: The Table 12.1 Geometry of PCBN insert Tool

Rake angle α

Clearance angle γ

Side angle λ

Nose radius r (mm)

PCBN

−6°

6°

0°

0.8

d (mm/v)

0.06

V (m/p)

119.3

3

a (mm)

0.13

t c (mm) 0.24

l c (mm) 0.46

r (t/t c )

Table 12.2 Experimental parameters to calculate the temperature 0.412

(rad) 136.5

V s (m/p) 55.07

V c (m/p)

410.6

F c (N)

250.4

F t (N)

275.6

F s (N)

206.2

F F (N)

136 D. T. Q. Nguyen

12 Prediction of Temperature Distribution in PCBN Cutting Tools …

137

Table 12.3 The values of heat flux at the heat generating centers τAB (N/mm2 )

As (mm2 )

q1 (W/mm2 )

γ˙sec 105 (1/s)

τ sec (N/mm2 )

τ s (N/mm2 )

q2max (W/mm2 )

q3 (W/mm2 )

919.32

0.45

1397

1.2

286

490

450

303

thermal properties can be considered as constant since they would not vary significantly within the range of testing temperature: k = 47 (W/mK); ρ = 7800 (kg/m3 ); c(20 °C) = 486 (J/kg K), ambient temperature T ∞ = 20 °C. The heat generation rates are calculated and summarized in Table 12.3.

12.2.6 Finite Element Model A two-dimensional heat transfer simulation model was established as shown in Fig. 12.3. The set-up of the simulation model includes the tool insert, tool holder, the chip and workpiece. The process of meshing elements of the model is accomplished in ABAQUS software with appropriate control parameters so that the heat-generating areas are divided with fine-sized elements to achieve high accuracy. In total, the whole model is divided into 557,758 tetrahedral elements, each element has 4 nodes with a total of 2,231,032 nodes as shown in Fig. 12.3a. With input parameters including the geometry of the survey area, the material properties of the tool and the workpiece, the specific heat flux and boundary conditions. The process of analyzing the temperature distribution in orthogonal turning 9XC hardened steel with PCBN cutting tool has been carried out and given the temperature distribution as shown in Fig. 12.3b. The temperature distribution in PCBN cutting tools when orthogonal turning 9XC hardened alloy steel is also determined experimentally. Isotherms in the tool are obtained from the boundaries between melted and unmelted zones of the thin

Gradient

2320C

µm 2500 2000 1500

3270C

Gradient 3270C

a)

b)

4190C

0 4180C 659 C

6920C

µm

2500 2000 1500 1000

Flank face

500

1000

Rake face

Theoretical Experiment

c)

500

9600C 11490C

0

9610C 10640C

Fig. 12.3 Meshing simulation model (a), temperature distribution (b), and isotherms in cutting tools obtained from empirical measurement and numerical model (c)

138

D. T. Q. Nguyen

layers of different materials with specific melting points coated on the surface of the cutting tool [16].

12.3 Results and Discussion The results from the numerical and experimental models indicate that the heat generated during orthogonal turning 9XC hardened steel by PCBN cutting tool is very large. Although most cutting heat is carried away by the chip and only a small portion of the heat is transferred into the cutting tool, the temperature at the edge of the cutting tool is still very high. It can reach 1163 °C at the beginning of machining and 1537 °C after only 2.19 s when the tool is worn. It can be seen that the reason for the very high temperature at the tool edge is the poor thermal conductivity of PCBN material while heat is continuously transferred to a fixed position on the tool. On the other hand, in the hard turning process, the machined materials have high hardness and durability. Thus, they require a large amount of destructive energy, which causes a large shear force which results in a high heat generation rate. The isotherms obtained from the numerical are highly compatible with those obtained from experimental measurements. The differences at the melting boundaries of the coated materials are relatively small, namely: 0.2% at 419 °C (Zn), 5% at 659 °C (Al), 0.1% at 919 °C (Ag) and 7.8% at 1064 °C (Au) (Fig. 12.3c).

12.4 Conclusion In this research, a numerical model investigating the temperature distribution in the PCBN cutting tool of the orthogonal turning 9XC hard ened alloy steel has been developed. The model is based on the calculations with certain assumptions. Results from calculation and measurement show that the temperature at the cutting area during the orthogonal turning of 9XC hardened steel by PCBN tool is very high. High temperatures cause the change in mechanical properties of the binder of the PCBN material, leading to rapid wear and plastic deformation of the tool edge while accelerating chemical interaction and promoting wear mechanisms, result in faster damage to the cutting edge. The isotherms achieved from the numerical model are highly compatible with those obtained from the experimental measurements since the differences are less than 7.8%. This demonstrates that the proposed numerical model has acceptable reliability and it can be applied to similar machining conditions.

12 Prediction of Temperature Distribution in PCBN Cutting Tools …

139

References 1. S. Jaspers, Metal Cutting Mechanics and Material Behaviour (Technische Universiteit Eindhoven, Holland, 1999) 2. S. Lo Casto, E. Lo Valvo, F. Micari, J. Mech. Work. Technol. 20, 35–46 (1989) 3. X.J. Ren, Q.X. Yang, R.D. James, L. Wang, J. Mater. Process. Technol. 147, 38–44 (2004) 4. T. Ueda, M. Al Huda, K. Yamada, K. Nakayama, Ann. CIRP 4 (1999) 5. P.D. Dhikale, S.M. Shinde, A.P. Kulkarni, Int. Conf. Mater. Process. Characterzation 2, 1907– 1914 (2015) 6. H. Yana, J. Huab, R. Shivpuri, Sci. Technol. Adv. Mater. 6, 540–547 (2005) 7. N.E. Karkalos, A.P. Markopoulos, J. Chem. Technol. Metall. 52, 288–293 (2017) 8. A.O. Tay, M.G. Stevenson, G. de Vahl Davis, P.L.B. Oxley, Int. J. Mach. Tool Des. Res. 16, 335–349 (1976) 9. Y. Dogu, E. Aslan, N. camuscu, J. Mater. Process. Technol. 171, 1–9 (2006) 10. A.O. Tay, M.G. Stevenson, G. de Vahl Davis, Proc. Inst. Mech. Eng. Proc. 188, 627–638 (1974) 11. M. Trent Edward, K. Paul Wright, Metal Cutting, Butterworth-Heinemann, New Delhi (2000) 12. M.C. Shaw, Metals Cutting Principles (Oxford University Press, New York, 1984) 13. X. Li, E.M. Kopalinsky, P.L.B. Oxley, Proc. Inst. Mech. Eng. 209, 33–43 (1995) 14. N.N. Zorev, International Research in Productions Engineering (ASME, New York, 1963), pp. 48–57 15. P. Majumdar, R. Jayaramachandran, S. Ganesan, Appl. Therm. Eng. 25, 2152–2168 (2005) 16. N.T.Q. Quoc Dung, P.Q. The, in International Symposium on Technology for Sustainability, Bangkok, Thailand, pp. 560–562 (2012)

Chapter 13

Study on the Optimal Sealing Technological Regime for Making Sport Wears from Waterproof Fabric Tran Thuy Trang and Phan Thanh Thao

Abstract The article focuses on the separate and simultaneous influences of sealing technological effects: air temperature, sealing speed, roller pressure and nozzle pressure on resistance to water penetration, ultimate tensile strength, the adhesive strength of seam sealing after washed in processing sportwears made from waterproof fabrics. In this research, we used the analysis of variance method for two-elements case, planning method orthogonal experimental variety of factors, Microsoft Excel 2013 and Design Expert 11.0 software to process and analyse experiment results. The result which is to identify sealing technological elements has important effects on resistance to water penetration, ultimate tensile strength, the adhesive strength of seam sealing after washed. The result of this study is an useful guide in the actual production to improve the quality of links in order to save time and costs in the actual production in sportwear garment enterprises as well as Seam tape supplier in general and at TNG Investment and Trading Join Stock Company in particular.

13.1 Introduction Nowadays, some products in fashion industry such as tents, single-layer or multilayer jackets need to have waterproof function with certain levels of waterproofing. To achieve water-proof ability, in production, people not only use traditional sewing methods but also use one of two methods: welding sealing and sealing seam. Actual productions at Song Cong 2 Garment Company of TNG Investment and Trading Joint Stock Company, sportswear products using the method of sealing seam are the dominant products. In order to evaluate product quality, the criteria of washing resistance, adhesive strength and water resistance are very important. Therefore, within the scope of the research, the authors focus on studying, conducting exploration and screening experiments, using mathematical tools to analyze the specific T. T. Trang (B) · P. T. Thao Hanoi University of Science and Technology, Hanoi, Vietnam e-mail: [email protected] P. T. Thao e-mail: [email protected] © Springer Nature Switzerland AG 2020 I. A. Parinov et al. (eds.), Advanced Materials, Springer Proceedings in Materials 6, https://doi.org/10.1007/978-3-030-45120-2_13

141

142

T. T. Trang and P. T. Thao

Table 13.1 Technical specification required

STT

Physical properties

Value

1

Layers

2

Width (inch)

58 inch

3

Face fabric

100% PET (PU: Laminated on face fabric)

4

Weight (g/m2 )

150

5

Weave type

Woven, Twill Fabric

6

Thickness (mm)

0.2 mm

7

Waterproofness (before washing)

≥12,000 mm H2 O

8

Waterproofness (after washing)

≥10,000 mm H2 O

9

Breaking strength (before washing)

≥1.1 dN/20 mm

10

Breaking strength (after washing)

≥0.9 dN/20 mm

2

levels of influence after washing. There are many technological factors that influence on the sealing seam quality, such as sealing temperature, sealing speed, wind pressure and compression strength of axis plots, etc. Experimental use of waterproof cloth with high quality processed products for sportswear at Song Cong 2 Garment Company of TNG Investment and Trading Joint Stock Company.

13.2 Experimental Research 13.2.1 Object of Researching 13.2.1.1

Fabric

Select the common waterproof fabrics used for sportswear produced at Song Cong 2 Garment Company of TNG Investment and Trading Joint Stock Company. Some specifications of ELM PES 2L TRANS T—experimental fabric are shown in Table 13.1.

13.2.1.2

Tape

Adhesive tape is a material which is used to paste over temporary seams of waterproofing materials (sealing seams or welding seams) with the aim of giving the

13 Study on the Optimal Sealing Technological Regime for Making …

143

Table 13.2 Thermal and physical properties Information

Tape ST604

Supplier

BEMIS

Tape type

ST604

Width

20 mm

Composition

100% PU

Gauge

89 µm

Softening point

105 °C

Note : a. 1st layer fabric b. 2st layer fabric c. Tape 1. Single needle Lockstitch 2. Topstitching

Fig. 13.1 Structure of seam sealing section

seams the necessary waterproofing and mechanical strength. Therefore, the structure, properties and number of layers of adhesive materials must be compatible with the structure, properties and number of layers of a waterproof fabric. In this research, select ST604 tape from BEMIS supplier. Technical information of the tape is shown in Table 13.2 [1].

13.2.1.3

Section: Figure 13.1

See Fig. 13.1.

13.2.1.4

Measuring Device

Experiments of the research was carried out at the technical department of Song Cong 2 Garment Company and the Company’s Internal Lab, including the following equipment: lockstitch sewing machine, hot air tape sealing machine, washing machines, leaking test machine, and tensile testing machine. Washing test was performed according to DS034 standard, waterproof test—to DS270 standard, testing the adhesive strength of the sealing seam according to DS044 standard—standards of Decathlon Co., Ltd. (Strategic customer of Song Cong Garment Company 2) [2].

144

T. T. Trang and P. T. Thao

13.2.2 Research Methodology We use ANOVA variance analysis method with one factor on Microsoft Excel 2013 software to process and analyze empirical data to evaluate the degree of individual impact of each paste technology to adhesion of sealing seam [3]. We use multivariate empirical planning method with the help of Design Expert 11.0 software, to design experiments, process and formulate empirical regression equations to study the simultaneous effects of the factors. Technology factors to the adhesion strength of the surface of all details glued on the research cloth [4].

13.2.2.1

Studying the Unique Effect of Each Factor to the Adhesive Strength of the Sealing Seam

The empirical data for these experiments is established by considering the influence of one factor, the values of this factor is changed, and the other factors remain at the value set by the technical department (the parameter is using in production) [3, 4]. Specifically, the recommended parameters from the technical department are [5]: (i) (ii) (iii) (iv)

air temperature 500 °C; sealing speed 22 ft/min; roller pressure 0.45 MPa; nozzle pressure 0.06 MPa.

All of the factors are measurable and controllable variables. The change in the value of these factors is regular and based on the average value, the upper and lower values are wider than the value ranges commonly established in enterprises to ensure the total general and accurate experiments. Based on the actual production and recommended parameters of the Bemis supplier, we choose the range of variations of the paste technology factors in Table 13.3 [5–7]. Number of samples tested: (v) the number of testing samples for each factor is 15 samples (each factor has 5 levels of change value; each level of sample is measured 3 times); (vi) total number of testing: 15 × 4 = 60 (samples).

Table 13.3 Interval of 4 variables in the research Elements

Air temperature (°C)

Sealing speed (ft/min)

Roller pressure (MPa)

Nozzle pressure (MPa)

Value

480

20

0.35

0.04

490

21

0.40

0.05

500

22

0.45

0.06

510

23

0.50

0.07

520

24

0.55

0.08

13 Study on the Optimal Sealing Technological Regime for Making …

13.2.2.2

145

Studying the Effect of 4 Factors on the Adhesion Strength of the Sealing Seam

Number of samples tested: we use the orthogonal planning level 2 for 4 influencing factors. Then number of experiments is N = 2k−p + n0 + 2k = 24−1 + 4 + 2 × 4 = 20 experiments. Each experimental plan is measured 3 times. Total number of tests: 20 × 3 = 60 (samples). The change in the value of these technological parameters is regular and based on the average value. Based on the actual productions and recommended documents of the fabric and adhesive supplier, we choose the range of variability of factors in Table 13.4 [5–7].

13.3 Research Results 13.3.1 The Results of Each Factors Affect the Adhesion Strength of the Sealing Seam See Table 13.5.

13.3.2 Effect of Air Temperature on Adhesive Strength of the Sealing Seam Results of surveying the adhesive strength of seams on waterproofing fabrics in research of the individual effect of air temperature are presented in Table 13.5. Using Microsoft Excel 2013 software to conduct ANOVA variance analysis to assess the influence of the air temperature on the adhesive strength of the sealing seam. Results are presented in Table 13.6. ANOVA analysis results in Table 13.6. Table 13.4 Values and codes of 6 variables in the research No.

Variable in research X j

Value of real variable −1.41

(o C)

−1

0

1

1.41

1

Air temperature

450

470

500

530

550

2

Sealing speed (ft/min)

20

21

22

23

24

3

Roller pressure (MPa)

0.35

0.4

0.45

0.5

0.55

4

Nozzle pressure (MPa)

0.04

0.05

0.06

0.07

0.08

Nozzle pressure (Mpa)

Roller pressure (Mpa)

22

22

22

22

500

500

500

22

500

500

22

500

22

22

500

22

500

24

500

500

23

500

22

22

500

21

500

22

520

500

22

510

20

22

500

500

22

490

Sealing speed (ft/min)

22

480

Air temperature (o C)

Sealing speed (ft/min)

Air temperature (°C )

Variable

0.45

0.45

0.45

0.45

0.45

0.55

0.50

0.45

0.40

0.35

0.45

0.45

0.45

0.45

0.45

0.45

0.45

0.45

0.45

0.45

Roller pressure (MPa)

0.08

0.07

0.06

0.05

0.04

0.06

0.06

0.06

0.06

0.06

0.06

0.06

0.06

0.06

0.06

0.06

0.06

0.06

0.06

0.06

Nozzle pressure (MPa)

Ok

Ok

Ok

Ok

Ok

Ok

Ok

Ok

Ok

Nok

Ok

Ok

Ok

Ok

Ok

Ok

Ok

Ok

Ok

Ok

Waterproofness (before washing)

Table 13.5 Summary of test results measuring adhesive strength when changing each factor

Ok

Ok

Ok

Nok

Nok

Ok

Ok

Ok

Nok

Nok

Ok

Ok

Ok

Ok

Ok

Ok

Ok

Ok

Ok

Ok

Appearance after washing

Ok

Ok

Ok

Nok

Nok

Ok

Ok

Ok

Nok

Nok

Ok

Ok

Ok

Ok

Ok

Ok

Ok

Ok

Ok

Ok

Water-proofness (after washing)

17.56

17.34

17.68

18.23

15.77

17.66

17.36

17.27

16.82

16.34

16.60

12.45

14.49

17.18

17.96

15.47

17.44

13.58

14.63

17.61

Adhesive strength (N)

146 T. T. Trang and P. T. Thao

13 Study on the Optimal Sealing Technological Regime for Making …

147

Table 13.6 ANOVA analysis results on the effect of air temperature factors to the adhesive strength of the seam sealing Source of variation

SS

Between groups

37.04967

Within groups Total

7.696867 44.74653

df

MS

F

P-value

F crit

4

9.262417

12.03401

0.000774

3.47805

10

0.769687

–

–

–

14

–

–

–

–

Table 13.7 ANOVA analysis results on speed factors to the adhesive strength of the sealing seam Source of variation

SS

Between groups

80.47929

Within groups Total

7.879267 88.35856

df 4 15 19

MS

F

P-value

F crit

20.11982

38.30272

1.05E−07

3.055568

–

–

–

–

–

–

0.525284 –

(i) F = 12.03401 > Fth = 3.47805, i.e. air temperature affects the adhesive strength of the sealing seam with approximately 100% reliability; (ii) the effect of the air temperature on the adhesive strength according to the rule of quartic equation: y = −6E − 05x 4 + 0.1115x 3 − 81.454x 2 + 26434x − 3E + 06; R2 = 1.

13.3.2.1

Effect of Sealing Speed on Adhesive Strength of the Sealing Seam

Results of surveying the adhesive strength of seams on waterproofing fabrics in research of the individual effect of sealing speed are presented in Table 13.5. Using Microsoft Excel 2013 software, we conducted ANOVA variance analysis to assess the influence of the sealing speed on the adhesive strength of the sealing seam. Results are presented in Table 13.6. ANOVA analysis results in Table 13.7. (i) F = 38.30272 > Fth= 3.055568, i.e. sealing speed affects on the adhesive strength of the sealing seam with approximately 99% reliability; (ii) the effect of sealing speed on the adhesive strength according to the rule of cubic equation: y = 0.675x 3 −39.75x 2 + 776.95x − 5024.9; R2 = 0.9936.

13.3.2.2

Effect of Roller Pressure Force on Adhesive Strength of the Sealing Seam

Results of surveying the adhesive strength of seams on waterproofing fabrics in the study of the individual effect of roller pressure are presented in Table 13.5.

148

T. T. Trang and P. T. Thao

Table 13.8 ANOVA analysis results on the effect of roller pressure factors to the adhesive strength of the sealing seam Source of variation

SS

df

MS

F

P-value

F crit

Between groups

4.229778

4

1.057444

2.081074

0.134146

3.055568

Within groups

7.621867

15

0.508124

–

–

–

19

–

–

–

–

Total

11.85164

We use Microsoft Excel 2013 software to conduct ANOVA variance analysis to evaluate the impact of roller pressure on the adhesive strength of the sealing seam. Results are presented in Table 13.8. ANOVA analysis results in Table 13.8: (i) F = 2.081074 < Fth = 3.055568, i.e. the roller pressure has little effect on the adhesive strength of the sealing seam with approximately 98% reliability. (ii) the influence of roller pressure on the adhesive strength of the sealing seam follows the quadratic equation: y = −20.476x 2 + 24.769x + 10.193; R2 = 0.985.

13.3.2.3

Influence of Nozzle Pressure on Adhesive Strength of the Sealing Seam

Results of surveying the adhesive strength of seams on waterproofing fabrics in the study of the individual effect of nozzle pressure are presented in Table 13.5. We use Microsoft Excel 2013 software to conduct ANOVA variance analysis to evaluate the impact of nozzle pressure on the adhesive strength of the sealing seam. Results are presented in Table 13.9. ANOVA analysis results in Table 13.8 show: (i) F A = 31.01385 > Fth = 4.351244, i.e. the nozzle pressure affects on the adhesive strength of the sealing seam with approximately 98% reliability; (ii) the effects of the nozzle pressure on the adhesive strength according to the rules of cubic equation: y = 170131x 3 −30501x 2 + 1740.9x − 13.567; R2 = 0.9847.

Table 13.9 ANOVA analysis results on the effect of nozzle pressure factors to the adhesive strength of the sealing seam Source of variation

SS

Between groups

13.64165 6.7256 20.36725

19

Within groups Total

df

MS

F

P-value

F crit

4

3.410413

7.606191

0.001482

3.055568

15

0.448373

–

–

–

–

–

–

–

13 Study on the Optimal Sealing Technological Regime for Making …

13.3.2.4

149

Simultaneous Effect of 4 Factors to the Adhesive Strength of the Sealing Seam

Design expert software is used in designing experiments, data processing and building experimental recurrent equation display the principal that 4 variables in researching influence on adhesive strength of the sealing seam. The adhesion strength equation is obtained after data processing (Table 13.10): Y = 17.05893 + 0.449013X 1 + 1.58392X 2 + 0.587240X 3 + 1.34350X 4 + 1.03725X 1 X 2 + 0.72125 X 1 X 3 + 1.77517X 1 X 4 + 0.32625X 2 X 3 + 0.250263X 2 X 4 − 0.15125X 3 X 4 + 0.31357X 12 − 0.478929X 22 − 0.496429X 32 + 0.856071X 42

(13.1)

R2 = 0.9267 X 1 is the air temperature; X 2 is the sealing speed; X 3 is the roller pressure and X 4 is the nozzle pressure. Table 13.10 Summary of adhesive test results when changing 4 factors simultaneously No.

x1

x2

x3

x4

Y 1st

2st

3st

Average

1

−1

−1

−1

−1

18.27

17.21

16.89

17.46

2

1

−1

−1

1

16.11

18.66

17.22

17.33

3

−1

1

−1

1

17.48

16.11

18.43

17.34

4

1

1

−1

−1

15.71

15.21

15.23

15.38

5

−1

−1

1

−1

17.12

17.12

16.34

16.86

6

1

1

1

−1

19.61

19.21

18.09

18.97

7

−1

1

1

1

16.89

17.43

18.01

17.44

8

1

−1

1

1

19.81

19.12

18.09

19.01

9

−1.41

0

0

0

17.60

16.34

15.89

16.61

10

1.41

0

0

0

18.62

17.12

17.89

17.88

11

0

−1.41

0

0

14.93

13.22

12.11

13.42

12

0

1.41

0

0

18.47

17.68

17.56

17.90

13

0

0

−1.41

0

15.13

14.21

15.11

14.82

14

0

0

1.41

0

17.25

15.72

16.32

16.43

15

0

0

0

−1.41

16.54

17.09

15.67

16.43

16

0

0

0

1.41

19.07

21.61

20.00

20.23

17

0

0

0

0

17.91

17.14

16.91

17.32

18

0

0

0

0

18.08

17.38

16.22

17.23

19

0

0

0

0

17.88

17.22

17.20

17.43

20

0

0

0

0

18.66

17.48

17.91

18.02

150

13.3.2.5

T. T. Trang and P. T. Thao

Comment

Considering the value of X i (i = 1 ÷ 4) if we stand alone, then in the 4 coefficients (a1 , a2 , a3 , a4 ) from (13.1), we see that the coefficient a2 has the highest absolute value |a2 | = 1.58392, so the influence of X 2 or the sealing speed on adhesive strength is the greatest compared to the remaining variables X 1 , X 3 , X 4 .

13.3.2.6

Analyze of the Effect of Each Factor on Adhesive Strength

Analyze the Effect of Air Temperature on Adhesive Strength From (13.1) we have: a1 X 1 = 0.449013X 1 → a1 = 0.449013 > 0 → The variation of Y and X 1 is covariant. That is when X 1 ↑ → Y ↑ and X 1 ↓ → Y ↓. To increase adhesion strength (Y ), it is necessary to increase (X 1 ), that is, increase the paste temperature. However, if the temperature is too high, it will lead to an unqualified fire.

Analyze the Effect of Sealing Speed on Adhesive Strength From (13.1) we have: a2 X 2 = 1.58392X 2 → a2 = 1.58392 > 0 → The variation of Y and X 2 is covariant. That is when X 2 ↑ → Y ↑ and X 2 ↓ → Y ↓. To increase adhesion strength (Y ), it is necessary to increase (X 2 ), that is, increase the speed of gluing. However, if the paste speed is too fast, the tape and fabric will not receive enough heat to bond.

Analysis of Effect of Roller Pressure on Adhesive Strength From (13.1) we have: a3 X 3 = 0.587240X 3 → a3 = 0.587240 > 0 → The variation of Y and X 3 are covariant. That is when X 3 ↑ → Y ↑ and X 3 ↓ → Y ↓. To increase adhesion strength (Y ), it is necessary to increase (X 3 ), that is, increase the roller compression force. However, if the compression pressure is too high, the glue in the tape will be exposed to the edge of the adhesive, affecting the aesthetics and quality of the seam.

Analysis of Effect of Nozzle Pressure on Adhesive Strength From (13.1) we have: a4 X 4 = 1.34350X 4 → a4 = 1.34350 > 0 → The variation of Y and X 4 is covariant. That is when X 4 ↑ → Y ↑ and X 4 ↓ → Y ↓. To increase adhesion strength (Y ), it is necessary to increase (X 4 ), that is, the wind pressure. However, if the increase in wind pressure is too high, it will cause unqualified fire.

13 Study on the Optimal Sealing Technological Regime for Making …

151

Fig. 13.2 3D graph showing the simultaneous effect of air temperature and sealing speed on adhesive strength

13.3.2.7

Analyze of the Interaction Effect of Technological Factors on Adhesive Strength

Interaction Effect Between Air Temperature and Sealing Speed on Adhesive Strength From (13.1) we have: a12 X 1 X 2 = 1.03725X 1 X 2 → a12 = 1.03725 > 0 → X 1 X 2 ↑ → Y ↑ and X 1 X 2 ↓ → Y ↓. To increase adhesion strength (Y ), X 1 X 2 increases → X 1 X 2 > 0, then X 1 > 0 and X 2 > 0 or X 1 < 0 and X 2 < 0. Due to the fact that productions need to increase productivity, choose X 1 > 0 and X 2 > 0 and moreover, the quality is also focused, so it is necessary to select the sealing speed and air temperature to ensure high productivity and good adhesive quality (see Fig. 13.2).

Interaction Effect Between Air Temperature and Roller Pressure on Adhesive Strength From (13.1) we have: a13 X 1 X 3 = 0.72125X 1 X 3 → a13 = 0.72125 > 0 → X 1 X 3 ↑ → Y ↑ and X 1 X 3 ↓ → Y ↓. In order to increase the adhesion strength (Y ), the X 1 X 3 decreases → X 1 X 3 > 0, then X 1 > 0 and X 3 > 0 or X 1 < 0 and X 3 < 0. This means that the variation of air temperature and roller pressure is uniform, It is necessary to adjust these parameters appropriately to achieve productivity and quality (see Fig. 13.3).

152

T. T. Trang and P. T. Thao

Fig. 13.3 3D graph showing the simultaneous effect of air temperature and roller pressure on adhesive strength

Fig. 13.4 3D graph showing the simultaneous effect of air temperature and the nozzle pressure on adhesive strength

Interaction Effect Between Air Temperature and Nozzle Pressure on Adhesive Strength From (13.1) we have: a14 X 1 X 4 = 1.03725X 1 X 4 → a14 = 1.77517 > 0 → X 1 X 4 ↑ → Y ↑ and X 1 X 4 ↓ → Y ↓. To increase adhesion strength (Y ), X 1 X 2 increases → X 1 X 4 > 0, then X 1 > 0 and X 4 > 0 or X 1 < 0 and X 4 < 0. Due to the fact that production needs to increase productivity, choose X 1 > 0 and X 4 > 0 and moreover, the quality is also focused, so it is necessary to choose roller pressure and air temperature to ensure high productivity and good adhesive quality (see Fig. 13.4).

13 Study on the Optimal Sealing Technological Regime for Making …

153

Fig. 13.5 3D graph showing the simultaneous effect of sealing speed and roller pressure on adhesive strength

Interaction Effect of Sealing Speed and Roller Pressure on Adhesive Strength From (13.1) we have: a23 X 2 X 3 = 0.023625X 2 X 3 → a23 = 0.032625 > 0 → X 2 X 3 ↑ → Y ↑ and X 2 X 3 ↓ → Y ↓. To increase adhesion strength (Y ), X 2 X 3 increases → X 2 X 3 > 0, then X 2 > 0 and X 3 > 0 or X 2 < 0 and X 3 < 0. Due to the fact that production needs to increase productivity, choose X 2 > 0 and X 3 > 0 and moreover, the quality is also focused, so it is necessary to choose the sealing speed and roller pressure to ensure high productivity and good adhesive quality (see Fig. 13.5).

Effect of Interaction Between Sealing Speed and Nozzle Pressure on Adhesive Strength From (13.1) we have: a24 X 2 X 4 = 0.250263X 2 X 4 → a24 = 0.250263 > 0 → The variation of Y and X 2 X 4 are covariant. That is when X 2 X 4 ↑ → Y ↑ and X 2 X 4 ↓ → Y ↓. To increase adhesion strength (Y ), X 2 X 4 increases → X 2 X 4 > 0, then X 2 > 0 and X 4 > 0 or X 2 < 0 and X 4 < 0. Due to the fact that production needs to increase productivity, choose X 2 > 0 and X 4 > 0 and moreover, the quality is also focused, so it is necessary to choose the paste speed and wind pressure to ensure high productivity and good adhesive quality (see Fig. 13.6).

Influence of Interaction Between Roller Pressure and Nozzle Pressure on Adhesive Strength From (13.1) we have: a34 X 3 X 4 = −0.15125X 3 X 4 → a34 = −0.15125 < 0 → The variation of Y and X 3 X 4 is inversely. That is when X 3 X 4 ↑ → Y ↓ and X 3 X 4 ↓ → Y↑.

154

T. T. Trang and P. T. Thao

Fig. 13.6 3D graph showing the effect of sealing speed and nozzle pressure on adhesive strength

Fig. 13.7 3D graph showing the simultaneous effect of roller pressure and nozzle pressure on adhesive strength

To increase adhesion strength (Y ), X 3 X 4 decreases → X 3 X 4 < 0, X 3 > 0 and X 4 < 0 or X 3 < 0 and X 4 > 0. This means the variability of roller compression and torch pressure are reversible variables. It is necessary to adjust these parameters reasonably to achieve productivity and quality (see Fig. 13.7).

13 Study on the Optimal Sealing Technological Regime for Making …

13.3.2.8

155

Determining the Optimum Value of the Paste Technology Parameters Ensures the Adhesive Strength of the Surface of the Part Is the Largest

From the empirical regression equation expressing the law of the effect of 4 factors of gluing technology on the adhesive strength of the sealing seam in research, we conduct optimization of problems by Design Expert 11.0 software. Data processing results find an optimal solution: (i) optimal value of variables (coded form): X 1 = 0.912315; X 2 = 0.901385; X 3 = 0.764905; X 4 = 0.190739; (ii) the maximum value of the adhesive strength: Y max = 21.1254 (N). From the calculation result for the coding variable, we can calculate the value of the real variable: X 1 = 530 (o C); X 2 = 23 (ft/min); X 3 = 0.49 (MPa); X4 = 0.06 (MPa).

13.4 Conclusion (1) We performed experimental exploration to evaluate the individual influence of some technological factors of taping machines such as: air temperature, sealing speed, roller pressure, and nozzle pressure to adhesive strength of the sealing seam on 2-layer waterproof fabrics, 100% PET base layers and coated with PU used for sewing sportswear at Song Cong 2 Garment Company branch of TNG Corporation. It has shown that there are three technology factors of a research tape machine: (i) the air temperature, (ii) the sealing speed, (iii) the nozzle pressure, which significantly affect on the adhesive strength; the roller pressure has influence but lesser extent. (2) ANOVA analysis results show that the air temperature affects on the adhesion strength with a high confidence of approximately 100%: y = −6E − 05x 4 + 0.1115x 3 − 81.454x 2 + 26434x − 3E + 06; R2 = 1 (3) ANOVA analysis results show that the sealing speed affects on the adhesion strength with approximately 99% reliability: y = 0.675x 3 − 39.75x 2 + 776.95x − 5024.9; R2 = 0.9936 (4) ANOVA analysis results show that the roller pressure has little effect on the adhesion strength with approximately 98% reliability: y = −20.476x 2 + 24.769x + 10.193; R2 = 0.985 (5) ANOVA analysis results show that the nozzle pressure has little affects on the adhesion strength with approximately 98% reliability: y = 170131x 3 − 30501x 2 + 1740.9x − 13.567; R2 = 0.9847 (6) The adhesion strength equation is obtained after data processing: Y = 17.05893+ 0.449013X 1 + 1.58392X 2 + 0.587240X 3 + 1.34350X 4 + 1.03725X 1 X 2 + 0.72125X 1 X 3 + 1.77517X 1 X 4 + 0.32625X 2 X 3 + 0.250263X 2 X 4 − 0,15125X 3 X 4 + 0.31357X 21 – 0.478929X 22 − 0.496429X 23 + 0.856071X 24

156

T. T. Trang and P. T. Thao

(7) Study on using 100% polyester woven fabric and PU coating, Bemis ST604 tape and the parameter as below: – air temperature is 530°C; sealing speed is 23 ft/min; roller pressure is 0.49 MPa; nozzle pressure is 0.06 MPa; – the highest value of the adhesive strength is 21.1254 N. (8) The above results are useful guides in the actual production at Song Cong 2 Garment Company, helping technicians to adjust the optimal technology regime to ensure product quality stability, contributing to increasing the efficiency of high-class sports clothing products from waterproof fabrics productions.

References 1. Seam Sealing Tape (Bemis Associates Inc., Shirley, 2019) 2. Decathlon Standard (Decathlon, Ascq, 2019) 3. N. Van Lan, Processing Statistical Data and Applied Examples in the Textile Industry. (National University Press, Ho Chi Minh, 2003) 4. P.T. Thao, Building data-sheet of amendment to correct the optimal sealing technological regime for making high quality garment products from waterproof fabrics in the tropical seasonal climate of Vietnam, 2007–2008 (2008) 5. Parameter Document for 305122 Black (TNG Investment and Trading JSC, Thai Nguyen, 2019) 6. ST604 Data Sheet (Bemis Associates Inc., Shirley, 2019) 7. Test Report for ST604 305122 (Bemis Associates Inc., Shirley (2019)

Part II

Physics of Advanced Materials

Chapter 14

Equation for Density Matrix Systems of Identical Particles Boris V. Bondarev

Abstract The equations for the statistical operator and the density matrix are considered here for a single particle and a system of identical particles when dissipative forces act on them. From the equation for the density matrix, a kinetic equation can be obtained when the density matrix is diagonal. These equations are the basis for the study of the simplest models of nanophysics.

14.1 Introduction In quantum mechanics, the most general description of the system is the statistical operator . ˆ The statistical operator must be normalized at any time Tr ˆ = 1,

(1.1)

ˆ ∗ = ˆ

(1.2)

self-adjoint

and positively definite. A correct equation describing the evolution of a statistical operator must ensure that these properties are preserved over time. For the first time the equation for the statistical operator: ˆ = (t, ˆ q),

(1.3)

where q is the quantum coordinate of the system was obtained by Lindblad [1]. This equation has the form: ˆ i ˙ˆ = [H ] ˆ + i D,

(1.4)

B. V. Bondarev (B) Moscow Aviation Institute, Moscow, Russia e-mail: [email protected] © Springer Nature Switzerland AG 2020 I. A. Parinov et al. (eds.), Advanced Materials, Springer Proceedings in Materials 6, https://doi.org/10.1007/978-3-030-45120-2_14

159

160

B. V. Bondarev

where Hˆ is the Hamiltonian of the system, Dˆ =

C jk {[aˆ j , ˆ aˆ k+ ] + [aˆ j , ˆ aˆ k+ ]},

(1.5)

jk

C jk are some numbers, and aˆ j is an arbitrary operator. The operator Dˆ is called the dissipative operator. This statement can be written as Dˆ =

C jk {2aˆ j ˆ aˆ k+ − aˆ k+ aˆ j ˆ − ˆ aˆ k+ aˆ j }.

(1.6)

jk

14.2 Equation for the Density Matrix of One Particle The density matrix is related to the operator ˆ (t, q) formula nn (t) =

ϕn∗ (t, q)(t, ˆ q)ϕn (t, q)dq.

(2.1)

This formula specifies the density matrix nn (t) in the n-representation. Wave function ϕn (t,q) can be found from the Schrödinger equation: i ϕ˙n = Hˆ ϕn .

(2.2)

The equation for the density matrix was derived from the Liouville–Von Neumann equation in [2, 3]. This equation is analogous to the Lindblad equation and has the form: (Hnm mn − nm Hmn ) i ˙ nn = m

+ i {

γnm,m n mm − 1/2

mm

(γnm mn + nm γmn )},

(2.3)

m

where Hnm are the matrix elements of the Hamiltonian Hˆ system, γnm,m n is some matrix, γmn nm . (2.4) γnn = m

Equation (2.3) can be written as i˙ nn =

m

(Hnm mn − nm Hmn ) + iDnn ,

(2.5)

14 Equation for Density Matrix Systems of Identical Particles

161

where Dnn is a dissipative matrix, which will now be equal to Dnn =

γnm,m n mm − 1/2

mm

(γnm mn + nm γmn ).

(2.6)

m

Compare this formula with the formula (1.6), we establish that γnm,m n = 2

C jk anm, j am+ n ,k ,

(2.7)

jk

where anm, j are matrix elements of the operator aˆ j . The diagonal element nn is the probability wn that the system is in the state n. This value satisfies the normalization condition: nn = 1. (2.8) n

This formula is similar to the formula (1.1). In addition, the density matrix nm satisfies the following condition: ∗ = mn . nm

(2.9)

The same condition is subject to Hamiltonian: ∗ = Hmn . Hnm

(2.10)

Consider the system where the density matrix nm at an arbitrary time t is in the diagonal state: nm = wn δnm ,

(2.11)

where δnm is the Kronecker symbol. Then from (3.3) we obtain w˙ n =

( pnm wm − pmn wn ),

(2.12)

m

where pnm = γnm,mn = 2π/

υn N ,m M 2 W M δ(εn − εm + E N − E M ),

(2.13)

NM

there is a probability of transition of the system in a unit of time from the state m to the state n, W N = v exp(−β E N )

162

B. V. Bondarev

there is a possibility that the environment is in an equilibrium state with quantum numbers N, and E N is its energy in this state, ν is the normalization factor, β = 1/(kB T ) is the inverse temperature; υn N ,m M are the matrix elements of the system interaction with its environment. Formula (2.13) is the Golden rule of Fermi.

14.3 The Hierarchy for the Statistical Operators Consider a system consisting of N identical particles. The statistical operator ˆ describing the state of such a system can be written as ˆ 2, . . . , N . ˆ = (t, ˆ q1 , q2 , . . . , q N ) ≡ (1,

(3.1)

Here, the numbers in parentheses indicate the indices of the variables that are affected by this operator. The statistical operator, as well as any other operator describing the state of the system of identical particles, must be symmetric: (. ˆ . . , i, . . . , j, . . .) = (. ˆ . . , j, . . . , i, . . .).

(3.2)

We take the following normalization condition for the statistical operator: ˆ 2, . . . , N ) = N !. Tr1...N (1,

(3.3)

The Hamilton operator for the system of identical particles can be represented as a sum Hˆ (1, 2, . . . , N ) =

N i=1

N

Hˆ (i) + 1/2

Hˆ (i, j)

(3.4)

i=1, j=1, j=i

where Hˆ (i) is a single-particle Hamiltonian, i.e. the energy operator of one particle without taking into account its interaction with other particles; Hˆ (i, j) is the interaction operator of two particles. A single-particle Hamiltonian may contain dissipative terms. The two-particle Hamiltonian must be symmetric: Hˆ (i, j) = Hˆ ( j, i).

(3.5)

Under this condition, the Hamiltonian (3.4) will also be symmetric. Let us temporarily omit the summation operation in the expression (1.5) and write it as follows: ˆ ˆ aˆ + . Dˆ = aˆ , ˆ aˆ + + a,

(3.6)

14 Equation for Density Matrix Systems of Identical Particles

163

Suppose that the dissipative processes occurring in the system are due to the stochastic interaction of particles with the heat reservoir. Each particle interacts with it independently of other particles. In this case, the multi-particle operator a in the expression (3.6) can be represented as a sum: aˆ = a(1, ˆ . . . , N) =

N

a(i), ˆ

(3.7)

i=1

where operator a(i) ˆ characterizes the effect of the heat reservoir on one of the particles. Substituting this sum into the expression (3.6) gives Dˆ =

N N a(i) ˆ , ˆ aˆ + ( j) + a(i), ˆ ˆ aˆ + ( j) .

(3.8)

i=1 j=1

Of practical interest is the equation for the single-particle statistical operator (1), ˆ which is determined by the ratio: ˆ 2, . . . , N ). (1) ˆ = 1/(N − 1)!Tr2...N (1,

(3.9)

From this definition, condition (3.3) implies the normalization condition for the ˆ = N. Tr1 (1)

(3.10)

We define a two-particle statistical operator (1, ˆ 2) as ˆ 2, . . . , N ). (1, ˆ 2) = 1/(N − 2)!Tr3...N (1,

(3.11)

This operator satisfies the normalization condition: ˆ 2) = N (N − 1). Tr12 (1,

14.4 The Equation for the Statistical Operators We assume that (1.4) is true for the operator (3.1). To obtain the equation for the derivative of the one-particle operator (1), ˆ we apply to both parts of (1.4) the convolution operation Tr2...N . Since ˆ 2, . . . , N )] ≡ 0, Tri [ Hˆ (i)(1, using the definition (3.9), we obtain:

164

B. V. Bondarev

Tr2...N

N [ Hˆ (i)(1, ˆ 2, . . . , N )] = (N − 1)![ Hˆ (1)(1)]. ˆ i=1

By virtue of identity: ˆ 2, . . . , N )] ≡ 0, Tri j [ Hˆ (i, j)(1, taking into account the property (3.5) and the definition (3.11), we will have N

Tr2...N 1/2

[ Hˆ (i, j)(1, ˆ 2, . . . , N )]

i=1, j=1, j=i

= 1/2Tr2...N

⎧ ⎨ ⎩

N

[ Hˆ (1, j)(1, ˆ 2, . . . , N )]

i=1, j=2, j=i

N

+

[ Hˆ (1, j)(1, ˆ 2, . . . , N )]}

i=2, j=2, j=i

ˆ 2)]. = 1/2(N − 1)!Tr2 [ Hˆ (1, 2)(1, Likewise ˆ , ˆ aˆ + (1)] + [a(1), ˆ ˆ aˆ + (1)] Tr2...N Dˆ = Tr2...N {[a(1) +

N ([a(i) ˆ , ˆ aˆ + (1)] + [a(i), ˆ ˆ aˆ + (1)] i=2

ˆ ˆ aˆ + (i)]) + [a(1) ˆ , ˆ aˆ + (i)] + [a(1), +

N N ([a(i) ˆ , ˆ aˆ + ( j)] + [a(i), ˆ ˆ aˆ + ( j)])} i=2 j=2

= (N − 1)!{[a(1) ˆ (1), ˆ aˆ + (1)] + [a(1), ˆ (1) ˆ aˆ + (1)] ˆ (1, ˆ 2), aˆ + (1)] + [a(1), ˆ Tr2 (1, ˆ 2)aˆ + (2)]}, + [Tr2 a(2) since ˆ ˆ aˆ + ( j) ≡ 0, Tr j a(i) ˆ , ˆ aˆ + ( j) ≡ 0. Tri a(i), Having collected together the expressions, we come to the equation: ˙ˆ ˆ 2)] i(1) = [ Hˆ (1)(1)] ˆ + 1/2Tr2 [ Hˆ (1, 2)(1, + i{[a(1) ˆ (1), ˆ aˆ + (1)] + [a(1), ˆ (1) ˆ aˆ + (1)] ˆ (1, ˆ 2), aˆ + (1)] + [a(1), ˆ Tr2 (1, ˆ 2)aˆ + (2)]}. + [Tr2 a(2)

(4.1)

14 Equation for Density Matrix Systems of Identical Particles

165

14.5 The Equation for the Density Matrix We denote the matrix elements of operators (1), ˆ (1, ˆ 2), Hˆ (1), Hˆ (1, 2) and a(1) ˆ in a certain n-representation as n 1 n 1 = 11 , n 1 n 2 ,n 1 n 2 = 12,1 2 , Hn 1 n 1 = H11 , Hn 1 n 2 ,n 1 n 2 = H12,1 2 , an 1 n 1 = a11 , and write (4.1) in matrix form: i˙ 11 =

[H12 21 ] + 1/2 [H12,34 43,21 ] n2

n2 n3 n4

+ + + i{ ([a12 23 , a31 ] + [a12 , 23 a31 ]) n2 n3

+

+ + ([a34 43,12 , a21 ] + [a12 , 21 ,34 a43 ])}.

(5.1)

n2 n3 n4

The two-particle density matrix 12,1 2 , describing the state of the boson system must be symmetric. Whereas the two-particle density matrix of the fermion system must be antisymmetric. Approximately this matrix can be expressed through a singleparticle density matrix as follows: 12,1 2 = 11 22 ± 12 21 ,

(5.2)

where the plus sign corresponds to bosons and the minus sign corresponds to fermions. Swap the first two variables and the second two in this formula and get 21,2 1 = 22 11 ± 21 12 .

(5.3)

It is seen that these two-particle density matrices are symmetric: 12,1 2 = 21,2 1 .

(5.4)

Substitute the expression (5.2) in (5.1). We come to the equation for a singleparticle density matrix: i˙ 11 =

[H12 21 ]

n2

+ 1/2

n2 n3 n4

[H12,34 (42 31 ± 41 32 )]

166

B. V. Bondarev

+ i{

+ + ([a12 23 , a31 ] + [a12 , 23 a31 ]) n2 n3

+

+ ([a34 (41 32 ± 42 31 ), a21 ]

n2 n3 n4 + + [a12 , (23 1 4 ± 24 1 3 )a43 ])}.

(5.5)

Two-part matrix H12,1 2 the fermions are anti-symmetric, i.e. it satisfies the relations: H12,1 2 = −H21,1 2 = −H12,2 1 = H21,2 1 .

(5.6)

For bosons, this matrix is symmetric: H12,1 2 = H21,1 2 = H12,2 1 = H21,2 1 .

(5.7)

We transform the summand with a two-particle Hamiltonian:

([H12,34 (42 31 ± 41 32 )]

n2 n3 n4

=

([H12,34 , 42 31 ] ± [H12,34 , 41 32 ]).

n2 n3 n4

Swap the indexes n 3 and n 4 in the second part of this equation. We will have

([H12,34 (42 31 ± 41 32 )]

n2 n3 n4

=

([H12,34 , 42 31 ] ± [H12,43 , 31 42 ])

n2 n3 n4

=

[(H12,34 ± H12,43 ), 42 31 ]

n2 n3 n4

=2

[H12,34 , 42 31 ].

n2 n3 n4

This equality is true by virtue of the formulas (5.6) and (5.7). Enter the symbol: + γ12,31 = 2a12 a31 ,

Write (5.5) with this notation [4, 5]: i˙ 11 =

[H12 21 ] + [H12,34 , 42 31 ] n2

n2 n3 n4

(5.8)

14 Equation for Density Matrix Systems of Identical Particles

(2γ12,31 23 − γ23,12 31 − γ31 ,23 12 )

+ i /2 +

167

n2 n3

{(14 23 ± 24 13 )γ34,21

n2 n3 n4

− γ34,12 (24 1 3 ± 1 4 23 ) + γ12,43 (32 41 ± 42 31 ) − (31 42 ± 41 32 )γ21 ,43 }.

(5.9)

This is the desired equation for the density matrix.

14.6 Kinetic Equation Substitute the diagonal matrix (2.11) in (5.9): 12 = w1 δ12 .

(6.1)

We will have after we put n 2 = n 1 , the following equation: ∂w1 /∂t =

(γ12,21 w2 − γ21,12 w1 )

n2

+ 1/2

w1 w2 {γ21,21 ± γ12,21 − (γ12,12 ± γ21,12 )

n2

+ γ12,12 ± γ12,21 − (γ21,21 ± γ21,12 )}. Reducing the terms containing elements of the matrix γ12,12 and γ21,21 , we obtain the kinetic equation: ∂w1 /∂t =

{γ12,21 w2 (1 ± w1 ) − γ21,12 w1 (1 ± w2 )}.

(6.2)

n2

Substitution of formula (2.13) in p12 = γ12,21 ,

(6.3)

results that (6.2) can be written as ∂w1 /∂t =

{ p12 w2 (1 ± w1 ) − p21 w1 (1 ± w2 )}.

(6.4)

n2

where p12 is the probability of transition of a particle per unit time from the state n 2 to the state n 1 .

168

B. V. Bondarev

14.7 The Energy of the System of Identical Particles Unitary Matrix We write a known expression for the average energy of the particle system: E=

H12 21 + 1/2

H12,34 34,12 ,

(7.1)

{n}

n1 n2

where {n} = n 1 , n 2 , n 3 , n 4 . Let a κ-representation of the density matrix will be diagonal, i.e., has the form: ˜ κκ = wκ δκκ ,

(7.2)

(11) ˜ κ1 κ2 ,κ1 κ2 ≡ ˜ 12,1 2 = w12 (δ11 δ22 ± δ12 δ21 ).

(7.3)

(11) where probabilities wκ and w12 satisfy the conditions:

wκ = N ,

κ

(11) w12 = N (N − 1).

(7.4)

κ1 κ2=κ1

(11) The probability w12 determines that both of the condition of κ1 and κ2 = κ1 occupied by particles. The transition from the n-representation to the κ-representation is carried out using the unitary matrix Unκ , which is determined by the relation:

∗ Unκ Unκ = δκκ .

(7.5)

n

If the unitary matrix is known, then the density matrix in the κ-representation is found by the formula: ˜ κκ =

Unκ nn Un∗ κ .

(7.6)

nn

Since the expression (7.1) in any representation has the same form, substituting the expression (7.2) and (7.3) in this formula will give E=

εκ wκ + 1/2

κ

(11) ε12 w12 ,

(7.7)

κ1 κ2=κ1

where εκ =

nn

∗ Unκ Hnn Un κ

(7.8)

14 Equation for Density Matrix Systems of Identical Particles

169

is the energy of a particle in a state κ, ε12 = 2

∗ ∗ U1κ U2κ H12,34 U3κ1 U4κ2 1 2

(7.9)

{n}

is the interaction energy of two particles, one of which is in the state κ1 , and the other is in the state κ2 .

14.8 Variational Principle In thermodynamics, the variational principle was developed, which along with the quantum (5.7) leads to the same results. Only now we are talking about systems of particles in the state of thermodynamic equilibrium. That is why now in a few words we will talk on the variation principle. The thermodynamic potential of the particle system is related to the average internal energy E, entropy S, absolute temperature T, chemical potential μ and the average number of particles N:

= E−S T −μN .

(8.1)

The function y = y(x) describing the equilibrium state of the system can be found by the Lagrange method. To do this, the thermodynamic potential should be expressed through this function = (y), differentiated by this function and to equate the derivative with zero: ∂ /∂ y = 0.

(8.2)

As a result, we obtain the equations for the equilibrium function. With energy, almost everything is clear from the previous section, but it is not clear why we started talking about the unitary matrix. The fact is that entropy can be written only for the density matrix in the diagonal form (7.2). For example, the entropy of the fermion system in the first approximation, when the binary probability (11) = w1 w2 w12

(8.3)

for κ1 = κ2 , equal to S = −kB

{(1 − wκ ) ln(1−wκ ) + wκ ln wκ }. κ

In the first approximation, the energy of the fermions is

(8.4)

170

B. V. Bondarev

E=

εκ wκ + 1/2

κ

ε12 w1 w2

(8.5)

κ1 κ2=κ1

provided that ε11 = 0. Now that we know the thermodynamic potential as a function of wκ , we will find the derivative of it. As a result, we get [6]: wκ = 1/ 1 + eβ(εκ −μ) ,

(8.6)

where εκ = εκ +

εκκ wκ

(8.7)

κ

is the average energy of one fermion in the state κ.

14.9 Correlation Function The variational principle allows us to find not only the probability wκ , but also the (11) . To do this, we introduce the so-called correlation function binary probability w12 ξκκ using the ratio (11) wκκ = wκ wκ (1 − δκκ ) + ξκκ .

(9.1)

14.10 The Probability of Transition of a Particle The probability of transition p12 particles from the state of κ2 to the state κ1 , according to the Fermi rule (2.13) must depend on the difference ε1 − ε2 medium energy particles in these states. As it is known, the thermodynamic equilibrium of a particle system obeys the Boltzmann rule. Thus, the probability of transition of a particle in equilibrium can always be represented as (o) −β(ε1 −ε2 )/2 e , p12 = p12

where (o) (o) = p21 , p12

εi is the average energy of particles in a state of κi .

(10.1)

14 Equation for Density Matrix Systems of Identical Particles

171

Let the system of particles come to a state of thermodynamic equilibrium. Since the probability wκ is now time-independent, the right side of (6.4) is zero. Thus, the principle of detailed equilibrium in this case is expressed by the equality: p12 w2 (1 ± w1 ) = p21 w1 (1 ± w2 )

(10.2)

Substituting the expression (10.1) into this equation, after simple transformations, we obtain (1 ± w1 )/w1 e−βε1 = (1 ± w2 )/w2 e−βε2 ,

(10.3)

where the left part depends on κ1 , and the right on κ2 . This is possible only if both parts of the equality are equal to the same constant value. We denote this value as e−βμ , where μ is the chemical potential. Come to the equation: (1 ± w)/w = eβ(¯ε−μ) ,

(10.4)

in which the average energy of the particle ε¯ according to the formula (8.7) is a functional depending on the distribution function w. Only knowing the dependence of the energy ε¯ on the probability w, it is possible to find the distribution of particles by states. For equilibrium systems of non-interacting particles, (10.4) leads to Fermi–Dirac or Bose–Einstein functions: w = 1/ 1 ± eβ(ε−μ) ,

(10.5)

where the energy ε is the eigenvalue of a single-particle Hamiltonian.

14.11 Conclusion Equation (5.9) given here gives an opportunity to use it to describe the motion of identical particles in various problems of nanophysics. It should be noted that the presence of a dissipative term in this equation leads this equation to a kinetic equation for the probability.

References 1. G. Lindblad, Commun. Math. Phys. 48, 119–130 (1976) 2. B.V. Bondarev, Theor. Math. Phys. 100, 33–43 (1994) 3. B.V. Bondarev. The Method of Density Matrices in the Quantum Theory of Cooperative Phenomena, 2nd edn. (Sputnik+, Moscow, 2013), p. 621 (in Russian) 4. B.V. Bondarev, Phys. A 176, 366–386 (1991)

172

B. V. Bondarev

5. B.V. Bondarev, Vestn. MAI 8, 61–64 (2001) 6. B.V. Bondarev The Method of Density Matrices in the Quantum Theory of Superconductivity, 2nd edn. (Sputnik+, Moscow, 2016), p. 112 (in Russian)

Chapter 15

Crystal Structure and Dielectric Properties of Layered Perovskite-Like Solid Solutions Bi3−x Lux TiNbO9 (x = 0, 0.05, 0.1) with High Curie Temperature S. V. Zubkov and S. I. Shevtsova Abstract The structural and electrophysical characteristics of a number of solid solutions of layered perovskite-like oxides Bi3−x Lux TiNbO9 (x = 0, 0.05, 0.1) have been studied. According to the data of powder X-ray diffraction, all the compounds are single-phase with the structures of two-layer Aurivillius phases) (m = 2) with the orthorhombic crystal lattice (space group A21am). The temperature dependence of the relative permittivity ε/ε0 (T ) compounds have been measured and showed that the Curie temperature of the perovskite-like oxides Bi3−x Lux TiNbO9 increases with the doping parameter x up to T C = 964 °C.

15.1 Introduction The Aurivillius phases (APs) [1–4] are a large family of bismuth-containing layered perovskite-like compounds, the chemical compositions of which are described by the general formula Am−1 Bi2 Bm O3m+3 . The crystal structure of APs is alternating [Bi2 O2 ]2+ layers, between which there are m perovskite-like [Am−1 Bm O3m+1 ]2− layers, where positions A are occupied by ions with large radii [Bi3+ , Ca2+ , Sr2+ , Ba2+ , Y3+ , Pb2+ , Na+ , K+ , Th4+ , Ln3+ , and Lu3+ (lanthanides)] and the positions B inside oxygen octahedra are occupied with ions of small radii (Ti4+ , Nb5+ , Ta5+ , W6+ , Mo6+ , Fe3+ , Mn4+ , Cr3+ , and Ga3+ ). Layered perovskite-like compounds of bismuth oxides of the APs family are promising lead-free materials for applying in piezoelectric devices, in particular, at high temperatures and high frequencies. They demonstrate low temperature coefficients of dielectric and piezoelectric losses, and low aging temperatures, in addition to high Curie temperatures (T C ≤ 965 °C) [5, 6]. In recent years, more attention has been placed on the design and studies of new S. V. Zubkov (B) Research Institute of Physics, Southern Federal University, 194, Stachki Ave, Rostov-on-Don, Russia 344090 e-mail: [email protected] S. I. Shevtsova Institute of Earth Science, Southern Federal University, 40, Zorge Str., Rostov-on-Don, Russia 344090 © Springer Nature Switzerland AG 2020 I. A. Parinov et al. (eds.), Advanced Materials, Springer Proceedings in Materials 6, https://doi.org/10.1007/978-3-030-45120-2_15

173

174

S. V. Zubkov and S. I. Shevtsova

APs [7–11]. The APs such as SrBi2 Nb2 O9 (SBN), SrBi4 Ti4 O15 (SBTi), SrBi2 Ta2 O9 (SBTa), La0.75 Bi3.25 Ti3 O12 (BLT) and so on were accepted as excellent materials for the energy independent ferroelectric memory with small access time (FeRAM) [12–16]. Bi3 TiNbO9 (BTNO) with m = 2 that consists of (Bi2 O2 )2+ layers between which there are (BiTiNbO7 )2− layers [17] is a promising material for fabricating high temperature piezoelectric sensors because of their very high Curie temperature T C (914–921 °C) [5, 17], despite the fact that the piezoelectric modulus of BTNO ceramic is fairly low (d 33 < 7 pC/N) [18]. Numerous examples [19–31] showed that replacements of atoms in A- and also in B-positions of an APs crystal lattice led to the change in the structure, the dielectric properties and significantly influenced the polarization processes in these compounds. In this work, we have synthesized a number of new solid solutions of layered perovskite-like oxides Bi3−x Lux TiNbO9 (x = 0, 0.05, 0.1) in which proportions between amounts of Bi3+ and Lu3+ ions entering in A-position was varied. We have studied their crystal lattices, the dielectric and electrophysical characteristics. The ionic radius of Lu3+ is significantly smaller than the ionic radius of Bi3+ ion, which must lead to significant distortions of the crystal structure of the obtained substitutional solid solutions and influence their dielectric characteristic and the value of Curie temperature, T C .

15.2 Experimental The polycrystalline solid solutions of layered perovskite-like oxides Bi3−x Lux TiNbO9 (x = 0, 0.05, 0.1) have been synthesized by two stage solid phase reaction, consisting of a synthesis stage and a sintering stage. The powders of oxides Bi2 O3 , TiO2 , Nb2 O5 and oxide Lu2 O3 with 99% purity became the starting materials for the synthesis, and were taken in the calculated stoichiometric ratio. After the initial compounds were weighted and preliminarily ground, the synthesis was carried out at a temperature of 860 °C for 6 h. Then, the repeated grinding was performed, and the powder was pressed into 1–1.5 mm thick pellets of a 10 mm in diameter, and the final burning was carried out at a temperature of 1100 °C for 4 h. Structural analysis of the sintered materials was carried out using X-ray DRON3 M diffractometer a BSV21-Cu X-ray tube. The CuK α1,α2 radiation was selected from the total spectrum using a Ni filter. The X-ray diffraction patterns were measured in the range of 2θ angles from 10° to 65° with a pitch of 0.04° and exposure for 4 s. The spectrum profile was analyzed and the line position were determined and their indexing (hkl) according to the chosen unit cell model were performed using the PCW-2.4 program [32]. To perform the electric measurements, Ag–Pd electrodes were deposited on the plane surface of the ceramic samples. The measurements were carried out using an E7-20 LCR immittance meter in the frequency range 100 kHz–1 MHz in the temperature range from room temperature to 980 °C.

15 Crystal Structure and Dielectric Properties of Layered …

175

15.3 Results and Discussion The crystal structure of APs Bi3−x Lux TiNbO9 (x = 0, 0.05, 0.1) was determined by X-ray powder diffraction. The diffraction patterns of all the compounds correspond to the AP phase with m = 2. Figure 15.1 shows the XRD patterns of the Lux samples. It was found that all prepared APs crystallized in the orthorhombic system with unit cell space group A21am (36) (Joint Committee for Powder Diffraction Standard (JCPDS) No. 38-1257) and no other impurity diffraction peaks are observed, which indicates that the Lu ions are successfully entered into the crystal structure of BLuTN. The highest intensity diffraction peaks are referred to the (115) orientation, according to the (112 m + 1) peak of the AP compounds. The highest intensity of the main diffraction peak (115) indicates that all the samples are randomly oriented and polycrystalline. As seen at the inset of Fig. 15.1, the diffraction peak (115) shifts toward higher angle with the increasing x, implying the decrease in the cell volume. Table 15.1 gives the unit cell parameters and volumes, calculated tolerance factors, t, the maximum values of the relative permittivity ε/ε0 at a frequency of 100 kHz 12000

Y Axis Title

115

10000

0.0 0.05 0.1

8000 6000 4000 2000

3000

0 29.0

29.1

29.2

29.3

29.4

29.5

29.6

29.7

135

1113 315

X Axis Title

0210 2010

222

0010

119

200 020

113

008

006

004

Intesity,(a.u.)

28.9

BLuTN-0.1

2000 BLuTN-0,05 1000 pure BTN

0 10

20

30

40

50

60

70

2θ,grad

Fig. 15.1 X-ray diffraction patterns of powders: (1) Bi3 TiNbO9 , (2) Bi2.95 Lu0.05 TiNbO9 , (3) Bi2.9 Lu0.1TiNbO9

Table 15.1 Unit cell parameters a, b, c and volume V, tolerance-factor, t, relative permittivity ε/ε0 at a frequency of 100 kHz, Curie temperature, T C , and activation energy Compound

a, Å

b, Å

c, Å

V, Å3

t

ε/ε0

T C , °C

Bi3 TiNbO9

5.3941

5.4339

25.099

735.67

0.972

1500

921

Bi2.95 Lu0.05 TiNbO9

5.3933

5.43033

25.068

734.176

0.9709

1450

958

Bi2.9 Lu0.1 TiNbO9

5.3923

5.4292

25.0625

733.726

0.97016

800

964

176

S. V. Zubkov and S. I. Shevtsova

5,435

(1)

25,100

5,430

25,095

5,425

25,090 25,085

5,415

c

a,b

5,420

(2)

5,410

25,080 25,075

5,405

25,070

5,400

25,065

5,395

25,060

5,390 0,00

0,02

0,04

0,06

0,08

0,10

0,00

0,02

x

0,04

0,06

0,08

0,10

x

Fig. 15.2 Dependence of the unit cell parameters a, b, c on x in solid solutions Bi3−x Lux TiNbO9 (x = 0, 0.05, 0.1): (1) parameters a, b (Å) and (2) parameter c (Å)

and the Curie temperatures T C . As is seen from Table 15.1, the unit cell volume in the noted series of solid solutions decreases by more than 2.5% as x increases to 0.1 (Fig. 15.2). This is related to the difference in the values of ionic radii in positions A of the perovskite-like layers, where Bi3+ ions are replaced with Lu3+ ions with smaller radius (Bi = 1.38 Å, Lu3+ = 1.1 Å [33]). It can be noted that a decrease in the unit cell volume with an increase in x is due to significant decrease in parameter c along the crystallographic direction [001], whereas, in this case, parameters a and b increase. The changes of the unit cell parameters of the Bi3−x Lux TiNbO9 (x = 0, 0.05, 0.1) solid solutions with the AP structure take place according to the Vegard law (Fig. 15.2). The obtained values of the rhombic b = (b − a)/a and tetragonal c = (c − at )/at deformations (where at = (a + b)/a is the average tetragonal period and c = 3c/(8 + 6m) is the average thickness of the single perovskite layer) (Table 15.2) [4]. As is seen from Table 15.2, the rhombic distortion of the pseudo-perovskite cell of APs substantially decreases as parameter x is varied from 0 to 0.1 as compared to that in undoped Bi3 TiNbO9 . All the APs series demonstrates an increase in the tolerance factor, t, due to a decrease in the amount of Bi3+ ions with the largest ionic radius, while the average tetragonal period at and the average thickness of a single perovskite layer decrease systematically. Table 15.2 Unit cell volume, V, parameter of the tetragonal period, at , octahedron height along c-axis, c , deviation of the unit cell of cubic shape, δc , rhombic distortion, b, relative change in the unit cell volume, (V − V x )/V x , bismuth–oxygen layer, c0 Compound

V, Å3

at , Å

c , Å

δc , %

δb, %

(V − V x )/V x , %

c0 ,

Bi3 TiNbO9

735.67

3.8288

3.765

−1.67

0.732

0.0

3.765

Bi2.95 Lu0.05 TiNbO9

734.176

3.7602

3.7602

−1.73

0.7

0.2

3.7602

Bi2.9Lu0.1TiNbO9

733.72

3.7593

3.776

−1.75

0.661

0.25

3.77593

15 Crystal Structure and Dielectric Properties of Layered …

177

The tetragonal distortion of APs significantly changes in the range of x = 0−0.1; the octahedra are in a compressed state along c-axis in pseudo-perovskite layers. The relative permittivity ε/ε0 and the dielectric loss tangent tanδ were measured in Bi3−x Lux TiNbO9 (x = 0, 0.05, 0.1) at frequencies 100–1000 kHz (Fig. 15.3a–d). All the temperature dependences of the permittivity have sharp maxima, the positions of which are associated with the Curie temperatures, T C of these compounds.

(a) 100kHz 200kHz 500kHz 1MHz

1600 1400

35

921

Bi3TiNbO9

1200

25

e/e0

1000

e/e0

100kHz 200kHz 500kHz 1MHz

30

800

Bi3TiNbO9

20 15

600 10 400 5 200 0 0

100

200 300 400 500 600 700 800 900 1000 1100

0

100

200 300 400 500 600 700 800 900 1000 1100

T,C

T,C

(b)

1600

958 30

1400

100kHz 200kHz 500kHz 1MHz

Bi2.95Lu0.05TiNbO9 1200

Bi2.95Lu0.05TiNbO9

20

800

tgd

e/e0

1000

25

C4 C10 C16 C22

15

600 10 400 5 200 0 0

100

200 300 400 500 600 700 800 900 1000 1100

0

100

200 300 400 500 600 700 800 900 1000 1100

T,C

T,C

(c) 800

964

100kHz 200kHz 500kHz 1MHz

600

e/e0

500 400 300 200 100

0

100

200 300 400 500 600 700 800 900 1000 1100

T,C

tgd

Bi2.9Lu0.1TiNbO9

700

30 28 26 24 22 20 18 16 14 12 10 8 6 4 2 0

Bi2.9Lu0.1TiNbO9

100kHz 200kHz 500kHz 1MHz

0

100

200 300 400 500 600 700 800 900 1000 1100

T,C

Fig. 15.3 Temperature dependence of the relative permittivity ε/ε0 and the loss tanδ for APs Bi3−x Lux TiNbO9 (x = 0, 0.05, 0.1) at 0.1–1.0 MHz: a Bi3 TiNbO9 , b Bi2.95 Lu0.05 TiNbO9 , c Bi2.9 Lu0.1 TiNbO9

178

S. V. Zubkov and S. I. Shevtsova

Correspondingly, the dielectric loss curves have clear minima at the Curie temperature T C . The positions of the dielectric loss maxima are independent of frequency for all APs, which indicate the absence of relaxor properties in these compounds. The maximum Curie temperature T C ≈ 964 °C was obtained for the Bi2.9 Lu0.1 TiNbO9 composition. The Curie temperature T C of the studied APs decreases with an increase in the unit cell parameters a and b and its volume V and decreases with parameter c. This dependence is directly related to the correlation between the tolerance-factor, t and the value of Curie temperature, T C , characteristic of APs [19, 21]. Tolerance factor, t was introduced by Goldschmidt√[34] as a parameter that determines the ionic packing in cubic cells: t = (RA + RO )/ 2(RB + RO ), where RA and RB are cation radii in positions A and B, respectively, and RO is the oxygen ion radius. Later this rule was also used for determination of the stability of the perovskite-like [Am–1 Bm O3m+1 ]2− layers. In this work, we calculated tolerance-factor, t, using the values of the ionic radii by Shannon (O2+ (coordination number (CN) = 6) RO = 1.40 Å; R3+ Bi (CN = 12) = 5+ 4+ (CN = 12) = 1.1 Å, Nb (CN = 6) R = 0.64 Å; Ti (CN = 6) = 1.38 Å; R3+ Nb Lu 3+ 0.605 Å). The ionic radii for the coordination with RBi (CN = 12) and R3+ Lu (CN = 12) are not given in [33], and these values were determined from the dependences of their ionic radii on the coordination numbers extrapolated to the region of high values. As is seen from Table 15.1, the members of the series Bi3−x Lux TiNbO9 (x = 0, 0.05, 0.1) demonstrated dependence of Curie temperature, T C , on the calculated values t of the tolerance-factors, which enables us to predict its value for other values of x. The temperature dependences of the loss tangent tanδ (Fig. 15.3) show the sharp increase in the dielectric losses at high temperatures (>650 °C) for Bi3 TiNbO9 and at lower temperatures (>350 °C) for the Bi3−x Lux TiNbO9 (x = 0, 0.05, 0.1) series. This was due to a high amount of charge carriers, whose concentration sharply increases at high temperatures due to the formation of oxygen vacancies. However, the consideration of the values of tanδ for various APs at a certain temperature, e.g., Curie temperature, T C , showed that they differ by several times, indicating substantially different degrees of imperfection of the APs crystal structure. The obtained values of the activation energies of the charge, E a , in Bi3−x Lux TiNbO9 (x = 0, 0.05, 0.1) are given in Table 15.3 for low- and hightemperature regions. The typical dependence of lnσ on 1000/T, where σ is the specific conductivity that was used for determination of E a is shown in Fig. 15.4 for APs Bi2.9 Lu0.1 TiNbO9 . From Fig. 15.4, it is well seen that there are free temperature Table 15.3 Activation energy (E a ) obtained from the Arrhenius plot Compound

T (E a = 0.05 eV), °C

T (E a = 0.3 eV), °C

T (E a = 0.7 eV), °C

T (E a = 1.1–1.2 eV), °C

Bi3 TiNbO9

20–170

170–300

300–640

640–921

Bi2.95 Lu0.05 TiNbO9

20–280

280–320

320–630

630–958

Bi2.9 Lu0.1 TiNbO9

20–300

300–360

360–730

730–964

15 Crystal Structure and Dielectric Properties of Layered … Fig. 15.4 Dependence of ln σ0 on 1000/T for Bi2.95 Lu0.05 TiNbO9 sample

179

4

Ea1= 1.14eV

2

0

Ea2= 0.7eV

lgσ -2

-4

Ea3= 0.04eV

-6 0,5

1,0

1,5

2,0

2,5

3,0

3,5

1000/T

regions, in which E a has substantially different values. The activation energy, E a , is calculated using the Arrhenius relationship: ρ = ρ0 exp(E a /k B T )ln(σ ) = −(W/k B T ) + ln(σ0 ), where E a is the activation energy of the charge carriers, k B is the Boltzmann constant, and T is the absolute temperature. From this above equation, it can be seen that the relationship between ln ρ and 1/T is a linear relationship. The behavior of activation energy for all compounds can be separated into three temperature regions. The values of activation energy for Bi2.95 Lu0.05 TiNbO9 ceramics in different temperature regions are 0.04, 0.7 and 1.14 eV as shown in Fig. 15.4. The E a value of the Bi2.95 Lu0.05 TiNbO9 ceramic in region I at 1 MHz is 0.04 eV. This value is very similar to the first-ionization energy of oxygen vacancies (VO → VO + e •, ~ 0.1 eV). The values are close to 0.7 eV, consistent with half of the second-ionization energy of oxygen vacancies. By increasing donor additives, the temperature interval with the activation energy E a for pure Bi3 TiNbO9 varies from 20–170 to 20–280 K for Bi2.95 Lu0.05 TiNbO9 and Bi2.9 Lu0.1 TiNbO9 [35, 36]. This is due to the fact that, at high temperatures, intrinsic defects, the formation of which requires high activation energy, are main charge carriers. At low temperatures, the activation energy is mainly determined by impurity defects and has significantly lower values. It should be noted that the value of activation energy for Bi3 TiNbO9 at high temperatures increases with increasing parameter a. For x = 0.1, it actually increases by 2 times compared with a pure compound and becomes higher two times than for all members of the Bi3−x Lux TiNbO9 (x = 0, 0.05, 0.1), whereas their values are comparable at low temperatures. As it was shown in [35–39], the dielectric properties of APs can be substantially dependent on microstructure characteristics of the samples such as the density, the grain sizes, and the porosity of the ceramics. Figure 15.5 shows the electron-microscopy images of the fracture surfaces of the

180

S. V. Zubkov and S. I. Shevtsova

Fig. 15.5 SEM images of the fracture surfaces of a Bi3−x Lux TiNbO9 (x = 0), b Bi3−x Lux TiNbO9 (x = 0.05) and c Bi3−x Lux TiNbO9 (x = 0.1) ceramics

Bi3−x Lux TiNbO9 (x = 0.0, 0.05, 0.1) ceramics. We can see in all the images that the ceramic samples consist of plane grains are characteristic for the APs samples. These plane grains form during their high-anisotropic growth when the growth rate in the direction perpendicular to c-axis is significantly higher than that along c-axis [24]. The grain thickness in the Bi3−x Lux TiNbO9 (x = 0.0, 0.05,0.1) samples is equal to 0.2–0.4 μm, which is an order of magnitude less than their diameter of 20–30 μm. It can be noted as well that the grain sizes increase as the Lu content in the samples increases. The increase in the grain size is associated with formation of intermediate low-melting phases favoring the grain growth at the grain boundaries during their crystallization. The image of a thin cross-section of ceramic (Fig. 15.6) shows the presence of two phases (not in a structural sense). The main phase (light in Fig. 15.6) is close to the estimated stoichiometry ~ Bi2.87 Lu0.04 Ti Nb0.95 O7.7 (the error of the method is 5–10%, rel. Bi = ±0.3, Lu = ±0.02, Ti = ±0.1, Nb = ±0.2, O = ±0.5). The formula is based on the normalization that the number of Ti atoms is equal to unity. The secondary phase (gray in Fig. 15.6) can be represented by the formula Bi15 Lu2 Ti15 Nb5 O63 . Perhaps this is an amorphous phase (see Fig. 15.5). This compound includes not only large pores, but also the surface of microcrystals, which can also be seen from their fuzzy forms in the electron-microscopy images (Fig. 15.5). Since the secondary phase is a dielectric, it can significantly affect the ferroelectric

15 Crystal Structure and Dielectric Properties of Layered …

181

Fig. 15.6 Image of thin cross-section of ceramics

parameters of ceramics. In the remaining samples, an estimated analysis of the composition on ceramic chips was performed. They also found two phases. The main phase with Lux . The secondary phase has approximately the same composition as the sample presented here.

15.4 Conclusion A new series of layered perovskite-like oxides Bi3−x Lux TiNbO9 (x = 0, 0.05, 0.1) has been synthesized. The X-ray diffraction studies show that all the compounds are single-phase and have the APs structure with orthorhombic unit cells (space group A21am). The microstructural study of the synthesized compounds revealed the presence of two phases, one of which is amorphous. The amorphous phase is not only between the crystals, but also covers them and exerts an effect on the growth of the crystals and the dielectric properties. The permittivity was measured to a temperature of 980 °C. The Curie temperature T C increases from 921 °C (x = 0) to 964 °C (for x = 0.1). The value T C = 964 °C for Bi2.9 Lu0.1 TiNbO9 is one of the highest values observed for the perovskite-like bismuth-titanium AP oxides known to date. Acknowledgements This work was financially supported by the Ministry of Science and Higher Education of the Russian Federation (State assignment in the field of scientific activity, Southern Federal University, 2020).

182

S. V. Zubkov and S. I. Shevtsova

References 1. 2. 3. 4. 5. 6. 7. 8. 9. 10. 11. 12. 13. 14. 15. 16. 17. 18. 19. 20. 21. 22. 23. 24. 25. 26. 27. 28. 29. 30. 31. 32. 33. 34. 35. 36. 37. 38. 39.

B. Aurivillius, Arkiv. Kemi. 1, 463 (1949) B. Aurivillius, Arkiv. Kemi. 1, 499 (1949) B. Aurivillius, Arkiv. Kemi. 2, 512 (1950) V.A. Isupov, J. Inorg. Chem. 39, 731 (1994) S.V. Zubkov, V.G. Vlasenko, J. Phys. Solid State 59(12), 2325 (2017) S.V. Zubkov, V.G. Vlasenko, V.A. Shuvaeva, S.I. Shevtsova, J. Phys. Solid State 58(1), 42 (2016) I.A. Zarubin, V.G. Vlasenko, A.T. Shuvaev, Inorg. Mater. 45, 555 (2009) V.G. Vlasenko, A.T. Shuvaev, I.A. Zarubin, V.V. Vlasenko, Phys. Solid State 52, 744 (2010) Z.G. Gai, M.L. Zhao, W.B. Su, C.L. Wang, J. Liu, J.L. Zhang, J. Electroceram 31, 143 (2013) M.A. Bekhtin, A.A. Bush, K.E. Kamentsev, A.G. Segalla, Inorg. Mater. 52, 557 (2016) Z. Zhang, H. Yan, X. Dong, Y. Wang, Mater. Res. Bull. 38, 241 (2003) A. Ando, M. Kimura, Y. Sakabe, Jpn. J. Appl. Phys. 42, 520 (2003) R.Z. Hou, X.M. Chen, J. Mater. Res. 20, 2354 (2005) R.Z. Hou, X.M. Chen, Solid State Commun. 130, 469 (2004) Y. Noguchi, I. Miwa, Y. Goshima, M. Miyayama, Jpn. J. Appl. Phys. 39, 1259 (2000) Y. Yao, C. Song, P. Bao, D. Su, D.X. Lu, J. Appl. Phys. 95, 3126 (2004) R.W. Wolfe, R.E. Newnham, D.K. Smith, Ferroelectrics 3, 11971 (2004) A. Moure, L. Pardo, C. Alemany, J. Eur. Ceram. 21, 1399 (2001) V.G. Vlasenko, S.V. Zubkov, V.A. Shuvaeva, Phys. Solid State 57, 900 (2015) Z.Y. Zhou, X.L. Dong, H. Chen, H.X. Yan, J. Am. Ceram. Soc. 89, 1756 (2006) S.V. Zubkov, V.G. Vlasenko, V.A. Shuvaeva, S.I. Shevtsova, Phys. Solid State 58, 42 (2016) Z.X. Cheng, X.L. Wang, Appl. Phys. Lett. 90, 222902 (2007) R. Aoyagi, H. Takeda, S. Okamura, T. Shiosaki, Mater. Res. Bull. 38, 25 (2003) H.X. Yan, C.G. Li, J.G. Zhou, Jpn. J. Appl. Phys. 40, 6501 (2001) Z.X. Cheng, X.L. Wang, Appl. Phys. Lett. 89, 032901 (2006) Z.G. Gai, J.F. Wang, Appl. Phys. Lett. 90, 052911 (2007) S.J. Zhang, Solid State Commun. 140, 154 (2006) Z.X. Cheng, X.L. Wang, J. Phys. D 43, 242001 (2010) M. Matsushita, R. Aoyagi, H. Takeda, Jpn. J. Appl. Phys. 43, 7164 (2004) R. Aoyagi, S. Inai, Y. Hiruma, T. Takenaka, Jpn. J. Appl. Phys. 44, 7055 (2005) Z.X. Cheng, X.L. Wang, J. Appl. Phys. 107, 084105 (2010) W. Kraus, G. Nolze, Powder Cell for Windows, Version2.3 (Federal Institute for Materials Research and Testing, Berlin (1999) R.D. Shannon, Acta crystallographica Section A. crystal physics. Diffr. Theor. Gen. Crystallogr. 32, 75 (1976) V.M. Goldschmidt, Geochemisca Veterlun (NorskeVidenkap, Oslo, 1927) A. Moure, L. Pardo, J. Appl. Phys. 97, 084103 (2005) H. Zhang, H. Yan, M.J. Reece, J. Appl. Phys. 108, 014109 (2010) V.G. Vlasenko, S.V. Zubkov, V.A. Shuvaeva, K.G. Abdulvakhidov, S.I. Shevtsova, Phys. Solid State 56(8), 1554 (2014) B. Jiménez, L. Pardo, A. Castro, P. Millán, R. Jiménez, M. Elaatmani, M. Oualla, Ferroelectrics 241, 279 (2000) D. Kajewski, Z. Ujma, K. Szot, M. Paweczyk, Ceram. Int. 35, 2351 (2009)

Chapter 16

Fabrication and Investigation of InSb Thin Films for IR SAW Photodetectors M. E. Kutepov, T. A. Minasyan, D. A. Zhilin, V. E. Kaydashev, G. Y. Karapetyan, K. G. Abdulvakhidov, S. I. Shevtsova, and E. M. Kaidashev

Abstract The two-stage pulsed laser deposition growth of thin InSb films on (111) Si and on LiNbO3 YX-128° substrates was studied using a thin InSb buffer layer deposited at a low temperature. This approach improves carrier mobility in InSb base layer, which largely determines the sensitivity of IR photodetectors at room temperature. The response speed in the near-IR range at λ = 985 nm was 1.92 ms, and the decay time was 1.67 ms, under xenon lamp radiation with mechanical modulation. The photosensitivity of the InSb/(111) Si film was about 1 A/W at 293 K. The response time of the sample was~6.8 μs, the time of complete recovery was ~34.5 μs, under laser diode radiation with a wavelength of 840 nm, power 1 mW.

16.1 Introduction Among the AIII BV semiconductors, InSb has the smallest band gap (~0.17 eV) at room temperature and an extremely high electron mobility. Due to these characteristics, InSb is widely used in infrared (IR) optoelectronics, microwave and THz range devices, and magnetic field sensors. Another promising application of thin films, as well as various InSb nanostructures, may be IR surface acoustic wave (SAW) photodetectors. It is well known that in such devices ZnO films and nanorods are widely used for detecting UV radiation. The use InSb thin films and nanostructures as a sensitive element in SAW photodetectors will expand the range of applications of these devices by adding the IR region. InSb is a narrow-gap semiconductor with a low effective mass and has the highest electron mobility among III–V semiconductors. Due to these electronic characteristics, InSb is a good candidate for use in infrared detectors, various high-speed devices, and magnetic sensors [1–3]. M. E. Kutepov · T. A. Minasyan · D. A. Zhilin · V. E. Kaydashev · G. Y. Karapetyan · K. G. Abdulvakhidov · S. I. Shevtsova · E. M. Kaidashev (B) Southern Federal University, 200/1 Stachki Ave, Rostov-on-Don, Russia 344090 e-mail: [email protected] V. E. Kaydashev Moscow Institute of Physics and Technology, 9, Institutskiy, per, Dolgoprudny, Russia 141701 © Springer Nature Switzerland AG 2020 I. A. Parinov et al. (eds.), Advanced Materials, Springer Proceedings in Materials 6, https://doi.org/10.1007/978-3-030-45120-2_16

183

184

M. E. Kutepov et al.

InSb heteroepitaxy on Si substrates is very difficult to achieve due to the large mismatch of the lattice parameters between (approximately 19.3%) these materials. Two main methods are used to solve this problem. The first method uses various buffer layers, such as GaAs and/or Ge [4–6]. In the second method, at the initial stage of growth, surface reconstruction is formed on Si substrates by In and Sb atoms [7, 8]. Some groups [9, 10] managed to grow InSb films on substrates that are very different in structural characteristics (GaAs and Si) using a two-stage growth method. It was shown that this method is more efficient and suitable for most tasks [11, 12]. The method consists of the growth of a low-temperature InSb layer (180–240 °C) and the subsequent growth of a high-temperature InSb layer (350–440 °C) using molecular beam epitaxy. It is well known that films with a better crystalline structure and smaller defects have better electrical characteristics (mobility and carrier concentration, conductivity, etc.). Since the first InSb layer is grown at a relatively low temperature, it is of low quality. Further, the temperature rises (about 350 °C) to spray the second layer with a better crystalline structure. However, the authors of [1] report that the growth temperature of the second InSb layer is limited due to the degradation of the first InSb layer at higher temperatures. The authors of [1] managed to grow an InSb film with high crystal quality and good electrical properties, using a gradual increase in the growth temperature of the second InSb layer during deposition.

16.2 Experimental 16.2.1 Synthesis InSb films were synthesized on YX-128° LiNbO3 piezoelectric substrates and on (111) Si substrates by pulsed laser deposition (PLD). As a target, we used a singlecrystal InSb target of stoichiometric composition. The radiation from an excimer KrF laser (248 nm, 15 ns) was focused on a rotating InSb target (2 × 5 mm2 , energy density 2 J/cm2 ). The YX-128° LiNbO3 substrate (1 × 2) cm2 in size was located at a distance of 5 cm from the target at a temperature of (250–500) °C. The chamber was previously pumped out to a pressure of (2–5) × 10−5 mBar. To improve the structural, electrophysical, and optical properties of thin InSb films on (111) Si substrates, we used a two-stage synthesis method. First, an InSb buffer layer was deposited at a temperature of 250 °C with a thickness h1 = 5–30 nm. Then we deposited the main InSb layer with a thickness h2 = 150–200 nm.

16 Fabrication and Investigation of InSb Thin Films …

185

16.2.2 Study of InSb Thin Films Structure X-ray diffraction studies of thin InSb films on LiNbO3 and (111) Si substrates were carried out on a D2 Phaser Bruker X-ray diffractometer with a position-sensitive detector LYNXEYE with Cu Kα radiation (30 kV, 10 mA, scan step 0.01°). A study of the structure of films on LiNbO3 substrates obtained at synthesis temperatures of 400–475 °C showed that with an increase in the synthesis temperature from 400 to 450 °C, the structure of the films improves, the intensity of the (111) InSb reflection (25.4°) increases, and the (222) reflex appears InSb (52.17°) (Fig. 16.1). This InSb/Si (111) film (Fig. 16.2) was synthesized as follows: a thin InSb buffer layer with a thickness of h1 = 20 nm was sprayed at a low temperature T 1 = 250 °C and a reduced laser pulse repetition rate of 1 Hz, and the main layer with a thickness of h2 = 150 nm was sprayed at a temperature of T 2 = 500 °C and a pulse repetition rate of 10 Hz. The reduced laser pulse repetition rate and the growth temperature of the buffer layer improve its crystalline structure and reduce mechanical stresses. The subsequent growth of the InSb main layer, proceeding on its own sublayer, leads to the formation of a cubic structure with the film predominantly oriented in the (111) direction, with (111) InSb || (111) Si (Fig. 16.2) (Fig. 16.3).

Fig. 16.1 X-ray diffraction patterns of InSb films on LiNbO3 substrates

186

M. E. Kutepov et al.

Fig. 16.2 X-ray diffraction pattern of the InSb film on the Si (111) substrate. h1 = 20 nm, h2 = 150, T1 = 250 °C, T2 = 500 °C

Fig. 16.3 Dependences of the concentration (a) and mobility (b) of charge carriers on the thickness of the first InSb layer

16.2.3 Investigation of the Electrical Properties of Thin InSb Films on LiNbO3 and (111) Si Substrates The concentration and mobility of charge carriers were investigated by van der Pauw method. To study the Hall effect, ohmic contacts made of gold were deposited on the samples by pulsed laser deposition. The current flowing through the sample is measured using a Keithley 2000 multimeter. The magnetic field in the sample is created using two permanent magnets, the value of the magnetic field induction in

16 Fabrication and Investigation of InSb Thin Films …

187

Fig. 16.4 Plot of the photosensitivity of InSb/Si (111) films versus wavelength in the range 650– 1150 nm; h1 —thickness of buffer layer

the gap between them is 0.3 T. The sample is located between the permanent magnets so that the magnetic field is perpendicular to the plane of the sample. The Hall U voltage between the Hall contacts was measured using another Keithley 3 multimeter. The plots of the concentration and mobility of InSb film carriers on the thickness of the buffer layer (Fig. 16.4) show that the maximum mobility and minimum carrier concentration are observed at a buffer layer thickness of 5 nm.

16.2.4 Optical Properties of Thin InSb Films The photosensitivity, the photoresponse times, and the photocurrent decay times of thin InSb/(111) Si films in the near IR range were studied using a monochromator. The change in the resistance of the InSb films was measured using a Keithley 2000. The R/R × 100% dependence on the wavelength for the InSb film (μ = 425 cm2 /V s, n = 2.4 × 1018 cm−3 , ρ = 6 × 10−3 cm) in the range 650–1150 nm is shown in Fig. 16.4. The maximum photosensitivity was observed at a wavelength of λ = 985 nm (Fig. 16.5). The photo-response speed and decay time of a sample with h1 = 5 nm at a wavelength of λ = 985 nm (IR radiation power 1 mW) were measured using a Tektronix TDS 2024B digital storage oscilloscope (Fig. 16.6). IR radiation was modulated with a rotating shutter. The response speed in the near-IR range at λ = 985 nm was 1.92 ms, and the decay time was 1.67 ms. The maximum photosensitivity of the InSb/(111) Si film 1 A/W.

188

M. E. Kutepov et al.

Fig. 16.5 Plot of the photosensitivity of InSb/Si (111) films on the carrier concentration at a wavelength of λ = 985 nm. With increasing carrier concentration, photosensitivity decreases. The concentration and mobility of charge carriers at the maximum are n = 2.43226 × 1018 cm−3 and μ = 425.2504522 cm2 /V s, respectively

Fig. 16.6 Oscillogram of the photo-response (at room temperature) of an InSb film (μ = 425 cm2 /V s, n = 2.4 × 1018 cm−3 , ρ = 6 × 10−3 cm) at a wavelength of λ = 985 nm (IR radiation power 1 mW)

16 Fabrication and Investigation of InSb Thin Films …

189

Fig. 16.7 Photo-response (at room temperature) of sample InSb (111) Si (μ = 425 cm2 /V s, n = 2.4 × 1018 cm−3 , ρ = 6 × 10−3 cm) to the KEM-34 quantum module pulse. The response time of the sample was ~6.8 μs, the time of complete recovery was ~34.5 μs. A response of a pin photodetector DET 10A/M to the KEM-34 quantum module pulse is inserted for comparison

The speed of the sample in Fig. 16.6 is determined by the speed of the modulator. For a more accurate estimation of speed, the sample was irradiated with an IR laser diode (KEM-34 quantum diode module) used to modulate the signals of optical communication lines. Modulation of laser diode radiation with a wavelength of 840 nm, power 1 mW, was carried out by a rectangular pulse generator. The rise time of the response of the sample was ~6.8 μs, the time of complete recovery was ~34.5 μs under laser diode pulse radiation (Fig. 16.7).

16.3 Conclusion A technique has been developed for pulsed laser deposition of InSb thin films on YX-128° LiNbO3 piezoelectric substrates and on (111) Si substrates. The structural, electrical, and optical properties of InSb films were studied. The two-stage growth of thin InSb films on (111) Si substrates was studied using a thin InSb buffer layer deposited at a low temperature, which makes it possible to increase the electronic mobility of the InSb base layer, which largely determines the sensitivity of IR photodetectors at room temperature. The maximum sensitivity was observed for a sample with a thickness of the first layer of 5 nm. The photosensitivity of the InSb/(111) Si film was about 1 A/W at 293 K. The response time of the sample was ~6.8 μs, the time of complete recovery was ~34.5 μs, under laser diode radiation with a wavelength of 840 nm, power 1 mW.

190

M. E. Kutepov et al.

Acknowledgements This research work is supported by Russian Education and Science Ministry, the project No. 16.5405.2017/8.9.

References 1. S. Khamseh, Y. Yasui, K. Nakayama, K. Nakatani, M. Mori, K. Maezawa, Jpn. J. Appl. Phys. 50, 04DH13 (2011) 2. X. Zhu, W. Sun, X. Cao, X. Zhang, L. Zhang, F. Tao, Proc. SPIE 8419, 841915 (2013) 3. T. Zhang, S.K. Clowers, M. Debnath, A. Bennett, C. Roberts, J.J. Haris, R.A. Stradling, L.F. Cohen. Appl. Phys. Lett. 84, 4463 (2004) 4. J.I. Chyi, D. Biswas, S.V. Lyer, N.S. Kumar, H. Morkoc, R. Bean, K. Zanio, H.Y. Lee, H. Chen, Appl. Phys. Lett. 54, 1016 (1989) 5. M. Mori, D.M. Li, M. Yamazaki, T. Tambo, H. Ueba, Appl. Surf. Sci. 104–105, 563 (1996) 6. M. Mori, Y. Tsubosaki, T. Tambo, H. Ueba, C. Tatsuyama, Appl. Surf. Sci. 117–118, 512 (1997) 7. D.M. Li, M. Atoji, T. Okamoto, T. Tambo, C. Tatsuyama, Surf. Sci. 417, 210 (1998) 8. D.V. Gruznev, B.V. Rao, T. Tambo, C. Tatsuyama, Appl. Surf. Sci. 190, 134 (2002) 9. K. Kanisawa, H. Yamaguchi, Y. Huirayama, Appl. Phys. Lett. 76, 589 (2000) 10. M. Mori, M. Saito, Y. Yamashita, K. Nagashima, M. Hashimoto, C. Tatsuyama, T. Tambo, J. Cryst. Growth 301–302, 207 (2007) 11. M. Mori, M. Saito, K. Nagashima, K. Ueda, Y. Yamashita, C. Tatsuyama, T. Tambo, K. Maezawa, Phys. Status Solidi C 5, 2772 (2008) 12. M. Mori, M. Saito, K. Nagashima, K. Ueda, T. Yoshida, K. Maezawa, J. Cryst. Growth 311, 1692 (2009)

Chapter 17

The Investigation of Optical and Dielectric Properties of Ferroelectric BSN Ceramics Doped with Rare-Earth Elements L. V. Grigoryev, A. A. Semenov, and P. Yu Belyavskiy Abstract The chapter presents the results of studies of X-ray diffraction analysis, the temperature dependence of the permittivity, the frequency dependence of ε(T ) and the absorption coefficient of electromagnetic radiation in the frequency band 0.1–1.0 THz for samples of Sr0,61 Ba0,39 Nb2 O6 ceramics doped with rare-earth ions Ce, La, Nd, Yb.

17.1 Introduction Ferroelectric barium-strontium niobate (BSN) ceramics is a solid solution of the composition Srx Ba1−x Nb2 O6 with different variations of the parameter x, lying in the range from 0.25 to 0.75. BSN has the structure of tetragonal tungsten bronze and are uniaxial polar compounds. BSN are typical representatives of relaxor ferroelectrics, which causes interest to them due to the set of their unique electro-optical, pyroelectric, and piezoelectric properties [1–3]. In BSN ceramics, we can control the degree of smearing of the phase transition, its temperature position of transition between the ferroelectric to the paraelectric state, and the optical and electrophysical properties by varying the composition of the ceramic or introducing dopants [4]. From an analysis of the literature data on the electrophysical and electro-optical properties of Srx Ba1−x Nb2 O6 ceramics, it follows that doping of ceramics with rareearth ions leads to an increase in pyroelectric properties, piezoelectric properties, electro-optical and photorefractive characteristics of the material, which makes it possible to successfully use the barium-strontium niobate ferroceramics at MW and THz spectral range, radio photonics devices, dynamic holography devices, optical memory, laser beam control devices and nonlinear optical photonics devices [5–7].

L. V. Grigoryev (B) ITMO University, St. Petersburg, Russia e-mail: [email protected]; [email protected] L. V. Grigoryev · A. A. Semenov · P. Y. Belyavskiy ETU “LETI”, St. Petersburg, Russia © Springer Nature Switzerland AG 2020 I. A. Parinov et al. (eds.), Advanced Materials, Springer Proceedings in Materials 6, https://doi.org/10.1007/978-3-030-45120-2_17

191

192

L. V. Grigoryev et al.

This chapter presents the results of a study of the optical, photoelectric, and dielectric properties of BSN ferroelectric ceramics (x = 0.61) doped with Ce, La, Yb, and Nd ions.

17.2 Sample Preparation The synthesis of samples of BSN ferroelectric ceramics and doped with rare-earth metal ions ceramics BSN: Ln, where Ln is a rare-earth element from a number of lanthanides, was carried out according to the classical ceramic technology of solidphase synthesis from Nb2 O5 , BaCO3 , SrCO3 precursors. Alloying impurities in the form of oxides or nitrates of rare-earth metals: La2 O3 , Nd2 O3 , Yb2 O3 , Ce(NO3 )3 were loaded into the initial charge. The concentration of dopants was set in the range 1.2–1.3%. In order to remove moisture from the feedstock for synthesis, the oxide powders were heated to 150 °C and dried at this temperature for 3 h. Homogenization and grinding of the feedstock for the charge was carried out in a ball mill with agate balls in anhydrous alcohol for 8 h. Next, the charge was dried, polyvinyl alcohol was added to the dried feedstock, and then tablets with a diameter of 15.0 mm and a thickness of 2.5 mm were formed under the pressure of 200 MPa. Pressed tablets were placed in a muffle furnace on a platinum base and sprinkled with powder of the same composition in order to prevent the volatilization of the components during the synthesis. Solid phase synthesis of ferroelectric ceramics was carried out in a muffle furnace in a normal atmosphere. The exposure time of the samples at the synthesis temperature was 2 h. Next, the samples cooled with the furnace. Then, the ceramic samples were ground, and Pt electrodes were deposited on their surface.

17.3 Structural Properties The structural properties of BSN ceramic samples were studied by soft X-ray diffractometry using an DRON-3M automated X-ray diffractometer. Obtaining diffraction X-ray diffraction patterns from ceramic samples without the presence of artifacts on them directly depends on both the choice of the X-ray source and the magnitude of the accelerating voltage applied to the anode of the X-ray tube. The reason for the sharp decrease in the signal-to-noise ratio in the X-ray diffraction pattern, as a rule, is the response of the X-ray photodetector to spurious fluorescence radiation present in the measuring channel of the diffractometer. In this regard, to obtain the correct diffraction pattern, we used an X-ray tube with an anode made of copper. To obtain stable characteristic radiation, the voltage at the anode of the tube should be in the range from 25.0 to 28.0 kV and was chosen equal to 26.0 kV. Given the magnitude of the accelerating voltage applied to the anode of the X-ray tube, Cu-Kα radiation was used. In order to monochromatize X-rays—to isolate the Cu-Kα line from the

17 The Investigation of Optical and Dielectric Properties …

193

output spectrum of a tube, a selectively absorbing β-filter was placed in front of the ceramic sample. The Bragg angles 2θ were measured in the range from 20° to 50° with a step of 2θ = 0.05°. The pulse accumulation time at the measurement point was 15 s; the measurements were carried out at room temperature. As it is known, almost all the physical properties of ceramic samples of ferroelectrics are determined by the degree of defectiveness of their structure. The difference between ceramic and single-crystal ferroelectrics is that the ceramic structure consists of a “mosaic” randomly distributed in the sample volume, from regions in which three-dimensional periodicity in the arrangement of ferroelectric atoms is maintained. In the “mosaic” version of the structure of ferroelectric ceramics of strontium niobate-barium, the size of the coherent scattering (CSR) regions of X-ray radiation can be taken as a measure of the structural defectiveness. In essence, these will be micro-sized areas (mosaic elements). Therefore, based on the estimation of CSR sizes using the Selyakov–Scherrer formula [8], it is possible to estimate the sizes of “mosaic” structural trace elements of a ferroelectric present in the volume of BSN ferroelectric ceramics [9]. The barium-strontium niobates in the concentration variation range x = 0.25–0.75 are single-phase and belong to the structure of unfilled tetragonal tungsten bronze, in which 5/6 cationic positions in the three-dimensional structure are filled. The main structural element of this ferroelectric is a three-dimensional framework of niobium oxide Nb2 O6 , which is formed by joining the vertices of the NbO6 octahedra and forming three types of structural channels along the polar axis: triangular, pentagonal and quadrangular [10]. The general structural formula for the BSN ferroelectric can be represented as the expression A2 B4 C4 Nb10 O30 . In the barium-strontium niobates structure, positions A located inside the quadrangular channels are partially filled with Sr. Positions B inside the pentagonal channels are filled with statistically distributed atoms Ba and Sr. C positions located inside the narrowest channels of a triangular section are not filled with atoms. The presence of the filling of B channels by barium and strontium atoms, obeying a statistical distribution, allows variation in the percentage composition of barium and strontium atoms to affect the relaxing characteristics of a ferroelectric. In addition, the introduction of dopants, the ionic radius of which is commensurate with the ionic radius of barium or strontium atoms, also allows us to widely vary the relaxation characteristics of a ferroelectric, but without changing the percentage composition of barium and strontium atoms. In addition, the introduction of doping atoms into the BSN composition with an ionic radius close to the ionic radii of barium and strontium can lead to the presence of bulk fluctuations in the composition of the ferroelectric. The X-ray diffraction pattern of the synthesized ceramic sample without the introduction of doping impurities is shown in Fig. 17.1. Only a set of reflections corresponding to the BSN material are observed in the X-ray diffraction pattern. The average size of the coherent scattering regions in the studied ceramics amounted to 280 Å in the (001) direction. An analysis of X-ray diffraction data confirmed that the studied samples of barium-strontium niobates ceramic had a structural type of tetragonal tungsten bronze. The unit cell parameters of ceramics had values of a = 12.466 Å and c = 3.954 Å, which is in good agreement with published data [11].

194

L. V. Grigoryev et al.

Fig. 17.1 X-ray diffraction pattern of Sr0.61 Ba0.39 Nb2 O6

17.4 Dielectric Properties The temperature dependences of the permittivity ε were studied in the temperature range from 288 to 400 K at frequencies of 10 kHz, 100 kHz, 1 MHz. The measurements were carried out on the basis of a stand consisting of HIOKI 3535, HIOKI 3533 RLC meters, a specially designed sample holder with a heater and shielded RF inputs, placed in a fore-vacuum cryostat, a programmable precision PID temperature regulator, a thermocouple temperature meter, and a PC controller with special software. All devices were integrated into the command-measuring network of the test bench, which made it possible to measure temperature, heat the sample according to a linear law, and study dielectric characteristics in real time. The heating rate of the sample was 0.2 K/s. The temperature dependence of the permittivity of BSN ceramic samples with a Sr/Ba percentage of 61% (Sr0.61 Ba0.39 Nb2 O6 ) is shown in Fig. 17.2. The measurements were performed at a frequency of 100 kHz, the amplitude was 0.5 V. It can be seen from the figure that the temperature dependence ε(T ) for non-doped barium-strontium niobates ceramics had the form of a monotonic asymmetric with respect to the position of the curve maximum with regions of monotonous growth and sharp decline. The phase transition temperature for undoped ceramics corresponds to 83 °C. The type of temperature dependence of the permittivity, as well as the position of the maximum (phase transition temperature), coincides with published data [12]. Figure 17.3 shows the temperature dependence of the permittivity, measured for ceramic samples of barium-strontium niobates doped with cerium, neodymium, lanthanum, and ytterbium ions. The frequency and amplitude of the sinusoidal signal were the same as measured by ε(T ) for a sample of non-doped BSN ceramics.

17 The Investigation of Optical and Dielectric Properties …

195

Fig. 17.2 Temperature dependence of the permittivity of BSN-61 ceramics

Fig. 17.3 Temperature dependence of the permittivity of BSN: REM ceramic samples: 1-BSN:Ce; 2-BSN:Nd; 3-BSN:La; 4-BSN:Yb

The temperature dependences of the permittivity of the doped samples changed in comparison with Fig. 17.2. For the cerium-doped sample, there is a sharp increase in the dependence ε(T ) and its gentle decline. The position of the maximum shifted significantly to lower temperatures and amounted to 47.6 °C. For the neodymiumand ytterbium-doped samples, the positions of the maxima ε(T ) are close in position:

196

L. V. Grigoryev et al.

for BSN: Nd T max = 61.1 °C, and for BSN: Nb T max = 63.7 °C. However, the form of the temperature dependences ε(T ) for these samples is radically different: the ε(T ) dependence for the BSN: Nd sample has regions of gentle growth and gentle decline, the graph is close to symmetric with respect to the maximum point. For the BSN: Yb sample, the plot of ε(T ) also contains a region of growth and a region of gentle decline, however, the region of growth consists of two regions: a quasilinear region of growth of ε(T ) from 15 to 35 °C and a region of sharp increase in permittivity ε in the range temperatures from 35 °C to the phase transition point. The temperature dependence of the permittivity for a lanthanum-doped sample looks in a separate way. The temperature dependence of the permittivity ε(T ) consists of a growth region consisting of a quasilinear region in the temperature range from 15 to 33 °C, a region of a sharp increase in permittivity in the temperature range from 35 °C to the phase transition point. After the phase transition point, the dependence ε(T ) decreases almost at the same rate as it grows. The temperature position of the maxima of the ε(T ) dependence in the doped samples practically coincides; the phase transition temperatures differ by 2.6°. In addition, the permittivity values for these samples have close values. The lanthanum-doped sample has the highest permittivity; the ε value in the vicinity of the phase transition point is 1.7 times larger than the samples containing neodymium or ytterbium ions and 2.83 times larger than the ε value corresponding to the phase transition point for the sample containing cerium or sample BSN non-doped ceramics. Thus, when the Sr/Ba ratio in the studied ceramics is 61% (BSN-61 ceramics), the alloying of barium-strontium niobates ceramics with rare-earth metal ions, in a percentage ratio of 1.2–1.3%, made it possible to significantly change the phase transition temperature compared to the initial ceramics. The values of the temperature of the phase transition from the type of alloying ions of rare-earth metals are given in Table 17.1. The results of studies of the temperature dependences of the permittivity ε(T ) for lanthanum-doped ceramics are shown in Fig. 17.4. The measurements were performed at frequencies of 10 kHz, 100 kHz, and 1 MHz. From literature data, it is known that in non-doped BSN ceramics, the frequency dependence of the position of the maximum of the permittivity on temperature is characteristic of ferroelectric relaxators [13]. For samples of barium-strontium niobates ceramics doped with rare-earth metal ions, with an increase in the frequency of the measuring signal from 10 kHz to 1 MHz, a shift in the position of the maxima Table 17.1 Effect of doping with rare-earth metal ions on the phase transition temperature in BSN-61 ceramics

Ceramic sample

The concentration of rare earth ions, %

Phase transition temperature, T, °C

BSN-61

0

85

BSN-61: Nd2 O3

1.3

61.1

BSN-61: La2 O3

1.2

59.2

BSN-61: Yb2 O3

1.3

63.7

BSN-61: CeO2

1.3

47.6

17 The Investigation of Optical and Dielectric Properties …

197

Fig. 17.4 Change in the ε(T ) dependence of BSN:La ceramics for different measurement frequencies: 1—the measurement frequency is 10 kHz; 2—measurement frequency is 100 kHz; 3— measurement frequency is 1000 kHz

of the permittivity curves to a region of higher temperatures is observed, and at the same time, the permittivity decreases. Thus, the behavior of the ε(T ) dependence for ceramic samples doped with rare-earth metal ions completely coincides with that described in the literature for relaxor ferroelectrics.

17.5 Optical Properties at THz The spectral dependence of the absorption coefficient in the terahertz spectrum α(ν) for barium-strontium niobates ceramic was studied using a radio-frequency photon generation of THz radiation with a time resolution [9]. The spectral band of the installation was in the range 0.1–1.0 THz. The terahertz radio photon spectrometer is based on the classical scheme: a pulsed IR femtosecond laser was used to pump a direct-gap semiconductor (InAs), which was placed inside a cryostat through which a magnetic field was transmitted from a powerful solenoid. The irradiation of the surface of a direct-gap semiconductor by the incident radiation of a femtosecond IR laser coupled with a magnetic field applied to the semiconductor determined the emission characteristics of the generated electron-hole pair in the semiconductor. Then, terahertz radiation passed through the BSN ceramic sample under study and focused on a nonlinear electro-optical crystal. The polarization of the crystal medium changed in proportion to the absorbed energy of the incident terahertz radiation, which affects the polarization state of the probe beam. The probe beam was subsequently divided

198

L. V. Grigoryev et al.

Fig. 17.5 Scheme of a terahertz radio photon spectrometer with time resolution

by a Wollaston prism into two beams with orthogonal polarizations and the difference in their intensities was recorded using a balanced detector. The waveform was obtained by changing the phase between the pump beam and the reference beam by the operation of the optical delay line. To obtain the desired dependence α(ν), the recorded signal was subjected to Fourier transform to obtain the frequency domain of the transmission spectrum of the sample (Fig. 17.5). The spectral dependences of the absorption coefficient α(ν) of BSN ceramic samples in the terahertz range are shown in Fig. 17.6. The spectral dependence α(ν) for non-doped BSN ceramics in the spectral range of 0.1–1.0 THz is a flat monotonic curve with a region of slight increase in the absorption coefficient in the band of 0.45–0.65 THz. The absorption coefficient for non-doped BSN ceramics does not exceed 15%. A completely different type of dependence α(ν) takes place for ceramic samples doped with rare-earth metal ions. The spectral dependence α(ν) for the lanthanum-doped sample has the form of a monotonically decreasing curve with a plateau region in the spectral band of 0.35–0.9 THz. For neodymium-doped ceramics, the dependence α(ν) has the form of a complex curve consisting of several regions: a monotonically decreasing curve in the band of 0.1–0.5 THz, a plateau region in the band of 0.5–0.6 THz, and a broad peak of insignificant intensity in the band of 0.67–0.75 THz passing into the region of monotonic decay in the band of 0.75–1.0 THz. The spectral dependence of α(ν) for cerium-doped ceramics has the form different from the curves of α(ν) for the previously considered samples. In the 0.1–0.33 THz band, the curve monotonically decreases from 40 to 35% and further, in the 0.33–1.0 THz band, there is a broad peak with a maximum of about 0.6 THz.

17 The Investigation of Optical and Dielectric Properties …

199

Fig. 17.6 Spectral dependence of the absorption coefficient of BSN ceramic samples at the terahertz range: 1-BSN-61; 2-BSN:Nd; 3-BSN:La; 4-BSN:Ce

17.6 Conclusions Doping of BSN ceramics with rare-earth metal ions leads to a significant decrease in the phase transition temperature relative to the temperature position of the phase transition for non-doped ceramics Srx Ba1−x Nb2 O6 , x = 0.61. The influence of rareearth metal ions doping on the behavior of the temperature dependence in BSN ceramics is more significant than a change in the Sr/Ba ratio in the composition of the ceramic. According to published data, a change in the Sr/Ba ratio from 61 to 75% changes the phase transition temperature from 85 to 48 °C. At the same time, when the Sr/Ba ratio is equal to 61% in barium-strontium niobate ceramics, the introduction of rare-earth metal ions in its composition in a percentage ratio of about 1.5% allows one to reduce the phase transition temperature from 85 °C for pure BSN-61 to 61.1 °C when doping ceramics Nd-ions. In the case of introducing Yb-ions into the ceramic composition, the phase transition temperature was 63.7 °C. In the case when lanthanum ions were introduced into the composition of the initial ferroelectric ceramics, the phase transition temperature was 59.2 °C. The greatest shift in the temperature of the phase transition to lower temperatures was found when doping ferroelectric ceramics with cerium ions, in this case the phase transition temperature was 47.6 °C. For all samples of barium-strontium niobate ceramics, both doped with rare-earth metal ions and non-doped (BSN-61), the behavior of the dependence of ε(T ) on the frequency of the measuring signal was studied. For this, the dependences ε(T ) at three frequencies of the sinusoidal measuring signal were studied for all samples: 10 kHz, 100 kHz, and 1 MHz. The amplitude of the measuring signal supplied to the sample was maintained in all cases equal to 0.5 V. In the experiment, all samples

200

L. V. Grigoryev et al.

showed a shift in the position of the maxima of the permittivity curves ε(T ) to higher temperatures with increasing frequency, and at the same time, the permittivity decreased. Thus, the behavior of the ε(T ) dependence for ceramic samples doped with rare-earth metal ions completely coincides with that described in the literature for relaxor ferroelectrics. The study of the spectral dependence of the absorption coefficient α(ν) in all types of the studied samples showed that the introduction of rare-earth metal ions into the Sr0.61 Ba0.39 Nb2 O6 ceramic composition leads to a significant change in the dependence α(ν). The spectral dependence of the absorption coefficient of non-doped BSN ceramics has the form of a flat curve with a region of slight excess. The absorption coefficient for this material lies in the terahertz range of the spectrum in the range of 10–15%. This allows the use of such ceramics as part of THz radiation sensors, only if a layer absorbing submillimeter radiation is deposited on the ceramic surface. The introduction of rare-earth metal ions into the Sr0.61 Ba0.39 Nb2 O6 ceramic composition can significantly increase the absorption coefficient of radiation in the terahertz region of the spectrum and form materials having regions of increased absorption or materials having α(ν) in individual terahertz spectral bands. The introduction of cerium ions makes it possible to synthesize ferroelectric ceramics suitable for creating pyroelectric sensors in the THz range with increased sensitivity in the band of 0.4–0.9 THz. Alloying BSN ceramics with neodymium ions allows one to synthesize a ferroelectric medium for a pyrodetector, which has a uniform sensitivity in the band of 0.5–0.65 THz and an increased sensitivity in the band of 0.7–0.75 THz. The introduction of lanthanum ions into the composition of Sr0.61 Ba0.39 Nb2 O6 ceramics makes it possible to synthesize ferroelectric material suitable for creating pyroelectric sensors in the THz range with uniform sensitivity in the spectral band of 0.35–0.95 THz.

References 1. G.N. Tolmachev, A.P. Kovtun, I.N. Zakharchenko, I.M. Aliev, A.V. Pavlenko, L.A. Reznichenko, I.A. Verbenko. Phys. Solid State 57, 2050 (2015) 2. P.R. Wilmont, R. Herger, B.D. Patterson, R. Windiks, Phys. Rev. B 7, 144114 (2005) 3. K.A. Vorotilov, V.M. Mukhortov, A.S. Sigov, Integrated Ferroelectric Devices. (M. Energoatomizdat, 2011), 175p (in Russian) 4. T.R. Volk, V.A. Salobutin, L.I. Ivleva, N.M. Polozkov, R. Pankrat. M. Veleke, Phys. Solid State 42, 2066 (2000) 5. D.V. Isakov, M.S. Belsley, T.R. Volk, L.I. Ivleva, Appl. Phys. Lett. 92, 032904 (2008) 6. U. Doerfler, R. Piechatzek, T. Woike, M.K. Imlay, V. Wirth et al. Appl. Phys. B 68(5), 843 (1999) 7. D. Kasprowicz, T. Runka, A. Speghini, D. Falcomer, J. García Solé, M. Bettinelli, J. Lumin. 128, 985–987 (2008) 8. A.A. Rusakov, X-ray Analysis of Metals (Atomizdat, Moscow, 1977), 480p (in Russian) 9. V.I. Iveronova, G.P. Revkevich. Theory of X-ray Scattering. (Moscow State University Press, Moscow, 1972), 246p (in Russian) 10. P.B. Jameison, J. Chem. Phys. 48(11), 5048–5057 (1968) 11. T. Tsurumi, Y. Hoshino, J. Am. Ceram. Soc. 72, 278 (1989)

17 The Investigation of Optical and Dielectric Properties … 12. J. Oliver, R.R. Neurgaonkar, L. Corss, J. Appl. Phys. 64(1), 37 (1988) 13. W.H. Huang, D. Viehland, R.R. Neurgaonkar, J. Appl. Phys. 76(1), 490 (1994)

201

Chapter 18

Universal Technique to Determine the Intensity of the Optical Fields, Generated by Laser Interference Meter of Displacements I. P. Miroshnichenko, I. A. Parinov, and V. P. Sizov Abstract Universal technique is proposed in the work. The relationships for determining the intensity of the optical fields generated by the laser interference displacement meter based on a two-way laser interferometer with combined branches and implementing the method of highlighting the surface of the test object are described in detail. The proposed relations allow one to carry out computational and theoretical modeling and study of functional characteristics in the interests of creating new promising optical instruments for measuring the displacements of the surfaces of objects under control.

18.1 Introduction, Problem Statement, Initial Relations and Assumptions Currently, one of the most relevant and promising areas for improving stationary and mobile diagnostic systems is the development of high-precision non-contact measurement tools for measuring the movement of surfaces of control objects to diagnose the state of structural materials and products, for example, when using acoustic active methods of non-destructive testing. There are known high-precision non-contact means for measuring the movement of surfaces of control objects [1–3], based on a two-way laser interferometer with combined branches [4, 5], and implementing the method of highlighting the surface of the control object [6]. They are developed using modern laser technologies and new methods of optical interferometry, scientifically justified [6–8], tested and used in solving various problems [9, 10]. Successful application and further development of these devices is possible when creating a scientific and methodological apparatus that allows for computational and I. P. Miroshnichenko (B) Don State Technical University, Rostov-on-Don, Russia e-mail: [email protected] I. A. Parinov · V. P. Sizov Southern Federal University, Rostov-on-Don, Russia © Springer Nature Switzerland AG 2020 I. A. Parinov et al. (eds.), Advanced Materials, Springer Proceedings in Materials 6, https://doi.org/10.1007/978-3-030-45120-2_18

203

204

I. P. Miroshnichenko et al.

theoretical modeling and research of functional characteristics in the interests of creating new promising optical means for measuring the movement of surfaces of control objects that implement the method of highlighting the surface of the control object. It is the purpose of developing the results described in this chapter. The pointed laser interference displacement meter (see Fig. 18.1) can be represented as optically coupled and sequentially placed coherent electromagnetic radiation source 1, optical system 2, beam splitter 3, reflector 4, and photodetector 5. In this case, the beam splitter with a known amplitude transmission is located in the plane S. The Cartesian coordinate system {x, y, z} is associated with this plane. The reflector is located in a plane S 3 that is under an angle α to the beam splitter and at a distance h from it. The beam splitter receives coherent radiation from a luminous point O’ that is initially determined by coordinates x0 , y0 , z 0 = 0. For example, a sinusoidal diffraction grating can be used as a beam splitter. The photodetectors used to analyze the interference pattern are located in the Fresnel or Fraunhofer zone.

Fig. 18.1 Scheme of the displacement meter

18 Universal Technique to Determine the Intensity of the Optical …

205

This device allows one to determine the movement of the surface of the control object in two cases by creating an interference pattern in the area where the photodetector devices are located. In the first case, when there is a “luminous point” on the surface of the control object, which occurs when the focused laser radiation is reflected and is indicated on the scheme O . In the second case, a reflector is connected to the surface of the control object. In the first case, the parameters of the interference pattern must determine the change of coordinates x0 , y0 , in the second, if x0 , y0 are unchanged, it is necessary to find the values α and h. Thus, to determine the movement of the surface of object, it is necessary to find an electromagnetic field, scattered by the device in the Fresnel zone, where there is an interference pattern and its dependence on the position of a luminous point x0 , y0 or from the parameters characterizing the location of the reflecting surface α and h. The mathematical formulation of the problem is as follows. The electromagnetic field E, H according to the uniqueness of the solution of the boundary value problem must satisfy: (i) Maxwell Equations:

r ot H = iω˜ε0 E; r ot E = −iωμ˜ 0 H,

(18.1)

where μ˜ 0 and ε˜ 0 are the magnetic and dielectric permittivity of vacuum. (ii) Radiation condition: lim

R→∞

∂E + ik E ∂R

= 0.

(18.2)

(iii) Boundary conditions on the surface of the interferometer. It is assumed that the thickness of the beam splitter and its absorption coefficient are zero. It is necessary to solve the electrodynamic problem of determining the intensity of the optical field in the area where the photodetector devices are located, depending on the movement of the “luminous point” and the parameters of the measuring device.

18.2 Relations for Determining the Strength and Intensity of the Electromagnetic Field at Observation Points To determine the distribution of the field intensity in the area of the location of photodetectors, we use Green’s theorem in tensor form, which connects vector fields in different areas of space [11]:

206

I. P. Miroshnichenko et al.

Fs (P ) =

Q s G ss dv +

1 4π

V

[G ss ∇r F r − F s ∇ p G ps ) S

+ εrsm n r G ss εikm ∇i Fk − εrsm n r F s εikm ∇i G ks )]dS.

(18.3)

We impose mixed Dirichlet–Neumann boundary conditions on the Green’s tensor function [12], and also take into account that the electromagnetic field has a transverse character and satisfies the Maxwell equations. Then, the components of the vector E in the observation area can be expressed as tangent components of the electric field strength vector E τ on the surface where the sources are located: (18.4) Here, the dashed indices are referred to theobservation points that we will define in the spherical coordinate system r , , ψ , and the 1, 2, 3 indices are referred to the source points that lie on the surface of the beam splitter (y = 0). The coordinate with the index “1” coincides (with the opposite sign) with the unit normal n¯ to S, external to the area V under consideration. If a spot close to a circle is formed on the beam splitter from the source, it is convenient to enter a cylindrical coordinate system, where “1” → y, “2” → ρ, “3” → ϕ; E s is the covariant vector, E i is the contravariant vector, ∇i is the covariant is the Green’s tensor function that satisfies a non-uniform equation: derivative, ∇ p ∇ p G is + k 2 G is = −4πgis δ r − r ,

(18.5)

where gis is the operator of coordinate transformation: gis =

∂ξv ∂ξv . ∂ x i ∂ x s

(18.6)

In this case, it is performed a summing on ν, and the coordinates ξv are Cartesian. The Green’s tensor function must satisfy the following boundary conditions: N

∇ 1 G 1 S˜ =

D D ∂ N G y S˜ = 0; G 2 S˜ = G 3 S˜ = 0 ∈ S. ∂y

(18.7)

For a round spot on the surface of the beam-splitter, it is convenient to describe the sources in a cylindrical coordinate system {ρ(2), ϕ(3), y(1)}: x = ρ · sin ϕ;

y = y; z = ρ · cos ϕ.

Lam´e coefficients : h ρ = 1, h ϕ = ρ, h y = 1.

(18.8)

18 Universal Technique to Determine the Intensity of the Optical …

207

points are usually defined in a spherical coordinate system Observation r , , : x = r sin sin ; y = r cos ; z = r sin cos .

(18.9)

Lam´e coefficients : h r = 1; h = r ; h ϕ = r · sin . With this in mind, the coordinate conversion operator calculated by (18.6) has the following form: gρr = sin ϕ sin sin ψ + cos ϕ sin cos ψ = sin cos(ϕ − ψ ); gρ = sin ϕr cos sin ψ + cos ϕ cos cos ψ r = r cos cos ϕ − ψ ; gρψ = sin ϕr sin cos ψ − cos ϕr sin sin ψ = r sin sin ϕ − ψ ; gϕr = ρ cos ϕ sin sin ψ − ρ sin ϕ sin cos ψ = ρ sin sin ψ − ϕ ; gϕ = ρ cos ϕr cos sin ψ − ρ sin ϕr cos cos ψ = ρr cos sin ψ − ϕ ; gϕψ = ρ cos ϕr sin cos ψ + ρ sin ϕr sin sin ψ = ρr sin cos ϕ − ψ ; g yr = cos ; g y = −r sin ; g yψ = 0.

(18.10)

By using (18.4), we write the expressions for the th component of the electric field strength: EΘ =

1 4π

D N ϕ D N (E ρ (∇ y G ρΘ − ∇ρ G yΘ ) + E (∇ y G ϕΘ − ∇ϕ G yΘ ))ds.

(18.11)

s

Here: D D N N D D G ρ G y G ϕ = G gρ ; = G g y ; = G gϕ ,

where

(18.12)

208

I. P. Miroshnichenko et al. ∗

∗

eikr eikr eikr eikr + ∗ ; GD = − ∗ , G = r r r r N

(18.13)

r ∗ is the distance between the observation point and the point that is a mirror image of the source point; it is defined by the following expression: (r ∗ )2 = (x − x )2 + (y + y )2 + (z − z )2 = (ρ · sin ϕ − r · sin Θ · sin Ψ )2 + (y + r · cos Θ )2 + (ρ · cos ϕ − r · sin Θ · cos Ψ )2 ;

(18.14)

r is the distance between the observation point and the source point; r 2 = (x − x )2 + (y − y )2 + (z + z )2 = (ρ · sin ϕ − r · sin Θ · sin Ψ )2 + (y − r · cos Θ )2 + (ρ · cos ϕ + r · sin Θ · cos Ψ )2 .

(18.15)

By using (18.10), we write the covariant derivatives, included in (18.11): D D ∇ y G ρΘ = ∇ y G (ρΘ ) [r cos Θ cos(ϕ − ψ )]

∂G D · r · cos Θ · cos(ϕ − ψ / ) ∂y ∂r ∂G D · · r · cos Θ · cos(ϕ − ψ ), = ∂y ∂r =

(18.16)

where ∂r y − y y − r cos = = ; ∂y r r ∂r 1 = ((ρ sin ϕ − r sin sin ψ ) sin ψ + (ρ cos ϕ − r sin cos ψ ) cos ϕ) ∂ρ r 1 = (ρ − r sin cos(ϕ − ψ ); r ∂r 1 = ((ρ sin ϕ − r sin sin ψ )ρ cos ψ − (ρ cos ϕ − r sin cos ψ )ρ sin ϕ) ∂ϕ r ρ = r sin cos(ϕ − ψ ); r y + y y + r cos ∂r ∗ = = . (18.17) ∂y r r Substituting (18.17) and taking into account that obtain:

∂ ∂r

·

eikr r

ikr

= − er 2 (1 − ikr ), we

18 Universal Technique to Determine the Intensity of the Optical … N ∇ρ G yΘ

N ∇ y G ρΘ

209

ikr e 1 = − 2 [ρ − r sin Θ cos(ϕ − ψ )](1 − ikr ) r r

ikr∗ 1 e ∗ − ∗ 2 ∗ [ρ − r sin Θ cos(ϕ − ψ )](1 − ikr ) · r · sin Θ ; (r ) r ikr ∗ eikr e y − r · cos Θ y + r · cos Θ ∗ + ∗ 2 (1 − ikr ) · = − 2 (1 − ikr ) r r (r ) r∗ × ρ · r · cos Θ · sin(ψ − ϕ);

eikr 1 N · (1 − ikr ) · ρ · r · sin Θ sin(ϕ − ψ ) · r · sin Θ ; ∇ϕ G yΘ = −2 2 r r ikr ∗ e 1 eikr D ∇ y G ρΘ = − 2 · (1 − ikr ) · · (y − r cos Θ ) + ∗ 2 · (1 − ikr ∗ ) r r (r ) 1 · ∗ (y + r cos Θ ) × r · cos Θ · cos(ϕ − ψ ). r

(18.18)

The expression for the th component of the electric field strength is defined as: N N ∇ρ G y = ∇ρ G (y ) · (−r · sin ) = −

∂G N · r · sin ∂ρ

∂r ∂G N · · r · sin ; ∂ρ ∂r D = ∇ y G (ϕ· ) ρ · r · cos · sin(ψ − ϕ) =−

D ∇ y G ϕ·

∂G D · ρ · r · cos · sin(ψ − ϕ) ∂y ∂r ∂G D · ρ · r · cos · sin(ψ − ϕ); = ∂ y ∂r =

N N ∇ϕ G y· = ∇ϕ · G (y· ) · (−r · sin ) = −

=−

(18.19)

∂G N · r · sin ∂ϕ

∂r ∂G N · · r · sin . ∂ϕ ∂ϕ

(18.20)

Substituting (18.20) into (18.11) at y = 0 and using the Lamé coefficients for cylindrical (18.8) and spherical (18.9) coordinate systems, we consider the physical components of the vector E. The expression for determining the th component of the electric field strength vector has the form: E (Θ )

r eikr cos2 Θ cos(ϕ − ψ ) 2 2 (1 − ikr ) E (ρ) r r s ρ r 2 − sin Θ + sin Θ cos(ϕ − ψ ) r r

1 = 4π

210

I. P. Miroshnichenko et al.

+E (ϕ)

r r · cos2 Θ · sin(ψ − ϕ) − · sin2 Θ · sin(ϕ − ψ ) r r

ds;

(18.21)

r eikr ρ cos(ϕ − ψ ) − sin · (1 − ikr ) · E (ρ) 2 r r r s

r (18.22) +E (ϕ) · · sin(ψ − ϕ) ds. r

E ( ) =

1 2π

Similarly, we can write for the th component of the vector E at the observation point: Eψ =

1 4π

D N ϕ D N [E ρ (∇ y G ρ·ψ (18.23) − ∇ρ G y·ψ ) + E (∇ y G ϕ·ψ − ∇ϕ G y·ψ )]ds,

s

where D D D ∇ y G ρ·ψ = ∇ y G (ρψ ) gρψ = ∇ y G (ρψ ) · r · sin · sin(ϕ − ψ )

eikr r · cos · r · sin(ϕ − ψ ) · sin ; · (1 − ikr ) · r2 r eikr 1 = −2 · 2 · (1 − ikr ) · [ρ − r sin cos(ϕ − ψ )] · 0 = 0; r r eikr r = 2 · 2 · (1 − ikr ) · · cos · ρ · r · sin · cos(ϕ − ψ ); r r = 0. (18.24) =2·

N ∇ρ G yψ D ∇ y G ϕψ N ∇ϕ G yψ

The expression for determining the th component of the electric field strength vector will have the following form: E (ψ )

E (ψ ) =

1 2π

s

eikr r cos Θ sin(ϕ − ψ ) · (1 − ikr ) · E · (ρ) r2 r s

r +E (ϕ) · · cos Θ · cos(ϕ − ψ ) ds; r

1 = 2π

eikr r · cos Θ · E (ρ) · sin(ϕ − ψ ) + E (ϕ) cos(ϕ − ψ ) ds. · (1 − ikr ) · 2 r r

(18.25) (18.26)

Thus, to determine the field in the observation area, we need to know the field on the surface of the beam-splitter. For the case of placing the photodetector in the far zone, we can put r = r = R0 in the amplitude multiplier. Taking into account only the terms with the first degree (1/R0 ) in the amplitude and leaving the difference of the stroke in the phase multiplier r and r , we get:

18 Universal Technique to Determine the Intensity of the Optical …

E (Θ )

ik eik R0 =− · R0 2π

ρ0 2π 0

E (ρ) · cos(ϕ − ψ )

0

−E (ϕ) · sin(ϕ − ψ ) e−ik·ρ·sin Θ ·cos(ϕ−ψ ) ρdρdϕ;

E (Ψ )

ik eik R0 =− · R0 2π

ρ0 2π 0

211

(18.27)

cos Θ · e−ik·ρ·sin Θ ·cos(ϕ−ψ ) · E (ρ) sin(ϕ − ψ )

0

+E (ϕ) · cos(ϕ − ψ ) ρdρdϕ.

(18.28)

The intensity distribution in the observation area can be determined using the formula: I = E · E + E · E ,

(18.29)

where E , E are the complex conjugate values to E , E . By using the relations (18.22) and (18.26), we can calculate the distribution of the intensity of the optical field at any point of space y > 0. By using the Formula (18.27) and (18.28), we can find the field at points remote from the surface of the beam-splitter at a distance corresponding to the far zone. To do this, it is necessary to find the components of the electric field vector tangent to the beam-splitter surface. The field can be represented as a field falling on the surface of the beam-splitter and a mirror-reflected field. A falling field is a field from a source that can be represented as a round hole. The reflected field can be determined using the image method [13], taking into account the beam splitter’s transmittance.

18.3 Relations for Determining the Field Falling on the Beam-Splitter Surface Let us find the calculated relations for determining the field falling from the source to the beam splitter surface using a spherical coordinate system. The source of the field is represented as the radiation of the source passing through a circular aperture with a radius a that is in the plane y˜ = 0 (Fig. 18.2). Consider two cases of polarization of a plane wave falling on a circular diaphragm in perpendicular and in parallel: (i) at polarization along z˜ − axis, we get E = k · E z ;

(18.30)

(ii) at polarization along x˜ − axis, we get E = i · E x .

(18.31)

To solve the problem, we introduce two coordinate systems (cylindrical and spherical) with the beginning at the center of the diaphragm (Fig. 18.2). The polar

212

I. P. Miroshnichenko et al.

Fig. 18.2 Calculation scheme

coordinate system {ρ, ˜ ϕ} ˜ is related to the Cartesian coordinate system {x, ˜ z˜ } as follows: x˜ = ρ˜ sin ϕ; ˜ z˜ = ρ˜ cos ϕ. ˜

(18.32)

We write the tangent components E ρ˜ and E ϕ˜ in the plane y = 0 for perpendicular polarization, through (18.30), or parallel polarization, through (18.31), using a formula coupling the components of vectors in different orthogonal coordinate systems: E k¯ h k¯ =

∂xm Em hm , ∂ x¯ k

(18.33)

where E k¯ and E m are the physical components of the vector E in different coordinate systems, respectively, hi are the corresponding Lamé metric coefficients. In this case, the index k is referred to a cylindrical coordinate system, and the index m is referred to a Cartesian coordinate system. Lamé coefficients in a cylindrical coordinate system have the form: h ρ = 1; h ϕ = ρ; h y = 1.

(18.34)

18 Universal Technique to Determine the Intensity of the Optical …

213

I. For perpendicular polarization:

∂ z˜ E z h z → E ρ = E z cos ϕ; ˜ ∂ ρ˜ ∂ z˜ E z h z → E ϕ = −E z sin ϕ. ˜ Eϕ hϕ = ∂ ϕ˜ Eρ hρ =

(18.35)

Cylindrical components E ρ , E ϕ in the opening of the diaphragm, are the sources of the field that falls on the beam-splitter. To determine the field falling on diaphragm we can use the relations (18.22) and (18.26), which couple E τ on some surface (in this case, the diaphragm aperture) and field at observation points (in this case, the points on the surface of the beam splitter). To do this, substitute (18.35) in the expressions (18.22) and (18.26), assuming that E z = const = 1, and we get: E =

1 2π

eikr r ρ ds; · cos ψ · cos ϕ · sin · (1 − ikr ) · − r2 r r

S

Eψ

1 = 2π

eikr r · cos · sin ds, · (1 − ikr ) · r2 r

(18.36)

(18.37)

S

where r is the distance between the diaphragm aperture points and the observation points, r is the distance between the center of the spherical coordinate system and the observation points. The beginning of this spherical coordinate system is located at the center of the diaphragm aperture and differs from the spherical coordinate system introduced earlier in (18.9). Assuming in the amplitude multiplier r = r and kr 1, we have: ik 1 ρ E Θ˜ = − · eikr · cos ψ˜ − · cos φ˜ · sin Θ˜ ds r 2π r S ik 1 ik 1 = − · cos ψ˜ · eikr ds + 2 · cos Θ˜ · eikr · ρ · sin φ˜ · ds; r 2π (r ) 2π S

E ψ˜ =

S

ik 1 · cos · sin ψ · r 2π

(18.38)

eikr ds.

(18.39)

S

or, neglecting the second term in (18.38), we get expressions for spherical components of the electric field strength:

214

I. P. Miroshnichenko et al.

E ˜ = −

ik 1 · cos ψ˜ · r 2π

eikr ds; S

E ψ˜

ik 1 ˜ · sin ψ˜ · = · cos r 2π

(18.40)

eikr ds.

(18.41)

S

II. Similarly, for the parallel polarization, instead (18.35), we have:

E ρ = E x · sin ϕ;

E ϕ = E x · cos ϕ.

(18.42)

and instead (18.40) and (18.41), we have: E Θ˜ = −

ik 1 · sin ψ · r 2π

eikr ds; S

E ˜

ik 1 = · cos · cos ψ · r 2π

(18.43)

eikr ds.

(18.44)

S

Consider the integral in these expressions: I =

eikr ds,

(18.45)

S

where r = (ρ sin ϕ − r sin sin ψ )2 + (r cos )2 + (ρ cos ϕ − r sin cos ψ )2 ; ρ 2 sin2 ϕ − 2ρr sin ϕ sin sin ψ + r 2 sin2 sin2 ψ + r 2 cos2 + ρ 2 cos2 ϕ − 2ρr cos ϕ sin cos ψ + r 2 sin2 cos 2 ψ = ρ 2 − 2ρr sin cos(ϕ − ψ ) + r 2 sin2 + r 2 cos2 = r 2 = ρ 2 − 2ρr sin cos(ϕ − ψ ) + r 2 .

(18.46)

Then a 2π I =

eik 0

0

r ≈r

√

ρ 2 −2ρ·r ·sin ·cos(ϕ−ψ )+(r )2

1−

For the Fresnel zone, we have:

ρdρdϕ;

2ρ sin cos(ϕ − ψ ). r

(18.47)

18 Universal Technique to Determine the Intensity of the Optical …

215

ρ r = r 1 − sin cos(ϕ − ψ ) ; r

(18.48)

I =e

ikr

a 2π 0

e−ik·ρ·sin ·cos(ϕ−ψ ) ρdρdϕ.

0

Due to [14]: 2π

e−ikρ sin

cos(ϕ−ψ )

dϕ = 2π J0 (kρ sin ),

(18.49)

0

then we have: I =e

a

ikr

ρ2π J0 (kρ sin )dρ = eikr 2π

0

a J1 (ka sin ), k sin

(18.50)

where J1 is the Bessel function of 1st order. Substituting (18.50) into (18.40) and (18.41), we get for perpendicular polarization: I.

EΘ

eikr a cos ψ = −i J1 (ka sin Θ ) = −A cos ψ ; r sin Θ

(18.51)

Eψ = i

eikr a cos sin ψ J1 (ka sin ) = A cos cos ψ . r sin

(18.52)

Similar for parallel polarization, we get: II.

E Θ = −i

eikr a sin ψ J1 (ka sin Θ ) = −A sin ψ ; r sin Θ

(18.53)

Eψ = i

eikr a cos cos ψ J1 (ka sin ) = −A cos cos ψ , r sin

(18.54)

where

A=i

eikr a J1 (ka sin ) . r sin

(18.55)

216

I. P. Miroshnichenko et al.

Relationships (18.51)–(18.55) determine the field that passed through the diaphragm, and they can be used to calculate the field falling on the surface of the beam-splitter at different polarizations.

18.4 Relations for Determining the Total Field on Beam-Splitter Surface To determine the distribution of light intensity in the observation area, it is necessary to calculate the field on the surface of the beam-splitter, which consists of the falling field found in Sect. 18.3 and the field of the imaginary source. To solve this problem, it is convenient to introduce three local Cartesian coordinate systems {x, y, z} and the spherical coordinate systems {r, , ψ} coupled with them, having origins at points O, O , O . Coordinates without strokes are referred to the coordinate systems with origins on the beam-splitter surface at a point O; coordinates with one stroke correspond to the coordinate systems at a point O located at the center of aperture; and two strokes are referred to a coordinate system with an origin at the center of the mirror source O (Fig. 18.3). It is necessary to determine the tangent components of the falling field on the surface y = 0 in a cylindrical coordinate system with the origin at a point O. Therefore, knowing E ˜ , E ˜ , Er˜ ≈ 0 let us go to E ρ and E ϕ . The relationship between the entered coordinate systems is defined as follows. The coordinate system {x , y , z } is obtained by rotating around the z-axis by an angle α 0 in the positive direction and then parallel translation on (−x 0 ) and y0 , respectively (see Fig. 18.3). The coordinate system {x , y , z } is mirrored with respect to {x , y , z }, where the y-axis direction is changed to opposite. This system is derived from {x, 0 + 2α)] and parallel shear along the x-axis on y, z} by turning on an angle[−(α −x0 and along the y-axis on −y0 . The relationships between these coordinate systems and the main coordinate system are as follows: x = (x + x0 ) cos α0 + (y − y0 ) sin α0 ; y = −(x + x0 ) sin α0 + (y − y0 ) cos α0 ; z = z.

(18.56)

x = x + x0 cos(α0 + 2α) − y + y0 sin(α0 + 2α); y = x + x0 sin(α0 + 2α) + y + y0 cos(α0 + 2α); z = z, where x0 = x0 cos 2α + 2h sin α + y0 sin 2α;

(18.57)

18 Universal Technique to Determine the Intensity of the Optical …

217

Fig. 18.3 Calculation scheme

y0 = −x0 sin 2α + 2h cos α + y0 sin 2α.

(18.58)

In these expressions, the values of the parameters x 0 , y0 , α 0 and α, h, respectively, determine the position in space of the luminous point and the reflecting surface; they are clear from Fig. 18.3. The Cartesian coordinates with origin at a point O are expressed in spherical coordinates with origin at the point O : x = r · sin · sin ; y = r · cos ; z = r · sin · cos .

(18.59)

Cartesian coordinate system can be expressed in terms of a basic cylindrical coordinate system {y, ρ, ϕ} that is coupled with a point O: x = ρ sin ϕ;

y = y; z = ρ cos ϕ.

(18.60)

From the Formula (18.56), we express the relationship of the main Cartesian coordinate system with the entered Cartesian coordinate system with the origin at

218

I. P. Miroshnichenko et al.

the point O : x = −x0 + x · cos α0 − y · sin α0 ; y = y0 + x · sin α0 − y · cos α0 ; z = z.

(18.61)

Substitute (18.59) into (18.61) and get the relations that connect the main Cartesian coordinate system and the spherical coordinate system with the origin at the point O: x = −x0 + r sin sin cos α0 − r cos ; y = y0 + r sin sin sin α0 + r cos cos α0 ; z = r sin cos .

(18.62)

Substitute (18.62) into (18.60) and get relations, defining cylindrical coordinates centered at the point O, through Cartesian coordinates centered at the point O : ρ sin ϕ = −x0 + x cos α0 − y sin α0 ; ρ cos ϕ = z ; y = y0 + x sin α0 + y cos α0 .

(18.63)

Let us express cylindrical coordinates centered at a point O through spherical coordinates centered at a point O : y = y0 + r sin sin sin α0 + r cos cos α0 ; −x0 + r sin sin cos α0 − r cos sin α0 x tgϕ = = ; z r sin cos ρ = r 2 sin 2 cos2 + (−x0 + r sin sin cos α0 − r cos sin α0 )2 . (18.64) Let us express spherical coordinates centered at a point O through cylindrical coordinates at a point O: r =

ρ 2 + 2ρx0 sin ϕ + x02 + (y − y0 )2 ;

(ρ sin ϕ + x0 ) cos α0 + (y − y0 ) sin α0 ; ρ cos ϕ −(ρ · sin ϕ + x0 ) sin α0 + (y − y0 ) cos α0 cos = . ρ 2 + 2ρ · x0 sin ϕ + x02 + (y − y0 )2

tg =

(18.65)

The electromagnetic radiation of the laser passed through a circular diaphragm and polarized along the x -axis in a spherical coordinate system with the origin at

18 Universal Technique to Determine the Intensity of the Optical …

219

a point O was obtained above (18.53) and (18.54). Next, we need to get a falling field expressed in a cylindrical coordinate system with the origin at a point O. This requires the transverse components of the vector E: Eρ =

∂ h ∂ h E + E ; ∂ρ h ρ ∂ρ h ρ

Eϕ =

∂ h ∂ h E + E , (18.66) ∂ϕ h ϕ ∂ϕ h ϕ

where h = r ; h ρ = 1; h ϕ = ρ; h ϕ = ρ; h = r · sin · ; h y = 1.

(18.67)

Define the necessary components of expression (18.66): ∂ ∂ρ ∂ ∂ρ

h hϕ h hρ

= r ∂ ; ∂ρ = r sin ∂ψ ∂ρ

∂ ∂ϕ ∂ ∂ϕ

h hϕ h hϕ

= =

r ∂ ; ρ ∂ϕ r sin ∂ ρ ∂ϕ

(18.68)

From (18.65) we have: r =

ρ 2 + 2 · ρ · x0 · sin ϕ + x02 + (y − y0 )2 ;

= arccos

−(ρ sin ϕ + x0 ) sin α0 + (y − y0 ) cos α0 y = arccos . r ρ 2 + 2ρx0 sin ϕ + (y − y0 )2

(18.69)

Derivatives in (18.66) have the forms: ∂ψ = ∂ρ = ∂Ψ h Ψ = ∂ρ h ρ

∂Ψ = ∂ϕ

1+ ρ2

1 (ρ sin ϕ+x0 ) cos α0 +(y−y0 ) sin α0 ρ cos ϕ

2

−x0 cos ϕ cos α0 + (y − y0 ) sin α0 cos ϕ ; ϕ + [(ρ sin ϕ + x0 ) cos α0 + (y − y0 ) sin α0 ]2

cos2

r 2 − y 2 · [−x0 · cos ϕ · cos α0 − (y − y0 ) · sin α0 · cos ϕ] ; (18.70) ρ 2 cos2 ϕ + [(ρ · sin ϕ + x0 ) cos α0 + (y − y0 ) sin α0 ]2

1

(ρ sin ϕ+x0 ) cos α0 +(y−y0 ) sin α0 2 1+ ρ cos ϕ

ρ · cos ϕ · ρ · cos ϕ · ρ cos α0 + ρ · sin ϕ[(ρ · sin ϕ + x0 ) cos α0 + (y − y0 ) sin α0 ] ρ 2 cos2 ϕ ρ 2 · cos α0 + ρ · x0 sin ϕ · cos α0 + ρ(y − y0 ) sin ϕ · sin α0 = ; ρ 2 · cos2 ϕ + [(ρ · sin ϕ + x0 ) cos α0 + (y − y0 ) sin α0 ]2 r 2 − y 2 [ρ · cos α0 + x0 sin ϕ · cos α0 + (y − y0 ) sin ϕ · sin α0 ] ∂Ψ h Ψ = ; (18.71) ∂ϕ h ϕ ρ 2 · cos2 ϕ + [(ρ · sin ϕ + x0 ) cos α0 + (y − y0 ) sin α0 ]2 =

220

I. P. Miroshnichenko et al.

∂ h r [−(ρ sin ϕ + x0 ) sin α0 + (y − y0 ) cos α0 ](ρ + sin ϕ) sin ϕ · sin α0 + ; = ∂ρ h ρ (r )2 r 2 − y 2

(18.72)

∂ h 1 [−(ρ sin ϕ + x0 ) sin α0 + (y − y0 ) cos α0 ]x0 cos ϕ cos ϕ · sin α0 · r + . = ∂ϕ h ϕ r r 2 − y 2

(18.73)

Thus, the following field falling from the diaphragm, expressed in the components of the cylindrical coordinate system, takes place on the surface y = 0:

– (18.74)

–

–

–

– – (18.75) where r¯ =

ρ 2 + 2 · ρ · x0 sin ϕ + x02 + y02 ;

x¯ = (ρ · sin ϕ + x0 ) cos α0 − y0 sin α0 ; y¯ = −(ρ · sin ϕ + x0 ) sin α0 − y0 cos α0 .

(18.76)

Expressions for the field of imaginary source are obtained similarly to the falling field from the aperture, only in formulae (18.74)–(18.76), it is necessary to replace one stroke with two, and instead x0 , y0 , α0 substitute them on x0 , y0 , −(α0 + 2α), respectively: y¯ (ρ + x0 sin ϕ) r¯ E ρ3 = sin ϕ · sin(−α0 + 2α) + E (¯r )2 (¯r )2 − ( y¯ )2

(¯r )2 − ( y¯ )2 · −x0 cos ϕ · cos(−α0 + 2α) − y0 cos ϕ · sin(−α0 + 2α) + E ; ρ 2 cos2 ϕ + (x¯ )2 y¯ · x0 sin ϕ r¯ E ϕ3 = cos ϕ · sin(−α0 + 2α) + E (¯r )2 (¯r )2 − ( y¯ )2

(18.77)

18 Universal Technique to Determine the Intensity of the Optical … +

221

(¯r )2 − ( y¯ )2 · ρ · cos(−α0 + 2α) + x0 · sin ϕ · cos(−α0 + 2α) − y0 sin ϕ · sin(−α0 + 2α) ρ 2 cos2 ϕ + (x¯ )2

E ,

(18.78)

where x0 = x0 cos 2α + 2h sin α + y0 sin 2α; y0 = −x0 sin 2α + 2h cos α + y0 sin 2α.

(18.79)

The total field on the surface of the beam-splitter can be written as the sum of the field falling from the source that is passed through the diaphragm, and the field from the imaginary source that is diffracted on the beam-splitter: (18.80) where T (ρ, ϕ) is the amplitude transmission of the beam-splitter. Thus, the relationships to determine the field distribution on the surface of beamsplitter of laser interferometer are obtained. The field distribution is presented in the form of the tangential components of the electric field strength vector E ρ and E ϕ , expressed in cylindrical coordinates, taking into account the diffraction at a circular aperture and transmittance of the beam-splitter.

18.5 Relations for Determining the Field and Intensity in the Location Area of Photodetectors in the Case of Using Sinusoidal Diffraction Grating as Beam-Splitter Thus, we can say that in Sect. 18.3 the calculated relations were found for determining the field falling from the source on the beam-splitter surface using a spherical coordinate system. In Sect. 18.4, we obtained the relations for determining the field on the surface of the beam-splitter of a laser interferometer, which are represented as tangent components of the electric field strength vector E ρ and E ϕ , expressed in cylindrical coordinates, taking into account the diffraction on the round hole and the transmission coefficient of the beam-splitter. Now consider the case when a sine wave grating with a period τ and transmittance T (x, z) is used as a beam-splitter. If the beam-splitter is fully illuminated, then the surface of the interferogram is rectangular and in this case, it is convenient to use a Cartesian coordinate system. In this regard, it is necessary to make a transition from formulae (18.27) and (18.28) with components E and E , expressed in cylindrical coordinates to formulae with the same components expressed in Cartesian coordinates. With this aim, we define E ρ and E ϕ through E x and E z :

222

I. P. Miroshnichenko et al.

E ρ = E z · cos ϕ + E x · sin ϕ; E ϕ = −E z · sin ϕ + E x · cos ϕ.

(18.81)

So, expressions (18.27) and (18.28) take the forms: E

(Θ )

E (ψ )

r eikr z cos ψ − sin Θ · (1 − ikr ) · E z r2 r r s r x · sin ψ − · sin Θ ds; +E x · r r ikr e 1 r = · (1 − ikr ) · · cos Θ · (E x · cos ψ − E z sin ψ )ds. 2 2π r r 1 = 2π

s

(18.82) If the interference pattern is observed in the far zone, and the source is located near the y-axis in the Fresnel zone, then the formulae for calculating the transverse components of the vector E have the forms: E Θ⊥ = A0 · cos ψ · U (Θ, ψ); E Ψ ⊥ = −A0 · cos Θ · sin ψ · U (Θ, ψ);

(18.83)

E Θ|| = A0 · sin ψ · cos α0 · U (Θ, ψ); E Ψ || = −A0 · cos ψ · cos Θ · cos α0 · U (Θ, ψ).

(18.84)

Here U (θ, ψ) = U0

U (x, z)e

2

ik x 2R+z 0

2

e−ik sin θ(x sin ψ+z cos ψ) ds,

(18.85)

S

where U (x, z) is the complex amplitude of the wave field; θ, ψ, R0 are the spherical coordinates of observation points; x, z are the coordinates of source points that locate on the surface of the beam splitter (Fig. 18.1). Expression (18.85) includes a function U (x, z) describing the optical field in the plane of the beam-splitter. To determine it, we use the image method [13], when the total field on the surface of the beam splitter is represented by a superposition of waves from a luminous point x0 , y0 and an imaginary mirror point formed by the reflector, and it is necessary to take into account the amplitude transmission of the beam splitter. In accordance with the image method expressions for the complex amplitude of the light field on the surface of the beam splitter can be written as follows:

U (x, z) = A0 eikr − T (x, z)eikr , where for the Fresnel zone:

(18.86)

18 Universal Technique to Determine the Intensity of the Optical …

223

2 2 2 x + x0 − x0 + z 2 (x + x0 )2 − x02 + z r = r0 + ; r = r0 + ; 2r0 2r0 r0 = x02 + y02 , (18.87)

where A0 is a constant, T (x, z) is the amplitude transmission of the beam-splitter. Substituting (18.86) and (18.87) in (18.85), as well as specifying T (x, z), we get the ratio for calculating the field at the observed points. The intensity to which the photodetector reacts is equal to the square of the expression module (18.85). Consider the case where the field does not depend on z, and a sinusoidal lattice is used as the beam-splitter. Diffraction by a sinusoidal grating, as is known, leads to the formation of maxima of the first order (m = ±1). In this regard, it is advisable to place photodetectors in the regions corresponding to these maxima and consider the interference pattern in these directions, which is formed by the falling wave and the waves diffracted on the lattice. To do this, we write the optical field in space y > 0 in accordance with (18.85) as follows (the amplitude multiplier is omitted here):

U1 =

d

x2 λ ik eikr + e±ik τ x eikr e 2R0 e−ikx sin θ dx,

(18.88)

−d

where τ is the period of the lattice, and the sign in the exponent of the second term is taken in accordance with the considered main maximum. Substituting the values from (18.87) into this expression, we get the ratio for calculating the complex amplitude of the wave field in the form:

U1 = eikr0 J1 + eikr0 J2 ,

(18.89)

where d J1 =

e

x i k 2r1 + 2R1 x 2 +k r 0 −sin θ x 0

0

0

dx;

(18.90)

−d

d J2 =

e

x i k 2r1 + 2R1 x 2 +k r 0 −sin θ± τλ x 0

0

0

dx.

(18.91)

−d

By using table values [26], integrals (18.90) and (18.91) can be reduced to Fresnel integrals of the form: d J=

e −d

i (ax 2 +bx )

1 d x = √ eiν a

ξ2 −ξ1

cos ξ 2 + i sin ξ 2 dξ ,

(18.92)

224

I. P. Miroshnichenko et al.

where √ √ √ √ b2 ; ξ1 = −d a + ν; ξ2 = d a + ν, (18.93) 4a a is the coefficient before i x 2 in the exponent of expressions (18.90) and (18.91), respectively, and b is the coefficient before (i x) in these exponents. The light intensity according to (18.89) is calculated using the following formula: ν=

I (θ ) = (eikr0 J1 (θ ) + eikr0 J2 (θ ))(eikr0 J1 (θ ) + eikr0 J2 (θ ))∗ ,

(18.94)

where (*) denotes a complex-conjugate quantity. If the size of the beam-splitter is so large that diffraction at the edges can be neglected and the limits in (18.88) can be replaced by infinite ones, then the integrals (18.90) and (18.91) can be calculated using the following formulae [14]:

2 r R x0 2π R 0 r0 ik 0 0 −sin θ e 2(r0 +R0 ) r0 ; k r 0 + R0 2 r R x0 ik 2 r 0+R0 −sin θ± τλ 2π R 0 r0 ( 0 0 ) r0 i π4 e . J2 = e k r0 + R0 J1 = e

i π4

(18.95)

(18.96)

In accordance with these expressions and for simplicity, taking into account the amplitude multipliers of interfering waves (18.95) and (18.96), r0 = r0 = R0 , the intensity at the observed points can be written as follows: I = A0 (1 − cos γ ),

(18.97)

where 2 2 x0 x R r 0 R0 r λ k 0 0 − sin θ + r0 − 0 − sin θ ± γ = . −r0 + 2 r 0 + R0 r 0 r0 + R0 r0 τ (18.98) If the beam-splitter is large, we can determine the spatial frequency of the phase change. The dependence of the spatial frequency at different points θ on the measured parameters is determined by the following relation: ω=

x0 x0 r 0 R0 r R0 λ ∂γ =k − cos θ . − sin θ cos θ + 0 − sin θ ± ∂θ r 0 + R0 r 0 r0 + R0 r0 τ (18.99)

These formulae determine the dependence of the measured parameters of the interference pattern in the directions θ1 and θ2 , where the photodetectors are located,

18 Universal Technique to Determine the Intensity of the Optical …

225

on the coordinates of the highlighted point x0 , y0 on the surface, as well as on the location of the reflector α, h. So, if we put θ = θ1 in (18.94), we get an expression of intensity in the right part, the value of which depends on the measured parameters:

I1 (x0 , y0 , α, h) = (eikr0 J1 (θ1 ) + eikr0 J2 (θ1 ))(eikr0 J1 (θ1 ) + eikr0 J2 (θ1 ))∗ . (18.100) Similarly, for the intensity measured by the second photodetector, which is located in the direction θ2 , we have:

I2 (x0 , y0 , α, h) = (eikr0 J1 (θ2 ) + eikr0 J2 (θ2 ))(eikr0 J1 (θ2 ) + eikr0 J2 (θ2 ))∗ . (18.101) If the control object surface is highlighted at constant parameters α, h of the interferometer, then the expressions (18.100) and (18.101) are a system of equations with respect to x0 , y0 . In the second case, when the reflector is a control object surface and the luminous point is stationary, a system of equations for determining the values of α, h is obtained. Similar considerations can be made in the case of large beamsplitter sizes. Thus, by measuring, for example, the spatial frequency of interference bands ω in the directions θ1 and θ2 , it is possible to obtain a system of transcendental equations for determining x0 , y0 or α, h, which can be solved in any known way.

18.6 Conclusion It was developed universal technique, and also are derived and described in details the formulae for determining the intensity of the optical fields created by the laser interference meter of displacements based on two-way laser interferometer with combined branches, and implementing a method onto the surface of the test object. The proposed relationships allow for computational and theoretical modeling and research of functional characteristics in the interests of creating new promising optical means for measuring the displacement of control object surfaces. Acknowledgements The work was supported by the grant of Russian Foundation for Basic Research, No. 19-08-00365, Ministry of Education and Science of the Russian Federation: projects Nos. 3.5378.2017/VU (organization of the implementation of researches), 9.9770.2017/BCh (the basic part of the state task).

References 1. V.E. Alekhin, I.P. Miroshnichenko, A.G. Serkin, V.P. Sizov, Optical device for measuring surface movements of control objects. Russian Patent No. 2343402, 10.01.2009 (in Russian)

226

I. P. Miroshnichenko et al.

2. I.P. Miroshnichenko, I.A. Parinov, E.V. Rozhkov, Optical interference device for measuring surface movements of control objects. Russian Patent No. 2512697, 10.04.2014 (in Russian) 3. I.P. Miroshnichenko, I.A. Parinov, IOP Conf. Ser.: Mater. Sci. Eng. 572, 012065 (2019) 4. A.N. Matveev, Optics (Higher School, Moscow, 1985), p. 351 (in Russian) 5. A.S. Batrakov, M.M. Butusov, G.P. Grechka, Laser Measuring Systems (Radio and Communications, Moscow, 1981), p. 456 (in Russian) 6. V.E. Alekhin, I.P. Miroshnichenko, V.P. Sizov, Russ. J. Nondestr. Test. 43(2), 113 (2007) 7. V.E. Alekhin, I.P. Miroshnichenko, V.A. Nesterov, V.P. Sizov, Russ. J. Nondestr. Test. 43(9), 592 (2007) 8. V.E. Alekhin, I.P. Miroshnichenko, A.G. Serkin, Meas. Tech. 51(10), 26 (2008) 9. I.P. Miroshnichenko, I.A. Parinov, E.V. Rozhkov, A.G. Serkin, Metallurgist 50(7–8), 408 (2006) 10. I.P. Miroshnichenko, A.G. Serkin, Metallurgist 54(3–4), 189 (2010) 11. F.M. Morse, G. Feshbach, Methods of theoretical physics. Mosc. Inostr. Lit., 2, 896 (1960) 12. N.V. Kovalenko, Antenna Gratings (Rostov State University Press, Rostov-on-Don, 1971), pp. 17–33 (in Russian) 13. F.M. Morse, G. Feshbach, Methods of theoretical physics. Mosc. Inostr. Lit. 1, 930 (1958) 14. E. Janke, F. Emde, F. Lesh, Special Functions (Science, Moscow, 1977), p. 342

Chapter 19

Strength of Interatomic Bonds at High-Angle Grain Boundaries in Iron Yuri F. Migal

Abstract The numerical model of the high-angle boundary is used for quantumchemical calculations of the binding energy of atoms of impurity and alloying elements at the grain boundaries in iron. Elements of the fourth period, from potassium to krypton, are considered as impurity. It is shown that the bond strength between grains is primarily determined by the type of atoms located at the boundaries. To a lesser extent, the bond strength depends on the details of the arrangement of atoms.

19.1 Introduction The properties of metals, including the strength properties of their surface, largely depend on grain boundaries (GBs) in metals [1–3]. In various metals, including steels, along with atoms of the base metal at grain boundaries there are atoms of impurities and alloying elements. Some of these elements can strengthen the bond between the grains, and others, on the contrary, weaken this bond depending on the relative arrangement of atoms at the boundaries, as well as on the magnitude of the chemical bond between these atoms and the surface of the grains. The degree of dependence of the GBs strength in metals on the presence of various elements at the boundaries is one of the actual issues in the theory of metals. The segregation phenomenon in iron and its influence on the strength properties of iron have been studied in a significant number of works devoted to the GBs. For example, in [4–6] detailed studies using specific models were conducted for segregating elements, including C, P, S, Zn, Cu. The peculiarity of these works is that they study particular situations when certain impurity atoms are considered in a certain configuration of iron atoms. Along with this, works of a more general content are known [7–9], where atoms of different elements are studied in typical configurations of atoms of the base metal. The main task of these works is to compare these elements according to the degree of strengthening of the metal. Y. F. Migal (B) Southern Scientific Center of Russian Academy of Sciences, 41, Chekhov prosp, Rostov-on-Don, Russian Federation 344006 e-mail: [email protected] © Springer Nature Switzerland AG 2020 I. A. Parinov et al. (eds.), Advanced Materials, Springer Proceedings in Materials 6, https://doi.org/10.1007/978-3-030-45120-2_19

227

228

Y. F. Migal

In our opinion, it is interesting to consider and compare the strengthening and softening properties of a large group of elements containing entire periods of these elements. Such a statement of the problem is possible within the framework of some generalized model of segregation in metal (for example, in iron). With its help, it would be possible to classify the strengthening properties of various elements in relation, for example, to iron, regardless of the atomic configuration characteristics of these elements in iron. This approach would be most useful when creating steels with specified properties. Another, more accurate approach to the study of the strengthening properties of elements should be obviously based on the analysis of all possible configurations of atoms of these elements in the metal and the subsequent summation of the data obtained. Since any metal contains at the same time a huge variety of atomic impurities with a variety of properties, the exact approach is an almost impossible task. In favor of a less accurate generalized model, experimental facts indicate that many elements, regardless of what different equilibrium positions they have in the structure of iron, generally harden iron. It follows from this unambiguity that the strengthening effect of an element depends more on the pair interaction of atoms of this element with iron atoms than on the details of the relative arrangement of atoms. Such a statement is difficult to prove, but in many known cases it turns out to be true. Based on the experience of our previous studies, we can assume that to obtain generalized results about the influence of various impurity elements on the strength of iron, it is possible to use simplified models in which the different types of configurations characteristic of this element are averaged in some way. In [10, 11] we calculated the binding energy of polyatomic complexes simulating grain boundaries in iron. We investigated the influence of the chemical composition of grain boundaries, including atoms of impurity and alloying elements, on the bond strength between grains. In these case methods based on the DFT approximation were applied. With their help, quantum-chemical calculations of the binding energy of complexes including elements from the first six periods of the periodic table were carried out. The results of the calculations are in qualitative agreement with the well-known theoretical and experimental data on the influence of these elements. In these calculations, we used two different models of GBs, the cluster model and the slab model, which contain a large number of simplifications. These models did not take into account the variety of specific conditions available on different types of GBs (more details will be discussed below). In this chapter, we propose a new slab model that simulates a common defect in metals, namely the high-angle grain boundary. The main purpose of this article is to show that the dependences in the distribution of chemical elements by the degree of hardening of iron obtained in different ways are close to each other, despite the significant differences in both the variants of the mutual arrangement of atoms in iron and the models used.

19 Strength of Interatomic Bonds at High-Angle Grain …

229

19.2 High-Angle Grain Boundary Model First, we describe a simplified (“flat”) slab model, which was used earlier in our calculations [10, 11]. This model consists of several atomic layers. The central inner layer contains atoms of impurity elements, and the outer layers consist of iron atoms. If the system is subjected to thermal or mechanical action, it can decay into two parts. In this case, the impurity atoms, as shown by calculations, are located on the surface of one of these parts (Fig. 19.1). The energy E d required to disintegrate the system into two parts was determined by the formula E d = |E 0 − E 1 − E 2 |,

(1)

where E 0 is the binding energy of the whole system, E 1 and E 2 are the binding energies of the decayed parts. By using this model, it was found, in particular, that in the presence of carbon or boron atoms on the GB, the energy required for the disintegration of the system is greater than in the presence of sulfur or phosphorus atoms. These and other obtained results are in agreement with the experimental data and theoretical results of other authors (see, for example, [12–15]). In this chapter, an attempt is made to obtain similar results using a model that more accurately simulates the interactions of atoms at the grain boundaries. From all variety of known types of GB, it is necessary to choose some type of boundary allowing introduction on this boundary of atoms of impurity elements. Such boundaries include, in particular, the high-angle boundary, which can be represented as a set of points of contact of two sets of atomic planes with two different orientations in space. The angle between these planes must exceed 20° [16]. Atoms of impurity or alloying elements may be located in the voids arising from such a contact.

+Ed

Fig. 19.1 Flat model of the grain boundary in iron with the surface (100) and the decay of this boundary into two parts [10]; atoms of alloying or impurity elements are in the middle layer

230

Y. F. Migal

Thus, the system of parallel atomic planes, used in the case of the flat model, in this more realistic model is replaced by two systems of planes that touch each other inside some layer. In fact, this layer is the grain boundary. Next, we consider a variant in which two systems of contacting atomic layers with Miller indices (100) are located to each other under an angle equal to 43°. This angle is chosen so that the position of atoms in space can be represented as a set of elementary cells in the crystal. This configuration of atoms allows the use of classical methods for calculating crystal structures. Elements of the fourth period of the periodic table were considered as impurity and alloying elements in this work. If the size of the atoms or ions of these elements is smaller or comparable to the size of the iron atom, then such atoms are freely placed in the voids available on the GB. If such placement is energetically disadvantageous, the whole complex is unstable and will be disintegrated. The left part of Fig. 19.2 presents the scheme of arrangement of atoms of iron and one more of representatives of the fourth group—titanium in new model on start of calculations. The arrangement of atoms in this case has been chosen so that only the outer surfaces of the system and the high-angle boundaries are defects of this periodic atomic structure. The structure shown in the figure is a fragment of a system that periodically repeats in a plane parallel to two mutually perpendicular x- and y-axes. Here three elementary cells conjugated along the x-axis are shown. Geometric parameters of one elementary cell are: ax = 6.425 a.u., ay = 2.87 a.u. Total number of atoms in such a cell is 22. Among them there are 20 atoms of Fe and 2 atoms of Ti. The vertical layer in the middle of the picture, which consists of alternating Fe and Ti atoms, depicts the common boundary of the two grains in given projection.

Fig. 19.2 Decay of high-angle GB containing impurity titanium atoms; Ti atoms are represented by light grey balls; the atomic system is presented in an unrelaxed form

19 Strength of Interatomic Bonds at High-Angle Grain …

231

The right side of the picture shows the system after the decay that occurred at the grain boundary. The initial atomic configuration shown in Fig. 19.2, corresponds to the periodic arrangement of atoms specified at the start of calculations. In the result of atomic interactions taken into account in the model, relaxation occurs in the system, and the arrangement of atoms becomes less symmetrical. The configuration of atoms after relaxation is presented in Fig. 19.3. The main results of relaxation are: (i) violation of the order in the atomic configuration characteristic of an ideal solid (this violation is a consequence of the existence of the grain boundary); (ii) compression of the atomic system along the z-axis caused by the action of transverse internal forces in the system. The latter phenomenon is an artifact of the model. It is explained by the fact that the model does not take into account the interaction of the investigated system with neighboring atoms located in the metal outside this system. Fig. 19.3 GB model containing titanium atoms (relaxed state)

232

Y. F. Migal

19.3 Results of Calculations and Discussion This model was used to calculate the same values that were calculated earlier in [10, 11]. These values include the binding energy E 0 of the initial cell, the energies of its parts E 1 and E 2 , as well as the energy E d required for decay of the cell into parts. The energy E 1 corresponds to the part of the cell that contains the impurity atoms. The value of E d was calculated by using formula (1). Calculations of the values E 0 , E 1 and E 2 were carried out using the ADF-BAND software package [17], based on the DFT approximation. The results of the calculations are presented in Table 19.1. From the obtained data it follows that the values of E 0 , E 1 and E d for iron containing elements of the fourth period as impurities, initially increase and then decrease with the growth of the atomic number of the element. In the case of krypton, the decay energy of the cell is zero, i.e., in the presence of this element, the cell spontaneously decays. It should be noted that the results obtained are actually a consequence of the Periodic Law. Table 19.1 Total energy E 0 of initial cell, energies E 1 , E 2 of decayed parts and energy E d , required for decay of cell Element’s number

Impurity element

E 0, eV

E 1 , eV

E 2 , eV

E d , eV

19 20

K

−188.9

−105.1

−82.5

1.3

Ca

−193.6

−108.7

−82.5

2.4

21

Sc

−201.2

−115.5

−82.5

3.2

22

Ti

−207.8

−119.7

−82.5

5.6

23

V

−210.9

−122.3

−82.5

6.1

24

Cr

−211.8

−122.8

−82.5

6.5

25

Mn

−212.0

−123.2

−82.5

6.3

26

Fe

−211.2

−122.4

−82.5

6.3

27

Co

−209.8

−121.4

−82.5

5.9

28

Ni

−203.6

−115.3

−82.5

5.8

29

Cu

−199.4

−111.9

−82.5

5.0

30

Zn

−195.2

−108.3

−82.5

4.4

31

Ga

−199.8

−112.8

−82.5

4.5

32

Ge

−202.9

−116.1

−82.5

4.3

33

As

−203.6

−117.3

−82.5

3.8

34

Se

−200.5

−115.8

−82.5

2.2

35

Br

−194.4

−110.4

−82.5

1.5

36

Kr

?

−101.8

−82.5

0

Note the “?” sign in the column with E 0 means that the corresponding value for this element is undefined. A cell with such an element disintegrates spontaneously

19 Strength of Interatomic Bonds at High-Angle Grain …

233

Fig. 19.4 Dependence of the decay energy of an atomic system on the atomic number of an impurity element located at the grain boundary

These numerical data are consistent with data from our previous work obtained by using the flat model. From the fact that the energy required for the decay of the cell is maximum for the atoms of titanium, vanadium, chromium, manganese, cobalt and nickel, and it is greater or comparable to the decay energy in the case of pure iron, it follows that these elements strengthen iron. This conclusion is consistent with known experimental and theoretical data (see, for example, [14, 15]). In Fig. 19.4, the data from Table 19.1 relating to E d are shown graphically. Here, for comparison, the data corresponding to the results of calculations performed earlier [10, 11] with the help of simpler cluster and slab models are presented. This representation allows us to clearly see that in this case there is a relationship of the decay energy on the atomic number of elements, similar to the dependencies obtained in previous calculations.

19.4 Conclusions The binding energies of different atomic structures which were calculated by using the high-angle boundary model are qualitatively consistent with the results obtained earlier by using the flat model. It follows that the bond strength at grain boundaries in iron is mainly determined by the effects that are equally reproduced in these models - that is, the pair interactions between the atoms of the base metal (in this case, iron) and the atoms of alloying and impurity elements on the grain surface. The

234

Y. F. Migal

dependence of the bond strength on details of the mutual arrangement of atoms is manifested to a lesser extent. These facts make it possible to rank the elements located at grain boundaries by the magnitude of the chemical bonds between these elements and iron. The whole set of elements can be divided into three groups: (i) strengthening; (ii) softening and (iii) not significantly affecting the strength of boundaries. The elements of the fourth period which can be attributed to the strengthening elements are titanium, vanadium, chromium, manganese, cobalt and nickel. The softening elements include potassium, calcium, arsenic, scandium, selenium, bromine. These results are consistent with known experimental information about these elements. Acknowledgements This work was performed within the framework of the state assignment of the South Scientific Center of RAS, number of state registration is AAAA-A16-116012610052-3.

References 1. P. Lejcek, Grain Boundary Segregation in Metals. Springer Series in Materials Science, vol. 136 (Springer, Berlin, 2010) 2. B.S. Bokstein, A.O. Rodin, B.B. Straumal eds. in Selected, peer reviewed papers from the international conference on grain boundary diffusion, stresses and segregation, DSS 2010, Moscow, Russia, 1–4 June 2010, pp 308 (2011) 3. M. Herbig, D. Raabe, Y.J. Li, P. Choi, S. Zaefferer, S. Goto, Phys. Rev. Lett. 112, 126103 (2014) 4. W. Peng, H. Peng, G. Wu, J. Zhang, Comp. Mater. Sci. 171, 109204 (2020) 5. M. Yuasa, M. Mabuchi, Phys. Rev. B 82, 0941081 (2010) 6. J.L. Wang, R. Janisch, G.K.H. Madsen, R. Drautz, Acta Mater. 115, 259 (2016) 7. M. Yamaguchi, M. Shiga, H. Kaburaki, Mater. Trans. 47, 2682 (2006) 8. K.D. Bauer, M. Todorova, K. Hingerl, J. Neugebbauer, Acta Mater. 90, 69 (2015) 9. M. Yamaguchi, Y. Nishiyama, H. Kaburaki, Phys. Rev. B 76, 0354181 (2007) 10. YuF Migal, V.I. Kolesnikov, I.V. Kolesnikov, Comp. Mater. Science 111, 503 (2016) 11. V.I. Kolesnikov, Y.F. Migal, I.V. Kolesnikov, E.S. Novikov, Dokl. Phys. Chem. 464(1), 194 (2015) 12. M.P. Seah, Acta Metall. 28, 955 (1980) 13. E.P. DeCarmo, J.T. Black, R.A. Kohser, Materials and Processes in Manufacturing, 10th edn. (Wiley, Hoboken, NJ, 2007) 14. P.-J. Cunat, The Euro Inox Handbook of Stainless Steel (Brussels, 2002) 15. H.J. Grabke, in Impurities in Engineering Materials. Impact, Reliability, and Control, ed. by C.L. Briant Marcel Dekker, New York, 1999), p. 143 16. G. Gottstein, Physical Foundations of Materials Science (Springer, Berlin, 2014) 17. G. te Velde, F.M. Bickelhaupt, E.J. Baerends, F.C. Guerra, S.J.A. van Gisbergen, J.G. Snijders, T. Ziegler, J. Comp. Chem. 22, 931 (2001)

Chapter 20

Digital Microscopy Image Enhancement Technique for Microstructure Image Analysis of Bottom Ash Particle Polymer Composites F. A. Hermawati, I. M. Kastiawan, and Muhyin Abstract Polymer composites are composite materials with matrices of polymers with reinforcements using fibers or particles or both together. This study uses polypropylene polymer composite material with reinforcement of bottom ash particles. In the manufacture of polypropylene-shaped sheet (lamina) polymer composite materials with bottom ash particles, the process of assessing the composite characteristics of the polypropylene matrix such as the level of distribution of bottom ash particles as fillers in the polypropylene matrix through microscopic images is necessary. Analysis of the level of distribution of reinforcement particle is used to avoid the formation of filler particle agglomerates during the dispersion of various types of fillers in polymer resins. Bottom ash particles themselves have an irregular shape that requires particular analysis to distinguish a single particle and an agglomerate particle. Before the analysis step, the most crucial step at the beginning is to carry out the process of improving the quality of the input image, which aims to improve image contrast and eliminate unwanted noise. This chapter proposes an image enhancement method to enhance the quality of the microstructure image of a polymer composite that is analyzed using a digital microscope. The proposed method combines the multiresolution approach and the anisotropic diffusion method. From the experiment, this image enhancement method gives the best performance when it is compared with other techniques in the state of the arts.

20.1 Introduction In the manufacture of polypropylene-shaped sheet (lamina) polymer composite materials with bottom ash particles, the process of assessing the composite characteristics of the PP matrix such as the level of distribution of bottom ash particles as fillers in the PP matrix through microscopic images is an essential act. We need an analysis F. A. Hermawati (B) Department of Informatics, Universitas 17 Agustus 1945, Surabaya, Indonesia e-mail: [email protected] I. M. Kastiawan · Muhyin Department of Mechanical Engineering, Universitas 17 Agustus 1945, Surabaya, Indonesia © Springer Nature Switzerland AG 2020 I. A. Parinov et al. (eds.), Advanced Materials, Springer Proceedings in Materials 6, https://doi.org/10.1007/978-3-030-45120-2_20

235

236

F. A. Hermawati et al.

of the level of distribution of reinforcement particles to avoid the formation of filler particle agglomerates during the dispersion of various types of fillers in polymer resins [1, 2]. Bottom ash particles have an irregular shape that requires particular analysis to distinguish a particle or an agglomerate of particles. Before the analysis step, the most crucial step at the beginning is to carry out the image enhancement process to improve the quality of the input image, which aims to improve image contrast and to eliminate noise. In several studies of image analysis for composite materials, a microscopic image quality improvement technique is needed to reduce noise or unwanted artifacts in the image but still retain the characteristics and details of the image. As state of the art, we present several studies related to image enhancement techniques for analyzing microstructural images using Scanning Electron Microscope (SEM), Transmission Electron Microscope (TEM), or digital microscopes. Gaussian filter is a filter that is widely used to reduce noise both in the signal as performed by Hermawati et al. [3] or on the image. Campbell et al. [4] used Gaussian filters to reduce noise while maintaining differences in intensity between adjacent grains. According to Campbell, finding effective Gaussian filtering can also cause distortion. The chosen size of the filter will be able to reduce noise and distortion. They proposed a 3 × 3 filter size for optical image s of titanium Microstructures of the Ti6 Al4 V alloy taken using a digital microscope. Kundu et al. [5] also applied a 5 × 5 Gaussian filter with standard deviation σ = 1.2 to eliminate noise in the SEM image of a polymer composite using the natural blend system of natural rubber matrix (NR)—polybutadiene rubber (PBR)—reclaim rubber (RR) with silica as a reinforcement. Meanwhile, Hiremath et al. [6] proposed the selective median switching filter in [7] to eliminate noise in the image of ductile cast iron microstructure. Martin-Herrero [8] implemented the image processing techniques in the reconstruction task of the 3D microstructure image of the C/C fiber composites from an X-ray contrast phase micro tomography. In the preprocessing stage, they applied the anisotropic diffusion method in [9] that can eliminate high-frequency noise while maintaining the edge. Duval et al. [10] suggested a bilateral filtering method to reduce noise in the homogeneous areas by slightly modifying the area of interest. They implemented this filter in the SEM image of the catalyst section that illustrates black cracks, partially filled pores that have a round dark grey shape with white spots and inclusion of zeolites which is scattered or aggregated white dots in neutral substrates (aluminum). This study proposed an image enhancement technique for improving the microscopic image quality of polymer composites with reinforcement of bottom ash. This method will eliminate noise that can be the granules or white lines due to the forming process of the sheet material, for example, due to the operation of rolling or pressing. The proposed method combines the frequency-based technique with some spatial filtering based methods. This hybrid method, as presented by Hermawati et al. [11], can reduce noise in the image while maintaining the edge. We also propose a dark region enhancement stage to increase the contrast of the black area, which is the bottom ash particles area. The application of the proposed image enhancement method aims to improve the accuracy of the analysis of filler dispersions in the polymer matrix in measuring the strength of the tested material.

20 Digital Microscopy Image Enhancement Technique …

237

This chapter is composed of four sections. The second section presents how to obtain the Microstructure image from polymer composite material for the research and explain the proposed method to enhance the image. The results of the conducted experiment are presented in the third section. In this section, we also compare our proposed method with other techniques in state of the art. The fourth section presents conclusions and steps that need to be done in the next study.

20.2 Material and Method 20.2.1 Material Preparation The materials used to make polymer composites with sisal fibers as reinforcement are thermoplastic polymers (polypropylene), bottom ash with specific mesh, and sisal fibers of a certain length. Concentrations based on weight will be prepared according to the variables determined before polymer melting. Polypropylene polymers with a specific weight are poured into a heating container with a temperature of 170 °C. This temperature corresponds to the melting temperature of polypropylene. After 100% melting, which takes almost 2 h for the weight of 300 g of polypropylene, bottom ash powder of coal is weighed and has a specific mesh particle size. Then, sisal fibers of a certain length were inserted into them in an amount that was also determined. After all fillers and boosters have been poured, stirring is carried out for 30 min at a certain speed. After the stirring time, the polymer composite material mixture is ready to be printed into a rectangular mold, 10 mm thick, 20 mm wide and 200 mm long with a pressure of 20 kg/mm2 during 5 min. The polymer composite material after cooling is ready to be removed from the mold. For testing of filler distribution, the content is flattened or printed in the sheet form with a certain thickness and then captured by using a digital optical microscope Dino-lite with 200 times magnification. Figure 20.1 is the example of a microscopic image with bottom ash particles percentage of 2 and 5%. The image size obtained is 1280 × 1024 pixels.

20.2.2 Proposed Method The proposed method is the development of the technique proposed by Hermawati et al. [11], which is used to eliminate speckle noise in ultrasound images, namely hybrid speckle noise reduction method, as described in Fig. 20.2. This method combines multiresolution wavelet approach with bilateral filtering and anisotropic diffusion technique. We add a method to increase the black pixels of the image that indicate the bottom ash particles and will be further analyzed. The proposed method consists of five main steps.

238

F. A. Hermawati et al.

Fig. 20.1 Examples of microscopy image of polymer composite with bottom-ash particle percentage of a 2% and b 5%

Fig. 20.2 Block diagram of proposed method

20 Digital Microscopy Image Enhancement Technique …

239

Firstly, the process of enhancing dark regions is done by using local statistics enhancement using a 3 × 3 neighboring window. Suppose f (x, y) is an image, the enhanced image g(x, y) is expressed as g(x, y) = 0.5 f (x, y); if μ(x, y) < 0.5 μG

(20.1)

where μ(x, y) is a local mean in 3 × 3 neighbourhood area with coordinates (x, y) at its centre and μG is an average of image intensities. After that, the enhanced image g is decomposed using three-level discrete wavelet transform into one approximation image, A3 , and nine detail images, i.e. D31 , D32 , D33 at the third level; D21 , D22 , D23 at the second level and D11 , D12 , D13 at the first level as described in Fig. 20.3. The detail images are processed sequentially using thresholding and anisotropic diffusion, whereas the approximation image is processed using bilateral filters starting from the third level. Furthermore, the four subbands at level 3 that have been processed are synthesised using the inverse discrete wavelet transform (IDWT) to get the approximation image at level 2. The same process is carried out until the first decomposition level. We implement the best parameters in [11]. Suppose A is an approximation image with i as centre coordinate of 5 × 5 neighbourhood window, w, and j ∈ w is a pixel coordinate in window w that i = j. The bilateral function A, denoted as, Aˆ is expressed as the following expression [11]: 2 2 − ( j−i)2 1 1 1 − (A( j)−A(i) 2σ 2σr2 ˆ = d A( j) A(i) √ e √ e C j∈w σd 2π σr 2π

Fig. 20.3 Three-level wavelet decomposition

D13

A3

D12 D23

D33

D13 D22

D32

D1 3

D13

(20.2)

240

F. A. Hermawati et al.

where (i) and A(i) are the intensities at coordinate i; σd and σr are the standard deviations of Gaussian filter that control smoothing strength in the image domains, and C is a normalization constant. In this research, we use controlling parameter σd = 3 and σr = 7σn , where σn is the standard deviation of noise that equal to the threshold value of T in (3). The following function obtains the threshold value, T that is implemented in the thresholding step for the detail images, D1 , D2 , D3 [11]: T =

median D 3 i

0.6745

(20.3)

where Di3 are image coefficients in diagonal image D3 .

20.3 Results and Discussion Optical microscopic images used in the experiment can be seen in Fig. 20.1, with percentages of bottom ash reinforcement equals to 2%. Composite lamina sheets used have not been done by finishing or polishing, so that there are parts of pressure marks due to the rolling process during the process of making lamina, which is indicated by bright coloured lines. This is also a challenge in the process of improving the quality of microscopic images. To evaluate the results of enhanced microscopic image quality of polymer composites, we compared them with other methods used in state of the art research, i.e. Gaussian filter size 3 × 3, Gaussian filter size 5 × 5 with standard deviation 1.2, anisotropic diffusion, bilateral filter and selective median filter. Visually, the enhancement result for each method can be seen in Fig. 20.4. In Fig. 20.4, the bottom ash particles in the image that is processed by the proposed method are more clear and sharp than in the other images. Since in this problem there is no reference image or ground truth of the processed image, then to evaluate the noise reduction level we use ENL (Equivalent Number of Looks) which is formulated as the ratio between (mean/standard deviation)2 from the homogeneous image area [13–15]. Where the higher the value of ENL, the better the rate of removal of the number. However, to see the quality of the noise reduction method in maintaining edges, we measured ENL for the entire image. A low ENL value, which means that the variation of the intensities is high, will indicate that the level of edge presence is high. So the smaller the ENL value, the better the method of maintaining edges. The performance comparison of the image enhancement methods is presented in Table 20.1. In Table 20.1, it can be seen that the proposed hybrid method gives the lowest ENL value. The ENL value is comparable to the view in Fig. 20.4a in which appears a significant difference in intensity between the object and the background. The anisotropic diffusion method has a lower ENL value and is followed by the bilateral filtering technique. The Gaussian filter method for a 3 × 3 filter and a 5 × 5 filter and also the selective median filter have almost identical ENL value.

20 Digital Microscopy Image Enhancement Technique …

241

Fig. 20.4 Comparation of enhancement result using: a proposed method; b anisotropic diffusion; c bilateral filter; d selective median filter; e Gaussian filter 3 × 3; f Gaussian filter 5 × 5 with σ = 1.2

242

F. A. Hermawati et al.

Table 20.1 Performance comparison of image enhancement method

Method

ENL

Hybrid enhancement method (proposed method)

152.769

Anisotropic diffusion (Perona Malik) [8]

159.5305

Bilateral filter [12]

160.0842

Selective median filter [6]

161.4238

Gaussian filter 3 × 3 [4]

161.1195

Gaussian filter 5 × 5 with σ = 1.2 [5]

161.1191

Figure 20.5 presents the histogram of the image enhancement results. From the histogram of the proposed method in Fig. 20.5a, we can separate precisely between the object (bottom ash particles) and the background (matrix). So the image segmentation result for getting the bottom ash particles has become more accurate when compared to other image enhancement methods such as shown in Fig. 20.6. We implemented the thresholding method with a threshold equal to 0.2 to obtain the binary images in Fig. 20.6. 10

2.5

4

10

2

4

10

2

2

1.5

1.5

1

1

0.5

0.5

1.5

1

0.5

0

0

0 0

50

100

150

200

0

250

50

100

(a) 10

4

150

200

250

Selective median switching filter

10

Gaussian 3x3

4

10

1.5

1.5

1

1

1

0.5

0.5

0.5

0

0

2

1.5

100

150

(d)

50

100

200

250

0

150

200

250

(c)

2

50

0

(b)

2

0

Bilateral Filtering

4

gaussian 5x5

4

0 50

100

150

(e)

200

250

0

50

100

150

200

250

(f)

Fig. 20.5 Histograms of the enhanced image using: a proposed method; b anisotropic diffusion; c bilateral filter; d selective median filter; e Gaussian filter 3 × 3; f Gaussian filter 5 × 5 with σ = 1.2

20 Digital Microscopy Image Enhancement Technique …

243

Fig. 20.6 Segmentation results of the enhanced image using: a proposed method; b anisotropic diffusion; c bilateral filter; d selective median filter; e Gaussian filter 3 × 3; f Gaussian filter 5 × 5 with σ = 1.2

244

F. A. Hermawati et al.

20.4 Conclusion Hybrid speckle-noise reduction method, which was preceded by the technique of repairing dark areas in microscopic images of polymer composites with bottom ash reinforcement was able to eliminate noise and scratches while maintaining image details. By applying this proposed noise reduction technique, the results of image segmentation by thresholding become more precise compared to other methods in state of the art. Furthermore, to analyze the dispersion level of bottom ash particles in polymer composites, segmentation and filler particle analysis need to be done. Acknowledgements This research was funded from a leading applied research universities from The Ministry of Research, Technology & Higher Education of the Republic of Indonesia based on Grant No. 229/SP2H/LT/DRPM/2019 dated March 11, 2019 and contract number: 374/06/ST/LPPM/Lit/III/2019.

References 1. T. Glaskova, M. Zarrelli, A. Borisova, K. Timchenko, A. Aniskevich, M. Giordano, Compos. Sci. Technol. 71, 1543 (2011) 2. T. Glaskova, M. Zarrelli, A. Aniskevich, M. Giordano, L. Trinkler, B. Berzina, Compos. Sci. Technol. 72, 477 (2012) 3. F.A. Hermawati, Sugiono, Evonda, in Advanced Materials Techniques, Physics, Mechanics and Applications, ed by I.A. Parinov, S.-H. Chang, M.A. Jani, Springer International Publishing, Berlin, pp. 535–543 (2017) 4. A. Campbell, P. Murray, E. Yakushina, S. Marshall, W. Ion, Mater. Des. 141, 395 (2018) 5. S. Kundu, P. Jana, D. De, M. Roy, in Proceedings of 2015 IEEE International Conference on Electrical, Computer and Communication Technologies, ICECCT 2015 (2015) 6. P.S. Hiremath, A. Sadashivappa, P. Pattan, Int. J. Comput. Appl. 107, 975 (2014) 7. P.S. Hiremath, A. Sadashivappa, Int. J. Image Process. 7, 101 (2013) 8. J. Martin-herrero, C. Germain, Carbon, Elsevier, vol. 45, pp. 1242 (2007) 9. P. Perona, J. Malik, IEEE Trans. Pattern Anal. Mach. Intell. 12, 629 (1990) 10. L. Duval, M. Moreaud, C. Couprie, D. Jeulin, H. Talbot, J. Angulo, in 2014 IEEE International Conference on Image Processing, ICIP 2014, pp. 4862 (2014) 11. F.A. Hermawati, H. Tjandrasa, N. Suciati, Int. J. Electr. Comput. Eng. (IJECE) 8, 1747 (2018) 12. L. Duval, M. Moreaud, C. Couprie, D. Jeulin, H. Talbot, J. Angulo, in 2014 IEEE International Conference on Image Processing, ICIP 2014, pp. 4862–4866 (2014) 13. X. Fu, Y. Wang, L. Chen, J. Tian, Biomed. Signal Process. Control 18, 30 (2015) 14. Y.M.M. Babu, M.V. Subramanyam, M.N.G. Prasad, Int. J. Electr. Comput. Eng. 5, 984 (2015) 15. F. A. Hermawati, S. Sugiono, R. Octaviany, in Seminar Nasional Otomasi Industri Dan Teknologi Informasi 2015 (SNOITI 2015) (2015) (in Indonesian)

Chapter 21

Analysis of Effect of Oil Viscosity and Temperature on Dynamic Pressure Distribution in Internal Gear Motor and Pump Pham Trong Hoa Abstract The chapter analyzes the effect of oil temperature and dynamic viscosity on hydrodynamic pressure distribution of the oil lubrication film in the internal gear motor and pump. The Reynolds equation with appropriate boundary condition is solved to obtain 2D hydrodynamic pressure distribution by using the finite difference method (FDM). Numerical calculations point out that the oil temperature and viscosity have great effect on hydrodynamic pressure distribution as well as the maximum value of pressure.

21.1 Introduction Internal gear motor and pump (IGMaP) is very popular in the field of hydraulic power applications [1]. Oil lubrication film is very important for rotating machines. Its role is to separate the relative rotating surfaces during operation or even at the rest [2]. In study [3], Pham pointed out that the hydrodynamic pressure in the oil film is much dependent on the rotating speed. The hydrodynamic pressure mountain will produce the capacity for the oil lubrication film to against with the radial load acting on the ring gear. The outer ring gear and inner housing surfaces is, therefore, protected during operation. It also means that if the oil film is failure, then the outer ring gear and inner housing will be in solid contact. It makes the IGMaP damages much sooner. Consequently, the lifespan of IGMaP is strongly reduced. This is unwanted phenomenon. Thus, calculation of hydrodynamic pressure distribution and estimation of the effect of working conditions are the fundamental issue to improve the performance of IGMaP [4]. Studying about the hydrodynamic pressure in the oil lubrication film have been performed by researchers such as [5, 6]. Lots of works have been studied regarding to IGMaP [7–9], however, the effect of oil temperature and viscosity on hydrodynamic pressure distribution has been not released so far. In P. T. Hoa (B) University of Transport and Communications (UTC), No. 3 Cau Giay, Lang Thuong, Dong Da, Hanoi, Vietnam e-mail: [email protected] © Springer Nature Switzerland AG 2020 I. A. Parinov et al. (eds.), Advanced Materials, Springer Proceedings in Materials 6, https://doi.org/10.1007/978-3-030-45120-2_21

245

246

P. T. Hoa

this study, by using the Finite Difference Method to solve the Reynolds equation, the effect of oil temperature and viscosity on the hydrodynamic pressure distribution are analyzed.

21.2 Formation of the Equation An internal gear motor and pump has three main elements which are described in Fig. 21.1, e.g., a ring gear which is consider as rotor, a fixed-pinion gear which connected to shaft, and the housing (stator). The diameter of inner housing is slightly larger than that of the outer ring gear. The space between the outer ring gear and the inner housing is fully filled by working oil. This is called the thin lubrication film. During operation, the oil film thickness is various for different position over circumferential direction as in Fig. 21.2. The oil film profile is calculated as follows, h (θ,e) = c(1 + ε cos θ )

(21.1)

where ε is the eccentricity ratio; i.e., the ratio of eccentricity to radial clearance (e/c); θ is the angle from the central line (ZZ0 ) to the measured point (H) along with the circumferential direction; c is the radial clearance.

Fig. 21.1 Internal gear motor and pump

21 Analysis of Effect of Oil Viscosity and Temperature on Dynamic …

247

Fig. 21.2 Geometry of the ring gear

21.2.1 Hydrodynamic Pressure Distribution The well-known Reynolds equation is used to calculate the pressure distribution. The Reynold’s equation for incompressible liquid is described as follows [1]: ∂ ∂h ∂ 3 ∂p 3 ∂p h + h = 6Uμ ∂θ ∂θ ∂z ∂z ∂θ

(21.2)

where h is the film thickness [m]; r is the ring gear radius [m]; L is the length of ring gear [m]; D is the diameter of the ring gear [m]; μ is the dynamic viscosity [Pa · s]; p is the pressure [Pa]; θ , z are hydrodynamic film co-ordinates [m]. Dynamic viscosity of the lubricant oil as a function of temperature can be computed according to Vogel-Cameron [10] as follows, B

μT = A · e T +C

(21.3)

where C = 95 °C is the constant coefficient; A and B is the fluid specific constant, for HLP 46, A = 0.054 mPa · s, B = 921 °C, T is the oil temperature. The Reynolds equation has been solved by using the finite difference method (FDM) with appropriate boundary condition to obtain 2D hydrodynamic pressure distribution. Details of finite difference solution has been presented in study [1]. The computational calculation is present in Fig. 21.3. An in-house calculation tool has been coded in Matlab environment to optimize the calculation time. All the operating parameters and geometric parameters are considered as the input parameters for calculation. The mobility method is used firstly to predict the ring the eccentricity

248

P. T. Hoa

Fig. 21.3 Computational flow chart

of ring gear center. These parameters are considered as the input parameters to solve the Reynolds equation to obtain 2D hydrodynamic pressure distribution.

21.3 Simulation Results and Discussion The input parameters for calculation are present in Table 21.1. Table 21.1 Initial data input

Parameter

Symbol

Value

Unit

Length of ring gear

L

0.34

m

Diameter of ring gear

D

0.115

m

Radial clearance

c

60 × 10−6

m

Rotating speed

n

1500

rpm

Working pressure

p

100

bar

21 Analysis of Effect of Oil Viscosity and Temperature on Dynamic …

249

21.3.1 Effect of Oil Temperature 2D dynamic pressure mountain in the oil lubrication film for various values of oil temperature is depicted in Fig. 21.4. The dynamic pressure distributes evenly over the axial direction. For circumferential direction, the dynamic pressure area ranges from 110° to 290°. From Fig. 21.4, one can observe that for low values of oil temperature, the dynamic pressure mountain is higher than that of high values of oil temperature. For example, as oil temperature at value of 0 °C the maximum dynamic pressure is 27.20 bar. The maximum dynamic pressure downs to 10.82 bar when the oil temperature increases up to 90 °C. The eccentricity is also changed according to the change of oil temperature as shown in Fig. 21.5. The eccentricity increases with the increase of the oil temperature, e.g., the eccentricity increases from 0.6 to 0.91 as the temperature increases from 0 to 90 °C. This is an unwanted phenomenon. Because it reduces the minimum film thickness. Consequently, the solid contact between the outer ring gear and inner housing is easy occurred. The changing of maximum dynamic pressure for various values of oil temperature is presented in Fig. 21.6. Contrary to the changing of

(a) Oil temperature at 0 °C

(b) Oil temperature at 30 °C

(c) Oil temperature at 60 °C

(d) Oil temperature at 90 °C

Fig. 21.4 Effect of oil temperature on 2D hydrodynamic pressure distribution

250

P. T. Hoa

Fig. 21.5 Eccentricity over oil temperature

Fig. 21.6 Value and position of maximum pressure

eccentricity, the maximum pressure decreases with the increase of oil temperature. The decrease of maximum pressure leads to the decrease of the oil film capacity. In other words, it reduces the working ability of the internal gear motor and pump. Moreover, the position of maximum pressure also decreases with the increase of oil temperature, e.g., the position angle of maximum pressure decreases from 220° to 206° when the temperature increases from 0 to 90 °C. From these results one can conclude that the internal gear motor and pump should not operate at high values of oil temperature.

21.3.2 Effect of Oil Viscosity Effect of oil type or oil viscosity on 2D dynamic pressure distribution is described in Fig. 21.7. It is obviously to see that for high values of dynamic viscosity, the dynamic pressure mountain is lower than that of high values of dynamic viscosity, e.g., the

21 Analysis of Effect of Oil Viscosity and Temperature on Dynamic …

(a) HPL10 ( µ = 0.00087 Pa·s)

(b) HPL32 ( µ = 0.00278 Pa·s)

(c) HPL68 ( µ = 0.00591 Pa·s)

(d) HPL150 ( µ = 0.1305 Pa·s)

251

Fig. 21.7 Effect of oil dynamic viscosity on 2D hydrodynamic pressure distribution

maximum dynamic pressure increases about 3.7 times, from 10.25 to 37.1 bar as the oil viscosity increases from 0.00087 Pa·s for HLP10 to 0.1305 Pa·s for HP150. The eccentricity of ring gear dependent on the dynamic viscosity is presented in Fig. 21.8. The eccentricity decreases with the increase of oil viscosity. For example, the eccentricity decreases from 0.95 to 0.42 when the dynamic viscosity increases from 0.0087 Pa·s for HLP 10 to 0.1305 Pa·s for HLP150. Contrary to the decrease of eccentricity, the value and position angle of maximum dynamic pressure increase with the increase of oil viscosity as depicted in Fig. 21.9. This will increase the oil film capacity. Consequently, the working ability of internal gear motor and pump is better when IGMaP operated at high value of dynamic viscosity.

252

P. T. Hoa

Fig. 21.8 Eccentricity versus oil viscosity

Fig. 21.9 Value and position of maximum pressure

21.4 Conclusion Temperature and dynamic viscosity are two important parameters of hydraulic oil, which have great effect on dynamic pressure distribution, however it is not easy to assess. Based on the results presented in this study, some following conclusions can be drawn. (1) The hydrodynamic pressure is proportional with the oil dynamic viscosity. The capacity of oil film increases with the increase of viscosity. If the dynamic viscosity of working oil is too low, the hydrodynamic pressure produces insufficient capacity for the oil film. It can lead to the solid contact. Therefore, it must be chosen the suitable oil type for each specific working condition. (2) The hydrodynamic pressure is inversely proportional with the oil temperature. The solid contact between the outer ring gear and inner housing can be occurred, if IGMaP operates under high values of oil temperature. Therefore, if

21 Analysis of Effect of Oil Viscosity and Temperature on Dynamic …

253

IGMaP operates at high temperature, it must be checked the allowable condition otherwise the IGMaP will be damaged much sooner. Acknowledgements This research is funded by Vietnam National Foundation for Science and Technology Development (NAFOSTED) under grant number 107.03-2019.17.

References 1. Trong Hoa Pham, Analysis of the Ring Gear Orbit, Misalignment, and Stability Phenomenon for Internal Gear Motors and Pumps (Shaker Verlag, Germany, 2018) 2. B.J. Hamrock, S.R. Schmid, B.O. Jacobson, Fundamentals of Fluid Film Lubrication, 2nd edn. (McGraw-Hill, New York, 2004) 3. T.H. Pham, L. Müller, J. Weber, J. Mech. Sci. Technol. 32(7) (2018) 4. Trong Hoa Pham, J. Mech. Sci. Technol. 33(2), 602–612 (2019) 5. M.A. Ahmad, S. Kasolang, R. Dwyer-Joyce, Appl. Mech. Mater. 315, 977–981 (2013) 6. M. A. Omer, T.V.V.L.N. Rao, A.M.A. Rani, T. Nagarajan, F.M. Hashim, Pressure Distribution in Hydrodynamic Journal Bearing. MATEC Web of Conference. 13, 05006 (2014). https://doi. org/10.1051/matecconf/20141305006 7. N.Y.Y. Inaguma, JTEKT Eng. J., No. 1011E, 64–73 (2014) 8. W. Song, Y. Chen, H. Zhou, Adv. Mech. Eng. 8(10), 1–15 (2016) 9. D. Khalid, R. B. Weli, In: 1st International Conference on Recent Innovations in Engineering and Technology, SU-ICEIT 2016, 162–168 (2016) 10. J. Ivantysys, M. Ivantysys, Hydrostatische Pumpen und Motoren: Kontruktion und Berechnung (Vogel Buchverlag, 1993) (in Germany)

Chapter 22

Experimental Investigation of Effect of Process Parameters on Surface Roughness in Electrochemical Machining Loc P. Ngo, Tai P. Nguyen, and Thanh T. Tran

Abstract With the rapid development of removal technology of materials, manufacturing methods of advanced materials with highly flexible shape has been improved. Electro-chemical machining (ECM) is one of the most advanced manufacturing methods for not only manufacturing the high hardness metal with flexible profiles, but also provides a better solution to surface roughness of finished products and rate of material removal in the comparison with other advanced manufacturing methodologies such as electric discharge machining (EDM). However, there are many parameters involving to the ECM process such as velocity of the electrode, pressure of water, voltage, frequency and pulse of the current. Therefore, a set of optimization parameters for machining process of a material type is necessary to provide the best solution in industrial applications. This research focuses on investigating an optimal set of process parameters of the ECM machine by using the surface response methodology (SRM). A database of process parameters is generated by machining and minimizing the surface roughness of the SS AISI 316 stainless steel via suing the copper electrode. Then, an objective function (or regression function) is generated by applying the SRM to the selected database. Finally, genetic algorithm is used to achieve the optimal process parameters. Experiments are implemented with achieved processing parameters to analyze and validate the proposed method.

22.1 Introduction The electro-chemical machining (ECM) is an anodic electrochemical dissolution process, in which the tools are used as a cathode and the workpiece play a role as an anode [1]. The surface roughness (SR) of the ECM processing plays an important role for the quality of a product after being manufactured [2, 3]. Thus, a method which is used for determining an optimal set of processing parameters to improve the SR of finished products in the ECM is necessary for recommending end-users L. P. Ngo · T. P. Nguyen · T. T. Tran (B) Department of Global Production Engineering and Management, Vietnamese-German University, 2 Le Lai, Thu Dau Mot City, Binh Duong, Vietnam e-mail: [email protected] © Springer Nature Switzerland AG 2020 I. A. Parinov et al. (eds.), Advanced Materials, Springer Proceedings in Materials 6, https://doi.org/10.1007/978-3-030-45120-2_22

255

256

L. P. Ngo et al.

in product fabrication. A new approach to improving the possibility of processing microstructure is presented in work [4]. In the paper, the researchers propose the possibility to manufacture different operation activities with the highly flexible for the control system in the term of feed rate, electrolyze flow across the surface of the tool and the workpiece [4]. The most important thing for the ECM processing is pulse power supply for the whole system. However, there are still many other aspects that must be done as the future research. Two of the most important things requires in this research is about the controller for the inter-electrolyze gap and the controller for control the anodic dissolutions. The work [2] has highlighted the current trend of the ECM and the future for this method. Based on this research, the micro-ECM (EMM) can be used as an effective post-processing method for treating the surface of the component after being manufacturing. The paper also points out many aspects in which that are not explored about electrochemical processing. As a conclusion, the paper suggests with the high precision development of medical and automotive industries, the development of micro-ECM will increase sharply in the next few years. A set of experiments are implemented in [5] in which the effect of pulsating current is validated for improving the quality of the components and its advantages in the comparison with the traditional power supply method. By using the technique to simplify the model for checking the condition of one to some parameters allows authors to achieve the result of a high rate for mass transport and minimizing the electrolyte heating during the process. The research also pointed out the average dissolution rate in PECM as controlled in the limitation by electrolyte heating. The final part of the research shows the produced gas bubbles in the anode and cathode. By applying pulsating current, the method could eliminate the generating of heat due to electrolyte process and control the accuracy and surface roughness of the final products. An approach is proposed in the research [6], in which a theoretical and experimental research is conducted for a relationship between the surface condition of the anode (or workpiece) and the prepared profiled of the cathode (tool). The tool is designed especially in microstructure in which the relationship could be determined. The manufacturing condition is controlled in the limitation of copying the profile of cathode to the anode. At the end of his research, the author has suggested the method for improving the micro-structure ability of ECM processes. The ultra-short pulse current in [7] was proposed for examining the change of electrode during the electrochemical machining processes based on the simulation methodology. In this research, a method called marker is used for building the 3D application which can simulate the condition of the surface of the electrode. The output of this research is a numerical approach for simulating the desired object using the 3D method. By using the mentioned tool combined with the BEM approach, the model was developed following Faradays law. This method can open a new technique for non-touch monitoring the surface of the electrode. Finally, this model has performed fully potential with medium to the very high complex shape of the electrode. An optimal combination of process parameters for an electrochemical machining process is proposed by using the particle swarm optimization algorithm [8]. Also, many works have been carried out for comparing the advantages of ECM and EDM in the production conditions [9, 10]. The results pointed out that ECM provides a more effective solution

22 Experimental Investigation of Effect of Process Parameters …

257

for manufacturing these materials in high volume condition. In this meaning, the application of the ECM in this materials processing is the high-impact improvement for reducing processing time and the cost for manufacturing the tool electrode in the comparison with EDM process [12]. In [8, 9, 11], single objective or multi-objective optimization models are proposed for optimizing a set of process parameters of the electro-chemical machining process. The selection of optimum values of important process parameters such as the tool feed rate, electrolyte flow velocity, and applied voltage is proposed for the electrochemical machining processes [8]. However, this study ignores the important effect of pressure of water and frequency which play a very important role on the surface rough of finished products. The effect and parametric optimization of process parameters in [11] that are electrolyte concentration, feed rate and applied voltage is proposed for the electrochemical machining of EN31 steel. This work also ignores the important effect of pressure of the fluid and frequency in machining process of the ECM. In this chapter, the research focuses on the study about effectiveness of the processing parameters, which are current, voltage, the pressure of the fluid, cutting speed and pulse, of the ECM to the surface roughness of the finished product. Experiments are setup to collect the data of the effect from these parameters by using the design of the experiment. With achieved results, Minitab software is used to calculate the result from practical experiments. A Taguchi orthogonal array is built to narrow down the factors that can affect the variance of the SR. Then, WEKA software is used to a statistical model (or regression function) which illustrates the relationship between processing parameters to the SR of finished products. Finally, the mathematical model is validated by practical experiment with the optimal parameters determined by using the genetic algorithm (GA). A set of optimal parameters is used to repeat the experimental results that then are validated via measuring the SR of the achieved finished product by using the RTEC Universal 3D Profilometer. The achieved results are then compared to the ones in which another set of parameters are used for the ECM to show advancement of the proposed method.

22.2 Experimental Study In this section, an experimental setup is introduced firstly with facilities that needed for experiments. In the next section, a section of work piece and tool materials are discussed. Then, a necessary procedure of the method of design of experiments are provided. Finally, experiments and data collections are made in the end of the section.

22.2.1 Experimental Preparation and Setup For carrying out experimental studies, a list of equipment is used for the not only process the workpiece but also for preparing the workpiece and measuring the SR of

258

L. P. Ngo et al.

the workpiece after manufacturing. Additionally, the main purpose of this research is to find out the optimized parameter for industries applications, therefore, a set of modern machines have been used to examine the surface roughness of the final product. Facilities are used for experimental study including the ECM machine, AMADA Surface Grinder 126, Mitutoyo Portable Surface Roughness Measurement Surftest SJ-210, and RTEC Universal 3D Profilometer. PEM Technology-PEM 600. Figure 22.1 shows an ECM machine which uses the pulse power monitoring. The machine consists of four main blocks as illustrated in Fig. 22.1. There are many control factors for this machine such as Velocity/feed rate (Vmin ), Electrolyze flow control (P), Voltage (U), Frequency (f), The pulse control unit (ms), Pressure of fluid (KPa) and Initial gap (mm). AMADA Surface Grinder 126. This machine is used to eliminate the effect of the initial surface roughness of the workpiece to the surface quality of post-production. This machine is used to grind the workpiece for approximately achieving the SR of Ra = 0.1 µm. The advantage of this machine is that it applies the NC controller for controlling the wear of grinding disc. Mitutoyo Portable Surface Roughness Measurement Surftest SJ-210. This instrument, shown in Fig. 22.2, is used for measuring the surface roughness of the tool before and after processing material as well as for measuring the finished surface. The initial assumption for this calibration is with normal value of 2.97 µm, tolerance is 0.02 µm. The whole measurement system is adjusted and measured until the value of Ra equal to 2.970 µm. After that, 50 experiments are recorded continuously. This process is used to set up a desired position for the whole system. The measurement system is shown in Fig. 22.3. RTEC Universal 3D Profilometer. This instrument is used to measure the finish surface of the product for validation phrase.

Fig. 22.1 Electrochemical machining

22 Experimental Investigation of Effect of Process Parameters …

259

Fig. 22.2 Mitutoyo SJ-210 (4 mN type)

Fig. 22.3 Measurement system of Mitutoyo instrument

22.2.2 Selection of Work Piece and Tool Materials Workpiece. To simulate the practical condition in industry, SS AISI 316 Stainless Steel which is already extruded to cylinder form with the diameter equal to 150 mm is chosen. AISI 316 Stainless Steel is the alloy of steel (around 62%) with Cr (maximum 18%), Ni (Maximum 14%), Mo (3%), Mn (%), C (0.8%) (“ASM materials Data Sheet”). With the hardness around HR = 79, higher corrosion compares with AISI 302 and AISI 304 and high melting point (around 1370 °C), AISI 316 stainless steel is widely used in food and pharmacy process equipment such as surgical implants and or the handle tools requires high chemical resistance process. The workpiece

260

L. P. Ngo et al.

Fig. 22.4 Surface of the workpiece after manufacturing

is then milled to achieve the initially flat surface. In the next step, the workpiece is processed throughout the drilling and the grinding machine to achieving the surface roughness Ra = 0.1 µm as shown in the Fig. 22.3. The homogeneous SR ensures that the effect of initial surface quality of the workpiece does not affect to the final surface roughness of the finished product. The condition of the workpiece after manufacturing is shown in Fig. 22.3. The surface condition of the workpiece is different from the setting parameters. However, there is some zone in which the surface roughness of the workpiece after processing are quite high. Moreover, the surface roughness condition of the workpiece is nearly not changed during the testing condition, but the surface is oxidized after manufacturing the parameter set that caused high surface roughness. Tool. PEM600 has the capability to use many types of conductive material for the ECM process. However, for the cost saving in industry, the cooper is used to manufacture the tool. Since, this paper focuses only on optimizing the surface roughness of the final product, this design ensures the uniformity effect of the substance flow in the whole area. For each experiment, the tool is manually ground by 2000 grit sandpaper which makes the SR of the tool achieve the value of Ra that is less than 0.1 µm. Figure 22.5 shows a sample surface of high roughness surface (left) and the surface of electrode after manufacturing (right). The surface roughness of the tool is measured in four positions and takes the average value of these four measures. They are the same method for measuring the finished surface of the workpiece, as shown in Fig. 22.4.

22 Experimental Investigation of Effect of Process Parameters …

261

Fig. 22.5 Sample surface of high roughness surface (left) and the surface of electrode after manufacturing (right)

22.2.3 Design of Experiments For the purpose of examining the influence of the machining parameters including feed rate, pressure, voltage frequency, and pulse on the SR on tested specimens, a full factorial design approach with range of each parameter is considered in Table 22.1 for the experiments These parameters of feed rate, pressure, voltage, frequency and pulse, shown in Table 22.1, are selected by basing on the recommended parameters from manufacturers of the PEM600 machine. These parameters are also conducted via our experiences as we are operating the machine. The range of each parameter is chosen specifically as in Table 22.1. These ranges are divided into five levels for assessing the effect of each range into the response of surface roughness for the initial experiments. In other words, a single replicate of 5 factors with 5 levels would be used for experimental setup. The selection for an experimental matrix of five control parameters can be based on a full factorial design in which the correlation between these control factors can be Table 22.1 Electrochemical machining process parameters Process parameters

Level 1

Level 2

Level 3

Level 4

Level 5

Feed rate (mm/min)

0.02

0.115

0.21

0.305

0.4

Pressure (kPas)

300

350

400

450

500

Voltage (V)

6

7.5

9

10.5

12

Frequency (Hz)

40

52.5

65

77.5

90

Pulse (ms)

0.5

1.625

2.75

3.875

5

262

L. P. Ngo et al.

examined and predicted. However, due to the wide range of each parameter (which are chosen from the suggested control parameters of machine manufacturer), the number of the experiment (n) is the combination of five parameters and which are divided into five level. It means that there are 55 (= 3125) experiments that must be implemented to obtain database for analysis. For optimizing the cost and time for collecting data, the approach of Taguchis’s method is applied for five control parameters (Velocity/feed rate (Vmin), flow control (P), Voltage (U), Frequency (f), The pulse control unit (ms)). Based on the suggestions from Minitab software for fives control factors with five levels, the Taguchis L25 orthogonal arrays is chosen as shown in Table 22.2. Corresponding values for the Taguchis L25 orthogonal arrays are shown in Table 22.3. This array consists of 25 experiments which insignificantly Table 22.2 Taguchis L25 orthogonal arrays Number of experiments

Feed rate (mm/min)

Pressure (kPas)

Voltage (V)

Frequency (Hz)

Pulse (ms)

1

1

1

1

1

1

2

1

2

2

2

2

3

1

3

3

3

3

4

1

4

4

4

4

5

1

5

5

5

5

6

2

1

2

3

4

7

2

2

3

4

5

8

2

3

4

5

1

9

2

4

5

1

2

10

2

5

1

2

3

11

3

1

3

5

2

12

3

2

4

1

3

13

3

3

5

2

4

14

3

4

1

3

5

15

3

5

2

4

1

16

4

1

4

2

5

17

4

2

5

3

1

18

4

3

1

4

2

19

4

4

2

5

3

20

4

5

3

1

4

21

5

1

5

4

3

22

5

2

1

5

4

23

5

3

2

1

5

24

5

4

3

2

1

25

5

5

4

3

2

22 Experimental Investigation of Effect of Process Parameters …

263

Table 22.3 Taguchis L25 orthogonal arrays: experimental values Number of experiments

Feed rate (mm/min)

Pressure (kPas)

Voltage (V)

Frequency (Hz)

Pulse (ms)

1

0.02

300

6

40

0.5

2

0.02

350

7.5

52.5

1.625

3

0.02

400

9

65

2.75

4

0.02

450

10.5

77.5

3.875

5

0.02

500

12

90

5

6

0.115

300

7.5

65

3.875

7

0.115

350

9

77.5

5

8

0.115

400

10.5

90

0.5

9

0.115

450

12

40

1.625

10

0.115

500

6

52.5

2.75

11

0.21

300

9

90

1.625

12

0.21

350

10.5

40

2.75

13

0.21

400

12

52.5

3.875

14

0.21

450

6

65

5

15

0.21

500

7.5

77.5

0.5

16

0.305

300

10.5

52.5

5

17

0.305

350

12

65

0.5

18

0.305

400

6

77.5

1.625

19

0.305

450

7.5

90

2.75

20

0.305

500

9

40

3.875

21

0.4

300

12

77.5

2.75

22

0.4

350

6

90

3.875

23

0.4

400

7.5

40

5

24

0.4

450

9

52.5

0.5

25

0.4

500

10.5

65

1.625

afford for carrying out the practical experiments, but it still can be used to be analyzed based on Minitab software for plotting the effect of the single effect of each factor to the surface roughness of finished products. For further study and analysis, a set of control parameters are re-peat two times to avoid rare variations in setup of experiments. Also, two experiments with the same parameters are used for estimating the robustness of experiments.

264

L. P. Ngo et al.

22.2.4 Experiments and Data Collection Based on the initial data and experimental setup as discussed in Sect. 22.2, Table 22.1 and the depth of cut for all experiments is set at a value of 0.1 (mm) in combination with above parameters. Due to the change in the initial position after grinding the surface of the workpiece and the tool, the processing time is not recorded. By applying these setting parameters, the achieved results of experiments are shown in Table 22.4 that shows the data after cutting the first and second sets of parameters. Due to a high noise in experimental process, Dixon’s Q test (or Q-Test) is applied for eliminating the strange value from the collected data of the achieved data in which the surface Table 22.4 Experimental results of surface response (SR, µm) Number of experiments

Feed rate (mm/min)

Pressure (kPas)

Voltage (V)

Frequency (Hz)

Pulse (ms)

Surface rough (µm)

1

0.02

300

6

40

0.5

0.3

2

0.02

350

7.5

52.5

1.625

0.35

3

0.02

400

9

65

2.75

0.45

4

0.02

450

10.5

77.5

3.875

0.82

5

0.02

500

12

90

5

0.43

6

0.115

300

7.5

65

3.875

0.14

7

0.115

350

9

77.5

5

0.23

8

0.115

400

10.5

90

0.5

0.98

9

0.115

450

12

40

1.625

0.2

10

0.115

500

6

52.5

2.75

0.53

11

0.21

300

9

90

1.625

0.74

12

0.21

350

10.5

40

2.75

0.55

13

0.21

400

12

52.5

3.875

0.86

14

0.21

450

6

65

5

0.24

15

0.21

500

7.5

77.5

0.5

0.59

16

0.305

300

10.5

52.5

5

0.22

17

0.305

350

12

65

0.5

0.38

18

0.305

400

6

77.5

1.625

0.53

19

0.305

450

7.5

90

2.75

0.36

20

0.305

500

9

40

3.875

0.19

21

0.4

300

12

77.5

2.75

0.24

22

0.4

350

6

90

3.875

0.22

23

0.4

400

7.5

40

5

0.33

24

0.4

450

9

52.5

0.5

1.66

25

0.4

500

10.5

65

1.625

1.67

22 Experimental Investigation of Effect of Process Parameters …

265

Main Effects Plot for Surface Roughness Data Means

Velocity

1.2

Pressure

Voltage

Pulse

Frequency

Surface Roughness

1.0

0.8

0.6

0.4

0.2

0.0 1

2

3

4

5

1

2

3

4

5

1

2

3

4

5

1

2

3

4

5

1

2

3

4

5

Fig. 22.6 Response value for each level of each control factors

roughness is the average number of the processed data. By using Minitab software for analyzing the results from the first 25 experiments (As L25 orthogonal arrays), the effect of each control parameter for the response value (surface roughness) is shown in Fig. 22.6. Indicating that Fig. 22.6 just illustrates the response for every single factor, the interaction between each factor cannot be shown by this analysis. Based on the analysis results from Minitab, each factor has the range in which the response for surface get the better value (smaller SR). This suggest that a higher accuracy will be improved with a higher amount of data. Thus, a new set of the control parameter might provide a further accuracy. In this research, results in Table 22.4 will be used for generating a statistical model (or regression function) and then an optimization process using the genetic algorithm is applied for an optimal set of process parameters. A further work will be explained in detail in the next section.

22.3 Optimal Selection of Process Parameters in ECM Process 22.3.1 Weka Software for Regression Model We illustrate the relation between the control factors and the response of surface roughness of processed surface by ECM. A statistical model is built in which the output of this model is the value of surface roughness and the input is the value of

266

L. P. Ngo et al.

control parameters. In general, and for simplifier, a statistical model is a mathematical model in which the reality is described by an equation made by one or many input parameters and the output is the questionable factor. This model can be used for predicting the output value based on the input parameters. There are two kinds of the variable in a statistical model, the first one is dependent variables which is the value that needs to be explained or predicted. In this study, the dependent variables are the response of surface roughness. The second variables are the independent variable(s) which are used to explain or predict the dependent variables. In this study, independent variables are feed rate, flow pressure, voltage, frequency, and pulse. There are many approaches to build a statistical model. However, in this paper, the software called WEKA (Waikato Environment for Knowledge Analysis) is used. This software is widely used for the study of machine learning in many purposes such as classify and cluster. Based on the requirement for building the statistical model that illustrates that relationship between given parameters and the value of surface roughness, the classify function of WEKA is used. In simplify term, the classify term is usually used in machine learning science and it is referred to build an identification for of population based on the observed sample in that population. There are many kinds of filters (with difference algorithm) used for classification in WEKA. However, for simplify, this paper focuses only on two kinds of filter: Linear Regression and Least Square Regression. After choosing the filter that is used in WEKA for building the statistical model or objective function, the collected data is input into WEKA by excel CSV type. Cross-validation is chosen with the test option of building this model. As the above results in Table 22.4, there is several statistical models that can been achieved by different methods via WEKA software. All these models can be used to machine setup and find the optimal sets of parameters for the response of surface roughness. However, the linear statistical model which is built by using the achieved data is not convenient for further optimization process. In stead of a linear statistical model, a nonlinear statistical model which is built by using the extension of achieved data in Table 22.4 is generated by using the WEKA software, the achieved results of a nonlinear statistical model (or regression function) are shown in (22.1) as SR = −0.131 V − 0.0099 U + 0.0323 MS + 1.3213 V2 + 0.30 U 2 + 0.0084 MS2 + 0.0014 VU − 0.2707 VMS + 0.3048

(22.1)

where V is velocity/feed rate, U is voltage, MS is the pulse control unit (ms). From the achieved results with WEKA software, the correlation coefficient is 0.3597, the root mean squared error is 0.5189 for the total number of instances of 45. As a prediction, the results also confirm that the weights of pressure of fluid and frequency, 0.0006 and 0.00035 respectively, play an insignificant role in reducing the SR in comparison with other factors. So, the terms of pressure of fluid and frequency are ignored in (22.1) for further optimization procedure. From (22.1) and Fig. 22.6, one can realize that the feed rate of machining processing plays an important role in reducing the

22 Experimental Investigation of Effect of Process Parameters …

267

SR of finished products and the applied voltage can also be considered to support to reduce the surface roughness of finished products.

22.3.2 Optimal Selection of Process Parameters In this statistical model, the single objective target has been solving for finding the optimized solution for the response of the surface roughness with objective function in (22.1). As mentioned above, based on the result with a high correlation coefficient of the statistical model built from the mixed results from two sets of original data with the processed data from Minitab is used for optimizing. The problem statement is stated as finding optimal processing parameters such that the objective function (22.1) is minimized subject to constraints and boundary conditions as shown in design matrix in Table 22.1. By using the genetic algorithm (GA), the optimal values of machining parameters are archived as feed rate of 0.4 mm/min, voltage of 12 V, and pulse of 0.5 ms. These values corresponding to the surface roughness of 0.17 µm are setup with new experiments for samples with goals for comparison and validation of the proposed method in the next section.

22.3.3 Analysis and Validation of Experimental Results In the chapter, the achieved model a nonlinear statistical model will be validated and compared by practical ECM process for assessing the quality of the surface. In this approach, the optimal values of machining parameters are used to machine three sets of new samples with the optimal parameters for validation and comparison. After analyzing three manufactured samples, the results show that the averages of the SR of finished products corresponding to three times of experiments are 0.159 µm, 0.182 µm, and 0.212 µm, respectively. These numbers indicate the reliability of experiments with the same set of parameters. These values are also smaller than the calculated value in term of a formula [12] which is 0.21 µm. Figure 22.7 shows a small area of surface of manufactured sample with optimal parameters that is equivalent to the average of 0.159 µm. To show the variations of the SR of the achieved sample, the three lines (upper, middle, bottom) in Fig. 22.7 are investigated for validation. Figure 22.8 shows the distributions of the arithmetical mean height (Ra) of the manufactured sample with the optimized parameters. The upper, middle, and bottom lines in Fig. 22.8 show variations of the Ra corresponding to the upper, middle, and bottom lines in Fig. 22.7. The results in Fig. 22.8 indicate that the averages of Ra are 0.132 in the upper line, 0.123 µm in the middle line, and 0.144 µm in the bottom line. Thus, these results show that the experimental surface roughness of the finished product is closer to the theoretical value that is 0.17. Also, based on the captured image in Figs. 22.7 and 22.8 about the surface of the sample after manufacturing by ECM, the surface of the products is in the familiar condition as the surface or the tool

268

L. P. Ngo et al.

Fig. 22.7 Surface condition of the sample with optimized parameters

(for the optimized condition only). These results indicate that the achieved regression function is validated and useful for ECM users for manufacturing applications.

22.4 Conclusion This paper investigates effects of the processing parameters, which are current, voltage, the pressure of the fluid, cutting speed and pulse, of ECM processing on the surface roughness of the finished products. In this approach, experiments are prepared, implemented, and collecting the data of the effect from these parameters by using the surface response methodology. With achieved results, the Minitab software is used to calculate and analyze the results of practical experiments in order to show considerable effects of each factor. Then, the WEKA software is used to generate a statistical model (or regression function) which illustrates the relationship between processing parameters to the SR of finished products. With the achieved model, a set of optimization parameters is achieved by using the genetic algorithm. Finally, the mathematical model is validated again by practical experiments with the optimal parameters for comparison. Further, as suggested in the discussion section, the five control parameters of the surface roughness could be a collapse by skipping the relationship of fluid pressure and the frequency. For the extension of future study, the value of fluid pressure and frequency must be chosen from the provided range. Also, a new approaching with the different filters should be used to illustrate the truly non-linear regression model in the future work.

22 Experimental Investigation of Effect of Process Parameters …

269

Fig. 22.8 Plot of the surface roughness of the sample with optimized parameters

Acknowledgements This work was supported by to the Ministry of Education and Training for the funded project of code KC-519 (Decision 5652 on 28/12/2018).

270

L. P. Ngo et al.

References 1. R.H. Todd, D.K. Allen, L. Alting, Manufacturing Processes Reference Guide (Industrial Press, New York, 1994) 2. B. Bhattacharyya, J. Munda, M. Malapati, Int. J. Mach. Tools Manuf 44(15), 1577–1589 (2004) 3. K. Rajurkar, M.M. Sundaram, A.P. Malshe, Procedia CIRP 6, 13–26 (2013) 4. B. Bhattacharyya, S. Mitra, A.K. Boro, Robot. Comput.-Integr. Manuf. 18(3–4), 283–289 (2002) 5. M. Datta, D. Landolt, Electrochem. Acta 26(7), 899–907 (1981) 6. J. Kozak, K. Rajurkar, Y. Makkar, J. Mater. Process. Technol. 149(1–3), 426–431 (2004) 7. M. Purcar, L. Bortels, B. van den Bossche, J. Deconinck, J. Mater. Process. Technol. 149(1–3), 472–478 (2004) 8. R.V. Rao, P.J. Pawar, R. Shankar, Proc IMechE J. Engg. Manuf. 222, 949–958 (2008) 9. P. Asokan, R. Ravi Kumar, R. Jeyapaul, M. Santhi, Int. J. Adv. Manuf. Tech. 39, 55–63 (2008) 10. C.-K. Yang, C.-P. Cheng, C.-C. Mai, A. Cheng Wang, J.-C. Hung, B.-H. Yan, Int. J. Mach. Tools Manuf. 50(12), 1088–1096 (2010). https://doi.org/10.1016/j.ijmachtools.2010.08.006 11. D. Chakradhar, A.V. Gopal, Int. J. Mode. Optim. 1, 113–117 (2011) 12. L.P.T. Huynh, H.A. Nguyen, H.Q. Nguyen, L.K.H. Phan, T.T. Tran. J. Korean Soc. Precis. Eng. 36(8), 705–712 (2019) 13. K.-H. Choi, T.T. Tran, B.-S. Yang, D.-S. Kim, An new approach for intelligent control system design using the modified genetic algorithm, Int. J. Intelligent Systems Technologies and Applications, 9(3/4), 300–315 (2010)

Chapter 23

Optimization of Surface Roughness and Vibration During Thermal—Assisted Milling SKD11 Steel Using Taguchi Method Thi-Bich Mac, Banh Tien Long, and Duc-Toan Nguyen Abstract This chapter used the Taguchi experimental design method in order to study the surface roughness and vibration during thermal-assisted milling of SKD11 steel. The effect of cutting parameters such as cutting speed, feed rate, cutting depth and support elevated temperatures on the output data were evaluated. Multi-objective optimization for minimum both surface roughness and vibration was also estimated to improve the cutting process. The optimal set of control parameters to achieve the minimum of surface roughness and vibration amplitude could be obtained as V c = 280 m/min, f = 230 mm/min, t = 0.5 mm, T = 400 °C.

23.1 Introduction The introduction and widespread use of high-strength, heat-resistant and hard-tocut materials have increased the difficulty for manufacturing processes. A proposed solution to overcome these problems is to work with the thermal—assisted machining (TAM), also called hot machining processing. The manufacturing industry has been developed with various thermal—assisted machining (TAM) such as electric, arc heating, high-frequency electromagnetic induction, laser beam, electron beam, plasma and so on. However, these technologies are suitable for some special machining methods, not for all. It is important to select the appropriate heating method otherwise the heat generation may damage the workpiece and then not to achieve the desired results [1]. Amin and Abdelgadir [2] have shown that electromagnetic induction heating can reduce vibrations by up to 98% and increase tool life many times when processing steel. Other works on induction

T.-B. Mac Department of Mechanical Engineering, Hung Yen University of Technology and Education, Dan Tien, Khoai Chau, Hung Yen, Vietnam B. T. Long · D.-T. Nguyen (B) School of Mechanical Engineering, Hanoi University of Science and Technology, No. 1A, Dai Co Viet, Hai Ba Trung, Hanoi, Vietnam e-mail: [email protected] © Springer Nature Switzerland AG 2020 I. A. Parinov et al. (eds.), Advanced Materials, Springer Proceedings in Materials 6, https://doi.org/10.1007/978-3-030-45120-2_23

271

272

T.-B. Mac et al.

heat machining have been reported advantages of hot machining by investigators [3–6], and plasma-assisted machining [7, 8] and laser-assisted machining [9–11]. There are many studies on the influence of input parameters such as cutting speed, tool speed, cutting depth to output parameters including cutting force, cutting vibration, surface roughness, etc. at room and elevated temperatures [12–14]. Surface roughness and cutting vibration are some of the important output data to assess the quality of products and production costs. Kumar et al. [15] studied the effect of spindle rotation speed and tool speed on surface roughness when turning Carbon steel on CNC lathes. Five types of steel SAE8620, EN8, EN19, EN24 and EN47 are used for research, respectively. The results show that the spindle rotation and tool speed has a direct effect on surface roughness. Surface roughness increases as feed rate increases and spindle speed decreases. The study of cutting process optimization was studied by various works [12, 16– 20]. Chang et al. [17] analyzed surface roughness when processing Al2 O3 embryos in the laser-heated process. The test results were analyzed by the Taguchi method and the optimal technology parameter set was established. Cutting speed has the strongest influence on surface roughness with 42.68% of the influence. Other parameters include the depth of cut, step forward and the frequency of pulses with less influence in order of 20.73%, 22.58%, and 14.01%, respectively. The optimal control parameter set is defined as t = 0.2 mm, V = 1500 rpm, f = 0.03 mm/r, and pulse frequency of 40 kHz. In this chapter, the effect of cutting parameters on the surface roughness and vibration amplitude of the cutting process when processing SKD11 steel materials in the electromagnetic heating environment was studied. Processing experiments at room temperature and heating conditions are performed continuously. Subsequently, the optimum cutting and temperature parameters were obtained to achieve the multiobjective surface roughness and vibration amplitude based on the Taguchi method. The relationship between surface roughness and vibration amplitude depends on the cutting parameters at elevated temperatures that were built on the nonlinear tool— regression of Minitab software [17]. The results of the study were finally compared with experimental data for highly compatible results.

23.2 Experimental Work 23.2.1 Material The Japanese standard SKD11 [JIS-G4404] is alloy steel commonly used in mold machining [21]. SKD11 steel has high-strength, impact resistance, and good deformation resistance. Moreover, it has the ability to keep the hardness at high temperatures for a long time. Therefore, SKD11 steel is often used in the production of extrusion molds, plastic injection molds, pressure molds, details that require special use properties and so on. Tables 23.1 and 23.2 are the chemical composition and

23 Optimization of Surface Roughness and Vibration During Thermal …

273

Table 23.1 Chemical composition of SKD11 steel,% mass [21] C

Cr

Mo

Si

Mn

Ni

V

1.4–1.6

11–13

0.7–1.2

≤0.6

≤0.6

–

0.15–0.3

Table 23.2 Physical properties of SKD11 steel [22] Physical properties Specific weight

(kg/m3 )

Value

Physical properties

Value (10−6 /k)

8400

Thermal expansion coefficient

Poisson’s coefficient

0.3

Specific heat (J/kg °C)

461

11

Melting temperature (°C)

1733

Thermal conductivity (W/m K)

20.5

physical properties of SKD11 steel, respectively.

23.2.2 Experimental Design The experiment was carried out on Taiwan’s MC500 milling machine. Spindle rotation speed 100–30,000 rpm, spindle power of 15 kW, the movement speed of the machine table when processing 30,000 mm/min, the maximum running speed: 48,000 mm/min, travel stroke X × Y × Z version = 500 × 400 × 300 mm. Do not use coolant during processing. Figure 23.1 shows a schematic diagram of SKD11 steel milling with thermostatic support. The heating element consists of induction power source, frequency generating device and induction coil. Test pieces of dimensions 70 mm × 31 mm × 80 mm are placed on a jig. The amplitude of the cutting process vibration is assessed by the accelerometer mounted on the jig. Study on using roughness meter SV—C3200 from Mitutoyo with Formtracepak software is shown in Fig. 23.2. The X- and Z-axis unit controllers are equipped with a linear encoder (ABS type on Z-axis) with high accuracy. Measuring the speed of the device: 0.02–5 mm/s. Method of measurement: the probe moves perpendicular

Fig. 23.1 Experimental diagram

274

T.-B. Mac et al.

Fig. 23.2 Roughness meter and measuring positions

to the machining trace; measure at three positions 1, 2 and 3 as shown in Fig. 23.2 then calculate the average result. The vibration measurement device is shown in Fig. 23.3. The LAN—XI data acquisition module has 4 inputs and 2 51.2 kHz frequency outputs from Bruel & Kjaer Denmark. PULSE FFT 7770 analysis module, 1–3 channels, PULSE FFT of Bruel & Kjaer Denmark. Triaxial DeltaTron 3-way accelerometer with TEDS 4525-B-001, titanium shell material.

23.3 Control Parameters and Levels With the goal of experimental design and optimization of control parameters in a simple, effective, economical and experimental manner, the Taguchi experimental design method has been selected. This method allows each parameter to be independently evaluated and randomized by the orthogonal array (OA). With the ability to narrow the scope of specific studies or identify production problems with existing data by appreciating the characteristic value for the average performance close to the target value. The Taguchi method has become a popular option to improve product quality [23]. This study investigates the effect of cutting mode parameters such as cutting speed (Vc ), cutting speed (f), cutting depth (t) and temperature (T) on surface roughness and vibration amplitude during the machining process. The measurement of the interaction between parameters through the S/N ratio. The S/N ratio is built for three

23 Optimization of Surface Roughness and Vibration During Thermal …

275

Fig. 23.3 Vibration measurement device for cutting process

goals following: bigger is better, smaller is better and normal is better. In this study, smaller is the better target is chosen. A better S/N ratio with a lower goal is expressed as (23.1). n 1 2 S = −10 log10 y N n i=1 i

(23.1)

n yi2 is the sum of squares for all results of each experiment, n is the where i=1 number of measurements for each experiment. Table 23.3 is a level set of cutting parameters and temperature for work-piece with cutting speed (V c = 190–280 m/min), feed rate (f = 230–380 mm/min), cutting depth (t = 0.5–1.5 mm) and temperature (T = 200–400 °C), respectively. The experiment Table 23.3 Control parameters and levels No

Control parameter

Unit

Level 1

Level 2

Level 3

1

V c (A)

m/ph

190

235

280

2

f (B)

mm/ph

230

305

380

3

t (C)

mm

0.5

1.0

1.5

4

T (D)

°C

200

300

400

276

T.-B. Mac et al.

Table 23.4 Experimental matrix and output data TN

V c (m/min)

f (mm/min)

t (mm)

T (°C)

Ra (μm)

AXY (dB)

1

190

230

0.5

200

0.128

141.601

2

190

305

1

300

0.137

147.405

3

190

380

1.5

400

0.159

148.931

4

235

230

1

400

0.091

141.919

5

235

305

1.5

200

0.176

151.139

6

235

380

0.5

300

0.126

139.388

7

280

230

1.5

300

0.109

148.343

8

280

305

0.5

400

0.090

137.004

9

280

380

1

200

0.162

147.632

is designed according to the method of orthogonal array Taguchi L9 with results of surface roughness (Ra) and vibration amplitude (AXY ), respectively, as Table 23.4.

23.4 Results and Discussion 23.4.1 Surface Roughness Table 23.5 presents the ANOVA results for surface roughness (Ra) during the SKD11 cutting with the thermal—assisted machining (TAM). The results indicated that the elevated temperature had the greatest influence on the surface roughness with the percentage of 37.6%. The feed rate had a second influence level of 31.6%. Cutting speed and cutting depth have less influence of 24.1% and 21.8%, respectively. Figure 23.4 shows the effect of the S/N ratio of each control parameter on the surface roughness during processing. The optimal set of parameters could be obtained as A3B1C1D3 corresponding to V = 280 m/min, f = 230 mm/min, t = 0.5 mm and T = 400 °C, respectively. Table 23.5 ANOVA results for surface roughness (Ra) Parameter

Mean of multiple S/N ratio

Sum of squares

Contribution

1

2

3

A

17.03

17.96

18.68a

0.000683

0.241

B

19.31a

17.77

16.6

0.002387

0.316

C

18.93a

17.95

16.79

0.001647

0.218

D

16.26

18.17

19.24a

0.002839

0.376

a Optimal

value

23 Optimization of Surface Roughness and Vibration During Thermal …

277

Fig. 23.4 S/N ratio of control parameters to surface roughness (Ra)

Table 23.6 ANOVA results for vibration amplitude (AXY-T ) during machining Parameter

Mean of multiple S/N ratio 1

2

3

A

−43.28

−43.17a

−43.18

B

−43.16a

−43.23

−43.24

3.383

0.018

C

−42.88a

−43.26

−43.49

157.371

0.814

D

−43.33

−43.23

−43.08a

26.350

0.136

a Optimum

Sum of squares 6.112

Contribution 0.032

level

23.4.2 Vibration Table 23.6 presents the ANOVA results for the vibration amplitude of cutting process by TAM for SKD11 steel. The results show that during processing, the cutting depth has the greatest impact on the vibration amplitude of 81.4%, followed by the temperature supporting the cutting process of 13.6%, the effect of cutting speed and feed rate on the vibration amplitude is negligible. Figure 23.5 shows the influence of S/N ratio of control parameters on the vibration amplitude during processing. The optimal set of control parameters could be obtained as A2B1C1D3 corresponds to V = 235 m/min, f = 230 mm/min, t = 0.5 mm, T = 400 °C.

23.4.3 Multi-response Optimization The above analysis presents the single optimization of output evaluation criteria such as surface roughness or cutting vibration. To find out the optimal set of parameters simultaneously for both surface roughness and cutting vibration, the study utilized Gray relational analysis (GRA). This method is effective in the study of objects with

278

T.-B. Mac et al.

Fig. 23.5 S/N ratio of control parameters to the vibration amplitude AXY-T

limited information. This technology effectively determines the complex relationship between the characteristics and qualities. Therefore, it becomes a powerful tool in the design of multi-objective optimization. The output target of both surface roughness and vibration amplitude is “lower-the-better”. The normalized form of the original sequence as follows: Sk j =

maxX k j − X k j maxX k j − minX k j

(23.2)

where j = 1 … 9; m is the number of experiments of Taguchi orthogonal array; k = 1… n, n is the number of process responses; max X kj and min X kj are corresponding the largest and smallest value of X kj for the kth response; S kj is the value after grey relational generation. To determine the relationship between the best and actual experimental results, a gray relationship factor GZkj is calculated using the following formula: GZk j =

Skmin − ξ Skmax Sk j + ξ Skmax kmax

(23.3)

where ξ is the distinguishing coefficient, 0 < ξ < 1. In this study, due to moderate discriminatory effects and good result stability, we select ξ = 0.5. GZkj is the coefficient of the gray relation of kth response in the jth experiment. The grade of grey relation (Gj ) is a coefficient that describes the weighted total of the gray relation, representing an overall evaluation of empirical data for multiobjective optimization. Gj is calculated using the formula: Gj =

n 1 GZk j n k=1

(23.4)

23 Optimization of Surface Roughness and Vibration During Thermal …

279

The normalized values of Ra and AXY , the process reactions and the levels of gray relationships are given in Table 23.7. The higher the gray relationship level, the combination of quality characteristics are close to the desired level. Thereby, better process parameters correspond to better process responses. The results in Table 23.7 and Fig. 23.6 show that experiment No. 8 has the highest gray relationship. Therefore, this test is the first priority, followed by test numbers No. 4 and No. 6. Therefore, A3B2C1D2 is the optimal set of control parameters to achieve the minimum target Ra and AXY . Table 23.8 evaluates the percentage of influence of the control parameters on the gray relational grade. The results show that factor C (cutting speed) has the highest contribution to overall performance with 39.84%. The factor D (elevated temperature) has the second-highest contribution with 35.63%. Eventually, the factor A (cutting speed) and B (feed rate) with 14.04% and 10.49%, respectively. Figure 23.7 presents the effects of process parameters on the gray relational grade. The optimal set of Table 23.7 Grey relational analysis results Exp. No.

S (for Ra)

S (for AXY )

GZ (for Ra)

GZ (for AXY)

G

Order

1

0.525

0.336

0.488

0.598

0.543

4

2

0.627

0.745

0.444

0.401

0.423

6

3

0.849

0.850

0.371

0.370

0.371

8

4

0.016

0.359

0.968

0.582

0.775

2

5

1.000

0.999

0.333

0.333

0.333

9

6

0.502

0.175

0.499

0.740

0.620

3

7

0.286

0.809

0.636

0.382

0.509

5

8

0.000

0.000

1.000

1.001

1.000

1

9

0.876

0.760

0.363

0.396

0.380

7

Fig. 23.6 The grey relational grade at various experiments

Factor

Vc

f

t

T

Symbol

A

B

C

D

0.419

0.721

0.609

0.445

1

0.517

0.526

0.585

0.576

2

Grey relational grade

Table 23.8 Grey relational analysis results

0.715

0.404

0.457

0.630

3

0.297

0.317

0.152

0.184

Max–min

2

1

4

3

Rank

0.0457

0.0511

0.0134

0.0180

Sum of squares

0.0228

0.0255

0.0067

0.0090

Mean square

35.63

39.84

10.49

14.04

Contributiton

280 T.-B. Mac et al.

23 Optimization of Surface Roughness and Vibration During Thermal …

281

Fig. 23.7 Effects of each process parameter on the Grey relational grade

control parameters for surface roughness and vibration amplitude is A3B1C1D3, corresponding to Vc = 280 m/min, f = 230 mm/min, t = 0.5 mm, T = 400 °C.

23.5 Conclusions The Taguchi method is used to experimentally design SKD11 steel milling in thermal—assisted machining (TAM) by electromagnetic induction. The influence of cutting parameters and elevated temperature on output parameters including surface roughness and cutting vibration amplitude were analyzed. The optimal design is implemented to determine the control parameters with multi-objective of both surface roughness and vibration amplitude could be obtained as cutting speed of 280 m/min, the feed rate of 230 mm/min, cutting depth of 0.5 mm and elevated temperature of 400 °C, respectively. Acknowledgements This research is funded by Vietnam National Foundation for Science and Technology Development (NAFOSTED) under grant number 107.02-2019.300.

References 1. 2. 3. 4.

G. Gurav, P. R. B, S. Patil, Int. J. Eng. 4(2), 55–61 (2016) A.K.M.N. Amin, M. Abdelgadir, J. Manuf. Sci. Eng. Trans. ASME 125(4), 674–680 (2003) K.M.A. Lajis, A.K.M.N. Amin, A.N.M. Am, J. Eng. Appl. Sci. 2, 421–427 (2009) M. Baili, V. Wagner, G. Dessein, J. Sallaberry, D. Lallement, Appl. Mech. Mater. 62, 67–76 (2011) 5. A. Amin, N.V. Talantov, Mech. Eng. Res. Bull. 9, 52–62 (1986) 6. M. Thi-Bich, D. Van-Chien, B. Tien-Long, N. Duc-Toan, Metals (Basel) 8(12) (2018) 7. G. Madhavulu, B. Ahmed, J. Mater. Process. Tech. 44(3–4), 199–206 (1994)

282

T.-B. Mac et al.

8. Z.Y. Wang, K.P. Rajurkar, J. Fan, S. Lei, Y.C. Shin, G. Petrescu, Int. J. Mach. Tools Manuf 43(13), 1391–1396 (2003) 9. P. Dumitrescu, P. Koshy, J. Stenekes, M.A. Elbestawi, Int. J. Mach. Tools Manuf 46(15), 2009–2016 (2006) 10. B. Shi, H. Attia, R. Vargas, S. Tavakoli, Mach. Sci. Technol. 12(4), 498–513 (2008) 11. M.J. Bermingham, P. Schaffarzyk, S. Palanisamy, M.S. Dargusch, Int. J. Adv. Manuf. Technol. 74(9–12), 1487–1494 (2014) 12. R. Makwana, H. Prajapati, Int. Conf. Multidiscip. Res. Pract. I(Viii), 488–489 (2014) 13. L. Özler, A. Inan, C. Özel, Int. J. Mach. Tools Manuf 41(2), 163–172 (2001) 14. T.L. Ginta, A.K.M.N. Amin, Int. J. Mach. Mach. Mater. 14(2), 194–212 (2013) 15. N. S. Kumar, A. Shetty, A. Shetty, K. Ananth, H. Shetty, Procedia Eng. 38(Icmoc), 691–697 (2012) 16. A.K.M.N. Amin, M.H.B.M. Saad, M.D. Arif, Adv. Mater. Res. 538–541, 799–803 (2012) 17. C.W. Chang, C.P. Kuo, Int. J. Mach. Tools Manuf 47(1), 141–147 (2007) 18. T.-B. Mac, V.-C. Dinh, T.-L. Banh, D.-T. Nguyen, Metals. 8, 992 (2018) 19. P. Thi-Hoa, M. Thi-Bich, T. Van-Canh, B. Tien-Long, N. Duc-Toan, Int. J. Adv. Manuf. Technol. (2017). https://doi.org/10.1007/s00170-017-1063-x 20. T.-H. Pham, T.-B. Mac, V.-C. Tong, T.-L. Banh, D.-T. Nguyen, Adv. Mech. Eng. 8(10), 168781401667329 (2016). https://doi.org/10.1177/1687814016673297 21. C. Wang, Y. Xie, L. Zheng, Z. Qin, D. Tang, Y. Song, Int. J. Mach. Tools Manuf 79, 31–48 (2014) 22. C. Wang, F. Ding, D. Tang, L. Zheng, S. Li, Y. Xie, Int. J. Mach. Tools Manuf 108, 13–26 (2016) 23. S. Du, M. Chen, L. Xie, Z. Zhu, X. Wang, Adv. Mech. Eng. 8(10), 1–12 (2016)

Chapter 24

Assessment of the Surface Roughness of Metal Mechanical Parts by Microsoft Kinect V2 Bui Van-Bien, Banh Tien Long, and Nguyen Duc-Toan

Abstract In mechanical manufacturing, the surface roughness of a machined part is a significant parameter to evaluate the products’ quality, and as a result, it must be thoroughly measured. Many researches have been studied over the past few to reduce the inherent drawbacks, such as contact, off-line inspection, speed of limited measurement, in the conventional measurement system using contact method. In this paper, the feasibility of the contactless inspection of part surface roughness using Microsoft Kinect v2 have been demonstrated. The part roughness parameters have been estimated by using of PCA plane fitting on point cloud data. In addition, the results received with the Microsoft Kinect v2 system are finally compared to those received with a stylus contact surface roughness measurement system to verify the proposed approach within this paper.

24.1 Introduction Surface roughness, irregular geometry characteristic, consists of peaks and valleys on the produced part surfaces. In the result of the extremely effect to many functional attributes of mechanical part as well the cost of production, surface roughness is an important factor of part quality in industry. The assessment of surface roughness can be achieved in several aspects. Fundamentally, the surface roughness measurement methods can be categorized into two groups: direct measurement methods and noncontact methods [1]. The most common method uses the stylus probe instrument to move across the surface to determine vibrations generated by the surface roughness. In agreement with the given precision, the size of stylus head can be chosen. A main disadvantage of this method is the possibility to damage the surface being measured by the stylus tip. Another drawback besides is that the resolution of this instrument depends principally on the diameter of the probe tip. Non-contact methods have B. Van-Bien (B) Department of Mechanical Engineering, Haiphong University, Haiphong, Vietnam e-mail: [email protected] B. T. Long · N. Duc-Toan School of Mechanical Engineering, Hanoi University of Technology and Science, Hanoi, Vietnam © Springer Nature Switzerland AG 2020 I. A. Parinov et al. (eds.), Advanced Materials, Springer Proceedings in Materials 6, https://doi.org/10.1007/978-3-030-45120-2_24

283

284

B. Van-Bien et al.

been developed to overcome these limitations. In this paper, a new approach using point cloud data from Microsoft Kinect v2 for inspecting surface roughness has been proposed. Over the last few decades, the procedure of digitizing the shape of physical objects, often abbreviated as the 3D-reconstruction, tends to be increasingly used everywhere from the entertainment to the industry [2, 3]. This has been nowadays widely made possible thanks to numerous technologies, namely laser scanners, stereovision, structured-light or the time of flight (ToF) for example. New applications still are found and existing applications to expand. On the issue of large objects, terrestrial laser scanners (TLS) are typically chosen because this technology allows collecting a large amount of accurate data very quickly. While trying to reduce costs and working on smaller pieces, on the contrary, digital cameras are regularly selected. Within this framework, concerning some features such as price or computation time, RGB-D cameras supply new possibilities for the modeling of complex structures, for instance in door mapping [2]. One of them, the Microsoft Kinect v1 launched in 2010, used the structured light technology to acquire the depth data, have met a great success in developer and scientific communities. The second version of Microsoft Kinect was released in 2014, which much improved the depth measurement accuracy. The latest Microsoft Kinect uses a ToF technology for acquiring the depth data. Compared with Kinect v1, the obtained point clouds from Kinect v2 have better quality and resolution as well as without limiting the interference from outside sources. The aim of this study was to identify the method for processing the point cloud data using of PCA plane fitting to estimate surface roughness according to a prepared experiment plan of measurements on Microsoft Kinect v2. The rest of the paper is structured as follows. First, some researches related existing works about surface roughness assessment using machine vision are introduced in Sect. 24.2. How to calculate the surface roughness from point cloud data by a method known as Principal Component Analysis (PCA) is presented in detail in the Sect. 24.3. The experimental tests and discussions are depicted in Sect. 24.4. Finally, the conclusion and the potential improvement of this paper are discussed in the last section.

24.2 Related Works Machine vision inspection is by far the most widely applied technology for quality control process. Using the computer vision techniques to investigate the surface roughness of a workpiece under various turning operations was introduced in [1]. The usefulness of this method was the non-contact measurements and ease of automation. In their works, to obtain the surface roughness of the workpiece by processing the surface image, a polynomial network with self-organized adaptive learning ability was selected. There was evidence that the polynomial network appropriately connected the input variables (cutting speed, feed rate, depth of cut, and the feature of surface image) with the output variable, surface roughness of the workpiece.

24 Assessment of the Surface Roughness of Metal Mechanical Parts …

285

Hatemleh et al. [4] also informed that the surface roughness was one of the most important parameters describing the surface integrity of a component since a significant proportion of component failure starts at the surface due to either discontinuity or deterioration of the surface quality. Based on the differences between laser-peened, and unpeened samples, the significantly higher surface roughness on specimens processed with shot peening was realized in this study. Moreover, the roughness of the weld nugget was proved steadily higher than the corresponding base material undergoing the laser-peened or shot peening process, seemingly from the lower hardness found in the nugget. To evaluate texture features from images of turned surfaces, the applicability of a geometrical model based Voronoi tessellation was investigated in [5]. With the purpose of assessment their symmetry, the centroidal cross-moments of the polygons were determined. Based on the number of symmetric polygons in the Voronoi diagram, the degree of homogeneity of the machined surface image was specified. As a result, the number of symmetrical polygons with low centroidal cross-moment should be greater for a surface that was machined under optimal cutting conditions. Whereas, Kocer et al. [6] performed an experiment and demonstrated that the surface roughness measurements acquired by 3D image processing method was like the values received by a profilometer on machined samples. It was concluded that there had been limited research on estimating the surface roughness of castings by 3D scanning and the current methods such as stylus profilometry, optical microscopy and qualitative methods of visual inspection did not deliver repeatable results and was inefficient due to the time and cost involved. For systems with Microsoft Kinect v2, the feasibility of applying a low-cost RGB-D camera with an appreciate accuracy to measure pavement roughness was checked [7]. Their works focused on collecting RGB, infrared, and depth data from different surface types with the different roughness levels at 10-m sections. Based on pixel-wise averaging over the acquired frames at each imaging position, a single depth frame was computed. The noise in each depth frame was reduced, the RGB images and the depth images were matched, and the RGB and depth images were also registered to create a 3D surface on the pavement surface. Although there are lots of researches for machine vision inspection as well as the capacity of Microsoft Kinect v2, non-method evaluates surface roughness using the Microsoft Kinect v2 until now.

24.3 Methodology 24.3.1 Measuring of Surface Roughness As reported by International Standards Organization (ISO), average surface roughness (Ra) is defined as the average deviation of the surface profile from the mean line. The equation for average surface roughness can be written as follows

286

B. Van-Bien et al.

Fig. 24.1 Surface profile example

Data Acquisition

Data Processing

Fitting a nominal surface

Finding residuals

Calculating Ra

Fig. 24.2 Methodology: surface roughness determination

1 Ra = L

L |y(x)|dx,

(24.1)

0

where L is the sample length of the profile, y is the coordinate of profile curve (see Fig. 24.1). As can be seen from (24.1), the average surface roughness of mechanical parts can be determined by calculating the average of normal distances of the points in point cloud data from a nominal surface. A nominal surface can be defined as a surface that has not surface irregularities and is geometrically perfect. The framework of the methodology used while determining Ra using the Microsoft Kinect v2 is depicted in Fig. 24.2.

24.3.2 Data Acquisition Using Microsoft Kinect V2 The part surface whose surface roughness is to be measured first needs to be scanned using Microsoft Kinect v2. This device has two cameras, namely, an infrared camera and an RGB camera. Moreover, it also includes infrared light sources, each of which produces a modulated wave with a various amplitude. Each Microsoft Kinect v2 device has its own depth intrinsic parameters which are sensor and lens dependent. In the factory, the calibration process was implemented, and the intrinsic parameters of each Kinect v2 are stored in its internal memory. These parameters can be achieved with the help of the Kin2 toolbox developed for Matlab [8]. The depth intrinsic

24 Assessment of the Surface Roughness of Metal Mechanical Parts … Table 24.1 Depth intrinsic parameters

287

Parameters

Symbol

Values (pixels)

Focal length

Fx

362.8785

Fy

362.8785

Cx

253.8325

Principal point Radial distortion

Cy

204.4191

K 1 (2nd)

204.4191

K 2 (4th)

– 0.26981

K 3 (6th)

0.0888

parameters of the infrared camera in the Microsoft Kinect v2 device using in this paper are introduced in Table 24.1. Based on the depth intrinsic parameters, the acquired depth map and the perspective projection relationship, the point cloud data of the mechanical part is obtained. Each pixel p(u, v) in depth map corresponds to a point P(X, Y, Z) in point cloud data. Then, X and Y of the point P are computed as follow X=

u − Cx · Z, Fx

(24.2)

Y =

u − Cy · Z, Fy

(24.3)

where Z is the intensity value of the pixel p(u, v) in the depth map. In the next section, a brief overview of principal component analysis used to estimate the nominal surface is introduced.

24.3.3 PCA Plane Fitting Generally, PCA is a statistical procedure to determine the number of uncorrelated variables in a large, high-dimensional dataset. These uncorrelated variables are called principal components which are axes that explain where variance is coming from. Nonetheless, it is assumed here that this is known; namely, that the surface of the mechanical parts being measured explains most of the variation. Hence, in this paper, the purpose of PCA is simply to try to find a representation of the nominal surface that can be used for further calculations. Computationally, given a point cloud matrix P, the principal components are the eigenvectors of the cov(P), that is, the covariance matrix of P. The most common way to find the eigenvectors is through a process known as the Singular Value Decomposition (SVD). If a point cloud P is first conditioned by centering each column, the SVD will give the principal components and the amount of variance attributed to each component [9]. After obtaining the principal components, the principal component

288

B. Van-Bien et al.

scores are calculated. Specifically, these are the new coordinates of the dataset in the space spanned by the principal components. In the developed MATLAB code, each coordinate, X, Y, and Z, is imported from the point cloud data into a data cell of size N by 3, where N is the number of points in point cloud data. The PCA plane fitting program is then used to this data cell to fit a plane to the point cloud on the data matrix. In the end, this returns a 3 by 3 data cell containing the principal components; the first, second and third columns represent the ordering of the principal components, respectively. The first two columns, which are the first two principal components, span the 2D space, that is, “X–Y plane”. The third principal component is orthogonal to the first two and defines the normal vector of the plane. Combined, this generates a new 3D coordinate system. To obtain the points in this new coordinate system, the centered N by 3 data cell is multiplied with the 3 by 3 matrix containing the principal components. At the close, an N by 3 data cell is obtained that consists of the location of each point in the new coordinate system spanned by the principal components. At this time, the residuals are simply the new Z-coordinates since they are instantly referenced from X 0 , Y 0 , Z 0 . Put it another way, by projecting the normal vector onto the X–Y plane, the peaks and valleys of the corresponding point cloud can be evaluated. Naturally, the PCA plane fitting program automatically measures the distances and outputs the average surface roughness value.

24.4 Results and Discussion 24.4.1 Experimental Setup Using a Microsoft Kinect for Windows v2.0 sensor, a PC with system CPU Intel (R) Core i7-4790 3.6 GHz; RAM 12 GB; Video card Geforce NVIDIA GVN730D5-2GI, the hardware of this test is configured and shown in Fig. 24.3. Fig. 24.3 Experimental setup

24 Assessment of the Surface Roughness of Metal Mechanical Parts …

289

To capture and process data, the needed software are Window 10 operating system, MATLAB 2016a with image processing toolbox, Kinect for Windows hardware support package for MATLAB, Microsoft Kinect SDK V2.0_1409 and Microsoft Visual Studio 2015, Kin2 toolbox for MATLAB. The experimental process is proposed into the flowchart and depicted in Fig. 24.4. For this experiment, two test parts are designed and manufactured out of A6061 and CT3. These parts are produced in an MANFORD MCB 850 machine with the same machining conditions, illustrated in Fig. 24.5. Fig. 24.4 Experimental process

Request for digitization

Microsoft Kinect v2

3D Scanning

Enough data Yes Data Processing

Format conversion

PCA plane fitting

Residuals Evaluating

Ra

No

290

B. Van-Bien et al.

Fig. 24.5 Test parts

24.4.2 Assessment of Surface Roughness Initially, the Microsoft Kinect v2 is used for acquiring the point cloud of the test parts. Before performing the measurement step, a calibration procedure is done on horizonal table surface. The dense point clouds obtained after scanning the test parts are shown in Figs. 24.6a and 24.7a. In order to trim the unnecessary points, an open source 3D point cloud processing software, MeshLab, is used and the point cloud is edited and processed. The resulting point clouds are then represented in Figs. 24.6b and 24.7b. To compare the results obtained using the Microsoft Kinect v2 with a conventional instrument, the surface roughness is also measured using the portable surface roughness tester SJ-210 by Mitutoyo, Japan. The results are shown in Table 24.2. The results obtained using the Microsoft Kinect v2 yielded a surface roughness value of 89.6 µm with a deviation of 8.131 µm which was closer to the value obtained by SL-210. It is also evident from the Table 24.2 that the surface roughness value of

Fig. 24.6 Point cloud of steel cube surface: a before trimming, b after trimming

24 Assessment of the Surface Roughness of Metal Mechanical Parts …

291

Fig. 24.7 Point cloud of aluminum cube surface: a before trimming, b after trimming

Table 24.2 Comparison of contact/now-contact surface roughness measurement values

Surface roughness values (with SJ-210)

Surface roughness values (with Kinect v2)

Test part

µm

Test part

µm

Steel

81.469

Steel

89.6

Aluminum

80.325

Aluminum

91.5

aluminum measured by the Microsoft Kinect v2 is more than 14% of by SJ-210. This phenomenon comes from the highly reflective surface of aluminum then the point cloud includes lot of noises. Therefore, the proposed PCA method can be used as an alternative way for estimation surface roughness of independent metallic surfaces scanned by Microsoft Kinect v2.

24.5 Conclusion In this paper, a new system for surface roughness assessment is proposed. The Microsoft Kinect v2 is used for the point cloud acquisition. In order to estimate the nominal surface of the point cloud data, the PCA plane fitting is built and programmed to calculate the surface roughness value. After experiments, it was observed that there was similarity between the values calculated from the processed method and the measurement made by a stylus profilometer. For future improvement of the developed system, software will be developed to increase the accuracy of this system.

292

B. Van-Bien et al.

References 1. 2. 3. 4. 5. 6.

B.Y. Lee, Y.S. Tarng, Int. J. Mach. Tools Manuf 41(9), 1251 (2001) K. Khoshelham, S.O. Elberink, Sensors 12(2), 1437 (2012) K. Kowsari, M.H. Alassaf, Int. J. Adv. Comput. Sci. Appl. 7(1), 584 (2016) O. Hatamleh, J. Smith, D. Cohen, R. Bradley, Appl. Surf. Sci. 255(16), 7414 (2009) A. Datta, S. Dutta, S.K. Pal, R. Sen, J. Mater. Process. Technol. 213(12), 2339 (2013) E. Koçer, E. Horozo˘glu, I. Asiltürk, in Seventh International Conference on Machine Vision (ICMV 2014), vol. 9445 (2015), pp. 944525 7. A. Mahmoudzadeh, A. Golroo, M.R. Jahanshahi, S.F. Yeganeh, Sensors (Switzerland) 19(7) (2019) 8. J.R. Terven, D.M. Córdova-Esparza, Sci. Comput. Prog. 130, 97 (2016) 9. M.E. Wall, A. Rechtsteiner, L.M. Rocha, in A Practical Approach to Microarray Data Analysis, ed. by D.P. Berrar, W. Dubitzky, M. Granzow. vol. 91 (Kluwer Academic Publishers: Boston) (2003)

Chapter 25

New Materials for Road Construction N. I. Buravchuk, O. V. Guryanova, M. A. Jani, and E. P. Putri

Abstract The burned rocks of some mine dumps of the Rostov region are evaluated. The physicomechanical properties of the rocks as raw materials for the construction of the subgrade of the access railway track, the structural layers of pavement are investigated. The properties of fractioned gravel and crushing screenings from burned mine rocks are given. The features of hardening of the massif of a roadbed of burnt rocks of mine dumps are shown. The technology of the subgrade and pavement layers is described. The possibility of using materials from burned mine rocks in the construction of subgrade, the ground of roads and structural layers of pavement has been substantiated. The variants of pavement designs using materials from burnt rocks of mine dumps are considered. Practical work was done on the erection of the subgrade railway track and local technological roads, industrial sites and sidewalks. The successful operation of sections of the railway access road, technological roads and sidewalks confirms the feasibility of using burnt rocks of mine dumps in road construction. The use of mine dump rocks allows us to solve some environmental problems: reduce the number of quarries in the extraction of natural raw materials, preserve the natural landscape of the earth’s surface, free land from dumps, and reduce pollution of water and air basins.

25.1 Introduction Every year, the reserves of natural raw materials are depleted. Complicated conditions for its production, the cost of natural mineral raw materials increase. In the coalindustrial regions of any country, huge reserves of mine rocks are concentrated in N. I. Buravchuk (B) · O. V. Guryanova I. I. Vorovich Mathematics, Mechanics and Computer Sciences Institute, Southern Federal University, Rostov-on-Don, Russia e-mail: [email protected] O. V. Guryanova e-mail: [email protected] M. A. Jani · E. P. Putri University of 17 Agustus 1945, Surabaya, Indonesia © Springer Nature Switzerland AG 2020 I. A. Parinov et al. (eds.), Advanced Materials, Springer Proceedings in Materials 6, https://doi.org/10.1007/978-3-030-45120-2_25

293

294

N. I. Buravchuk et al.

dumps. These are simultaneously extracted rocks during the development of coal deposits, extracted to the surface and stored in dumps. Such waste is a new type of raw material being technogenic. The accumulation of these wastes in terms of the quantity and quality of the contained raw materials suitable for producing useful products should be attributed to technogenic deposits [1]. In the context of increasing needs for natural mineral raw materials, the problem of the integrated use of all extracted raw materials and environmental protection is becoming of paramount importance and more acute every year. The prospects of using technogenic raw materials are obvious. The concept of integrated development of natural mineral resources involves the mandatory processing of waste into useful products as the final stage in the extraction of minerals. The task of improving the environmental situation in industrialized regions and expanding the range of new materials make this stage an indispensable necessity. With significant bulks of mine dump rocks, their disposal level is low. Mine rocks are very diverse and unstable. This is one of the reasons hindering their use. However, with appropriate processing and preparation, the quality of this waste can be brought to the requirements of regulatory documents. The development of such technogenic deposits will expand the mineral resource base of many industries, solve some problems to improve the state of the environment in each coal-mining region. Potential consumers of large volumes of coal industry waste can be road construction. Road construction is the most material-intensive area for the use of natural mineral raw materials. In this industry, there is an acute question of both improving the quality of structural layers of pavement and replacing natural materials, especially imported from other regions, with local, cheaper raw materials, in particular, with burnt rocks from mine dumps and ash and slag waste of thermal power plants. The development of effective road-building materials based on burned rocks and ash and slag waste, capable of working under conditions of increasing loads and climatic influences, and technologies for the manufacture of structural layers of pavement of increased bearing capacity are relevant. The use of fly ash and ash-slag mixture in road construction is known [2–4]. The use of burned mine dumps is not common.

25.1.1 Purpose of Research The purpose of this work is to establish the possibility of using burnt mine rocks in the construction of the subgrade and structural layers of pavement.

25.1.2 Field of Study We study the following issues: 1. composition and properties of burnt mine rocks;

25 New Materials for Road Construction

295

2. ways to increase the uniformity and stability of the properties of burnt mine rocks; 3. physical and mechanical properties of burnt mine rocks as materials for the construction of the subgrade and structural layers of pavement; 4. features of the formation of the structure and properties of the materials of pavement based on burnt mine rocks.

25.2 Research Method The object of research was burnt mine rocks accumulated in dumps in the Rostov region (Russia). Preliminary preparation of research objects was crushing and fractionating. Analytical and laboratory studies have been carried out in order to obtain information on the chemical and material composition of raw materials, physical and mechanical properties of burnt mine rocks. Technological tests were carried out on the use of burnt rocks of mine dumps in road construction. A complex of physico-chemical and technological studies allows us to determine the effectiveness and feasibility of using products from technogenic raw materials to ensure the reliability of the foundations and structural layers of pavement. Practical work on the construction of the subgrade and experimental sections of access technological roads using burnt rocks of mine dumps has been completed.

25.3 Results and Discussion 25.3.1 Characteristics of Burnt Rocks In coal mining, the associated rocks with an admixture of coal are emitted to the surface and stored in dumps. Subsequent conversions of stockpiled rocks in the dump largely depend on their initial composition. Rocks in dumps are subjected to prolonged thermal exposure in an oxidizing environment. Self-firing of rocks in ovals occurs relatively evenly and lasts several years. The product of prolonged self-firing of mine rocks is burned rocks. According to the state of aggregation, the studied rocks belong to solid formations, namely grid materials (blocky, dispersed and finely dispersed). The grain composition largely depends on the characteristics of the source rocks. The rock in the dump is presented from dust and ash fines, fine gravel to blocks weighing several kilograms. On average, fragments from 6 to 100 mm in size prevail. Pieces larger than 600 mm are available. Chunks of unburned coal and layers of lightly burnt rock are found. A visual inspection of the rocks revealed the presence of sulfur, cementing rock fragments. Self-firing of fine-grained sandstones and sandstone shales gives the most durable burnt rocks, consisting of large pieces. The dump contains rocks of low strength and rocks having a compressive strength

296

N. I. Buravchuk et al.

of 110–120 MPa. The fine fraction is obtained from finely and coarse layered clay and carbonaceous shales, carbonate and glandular minerals having lower mechanical strength. Burned rocks with water absorption in the range of 5–10% are moderately burnt, and with water absorption less than 5% well burned. The color of the breed varies from dark pink to reddish-brown and purple. The presence of clastic material in burned rocks, bonded with pelitic and siliceous natural cement to a state of conglomerate, ensures their high water-resistance and mechanical strength, reinforced by rock pressure and heat treatment. Under natural conditions, compaction and formation of rock-like rock occurred, the physical and mechanical properties of which depend on the degree of metamorphism and other characteristics. In the dump along with dense, well-burnt material, unburnt weak rocks, as well as coarse slag sintered with pieces of rock, can also locate. The quality of burnt rock in the dump can be determined by external inspection by the density of the structure, color, and the nature of the surface of the fracture of its pieces. A fractured and roughened or oily to the touch surface in a fracture indicates a poor qualitative material with a low bulk density and high water-absorption. Well-fired burned rocks of homogeneous composition, with a dense structure and a smooth stone-like surface in a fracture from dumps of anthracite coals are characterized by increased mechanical strength, resistance to abrasion, thermal and atmospheric influences. The specific effective activity of the radionuclides of the studied burned rocks does not exceed 370 Bq/kg. By this indicator, burned rocks belong to first class of materials, the use of which is unlimited. By chemical composition (see Table 25.1), burned rocks are siliceous-aluminous, i.e. characterized by a relatively high content of silicon and aluminum oxides. The content of acid oxides is more than 70%. By the sum of the oxides of silicon, aluminum and iron, the burned rocks are acidic raw materials. According to the classification of Sivertsev [5], rocks can be characterized as siliceous-alumina. Minor losses during calcination indicate the completeness of firing rocks. The largest clay-glandular module (0.4–0.57), in accordance with the classification of Knigina [6, 7], burned rocks belong to group I: mudstones are active and highly active. Burned rocks have a high chemical resistance: in relation to mineral acids—95 to 99% to alkalis—65.5 to 77.8%. The chemical and mineral compositions of burned rocks are interconnected. Coal waste differs in mineralogical composition. The mineral component of mine rocks stored in heaps is represented by sedimentary rocks. These are clays, loams, mudstones, siltstones, sandstones, limestones, siliceous schists, carbonaceous rocks. Thermal effects on rocks during prolonged self-firing cause significant changes in their mineral mass and physical condition. At the same time, the structure, texture and properties of the source rocks change significantly. The different mineralogical composition of the rocks and the conditions of the natural process of burning out the carbonaceous component lead to the formation of products of varying degrees of calcination. According to the lithological composition, the rock masses of the studied dumps of former mines are clay. The composition of the clay component is hydromica with an admixture of kaolinite and chlorite. Clays in coal seams are

SiO2

55.24

55.82

54.77

56.58

54.33

57.35

54.90

Mine

Named Komsomol’skoy Pravdy

Named Petrovskogo

Named Vorovskogo

Mayskaya

No. 26

Sevryugovka

Sinegorskaya

18.68

19.95

21.98

21.32

22.18

22.84

21.78

Al2 O3

Table 25.1 Chemical composition of burnt mine rocks, %

7.50

5.47

6.67

5.75

7.21

6.42

6.25

Fe2 O3

1.89

1.43

1.33

1.27

1.16

1.13

1.61

CaO

2.23

0.65

1.86

2.54

1.47

1.44

1.82

MgO

4.34

3.09

2.73

2.78

2.37

1.73

2.17

SO3

1.09

1.21

1.12

1.00

1.18

1.11

1.15

TiO2

5.25

4.59

4.08

4.07

3.98

3.85

4.70

(K2 O, Na2 O)

4.50

6.16

5.22

4.32

5.32

4.92

5.26

Loss on ignition

25 New Materials for Road Construction 297

298

N. I. Buravchuk et al.

so compacted under the influence of rock pressure that they have lost their ductility. Clay material is already dehydrated and greatly modified during self-firing. In terms of their basic physical and chemical properties, burned rocks are close to clays calcined at 800–1000 °C. Changes that occur with rocks during thermal exposure were recorded during X-ray and differential thermal analysis of siltstones and mudstones [8]. In the initial sample of siltstone (Fig. 25.1a), the lines of diffraction reflection d/n = 0.238; 0.357 and 0.714 are characteristic of kaolinite, and peak intensities d/n = 0.331; 0.498 nm— for hydromica. Strong lines of montmorillonite 1.105 nm and quartz (d/n = 0.333; 0.425 nm) are noted. The diffraction pattern of a sample of aleurolite calcined at 550 °C (Fig. 25.1b) is characterized by hydromica (d/n = 0.329 and 0.495 nm), quartz with a reflection of 0.334 nm. The lines of kaolinite disappear, which indicates its dehydration. For mudstones (Fig. 25.2), the presence of kaolinite can be judged along the lines of 0.238; 0.357; 0.714 nm, hydromica—according to the peak intensity of 0.331; 0.495 and 1.078 nm. The presence of quartz is confirmed by reflexes of 0.425; 0.333 nm; siderite—0.281 nm. On the diffraction pattern, taken from a sample of calcined quartz, mica-chlorite is observed. When conducting petrographic studies using a MIN-8 polarizing microscope, it was found that burned rocks are composed of clay minerals, mainly represented by kaolinite and hydromica, terrigenous material in the form of quartz, feldspars, ferruginous minerals and carbonate inclusions.

Fig. 25.1 Diffraction pattern of siltstone: a initial siltstone; b siltstone calcined at 550 °C

25 New Materials for Road Construction

299

Fig. 25.2 Mudstone diffractogram: a initial mudstone; b argillite, calcined at 550 °C

The mineral composition of burned rocks contains quartz, clay minerals, carbonates in the form of calcite, magnesite, dolomite, gypsum and alkali metal sulfates, iron is in the form of pyrite, marcasite, hematite. There are feldspars, modifications of crystalline silica—tridymite, cristobalite. The vitreous phase is represented by glass mainly melilite composition. Unburned fuel particles present as impurities are metamorphosed to different degrees, are different from the initial state and are in the form of coke and semi-coke and graphitized carbonaceous matter. An X-ray study of burned rocks revealed the following basic crystalline minerals: quartz and its modifications: iron in the form of magnetite and hematite; clay substance in the form of corundum, mullite. Secondary minerals are kaolinite, feldspars, sulfur, etc. Endograms associated with the removal of hygroscopic and bound water, exothermic effects due to oxidation of ferrous minerals, polymorphic transformations of quartz, burnout of carbonaceous substances, and decomposition of carbonates are observed on thermograms. Peaks in the thermograms appear as a result of processes occurring in that part of the rock that underwent insufficient firing in the dump or burned at a lower temperature. A well-calcined rock is thermally inert, and thermal effects are hardly detected on the differential thermal analysis curves of such rocks.

25.3.2 Burnt Mine Rocks for Subgrade Construction The burnt rocks of mine dumps belong to the class of coarse-grained soils, which are uncemented deposits of fragments, between which there are no structural bonds

300

N. I. Buravchuk et al.

(gravel, pebble, wood, gravel, sand) thermally changed in the dump under conditions of prolonged self-firing at a temperature of about 1000 °C. The assessment of the studied rock masses allows us to consider them as potential raw materials for the construction of embankments, dams, subgrade. Mine rocks, unlike conventional soils, traditionally used for the construction of subgrade, have specific properties, and they should be attributed to special soils. The physical and mechanical properties of burnt mine rocks as soil for a subgrade were tested. Work was completed on the construction of a subgrade railway access track with a length of 27 km. For this, the rocks of the dumps of the mines of Sevryugovka and Sinegorskaya were used. The composition and condition of the mine rock provides the ability to replace the soil for the construction of the subgrade. The structural design of the subgrade of the access railway is shown in Fig. 25.3. For laying rocks in the subgrade, their maximum fineness should not exceed 70 mm. Pieces of rock over 70 mm were crushed. Multiple transshipment of rocks with a bulldozer during shipment from the dump contributes to the averaging of rocks. The technology for the construction of subgrade from mine rocks is similar to the layered construction of the embankment from the traditional soil used. Dump mine rocks are well compacted. At the beginning of compaction in loose placer, individual grains of rock and crushed stone are easily distributed and mutually move. At the same time, large fractions of crushed stone play the role of a kind of spatial framework. Small particles fill the voids of the frame. These materials are well compacted, and dense packing of grains in the layer of the array is achieved. During this period, compaction can be carried out without moisture. When the initial sedimentation of the layer is achieved, further compaction requires overcoming the friction between the particles. To increase the compaction of the rock mass, watering is carried out. Water in this case facilitates compaction, as well as moisturizes fines and dust from wellburnt rock resulting from breaking of the edges of rubble during rolling. Maximum compaction is achieved with optimum moisture in the rock mass. Estimated water consumption 12–20 l/m2 . Compaction was completed when the deformation stopped

Fig. 25.3 Construction of the subgrade: 1—underlying layer of loam; 2—fractionated burned mine rock; 3—insulating layer of clay; 4—sand; 5—crushed stone from natural stone; 6—insulating layer of clay; 7—fertile soil; b—width of the main site; H—embankment height

25 New Materials for Road Construction

301

after the passage of a heavy roller, and the density of the rock layer reached 1.85– 1.90 g/cm3 . Similarly, from the burnt rocks of mine dumps, the foundation of roads is built. The ash content of the rock mass is high (90–99%). However, dumps contain impurities of non-burnt rocks. Therefore, there is an option for laying waste rock with a protective and insulating screen made of clay soil or loam. When planning slopes, a layer of fertile soil was applied and sowing of perennial grasses was carried out on the slopes.

25.3.3 Physico-Mechanical Properties of Burnt Crushed Stone from Mine Dumps According to the physico-mechanical properties, burnt mine rocks can be attributed to type III rocks, including rocks of heterogeneous strength, containing weak differences. Therefore, to obtain material from burned rocks of the required strength and durability, it is necessary to process mine rocks with enrichment in strength. The strength enrichment principle is based on the separation of materials of small fractions, the bulk of which are weak differences. Therefore, if, after crushing, the fine fraction is sieved from the products, then the remaining oversize product will be more uniform and strength. When crushing from burnt rocks, fractionated gravel, sand and crushing screenings can be obtained. Grain screenings according to the grain composition correspond to a sand-gravel mixture. Crushed stone and crushed sand from burned rocks [9] are not inferior in properties and quality to similar products from natural raw materials. In the result of the research, it was found that the crushed stone obtained by the two-stage crushing scheme of burned rocks of various terricones has the following main characteristics: • grade of crushed stone by strength during the crushing test—800; 1000; 1200; • mark for abrasion—I1; I2; • frost resistance, the number of cycles of alternate freezing and thawing, not less than—25; • bulk density, kg/m3 —1020 to 1240; • voids, %—45 to 55; • water absorption, %—0.5 to 5.0; • porosity, %—3.0 to 12.0; • true density, g/cm3 —2.5 to 2.7. Particles of crushed stone from burnt rocks are characterized by a porous structure with a developed surface. This circumstance leads to a lower bulk density of such crushed stone in comparison with traditional. In this indicator, crushed stone from burnt rocks are similar to artificial porous aggregates. Unlike the latter, burned crushed stones have greater strength, determined by compression in the cylinder and lower values for water absorption. Due to the rigid structure of the crystal lattice,

302

N. I. Buravchuk et al.

micropores in the particles of crushed stone cannot pass into open pores, and water molecules do not penetrate into the space of micropores; therefore, water absorption of crushed stone from burnt rocks is low. There are no clay and silty particles in the crushed stone from burnt rocks, there is no clay in the lumps, and the content of grains of weak rocks does not exceed the permissible limits. The particle shape is angular, non-rounded, the surface is rough. The content in the crushed stone of lamellar and needle-like grains is up to 25%. Crushed stone withstands the tests for structural stability against all types of decay. Crushed stone does not contain impurities and components that are classified as harmful. However, metamorphosed unburned fuel particles may be present. In composition, they are different from the original fuel and consist of coking products. They are resistant to oxidation and durable when exposed to moisture and temperature extremes. Sand from burnt rocks has a particle size modulus from 2.3 to 3.5, bulk density is 1250–1420 kg/m3 , voids are 35–50%, frost resistance of crushed stone fraction is 15 cycles of alternate freezing and thawing. Crusher screenings are a mixture of sand fraction and crushed stone fraction 5–10 mm. The content of crushed stone fractions varies in the range from 10 to 30%. Grade on strength of crushed stone fraction—800.

25.3.4 Materials from Burnt Rocks of Mine Dumps in Structural Layers of Pavements Materials from mine rocks of a certain fractional composition are well compacted and are capable to form a monolith of increased bearing capacity over time. This feature of the rocks can be used in the construction of the subgrade, road foundations and structural layers of pavement. Road construction materials should provide increased durability of pavement structures. Particular requirements apply to the materials used for the construction of roadbed. The material of the base layer must be able to self-strengthen over time in order to provide resistance to the increasing load, since continuously increasing loads act on the bases during operation. Such a structural layer can be created using materials from burnt mine rocks. The specificity of the formation of burned rocks leads to some features of their properties. One of them is the presence of hydraulic activity [10–12]. Due to the presence of active components capable of exhibiting astringent properties, materials of burnt rocks can be, over time, at some moisture, cemented and harden the structure of the material of the structural layer. The dense packing of grains in the material of the carrier layer creates a monolith of increased bearing capacity and stability. This design will be resistant to the effects of loads and alternating change of positive and negative temperatures. Another feature of burned rocks is associated with the macro- and microporous particle structure to be characteristic of heat-insulating materials. From this it follows that the base layer of burnt

25 New Materials for Road Construction

303

rocks will also have heat-insulating properties. These materials can be used to create additional frost protection and thermal insulation layers. For the construction of the underlying layer, crushed stone was used after the first crushing with a grain size from 20 to 150 mm. For the lower and middle layers of the bases, crushed stone fractions from over 40 to 80 mm and from over 80 to 150 mm are used; for the upper layers of bases and coatings—from over 20 to 40 mm and from over 40 to 80 mm. Crushed stone from burnt rocks is well compacted. Therefore, it is most efficient to lay it by the method of optimal mixtures. This crushed stone layer should be carried out with fractions of small crushed stone with successively decreasing sizes: 5–10, 10–20 and 20–40 mm. For laying crushed stone from burnt rocks, we can use a mixture of fractions: 5(3) – 20, 0–20 and 0–10 mm. Fractionated crushed stone and crushed sand can be used in the structural layers of pavement. Figs. 25.4 and 25.5 show the variants of pavement, in the structural layers of which fractionated crushed stone from burnt rocks are used. The experimental sections of technological, access roads, industrial sites and sidewalks were made at the mines Almaznaya, Zamchalovskaya, Vostochnaya (Rostov Region, Russia).

Fig. 25.4 Pavement design of the access roads of enterprises: a 1—fine-grained asphalt concrete, crushed stone fraction up to 15 mm, h = 26 cm; 2—crushed stone fraction 5–10 mm, h = 26 cm; 3—sand, h = 15 cm; b 1—fine-grained asphalt concrete, crushed stone fraction up to 15 mm, h = 5 cm; 2—black crushed stone fraction of 5–10 mm; h = 20 cm; 3—sand, h = 35 cm

1 2 3

3

4 а

1 2

4 b

Fig. 25.5 Design of the road pavement roads improved light-weight type: a 1—surface treatment, crushed stone fraction 5–10 or 10–15 (20) mm; 2—crushed stone fraction 5–40 mm, treated bitumen, h = 8 cm; 3—crushed stone fraction 40–80 (150) mm, h = 20 cm; 4—sand, h = 26 cm; b 1—surface treatment, fraction crushed stone 5–10 or 10–15 (20) mm; 2—crushed stone fraction 5–40 mm, treated bitumen on the road, h = 8 cm; 3—crushed stone fraction 40–80 (150) mm, h = 16 cm; 4—sand, h = 16 cm

304

N. I. Buravchuk et al.

If the crushed stone mixture of the optimal grain composition is used for the construction of pavement layers, then the material is immediately distributed with a layer of the required thickness, leveled with a grader or bulldozer and compacted. The number of passes of the rollers is established empirically. The compacted layer can reach a thickness of 20 cm (in a loose body), but this requires at least 15–18 passes of the heavy roller in one place. With significant porosity of areas of the compacted layer, fines of 5–10 mm in size are scattered on them and additionally compacted with 1–2 passes of a heavy roller. Figure 25.6 shows the transverse profile of pavement using materials from burned rocks. The thickness of the base is 20 cm, which is made of fractioned crushed stone: the bottom layer is from the St. 20–80 mm, the upper—their fractions of St. 5–20 mm with bitumen impregnation. A two-layer asphalt concrete coating is applied to the base: the upper layer is fine-grained and the lower layer is coarse-grained asphalt concrete. The strength and particle size distribution of crushed stone from the base of the road with asphalt concrete pavement did not change during the operation of the road. Fraction of crushed stone of St. 20–80 mm has a brand of strength 800, the fraction from 5 to 20 mm of Mark 1000. Studies on the interaction of burned grains with bitumen show good adhesion. There is practically no exposure of crushed stone, the bitumen film is completely preserved on the surface of the crushed stone. Asphalt mixes for the upper layers of pavement use crushing screenings and crushed stone with grain sizes up to 40 mm. Thus, pavement for roads of category IV and V can be made using materials from burnt rocks of mine dumps. The positive experience in operating experimental sections of roads and sidewalks confirms the feasibility of using non-conventional technogenic raw materials in road construction. High-quality crushed stone from burnt rocks can be used in all structural layers of pavement. 4,50-6,00 0,50

2,25-3,00

0,08

1

0,50 0,75

2,25-3,00

0,02

2

3

4

0,75

0,04

5

Fig. 25.6 Constructive transverse profile of auto-drive-ways with a carriage-way width of 4.5– 6.0 m; pavement design: 1—medium-grained asphalt concrete, h = 4 cm; 2—coarse-grained asphalt concrete, h = 5 cm; 3—burnt rock crushed stone impregnated with bitumen, h = 6.5 cm; 4—base of burnt rock crushed stone, h = 20 cm; 5—sandy underlying layer, h = 10 cm

25 New Materials for Road Construction

305

25.4 Discussion Long-term service of any structure can be provided that the material of the structure meets the conditions of its operation. To ensure reliable resistance of the structure to increasing loads throughout the entire service life, it is necessary that the energy of structural bonds in the material of the structure is constantly increased. This is possible provided that the design has a self-densification system. Materials from mine rocks of a certain fractional composition have the ability over time to cement and reinforce the structure of the embankment massif, to form a monolith of increased bearing capacity and stability. Materials from burnt and burnt mine rocks can create a monolithic self-compacting system without introducing a binder. This ability of the rocks is due to their chemical and mineral composition, structural features, and activity. Burned rocks is the products of spontaneous firing, due to the nature of their formation and thermodynamic state; they have an increased supply of internal energy and corresponding reactivity and can significantly affect the strengthening of the massif. The main active components of burned rocks are metakaolinite, amorphous silica, aluminum oxides, and iron. The presence of these components is due to the specifics of their origin, and is associated with the presence of a number of structural defects that occur during physicochemical processes that occur during high-temperature firing of coal-bearing mine rocks. An important role is played by the nature of the surface of mineral particles, the presence of active surface centers, characterized by an increased energy potential. It is known that the surface of all solid materials contains Lewis acidic and basic branstedite active centers [13–16], which determine its activity. Obviously, for burnt rocks of mine dumps, when evaluating their activity, it is necessary to take into account both the presence of active components that appeared due to their formation and the Lewis and Brønsted type centers (synergistic effect). The presence of these factors has a structuring effect in the formation of an array of subgrade embankments. This new state of matter is the cause of the ability of burned rocks to cement. It is promising to use the potential of burnt mine crushed stone primarily for the construction of road pavement of III-IV road categories in the construction, reconstruction and repair of regional and local roads, and a large network of rural roads. The volumes of such work are large. When using such raw materials, in addition to saving natural mineral raw materials, the cost of transportation costs for delivering raw materials to the place of consumption is reduced, some environmental problems are solved to reduce the negative impact of the waste dump on the environment near its location. A general condition for the use of mine rocks in road construction is the compliance of the strength of the structural layers of pavement constructed from them with the mechanical and physico-mechanical effects that can be expected in this layer. To make a decision on the use of mineral materials from burned rocks, it is necessary to conduct a comprehensive assessment of this technogenic raw material. The methodology for a comprehensive assessment of mine rocks includes three stages: 1. an engineering-geological survey of the rocks of mine dumps to obtain the necessary information about the nature of the occurrence of materials, the distribution

306

N. I. Buravchuk et al.

of moisture, density along the depth of the dump, the degree of homogeneity, the method of producing rocks; 2. an engineering-geological assessment of the indicators of physical and mechanical properties of rocks and materials from them, as determined in the laboratory, and establishment of the possibility and conditions for their use as materials for road construction; 3. taking into account the obtained laboratory data, it is carried out a study of the feasibility to use certain materials from rocks in specific road structures. In the case of a positive decision, special recommendations are developed on the design of the subgrade and road pavement from rocks of a specific mine dump and the features of the technology for their construction. Due to the lower cost of materials from burnt rocks of mine dumps (on 25–30% lower than the cost of natural aggregates), the total cost of road construction works decreases. Acknowledgements This research was carried out within the framework of financing of the Ministry of Education and Science of the Russian Federation for the project No. BCH0110-11/2017-20. Research was financially supported by Southern Federal University, 2020 (Ministry of Science and Higher Education of the Russian Federation) on the project VnGr /2020-04-IM.

References 1. K.I. Trubetskoy, Z.A. Terpogosov, V.G. Shitarev, Mountain J. 3, 44–48 (1994). (In Russian) 2. The use of fly ash, ash and slag mixtures and slag from thermal power plants in road construction, in Proceedings of the Union State, vol. 82 (Moscow, 1975), 184p. (In Russian) 3. E.I. Putilin, B.C. Tsvetkov, The Use of Fly Ash and Ash and Slag Mixtures in the Construction of Roads. Overview of Domestic and Foreign Experience in the Application of Waste from the Combustion of Solid Fuels at Thermal Power Plants (Moscow, 2003), 123p. (In Russian) 4. N.F. Kosenko, V.V. Makarov, Ecology and Industry of Russia vol. 4 (2008), p. 44. (In Russian) 5. G.N. Sivertsev, Processes During Hardening of Fuel Slag and Burnt Rocks. Chemical Processes of hardening of Concrete (Moscow, Gosstroyizdat, 1961), pp. 108–122. (In Russian) 6. G.I. Knigina, Construction Materials from Burnt Rocks (Moscow, Stroyizdat, 1966), 206p. (In Russian) 7. G.I. Knigina, V.F. Zavadsky, Microcalorimetry of Mineral Raw Materials in the Production of Building Materials (Moscow, Stroyizdat, 1987), 144 p. (In Russian) 8. SZh Saybulatov, A.P. Kapustin, L.F. Kalmykova, V.T. Stanevich, News of universities. Constru. Archit. 3, 60–64 (1991). (In Russian) 9. N.I. Buravchuk, O.V. Guryanova, News of higher educational institutions. North-Caucasus Region. Tech. Sci. 1, 111 (2015). (In Russian) 10. L.I. Kataeva, Build. Mater. 7, 23 (1996). (In Russian) 11. N.I. Buravchuk, V.M. Budnitsky, V.F. Brazhnikov, News of universities. North-Caucasus Region. Tech. Sci. 4, 70 (1998). (in Russian) 12. N.I. Buravchuk, O.V. Guryanova, M.A. Jani, E.P. Putri, Advanced Materials—Proceedings of the International Conference on “Physics and Mechanics of New Materials and Their Applications”, PHENMA 2017, in Springer Proceedings in Physics, ed. by A. Ivan, Parinov, ShunHsyung Chang, V.K. Gupta, vol. 207 (Springer Cham, Heidelberg, New York, Dordrecht, London, 2018), pp. 605–619

25 New Materials for Road Construction

307

13. M.M. Sychev, E.N. Kazanskaya, A.A. Petukhov, University news. Chem. Technol. 10, 85–88 (1987). (In Russian) 14. K. Tanab, Solid Acids and Bases (Moscow, Mir. 1973), 183p. (In Russian) 15. A.P. Nechiporenko, Acid-Base Surface Properties Of Solids (Guidelines. Leningrad, LTI, Lensoviet, 1989). 22p. (In Russian) 16. V.V. Yadykina, News of universities. Building 9, 75 (2003). (In Russian)

Part III

Mechanics of Advanced Materials

Chapter 26

Finite Element Modelling of Active Composite Materials in ACELAN-COMPOS Package Andrey Nasedkin

Abstract The paper deals with computer modelling in finite element software ACELAN-COMPOS of multiscale two-phase magnetoelectric (piezomagnetoelectric) bulk composites that consist of piezomagnetic and/or piezoelectric fractions of irregular structures. The proposed technique is based on the models of micro- and nanoscale materials with interface or surface effects, the effective moduli method, the modelling of representative volumes, and the use of finite element technologies for solving the problems in the representative volumes.

26.1 Introduction In this paper, as active materials we will understand the materials in which sufficiently noticeable deformations can be caused by external nonmechanical influences. Such materials are piezoelectric, magnetoelectric, pyroelectric and other materials with coupling between mechanical fields and fields of a different nature: electric, magnetic or thermal. These materials are widely used in modern engineering as active elements of transducers, sensors, actuators and other devices. Recently, new materials with improved characteristics are being intensively developed to improve the efficiency of these devices. Especially important are the problems of developing active composite materials consisting of materials of different phases. Methods of mathematical and computer modelling help us to predict the effective properties of composite materials depending on the characteristics of the initial phases, their percentage ratio and the peculiarities of the internal structure. The problems of determining effective properties, also called homogenization problems, can be solved on the basis of various approaches known in the mechanics of composite materials. For active materials whose behaviour is described by a sufficiently complicated system of differential equations, it is convenient to use the method of effective moduli. For example, for piezoelectric composites according to A. Nasedkin (B) Institute of Mathematics, Mechanics and Computer Science, Southern Federal University, 8a, Milchakova Street, Rostov-on-Don, Russia 344090 e-mail: [email protected] © Springer Nature Switzerland AG 2020 I. A. Parinov et al. (eds.), Advanced Materials, Springer Proceedings in Materials 6, https://doi.org/10.1007/978-3-030-45120-2_26

311

312

A. Nasedkin

this method, it is necessary to solve a set of boundary-value problems of piezoelectricity (electroelasticity) with special boundary conditions providing for homogeneous materials the exact solutions with constant field gradients (strains, stresses, electric field and electrical induction). In a non-uniform representative volume, these gradients, naturally, will not be constant, but their averaged integral characteristics will permit to determine the effective moduli of the composite material [1, 2]. For nanostructured composites, in which inclusions or pores have nanodimensions, the nanoscale effect can be taken into account in the framework of the theory of surface stresses [3–8] and its generalizations to the problems with coupling fields [9–15]. In the theory of surface stresses for the interfaces of materials with different phases, the special equations are written that relate stress jumps in volumes with fields for surface stresses. Finally, in recent years, the technologies have been proposed for creating the new materials composed of piezoelectric matrix and of inclusions from other materials or pores, on which interface boundaries the particles of third type materials are deposited [16, 17]. To solve the homogenization problems for all active composites described in this paper, the specialized software was developed, which is based on the finite element solution of boundary problems in representative volumes and takes into account the main features of the internal structure of composites. Namely, the program systems written in the APDL ANSYS language were created, which allow in the automated mode to solve in the ANSYS package the homogenization problems for active composites of various types and determining their effective moduli. To generate the structures of representative volumes in addition to the simple random ANSYS algorithm, external programs that implement various algorithms were created [1, 2, 18]: 3–x algorithm implemented by S.V. Bobrov, supporting the connectivity of finite elements of the first phase, up to 90% of inclusions of the second phase; 3–0 algorithm with a regular structure of connectivity of the first phase in three axial directions and with a closed structure of the elements of the second phase; cluster algorithms implemented by V. V. Remizov (Witten–Sander method, cluster of the second phase method; method of “growth out of the plane”; method of initial concentration, etc.). However, in the ANSYS package there were no basic means for solving the problems of magnetoelectricity and there were no piezoelectric and magnetoelectric shell finite elements. In this regard, at the Department of Mathematical Modelling of Southern Federal University, a specialized finite element package ACELANCOMPOS was developed. The ACELAN-COMPOS package is focused on solving the homogenization problems with coupled mechanical and electromagnetic fields. In this package, implemented new algorithms 3–3 connectivity [19, 20], supporting the connectivity of the two phases; algorithm 3–0 connectivity, creating the granular structures [21, 22]; and algorithm 1–3 connectivity, creating the structures with rod elements in a matrix [20, 22]. For all these models of representative volumes, the algorithms have been developed for the automated search for finite elements located at the interphase boundaries and placing shell elements on them that simulate the presence of surface effects for nanoscale inclusions or pores. For transversely isotropic materials, an algorithm was additionally implemented for the plate surface

26 Finite Element Modelling of Active Composite Materials …

313

elements, parallel to the coordinate axes, with the material properties that inherit the anisotropy structure of the neighbouring volume elements. The models of magnetoelectricity and the models of representative volume elements of the ACELAN-COMPOS package are briefly presented in this paper. Other means of ACELAN-COMPOS and a more detailed presentation of models, algorithms and results are presented in [19–25].

26.2 Setting of Homogenization Problems The technology of homogenization problem solving implemented in ACELANCOMPOS is applicable for a fairly wide class of composite materials of various stochastic structures with coupling physical and mechanical fields. It is only important that linear stationary equations of divergent type should be considered. For example, let be the representative volume of a piezomagnetoelectric (magnetoelectric) composite body consisting of two materials. We assume that this volume is filled with materials of two types (phases): = (1) ∪ (2) . These phases can have various coupled fields. Thus, the phase (1) can have piezoelectric properties, while the phase (2) can be piezomagnetic. Another case is the active materials with inclusions or pores. Then, the first phase of the main fills up the volume or set of volumes (1) , and the second phase (inclusions or pores) fills the volume or set of volumes (2) . Here, for a porous material, the phase (1) should be connected. For modelling of nanoscale effects in the framework of the Gurtin–Murdoch theory and its generalizations, surface fields are set on the interfaces of the two phases s = ∂(1) ∩ ∂(2) . The external boundary of the representative volume = ∂ will be used to specify the boundary conditions in the homogenization problems. In accordance with the effective moduli method, we will consider in the volume the following boundary value problem of the static theory of magnetoelectroelasticity with respect to the displacement functions u(x), the electric potential ϕ(x) and the magnetic potential φ(x): LT (∇) · T = 0, ∇ · D = 0, ∇ · B = 0, x ∈ ,

(26.1)

T = c · S − eT · E − hT · H, D = e · S + κ · E + α · H, B = h · S + αT · E + μ · H,

(26.2)

S = L(∇) · u, E = −∇ϕ, H = −∇φ,

(26.3)

⎧ ⎫ ⎤ ∂1 0 0 0 ∂3 ∂2 ⎨ ∂1 ⎬ LT (∇) = ⎣ 0 ∂2 0 ∂3 0 ∂1 ⎦, ∇ = ∂2 , ⎩ ⎭ 0 0 ∂ 3 ∂2 ∂1 0 ∂3

(26.4)

⎡

314

A. Nasedkin

LT (n) · [T] = LT (∇ s ) · Ts , n · [D] = ∇ s · Ds , n · [B] = ∇ s · Bs , x ∈ s , (26.5) Ts = cs · S − esT · Es − hsT · Hs , Ds = es · Ss + κs · Es + αs · Hs , Bs = hs · Ss + αsT · Es + μs · Hs ,

(26.6) (26.7)

Ss = L(∇ s ) · (I − n ⊗ n) · u, Es = −∇ s ϕ, Hs = −∇ s φ, ∇ s = ∇ − n(∂/∂ n), (26.8) u = LT (x) · S0 , ϕ = −x · E0 , φ = −x · H0 , x ∈ .

(26.9)

Here T = {σ11 , σ22 , σ33 , σ23 , σ13 , σ12 }, S = {ε11 , ε22 , ε33 , 2ε23 , 2ε13 , 2ε12 } are the arrays of the stress components σi j and the strain components εi j ; D and E are the vectors of the electrical induction or the electric displacement and of the intensity electric field; B and H are the vectors of magnetic induction and of the intensity magnetic field, respectively; c = c E,H is the 6 × 6 matrix of stiffness moduli; e = e H is the 3 × 6 matrix of piezomoduli; h = h E is the 3 × 6 matrix of magnetostriction moduli or piezomagnetic moduli; κ = κ S,H = ε S,H is the 3 × 3 matrix of dielectric permittivity moduli (dielectric constants); α = α S is the 3 × 3 matrix of magnetoelectric coupling coefficients; μ = μ S,E is the 3 × 3 matrix of magnetic permeability moduli; S0 , E0 and H0 are constant six-dimensional array, and three-dimensional vectors, respectively; the superscripts of the moduli indicate for which constant fields they were calculated; (. . .)T is the transpose operation. Interface relations (26.5)–(26.8) on the interphase surface s are used only for modelling of composites at the nano-level. In (26.5)–(26.8), the surface fields and moduli are marked with superscript s; [(. . .)] = (. . .)(1) − (. . .)(2) is the jump of the corresponding quantity across the interphase boundary; n is the unit normal vector to s , external to the domain (1) . If the interface boundary conditions (26.5)–(26.8) are missing, then the problem (26.1)–(26.4), (26.9) is the homogenization problem for piezomagnetoelectric composite with usual phase sizes (inclusions or pores). In the case of a composite of arbitrary anisotropy class to determine the full set eff eff eff eff eff , eiζ , h iζ , κieff of its effective moduli cβζ j , αi j , μi j , it is required to solve the twelve problems (26.1)–(26.9), differing in boundary conditions (26.9), in which only one of the components S0 , E 0k , H0k should be set not equal to zero (γ = 1, 2, . . . , 6; k = 1, 2, 3): • problems I–VI (ζ = 1, 2, . . . , 6) eff eff eff = Tβ /S0 , eiζ = Di /S0 , h iζ = Bi /S0 , S0γ = S0 δ ςγ , E0 = 0, H0 = 0 ⇒ cβζ (26.10)

26 Finite Element Modelling of Active Composite Materials …

315

• problems VII–IX ( j = 1, 2, 3) eff eff S0 = 0, E 0 j = E 0 δ jk , H0 = 0 ⇒ eeff jβ = − Tβ /E 0 , κi j = Di /E 0 , α ji = Bi /E 0 ,

(26.11) • problems VII–IX ( j = 1, 2, 3) eff eff S0 = 0, E0 = 0, H0 j = H0 δ jk ⇒ h eff jβ = − Tβ /H0 , αi j = Di /H0 , μi j = Bi /H0 ,

(26.12) where δi j is the Kronecker symbol; β = 1, 2, . . . , 6; i = 1, 2, 3; ⎞ ⎛ 1 ⎝ s (•) = (•)d + (•) d ⎠. ||

(26.13)

s

As we can see from (26.9)–(26.13), taking into account the interface conditions leads to the necessary of calculation of the averaged field characteristics not only by the volume , but also by the interface boundary s . Since the interface boundaries complicate the internal structure of the representative volume, it is possible to solve boundary-value homogenization problems only numerically, for example, by the finite element method described below.

26.3 Finite Element Approximations In order to solve the problems of magnetoelectroelasticity I–XII for an inhomogeneous composite material in a representative volume , one can proceed to their weak statements and use the classical technique of finite element approximations. (2) Let h be the region occupied by a finite element mesh, h ⊆ , h = (1) h ∪ h , ( j) ( j) ( j) ( j) h ⊆ ( j) , h = ∪k ek , where ek is a separate finite element with the number k and with the material properties of the phase j = 1, 2. Let also hs be a grid of the (2) surface finite elements, conforming with the volume mesh h , hs = ∂ (1) h ∩ ∂ h , s s s h = ∪m em , where em is a separate surface finite element with number m, which ( j) is a common face of the corresponding volume elements ek on the phase interface (hs ≈ s ). We will use Lagrangian or serendipity finite elements with degrees of freedom of nodal displacements, electrical potentials and magnetic potentials. It is important that, due to the structure of the surface fields (26.5)–(26.8), we can use membrane elements with degrees of freedom of nodal displacements, electrical potentials and magnetic potentials (without degrees of freedom of the rotation angles). Then approximate solutions of uh ≈ u, ϕh ≈ ϕ, φh ≈ φ on the finite element mesh h can be searched in the form

316

A. Nasedkin

uh = NuT · U, ϕh = NϕT · , φh = NφT · ,

(26.14)

where NuT is the matrix of basis or form functions for displacements; NϕT , NφT are the row vector of basis functions for electric and magnetic potentials; U, , are the vectors of nodal displacements, electric potentials and magnetic potentials, respectively. In accordance with the classical finite element technique, we approximate the continual weak formulation of the problems I–XII in the finite dimensional spaces associated with the basis functions from (26.14). Substituting (26.14) and similar representations of the projection functions δ uh , δ ϕh , δ φh into weak statements of magnetoelectroelastic problem, we obtain the following finite element system K · a = F,

(26.15)

U Kuu Kub Fu , a= , K= , F= T Kub −Kbb −Fb b T Kuϕ Kϕϕ Kϕφ Fϕ U T , K . = = = , a = , F b ub T T Kϕφ −Kφφ Kuφ Fφ b

Kbb

(26.16)

(26.17)

Vectors Fu , Fϕ , Fφ in (26.16), (26.17) appear when taking into account the essential boundary conditions (26.9), and they are differ for various boundary conditions from (26.10)–(26.12). In (26.15)–(26.17) the matrices contain both usual for the problems of the magnetoelectroelasticity the matrices, calculated on the volumes of finite element mesh, and the additional matrices, calculated on the interface boundaries. For example, the stiffness matrix Kuu has the following structure: ek = Kuu = Kuu + Kuu , Kuu

BTu · c E · Bu d, Kuu =

h

s s BsT u · c · Bu d, hs

(26.18) Bu = L(∇) · NuT , Bsu = L(∇ s ) · (I − n ⊗ n) · NuT .

(26.19)

Taking into account (26.16)–(26.19), we can conlude that the matrix K of the system of linear algebraic (26.15) is symmetric. In addition, by virtue the properties of positive definiteness of the volume and surface energies, the matrix Kuu and Kbb will be at least non-negative definite. Therefore, the symmetric matrix K in (26.15) will have the properties of a quasi-defined matrix, typical for the problems with a saddle point. In this connection, in ACELAN-COMPOS package we use an effective algorithms for symmetric positive definite and quasi-definite matrices for solving the system of linear algebraic (26.15) [26–28]. All basic procedures that we need in finite element manipulations, such as the degree of freedom rotations, mechanical, electric and

26 Finite Element Modelling of Active Composite Materials …

317

magnetic boundary condition settings, etc., we can also provide in a symmetric form.

26.4 Models of Representative Volumes and Some Results In ACELAN-COMPOS package the representative volume element (RVE) is simulated in the form of a cubic array of finite elements, where the elements also have cubic shapes. In accordance with the accepted structure of second phase, we assign the properties of the skeleton material of the first phase to some part of the finite elements, and assign the properties of the second phase to the remaining part of the elements. In ACELAN-COMPOS there are the opportunities to create different types of representative volumes. Examples of representative volumes, created by different algorithms of the ACELAN-COMPOS package, are shown in Figs. 26.1, 26.2, 26.3 and 26.4. In all cases, the percentage of occurrence of the second phase was approximately the same (about 15%), and the order of RVE is the same and equal 16 ×16×16. Everywhere in Figs. 26.1a, 26.2a, 26.3a and 26.4a the whole RVE is shown, in Figs. 26.1b, 26.2b, 26.3b and 26.4b the elements of the first phase are shown, in Figs. 26.1c, 26.2c, 26.3c, and 26.4c the elements of the second phase are shown, and in Figs. 26.1d, 26.2d, 26.3d and 26.4d the surface elements are shown.

Fig. 26.1 Example of RVE of with a random arrangement of the elements of the second phase

Fig. 26.2 Example of RVE with 3–3 connectivity (direct algorithm)

318

A. Nasedkin

Fig. 26.3 Example of RVE with 3–3 connectivity (inverse algorithm)

Fig. 26.4 Example of RVE with 3–0 connectivity

In the first case, the finite elements of second phase are selected by a random number generator (Fig. 26.1). It is obvious that the model created by using a simple random number generator is easy to build. However, such model does not support the connectivity of the elements for the first phase and does not reflect the connectivity structure of the elements for the second phase. Two other algorithms in ACELAN-COMPOS create the structures of the twocomponent materials with the connectivity for both phases (3–3 connectivity) [19, 20, 22]. In the case of porous composites, the 3–3 connectivity algorithms generate materials with open porosity. In these algorithms, the representative volumes consist of domains with 8 × 8 × 8 finite elements. Number 8 for the domain size was chosen for the convenience of implementing numerical procedures to verify the phase connectivity and generate different data structures. In a direct version of the 3–3 algorithm, the process of the domain generation is implemented in such way that the connectivity of the elements of the first phase is maintained through the domain vertices, and the connectivity of the structure of the second phase is maintained through the elements located approximately in the midpoints of the domain edges. In the inverted version of this algorithm, the first phase and the second phase are interchanged. Each domain is created by a partially random way, and the representative volumes of 8n × 8n × 8n order are formed as a result of generating the sequence of n domains along each of three coordinate axes. Thus, generally speaking, each resulting domain differs from the other. Nevertheless, it maintains the connectivity of both phases and

26 Finite Element Modelling of Active Composite Materials …

319

the connectivity of the total volume structure, being formed either by a direct 3–3 algorithm or by an inverse 3–3 algorithm. A detailed description of these algorithms is given in [19, 20]. Some examples of the representative volumes with the porosity p ≈ 15 % for n = 2 (eight domains) are shown in Fig. 26.2 for direct algorithm and in Fig. 26.3 for inverse algorithm, respectively. As can be seen from Fig. 26.2, the direct algorithm distributes a significant amount of the framework elements (elements of the first phase) near the domain edges. On the contrary, the inverse algorithm gathers the most part of the framework elements (elements of the first phase) in the central part of the domain. For a larger number of domains (n = 3, n = 4, etc.), these effects are leveled, since some parts of the domain boundaries become located inside of the representative volume. For simulate the element of second phase as granules, consisting of one or more structural elements not connected with other granules, in ACELAN-COMPOS package the 3–0 algorithm exists [20–22]. In the case of porous composites, the 3–0 connectivity algorithms generate materials with closed porosity. In this algorithm, the representative volumes also consist of domains with 8 × 8 × 8 elements. The input user data are the granule size and the maximum quantum of inclusions. Random choice of the supporting elements for the granules ensures in the result the partially stochastic distribution of the elements of second phase in the RVE. The granule grows in the domain according to an algorithm that allows the granule to be shaped as possible close to the ball, while avoiding highly elongated elements. As in 3–3 algorithms, each domain in 3–0 algorithm is created by a partially random way, and the representative volumes of 8n × 8n × 8n order are formed in the result of generating the sequence of domains along three coordinate axes. Thus, here each resulting domain differs from the other. Nevertheless, it maintains the connectivity of the elements of the main first phase. A detailed description of the 3–0 algorithm is contained in [20, 21]. One example of the RVE for n = 2 (eight domains), constructed by the 3–0 algorithm, is shown in Fig. 26.4. In 1–3 (3–1) algorithm of the ACELAN-COMPOS package, the RVE contains rods placed in the skeleton of the main material. This is a simple algorithm based on placing two-dimensional pattern on the bottom of the volume and extruding it through the body [20, 24]. For nanostructured composites, for all variants of representative volumes, it is possible to automatically find the interphase boundaries s and place on them the shell (membrane) finite elements that simulate the surface effects (Figs. 26.1d, 26.2d, 26.3d and 26.4d). For the shell elements it is necessary to insure the anisotropy type, which corresponds to the anisotropy of the volume finite element. This correspondence was implemented only for transversely isotropic phases and for elements parallel to the O x1 x2 plane (painted in light green in Figs. 26.1d, 26.2d, 26.3d and 26.4d or x3 axis (painted in crimson in Figs. 26.1d, 26.2d, 26.3d and 26.4d. For representative volumes shown in Figs. 26.1, 26.2, 26.3 and 26.4, we will present here as an example the calculation results of solving the homogenization problem for a porous piezoceramic material without taking into account the surface effects (Table 26.1) and taking into account only uncoupled surface stresses according to the methodology presented in [29, 30] (Table 26.2). For RVE of this composite

320

A. Nasedkin

Table 26.1 Effective moduli of porous piezoceramics PZT-5 without surface stresses Relative moduli

SR, p = 14.99

3–3 (direct), p = 14.84

3–3 (inverse), p = 15.21

3–0, p = 15.04

r (c11 )

0.76

0.71

0.69

0.66

r (c12 )

0.72

0.65

0.62

0.61

r (c13 )

0.71

0.64

0.61

0.58

r (c33 )

0.75

0.69

0.68

0.64

r (c44 )

0.81

0.79

0.78

0.77

r (e31 )

0.73

0.66

0.64

0.56

r (e33 )

0.84

0.83

0.83

0.81

r (e15 )

0.80

0.77

0.77

0.74

r (κ11 )

0.85

0.85

0.84

0.84

r (κ33 )

0.84

0.83

0.83

0.83

r (d31 )

0.95

0.92

0.92

0.88

r (d33 )

0.99

0.98

0.99

0.98

r (d15 )

0.98

0.98

0.98

0.96

| s |/||

1.91

1.32

1.13

0.68

Table 26.2 Effective moduli of porous piezoceramics PZT-5 with surface stresses Relative moduli

SR, p = 14.99

3–3 (direct), p = 14.84

3–3 (inverse), p = 15.21

3–0, p = 15.04

r (c11 )

1.09

0.98

0.93

0.77

r (c12 )

0.93

0.85

0.80

0.70

r (c13 )

0.92

0.84

0.79

0.66

r (c33 )

1.09

0.98

0.92

0.75

r (c44 )

1.08

1.00

0.98

0.88

r (e31 )

0.84

0.78

0.74

0.63

r (e33 )

0.84

0.83

0.83

0.81

r (e15 )

0.83

0.80

0.79

0.76

r (κ11 )

0.84

0.83

0.83

0.83

r (κ33 )

0.83

0.82

0.82

0.82

r (d31 )

0.59

0.63

0.66

0.75

r (d33 )

0.60

0.66

0.69

0.83

r (d15 )

0.76

0.80

0.81

0.87

| s |/||

1.91

1.32

1.13

0.68

26 Finite Element Modelling of Active Composite Materials …

321

the domain (1) occupied by the dense piezoceramics and the domain (2) occupied E(i) S(i) (i) , e jβ = e(i) by the pores: cαβ = cαβ jβ , κ j j = ε j j for x ∈ , i = 1, 2. In Tables 26.1 and 26.2 we give the relative values of the effective material moduli eff eff eff /cαβ , r (e jβ ) = eeff r (cαβ ) = cαβ jβ /e jβ , r (κ j j ) = κ j j /κ j j and r (d jβ ) = d jβ /d jβ E(1) S(1) for porous piezoceramics PZT-5. Here cαβ = cαβ , e jβ = e(1) and jβ , κ j j = ε j j (1) −1 d jβ = d jβ are the corresponding values for the dense piezoceramics, d = e · c . For dense piezoceramics PZT-5 we take the following mechanical, dielectric and E(1) E(1) E(1) = 12.1 · 1010 ; c12 = 7.54 · 1010 ; c13 = 7.52 · 1010 ; piezoelectric constants: c11 E(1) (1) (1) (1) 10 E(1) 10 2 c33 = 11.1 · 10 ; c44 = 2.21 · 10 (N/m ); e33 = 15.8; e31 = −5.4; e15 = 12.3 S(1) S(1) 2 −12 (C/m ); ε11 = 916ε0 ; ε33 = 830ε0 ; ε0 = 8.85 · 10 (F/m). For the pores, we E(2) E(1) set negligibly small elastic moduli cαβ = η cαβ , η = 1 · 10−10 , piezomoduli (2) S(2) e jβ = η (x1 C/m2 ) and ε j j = ε0 . For the case of nanoporous piezoceramics with uncoupled surface stresses we accept the size of cube finite element a = 1 · 10−10 E(1) s s (m), cαβ = a cαβ , e jβ = 0, κ sj j = 0. It can be noted that even with the same porosity for the simple random (SR) algorithm, the area of interface boundaries | s | is larger than for the 3–3 connectivity direct algorithms, the area of interface boundaries for the 3–3 direct algorithms is larger than for the 3–3 inverse algorithms, and the area of interface boundaries for the 3–3 inverse algorithms is larger than for the 3–0 algorithms. So, as we can conclude from Tables 26.1 and 26.2, for the representative volumes with SR distribution of inclusions and with 3–3 or 3–0 connectivity for various interphase areas we obtain different values of the effective moduli, moreover the SR model is slightly stiffer and more electromechanical active than the 3–3 models, and the 3–3 connectivity models are stiffer and more electromechanical active than the 3–1 model. Accounting for surface stresses here is equivalent to the placement of elastic membrane elements on the interface boundaries. Therefore, when taking into account surface stresses, the size of the interface area has a very significant effect on the effective stiffness moduli (Table 26.2). Thus, we can conclude that the internal structures of nanoporous composites can have a significant effect on the effective stiffness moduli values. Meanwhile, from a comparison of Tables 26.1 and 26.2, we can infer that the uncoupled surface stresses have much less effect on the effective piezomoduli eeff jβ and almost do not influence on the dielectric permittivities κ eff . jj Note that using the described approaches in [1, 2, 19, 21, 22, 29] the of homogenization problems were solved for different structures of representative volumes. Anisotropic elastic and piezoelectric composites were investigated, both on ordinary scale levels and on nanoscale. It was found that the types of connectivity and the internal structure of a composite can have a significant influence on effective moduli (see also Tables 26.1 and 26.2), and taking into account surface or interface effects can even lead to a change in the decreasing properties of moduli on their growth and even lead to superiority of effective moduli compared to moduli of initial phases (Table 26.2). An analysis of the advantages and disadvantages of various algorithms for the formation of representative volumes is given in [20]. Additionally, it can be noted that

322

A. Nasedkin

the piezoceramic finite elements of all types of representative volume structures can be automatically equipped with their elemental coordinate systems rotated relative to the initial Cartesian coordinate system in accordance with the direction of the non-uniform polarization fields [1, 2, 23, 31], and for 3—0 connectivity models the algorithms for the account of electrode surfaces for metallized interfaces have been developed [30, 31]. Acknowledgements The author is grateful for the support of the Ministry of Science and Higher Education of the Russian Federation, project No. 9.1001.2017/4.6.

References 1. A.V. Nasedkin, M.S. Shevtsova, in Ferroelectrics and Superconductors: Properties and Applications, ed. by I.A. Parinov (Nova Science Publication, NY, 2011), p. 231 2. A.V. Nasedkin, M.S. Shevtsova, in Physics and Mechanics of New Materials and Their Applications, ed. by I.A. Parinov, S.-H. Chang, (Nova Science Publication, NY, 2013), p. 185 3. V.A. Eremeyev, Acta Mech. 227, 29 (2016) 4. M.E. Gurtin, A.I. Murdoch, Arch. Ration. Mech. Anal. 57, 291 (1975) 5. M.E. Gurtin, A.I. Murdoch, Int. J. Solid. Struct. 14, 431 (1978) 6. J.C. Hamilton, W.G. Wolfer, Surf. Sci. 603, 1284 (2009) 7. J. Wang, Z. Huang, H. Duan, S. Yu, X. Feng, G. Wang, W. Zhang, T. Wang, Acta Mech. Solida Sin. 24(1), 52 (2011) 8. K.F. Wang, B.L. Wang, T. Kitamura, Acta. Mech. Sin. 32(1), 83 (2016) 9. T. Chen, Acta Mech. 196, 205 (2008) 10. S.-T. Gu, Q.-C. He, J. Mech. Phys. Solids 59, 1413 (2011) 11. S.-T. Gu, J.-T. Liu, Q.-C. He, Comput. Mat. Sci. 94, 182 (2014) 12. S.-T. Gu, L. Qin, Int. J. Eng. Sci. 78, 89 (2014) 13. G.Y. Huang, S.W. Yu, Phys. Status Solidi B 243(4), R22 (2006) 14. X.H. Pan, S.W. Yu, X.Q. Feng, Sci. China Phys. Mech. Astron. 54(4), 564 (2011) 15. Z. Yan, L. Jiang, Nanomaterials 7, 27 (2017) 16. A.N. Rybyanets, A.A. Naumenko, J. Modern Physics. 4(8), 1041 (2013) 17. A.N. Rybyanets, I.A. Shvetsov, M.A. Lugovaya, E.I. Petrova, N.A. Shvetsova, J. Nano Electron. Phys. 10, 02005 (2018) 18. A.V. Nasedkin, A.A. Nasedkina, V.V. Remizov, Comput. Continuum Mech. 7(1), 100 (2014) 19. A.B. Kudimova, D.K. Nadolin, A.V. Nasedkin, A.A. Nasedkina, P.A. Oganesyan, A.N. Soloviev, Mater. Phys. Mech. 37, 16 (2018) 20. N.V. Kurbatova, D.K. Nadolin, A.V. Nasedkin, P.A. Oganesyan, A.S. Skaliukh, A.N. Soloviev, in Analysis and Modelling of Advanced Structures and Smart Systems, Ser. Advanced Structured Materials, ed. by H. Altenbach, E. Carrera, G. Kulikov, vol. 81 (Springer, 2018), p. 69 21. A.B. Kudimova, D.K. Nadolin, A.V. Nasedkin, P.A. Oganesyan, A.N. Soloviev, Mater. Phys. Mech. 37, 25 (2018) 22. N.V. Kurbatova, D.K. Nadolin, A.V. Nasedkin, A.A. Nasedkina, P.A. Oganesyan, A.S. Skaliukh, A.N. Soloviev, in Wave Dynamics and Composite Mechanics for Microstructured Materials and Metamaterials, Series Advanced Structured Materials, ed. by M.A. Sumbatyan. vol. 59 (Springer, 2017), p. 133 23. T.E. Gerasimenko, N.V. Kurbatova, D.K. Nadolin, A.V. Nasedkin, A.A. Nasedkina, P.A. Oganesyan, A.S. Skaliukh, A.N. Soloviev, in Wave Dynamics and Composite Mechanics for Microstructured Materials and Metamaterials, Ser. Advanced Structured Materials, ed. by M.A. Sumbatyan. vol. 59 (Springer, 2017), p. 113

26 Finite Element Modelling of Active Composite Materials …

323

24. A.B. Kudimova, I.V. Mikhayluts, D.K. Nadolin, A.V. Nasedkin, A.A. Nasedkina, P.A. Oganesyan, A.N. Soloviev, Procedia Struct. Integrity 6, 301 (2017) 25. A.V. Nasedkin, in VIII ECCOMAS Thematic Conference on Smart Structures and Materials, VI International Conference on Smart Materials and Nanotechnology in Engineering (CIMNE)— SMART 2017, 5–8 June 2017, Madrid, Spain, ed. by A. Guemes, A. Benjeddou, J. Rodellar, J. Leng, (2017), p. 1137 26. M. Benzi, G.H. Golub, J. Liesen, Acta Numer. 14, 1 (2005) 27. M. Benzi, A.J. Wathen, in Model Order Reduction: Theory, Research Aspects and Applications. Mathematics in Industry, ed. by W.H.A. Schilders, H.A. van der Vorst, J. Rommes, vol. 13 (2008), p. 195 28. R.J. Vanderbei, SIAM J. Optim. 5, 100 (1995) 29. G. Iovane, A.V. Nasedkin, in Dynamical Processes in Generalized Continua and Structures, Ser. Advanced Structured Materials, ed. by H. Altenbach, A. Belyaev, V. Eremeyev, A. Krivtsov, A. Porubov, vol. 103 (Springer, 2019), p. 293 30. A. Nasedkin, A. Nasedkina, A. Rybyanets, Ferroelectrics 508, 100 (2017) 31. A.V. Nasedkin, A.A. Nasedkina, A.N. Rybyanets, Mater. Phys. Mech. 40, 12 (2018)

Chapter 27

Finite Element Investigation of Effective Moduli of Transversely Isotropic Thermoelastic Materials with Nanoscale Porosity Andrey Nasedkin, Anna Nasedkina, and Amirtham Rajagopal Abstract Using the methods of effective moduli and finite elements, the effective properties of nanoporous thermoelastic transversely isotropic materials were studied for simple random and for closed structures of porosity. Nanoscale effects were modelled in the framework of the Gurtin-Murdoch model of interface stresses and of the high conductivity model. The modelling and solution of homogenization problems was performed in the ANSYS package, while structures of representative volumes with closed porosity were created in the ACELAN-COMPOS package. The effect of porosity, types of representative volumes and pore sizes on the values of the effective modules of nanoporous titanium is analysed.

27.1 Introduction In recent years, there has been increased an interest for the theoretical problems of nanomechanics. Numerous investigations have revealed a size effect, which consists in changing the effective material moduli for nanoscale bodies in comparison with the corresponding values for macrodimension bodies. Various theories have been proposed to explain the scale factor. One such theory is the widely used model of surface elasticity. There are several reviews devoted to research on the theories of surface elasticity, their generalizations and applications [1–4]. In turn, among these theories, the most famous is the Gurtin-Murdoch model [5–7]. It can be shown that the use of this model is reduced to the fact that the external boundaries of the nanoscale body are covered with elastic membranes, in which the internal tensions are caused A. Nasedkin (B) · A. Nasedkina Institute of Mathematics, Mechanics and Computer Science, Southern Federal University, 8a, Milchakova Street, Rostov-on-Don, Russia 344090 e-mail: [email protected] A. Nasedkina e-mail: [email protected] A. Rajagopal Department of Civil Engineering, Indian Institute of Technology, Hyderabad 502205, India e-mail: [email protected] © Springer Nature Switzerland AG 2020 I. A. Parinov et al. (eds.), Advanced Materials, Springer Proceedings in Materials 6, https://doi.org/10.1007/978-3-030-45120-2_27

325

326

A. Nasedkin et al.

by surface stresses. Elastic membranes can be placed on the interphase boundaries inside the body with inclusions or pores, which also allows modeling imperfect interfaces with stress jumps and interface surface effects for nanoinclusions or for nanopores [8–11]. For thermal problems the high conductivity model with surface thermal fluxes on the external boundaries or in the interphase surfaces is similar to the GurtinMurdoch model for elastic problems. The effective thermal conductivity coefficients for composite materials with imperfect boundaries and with micro- or nanoscale effects were determined in [12–19]. The Gurtin-Murdoch theory can be extended to thermoelastic problems for nanosized bodies and nanostructured composites. Thus, in [20–23] using this model the effective moduli of thermoelastic composites with spherical nanopores or nanoinclusions and the effective moduli of nanofibers have been studied. The finite element method was applied for thermoelastic materials with surface stresses or with interphase boundary conditions in [24–30]. In this chapter, we study the effective material properties of thermoelastic nanoporous materials of hexagonal syngony class or transversely isotropic materials with random and close structures of porosity. We considered porous material as extreme case of a two-phase bulk composite, when the stiffness moduli of inclusions have negligibly small. The nano-dimensionality of the pore boundaries was taken into account using the highly conducting model and the Gurtin-Murdoch model of surface stresses. This work is a continuation of the author’s researches [27–30]. Here, the scale factor is associated with pore sizes and the influence of the structure of porosity on the effective moduli is analysed. Finite element packages ANSYS and ACELAN-COMPOS were used to simulate representative volumes and to calculate the effective material properties. This approach is based on the theory of effective moduli of composite mechanics, modelling of representative volumes and the finite element method. In accordance with the effective moduli method we solve in the constructed volume the static thermoelastic and thermal problems with linear essential boundary conditions. Homogenization problems are solved numerically by the finite element method. We used the regular cubic representative volumes with hexahedral thermoelastic finite elements and random and granular distributions of pores. To take into account the nanosized internal structure, the contact boundaries between material and pores were covered by the surface membrane thermoelastic elements. We also specified transversely isotropic material properties for the membrane elements, in accordance with the location of the element coordinate systems and the anisotropy type of the volume elements in these coordinate systems. Next, we calculate the averaged stresses and thermal fluxes, which determine the effective thermoelastic moduli. As an example, the models of nanoporous material have been examined with different values of surface moduli, porosity and number of pores. The calculation results allowed us to analyze the dependence of the effective moduli on porosity and surface elements.

27 Finite Element Investigation of Effective Moduli …

327

27.2 Homogenization Problems Let is a representative volume of thermoelastic material with nanodimensional porosity; = (1) ∪ (2) ; (1) is the region occupied by the materials of the first phase (main material or matrix); (2) is the aggregate of the regions occupied by the materials of the second phase (pores); = ∂ is the external boundary of the representative volume ; i is the set of frontier surfaces of regions with different phases ( i = ∂(1) ∩∂(2) ); n = {n 1 , n 2 , n 3 } is the external unit normal vector to the boundary, outward with respect to (1) ; x = {x1 , x2 , x3 } is the vector of Cartesian coordinates. We assume that the parts (1) and (2) are filled with two different transversely isotropic thermoelastic materials. Then in the framework of linear static theory of thermoelasticity for x ∈ we assume the following system of equations: T (∇) · T = 0, T = c · S − bθ, S = (∇) · u,

(27.1)

∇ T · q = 0, q = −k · G, G = ∇θ,

(27.2)

⎧ ⎫ ⎧ ⎫ ⎪ ⎪ ∂1 0 0 0 ∂3 ∂2 ⎬ ⎬ ⎨ ∂1 ⎪ ⎨ u1 ⎪ ⎥ ⎢ T (∇) = ⎣ 0 ∂2 0 ∂3 0 ∂1 ⎦, ∇ = ∂2 , u = u 2 , ⎪ ⎪ ⎭ ⎭ ⎩∂ ⎪ ⎩u ⎪ 0 0 ∂3 ∂2 ∂1 0 3 3 ⎤ ⎡ k11 0 0 ⎥ ⎢ k = ⎣ 0 k11 0 ⎦, 0 0 k33 ⎡

⎡

c11 ⎢c ⎢ 12 ⎢ ⎢c c = ⎢ 13 ⎢ 0 ⎢ ⎣ 0 0

c12 c11 c13 0 0 0

c13 c13 c33 0 0 0

0 0 0 c44 0 0

0 0 0 0 c44 0

⎤

(27.3)

⎧ ⎧ ⎧ ⎫ ⎫ ⎫ ⎤ ⎪ ⎪ ⎪ ε11 ⎪ β11 ⎪ σ11 ⎪ 0 ⎪ ⎪ ⎪ ⎪ ⎪ ⎪ ⎪ ⎪ ⎪ ⎪ ⎪ ⎪ ⎪ ⎪ ⎪ ⎪ ⎪ ⎪ ⎪ ⎪ ⎪ ⎪ ⎪ ⎪ 0 ⎥ σ ε β 22 22 11 ⎪ ⎪ ⎪ ⎪ ⎪ ⎥ ⎪ ⎪ ⎪ ⎪ ⎪ ⎪ ⎪ ⎨ ⎨ ⎨ ⎬ ⎬ ⎥ ⎬ 0 ⎥ σ33 ε33 β33 , S= , b= , ⎥, T = ⎪ ⎪ ⎪ 0 ⎥ σ23 ⎪ 2ε23 ⎪ 0 ⎪ ⎪ ⎪ ⎪ ⎪ ⎪ ⎪ ⎪ ⎪ ⎪ ⎥ ⎪ ⎪ ⎪ ⎪ ⎪ ⎪ ⎪ ⎪ ⎪ ⎪ ⎪ ⎪ 0 ⎦ σ13 ⎪ 2ε13 ⎪ 0 ⎪ ⎪ ⎪ ⎪ ⎪ ⎪ ⎪ ⎪ ⎪ ⎪ ⎪ ⎪ ⎪ ⎩ ⎩ ⎩ ⎭ ⎭ ⎭ σ12 2ε12 c66 0 (27.4)

where σi j , εi j are the components of the stress tensor and the strain tensor, respectively; u i are the components of the displacement vector u; θ is the temperature increment from natural state; q is the heat flux vector; G is the temperature gradient vector; c is the 6 × 6 matrix of elastic stiffness moduli ci j ; b is the six-dimensional array of the thermal stress coefficients βi j ; k is the 3 × 3 matrix of thermal conductivities ki j ; c = c(m) , b = b(m) , k = k(m) for x ∈ (m) , m = 1, 2, and c, b, k have the structures characteristic transversely isotropic materials, c66 = (c11 − c12 )/2; (. . .)T is the transpose operation; (. . .) · (. . .) is the scalar product operation. According to Gurtin-Murdoch model of surface stresses, we suppose that on the nanosized boundaries s the following interphase condition is held: T (n) · [T] = T (∇ s ) · Ts , x ∈ s ,

(27.5)

328

A. Nasedkin et al.

where [T] = T(1) − T(2) is the stress jump over the interface between two phases; s s s s s s , σ22 , σ33 , σ23 , σ13 , σ12 } ∇ s = ∇ − n(∂/∂n) is the surface nabla-operator; Ts = {σ11 s is the array of the interface stresses σi j . We assume that the surface stresses σis j are related to the surface strains εis j and the temperature θ by the formulas Ts = cs · Ss − bs θ, Ss = (∇ s ) · us , us = A · u, A = I − n ⊗ n,

(27.6)

where cs is the 6 × 6 matrix of surface elastic stiffness moduli cisj ; bs is the sixdimensional array of the thermal stress coefficients βis j for the interface; Ss = s s s s s s , ε22 , ε33 , 2ε23 , 2ε13 , 2ε12 } is the array of the interface strains εis j . {ε11 Analogically, we accept the equation of highly thermal conducting interface on the nanosized boundaries s nT · [q] = ∇ s T · qs , qs = −ks · Gs , Gs = ∇ s θ, x ∈ s ,

(27.7)

where qs is the surface heat flux vector; Gs is the surface temperature gradient vector; ks is the 3 × 3 matrix of surface thermal conductivity. Note that the structure of the matrices cs , ks and the structure of the array bs , as well as the values of their coefficients depend on the shape and orientation of the interface boundary s . Since there is so little data for surface moduli, and they are quite contradictory, we will assume on the plane interface faces parallel to the coordinate axes the following structure of surface moduli. We assume that for a composite with two transversally isotropic phases, the following surface moduli are available ⎡

s c˜11 ⎢ c˜s ⎢ 12 ⎢ s ⎢ c˜ s c˜ = ⎢ 13 ⎢ 0 ⎢ ⎣ 0 0

s c˜12 s c˜11 s c˜13 0 0 0

s c˜13 s c˜13 s c˜33 0 0 0

0 0 0 s c˜44 0 0

0 0 0 0 s c˜44 0

⎧ ⎫ ⎤ s ⎪ ⎪ β˜11 0 ⎪ ⎪ ⎪ ⎪ ⎪ s ⎪ ⎪ ⎪ ⎤ ⎡ s β˜11 0 ⎥ ⎪ ⎥ ⎪ ⎪ k˜11 0 0 ⎨ ˜s ⎪ ⎥ ⎬ β33 0 ⎥ ˜s s , k˜ s = ⎣ 0 k˜11 0 ⎦, ⎥, b = ⎪ 0 ⎪ 0 ⎥ ⎪ ⎪ s ˜ ⎥ ⎪ ⎪ 0 0 k ⎪ ⎪ 33 ⎪ ⎪ 0 ⎦ 0 ⎪ ⎪ ⎪ ⎪ ⎩ ⎭ s c˜66 0

(27.8)

s s s where c˜66 = (c˜11 − c˜12 )/2. Then, on flat interface faces, parallel to the plane O x1 x2 , we have in (27.5)– (27.7) n = {0, 0, 1}, ∇ s = {∂/∂ x1 , ∂/∂ x2 , 0}, us = {u 1 , u 2 , 0}, Ts = s s s s s s , σ22 , 0, 0, 0, σ12 }, Ss = {ε11 , ε22 , 0, 0, 0, 2ε12 }, qs = {q1s , q2s , 0}, Gs = {σ11 s s s s(12) s s(12) s s(12) ,b =b ,k =k , where {G 1 , G 2 , 0}, c = c

27 Finite Element Investigation of Effective Moduli …

⎡

cs(12)

s c˜11 ⎢ c˜s ⎢ 12 ⎢ ⎢ 0 =⎢ ⎢ 0 ⎢ ⎣ 0 0

s c˜12 s c˜11 0 0 0 0

0 0 s c˜33 0 0 0

0 0 0 s c˜44 0 0

0 0 0 0 s c˜44 0

⎧ ⎫ ⎤ ⎪ β˜ s11 ⎪ 0 ⎪ ⎪ ⎪ ⎪ ⎪ ⎪ ⎪ β˜ s11 ⎪ 0 ⎥ ⎪ ⎥ ⎪ ⎪ ⎪ ⎨ ⎥ ⎬ 0 ⎥ s(12) 0 , ks(12) = k˜ s . = ⎥, b ⎪ 0 ⎪ 0 ⎥ ⎪ ⎪ ⎥ ⎪ ⎪ ⎪ ⎪ ⎪ 0 ⎦ 0 ⎪ ⎪ ⎪ ⎪ ⎪ ⎩ ⎭ s c˜66 0

329

(27.9)

Meanwhile, on flat interface faces, parallel to the plane O x1 x3 , in (27.5)– (27.7) we have n = {0, 1, 0}, ∇ s = {∂/∂ x1 , 0, ∂/∂ x3 }, us = {u 1 , 0, u 3 }, s s s s s s , 0, σ33 , σ13 , 0, 0}, Ss = {ε11 , 0, ε33 , 2ε13 , 0, 0}, qs = {q1s , 0, q3s }, Gs = Ts = {σ11 s s s s(13) s s(13) s s(13) ,b =b ,k =k , where {G 1 , 0, G 3 }, c = c ⎡

cs(13)

s c˜11 ⎢ 0 ⎢ ⎢ s ⎢ c˜ = ⎢ 13 ⎢ 0 ⎢ ⎣ 0 0

0 s c˜11 0 0 0 0

s c˜13 0 s c˜33 0 0 0

0 0 0 s c˜44 0 0

0 0 0 0 s c˜44 0

⎧ ⎫ ⎤ s ⎪ ⎪ β˜11 0 ⎪ ⎪ ⎪ ⎪ ⎪ ⎪ ⎪ ⎪ 0 ⎥ 0 ⎪ ⎥ ⎪ ⎪ ⎨ ˜s ⎪ ⎥ ⎬ 0 ⎥ s(13) β33 , ks(13) = k˜ s . = ⎥, b ⎪ ⎪ 0 ⎥ 0 ⎪ ⎪ ⎥ ⎪ ⎪ ⎪ ⎪ ⎪ 0 ⎦ 0 ⎪ ⎪ ⎪ ⎪ ⎪ ⎩ ⎭ s c˜66 0

(27.10)

Finally, on flat interface faces, parallel to the plane O x2 x3 , in (27.5)–(27.7) we have n = {1, 0, 0}, ∇ s = {0, ∂/∂ x2 , ∂/∂ x3 }, us = {0, u 2 , u 3 }, Ts = s s s s s s , σ33 , 0, σ23 , 0}, Ss = {0, ε22 , ε33 , 0, 2ε23 , 0}, qs = {0, q2s , q3s }, Gs = {0, σ22 s s s s(23) s s(23) s s(23) ,b =b ,k =k , where {0, G 2 , G 3 }, c = c ⎡

cs(23)

s c˜11 ⎢ 0 ⎢ ⎢ ⎢ 0 =⎢ ⎢ 0 ⎢ ⎣ 0 0

0 s c˜11 s c˜13 0 0 0

0 s c˜13 s c˜33 0 0 0

0 0 0 s c˜44 0 0

0 0 0 0 s c˜44 0

⎧ ⎫ ⎤ ⎪ 0 ⎪ 0 ⎪ ⎪ ⎪ ⎪ ⎪ ˜ s11 ⎪ ⎪ ⎪ β 0 ⎥ ⎪ ⎥ ⎪ ⎪ ⎨ ˜s ⎪ ⎥ ⎬ β 33 0 ⎥ s(23) , ks(23) = k˜ s . = ⎥, b ⎪ 0 ⎥ 0 ⎪ ⎪ ⎪ ⎥ ⎪ ⎪ ⎪ ⎪ ⎪ 0 ⎦ 0 ⎪ ⎪ ⎪ ⎪ ⎪ ⎩ ⎭ s c˜66 0

(27.11)

As we can see, a two-phase composite consisting of two thermoelastic transversely isotropic phases with interface boundaries is characterized by 27 material moduli, for (m) (m) (m) (m) (m) (m) (m) (m) (m) s s s s , c12 , c13 , c33 , c44 , β11 , β33 , k11 , k33 , m = 1, 2, c˜11 , c˜12 , c˜13 , c˜33 , example, c11 s s s ˜ s s ˜ c˜44 , β11 , β33 , k11 , and k33 . If the representative volume does not have a pronounced anisotropy in the distribution of its components, then an homogeneous “equivalent” material will also be transversely isotropic and will be described by nine independent eff eff eff eff eff eff eff eff eff , c12 , c13 , c33 , c44 , β11 , β33 , k11 and k33 . moduli, for example, c11 Note, that the (27.2), (27.7) are satisfied identically, if θ = θ0 = const for x ∈ , because for constant thermal field G = 0, Gs = 0, q = 0, qs = 0. Then, the thermal problem (27.2), (27.7) is not used for solving the mechanical problem with thermal stresses (27.1), (27.5), (27.6), if the temperature field is constant. Therefore, as we

330

A. Nasedkin et al.

eff eff eff eff eff eff eff will see, the effective moduli c11 , c12 , c13 , c33 , c44 , β11 , β33 and the effective moduli eff eff k11 , k33 can be found from separate problems. eff and β eff For determination the effective moduli cαβ j j , it is enough to solve the problems (27.1), (27.5), (27.6) in the representative volume with the following boundary condition

u = LT (x) · S0 , θ = θ0 , x ∈ ,

(27.12)

where S0 is constant six-dimensional array and θ0 = const. In the case of transversely isotropic composite to determine the effective thermoeff eff eff eff eff eff eff , c12 , c13 , c33 , c44 , β11 , β33 , it is required to solve the four probmechanical moduli c11 lems (27.1), (27.5), (27.6), (27.12), differing in boundary conditions (27.12), in which only one of the components S0γ , θ0 should be set not equal to zero (γ = 1, 2, . . . , 6): (i) problem I eff eff eff = σ11 /S0 , c12 = σ22 /S0 , c13 = σ33 /S0 , S0γ = S0 δ1γ , θ0 = 0 ⇒ c11 (27.13)

(ii) problem II eff eff = σ11 /S0 ≈ σ22 /S0 , c33 = σ33 /S0 , S0γ = S0 δ3γ , θ0 = 0 ⇒ c13 (27.14)

(iii) problem III eff = σ23 /(2S0 ), S0γ = S0 δ 4γ , θ0 = 0 ⇒ c44

(27.15)

(iv) problem IV eff eff = σ11 /θ0 ≈ σ22 /θ0 , β33 = σ33 /θ0 , S0 = 0, θ0 = 0 ⇒ β11

(27.16)

where δi j is the Kronecker symbol; ⎞ ⎛ 1 ⎝ s (. . .) = (. . .)d + (. . .) d ⎠. ||

(27.17)

s

eff eff , k33 it is sufficient to Next, in order to determine the effective coefficients k11 consider thermal conductivity (27.2) and interface relation (27.7) of highly thermal conducting. For setting the corresponding homogenisation problem, we adopt the boundary conditions in the following form (G0 = const)

θ = x · G0 , x ∈ .

(27.18)

27 Finite Element Investigation of Effective Moduli …

331

Here for the case of transversely isotropic composite to determine the effective eff eff , k33 we can solve the two problems (27.2), coefficients of thermal conductivities k11 (27.7), (27.18) with different boundary conditions (27.18) (l = 1, 2, 3): (v) problem V eff = −q1 /G 0 , G 0l = G 0 δ1l ⇒ k11

(27.19)

eff = −q3 /G 0 . G 0l = G 0 δ3l ⇒ k33

(27.20)

(vi) problem VI

In conclusion of this section we can mark that taking into account the surface effects for nanostructured composites leads to the appearance of boundary conditions (27.5)–(27.7) on the interface s and to the necessity of calculating by (27.17) the averaged stresses in (27.13)–(27.16) and heat fluxes in (27.19), (27.20) not only by the volume , but also by the interface s .

27.3 Finite Element Approaches and Models of Representative Volumes In order to solve the homogenization problems, we use the finite element approaches described in [27, 28]. These approaches include the simulation of the structure of a representative volume element (RVE) in the form of an array of finite elements and the finite element solution of elastic boundary problem with thermal stresses (27.1), (27.5), (27.6), (27.12) or thermal boundary problems (27.2), (27.7), (27.18). We create a representative volume in the form of a cubic array of finite elements, where the elements also have cubic shapes. In accordance with the accepted porosity structure, we assign the properties of the skeleton material to some part of the finite elements, and assign the properties of the pores to the remaining part of the elements. We compare two types of representative volumes. In the first case, the finite elements with properties of pores are selected by a random number generator. It is obvious that the model created by using a simple random number generator is easy to build. However, such model does not support the connectivity of the elements for the first phase and does not reflect the connectivity structure of the elements for the second phase (closed or open pores). We also use the 3–0 algorithm from ACELAN–COMPOS package for simulation of pores as granules, consisting of one or more structural elements not connected with other granules [31–33]. In this algorithm, the representative volumes consist of domains with 8 × 8 × 8 elements. Number 8 for the domain division was chosen for the convenience of implementing numerical procedures to generate data structures and verify the phase connectivity. The input user data are the size of RVE, the granule size and the maximum percentage of pores or inclusions in the representative volume.

332

A. Nasedkin et al.

Each domain is created by a partially random way, and the representative volumes of 8n × 8n × 8n order are formed in the result of generating the sequence of n domains along three coordinate axes. Thus, each resulting domain differs from the other. Nevertheless, it maintains the connectivity of the main phase in each domain and the connectivity of the total volume structure. A detailed description of the 3–0 connectivity algorithm from ACELAN–COMPOS package is contained in [32, 33]. At the next step, the generated structures were transferred to ANSYS finite element package, where all further operations were carried out. Then, the problems (27.1), (27.5), (27.6), (27.12) or (27.2), (27.7), (27.18) were solved for the representative volume using finite element technology and ANSYS package. In the end, in the ANSYS postprocessor the average stresses and thermal fluxes were automatically calculated by (27.17) according to (27.13)–(27.16), or (27.19), (27.20), and thus the full sets of the effective material moduli of thermoelastic composite were obtained. It is important to note, that we generate the representative volume in a dimensionless form, with the edge of a separate finite element taken equal to dimensionless 1. Thus, the dimensionless spatial parameter will be equal to the minimum pore size l0 . In order to model the surface effects in ANSYS for the elastic shell finite elements, we will specify only membrane stress options and a fictitious thickness h m . We take the stiffness moduli cmαβ proportional to the stiffness moduli of the main material: (1) , where k s is the dimensionless factor. For surface stiffness moduli cmαβ = k s cαβ (1) s s from (27.8) we assume that c˜αβ = lc cαβ , lc = 10−10 (m), and hence, cmαβ = c˜αβ (1) s = (k s /lc )c˜αβ . The dimensional analysis shows that l0 = lc /k s , and therefore k s cαβ s the coefficient k is inversely proportional to the minimum pore size l0 . Further, the dimensionless thickness of the shell elements was fixed h m = 1, and in the computational experiments we varied the coefficient k s and the porosity p. Similarly, we modeled the surface thermomechanical properties β˜ sj j and the surface thermal conductivity moduli k˜ sj j in the suitable shell elements. For solving the thermoelastic problems (27.1), (27.5), (27.6), (27.12) with (27.13)–(27.16) we used a coupled twenty-node finite element SOLID226 with the displacements and the temperature as degrees of freedom in each node and with capability of thermoelastic analysis with thermal stresses. For automatic coating of the inner boundaries of the pores in a cubic representative volume, the following algorithm has been used. First, the finite elements with the pore material properties are selected. Then the external boundaries of the obtained array of elements are covered by target contact elements TARGE170 using the command TSHAP, QUA8. Hence, the edges of all finite elements with the pore properties lying on the external surfaces of the set of these elements get covered by eight node contact elements (TARGE170 of the shape QUA8). Then the contact elements, located on the external border of the whole representative volume, are deleted and the remaining finite elements are changed to the eight node shell elements SHELL281 with the membrane stress only option. Further, it was necessary to provide an anisotropy type for the shell elements SHELL281 which would be conformable with the anisotropy of the volume finite

27 Finite Element Investigation of Effective Moduli …

333

elements SOLID226 and the structures of surface moduli (27.9)–(27.11). For a hexagonal system of anisotropy, supplementary procedure was implemented for the shell elements SHELL281 located perpendicular to the isotropy plane O x1 x2 by interchanging the stiffness moduli in rows and columns corresponding to the axes x3 and x2 . As a result, all contact boundaries where thermoelastic structural elements are in contact with pores have been coated by the membrane finite elements which simulate the effect of surface stresses. Some examples of the representative volume element for n = 2 (eight domains) are shown in Figs. 27.1 and 27.2, respectively. In these figures, percentage of pores p = 15% is the same. Figure 27.1 shows an example of the representative volume generated by the simple random algorithm and Fig. 27.2 shows an example of the representative volume generated by the 3–0 algorithm from ACELAN–COMPOS package. In Figs. 27.1 and 27.2 on the left all, elements are shown, in the center only volume elements of the second phase are shown, and on the right only shell elements are shown. The

Fig. 27.1 Example of RVE obtained by sample random algorithm, porosity 15%, 3002 surface elements

Fig. 27.2 Example of RVE obtained by ACELAN-COMPOS 3–0 algorithm, porosity 15%, 981 surface elements

334

A. Nasedkin et al.

shell elements located perpendicular to the plane O x1 x2 = O x y are shown in crimson color, and the shell elements located parallel to the plane O x1 x2 are shown in blue. The varicolored shell elements were endowed here with different anisotropic material properties, conformable to the structures of the surface stiffness moduli cs from (27.9) to (27.11). Here it can be noted that even with the same porosity for the simple random algorithm, the area of interface boundaries, usually, is substantially larger than for the 3–0 connectivity algorithm. For solving the thermal problems (27.2), (27.7), (27.18) with (27.19), (27.20), we used a twenty-node thermal element SOLID90 as volume finite element and a eight-node thermal element SHELL132 as surface finite element.

27.4 Numerical Results To provide an example, let us consider a nanoporous titanium. As it is known, the ordinary titanium is an anisotropic material of hexagonal symmetry. For numerical simulation we assume the following values of the material macro moduli of titanium with zero porosity: c11 = 16.24 × 1010 (N/m2 ), c12 = 9.2 × 1010 (N/m2 ), c13 = 6.9 × 1010 (N/m2 ), c33 = 18.7 × 1010 (N/m2 ), c44 = 4.67 × 1010 (N/m2 ), α11 = α33 = 8.4 × 10−6 (K−1 ), β11 = α11 (c11 + c12 + c13 ), β33 = α11 (2c13 + c33 ), (1) , etc.) k11 = k33 = 15.5 [W/(m K)], where superscript (27.1) is absent (cαβ = cαβ The material constants for the pores [marked by superscript (27.2)] were taken equal (2) (1) (1) (2) (2) = ηcαβ , η = 1 · 10−10 , α (2) to the following values: cαβ j j = α j j , k11 = k33 = 0.025 [W/(m K)]. In the numerical experiments, we varied the values of multipliers k s from s k = 10−6 ≈ 0 to 1. Figures 27.3 and 27.4 show the dependencies of the relative effective Young’s moduli r (E 1 ) = E 1eff /E 1(1) and r (E 3 ) = E 3eff /E 3(1) , with respect to the porosity p for the representative volumes constructed using the sample random algorithm and the 3–0 connectivity algorithm with two values of k s . Fig. 27.3 Dependencies of the relative effective modulus r(E 1 ) versus porosity for different coefficient k s and for two models of RVE

27 Finite Element Investigation of Effective Moduli …

335

Fig. 27.4 Dependencies of the relative effective modulus r(E 3 ) versus porosity for different coefficient k s and for two models of RVE

Fig. 27.5 Dependencies of the relative effective modulus r(c44 ) versus porosity for different coefficient k s and for two models of RVE

Here, E 1 = 1/s11 , E 3 = 1/s33 , s11 = (c11 c33 − (c13 )2 )/ c , s33 = (c11 + c12 )/Dc ,

c = (c11 − c12 )/Dc , Dc = (c11 + c12 )c33 − 2(c13 )2 . Similarly, Fig. 27.5 shows the dependencies of the relative effective shear modeff (1) /c44 with respect to the porosity p for the representative volumes ulus r (c44 ) = c44 constructed using the sample random algorithm and the 3–0 connectivity algorithm with two values of k s . As it can be seen from Figs. 27.3, 27.4 and 27.5, for small values of the coefficient k s the surface stresses do not affect the Young’s and shear moduli. However, for all values of porosity the surface stresses increase the effective stiffness moduli. Moreover, there are cases, where the nanoporous material have greater stiffness moduli than the same dense material. This situation takes place for the RVE obtained by the sample random algorithm with k s = 1 for the Young’s moduli E 1eff and E 3eff if p < 50%, and for shear modulus c44 if p < 25% (see the curves 3 in Figs. 27.3, 27.4 and 27.5, where we have the inequalities r (E j ) > 1 or r (c44 ) > 1). Figures 27.3, 27.4 and 27.5 illustrate that the values of the effective Young’s moduli and the values of the effective shear modulus are the largest for the simple random algorithm in the presence of surface stress. This effect is explained by the fact that for the composites obtained by the 3–0 connectivity algorithms the number of interface elements is much smaller than for similar composites with an arbitrary

336

A. Nasedkin et al.

Fig. 27.6 Dependencies of the relative pore surface versus porosity for two models of RVE

pore distribution (see Fig. 27.6). Thus, we can be conclude that the internal structures of nanoporous composites can have a significant effect on the values of effective stiffness moduli. We also emphasize that the porosity and the surface effects have the opposite influence on the effective stiffness: a simple increase of porosity leads to a decrease in effective stiffness moduli, but an increase of the surface stiffness moduli or a decrease of the pore size leads to a increase of the effective stiffness. The porosity growth up to certain limits enlarge the areas with surface stresses (see Fig. 27.6). Therefore, as the porosity of the nanostuctured material grows, the stiffness moduli can both decrease and increase. For example, for large values of the factor k s the increase of porosity for small p leads to a growth of the effective Young’s moduli and shear modulus, and with further increase of porosity the effective Young’s moduli and shear modulus begin to decrease. Thus, as in [1, 34–37], from the analysis of the computational experiments, we observed the following trends. If we compare two similar porous materials, one of which has an usual dimension of pores and the other has nanosized pores, then for the nanosized porous materials at the expense of the surface stresses the effective stiffness will be greater than for the porous materials of usual dimension of pores. Furthermore, for the porous solid of the macroscopic size of pores the effective stiffness moduli decrease with the porosity growth. Meanwhile, the effective stiffness moduli of nanoporous materials with the same porosity may either decrease or increase depending on the surface moduli values, porosity structure, type of connectivity, dimensions and number of pores. We can observe similar effects for the effective thermal conductivity coefficients. Acknowledgements The work was done in the framework of the Ministry of Science and Higher Education of Russia project No. 9.1001.2017/4.6 in part of the analysis of algorithms for creating granular composite structures and in the framework of the RFBR project 16-58-48009 IND_omi and DST in part of analyzing the effective properties of nanostructured porous thermoelastic composites.

27 Finite Element Investigation of Effective Moduli …

337

References 1. V.A. Eremeyev, Acta Mech. 227, 29 (2016) 2. J.C. Hamilton, W.G. Wolfer, Surf. Sci. 603, 1284 (2009) 3. J. Wang, Z. Huang, H. Duan, S. Yu, X. Feng, G. Wang, W. Zhang, T. Wang, Acta Mech. Solida Sin. 24(1), 52 (2011) 4. K.F. Wang, B.L. Wang, T. Kitamura, Acta. Mech. Sin. 32(1), 83 (2016) 5. M.E. Gurtin, A.I. Murdoch, Arch. Ration. Mech. Anal. 57, 291 (1975) 6. M.E. Gurtin, A.I. Murdoch, Int. J. Solids Struct. 14(6), 431 (1978) 7. A.I. Murdoch, Q. J. Mech. Appl. Math. 29, 245 (1976) 8. G. Chatzigeorgiou, A. Javili, P. Steinmann, Math. Mech. Solids. 20, 130 (2015) 9. H.L. Duan, J. Wang, Z.P. Huang, B.L. Karihaloo, J. Mech. Phys. Solids 53, 1574 (2005) 10. A. Javili, P. Steinmann, J. Mosler, Comput. Methods Appl. Mech. Engrg. 317, 274 (2017) 11. H. Le Quang, Q.-C. He, Mech. Mater. 40, 865 (2008) 12. H. Le Quang, T.-L. Phan, G. Bonnet, Int. J. Therm. Sci. 50, 1428 (2011) 13. H. Le Quang, D.C. Pham, G. Bonnet, Q.-C. He, Int. J. Heat Mass. Transf. 58, 175 (2013) 14. S. Graham, D.L. McDowell, J. Heat Transfer 125(3), 389 (2003) 15. V.I. Kushch, I. Sevostianov, V.S. Chernobai, Int. J. Eng. Sci. 83, 146 (2014) 16. H. Le Quang, Int. J. Heat Mass. Transf. 95, 162 (2016) 17. J.T. Liu, S.T. Gu, E. Monteiro, Q.-C. He, Comput. Mech. 53, 825 (2014) 18. L. Wu, Int. J. Eng. Sci. 48, 783 (2010) 19. J. Xiao, Y. Xu, F. Zhang, Compos. Struct. 189, 553 (2018) 20. T. Chen, G.J. Dvorak, C.C. Yu, Int. J. Solids Struct. 44(3–4), 941 (2007) 21. H.L. Duan, B.L. Karihaloo, J. Mech. Phys. Solids 55(5), 1036 (2007) 22. H. Le Quang, Q.-C. He, J. Mech. Phys. Solids 55, 1889 (2007) 23. H. Le Quang, Q.-C. He, Arch. Appl. Mech. 79, 225 (2009) 24. A. Javili, P. Steinmann, Int. J. Solids Struct. 47(24), 3245 (2010) 25. A. Javili, P. Steinmann, Comput. Methods Appl. Mech. Eng. 200(21–22), 1963 (2011) 26. A. Javili, A. McBride, P. Steinmann, Appl. Mech. Rev. 65(1), 010802 (2013) 27. A.V. Nasedkin, A.A. Nasedkina, A.S. Kornievsky, A.I.P. Conf, Proc. 1798, 020110 (2017) 28. A.V. Nasedkin, A.A. Nasedkina, A.S. Kornievsky, in Coupled Problems 2017—Proceedings of VII International Conference on Coupled Problems in Science and Engineering, 12-14 June 2017, Rhodes Island, Greece. ed. by M. Papadrakakis, E. Oñate, B.A. Schreflers, CIMNE, vol. 1140, (Barcelona, Spain, 2017) 29. A. Nasedkin, A. Nasedkina, A. Rajagopal, in Advanced Materials—Proceedings of International Conference on Physics and Mechanics of New Materials and Their Applications, PHENMA 2018. Springer Proceedings in Physics, ed. by I.A. Parinov, S.-H. Chang, Y-H. Kim, vols. 224, 399, (Springer, Berlin, 2019) 30. A.A. Nasedkina, A. Rajagopal, Mater. Phys. Mech. 37, 34 (2018) 31. A.B. Kudimova, I.V. Mikhayluts, D.K. Nadolin, A.V. Nasedkin, A.A. Nasedkina, P.A. Oganesyan, A.N. Soloviev, Procedia Struct. Integrity 6, 301 (2017) 32. N.V. Kurbatova, D.K. Nadolin, A.V. Nasedkin, P.A. Oganesyan, A.N. Soloviev, in Analysis and Modelling of Advanced Structures and Smart Systems. Advanced Structured Materials, ed. by H. Altenbach, E. Carrera, G. Kulikov, vol. 81, (Springer, Berlin, 2018), p. 69 33. A.B. Kudimova, D.K. Nadolin, A.V. Nasedkin, P.A. Oganesyan, A.N. Soloviev, Mater. Phys. Mech. 37(1), 25 (2018) 34. H.L. Duan, J. Wang, B.L. Karihaloo, Z.P. Huang, Acta Mater. 54, 2983 (2006) 35. V. Eremeyev, N. Morozov, Dokl. Phys. 55(6), 279 (2010) 36. A.V. Nasedkin, A.S. Kornievsky, Comput. Continuum Mech. 10, 375 (2017). (In Russian) 37. A.V. Nasedkin, A.S. Kornievsky, in Wave Dynamics and Composite Mechanics for Microstructured Materials and Metamaterials. Advanced Structured Materials, ed. by M.A. Sumbatyan, vol. 59, 107, (Springer, Berlin, 2017)

Chapter 28

Investigation of Initial Stresses’ Influence on Surface Wave Field in Bulk Metallic Glass Layer T. I. Belyankova, E. I. Vorovich, V. V. Kalinchuk, and O. M. Tukodova

Abstract The role of elastic moduli of the fourth order in the investigation of the dynamic characteristics of prestressed bodies made of materials that allow large static deformations is studied. The studies were carried out in the Lagrange coordinate system. Linearized defining relations and equations of motion of a prestressed medium are used, which allow us to consider nonlinear effects of the “second” and “third” orders. On the example of the problem of the propagation of shear harmonic oscillations, the influence of the initial stresses on the propagation velocity of surface waves is studied. Two, five, and nine constant models of a prestressed layer made of palladium-based bulk metal glass are considered. The results obtained in the framework of various models are compared. The difference of the effect of initial stresses on the velocities and critical output frequencies of the higher modes of surface waves, calculated with and without higher order moduli, is shown. A significant effect of the magnitude of the initial stresses is established for uniaxial and biaxial initial stress states.

28.1 Introduction The technological development of aircraft and cars building, devices making and electronics has led to the need to create new, high-tech, artificial materials that can retain their physical properties and unique qualities under any operating regime and conditions. The breadth and the variety of problems performed with the participation of new materials lead to the need for a detailed study of their physical properties, technological and strength characteristics. Carrying out such studies is associated with the need to solve complex applied problems of the theory of elasticity and to T. I. Belyankova (B) · V. V. Kalinchuk Southern Scientific Center of Russian Academy of Sciences, Rostov-on-Don, Russia e-mail: [email protected] I. I. Vorovich Institute of Mathematics, Mechanics and Computer Science, Southern Federal University, Rostov-on-Don, Russia E. I. Vorovich · O. M. Tukodova Don State Technical University, Rostov-on-Don, Russia © Springer Nature Switzerland AG 2020 I. A. Parinov et al. (eds.), Advanced Materials, Springer Proceedings in Materials 6, https://doi.org/10.1007/978-3-030-45120-2_28

339

340

T. I. Belyankova et al.

attract mechanical models of a hyperelastic medium [1, 2], with varying degrees of accuracy, reflecting the processes occurring in the materials under study. For isotropic materials, the elastic potential is represented as the scalar function of the invariants of one of the tensors of the strain measure or the strain tensor [2–6]. For hard materials (rocks, metals, alloys, crystals, etc.), the representation of the elastic potential proposed by Murnaghan in the form of a cubic function of the invariants of the Cauchy—Green strain tensor [7] with III-order constants is widely used. Due to theoretical and experimental studies, the values of constants of the third order are known for a wide range of metals, alloys, and various structural materials, crystals with various symmetry classes [6, 8–11], as well as for some rocks [12]. The use of models of hyperelastic material with moduli of elasticity of the third order made it possible to more accurately describe the properties of a prestressed medium: to study second-order effects [11, 12], to determine mechanical stresses [13, 14], to study the characteristics of the dynamics, propagation and localization of waves in prestressed media [15–26]. The review of works in this direction is presented in [15, 21]. In [15], a sequential linearization of the nonlinear equations of the mechanics of a solid elastic-deformable body was carried out in the Lagrange and Euler coordinate systems. Linearized defining relations and equations of motion of a prestressed medium are constructed in an arbitrary, generally curvilinear coordinate system. Expressions presented in a compact, convenient for research form were used in [15, 24–26] to solve a number of specific mixed problems of the dynamic theory of elasticity. In particular, for the model of an initially isotropic hyperelastic material with a potential in the Murnagan form, the influence of the nature of the initial mechanical influences on the formation, propagation, and localization of wave fields in both homogeneous and inhomogeneous prestressed media were studied [24–26]. Recently, a number of new materials, promising in practical applications and possessing unique physical properties has appeared. In particular, these materials are able to withstand a very high level of elastic deformation, at which the nonlinearity of the elastic properties becomes very significant. In [27–31], the results of studies to determine the elastic moduli of the third and fourth order for bulk metal glasses based on zirconium (Zr) and palladium (Pd) are presented. The study of the dynamics of structures involving such materials requires an improvement in the theory of linearized contact for prestressed bodies. In [32], a sequential linearization of the nonlinear equations of mechanics of an initially isotropic elastic body in the vicinity of a certain initial stress state was carried out. The linearization was carried out in the framework of the theory of small strains superimposed on a final one in the Lagrange coordinate system. The representation of the specific strain energy in terms of the algebraic invariants of the Green-Lagrange strain tensor is used as the elastic potential for an initially isotropic body. Linearized defining relations and equations of motion of a prestressed medium are obtained, allowing to consider the nonlinear effects of initial deformation on the elastic properties of an initially isotropic body. In this paper, we propose an approach to study the dynamics of prestressed initially isotropic elastic bodies with allowance for IV modules. Using the example of the problem of excitation of shear harmonic oscillations in a layer by a point surface

28 Investigation of Initial Stresses’ Influence on Surface Wave …

341

source, the effect of higher-order moduli on the propagation velocity of surface waves is studied. Two-, five-, and nine-constant models are considered, as well as a model of linear approximation in deformations. The effect of prestresses on the velocities and critical output frequencies of new modes is investigated.

28.2 Formulation of the Problem Consider the boundary-value problem of vibrations of a prestressed layer caused by the action of a surface load q = {q1 , q2 , q3 }e−iω t , distributed in a certain region . Outside this region, the surface of the medium is free of stresses. The lower edge of the layer | x1 |, | x2 | ≤ ∞, 0 ≤ x3 ≤ h is rigidly bonded to a non-deformable base. The layer material is assumed to be compressible, initially isotropic, having an elastic potential 1 1 4 1 1 χ = − p I1 + λI12 + μI2 + ν1 I13 + ν2 I1 I2 + ν3 I3 + γ1 I14 + γ2 I12 I2 2 6 3 24 2 4 1 2 + γ3 I 1 I 3 + γ4 I 2 . (28.1) 3 2 Here Ik = tr Sk , (k = 1, 2, 3) are the algebraic invariants of the Cauchy-Green strain tensor S; λ, μ are elastic moduli of the second order; ν1 , ν2 , ν3 and γ1 , γ2 , γ3 , γ4 are elastic moduli of the third and fourth orders, respectively. We assume that the state S = 0 is a state with minimal free energy, i.e. p = 0, the initial stress state is determined by a uniform initial deformation [3, 15, 32]: R = r · , = δk m vk ik im ; vk = const, k = 1, 2, 3

(28.2)

here R, r are the radius vectors of a point of the medium in the initial deformed and natural state (NS), respectively, vi = 1 + δi , δi are the relative elongations of the fibers directed in a natural configuration along the axes coinciding with the Cartesian coordinates, δi j is the Kronecker symbol. The studies are carried out in the Lagrangian coordinate system, which coincides with a rectangular Cartesian system, the oscillation mode is assumed to be steady, the time factor is omitted. Further, in the work we use dimensionless parameters: linear parameters are assigned to the layer thickness, density—to the density in the natural state, elastic parameters—to the shear modulus in the NS. √ As a dimensionless frequency, the parameter κ2 = ω h/VS0 is used, where VS0 = μ0 /ρ0 is the shear wave velocity in the NS; ω is the angular frequency. Within the framework of the accepted assumptions, the boundary-value problem of the oscillations of the prestressed layer in the Lagrange coordinates is described by the linearized equations of motion [15, 32]:

342

T. I. Belyankova et al.

∇0 · = ρ0

∂ 2u ∂t 2

(28.3)

and linearized boundary conditions on the surface o = o1 + o2 : o1 : n · = q, o2 : u = u∗

(28.4)

here ∇0 is the Hamilton operator, u = {u 1 , u 2 , u 3 } is the displacement vector, n is the vector of the external normal to the surface of the medium, defined in the coordinate system associated with the NS; ρ0 is the density of the material in the NS; is the linearized Piola stress tensor, whose components are representable in the form [2–4, 15, 32]: Θi j = Ci∗jkl

∂u k , i, j = 1, 2, 3. ∂ xl

(28.5)

The coefficients Ci∗jkl determine the properties of a prestressed body and, in accordance with [32] have the form: ∗ = vi2 ξii + 2vi2 (ψ1 + 3ψ2 Si ) + Pi , Cii∗ j j = vi v j ξi j , i = j, Ciiii 3 3 ∗ ∗ 2 Ci ji j = v j vi ψ1 + ψ2 Si + S j , Ci j ji = v j ψ1 + ψ2 Si + S j + Pi 2 2

ξkn = ψ01 + 2ψ02 Sn + 3ψ03 Sn2 + 2(ψ11 + 2ψ12 Sn )Sk + 4ψ21 Sk2 , k, n = 1, 2, 3 (28.6) other coefficients Ci∗jkl are zero. According to [32], taking into account (28.1), (28.2) for the components Sk and Pk following relations are valid: Sk =

1 2 vk − 1 , Pk = ψ0 + 2ψ1 Sk + 3ψ2 Sk2 , k = 1, 2, 3. 2

1 ψ01 = λ + ν1 I1 + γ1 I12 + γ2 I2 , ψ02 = ψ11 = ν2 + γ2 I1 , 2 4 ψ03 = ψ21 = γ3 , ψ12 = γ4 , ψ13 = ψ22 = ψ23 = 0, 3 Im = S1m + S2m + S3m , m = 1, 2, 3. 1 1 4 ψ0 = λI1 + ν1 I12 + ν2 I2 + γ1 I13 + γ2 I1 I2 + γ3 I3 , 2 6 3 4 2 ψ1 = μ + ν2 I1 + γ2 I1 /2 + γ4 I2 , ψ2 = (ν3 + γ3 I1 ). 3

(28.7)

(28.8)

(28.9)

In the absence of initial stresses (v1 = v2 = v3 = 1), taking into account (28.6)– (28.9), we obtain:

28 Investigation of Initial Stresses’ Influence on Surface Wave …

343

∗ Ciiii = λ + 2μ, Cii∗ j j = λ, Ci∗ji j = μ, Ci∗j ji = μ.

Taking into account representations (28.5), (28.6), we write the boundary-value problem (28.3), (28.4) in the form [15, 32]: Ci∗jkl

∂ 2u j ∂ 2uk = ρ0 2 , ∂ xl ∂ x i ∂t

j = 1, 2, 3

(28.10)

with the boundary conditions: ∗ x3 = h: C3113

∂u 1 ∂u 3 ∗ + C1313 = q1 , ∂ x3 ∂ x1

∂u 2 ∂u 3 ∗ + C2323 = q2 , ∂ x3 ∂ x2 ∂u 3 ∂u 1 ∂u 2 ∗ ∗ ∗ C3333 + C1133 + C2233 = q3 ∂ x3 ∂ x1 ∂ x2 x3 = 0: u k = 0, k = 1, 2, 3 ∗ C3223

(28.11)

28.3 Solution of the Problem To solve the boundary value problem (28.10), (28.11), the approach [15] is used: the solution is constructed in Fourier images in the form of an expansions: Up =

3

f pk (ck1 sh σk x3 + ck2 ch σk x3 ), p = 1, 2,

k=1

U3 =

3

ck1 ch σk x3 + ck2 sh σk x3 .

(28.12)

k=1

Here Uk are the Fourier transforms of the component of the displacement vector; f ik are coefficients selected from the condition when the solution (28.12) is satisfied to the equations of motion; cik are coefficients are determined by substituting (28.12) into the boundary conditions; σk are the values of the characteristic equation [15]. Using the inverse Fourier transform, the solution of the original boundary value problem (28.10), (28.11) is represented by the expressions (α1 , α2 are the Fourier transform parameters in coordinates x1 , x2 ): 1 u= 4π 2

¨ k(x1 − ξ, x2 − η, x3 , κ2 ) q(ξ, η) dξ dη

344

T. I. Belyankova et al.

k(s, t, x3 , κ2 ) =

K(α1 , α2 , x3 , κ2 )e−i(α1 s+α2 t) dα1 dα2

(28.13)

1 2

The form of the matrix—functions elements K(α1 , α2 , x3 , κ2 ) in the representation (28.13) essentially depends on the nature of the initial stress state of the medium.

28.3.1 Shear Layer Vibrations In the study of shear oscillations of a prestressed layer under the action of a surface source distributed in the region {Ω(x1 , x2 , x3 ): |x1 | ≤ 1, |x2 | < ∞, x3 = h}, in the boundary value problem (28.3), (28.4), it is necessary to take into account the conditions: u 2 = u 2 (x1 , x3 ), u 1 = u 3 = 0,

∂ = 0. ∂ x2

(28.14)

Taking into account conditions (28.14), solution (28.13) looks like: 1 u 2 (x1 , x3 ) = 2π k22 (s, x3 , κ2 ) =

1 k22 (x1 − ξ, x3 , κ2 )q(ξ ) dξ,

(28.15)

−1

K 22 (α, x3 , κ2 ) e−iα s dα, K 22 (α, x3 , κ2 ) = sh(σ2 x3 )−1 ,

∗ −1 ∗ ∗ σ2 = α 2 C1221 − κ22 (C3223 ) , = C3223 σ2 ch(σ2 h)

(28.16)

Contour G is selected according to the radiation conditions. Representation (28.15) determines the displacement of an arbitrary point of the layer. In the case of a point source of oscillation q(x1 ) = {0, δ(x1 ), 0} (here δ(x1 ) is the Dirac function) for the displacement in the layer, the following expression is valid: 1 u 2 (x1 , x3 , κ2 ) = K 22 (α, x3 , κ2 )e−iαx1 dα. (28.17) 2π Γ

It can be seen from representations (28.16), (28.17) that in this case the influence of the initial stresses on the displacements in the layer, is associated with changes in ∗ ∗ and C3223 . two coefficients C1221

28 Investigation of Initial Stresses’ Influence on Surface Wave …

345

28.4 Determination of Initial Stress State The state of a prestressed body is described by the Kirchhoff tensor, which in the case of a uniform initial deformation (28.2) is defined in (28.7) with coefficients (28.9). Grouping the terms by the degrees of the strain tensor S, for the components of the Kirchhoff tensor, we get: P1 = (λ + 2μ)S1 + λS2 + λS3 + H12 + H13 , P2 = λS1 + (λ + 2μ)S2 + λS3 + H22 + H23 , P3 = λS1 + λS2 + (λ + 2μ)S3 + H32 + H33 .

(28.18)

Following [32], we consider four models: Model I. In elastic potential (28.1), only terms with second-order modules are stored; coefficients ψk (k = 1, 2, 3) (28.9) are determined by the expressions: ψ0 = λI1 , ψ1 = μ, ψ2 = 0,

Hk2 = Hk3 = 0.

The components of the Kirchhoff tensor in this case are linearly related to the components of the strain tensor. Model II. The linear approximation for invariants of the strain measure is used: vk = 1 + δk , vk2 = 1 + 2δk , vk vi = 1 + δk + δi , i, k = 1, 2, 3, i = k Sk = δk , I1 = θ = δ1 + δ2 + δ3 , I2 = I3 = 0, The components of the Kirchhoff tensor (28.18) are expressed by the formulas: Pk = λθ + 2μδk , k = 1, 2, 3. The coefficients Ci∗jkl from the representation (28.6) in this case can be expressed as ∗ = Pi + (λ + 2μ) + ν1 θ + 2(λ + 2μ + 2ν2 )δi , Ciiii Cii∗ j j = λ + ν1 θ + (λ + 2ν2 ) δi + δ j , Ci∗ji j = μ + (μ + 2ν3 ) δi + δ j , Ci∗j ji = Pi + μ + 2μδ j + 2ν3 δi + δ j ,

i, j = 1, 2, 3, i = j. Model III. In the representation (28.1), only terms with elastic moduli of the second and third orders, for ψk (k = 1, 2, 3) are saved; 1 4 ψ0 = λI1 + ν1 I12 + ν2 I2 , ψ1 = μ + ν2 I1 , ψ2 = ν3 , 2 3

346

T. I. Belyankova et al.

in view (28.18) Hk2 = 0 i Hk3 = 0. Model IV. In (28.1), modules of the third and fourth orders are taken into account. In the representation of the components of the Kirchhoff tensor (28.18), Hk2 = 0 and Hk3 = 0, (k = 1, 2, 3), which allows us to take into account the influence of the second and third degrees of initial deformation. The form Hk2 and Hk3 is given in [32]. Relations (28.18) are the system of three, generally non-linear, equations for three unknowns: S1 , S2 , S3 , P1 , P2 , P3 or their combinations, depending on the method of setting the initial stress-strain state. In the combined setting of the initial state, it is assumed that deformation along one axis (for example, v1 ) and two stress conditions are known. Deformations and stresses along other axes are determined from system (28.18). Further, the influence of the magnitude of the initial stresses under uniaxial 1x1 (P1 = P, P2 = P3 = 0) and biaxial 2x1 (P1 = 0, P2 = P3 = P) initial stress states is investigated.

28.5 Numerical Analysis The material used was Pd40 Cu30 Ni10 P20 metal glass based on palladium (Pd) with the following parameters [29]: ρ = 9300 kg m−3 , λ = 1.453 × 1011 Pa, μ = 0.358 × 1011 Pa, ν1 = −2.27 × 1011 Pa, ν2 = −2.34 × 1011 Pa, ν3 = −0.818 × 1011 Pa, γ1 = −105.828 × 1012 Pa, γ2 = 15.556 × 1011 Pa, γ3 = 1.81 × 1011 Pa, γ4 = −2.98 · 1011 Pa. As noted, in the case of shear vibrations of a prestressed layer with a clamped lower face, it follows from (28.16), (28.17) that the influence of the initial stresses on ∗ ∗ and C3223 . the displacements is associated with changes in the two coefficients C1221 ∗ ∗ In Fig. 28.1a, b the dependence of the coefficients C1221 and C3223 on the magnitude of the initial strains v1 , acting along the axis x1 , is presented for uniaxial 1x 1 and biaxial 2x 1 initial stress states. The numbers 1, 2, 3, 4 mark the curves corresponding ∗ within the framework of the four models under consideration, curves to changes C1221 ∗ . Dotted lines (curves 1) correspond 1 , 2 , 3 , 4 correspond to the changes of C3223 to coefficients calculated without taking into account higher order modules [model I, Hk2 = Hk3 = 0 in (28.18)], dashed lines (curves 3)—taking into account modules of the third order Hk2 = 0, Hk3 = 0), solid lines (curves 4)—taking into account modules of the III and IV orders (model IV, Hk2 = 0, Hk3 = 0). The dash-dotted lines (curves 2) correspond to a linear respect to deformations approximation (model II).

28 Investigation of Initial Stresses’ Influence on Surface Wave …

(a)

(b) 2

1

3' 4

2 4'

stretch ratio v1

C1221*, C3223*

C1221*, C3223*

2'

3

347

1

2' 4 3 4'

1'

1'

3'

stretch ratio v1

∗ ∗ Fig. 28.1 Influence of the initial strain on the coefficients C1221 and C3223 of uniaxial 1x 1 a and biaxial 2x 1 b initial stress states

As follows from the graphs, the inclusion of higher order modules leads to significant nonlinearity in the behavior of the coefficients, the region of one-to-one correspondence, which determines the internal stability of the material, has significantly decreased. Taking into account IV constants to a greater extent narrows the range of elongations at which the material remains stable. It should be noted that, unlike model I, for the other three models there is a small region of small deformations in which the values of the coefficients are close.

28.5.1 Influence of Initial Stresses on Dispersion Properties of Layer An analysis of the solutions of dispersion equation (α, κ2 ) = 0 (28.16) showed that the form of the initial stress state and the magnitude of the stresses that significantly ∗ ∗ and C3223 lead to significant changes of the affect the behavior of the coefficients C1221 dispersion properties of the layer material. This is manifested in a shift of the critical frequencies of the appearance of surface wave modes upwards and in a change of the angle of the dispersion curves inclination. In Fig. 28.1a–d on the example of the 5th mode, fragments of dispersion curves are shown for I (Fig. 28.2a), II (Fig. 28.2b), and III (Fig. 28.2d) models in case of initial stress state 1x 1 . Figure 28.2d shows a fragment for the initial stress state 2x 1 . Curves 1, 2, 3, 4 in the Figures correspond to tensions v1 = 1.01, 1.02, 1.03, 1.04, curve 0 corresponds to the dispersion curve in the NS. It can be seen from the Fig. 28.2 that when using model I, the shift of the values of the critical frequencies occurs downward. For models II, III, and IV, the action of initial stresses leads to a shift of the critical frequencies upward; their values depend on the type of model, the type and magnitude of the initial stress state.

348

T. I. Belyankova et al.

(a)

(b) 1x1

1x1

II Wave number (ξ)

Wave number (ξ)

I 4 3

2 1

0 1 2 3 4

0

Dimensionless frequency κ2

Dimensionless frequency κ2

(c) 1x1

2x1

III

0 1 2 3 4

Wave number (ξ)

III Wave number (ξ)

(d)

0 1 2

3 4

Dimensionless frequency κ2

Dimensionless frequency κ2

Fig. 28.2 Fragment of the 5th mode of dispersion curves for models I (a), II (b) and III (c) in the case of uniaxial tension 1x 1 , d fragment of the 5th mode for model III, stress state 2x 1

28.5.2 Influence of Initial Stresses Magnitude on Surface Waves Velocity Figure 28.3a–d show the effect of the initial strains magnitude by the initial state 1x 1 onthe frequency distribution of the phase velocities of surface waves VFσ /VS0 [VFσ = ω ξ , ξ is the solution of dispersion (28.16)] for the models under consideration. As before, curves 1, 2, 3, 4 correspond to stretches v1 = 1.01, 1.02, 1.03, 1.04, the number 0 marks the curves for the NS. As follows from the figures, in models I, III, and IV, the initial stress mainly affects the asymptotic values of the velocities. In model I, this effect is directly proportional to the magnitude of the initial stresses, in models III and IV, it is inversely proportional. In model II, the initial influence is mainly influenced by the shift of critical frequencies; the effect on the asymptotic values of the velocities is negligible. A more visual representation of the influence of initial stresses on various modes of surface waves is given by the deviation and relative deviation of their phase velocities with respect to phase velocity in the NS: D = VF0 − VFσ VS0 , δ = VF0 − VFσ VF0 .

(28.19)

28 Investigation of Initial Stresses’ Influence on Surface Wave …

(а)

349

(b) 0

0 1

Phase velocity (VFσ/VS0)

Phase velocity (VFσ/VS0)

I

2 3 4

1 2

(c)

0

4

Dimensionless frequency κ2

VI Phase velocity (VFσ/VS0)

Phase velocity (VFσ/VS0)

3

(d) III

3

II

Dimensionless frequency κ2

Dimensionless frequency κ2

1 2

4

0

1 2

3

4

Dimensionless frequency κ2

Fig. 28.3 Effect of the initial deformation on the velosity of surface waves for models I (a), II (b), III (c) and IV (d)

Figure 28.4a–d show the graphs of deviation D (28.19) for odd velocity modes of surface waves. Curves 1, 2, 3, 4 correspond to tension 1.01, 1.02, 1.03, 1.04 by a uniaxial initial stress state of 1x 1 . The graphs in Fig. 28.4 illustrate the dependence of the asymptotic values of the phase velocities of surface waves on the initial deformation for various models. It can be seen from the Figures that the maximum influence of v1 takes place in model IV. The shift of the critical frequencies is insignificant in all models except for II, in which this shift is directly proportional to the tension v1 and increases with increasing mode number. Figure 28.5a–d show the graphs of relative deviation δ (28.19) for the first three modes of surface waves. The relative deviation, calculated in the framework of four models; in the case of a uniaxial 1x 1 initial stress state for v1 = 1.01 and 1.03, are given in Fig. 28.5a and b, respectively. For comparison, Fig. 28.5c, d show the graphs δ for the first three modes of model III in the case of uniaxial 1x 1 and biaxial 2x 1 tension v1 = 1.01 and 1.03. It can be seen from Fig. 28.5a, b that the maximum influence of the initial 1x 1 strain on the phase velocities of surface waves occurs in models III and IV. A somewhat smaller, but qualitatively opposite in character, effect of the initial deformation on surface waves is observed in model II. The second factor in the influence of the initial deformation on surface waves is the shift of critical frequencies. For the initial

350

T. I. Belyankova et al.

(b) I

2 1

4

3

II

Deviation of velocity (D)

Deviation of velocity (D)

(a)

1 2 3 4

Dimensionless frequency κ2

Dimensionless frequency κ2

(d) III

4 3 2 1

Dimensionless frequency κ2

Deviation of velocity (D)

Deviation of velocity (D)

(c) VI 4 3 2 1

Dimensionless frequency κ2

Fig. 28.4 The phase velocity deviation of the odd modes for models I (a), II (b), III (c) and IV (d)

deformation of the 1x 1 species, it is pronounced in model II; in models I, III, and IV, it is insignificant. From Fig. 28.5c, d it can be seen that a change in the form of the initial stress state leads to qualitatively different results. The determining factor of influence in model III for the initial 1x 1 state is phase velocity. For the initial 2x 1 state, the decisive factor in the effect is the shift in the value of the critical frequency. Comparing Fig. 28.5b and d it is easy to see that this shift in model III for the same values of v1 exceeds the shift in model II.

28.6 Conclusions An approach is proposed to study the dynamic characteristics of a prestressed layer under the influence of large initial stresses made of a material that allows significant static deformations. The studies were carried out in the Lagrange coordinate system using various theories of dynamics of prestressed bodies. Two-, five-, and nine-constant models are considered. Linearized defining relations and equations of motion of a prestressed medium are used, which allow one to take into account the

28 Investigation of Initial Stresses’ Influence on Surface Wave …

(b) v1 =1.01

IV

v1 =1.03

III II

I

Deviation of velocity (δ)

Deviation of velocity (δ)

(a)

Dimensionless frequency κ2

IV

III II I

Dimensionless frequency κ2

(c)

(d)

1x1

2x1

Dimensionless frequency κ2

v1 =1.03

III Deviation of velocity (δ)

v1 =1.01

Deviation of velocity (δ)

351

III

1x1

2x1

Dimensionless frequency κ2

Fig. 28.5 The relative deviation of the phase velocities of the first three modes: a, b comparison of models under initial stress state 1x 1 ; c, d comparison of the influence of the initial states 1x 1 and 2x 1 , model III

nonlinear effects of the “second” and “third” orders of influence of mechanical strains on the elastic properties of the starting material. Using the example of the problem of shear harmonic oscillations in a layer, we studied the influence of the magnitude and type of initial stresses on the structure of the surface field and the propagation velocity of surface waves. The results obtained in the framework of various models are compared. The effect of taking into account higher order moduli on the surface wave velocities at various values of the initial strains is shown. The influence of the type and magnitude of the initial uniaxial and biaxial effects on the transformation of the phase velocities of surface waves is established. It is shown that the decisive factor in the influence of the initial deformation on surface waves for some models may be the value of the phase velocity, for other models, the values of the critical frequencies of the appearance of surface wave modes. Which of the factors is decisive may depend on the type of initial stress state. Acknowledgements The work was prepared during the competitive part of the state assignment of the Russian Ministry of Education and Science under project No. 9.1001.2017/4.6 with partial financial support from the Russian Foundation for Basic Research (projects 19-08-01051, 19-48230042, 19-01-00719 and 18-08-01012).

352

T. I. Belyankova et al.

References 1. C. Truesdell, A First Course in Rational Continuum Mechanics (Academic, New York, 1977) 2. G.A. Maugin, Continuum Mechanics of Electromagnetic Solids (Elsevier Science Publishers, Amsterdam, 1968) 3. A.I. Lurie, Non-linear Theory of Elasticity (North-Holland, Amsterdam, 1990) 4. V.A. Krasil’nikov, V.V. Krylov, Introduction to Physical Acoustics (Nauka, Moscow, 1984). (In Russian) 5. M. Shams, M. Destrade, R.W, Wave Motion 48(7), 552 (2011) 6. M. Destrade, R.W. Ogden, J. Acoust. Soc. Am. 128(6), 3334 (2010) 7. F.D. Murnaghan, Am. J. of Math 59(2), 235 (1937) 8. R.N. Thurston, K. Brugger, Phys. Rev. 133(6A), A1604 (1964) 9. R.T. Smith, R. Stern, R.W.B. Stephens, J. Acoust. Soc. Amer 40(5), 1002 (1966) 10. S.S. Sekoyan. Akust. Zh 16(3), 453 (1970). (In Russian) 11. D.S. Hughes, J.L. Kelly, Phys. Rev. 92(5), 1145 (1953) 12. V.N. Bakulin, A.G. Protosenya, Dokl. Akad. Nauk SSSR 263(2), 314 (1982) 13. V. Erofeev, V.A. Zaznobin, R.V. Samokhvalov, Acoust. Phys. 53(5), 546 (2007) 14. N.Y. Nikitina, A.V. Kamyshev, S.V. Kazachek Russ. J. Nondestruct. Test 51(3),171 (2015) 15. V.V. Kalinchuk, T.I. Belyankova, Dynamic Contact Problems for Prestressed Bodies (Fizmatlit, Moscow, 2002). (In Russian) 16. M. Hayes, R.S. Rivlin, Arch. Ration. Mech. and Anal. 8(1), 15 (1961) 17. V.V. Kalinchuk, I.B. Polyakova, Int. Appl. Mech 18(6), 504 (1982) 18. V.V. Kalinchuk, I.B. Poliakova, J. of Appl. Math. Mech. 44(2), 224 (1980) 19. V.V. Kalinchuk, T.I. Belyankova, Izv. AN. MTT [Mechanics of Solids] 2, 89 (1998) 20. A.N. Guz, Elastic Waves in Initially Stressed Bodies. Vol. 1. General Aspects (Naukova Dumka, Kiev, 1986). (In Russian) 21. A.N. Guz, Elastic Waves in Initially Stressed Bodies. Vol. 2. Propagation Laws (Kiev, Naukova Dumka, 1986). (In Russian) 22. T.I. Belyankova, V.V. Kalinchuk, J. Appl. Math. Mech. 57(4), 713–724 (1993) 23. A.N. Guz, Int. Appl. Mech. 38(1), 23 (2002) 24. V.V. Kalinchuk, T.I. Belyankova, Dynamics of the Surface of Inhomogeneous Media (Fizmatlit, Moscow, 2009). (In Russian) 25. T.I. Belyankova, V.V. Kalinchuk, Mater. Phys. Mech. 23(1), 25 (2015) 26. T.I. Belyankova, V.V. Kalinchuk, Acoust. Phys. 63(3), 245 (2017) 27. N.P. Kobelev, E.L. Kolyvanov, V.A. Khonik, Phys. Solid State 49(7), 1209 (2007) 28. N.P. Kobelev, V.A. Khonik, A.S. Makarov, G.V. Afonin, YuP Mitrofanov, J. Appl. Phys. 115(3), 033513 (2004) 29. N.P. Kobelev, E.L. Kolyvanov, V.A. Khonik, Phys. Solid State 57(8), 1483 (2015) 30. H. Wang, M. Li, J. Appl. Phys. 113, 213515 (2013) 31. Z. Zhou, H. Wang, M. Li, J. Appl. Phys. 126, 145901 (2019) 32. T.I. Belyankova, V.V. Kalinchuk, D.N. Sheydakov, Mater. Phys. and Mech 40(2), 187 (2018)

Chapter 29

Comparison of Two Numerical Inverse Laplace Transform Methods with Application for Problem of Surface Waves Propagation in an Anisotropic Elastic Half-Space Ivan Markov and Leonid Igumnov Abstract The propagation of the surface waves in elastic media has been extensively studied and is very important in many fields. The Laplace domain Boundary Element Method (BEM) is powerful and accurate numerical method that can be employed for treating such problems. Since anisotropic elastic problems is very computationally challenging for any BEM formulation, the choice of particular numerical Laplace inversion algorithm is crucial for efficient anisotropic elastodynamic Laplace domain boundary element analysis. In this investigation, for a specific problem of anisotropic linearly elastic half space subjected to transient loading, we examine two different methods for numerical inversion of Laplace transforms. The first method we test is the renowned Durbin’s method which is based on a Fourier series expansion. The second method is the convolution quadrature method which is reformulated as a numerical Laplace transform inversion routine. Methods are compared in the context of their application in the framework of Laplace domain collocation boundary element formulation.

29.1 Introduction The propagation of the surface waves in elastic media has been extensively studied and is very important in the fields of dynamic soil-structure interaction analysis, seismology, earthquake engineering, etc. Among other powerful numerical methods Boundary Element Method (BEM) is particularly well-suited for modelling elastic wave propagation in infinite and semi-infinite domains. There are different BEM formulations that can be used for treating such problems and Laplace domain direct BEM approach is one of most well-studied and frequently employed. In case of linear anisotropic elasticity BEM can be implemented very efficiently. However, I. Markov (B) · L. Igumnov Research Institute for Mechanics, National Research Lobachevsky State University of Nizhny Novgorod, Nizhny Novgorod, Russia e-mail: [email protected] © Springer Nature Switzerland AG 2020 I. A. Parinov et al. (eds.), Advanced Materials, Springer Proceedings in Materials 6, https://doi.org/10.1007/978-3-030-45120-2_29

353

354

I. Markov and L. Igumnov

when anisotropic elastic materials are considered, implementation of any BEM that utilizes anisotropic elastic dynamic fundamental solutions gets complicated due to an issue with their efficient evaluation. As presented by Wang and Achenbach [1, 2], regular parts of three-dimensional anisotropic elastic fundamental solutions can be expressed as integrals over the surface of a half of a unit sphere. These integrals must be calculated using numerical quadrature which can be quite time consuming. Thus, a proper choice of a numerical inversion method can considerably boost the performance of frequency or Laplace domain BEM for linear anisotropic elastic materials. Durbin’s method [3] for numerical inversion of Laplace transforms is based on a Fourier series expansion and is a popular option for transient wave propagation problems. There is a number of works (e.g. [4–7]) that are dedicated to improvements of Durbin’s method, including, among other aspects, convergence acceleration of the Fourier series, reduction of error, choice of free parameters. Convolution Quadrature Method (CQM) is a relatively recent method originally developed by Lubich [8, 9] as a quadrature rule for convolution integrals. CQM can be reformulated as a numerical inversion procedure for Laplace transforms, and Schanz [10] stated that for a short time periods CQM is superior to other inversion methods. Pekeris [11] presented analytical solutions for horizontal and vertical displacements of the free surface of a homogeneous isotropic linearly elastic half-space due to a surface impulse loading. Eskandari-Ghadi and Sattar [12] derived analytical expressions for the surface and internal displacements of a transversely isotropic half-space under axisymmetric surface point loading. In the present chapter we present and discuss the comparison of the Durbin’s method and the CQM in the context of their application in the framework of Laplace domain collocation BEM formulation for transient surface waves propagation in anisotropic linearly elastic half-space. Test functions are the horizontal and vertical displacements of the surface of a transversely isotropic half-space subjected to Heaviside-type surface point load.

29.2 Preliminary Considerations and Test Functions The Laplace transform and its inversion are defined by the following relationships +∞ e−st f (t)dt, s = α + iω, F(s) = L{ f (t)} =

(29.1)

0

f (t) = L

−1

1 {F(s)} = 2πi

α+i∞

est F(s)ds, α−i∞

(29.2)

29 Comparison of Two Numerical Inverse Laplace Transform Methods …

355

with f (t) = 0 for t < 0, α is arbitrary real number greater than the real parts of all the singularities of F(s). Application of Laplace domain BEM for elastodynamic problems usually consists of obtaining Laplace domain responses for a set of sampling complex frequencies sl , l = 1, Ns , and then obtaining time-domain solutions via numerical inversion method. It is expected that the Laplace domain BEM is mesh sensitive, meaning that the spatial discretization and the frequency discretization are related and not independent. In other words, a certain minimum number of boundary elements per wavelength are required for a reliable dynamic boundary element analysis. Even more intricate this issue becomes for anisotropic elastic media since the wave velocities are dependent on direction. Additionally, integrals in the expressions of anisotropic elastic dynamic fundamental solutions can become highly oscillatory for high frequencies. From the practical point of view it means, that before starting Laplace domain boundary element calculations, we need to somehow determine maximum allowable value ωmax of imaginary part of complex Laplace transform parameter s. For all these reasons, further in our investigation we will assume, that in application of both considered numerical Laplace inversion methods, we are restricted by a certain value ωmax . For the original function in time-domain denoted as f (t) and approximation of f (t) obtained with a numerical inversion routine from its Laplace transform as f˜(t) we define relative error Rerr and pointwise absolute error Aerr (tk ) as follows

Rerr

⎛

2 ⎞ Nt f (tk ) − f˜(tk ) ⎜ k=0 ⎟ ˜(tk ), tk = k tmax , f , A = = − f (t (t ) ) ⎠ Nt err k k ⎝ 2 Nt k=0 f (tk ) (29.3)

where tmax is the largest value in the time range over which f˜(t) is obtained. As the test functions we use radial and vertical displacements of the free surface of transversely isotropic half-space under Heaviside-type surface point load. Transversely isotropic material of the half-space is characterized by mass density ρ and the elasticity tensor Ci jkl . In the cylindrical coordinates radial displacements u(r, z = 0, t) and vertical displacements w(r, z = 0, t) are given as follows [12] α3 Pmax t 2 Im u(r, z = 0, t) = − π 2r 3

π / 2

a22 β1 − a21 β2 cos θ dθ , f

(29.4)

0

w(r, z = 0, t) = Pmax t − 2 2 Im π r

π / 2 (1 + α1 )ψ 2 − ρ0 (a22 − a21 ) + α2 a22 β12 − a21 β22 cos θ dθ f 0

(29.5)

356

I. Markov and L. Igumnov

ψ(r, t, θ ) = α1 =

a11

t cos θ , f = a11 a22 − a12 a21 , r

C1212 + C1122 C1313 C1133 + C1313 ρ , α2 = , α3 = , ρ0 = , C1212 C1212 C1212 C1212 1 β1 = −k1 ψ 2 + k2 + k3 ψ 4 − k4 ψ 2 + k5 , 2 1 β2 = −k1 ψ 2 + k2 − k3 ψ 4 − k4 ψ 2 + k5 , 2 = −α3 C1133 + (1 + α1 )C3333 ψ 2 − ρ0 C3333 β1 + α2 C3333 β13 ,

(29.6) (29.7)

(29.8) (29.9)

a12 = −α3 C1133 + (1 + α1 )C3333 ψ 2 − ρ0 C3333 β2 + α2 C3333 β23 ,

(29.10)

a21 = −(1 + α1 )C3333 ψ 2 + ρ0 iψ + (α3 − α2 )iψβ12 ,

(29.11)

a22 = −(1 + α1 )C3333 ψ 2 + ρ0 iψ + (α3 − α2 )iψβ22 ,

(29.12)

2 h 21 + h 22 1 1 1 , k3 = h 22 − h 21 , , k2 = ρ + (29.13) k1 = 2 2 C3333 C1313 2 1 C1111 1 1 1 h 1 + h 22 − 2 , + + k4 = 2ρ C3333 C1313 C3333 C1111 C1313 2 1 1 2 k5 = ρ − , (29.14) C3333 C1313

where Pmax is the amplitude of the load, h 21 and h 22 are the roots of the following equation 2 − 2C1133 C1313 h 2 + C1111 C1313 = 0. C3333 C1313 h 4 − C1111 C3333 − C1133 (29.15) For our investigation we chose Pmax = 1 Pa, observation point is located at the distance r = 1m, the mass density of transversely isotropic material is ρ = 2000 kg/m3 and the elasticity tensor Ci jkl are given in the Voigt notation as follows ⎡

CT I

5.82 2.11 1.44 ⎢ 5.82 1.44 ⎢ ⎢ 4.1 ⎢ =⎢ ⎢ ⎢ ⎣ symm.

0 0 0 1.25

0 0 0 0 1.25

⎤ 0 0 ⎥ ⎥ ⎥ 0 ⎥ ⎥ × 108 Pa. 0 ⎥ ⎥ 0 ⎦ 1.855

(29.16)

29 Comparison of Two Numerical Inverse Laplace Transform Methods …

357

Fig. 29.1 Test functions a u(t), b w(t)

For convenience we work with dimensionless variables and quantities CT I = CT I p2 p12 / p3 , ρ = ρp23 / p3 , Pmax = Pmax p12 ( p2 p3 ), r = r/ p2 , t = t/ p1 , (29.17) p1 = 0.018 s, p2 = 1 m, p3 = 1 kg.

(29.18)

To avoid complicated procedure associated with dealing with the singularities of integrands [13] and to get meaningful error estimation around Rayleigh pole we introduce a small artificial damping into the elasticity tensor of the material as C = CT I (1 + 0.005i).

(29.19)

Under these considerations test functions u(t) and w(t) are depicted in Fig. 29.1.

29.3 Durbin’s Method We start with rewriting (29.1) as F(s) =

+∞ 0

+∞ e−αt = 0

+∞ −αt e−(α+iω)t f (t)dt = e (cos(ωt) − sin(ωt)) f (t)dt 0 0 ⎛ +∞ ⎞ f (t) cos(ωt)dt + i ⎝− e−αt f (t) sin(ωt)dt ⎠ = Re(F(s))

e−st f (t)dt =

+∞

0

+iIm(F(s)), (29.20)

+∞ Re(F(s)) = Re(F(α + iω)) = e−αt f (t) cos(ωt)dt, 0

(29.21)

358

I. Markov and L. Igumnov

+∞ Im(F(s)) = Im(F(α + iω)) = − e−αt f (t) sin(ωt)dt.

(29.22)

0

Recalling +∞ +∞ −αt e f (t) cos(−ωt)dt = e−αt f (t) cos(ωt)dt Re(F(α − iω)) = 0

0

= Re(F(α + iω)),

(29.23)

+∞ +∞ −αt Im(F(α − iω)) = − e f (t) sin(−ωt)dt = e−αt f (t) sin(ωt)dt 0

0

= −Im(F(α + iω)).

(29.24)

Rewriting (29.2)

f (t) =

1 2πi

α+i∞

est F(s)ds = α−i∞

1 2πi

+∞ e(α+iω)t F(s)idω −∞

+∞ 1 eαt (cos(ωt) + i sin(ωt))F(s)idω = 2πi −∞

eαt = 2π eαt = 2π eαt = 2π

+∞ (cos(ωt) + i sin(ωt))F(s)dω −∞

+∞ (cos(ωt) + i sin(ωt))[Re(F(s)) + iIm(F(s))]dω −∞

+∞ [Re(F(s)) cos(ωt) − Im(F(s)) sin(ωt)]dω −∞

eαt + i 2π

+∞ [Re(F(s)) sin(ωt) + Im(F(s)) cos(ωt)]dω. −∞

Expanding imaginary part in (29.25)

(29.25)

29 Comparison of Two Numerical Inverse Laplace Transform Methods … +∞ −∞

359

[Re(F(s)) sin(ωt) + Im(F(s)) cos(ωt)]dω

=

0

[Re(F(s)) sin(ωt) + Im(F(s)) cos(ωt)]dω

−∞ +∞

+

(29.26)

[Re(F(s)) sin(ωt) + Im(F(s)) cos(ωt)]dω,

0

and now using (29.21) and (29.22) we get for the first integral in (29.26) 0 −∞

[Re(F(s)) sin(ωt) + Im(F(s)) cos(ωt)]dω

= =

0 +∞ 0 +∞

− =

[Re(F(α + i(−ω))) sin(−ωt) + Im(F(α + i(−ω))) cos(−ωt)](−dω) [Re(F(α + iω))(− sin(ωt)) − Im(F(α + iω)) cos(ωt)](−dω)

0

+∞ 0

[Re(F(α + iω)) sin(ωt) + Im(F(α + iω)) cos(ωt)](−dω)

[Re(F(α + iω)) sin(ωt) + Im(F(α + iω)) cos(ωt)]dω

+∞ +∞

=−

[Re(F(s)) sin(ωt) + Im(F(s)) cos(ωt)]dω.

0

(29.27) It follows from (29.26) and (29.27) that the imaginary part in (29.25) is zero. Applying (29.21) and (29.22) to the real part in (29.25) we get the equivalent representation of (29.2): +∞ [Re(F(α + iω)) cos(ωt) − Im(F(α + iω)) sin(ωt)]dω, t ≥ 0.

eαt f (t) = π

0

(29.28) Durbin’s method (or sometimes also called the Fourier Series Method) consists of representing f (t) as ∞ − 21 Re(F(α)) + cos kπ Re F α + i kπ t T T k=1 ∞ kπ − sin T t − Derr , 0 < t < 2T, Im F α + i kπ T

f (t) =

eαt T

(29.29)

k=0

where Derr is the discretization error due to approximation of the integral by the Fourier series. Since infinite series in (29.29) can only be summed up to a finite number Nsum of terms, the approximating formula for f (t) is

360

I. Markov and L. Igumnov αt f (t) ≈ f˜(t) = eT − 21 Re(F(α)) N sum kπ kπ ! kπ kπ + Re F α + i T cos T t − Im F α + i T sin T t ,

(29.30)

k=0

for 0 < t < 2T. Durbin derived formula (29.29) using a Fourier series expansion of e−αt f (t) on the time interval [0, 2T ], which is formally equivalent to the application of the trapezoidal rule to (29.28) with the integration step size equal π/T . Aside from roundoff and discretization error in Durbin’s formula (29.30), there is the truncation error since the series is not summed up to infinity. When the maximum of imaginary parts of complex frequencies is given as ωmax , the Nsum is then determined as ωmax T . = π

Nsum

(29.31)

Assuming that tmax is the largest value of time range over which f˜(t) is obtained, then T is chosen so that 2T > tmax or T = T ∗ tmax , T ∗ > 0.5.

(29.32)

Slightly modifying the idea of Crump [4], α is chosen from the following relation α=

κ ln 10 κ ln 10 = ∗ . T T tmax

(29.33)

With (29.32) and (29.33) the input parameters in Durbin’s method are ωmax and tmax , the free parameters are κ and T ∗ . We start with presenting in Figs. 29.2, 29.3, 29.4 and 29.5 contour plots of Rerr (κ, T ∗ ) for inverted vertical displacements w(t) ˜ for two values of dimensionless time tmax = 0.5 and tmax = 1.0 and four different values of ωmax : 500, 2000, 4000, 15000. Vertical displacements are chosen since they seem to

˜ ωmax = 500 and a tmax = 0.5, b tmax = 1.0 Fig. 29.2 Contour plots of Rerr (κ, T ∗ ) for w(t),

29 Comparison of Two Numerical Inverse Laplace Transform Methods …

361

˜ ωmax = 2000 and a tmax = 0.5, b tmax = 1.0 Fig. 29.3 Contour plots of Rerr (κ, T ∗ ) for w(t),

˜ ωmax = 4000 and a tmax = 0.5, b tmax = 1.0 Fig. 29.4 Contour plots of Rerr (κ, T ∗ ) for w(t),

˜ ωmax = 15000 and a tmax = 0.5, b tmax = 1.0 Fig. 29.5 Contour plots of Rerr (κ, T ∗ ) for w(t),

present stricter error bounds than u(t). ˜ Numbers along the contour lines mean how min many times the error Rerr (κ, T ∗ ) along each line is greater than minimal value Rerr ∗ obtained for a given range of parameters κ and T . General observations following from Figs. 29.2, 29.3, 29.4 and 29.5 are that for each tmax there is a different κmin (ωmax ) that for all κ < κmin Durbin’s method produce exponentially growing error Rerr regardless of T ∗ and therefore of sampling points count Nsum . Value of κmin increases with increasing maximum value ωmax of

362

I. Markov and L. Igumnov

imaginary parts of complex frequencies. For the values κ > κmin levels of Rerr roughly correspond to the straight lines T ∗ (κ) defined for a fixed values of α. It is impossible to formulate universal relationship Rerr (κ, T ∗ ) for all possible values of ωmax and tmax . Frequently employed rule of a thumb is to choose κ in the range 2 ≤ κ ≤ 3 and it seem to provide adequate balance between accuracy and number of sampling points for T ∗ ≥ 0.75. It should be emphasized, that for increasing value of κ, value of T ∗ should also increase for a given accuracy, which corresponds to the error analysis presented by Durbin in [3]. This is demonstrated in Fig. 29.6 for tmax = 0.5, T ∗ = 1.0 and κ = 2.0, 2.5, 3.0 and 4.0. For the fixed T ∗ , starting from a certain value of κ, increasing it, and therefore α, leads to the rapid deterioration of the error Rerr with increasing of ωmax since roundoff and truncation errors are amplified by the eαt /T . In Fig. 29.7 inverted solutions u(t) ˜ and w(t), ˜ obtained by Durbin’s method with parameters tmax = 0.5, ωmax = 2000, T ∗ = 1.0, κ = 2.0, (Nsum = 319, α ≈ 9.21), are compared with the reference solutions u(t) and w(t). Corresponding pointwise absolute errors Aerr are depicted in Fig. 29.8. As it can be expected, points near the Rayleigh peak have the most deviation from the reference solutions. Gibb’s oscillations are present due to the truncation of integration range and usually are suppressed

Fig. 29.6 Error Rerr with T ∗ = 1.0 and tmax = 0.5 for a u(t), ˜ b w(t) ˜

Fig. 29.7 Comparison between reference and inverted solutions for a u(t), b w(t)

29 Comparison of Two Numerical Inverse Laplace Transform Methods …

363

Fig. 29.8 Pointwise absolute error Aerr for a u(t), b w(t)

using a data windowing technique [14, 15]. But in course of our experiments we tried several window functions (Blackman, Hanning, Lanczos and Riesz) and found that application of a data filter leads to severe undershooting around Rayleigh peak. Additionally we have tried to use Wynn’s epsilon method [4–6, 16] to accelerate the convergence of the series in Durbin’s method and found that for complicated functions like u(t) and w(t), performance of the epsilon algorithm heavily depends on a proper choice of ωmax , which is impossible to make beforehand.

29.4 Convolution Quadrature Method CQM was originally developed [8, 9] to numerically approximate convolution integrals t f (t) = y(t) ∗ g(t) =

y(t − τ )g(τ )dτ ,

(29.34)

0

as follows [10] f (nt) =

n "

ψn−k ( y¯ )g(kt), n = 0, Nt ,

(29.35)

k=0

where y¯ is the Laplace transform of y(t), t is the time step, Nt is the number of time steps. Now let F(s) denote the Laplace transform of f (t) with f (t) = 0 for t < 0. Consider the following convolution integral f (t) = L

−1

{F(s)} = L

−1

# # $ $ 1 −1 −1 1 s F(s) = L {s F(s)} ∗ L s s

364

I. Markov and L. Igumnov

= L −1 {s F(s)} ∗ H (t),

(29.36)

where H (t) is the Heaviside step function. Employing Backward Differential Formula of order two as an underlying time stepping method, we present slightly modified CQM to approximate convolution integral (29.36) f (mt) ≈ f˜(mt) =

n "

ψn−k (s F(s))H (kψ) =

k=0

n "

ψk (s F(s)),

(29.37)

k=0

tmax mt Nψ , Nψ ≥ Nt , ,n = (29.38) m = 0, Nt , t = Nt tmax ⎡ ⎤ π 2π −k R R −k s(φ)F(s(φ))e−ikφ dφ = Re⎣ s(φ)F(s(φ))e−ikφ dφ ⎦, ψk (s F(s)) = 2π π 0

0

(29.39) iφ 2 iφ 3 γ Reiφ Nψ Re iφ s(φ) = , , γ Re = − 2Re + tmax 2 2

(29.40)

where 0 < R < 1 is the free parameter of the method, tmax is the largest value of time range over which f˜(t) is to be obtained, Nψ is also the free parameter of the method. Suppose we are restricted by the maximum value ωmax > 0 of the imaginary parts of sampling frequencies s(φ). To determine value φmax corresponding to value ωmax , so that |Im(s(φmax ))| = ωmax , we first solve the following the equation ∂Im γ Reiφ = 0, ∂φ

(29.41)

to establish maximum value of |Im(s(φ))| and compare it to ωmax since imaginary part of the characteristic function γ Reiφ has only one local extremum in [0, π ]. Expanding (29.41) we get ∂Im γ Reiφ = −2R cos(φ) + R 2 cos(2φ) = 2R 2 (cos(φ))2 − 2R cos(φ) ∂φ − R 2 = 0, (29.42) % ∗

φ = φ = arccos

1−

& 2R 2 + 1 . 2R

√

(29.43)

If |Im(s(φ ∗ ))| > ωmax then we solve the following equation for the value φmax

29 Comparison of Two Numerical Inverse Laplace Transform Methods …

tmax ωmax Im(s(φmax )) = −ωmax or Im γ Reiφmax = − or Nψ −2R sin(φmax ) +

1 2 tmax ωmax , 0 < φmax < φ ∗ < π, R sin(2φmax ) = − 2 Nψ

365

(29.44) (29.45)

which we can solve using any suitable numerical root-finding method. If |Im(s(φ ∗ ))| ≤ ωmax then we set φmax = π. To evaluate integral in (29.39), we discard the part of the integral where φ > φmax φmax R −k ψk (s F(s)) = s(φ)F(s(φ))e−ikφ dφ 2π 0 ⎡ ⎤ φmax −k R = Re⎣ s(φ)F(s(φ))e−ikφ dφ ⎦, π

(29.46)

0

and use trapezoidal rule with L equal subintervals φmax /L for the rest '%

L s φ p F s φ p e−ikφ p p=0 ( s(0)F(s(0))+s(φmax )F(s(φmax ))e−ikφmax , − 2

ψk (s F(s)) =

φmax R −k Re πL

(29.47)

with φ p = φmax p/L . To make comparison with Durbin’s method easier we require that L satisfies the same relationship as Nsum L=

ωmax T π

=

ωmax T ∗ tmax , π

(29.48)

where T ∗ > 0 is the free parameter. Following [10], R can be determined from the relation 1

R = ε 2( Nψ +1) ,

(29.49)

where ε is problem dependent and usually 10−20 < ε < 10−1 . With (29.48) and (29.49) the input parameters in the CQM are same as in Durbin’s method, namely ωmax and tmax , the free parameters are Nψ , T ∗ and ε. Because of higher number of free parameters and the intertwined nature of their relationships in the CQM, it is difficult to produce explicit recommendations for choosing optimal values of the free parameters even for this particular problem. We performed a considerable number of numerical experiments and there are our general observations. For a fixed value of T ∗ the relative error Rerr significantly depends on Nψ and less on

366

I. Markov and L. Igumnov

ε. For the problem under consideration choosing 10−8 < ε < 10−2 yields acceptable results for a large range of ωmax and tmax . For a fixed value of ε again the relative error greatly depends on Nψ , which in turn depends on ωmax . The relationship seems to be similar to dependence of κ on ωmax in Durbin’s method – the greater ωmax the bigger Nψ should be. Error depends on value of T ∗ much less. Basically, values of T ∗ greater than 0.75 do not noticeably improve accuracy. For the large values of Nψ and therefore small value of φmax , taking ε = 10−2κ , where κ is the free parameter of Durbin’s method, leads to the sampling frequencies defined in (29.40) with real parts roughly the same as defined in (29.33). Overall, largest pointwise absolute errors are located around peaks. In Fig. 29.9 and 29.10 we present solutions u(t) ˜ and w(t) ˜ inverted with CQM with parameters tmax = 0.5, ωmax = 2000, T ∗ = 1.0, ε = 10−4 , Nψ = 5 · 105 (L = 319, Re(s(φ)) ≈ 9.21) and corresponding pointwise absolute errors Aerr . Results obtained with the CQM and depicted in Figs. 29.9 and 29.10 are very close to the results obtained with Durbin’s method. In Fig. 29.11 we compare the errors Rerr obtained with the CQM and Durbin’s method for 500 ≤ ωmax ≤ 30,000. The shared free parameters are tmax = 0.5 and T ∗ = 1.0, also κ = 3.0 for Durbin’s method and ε = 10−2κ = 10−6 , Nψ = 1 · 106 for the CQM. With this choice of

Fig. 29.9 Comparison of CQM inverted solutions and reference solutions for a u(t), b w(t)

Fig. 29.10 Pointwise absolute error Aerr with CQM for a u(t), b w(t)

29 Comparison of Two Numerical Inverse Laplace Transform Methods …

367

Fig. 29.11 Comparison of Durbin’s method and CQM for a u(t), ˜ b w(t) ˜

parameters both methods produce the same number of sampling frequencies for each ωmax . Until ωmax ≈ 11,000 both methods demonstrate very close accuracy.

29.5 Conclusions Both considered methods for numerical inversion of Laplace transforms are almost identical accuracy-wise with a right choice of free parameters. The Durbin’s method have only two free parameters and choosing their values is much more straightforward, while CQM have three free parameters and choosing their optimal values can be rather complicated. Overall CQM does not seem to provide any special features or present any apparent advantages over Durbin’s method in the problems such as considered. Acknowledgements The work is financially supported by the Russian Science Foundation under grant No. 18-79-00082.

References 1. C.Y. Wang, J.D. Achenbach, Elastodynamic fundamental solutions for anisotropic solids. Geophys. J. Int. 118(2), 384 (1994) 2. C.Y. Wang, J.D. Achenbach, Three-dimensional time-harmonic elastodynamic Green’s functions for anisotropic solids. Proc. R. Soc. A 449(1937), 441 (1995) 3. F. Durbin, Numerical inversion of Laplace transforms: An efficient improvement to Dubner and Abate’s method. Comput. J. 17(4), 371 (1974) 4. K.S. Crump, Numerical inversion of Laplace transforms using a Fourier series approximation. J. ACM 23(1), 89 (1976) 5. F. de Hoog, J. Knight, A. Stokes, An improved method for numerical inversion of Laplace transforms. SIAM J. Sci. Stat. Comput. 3(3), 357 (1982) 6. G. Honig, U. Hirdes, A method for the numerical inversion of Laplace transforms. J. Comput. Appl. Math. 10(1), 113 (1984)

368

I. Markov and L. Igumnov

7. X. Zhao, An efficient approach for the numerical inversion of Laplace transform and its application in dynamic fracture analysis of a piezoelectric laminate. Int. J. Solids Struct. 41(13), 3653 (2004) 8. C. Lubich, Convolution quadrature and discretized operational calculus. I. Numer. Math. 52(2), 129 (1988) 9. C. Lubich, Convolution quadrature and discretized operational calculus. II. Numer. Math. 52(4), 413 (1988) 10. M. Schanz, Wave Propagation in Viscoelastic and Poroelastic Continua: A Boundary Element Approach (Springer, Berlin, Heidelberg, 2001), 170p 11. C.L. Pekeris, The seismic surface pulse. Proc. Natl. Acad. Sci. 41(7), 469 (1955) 12. M. Eskandari-Ghadi, S. Sattar, Axisymmetric transient waves in transversely isotropic halfspace. Soil Dyn. Earthq. Eng. 29(2), 347 (2009) 13. H.G. Georgiadis, D. Vamvatsikos, I. Vardoulakis, Numerical implementation of the integraltransform solution to Lamb’s point-load problem. Comput. Mech. 24(2), 90 (1999) 14. J. Xiao, W. Ye, L. Wen, Efficiency improvement of the frequency-domain BEM for rapid transient elastodynamic analysis. Comput. Mech. 52(4), 903 (2013) 15. M. Schanz, W. Ye, J. Xiao, Comparison of the convolution quadrature method and enhanced inverse FFT with application in elastodynamic boundary element method. Comput. Mech. 57(4), 523 (2016) 16. P. Wynn, On a device for computing the em(Sn) transformation. Math. Tables Other Aids Comput. 10(54), 91 (1956)

Chapter 30

Twofold Re-reflections of Ultrasonic Waves from Obstacles in a Two-Dimensional Elastic Material, Taking into Account Any Laws of Their Reflections and Transformations Nikolay V. Boyev Abstract In this chapter, the problem of the diffraction of ultrasonic waves by cavity obstacles in an infinite two-dimensional elastic medium with double reflections is studied. A short pulse is introduced into the elastic medium with tonal filling with several periods of a plane high-frequency, monochromatic longitudinal or transverse elastic wave. Double re-reflections of waves with any possible reflections (longitudinal wave to longitudinal, transverse to transverse waves) and transformations (longitudinal waves to transverse, transverse waves to longitudinal) are considered. The integral representations of the displacements in the reflected waves are written out on the basis of the physical theory of Kirchhoff diffraction. An asymptotic estimate of multiple diffraction integrals using the multidimensional stationary phase method gives an explicit form of the geometrical optical approximation of displacements in doubly reflected and transformed waves.

30.1 Introduction High-frequency waves are used in ultrasonic testing of elastic materials to detect possible accumulations of cavity defects, solid and elastic inclusions, and also to study the properties of metamaterials. In the propagation of high-frequency waves in clusters of obstacles, both multiple re-reflections of waves and their transformation on the boundary contours of obstacles are possible. A numerical study of the problems of short-wavelength diffraction of elastic waves is significantly complicated if the wavelength is much less than the average size of the obstacle. In connection with this circumstance, obtaining and applying explicit analytical expressions for the characteristics of the wave field in the framework of the geometric theory of diffraction (GTD) is an urgent task. The filtration properties of the metamaterial, which is an elastic matrix of hardened epoxy resin and containing a three-period system of N. V. Boyev (B) Southern Federal University, 105/42 Bolshaya Sadovaya Str., Rostov-on-Don, Russia 344006 e-mail: [email protected] © Springer Nature Switzerland AG 2020 I. A. Parinov et al. (eds.), Advanced Materials, Springer Proceedings in Materials 6, https://doi.org/10.1007/978-3-030-45120-2_30

369

370

N. V. Boyev

hard balls, were studied experimentally [1] in a wide frequency range. A theoretical justification of these properties was obtained [2] in the acoustic approximation. The study of single and double scattering of short acoustic waves is the subject of [3–5]. A complete study of the features of the passage of high-frequency waves through clusters of obstacles in elastic media can be carried out on the basis of GTD methods taking into account all kinds of multiple reflections and transformations of elastic waves. In this paper, we consider all the laws of double reflections and transformations of short waves in a two-dimensional elastic medium containing obstacles in the form of cavities.

30.2 Problem Statement In an infinite two-dimensional elastic medium there is a cluster of cavity obstacles. An unsteady short pulse of a special structure propagating in an elastic medium was chosen as a dynamic effect on the accumulation of defects. The pulse is filled with 6–12 periods of a plane high-frequency monochromatic elastic wave. The diffracted waves that passed through with any possible reflections and transformations can be received in any region of the elastic medium. The task consists in a complete analytical study in the framework of GTD of all possible sequences of double reflections and transformations of elastic waves at the boundary contours of obstacles due to the fact that they form the basis for obtaining explicit expressions of the characteristics of the wave field for any laws of multiple reflections and wave transformations.

30.3 Solution Method The tonal filling of the short pulse introduced into the obstacle cluster with a sufficient number of periods (6–12 periods) of the monochromatic wave allows us to study the task in the mode of harmonic oscillations. In this case, the incident wave is a superposition of point sources of circular waves. During discretization, each circular wave is replaced by a system of radial propagation rays of the elastic wave and only those rays that are directed toward the obstacles and interact with them are taken into account. Thus, the problem reduces to solving the problem of shortwavelength diffraction of elastic waves, taking into account their re-reflections and transformations in a local setting.

30 Twofold Re-reflections of Ultrasonic Waves from Obstacles …

371

30.4 Study of the Problem in a Local Formulation At point x˜0 of an infinite elastic two-dimensional medium, there is a pulsating point source of a circular monochromatic wave generated by a concentrated force Qe−iωt , where ω is the oscillation frequency. We consider the directions q of wave propagation oriented on the boundary contour l of an obstacle or an accumulation of obstacles located in the elastic plane. In this case, the displacements at the point y˜ of the elastic plane caused by the point source are determined by the Kupradze matrix [6]. The goal is to study the amplitude characteristics of the scattered field at the contours of obstacles, taking into account all possible options for twofold reflections and transformations of elastic waves. In the directions q and q1 at y˜ , we have asymptotic representations of the amplitudes of displacements in the incident wave: Q q k 2p qi = 4μ ks2

2 −i π e 4 πkp Q 2 −i π q 1 uq(s)1 (y) = q1 i e 4 4μ π ks

uq( p) (y)

1 eik p R0 1+O , Q q = (Q, q), (30.1) √ k p R0 R0 1 eiks R0 1+O , Q q1 = Q, q1 . √ k R R0 s 0

(30.2)

Here, the tangential direction q1 is perpendicular to the direction of wave q propagation. Q q and Q q1 are projections of the force Q on the directions q1 and q. In Formulae (30.1), (30.2) and below, ρ is the density, λ, μ are the Lame coefficients, k p = ω/c p , ks = ω/cs , c p and c S are the wave numbers and velocities of the longitudinal and transverse waves. The components of the displacement vector of a wave reflected once from a free boundary contour at a point x˜ of the elastic plane are determined by the following integral [7]: ˜ = u k (x)

T y [U(k) ( y˜ , x)] ˜ · u( y˜ )dl, k = 1, 2,

(30.3)

l

∂U(k) + λn div U(k) + μ n × rot U(k) , T y U(k) ( y˜ , x) ˜ = 2μ ∂n

(30.4)

where the Kupradze matrix U(k) ( y˜ , x) ˜ is obtained from the matrix U(k) ( y˜ , x˜0 ) by ˜ T y is the force vector at the point y˜ ; u( y˜ ) replacing x˜0 by x˜ and R0 by R = | y˜ − x|; is the vector of the total displacement field on the boundary surface; n is the external normal to the contour l directed toward the elastic medium. In the vectors of total elastic displacement on the boundary contour and in the vector T y at the point y˜ , we select the terms determined by the longitudinal ( p-wave) and transverse (s-wave) waves.

372

N. V. Boyev

u k (x) ˜ =

T y [U(k) ˜ , x)] ˜ + T y [Us(k) ( y˜ , x)] ˜ · u( y˜ ; p) + u( y˜ ; s) dl y p (y

l

u k (x) ˜ =

T y [U(k) ˜ , x)] ˜ · u( y˜ ; p)dl y + p (y

l

+ l

(30.5)

T y [Us(k) ( y˜ , x)] ˜ · u( y˜ ; p)dl y

l

T y [U(k) ˜ , x)] ˜ · u( y˜ ; s)dl y + p (y

T y [Us(k) ( y˜ , x)] ˜ · u( y˜ ; s)dl y

(30.6)

l

The first and last terms in Formula (30.6) describe the p–p and s–s reflections, and the second and third terms p–s and s–p of the transformation. Direct use of the integral representation of displacements (30.3) over the entire “light” zone for an obstacle in the form of a cavity describes only once-reflected waves. In [3–5], for a two-dimensional and three-dimensional problems in the case of a single reflection, an asymptotic solution is constructed that is local in nature and gives a geometrical optical approximation of the diffracted field amplitude in a small neighborhood of any ray emerging from a point x˜0 reflected from the boundary contour of an obstacle at a point y˜ ∗ and arriving at the point x˜ of reception of the elastic medium.

30.5 Double Re-reflection of Elastic Waves from the Plane Contours of Obstacles, Taking into Account Possible Transformations Double reflection of the wave can occur both from the contour of one non-convex obstacle, and from two obstacles, including a non-convex shape. Obtaining explicit expressions of the displacement amplitude in re-reflected and transformed waves based on the use of geometric considerations and Keller GTD divergence coefficients [8]. In the short-wavelength diffraction problem, taking into account multiple reflections and transformations on obstacles in an elastic medium, it is more convenient, in our opinion, to proceed from integral representations of the Kirchhoff physical theory of diffraction [8]. For the asymptotic estimation of the arising diffraction multiple integrals of rapidly oscillating functions, it is possible to use the multidimensional stationary phase method. Note that the integral Formula (30.3) gives only a once reflected wave. For repeatedly reflected waves, the application of the integral representation (30.3) is possible only in the modification [9]. Following this modification, doubly reflected and transformed waves at the receiving point will be found by repeated integration of the rays successively over the neighborhoods l1∗ and l2∗ of the mirror reflection points y˜1∗ and y˜2∗ , respectively. The applied modification [9] of the integral representation (30.3) means that when finding the leading term of the asymptotics of the double diffraction

30 Twofold Re-reflections of Ultrasonic Waves from Obstacles …

373

integral, we will be in the framework of calculating the displacement amplitude in the wave twice reflected with possible transformations according to the GTD. We consider the re-reflection of a high-frequency wave using the example of re-reflection of a ray x˜0 − y˜1∗ − y˜2∗ − x˜3 emitted from a point x˜0 [p-wave (30.1)] and received at a point x˜3 with a possible twofold transformation p–s–p. The components of the p-wave displacement vector at the receiving point x˜3 are given by the following formula: ( p)

u k (x˜3 ) =

T y2 U(k) ˜2 , x˜3 ) · u( y˜2 ; s)dl2 . p (y

(30.7)

l2∗

Here u( y˜2 ) is the vector of complete displacement at the point y˜2 ∈ l2∗ of the neighborhood of the point y˜2∗ , which is determined after the first p–s transformation on the neighborhood l1∗ of the reflection point y˜1∗ . In the asymptotic estimate of the Kirchhoff integral in (30.7), the components of the vector of the total displacement field u k ( y˜2 ), k = 1, 2 under the sign of the integral should be chosen as a solution to the local diffraction problem of reflection of a plane incident s-wave [10], formed with p–s transformation on the neighborhood l1∗ of the reflection point y˜1∗ . u 1 ( y˜2 ; s) = Vss ( y˜2 ) − 1 − tgγ1 Vsp ( y˜2 ) u (s) ˜2 ), 1 (y kp ks2 u 2 ( y˜2 ; s) = Vss ( y˜2 ) + 1 + 1 − 2 sin2 γ1 Vsp ( y˜2 ) u (s) ˜2 ), 2 (y ks sin γ1 kp

(30.8)

where Vss ( y˜2 ) and Vsp ( y˜2 ) are the reflection coefficients s–s and s–p of the transformation [11]. ˜2 ), k = 1, 2 At the same time, the components of the displacement vector u (s) k (y in Formula (30.8) themselves are expressed by a similar formula: ˜2 ) = u (s) k (y

T y1 Us(k) ( y˜1 , y˜2 ) · u( y˜1 ; p)dl1 ,

(30.9)

l1∗

where the vector of the total displacement field u( y˜1 ; p) (30.9) at points y˜1 ∈ l1∗ of the neighborhood of y˜1∗ should be chosen as a solution to the local diffraction problem of reflection of a plane incident p− wave (30.1) [10]:

k 2p ks2

( p)

ks u 1 ( y˜ ; p) = 1 + V pp ( y˜ ) − k p sin 1 − sin2 γ V ps ( y˜ ) u 1q ( y˜ ), γ ( p) u 2 ( y˜ ; p) = 1 − V pp ( y˜ ) − tgγ V ps ( y˜ ) u 2q ( y˜ ),

(30.10)

where V pp and V ps are the reflection coefficients p–p and p–s of the transformation ( p) ( p) ( p) [10], and u 1q ( y˜ ) and u 2q ( y˜ ) are the components of the displacement vector uq ( y˜ )

374

N. V. Boyev

in the incident p-wave (30.1). After substituting (30.10) in (30.9) and (30.9) in (30.8) and (30.8) in (30.7) and moving to the local polar coordinate system r , θ at the specular reflection point y˜2∗ , we arrive at the components of radial displacement at the point x˜3 : 2 π Qq k p k k ( p) 2ks πk2 s 2kps − 2kps e−i 4 u r (x˜3 ) = − 4πμ ks ik φ ×V ps y˜1∗ Vsp y˜2∗ e p psp dl1 dl2 , l2∗

cos √ γ1 cos γ3 L0 L1 L2

(30.11)

l1∗

( p)

u θ (x˜3 ) = 0, φ psp = |x˜0 − y˜1 | + kksp | y˜1 − y˜2 | + | y˜2 − x˜3 |, L 0 = x˜0 − y˜ ∗ , L 1 = y˜ ∗ − y˜ ∗ , L 2 = y˜ ∗ − x˜3 . 1

1

2

(30.12)

2

At points of direct specular reflection y˜1∗ ∈ l1∗ and y˜2∗ ∈ l2∗ , we assign the neighborhoods of these points to Cartesian coordinate systems O1 X 1(1) X 2(1) and O2 X 1(2) X 2(2) defined by the normals n1 = O1 X 2(1) , n2 = O2 X 2(2) and tangent to the contour of the obstacle. Along the contours from the points y˜1∗ and y˜2∗ , we count the lengths of the arcs s1 in the vicinity of l1∗ and s2 in the vicinity of l2∗ . For small s1 and s2 up to small second-order inclusive expressions for the first and third terms in phase ϕ psp have the following form: ( p) 1 cos γ1 −1 2 ( p) |x˜0 − y˜1 | = L 0 + s1 sin + L 0 cos γ1 + ( s1 )2 , (30.13) 2 ρ1 ( p) 1 cos γ2 ( p) −1 2 ( p) | y˜2 − x˜3 | = L 2 − s2 sin γ2 + L 2 cos γ2 + ( s2 )2 . (30.14) 2 ρ2 ( p) γ1

( p) ( p) For p–s–p transformation, − sin γ1 , − cos γ1 is the vector which deter (s) mines the direction of the p-wave (30.1), and − sin γ1 , cos γ1(s) is the direction (1) (1) ∗ of the the coordinate system O1 X 1 X 2 at the point y1 , reflected wave relatively (s) (s) is the vector determining the direction of incidence of and − sin γ2 , − cos γ2 (2) (2) the s-wave reflectedat point y1∗ with respect to the coordinate system O2 X 1 X 2 at ( p)

( p)

is the direction of the reflected p-wave at the point y˜2∗ ; while − sin γ2 , cos γ2 the point y˜2∗ . Let us find the term | y˜1 − y˜2 | = |˜y2 y˜ 1 | in the phase φ psp (30.12). The points (1) y˜1 ∈ l1∗ and y˜2 ∈ l2∗ in the local Cartesian coordinate systems O1 X 1(1) X 2 and 1) 2) and y˜2 − s2 , − ( s , where O2 X 1(2) X 2(2) have the coordinates y˜1 − s1 , − ( s 2ρ1 2ρ2 ρi are the radii of curvature of the boundary contours l1 and l2 of the two obstacles, respectively, at points y˜1∗ and y˜2∗ . The distance | y˜1 − y˜2 | is considered in the coordinate 2

2

30 Twofold Re-reflections of Ultrasonic Waves from Obstacles …

375

system O2 X 1(2) X 2(2) . In this system we denote the coordinates of the points coordinate y˜1 (ξ1 , η1 ), y˜2 (ξ2 , η2 ), y˜1∗ ξ10 , η10 . Taking this into account, we represent the vector y˜ 2 y˜ 1 in the form: y˜ 2 y˜ 1 = y˜ 2∗ y˜ 1∗ + A˜y∗1 y˜ 1 − y˜ 2∗ y˜ 2 ,

y˜ 2 y˜ 1 = {ξ1 − ξ2 , η1 − η2 }, y˜ 2∗ y˜ 1∗ = ξ10 , η10 .

(30.15)

Here A = ai j , i, j = 1, 2 is the orthogonal transition matrix from the basis of the Cartesian coordinate system O2 X 1(2) X 2(2) at the point y˜2∗ to the basis of the Cartesian coordinate system O1 X 1(1) X 2(1) at the point y˜1∗ . The matrix A has the form: A=

cos α − sin α . sin α cos α

(30.16)

In the local coordinate systems, the vectors y˜ 1∗ y˜ 1 and y˜ 2∗ y˜ 2 have coordinates 2 i) . Substituting the coordinates of all the vectors in relation y˜ i∗ y˜ i − si , − ( s 2ρi (30.15), one obtains:

1 2 | y˜1 − y˜2 | = (ξ1 − ξ2 )2 + (η1 − η2 )2 / 2 ( s1 )2 ξ10 − s1 cos α + = + s2 2ρ1 1/2 ( s1 )2 ( s2 )2 0 + η1 − s1 sin α − cos α + 2ρ1 2ρ2

(30.17)

Expanding the square root in powers of s1 and s2 on the right-hand side of (30.17), we obtain the following asymptotic representation of the distance up to small second-order inclusive: | y˜1 − y˜2 | = L 1 − s1 sin γ1(s) + s2 sin γ2(s) 1 cos γ1(s) −1 2 (s) + L 1 cos γ1 + ( s1 )2 2 ρ1 (s) 1 cos γ (s) 2 2 + L −1 ( s2 )2 1 cos γ2 + 2 ρ2 (s) (s) + L −1 1 s1 s2 cos γ1 cos γ2 .

Summing up the expressions |x0 − y1 |, ( p) γ1

= ks sin law k p sin phase ϕ psp (30.12):

γ1(s) ,

ks sin

γ2(s)

ks |y kp 1

(30.18)

− y2 |, |y2 − x3 | and using Snell’s ( p)

= k p sin γ2 , we write out the relation for

376

N. V. Boyev

ks φ psp = L 0 + L 1 + L 2 kp ( p) ( p) 1 cos2 γ1 ks cos2 γ1(s) cos γ1 ks cos γ1(s) + + + + ( s1 )2 2 L0 kp L1 ρ1 k p ρ1 ( p)

cos γ1(s) cos γ2 L1 ( p) ( p) 1 ks cos2 γ2(s) cos2 γ2 ks cos γ2(s) cos γ2 + + + + ( s2 )2 . 2 kp L1 L2 k p ρ2 ρ2 +

Phase ϕ psp does not contain terms with the first powers s1 and s2 . This suggests that the specular reflection points are stationary for phase ϕ psp . The leading term in the asymptotic behavior of the diffraction double integral (30.11) can be obtained using the two-dimensional stationary phase method [11]: u r( p) (x˜3 )

( psp)

Here D2

Qq k p 2 −i π cos γ1 cos γ3 e 4 √ × V ps y˜ ∗ Vsp y˜ ∗ =− μ ks π ks L0 L1 L2 ( psp) exp i k p L 0 + ks L 1 + k p L 2 + π4 δ2 −2 × ( psp) det D2

is the Hessian matrix: ⎛

( psp)

D2

( psp)

(30.19)

⎞

( p)

cos2 γ1 ks cos2 γ1(s) + L0 kp L1 ( p) cos γ1 ks cos γ1(s) + + ρ1 k p ρ1

⎜ ⎜ ⎜ ⎜ ⎜ ⎜ =⎜ ⎜ ⎜ ⎜ ⎜ cos γ1(s) cos γ2( p) ⎜ L1 ⎝

( psp)

( p)

cos γ1(s) cos γ2 L1

( p)

ks cos2 γ2(s) cos2 γ2 + kp L1 L2 ( p) ks cos γ2(s) cos γ2 + + k p ρ2 ρ2

⎟ ⎟ ⎟ ⎟ ⎟ ⎟ ⎟, ⎟ ⎟ ⎟ ⎟ ⎟ ⎠

and δ2 = sign D2 = ν + − ν − is the difference between the number of positive ( psp) + − ν and negative ν eigenvalues of the Hessian matrix D2 . Thus, in this subsection we obtain the leading term of the asymptotics (30.19) ( p) of the displacement amplitude u r (x˜3 ) in the reflected high-frequency longitudinal wave during p-s-p transformation from the surfaces of one or two obstacles located in an elastic medium in the two-dimensional case. Explicit expressions of the main terms of displacements in doubly re-reflected waves along the ray x˜0 − y˜1∗ − y˜2∗ − x˜3 in the remaining seven cases of various possible

30 Twofold Re-reflections of Ultrasonic Waves from Obstacles …

377

reflections and transformations of elastic waves, namely: p-p-p, p-p-s, p-s-s, s-s-s, s-s-p, s-p-s, s-p-p were obtained by the method described above.

30.5.1 Case of p-p-p Transformation ( ppp) exp i k p (L 0 + L 1 + L 2 ) + π4 δ2 −2 , u r( p) (x) ˜ = M ( ppp) √ ( ppp) L 0 L 1 L 2 det D2 ( p)

u θ (x) ˜ = 0, M ( ppp) = ⎛ ( ppp)

D2

=⎝

cos

2

( p) γ1

2 ! n=1

( ppp) ( ppp) V pp y˜n∗ cos γn( p) , δ2 = sign D2

( p)

2 cos γ 1 + L11 + ρ1 1 L0 ( p) ( p) cos γ1 cos γ2 L1

( p)

cos γ1

cos

2

( p) γ2

L1 1 L1

⎞

( p)

cos γ2

+

1 L2

+

( p)

2 cos γ2 ρ2

⎠.

(30.20)

30.5.2 Case of p-p-s Transformation

u (s) ˜ θ ( x)

( pps) exp i k p L 0 + k p L 1 + ks L 2 + π4 δ2 −2 = M pps , √ ( pps) L 0 L 1 L 2 det D2

kp ( p) ( pps) (s) ( pps) , ˜ = 0, M ( pps) = V pp y˜1∗ V ps y˜2∗ cos γ1 cos γ2 , δ2 = sign D2 u r(s) (x) ks ⎛ ⎞ ( p) ( p) (s) 2 cos γ1 cos γ1 cos γ2 2 γ ( p) 1 + 1 cos − 1 ⎜ ⎟ ( pps) L0 L1 ρ1 L1 D2 =⎝ ( p) ( p) ( p) (s) (s) (s) ⎠. cos γ1 cos γ2 cos2 γ2 ks cos2 γ2 cos γ2 ks cos γ2 + + + L1 L1 k p L2 ρ2 k p ρ2

(30.21)

30.5.3 Case of p-s-p Transformation This case was considered in detail above in the text.

378

N. V. Boyev

30.5.4 Case of p-s-s Transformation ( pss) exp i k p L 0 + ks L 1 + ks L 2 + π4 δ2 −2 , u (s) ˜ = M pss θ ( x) √ ( pss) L 0 L 1 L 2 det D2 kp ( pss) ( pss) , V ps y˜1∗ Vss y˜2∗ cos γ1(s) cos γ2(s) , δ2 = sign D2 ks ⎞ ⎛ ( p) cos2 γ1 ks cos2 γ1(s) + ⎟ ⎜ cos γ1(s) cos γ2(s) L0 L1 ⎟ ⎜ ( p) (s) L1 ⎟ ⎜ = ⎜ + cos γ1 + ks cos γ1 ⎟. (30.22) ⎟ ⎜ ρ ρ ⎠ ⎝ 1 2 (s) (s) (s) cos γ1 cos γ2 2 cos γ2 1 2 (s) 1 − cos γ + 2 L1 L1 L2 ρ2

u r(s) (x) ˜ = 0, M ( pss) =

( pss)

D2

30.5.5 Case of s-s-s Transformation

u (s) ˜ θ ( x)

=M

(sss)

(sss) exp i ks (L 0 + L 1 + L 2 ) + π4 δ2 −2 , √ (sss) L 0 L 1 L 2 det D2 2 !

˜ = 0, M (sss) = u r(s) (x) ⎛

2 (s) ⎜ cos γ1

D2(sss) = ⎝

(s)

(sss) (sss) , Vss y˜n∗ cos γn(s) , δ2 = sign D2

n=1 1 L0 (s)

cos γ1 cos γ2 L1

+

1 L1

+

(s)

⎞

(s)

cos γ1 cos γ2 2 (s) L1 cos γ1 2 cos γ2(s) L11

+

1 L2

+

(s)

2 cos γ2 ρ2

⎟ ⎠

(30.23)

30 Twofold Re-reflections of Ultrasonic Waves from Obstacles …

379

30.5.6 Case of s-s-p Transformation

( p) u r (x) ˜

=M

(ssp)

(ssp) exp i ks (L 0 + L 1 ) + k p L 2 + π4 δ2 −2 √ (ssp) L 0 L 1 L 2 det D2

kp ( p) (ssp) (ssp) , Vss y˜1∗ Vsp y˜2∗ cos γ1(s) cos γ2 , δ2 = sign D2 ks ⎞ ⎛ ( p) (s) (s) 2 cos γ cos γ1 cos γ2 cos2 γ1(s) L10 + L11 + ρ1 1 L 1 ⎠. =⎝ ( p) ( p) ( p) (s) (s) (s) cos γ1 cos γ2 cos2 γ2 k cos2 γ cos γ k cos γ + s ks L 2 2 + ρ22 + p ρ2 2 L1 L1

˜ = 0, M (ssp) = u (s) θ ( x) (ssp)

D2

(30.24)

30.5.7 Case of s-p-s Transformation

u (s) ˜ θ ( x)

=M

(sps)

(sps) exp i ks L 0 + k p L 1 + ks L 2 + π4 δ2 −2 , √ (sps) L 0 L 1 L 2 det D2

kp ( p) (sps) (s) (sps) , Vsp y˜1∗ V ps y˜2∗ cos γ1 cos γ2 , δ2 = sign D2 ks ⎞ ( p) (s) cos2 γ1 k p cos2 γ1 + ( p) (s) ⎟ cos γ1 cos γ2 L0 L1 ⎟ ( p) (s) ⎟ L1 cos γ1 k p cos γ1 ⎟ + + ⎟ ⎟ ρ1 k s ρ1 (30.25) ( p) ( p) ⎟ 2 2 k p cos γ2 cos γ2 ⎟ ⎟ + ( p) (s) ⎟ cos γ1 cos γ2 ks L 1 L2 ⎟ ( p) (s) L1 k p cos γ2 cos γ2 ⎠ + + k s ρ2 ρ2

˜ = 0, M (sps) = u r(s) (x) ⎛

(sps)

D2

⎜ ⎜ ⎜ ⎜ ⎜ ⎜ =⎜ ⎜ ⎜ ⎜ ⎜ ⎝

380

N. V. Boyev

30.5.8 Case of s-p-p Transformation

( p) u r (x) ˜

=M

(spp)

(spp) exp i ks L 0 + k p (L 1 + L 2 ) + π4 δ2 −2 , √ (spp) L 0 L 1 L 2 det D2

( p)

˜ = 0, M (spp) = u θ (x) ⎛ (spp) D2

=⎝

(s)

kp ( p) ( p) (spp) (spp) Vsp y˜1∗ V pp y˜2∗ cos γ1 cos γ2 , δ2 = sign D2 ks ( p)

cos2 γ1 k cos2 γ + p L1 1 L0 ( p) ( p) cos γ1 cos γ2 L1

+

(s)

cos γ1 ρ1

+

( p)

k p cos γ1 k s ρ1

( p)

cos γ1

⎞

( p)

cos γ2 L1 ( p) 1 cos2 γ2 L1

+

1 L2

−

( p)

2 cos γ2 ρ2

⎠

(30.26)

30.6 Conclusion Thus, the main term of the asymptotics (30.19)–(30.26) of the displacement amplitude in a high-frequency longitudinal or transverse wave twice reflected along the x˜0 − y˜1∗ − y˜2∗ − x˜3 ray for an arbitrary sequence of reflections and transformations from one or two obstacles in an elastic medium in the two-dimensional case is obtained in the work. The amplitude of movement in the reflected elastic wave (30.19)–(30.26) is determined by the distances from the wave source to the first point y˜1∗ of the specular reflection L 0 , from the second point of the specular reflection y˜2∗ to the receiving point L 2 , and the distance L 1 between points y˜1∗ and y˜2∗ . Points y˜1∗ and y˜2∗ can belong both to the boundaries of two isolated obstacles and to the boundary l of one obstacle of complex non-convex shape. The main term of the asymptotics of displacement also explicitly contains the radii of curvature ρi of the boundary contours l1 and l2 of two obstacles, respectively, at points y˜1∗ and y˜2∗ of the direction of incident and reflected waves at points of specular reflection and coefficients of reflection and transformation. The phase of the reflected wave (30.19)–(30.26) is determined by the distances L 0 , L 1 , L 2 , wave numbers k p and ks , the sign of the Hessian matrix, and also the number of points of specular reflection.

References 1. Z. Liu, X. Zhang, Y. Mao, Y. Zhu, Z. Yang, C.T. Chan, P. Sheng, Science 289, 1734 (2000) 2. N.V. Boyev, M.A. Sumbatyan, in Wave Dynamics and Composite Mechanics for Microstructured Materials and Metamaterials, vol. 59, ed. by M.A. Sumbatyan (Springer, Heidelberg, 2017), p. 173 3. V.M. Babich, V.S. Buldyrev, Asymptotic Methods in Short-Wavelength Diffraction Theory (Alpha Science, New York, 2008)

30 Twofold Re-reflections of Ultrasonic Waves from Obstacles …

381

4. N.V. Boyev, in Wave Dynamics and Composite Mechanics for Microstructured Materials and Metamaterials, vol. 59, ed. by M.A. Sumbatyan (Springer, Heidelberg, 2017), p. 91 5. M.A. Sumbatyan, N.V. Boyev, J. Acoust. Soc. Am. 95(5), 2347 (1994) 6. V.D. Kupradze, Potential Methods in the Theory of Elasticity (Israel Program for Scientific Translations, Jerusalem, 1965) 7. V. Novatsky, Theory of Elasticity (Mir, Moscow, 1975). (in Russian) 8. H. Hyunl, A. Maue, K. Westpfal, Theory of Diffraction (Mir, Moscow, 1964). (in Russian) 9. V.A. Borovikov, B.Y. Kinber, Geometrical Theory of Diffraction (The Institution of Electrical Engineers, London, 1994) 10. L. Brekhovskikh, Waves in Layered Media (Academic Press, New York, 2012) 11. M.V. Fedorjuk, Saddle Point Method (Nauka, Moscow, 1977). (in Russian)

Chapter 31

On the Use of Models of the Tymoshenko Type in the Analysis of Wave Processes in Wedge-Shaped Waveguides Aleksandr Vatulyan and Lyubov Parinova

Abstract Wave processes in topographic waveguides are studied. A wedge-shaped waveguide with a triple cross-section is considered. Hypotheses for variable stiffness plates are taken into account. Dispersion dependencies for two orthotropic materials for a model of the Timoshenko type using the variational Hamilton-Ostrogradsky principle and the Ritz approximate calculation method are constructed. The results are compared with those obtained in the study of the Kirchhoff model. A mathematical software Maple was used for computational experiments.

31.1 Introduction The solution of the problems on the propagation of elastic waves traveling along the edge of a topographic waveguide is relevant in seismology, microelectronics, flaw detection and acoustics. The study of the kinematics of such waves can be used to develop new non-destructive testing methods and to create effective delay lines and filters. For the first time, wave processes in wedge-shaped topographic waveguides were studied in the 1970–80s in [1, 2]. The finite element method was used to study wave processes in a wedge-shaped waveguide at an arbitrary opening angle. In the same period the conditions for the existence of symmetric and antisymmetric vibration modes in a wedge-shaped waveguide were found using the generalized variational principle [3]. In the twenty-first century, the existence of wedge waves was rigorously proved in [4, 5]. The existence of waves in some types of topographic waveguides was proved in [6]. The most interesting case is a waveguide with a small aperture angle. While the use of approximate models based on models of oscillations of plates of variable stiffness is very fruitful. Approximate models were constructed in [7– 10] and antisymmetric vibration modes in topographic waveguides for orthotropic materials were studied taking into account the properties of the Kirchhoff model. A. Vatulyan · L. Parinova (B) I. I. Vorovich Mathematics, Mechanics and Computer Sciences Institute, Southern Federal University, Rostov-on-Don, Russia e-mail: [email protected] © Springer Nature Switzerland AG 2020 I. A. Parinov et al. (eds.), Advanced Materials, Springer Proceedings in Materials 6, https://doi.org/10.1007/978-3-030-45120-2_31

383

384

A. Vatulyan and L. Parinova

The purpose of this work is to study the propagation features of wave processes in wedge-shaped topographic waveguides of finite height based on more complex models of plates of variable stiffness, for example, the model of the Tymoshenko type, to obtain dispersion relations, to compare the results with the dependences obtained previously.

31.2 Formulation of Problem The natural vibrations of an orthotropic topographic waveguide with a cross-section in the form of a triangle with a small angle 2α at the apex of height h are considered. An elastic wave propagating along the edge of a wedge-shaped structure is studied. We assume that a Cartesian coordinate system O x1 x2 x3 is connected with the waveguide. The x3 -axis is directed perpendicular to the plane of the section S and passes through the apex of the angle of an isosceles triangle, not lying at the base. The base of the waveguide x1 = h is pinched. The remaining faces of the waveguide are free of loads. The solution to the problem for a topographic wedge-shaped waveguide is sought in the form of traveling waves: u 1 (x1 , x2 , x3 , t) = U1 (x1 , x2 ) cos(γ x3 − ωt) u 2 (x1 , x2 , x3 , t) = U2 (x1 , x2 ) cos(γ x3 − ωt) u 3 (x1 , x2 , x3 , t) = U3 (x1 , x2 ) sin(γ x3 − ωt) where γ is a wave number, ω is the oscillation frequency, Um (x1 , x2 ), m = 1, 2, 3 are amplitudes of propagating waves. Next, dimensionless parameters are entered: C11 C22 C33 C44 C12 , γ2 = , γ3 = , γ4 = , γ5 = , C55 C55 C55 C55 C55 C66 C23 C13 ρω2 h 2 γ6 = , γ7 = , γ8 = , = β, γ 2 h 2 = μ, C55 C55 C55 C55 γ1 =

where Ci j are elastic moduli of an orthotropic medium, ρ is density. As in [7–10], the problem of the propagation of an elastic wave along the edge of a wedge-shaped waveguide is reduced to finding the stationary value of some quadratic functional M: M[Ui ] = M0 dS (31.1) S

where the integrand has the form:

31 On the Use of Models of the Tymoshenko Type …

385

M0 = (γ1 U1,1 + γ5 U2,2 + γ8 U3,3 )U1,1 + (γ5 U1,1 + γ2 U2,2 + γ7 U3,3 )U2,2 + (γ8 U1,1 + γ7 U2,2 + γ3 U3,3 )U3,3 + γ6 (U1,2 + U2,1 )2 + (U1,3 + U3,1 )2 + γ4 (U2,3 + U3,2 )2 − β (U12 + U22 + U32 ) The condition of stationarity of the functional δ M[Ui ] = 0 leads to the solution of a homogeneous boundary-value problem with two parameters. We find such a relationship between these parameters μ and β, for which the variational equation has a nontrivial solution.

31.3 The Model of the Timoshenko Type Plate Oscillations of a symmetric region are divided into two problems, such as symmetric and antisymmetric oscillations. The studied types of motions are usually absent for the symmetric case. Therefore, to find a solution to the problem, the antisymmetric case is considered. It is assumed that the components of the displacement amplitudes Ui (x1 , x2 ) satisfy the following relation parity and oddness coordinate relations x2 : U1 (x1 , −x2 ) = −U1 (x1 , x2 ) U2 (x1 , −x2 ) = U2 (x1 , x2 ) U3 (x1 , −x2 ) = −U3 (x1 , x2 ) Generalized hypotheses are introduced due to the small opening angle α. These hypotheses are similar for the model of the Timoshenko type [11]: U1 = x2 W1 (x1 )

(31.2)

U2 = hW2 (x1 )

(31.3)

U3 = γ x2 hW3 (x1 )

(31.4)

Integration over x2 is made in the presentation of functional (1). New dimensionless variable: z = xh1 is introduced. A simplified value of functional (1) is found taking into account hypotheses (2–4). Thus, the task of studying localized waves for topographic wedge-shaped waveguides is reduced to the problem of finding the stationary value of the functional M: 1 M[W ] = 0

here

M0∗ dz

(31.5)

386

A. Vatulyan and L. Parinova

⎞ 1 3 2 2 2 2 2 z γ + t W + 2μγ W W + μ γ W + μ −W + W 1 8 3 3 1 1 1 3 3 ⎟ ⎜ M0∗ = ht ⎝ 3 ⎠ 2 −β W12 + μW32 + z γ6 W1 + W2 + γ4 μ(−W2 + W3 )2 − βW22 ⎛

where t = tgα. The stationary value of the functional M[W ] is found by the approximate method. This method is based on the Ritz method. The solution W (z) is selected taking into account the requirements for coordinate functions from the class of functions bounded and satisfying the boundary conditions of rigid pinching at z = 1. We shall look for a solution in the form: W1 = (z − 1)2

N

an ϕn (z)

n=1

W2 = (z − 1)2

N

bn ϕn (z)

n=1

W3 = (z − 1)2

N

cn ϕn (z)

n=1

A system of functions φn (z) = z n−1 , n = 1, 2, . . . is selected as coordinate functions. Then functional (5) takes a quadratic form of 3N variables: 1 M(a1 , b1 , c1 , a2 , b2 , c2 , . . . a N , b N , c N ) =

M1 dz

(31.6)

0

where M1 = M1 (a1 , b1 , c1 , a2 , b2 , c2 , . . . a N , b N , c N ). As an example, we consider a special case for N = 2. After integrating (6) over z the functional transforms into a quadratic form of 6 variables: M(a1 , b1 , c1 , a2 , b2 , c2 ) = k11 a12 + k12 a1 b1 + k13 a1 c1 + k14 a1 a2 + k15 a1 b2 + k16 a1 c2 + k22 b12 + k23 b1 c1 + k24 b1 a2 + k25 b1 b2 + k26 b1 c2 + k33 c12 + k34 c1 a2 + k35 c1 b2 + k36 c1 c2 + k44 a22 + k45 a2 b2 + k46 a2 c2 + k55 b22 + k56 b2 c2 + k66 a62 where ki j = ki j (β, μ), i, j = 1 − 6 due to bulkiness are not given, for example: k11 =

1 1 1 1 γ6 + γ1 t 2 − βt 2 + μt 2 , 30 45 840 840

A linear homogeneous system is formed with respect to the coefficients ak , bk , ck , k = 1, 2, . . . , N , according to the condition of stationarity of the functional. The

31 On the Use of Models of the Tymoshenko Type …

387

determinant of the obtained system of linear equations is equal to zero. It turns out an approximate dispersion, namely algebraic equation that relates β and μ.

31.4 Computational Experiments When finding dispersion dependences, the convergence of the Ritz method was studied depending on the number of coordinate functions. Calculations are performed for barite materials with parameters [12]: γ1 = 3.154, γ2 = 2.799, γ3 = 3.720, γ4 = 0.419, γ5 = 1.710, γ6 = 3.154, γ7 = 1.036, γ8 = 0.964 and austenitic steel with parameters [12]: γ1 = 2.036, γ2 = 2.036, γ3 = 1.674, γ4 = 1.000, γ5 = 0.761, γ6 = 2.036, γ7 = 1.124, γ8 = 1.124 The graphs of dispersion dependencies were constructed in respect to the relative dependencies μ(β) for these materials (see Fig. 31.1). Dispersion dependencies are shown by red and blue colors for the cases N = 3 and N = 8, respectively. Table 31.1 shows the values μ for different values of the frequency parameter for different values of frequency parameter β for various number of coordinate functions.

Fig. 31.1 Plots of parametric dependences for barite (a) and austenitic steel (b) materials for the opening angle α = 3◦

388

A. Vatulyan and L. Parinova

Table 31.1 Values of μ for barite for wedge at α = 3◦ and N = 8 Mode No.

β

Number of coordinate functions N =5

First mode

Second mode

Third mode

N =6

N =7

N =8

1

82.191

82.819

82.894

82.902

2

157.664

163.749

165.441

165.759

3

223.703

239.666

246.317

248.241

4

282.151

309.584

324.084

329.673

5

334.870

373.974

398.009

409.315

6

383.178

433.645

467.983

486.616

1

13.557

13.789

14.052

14.149

2

41.518

41.696

41.875

41.906

3

63.365

64.410

64.787

64.805

4

82.696

85.710

86.661

86.777

5

100.622

106.112

108.122

108.511

6

117.379

125.676

128.219

130.127

3

5.714

8.879

9.184

9.590

4

23.282

27.845

28.029

28.417

5

36.946

42.730

43.103

43.534

6

48.532

55.434

56.220

56.751

The monotonic growth of the sought values is characteristic for the implementation of the Ritz method. For N = 8, stabilization of values is achieved at the calculating the parameter μ for the first three propagating modes. The relative difference in the values μ corresponding to N = 7 and N = 8 does not exceed 5%. The comparison of the results of the dependence μ on the parameter β for the model of the Timoshenko type and the previously studied Kirchhoff model [8, 9] is made for N = 4. Graphs of dispersion dependencies are shown in Fig. 31.2. The digits 1, 2, 3 show in Fig. 31.2 first, second, and third modes, respectively. The dots illustrate the results of calculations for the Kirchhoff model. The solid cirves show the results of calculations for the model of the Timoshenko type. We can note that the dispersion dependences for both models practically coincide for the first mode. The discrepancy is slightly larger for the second and third modes.

31 On the Use of Models of the Tymoshenko Type …

389

Fig. 31.2 Plots of dispersion dependencies for the Kirchhoff model and the model of Timoshenko type

Acknowledgements The performed study was funded by RFBR, project No. 19-31-90079.

References 1. E.A. Ash, R.M.D.L. Rue, R.F. Humphryes, IEEE Trans. Microw. Theory Tech. 17(11), 882 (1969) 2. P.E. Lagasse, I. M. Mason, E.A. Ash, IEEE Trans. Microwave Theory Tech. MTT-21, 225 (1973) 3. H.F. Tiersten, D. Rubin, in Proceedings of the IEEE Ultrasonics Symposium, 117 (1974) 4. G.L. Zavorohin, A.I. Nazarov, Notes Sci. LOMI 380, 45 (2010). (in Russian) 5. I.V. Kamockij, Algebra Anal. 20(1), 86 (2008) (in Russian) 6. V.M. Babich, Algebra Anal. 22(1), 98 (2010) (in Russian) 7. A.O. Vatulyan, L.I. Parinova, Vestn. DGTU 5(4), 491 (2005) (in Russian) 8. A.O. Vatulyan, L.I. Parinova, in Advanced Materials—Techniques, Physics, Mechanics and Applications, ed. by I.A. Parinov, S.-H. Chang, M.A. Jani, Springer Proceedings in Physics, vol. 193 (Springer Cham, Heidelberg, 2017), 309 9. A.O. Vatulyan, L.I. Parinova, Univ News North-Caucasus Reg Nat Sci 3, 10 (2018). (in Russian) 10. L.I. Parinova, in Advanced Materials Proceedings of the International Conference on “Physics and Mechanics of New Materials and Their Applications”, PHENMA 2018, ed. by I.A. Parinov, S.-H. Chang, Y.-H. Kim, Springer Proceeding in Physics vol. 224 (2019), 487 11. R.D. Nedin, A.O. Vatulyan, I.V. Bogachev, Math. Methods Appl. Sci. 41(4), 1600 (2018) 12. V.S. Blistanov, V.S. Bondarenko, N.V. Peremolova et al., in: Acoustic Crystals, ed. by M.P. Shaskol’skaya (Nauka, Moscow, 1982), 632 p. (in Russian)

Chapter 32

Construction of the Mechanical Model of Keratoprosthesis of the Ocular Cornea Arkadiy Soloviev, Nadegda Glushko, Alexander Epikhin and Michael Swain

Abstract By developing ocular prostheses, a number of problems arise, one of which is the design of the connection between the rigid optical part and the soft tissue of the cornea; their Young’s modules can differ by three orders of magnitude. In this case, the problem arises of creating some intermediate layer, possibly with gradient properties, the purpose of which is to exclude injury to soft biological tissues. An analytical and finite element modeling of the interaction of a cylindrical optical prosthesis, an intermediate heterogeneous layer and the cornea, in the framework of elastic media, in two versions: (i) without taking into account curvature (round plate) and (ii) taking into account curvature (spherical dome or shell), was performed. In a simplified model, the intermediate layer is represented as a spring layer, the determination of the rigidity of which will allow one to create an original design. Based on the proposed models, the stress-strain state of soft biological tissues was calculated.

32.1 Introduction A keratoprosthesis is a cell-free artificial implant consisting of central optics held in a cylindrical frame. Keratoprosthesis replaces the removed part of the cornea. When developing keratoprostheses, scientists faced many difficulties, and many of the early corneal transplants had high rates of infection and rejection. In the late 1980s, a “coreand-skirt” device in which a bio-integrated “skirt” surrounds central optics became the most common design. Important parameters were not only the size, but also the location of the pores in the porous skirt. Keratoprostheses, such as AlphaCor, A. Soloviev (B) · N. Glushko Department of Theoretical and Applied Mechanics, Don State Technical University, Rostov-on-Don, Russia e-mail: [email protected] A. Epikhin Don State Medical University, Rostov-on-Don, Russia M. Swain Sydney University, Sydney, Australia © Springer Nature Switzerland AG 2020 I. A. Parinov et al. (eds.), Advanced Materials, Springer Proceedings in Materials 6, https://doi.org/10.1007/978-3-030-45120-2_32

391

392

A. Soloviev et al.

formerly known as Chirila keratoprostheses, were a polymethylmethacrylate device with a central optical region fused to the surrounding spongy skirt. Modern keratoprostheses consist of an optical element and a support plate. The optical element is mainly in the form of a cylinder or lens, consists of an optically transparent material. The base plate connected to the optical element may have various forms: the shape of a ring with holes or a “wheel with spokes”, can be made in the form of “ears” or “amoeba-shaped legs”. The book [1] provides descriptions of various types and forms of both mounts and keratoprostheses themselves. The main complication after keratoprosthetics is aseptic necrosis of the cornea that occurs in front of the implant support. It is a complication that quite often leads to rejection of the keratoprosthesis [1]. The main reason for the occurrence of aseptic necrosis is the blocking of the flow of vital substances into the layers of the cornea, which are located above the keratoprosthesis support. In this regard, for the manufacture of a support plate, it is necessary to use a biocompatible material that would allow corneal tissue to grow through the support mount. The patent [2] describes a microporous keratoprosthesis base plate made of stretched polytetrafluoroethylene (PTFE), the structure of which has a configuration in the form of polymer nodes that are connected by fibrils with a length of 7–8 µm. Based on the data, PTFE with a fibrillar structure has too small pores, which does not allow corneal tissue to grow. Therefore, it is necessary to additionally penetrate it with pores perpendicular to the surfaces of the support plate with a diameter of 20–150 µm and preferably 50 µm. The thickness of the base plate should be about 0.2 µm, but not more than 0.3 µm. In patent [3] a keratoprosthesis is described, consisting of an optical element and a support fixture made in the form of a ring. The optical element is made of an optically transparent substance, such as polymethylmethacrylate (PMMA), and the support mount is made of a hydrophilic porous material having a fibrous structure that can grow through the corneal tissues. A support plate with a thickness of 0.15– 0.30 µm is formed from said fiber; with an outer diameter of the ring of about 9.5 mm, is worn on an optical element, the front of which is made in the form of a cylinder. The part directed inside the eye has the shape of a truncated cone, a larger section of which is directed inward. The backing plate has “elastic characteristics necessary to prevent keratoprosthesis rejection and necrosis resulting from pressure from surrounding eye tissue. In patent [4], the keratoprosthesis support plate is made in the form of two parallel shells spaced 0.4–0.7 µm apart. The optimal distance is 0.3 ± 0.02 mm; the shells are slightly conical in shape and are attached to the cylindrical optical element. The material of the support plates should be “bio-populated”, therefore, it is assumed that the shells should be made of a material with a porosity of 50% and higher, the pores should be open and their diameter should be about 20–100 µm. The patent [5] describes a keratoprosthesis (Fig. 32.1), consisting of a support plate and an optical element. The base plate is made in the form of a convex-concave lens with a radius of curvature of 7–10 mm In each individual case, the radius of curvature of the base plate is selected in accordance with the radius of curvature of the cornea of the patient, which is determined using hard contact lenses or in another

32 Construction of the Mechanical Model of Keratoprosthesis …

393

Fig. 32.1 Scheme of keratoprosthesis [5]

way. In the part adjacent to the optical element, the support plate has a thickness of 0.3–0.7 mm, tapering at the edges to a thickness of about 0.01 mm. The outer diameter of the support plate can be 7–12 mm, depending on the individual diameter of the cornea of the patient’s eye. In the center, the support plate has a cylindrical hole necessary for attaching the optical element. The optical element is in the form of a cylinder, the outer end (directed from the eye) of which is always convex, and the inner end, depending on how many diopters the optical element is designed for, can be flat or slightly convex. The optical element is made of polymethyl methacrylate or polycarbonate. It is possible to perform optical elements in 40–60 diopters. Also, the optical element of the keratoprosthesis under consideration can be collapsible. In this case, a screw thread is applied along the lateral surface of the cylinder. The prosthesis is additionally equipped with a washer having an internal screw thread. The washer is connected (glued) with its outer side to the inner surface of the cylindrical hole of the base plate. A keratoprosthesis can be implanted into the intralamellar pocket of the cornea, while the support plate is located inside the cornea of the eye, and the optical element penetrates all layers of the cornea. The patent [6] describes an implant for strengthening the cornea, which is made in the form of a round or oval plate having the shape of a trefoil, chamomile, or in the form of a convex-concave lens, which has a radius of curvature of 7–10 mm. The lens may have a cylindrical hole in the center, which can be used for subsequent keratoprosthetics. The structure of the material from which the implant is made has a volume fraction of void space of 15–40%, a specific surface space of voids of 0.25– 0.55 µm2 /µm3 , an average distance between voids of 25–50 µm, and an average volume chord of 8–25 µm. The inventive implant is a convex-concave lens having a radius of curvature corresponding to the radius of curvature of the cornea of the patient. In the central part, the implant has a thickness of 0.3–0.7 mm, descending along the edges to 0.01 mm. The patent [7] describes the effectiveness of treatment using the method of surgical treatment of cataracts using keratoprosthetics as an implant with a support base of permeable-porous titanium nickelide, which copies the curvature of the eye and supports a cylindrical optical element located in its central hole. The support base is mounted on the surface of the cornea and is retentively fixed by the scleral allograft, which is superimposed on top of the lamellar support base. The support base has the following parameters. The variable thickness of the plate support base with its

394

A. Soloviev et al.

gradual increase to the hole located in the center, allows one to fix the optical element, made in the form of a cylinder, without an additional mounting sleeve, as well as a threaded connection, which is technically simple and operationally reliable. A simple and reliable way to fix the support base of the optical element in the hole is a tight fit. It is possible to produce it with a negative difference between the diameters of the hole and the actual bore diameter of the optical cylinder. A tight fit (the nature of the connection of parts) in the “hole-shaft” system is carried out in metals due to the elastic deformation of the material. Titanium nickelide is subject to deformation according to the law of elastic deformation, which is several times larger than the elastic deformation of metals. This is what makes it possible to insert a keratoprosthesis (a lightweight and precision construction) with the least mechanical effort, which reduces the possibility of technological defects and errors. The rough surface of the hole in the slice of the porous material prevents the migration of the optical element in the absence of additional fixing elements. The reliability of the fastening of the optical element is also enhanced by a decrease in porosity, as well as a predominant pore size near the hole, in the result of an increase in the mechanical strength of the material in the central part of the base, which carries the main load. The absolute values of pore size and porosity are selected taking into account the conditions for the optimal integration of porous titanium nickelide and body tissues: such as the cornea of the eye, on the one hand, and the allograft, on the other hand. Fast and successful integration of a porous implant (basis) with surrounding tissues, mechanically strong fixation of the optical element, i.e. a reduction in the risk of keratoprosthesis reposition is regarded as an increase in effectiveness in treating a cataract. In patent [8], attention is drawn to the fact that the support part of the implant in shape and area should provide maximum resistance to the buoyant effect of intraocular fluid pressure on the optical part of the keratoprosthesis, while minimizing the deformation of the proper tissue. The material of the supporting part should not only be biocompatible, but also structured in such a way that to be able to ensure fusion of the above and the underlying layers of the cornea, which are separated during the keratoprosthesis implantation. The author notes that keratoprostheses are known, including an optical element made of an optically transparent substance, for example, PMMA, and a ring-shaped support plate made of a hydrophilic porous material of polytetrafluoroethylene or polyethylene [3, 4], whose merit is the possibility of fusion over and supporting layers of the cornea due to the high porosity of the material from 50% and above, and pore diameters up to 100 µm. The main drawback of the designs is excessive flexibility and low mechanical strength. These characteristics do not allow for a long time to reliably hold and fix the installed keratoprosthesis with large optics. The combined keratoprosthesis described in the patent consists of an optical part, which is made of a transparent solid or elastic polymer saturated with ultraviolet adsorbent. It is a removable bolt with a diameter of 5–6 mm, having a mushroom-shaped front end and spherical and/or aspherical surfaces of the ends and a thread on the side surface of the haptic part, made in the form of a support disk with an outer diameter of 8–12 mm, the thickness of which can vary from 0.3 to 0.9 mm. It is made of porous and/or perforated solid and/or elastic reactive polymer

32 Construction of the Mechanical Model of Keratoprosthesis …

395

and/or metal with a volume fraction of void space no more than 50%. The haptic part includes two parts: (i) from the front, it consists of biological materials; (ii) from the back, it includes artificial biocompatible materials. The supporting disk of the rear part is made plane and connected perpendicularly to the centrally located supporting hollow cylinder by means of a groove and/or flange formed on the outer rear part of the cylinder. The cylinder is equipped with an internal thread, which corresponds to the profile and diameter of the thread of the optical bolt. In this case, the support disk can pass into the cover sleeve, which wraps around the support cylinder from the outside. The support plate in front is connected to a round bio-disk, which is cut from freshly taken or preserved sterile biological materials of different layered combinations of biological tissues. For this, parts of the keratoprosthesis are sterilized before joining. The connection is carried out under sterile conditions, immediately before the implantation of a keratoprosthesis or in advance with subsequent storage before surgery. The external diameter of the bio-disk is made larger than the external diameter of the supporting disk by 0.3–1 mm, a coaxial hole is made in the center of the bio-disk, the diameter of which must correspond to the outer diameter of the cover sleeve or supporting cylinder. In this work, we consider a keratoprosthesis, which has an optical element (first area is white) of a cylindrical shape and there is a certain intermediate layer on the cylindrical surface with mechanical properties inhomogeneous in radius. Semiaxial sections of the keratoprosthesis are shown in Fig. 32.2, (a) without taking into account the curvature and (b) taking into account the curvature of the cornea, a layer with functionally gradient properties is highlighted in gray (second area) and the cornea (third area—is the region with points). This layer is designed to provide non-traumatic contact of optics with soft tissues of the cornea. Analytical and numerical models of keratoprosthesis implantation into the cornea based on FEM are constructed. The stress-strain state of the cornea in the contact area was investigated.

Fig. 32.2 Semi-axial section, plate model (a), domes (b)

396

A. Soloviev et al.

32.1.1 Research Purpose The stress-strain state of the cornea is studied in the vicinity of the contact with the keratoprosthesis, the outer layer of which is a certain structure that allows one to reduce soft tissue injury. This intermediate (interface) layer is modeled by a hollow cylinder with functionally gradient mechanical properties.

32.1.2 Research Scope At this study, we consider the following frameworks of the problem: (i) (ii) (iii) (iv)

(v)

an analytical model of an implanted prosthesis based on the bending a composite circular plate; FEM model of an implanted prosthesis based on a composite circular plate; FEM model of an implanted prosthesis based on a composite spherical dome; FEM model of the cornea based on a circular plate, in which the interface layer is replaced by the spring type conditions for joining with an absolutely rigid optical part; FEM model of the cornea based on a spherical dome, in which the interface layer is replaced by the spring type conditions for joining with an absolutely rigid optical part.

32.2 Research Method 32.2.1 Continuous Formulation of the Problem The general mathematical formulation of the problem under study consists of the boundary-value problem of the theory of elasticity for a composite isotropic body, two of which are homogeneous cylindrical optical prostheses and corneas, with elastic moduli Er1 and Er3 , and the interface layer has a functionally gradient elastic modulus Er2 = Er2 (r). The right side is fixed on the left side, symmetry conditions are set, a uniformly distributed pressure acts on the lower border, which corresponds to an excess intraocular pressure compared to atmospheric pressure, continuity conditions are set at the interface. The system of differential equations for unknown components of the displacement vector u = (u 1 , u 2 , u 3 ) is presented as [9] σi j, j = 0, σi j = ci jkl εkl − α p δi j , εkl =

1 u k,l + u l,k 2

(32.1)

32 Construction of the Mechanical Model of Keratoprosthesis …

397

where σi j , ci jkl , εkl are the components of the tensors of stresses, elastic constants, deformations, respectively. The boundary conditions are set for the displacement and stress vectors on the corresponding surfaces Su and St : u i | Su = u i0 (x, t), x ∈ Su

(32.2)

ti | St = σi j n j | St = q(x, t), x ∈ St

(32.3)

where nj are the coordinates of the unit vector of external normal. In the case of modeling the second section by spring boundary conditions at the interface boundary S int with continuous displacements, the condition is the set σn = −k u n , where k is a certain stiffness coefficient, characterizing the elastic properties of the second section. To study model (i), boundary-value problem (1–3) reduces to a system of ordinary differential equations (4–6) for the first, second, and third sections, respectively, relatively to θ (r ) being the angle of rotation of the unit vector of normal with a power law of changing the elastic modulus of the second section along radius [10]: d2 d 1 2 θ1 (r ) r − θ1 (r ) = K 1lqr 3 θ1 (r ) r + (32.4) dr 2 dr 2 2 d d d 2 θ2 (r ) r + a θ2 (r ) r + aϑ2 θ2 (r ) + θ2 (r ) r − θ2 (r ) dr 2 dr dr 2 1 K 2 q r − r12 r 2−a = (32.5) 2 r 2 d d 1 2 r r − θ3 (r ) = K 3 3q r 2 − r22 r θ (32.6) θ + (r ) (r ) 3 3 2 dr dr 2

where K i = 1/Di , Di is the cylindrical stiffness i = 1, 2, 3. The general solution of the system of (4–6) is constructed 1 C1 K 1lqr 3 + 16 r √ √ 1 1 1 1 2 2 at second section: θ2 (r ) = r − 2 a+ 2 a −4aϑ2 +4 C4 + r − 2 a+ 2 a −4aϑ2 +4 C3 1 K 2 qr 1−a r 2 − r12 ϑ2 − r 2 + 3rl 2 a − 8rl 2 + 2 (8 + (ϑ2 − 3)a)a(ϑ2 − 1) at first section: θ1 (r ) = rC2 +

at third section: θ3 (r ) = where

1 C5 + rC6 − K 3 3q 4 ln(r )r22 − r 2 r r 16

(32.7)

398

A. Soloviev et al.

Er2 = Er1

r a 1

r

,

Di =

Eri h i3

Er1 Er3 r ln r2 1

r ln 1

, Er2 = Er1 r 12 1 − ϑi2

( )

Arbitrary constants C i are determined from the boundary conditions at the right end and the matching conditions, moreover C 1 = 0.

32.3 Results and Discussion Numerical modeling was carried out in the finite element software ACELAN [11, 12], the components of the stress-strain state in problem (ii) are presented in Figs. 32.3, 32.4, 32.5 and 32.6. The Characteristics of the stress-strain state in problem (iv) are presented in Figs. 32.7 and 32.8.

Fig. 32.3 Finite element grid (a), displacement vector distribution (b)

Fig. 32.4 Dependence of elastic modulus on radius (a), distribution of radial stresses (b)

32 Construction of the Mechanical Model of Keratoprosthesis …

399

Fig. 32.5 Dependence of radial stresses on radius on the upper border (a), and on the interface with cornea (b)

Fig. 32.6 Dependence of angular stresses on radius on the upper border (a), and on the interface with cornea (b)

The characteristics of the stress-strain state in problem (iii) are presented in Figs. 32.9, 32.10, 32.11 and 32.12. The characteristics of the stress-strain state in problem (v) are presented in Figs. 32.13, 32.14 and 32.15.

400

A. Soloviev et al.

Fig. 32.7 Distribution of radial stresses along radius (a), dependence of radial stresses on radius on left boundary (b)

Fig. 32.8 Distribution of angular stresses (a), dependence of angular stresses on the left boundary (b)

32.4 Conclusion The keratoprosthesis models are considered, the feature of which is the presence of an intermediate layer between a rigid optical prosthesis and the soft tissues of cornea. This intermediate layer may provide non-traumatic contact. Several models (analytical and finite element) of a prosthesis implanted in the cornea were built. The components of a stress-strain cornea at the contact region are calculated. The present analysis of the stress results will determine the stiffness of the intermediate layer and, in accordance with this, propose its design.

32 Construction of the Mechanical Model of Keratoprosthesis …

Fig. 32.9 Finite element grid (a), displacement vector distribution (b)

Fig. 32.10 Distribution of radial stresses in the region (a), at the interface with cornea (b)

Fig. 32.11 Distribution of angular stresses in the region (a), at the interface with cornea (b)

401

402

A. Soloviev et al.

Fig. 32.12 Distribution of shear stresses in the region (a), at the interface with cornea (b)

Fig. 32.13 Distribution of radial stresses in the region (a), at the interface with cornea (b)

Fig. 32.14 Distribution of angular stresses in the region (a), at the interface with cornea (b)

32 Construction of the Mechanical Model of Keratoprosthesis …

403

Fig. 32.15 Distribution of shear stresses in the region

Acknowledgements This research was supported by the Government of Russian Federation (grant no. 14.Z50.31.0046).

References 1. S.N. Fedorov, Z.I. Moroz, V.K. Zuev, Keratoprosthetics. Moscow, Medicine, 144 p. (1982) (in Russian) 2. Patent US 5713956 A, IPC A61F2/14 (1998) 3. Patent US 5489301, IPC A61F2/14 (1996) 4. Patent US 6106552, IPC A61F2/14 (2000) 5. V.E. D’yakov, Y.S. Astahov, R.T. Hapchaev, Y.A. Kortunov, L.M. Fedotova, Keratoprosthesis. Patent RU2270643C1 IPC A61F2/14 A61L27/56 (2006) (in Russian) 6. V.E. D’yakov, Y.S. Astahov, E.V. Bojko, N.A. Ushakov, R.T. Hapchaev, Y.A. Kortunov, L.M. Fedotova, The implant to strengthen the cornea, RU2270642C1 IPC A61F2/14 A61L27/56 (2006) (in Russian) 7. A.A. Berezovskaya, V.N. Hodorenko, I.V. Zapuskalov, V.E. Gyunter, Keratoprosthesis and method of surgical treatment of cataracts with its help, RU2367379C1 IPC A61F2/14 A61F9/07 (2009) (in Russian) 8. A.N. Epihin. Combined keratoprosthesis, RU2707646C1 IPC A61F9/07 A61F2/16 (2019) (In Russian) 9. V. Novackij, Theory of Elasticity. Moscow, Mir, 864 p. (1975) (in Russian) 10. S.V. Boyarshinov, Machine-Building Mechanics. Moscow, Mashinostroenie. 456 p. (1973) (in Russian) 11. A.V. Belokon, V.A. Eremeyev, A.V. Nasedkin, A.N. Solov’yev, J. Appl. Math. Mech. 64(3), 367 (2000) 12. A.V. Belokon, A.V. Nasedkin, A.N. Solov’yev. J. Appl. Math. Mech. 66(3), 481 (2002)

Chapter 33

Simulation of the Stress-Strain State of the Spline Joint of the Helicopter Tail Transmission M. I. Chebakov, S. A. Danilchenko, and E. M. Kolosova

Abstract In the present work, frictional contact interaction between the tip and the shaft of the tail transmission of the MI-26 helicopter is considered in the framework of the linear theory of elasticity. The geometrical dimensions of the joint elements are taken from the design documentation. To set the profile of the tooth section, the necessary parametric equations were derived. To solve the tasks set, the finite element method and the ANSYS software were used. The main attention in the calculations was paid to the study of contact pressure q and effective (equivalent) stresses σ e on the tip teeth surfaces that are in direct contact with the teeth of the cup. In accordance with one of the proposed ways to increase the operational life of the node under study, a thin coating with mechanical characteristics different from the teeth original material was designed placed on the contacting surface of the tip tooth. The stress-strain state of the node has been calculated for various geometrical and mechanical parameters of the coating.

33.1 Introduction There are some parts in mechanisms that operational life is sufficiently less than for others. Limited resource items primarily include the most loaded joints. Technological units, mentioned above, are braking systems, where due to the large magnitude of the friction forces work, to the presence of high sliding speeds of the contact surfaces and their significant heating, intensive wear of the brake pads occurs; helicopter tail transmission, in the shaft joints of which involute tooth gears are used. Such gears fail mainly due to crushing and wear of the working surfaces of the teeth. The interaction processes in the frictional contact area of the helicopter’s spline joint of the tail transmission are characterized by small amplitude relative vibrations and significant dynamic loads occurring in junction under operating conditions. M. I. Chebakov (B) · S. A. Danilchenko · E. M. Kolosova Southern Federal University, Rostov-on-Don, Russia e-mail: [email protected] M. I. Chebakov · S. A. Danilchenko Rostov State Transport University, Rostov-on-Don, Russia © Springer Nature Switzerland AG 2020 I. A. Parinov et al. (eds.), Advanced Materials, Springer Proceedings in Materials 6, https://doi.org/10.1007/978-3-030-45120-2_33

405

406

M. I. Chebakov et al.

Currently, various methods are used to reduce the wear of rubbing parts [1]. For example, the usage of lubricants and anti-friction materials that reduce friction [2– 4]. Also, one of the effective ways to increase the durability of working junctions is to modify the surfaces of the tribocontact including by hardening and coating them [5–8]. According to such approach the main difficulty is to obtain the optimal surface modification parameters for each particular joint. One way to solve this problem may be to assess the effect of various modification parameters on the stress-strain state of the joint. In theoretical terms, the problem of evaluating the stress-strain state of a heavily loaded tribo-conjugate assembly is reduced to solve the contact problem of the deformable solid mechanics. In spite of considerable advance in this field of knowledge, in practice, such problems require studying novel contact problems with complicated physical and mechanical properties in the contact area, calling in contemporary numerical-analytic and numerical only methods, integrated calculation and design methodology using finite element technologies, including the steps of creating finite element models, performing calculations and results estimation.

33.2 Formulation of the Transmission Spline Junction Contact Interaction Problem In the framework of linear theory of elasticity frictional contact interaction between the tip and the shaft of the tail transmission of the MI-26 helicopter is considered. The geometric dimensions of the connected elements are taken from the design documentation. To set the tooth cross-section profile, the necessary parametric equations were derived. To derive formulas the following involute parameters were used: m = 3 mm—engagement module, z = 27—number of gear teeth, α = 20◦ —profile angle of the original contour, h a∗ = 1—the height of the tooth head of the original contour, x ∗ = 0—displacement of the initial contour (worm cutter) when cutting a tooth, c∗ = 0.25—gear radial clearance, ri∗ = 0.38—the radius of the fillet of the tooth of the original contour (Fig. 33.1). An asterisk indicates the assignment of this linear quantity to the engagement modulus. Based on these data, auxiliary values were calculated: the radius of the pitch circle r = 0.5mz, tooth projections circle radius ra = r + m(x ∗ + h a∗ ), depressions teeth radius circle r f = r − m(x ∗ + h a∗ + c∗ ); μ = arcsin[r sin(π/2 + α)/ra ], β = π/2 − (α + μ), n = r sin β/ sin μ, k = m[h a∗ + c∗ − ri∗ (1 − sin α)]. As a result, we obtain parametric equations for the involute portion of the tooth (a − b)

33 Simulation of the Stress-Strain State of the Spline Joint …

407

Fig. 33.1 Cross-section tooth profile

where

,

, . Linear parameter U is varying from Umin = 0 (in point b), to Umax = ntgα + (k − mx ∗ )/ cos α(in point a) We also obtain the parametric equations of the tooth fillet portion (b − c):

where

, ,

. Angle parameter ϑ varies from ϑmin = α (in point b) to ϑmax = π/2(in point c). At the final step of calculation, the following checks were made: (1) at and ; 3) at point c, ; (2) at point b, point a, . The right side of the tooth profile is symmetrical to the left about the axis Oy, i.e.

and

408

M. I. Chebakov et al.

Fig. 33.2 Solid models of tip (a) and shaft (b) (axial section)

It is assumed that the shaft and tip are in perfect coaxial position. The end face of the shaft in the wider part is fixed in all directions, and a load in the form of the moment M is applied to the end face of the tip in the wider part, which causes rotation around its axis. Between the contacting surfaces of the teeth of the tip and the shaft, Coulomb friction with a coefficient k is set. Solid-state models of junction elements are shown in Fig. 33.2.

33.3 Finite-Element Simulation of Contact Interaction in Transmission Spline Junction To solve this problem, the finite element method and the ANSYS software package were used. To construct the finite element mesh, a ten-node tetrahedral elastic element SOLID187 was used. For better convergence and increased accuracy of calculations in accordance with the methodology for solving contact problems on the surfaces of the teeth of the shaft and tip, directly contacting each other, condensing of the finite element meshing was applied. To simulate contact interaction, the surfaces of the teeth of the tip and the shaft were coated with CONTA174 and TARGE170, respectively. The constructed finite element model of the junction is shown in Figs. 33.3 and 33.4.

33.4 Results To conduct numerical calculations, the following values of the mechanical characteristics of the materials were applied: for the tip—a material with Young’s modulus

33 Simulation of the Stress-Strain State of the Spline Joint …

409

Fig. 33.3 Finite-element models of tip (a) and shaft (b) (axial section)

Fig. 33.4 Finite-element meshing of the tip (a) and shaft (b) surfaces

E 1 = 2 × 105 MPa, Poisson’s ratio υ 1 = 0.3, density ρ 1 = 7850 kg/m3 ; for the shaft—a material with Young’s modulus E 2 = 3 × 105 MPa, Poisson’s ratio υ 2 = 0.28 and density ρ 2 = 7850 kg/m3 . The moment M applied to the tip was set to 5 × 104 N/m, the friction coefficient between the contacting teeth surfaces k = 0.15. The main attention in the calculations was given to the study of contact pressure q and effective (equivalent) stresses σ e on the surfaces of the teeth of the tip directly at contact with the teeth of the shaft. The results are given for one of the contacting surfaces, since with perfect alignment on all the teeth of the tip due to the uniformity of their geometry and the applied load, the results coincide. In a real junction, due to the volumetric design of the tail transmission and the complex connection scheme of its individual components during operation, it is not possible to achieve ideal alignment of the mating elements. In the individual transmission shafts, the axis of the tip and the cup deviate by an angle within 7 min

410

M. I. Chebakov et al.

(0.01°). To assess the effect of the misaligned arrangement of the spline joint elements on the stress-strain state, calculations were performed for cases when the axis of the cup has a horizontal deviation (rotation about the Oy-axis in Fig. 33.2a) or vertical (rotation about the Oz-axis in Fig. 33.2a) relative to the tip axis. Calculations show that the deviation of the axis of the shaft in the horizontal plane leads to a shift of the contact spot in the corresponding direction, while the contact pressure values change by no more than 4%, effective stresses by no more than 9% compared to those with the coaxial position. When the axis of the shaft deviates in the vertical plane, stress concentrators appear. The values of contact pressure and effective stresses in these spots increase by 42% and 25%, respectively. Further, in accordance with one of the proposed methods for increasing the service life of the test site on the contact surface of the tip tooth, a thin coating was modeled with mechanical characteristics different from the initial tooth material. It is assumed that the coating and tooth surface are rigidly joined. When setting the mechanical characteristics of the coating, the following condition was fulfilled: the elastic modulus of the E 3 coating should be higher than that of the material of the teeth of the tip, but not exceed the corresponding value for the teeth of the shaft. In order to estimate the effect of the elastic modulus and Poisson’s ratio for a coating with a thickness of 40 µm, contact pressure and effective stresses were calculated for various values of these characteristics. The results are shown in Table 33.1. It follows from the table that an increase in the elastic modulus and Poisson’s ratio leads to an increase in contact pressure and effective stresses on the surface of the coating, while the effective stresses on the boundary between the coating and the tooth edge practically do not change. It should be noted that a change in the Table 33.1 Maximum values of contact pressure and effective stress on the surface of the coating, as well as the effective stress at the interface between the coating and the tooth tip edge for various values of the elastic modulus and Poisson’s ratio of the coating Young’s modulus and Poisson’s ratio values of coating

Maximum contact pressure on the surface of the coating q, MPa

Maximum effective stress on the surface of the coating σ emax , MPa

Maximum effective stress in the interface of the coating and tooth σ emax , MPa

E 3 = 2.5 × 105 MPa, υ 3 = 0.25

533

936

205

E 3 = 2.5 × 105 MPa, υ 3 = 0.3

535

944

206

E 3 = 2.5 × 105 MPa, υ 3 = 0.35

537

956

207

E 3 = 3 × 105 MPa, υ 3 = 0.25

558

1066

206

E 3 = 3 × 105 MPa, υ 3 = 0.3

559

1092

206

E 3 = 3 × 105 MPa, υ 3 = 0.35

564

1095

207

33 Simulation of the Stress-Strain State of the Spline Joint …

411

Fig. 33.5 Dependences of maximum contact pressure (a) and effective stresses (b) on coating thickness of the coating surface

elastic modulus has a greater effect on the values of the calculated stresses than the Poisson’s ratio. To study the effect of the coating thickness on the stress-strain state, the contact pressure distributions and the effective stresses on the coating surface were compared, as well as the effective stresses at the interface between the coating and the tooth face on which it was applied. Using the obtained data, we plotted the dependence of the maximum contact pressure and effective stress on the coating surface, as well as the effective stress at the interface between the coating and the tooth edge (which is coated), from the coating thickness (Figs. 33.5, 33.6). The coating characteristics are given as following: E 3 = 3 × 105 MPa, υ 3 = 0.3, ρ 3 = 7850 kg/m3 .

33.5 Conclusions From the analysis of the results obtained, it follows that with perfect alignment of the shaft and tip and a large load, as well as taking into account the shape of the teeth, contact occurs in the middle of the surface of the tip tooth. In this case, the

412

M. I. Chebakov et al.

Fig. 33.6 Dependence of maximum effective stress σ e on coating thickness at the interface of coating and tooth

maximum values of contact pressure and effective stresses are reached at the point of intersection of the involute with the fillet, since this point is irregular. After estimation of the misaligned arrangement effect of the spline junction elements on the stressstrain state, it was found that deviation from the coaxial position in the vertical plane has a greater effect on the contact pressure and effective stresses on the tip tooth surface than the deviation in the horizontal plane. The study of the coating influence on the stress-strain state showed that with an increase in the elastic characteristics of the coating material, an increase in the contact pressure and effective stresses on the coating surface is observed. This is due to a decrease in contact area. The effective stresses at the boundary between the coating and the face of the tip tooth on which it is applied are practically unchanged. After assessing the thickness influence of the coating, it was found that with an increase in this parameter, a more uniform distribution of stresses occurs in the coating. Furthermore, this leads to a decrease in effective stresses both on the surface of the coating and on the boundary between the coating and the tooth edge, but the contact pressure increases in this case. Probably, this may be connected with a decrease in the influence of the material of the tip tooth, for which the value of the elastic modulus was set lower than that of the coating. The refinement of the developed model will allow us to solve contact problems for the components of the spline junction, taking into account the presence of coating on interacting surfaces. Based on the data obtained by such calculations, recommendations can be made on the choice of coating thickness for specific values of their physical and mechanical characteristics in order to optimize the stress-strain state of the assembly. Acknowledgements The research is carried out in accordance with the Federal Target Program “Research and Development in the Priority Areas of Development of the Russian Scientific and Technological Complex for 2014–2020” and is supported by the Government of the Russian Federation represented by the Ministry of Higher Education and Science of Russia (Agreement No. 14.607.21.0203, Project identifier RFMEFI60718X0203).

33 Simulation of the Stress-Strain State of the Spline Joint …

413

References 1. D.K. Dwivedi, Surface Engineering: Enhancing Life of Tribological Components (Springer, New Delhi, 2018), p. 224 2. B.N.J. Persson, Sliding Friction. Physical Principles and Applications (Springer, Berlin, 2000), p. 513 3. V.A. Levchenko, I.A. Buyanovsky, V.N. Matveenko, J. Mater. Sci. Chem. Eng. 5(1), 175 (2017) 4. L.R. Rudnick (ed.), Lubricant Additives Chemistry and Applications, 2nd ed. (CRC Press, New York, 2009), p. 778 5. L.H. Baldaev, Renovation and Hardening of Machine Parts Using Thermal Spraying Methods (KHT, Moscow, 2004), p. 134 (in Russian) 6. S. Armadar, R. Schmid, S. Equey, I. Fagoaga, N. Espallargas, J. Therm. Spray Technol. 22(1), 10 (2013) 7. D.V. Shtansky, A.N. Sheveiko, M.J. Petrzhik, E.E. Levashov, A. Leyland, A.L. Yerokhin, D. Mathews, Surf. Coat. Technol. 200(1–4), 208 (2005) 8. A.A. Voevodin, D.V. Shtansky, E.A. Levashov, J.J. Moore (ed.), Nanostructured Thin Films and Nanodispersion Strengthened Coatings (Springer Science & Business Media, 2004), p. 322

Chapter 34

Shell with Auxetic Properties in the Model Taking into Account the Transverse Shear Anatoly S. Yudin

Abstract The Tymoshenko type model of constructively anisotropic shell with auxetic properties is considered. Forced oscillations in the frequency range including the first resonances are analyzed. The internal scattering of vibrational energy is taken into account. The influence of the transverse shear on the amplitude-frequency characteristics (AFCs) of the input malleability is investigated. It is compared with the frequency response obtained from the equations of the theory of Kirchhoff-Love.

34.1 Introduction The intention to increase the level of operational properties of materials creates new areas of research. In particular, the direction of search for structures that have anomalous properties is developing. They include materials with a negative Poisson’s ratio, which can expand in a direction perpendicular to the direction of stretching (auxetics). Data on such materials, natural and artificial, are collected in the detailed review [1], in which typical structures are considered and their classification is given. The history of search of natural materials, experimental observations and development of mechanical models with properties of auxetics is also briefly presented. One of the methods for creating auxetic materials is the technology of composite materials. The possibilities of obtaining inexpensive quasi-isotropic auxetic materials in the form of two-phase composites, one of the phases of which are auxetic particles, are analyzed. The particles can have different shapes: spherical, ellipsoidal, disk, blade and needle. Auxetic composites, the matrix phase and the filler which are not authenticate, are also considered. Several approaches differ in the level of detail of the environment and scale levels. There are three levels: 1. macroscopic level, when the occurrence of a negative Poisson’s ratio is explained on the basis of the relations of the theory of elasticity of anisotropic bodies; A. S. Yudin (B) I. I. Vorovich Institute of Mathematics, Mechanics and Computer Sciences, Southern Federal University, Rostov-on-Don, Russia e-mail: [email protected] © Springer Nature Switzerland AG 2020 I. A. Parinov et al. (eds.), Advanced Materials, Springer Proceedings in Materials 6, https://doi.org/10.1007/978-3-030-45120-2_34

415

416

A. S. Yudin

macroscopic analysis covers, for example, composites formed by oblique-angle reinforcement of an elastic matrix; 2. mesoscopic level, when the auxetic properties are due to the form of structural units at the scale of cells, pores, inclusions, etc.; periodic inhomogeneities of the meso-level have foam, granular materials and some others; 3. microscopic level, when, the features of elastic behavior are explained by intraand intermolecular interaction, which is typical for many single crystals and some other materials [1]. Composites are characterized by properties associated with a decrease in shear stiffness. Therefore, in the case of shells, there is a need to apply refined models. Previously, the Kirchhoff-Love type theory was used in the trial analysis [2]. The calculations showed a noticeable effect of the negative Poisson’s ratio on the reduction of the amplitudes of forced vibrations. Here the effect of the transverse shift is estimated using the equations of the Tymoshenko-type theory in combination with the auxetic properties. The method of complex amplitudes and semi-analytical method of solution construction are used. In the case of a cylindrical shell freely supported at the ends, Fourier series in two coordinates are used. The problem of forced oscillations is solved by decomposition of the displacement amplitudes in the eigenforms of oscillations. This provides a separation of equations to determine the coefficients of the harmonic numbers. The algorithm on this basis allows one to build the amplitude-frequency characteristics necessary for analysis quickly, taking into account the losses in the material.

34.2 Basic Equations Let us consider the shell of rotation in a system of curvilinear orthogonal coordinates which lines coincide with the lines of the principal curvatures. According to the hypothesis of a direct non-orthogonal material normal, the displacements of shell points are defined as follows: U(α1 , α2 , z) = u(α1 , α2 ) + zϕ1 (α1 , α2 ), V(α1 , α2 , z) = v(α1 , α2 ) + zϕ2 (α1 , α2 ) W(α1 , α2 , z) = w(α1 , α2 ),

(34.1) where u, v, w are the components of displacements of points of the middle surface of the shell; ϕ1 , ϕ2 are angles of rotation normal to the middle surface. The number of degrees of freedom of the material here is five. In this case, the linear deformation relations have the form: ε11 (α1 , α2 , z) = E11 (α1 , α2 ) + zK11 (α1 , α2 ), ε13 (α1 , α2 , z) = E13 (α1 , α2 ), (1 ↔ 2), ε12 (α1 , α2 , z) = E12 (α1 , α2 ) + zK12 (α1 , α2 ), ε33 (α1 , α2 , z) = 0.

(34.2)

34 Shell with Auxetic Properties in the Model Taking into Account …

417

Here Ejj , E12 , Ej3 , Kj , K12 , (j = 1, 2) are the tensile-compression deformation, tangential and transverse shear, curvature changes, torsion of the middle surface of the shell, respectively. They are associated with the components of displacements and angles of rotation for normal formulae: 1 ∂u 1 ∂A1 + v + k1 w, E13 = ϕ1 − ϑ1 , (1 ↔ 2), A1 ∂α1 A1 A2 ∂α2 1 ∂v 1 ∂A1 1 ∂u 1 ∂A2 E12 = − u+ − v, A1 ∂α1 A1 A2 ∂α2 A2 ∂α2 A1 A2 ∂α1 1 ∂φ1 1 ∂A1 K11 = + ϕ2 , (1 ↔ 2), A1 ∂α1 A1 A2 ∂α2 1 ∂ϕ2 1 ∂ϕ1 1 ∂A1 1 ∂A2 K12 = − ϕ1 + − ϕ2 , A1 ∂α1 A1 A2 ∂α2 A2 ∂α2 A1 A2 ∂α1 1 ∂w 1 ∂w , ϑ2 = k2 v − , (34.3) ϑ1 = k1 u − A1 ∂α1 A2 ∂α2 E11 =

where: A1 , A2 are the Lame coefficients; k1 , k2 are the main curvatures of the middle surface of the shell. For rotation shells, the kinematic relations (34.3) can be written as follows: E11 = u + k1 w, E22 = v• + ψu + k2 w, E12 = v + u• − ψv, K11 = ϕ1 , K22 = ϕ2• + ψϕ 1 , K12 = ϕ2 + ϕ1• − ψϕ 2 , E13 = ϕ1 − ϑ1 , E23 = ϕ2 − ϑ2 , ϑ1 = k1 u − w , ϑ2 = k2 v − w• , 1 ∂() 1 ∂() 1 ∂A2 (·) = , (·)• = ,ψ = . A1 ∂α1 A2 ∂α2 A1 A2 ∂α1

(34.4)

In the cylindrical shell version: k1 = 0, k2 = 1/Rc , ψ = 0, A2 = Rc , E11 = u , E22 = v• + k2 w, E12 = v + u• , K11 = ϕ1 , K22 = ϕ2• , K12 = ϕ2 + ϕ1• , E13 = ϕ1 − ϑ1 , E23 = ϕ2 − ϑ2 , ϑ1 = −w , ϑ2 = k2 v − w• . t

(34.5)

Equations of motion of the envelope follow the principle of Hamilton: (δK − δU + δA)dt = 0, in which the integrand is formed by the algebraic sum of

0

the variations of the kinetic energy δK, the potential energy δU, and the elementary work of the external forces δA: ¨ δU =

(T11 δE11 + T22 δE22 + SδE12 + Q11 δE13 + Q22 δE23 + M11 δK11 + M22 δK22 s

+ 2HδK12 )A1 A2 dα1 dα2 ,

418

A. S. Yudin

¨ δK =

{b(u,t δu,t +v,t δv,t +w,t δw,t ) + c(u,t δϕ 1 ,t +v,t δϕ2 ,t +ϕ 1 ,t δu,t +ϕ2 ,t δv,t ) s

+ d(φ 1 ,t δϕ 1 ,t +ϕ 2 ,t δϕ 2 ,t )}A1 A2 dα1 dα2 , ¨ (q1 δu + q2 δv + q3 δw)A1 A2 dα1 dα2 . δA =

(34.6)

s

Here Tjj =

σjj dz, Qjj =

h

σj3 dz, H =

h

σ12 zdz, S =

h

σ12 dz , Mjj =

σjj zdz, j = 1, 2 h

h

(34.7) are the internal forces and moments, given to the main surface, respectively;

ρ dz , c =

b= h

ρ zdz , d =

h

ρ z 2 dz

(34.8)

h

are the inertia coefficients; ρ is the density of the shell material. In the future, the established forced oscillations of the shell with the dependence of the values on time t of the form are considered: F(α1 , α2 , t) = Fa (α1 , α2 )e−iωt , where Fa is the complex amplitude of the harmonic quantities included in the equation, ω is the circular frequency of the driving load. After substitution of expressions (34.6) for variations, execution of the procedure for transferring derivatives, separation of the time parameter and assembling the coefficients with independent variations δu, δv, δw, δϕ1 , δϕ2 , the equations of harmonic stationary oscillations for complex amplitudes are obtained from the Hamilton principle. They have the form in the embodiment of the shells of rotation: T11 + ψ(T11 − T22 ) + S• + k1 Q11 + ω2 (bu + cϕ1 ) + q1 = 0, S + 2ψS + T•22 + k2 Q22 + ω2 (bv + cϕ2 ) + q2 = 0, Q11 + ψQ11 + Q•22 − k1 T11 − k2 T22 + ω2 bw + q3 = 0, M11 + ψ(M11 − M22 ) + H• − Q11 + ω2 (cu + dϕ1 ) = 0, H + 2ψH + M•22 − Q22 + ω2 (cv + dϕ2 ) = 0.

(34.9)

For a cylindrical shell we have: T11 + S• + ω2 (bu + cϕ1 ) + q1 = 0, S + T•22 + k2 Q22 + ω2 (bv + cϕ2 ) + q2 = 0, Q11 + Q•22 − k2 T22 + ω2 bw + q3 = 0, M11 + H• − Q11 + ω2 (cu + dϕ1 ) = 0,

H + M•22 − Q22 + ω2 (cv + dϕ2 ) = 0,

(34.10)

34 Shell with Auxetic Properties in the Model Taking into Account …

419

where for complex amplitudes the designations of the initial values are left. The elasticity relations are taken in the form of constructive orthotropy: T11 = B11 E11 + B12 E22 + A11 K11 + A12 K22 , T22 = B12 E11 + B22 E22 + A12 K11 + A22 K22 , M11 = A11 E11 + A12 E22 + D11 K11 + D12 K22 , M22 = A12 E11 + A22 E22 + D12 K11 + D22 K22 , S = B33 E12 + A33 · 2K 12 , H = A33 E12 + D33 · 2K 12 , Q11 = G13 E13 , Q22 = G 23 E 23 ;

(34.11)

B11 =

λ=1

B1(λ) + Bp1 , B22 =

B12 = B21 = D11 = D22 = A22 = B11 = B33 = D22 = A11 = A12 =

λ=1 λ=1 λ=1 λ=1 λ=1 λ=1 λ=1 λ=1

λ=1

B1(λ) ν2(λ) =

λ=1

λ=1

B2(λ) + Bp2 ,

B2(λ) ν1(λ) , B33 =

(D1(λ) + z2(λ) B1(λ) ) + D p1 , D12 = (D2(λ) + z2(λ) B2(λ) ) + Dp2 , A11 = B2(λ) z(λ) + Bp2 zp2 , A12 = B1(λ) + Bp1 , B22 = ¯ (λ) , D11 = G

λ=1

λ=1

λ=1

λ=1 λ=1

λ=1

¯ (λ) , G

(D1(λ) + z2(λ) B1(λ) )ν2(λ) , B1(λ) z(λ) + Bp1 zp1 ,

B1(λ) z(λ) ν2(λ) ,A33 =

B2(λ) + B p2 , B12 = B21 =

2 B (D1(λ) + z (λ) 1(λ) ) + D p1 , D12 =

(D2(λ) + z2(λ) B2(λ) ) + D p2 , D33 = B1(λ) z(λ) + Bp1 zp1 , A22 = B1(λ) z(λ) ν2(λ) ,A33 =

λ=1

λ=1

λ=1

λ=1

λ=1

λ=1

¯ (λ) z(λ) , G

B1(λ) ν2(λ) =

λ=1

B2(λ) ν1(λ) ,

(D1(λ) + z2(λ) B1(λ) )ν2(λ) ,

¯ ˜ (λ) + z2 G ˜ ˜ (G (λ) (λ) ) + Gp1 + Gp2 ,

B2(λ) z(λ) + Bp2 zp2 ,

¯ (λ) z(λ) ; G

(34.12)

(34.13)

Here Ek(λ) are elastic constants of layers (k = 1, 2); h(λ) is the thicknesses; z(λ) are the eccentricities (normal coordinates of the middle surface of the λ-th layer); l pk is the distance between the ribs; Epk , Gpk are the Young’s moduli and shear of the material of the ribs; Fpk is the cross-section area (CSA) of ribs; Ipk are the moments of inertia CSA of the ribs relative to the axes passing through the center of gravity CSA of the ribs parallel to the tangent to the coordinate lines of the reference surface; Iok is the moment of inertia of the ribs CSA relative to the tangent of the k-th coordinate ˜ (λ) , are line; Jpk are the moments of inertia of the ribs in torsion; Bk(λ) , Dk(λ) , G(λ) , G

420

A. S. Yudin

the effective tensile stiffness of the λ-th layer-compression, bending, shear, torsion, ˜ k are the respectively; G13 , G23 are induced shear stiffness of the shell: Bpk , Dpk, G stiffness of the ribs in tension-compression, bending, torsion, respectively. The inertial characteristics of the shell (mass per unit area) are determined by the parameters: ρ1 j = ρ1 + j , j = 1, 2, 3, ρ1 =

λ=1

ρ(λ) h(λ) +

2

[ρ pk Fpk /(¯ν∗ ∫ )].

(34.14)

pk

k=1

Here ρ1 is the specific mass of the actually reinforced shell, ρ(λ) is the density of the materials of the layers, ρpk is the density of the materials of the ribs; j are the inertial components of the masses modeling the useful filling of the shell. These masses can be involved in various ways in oscillations in different coordinate directions. Their accounting can be carried out in different ways depending on the number of the circumferential harmonic. Input design information can be entered in both dimensional and dimensionless form. In the dimensional version should be put ν¯ ∗ = 1.

34.3 Method of Solution Since we consider axisymmetric constructions, it is possible to separate the circumferential coordinate α2 in the above equations. Let us limit the normal load q3 , symmetrically located relative to the origin of the circumferential coordinate. Then the decomposition in Fourier series can be performed either in cosines or in sines. For example: w= q3 =

∞ n=0 ∞

wn cos nα2 , v =

∞ n=0

q3n cos nα2 ,

vn sin nα2 , T11 =

∞ 11n

cos nα2 ,

n=0

(34.15)

n=0

and so on. The components of the stress-strain state are decomposed by cosines u, w, ϕ1 , ϑ1 , E11 , E22 , E12 , E13 , E23 , K11 , K22 , K12 , T11 , T22 , M11 , M22 , Q11 , by sine – v, ϕ2 , ϑ2 , E12 , K12 , S, H, Q22 . Let us proceed in the basic relations and equations to dimensionless quantities, using the basic normalizing parameters E* , ν* , R* , h* , ρ* . They make sense and dimension of the characteristic, respectively, Young’s modulus, Poisson’s ratio, radius of curvature or linear size (large), thickness (small size), density of the material. Combinations of divisors having the dimension of normalized quantities are formed from the main normalizing parameters.

34 Shell with Auxetic Properties in the Model Taking into Account …

421

Symbols are entered: ε∗ = h∗ /R∗ is the thin-walled parameter; ν¯ ∗ = 1 − ν2∗ ; B∗ = E∗ h∗ /¯ν∗ , A∗ = E∗ h2∗ /¯ν∗ , D∗ = E∗ h3∗ /¯ν∗ are the normalizing √ values for the coefficients of reduced stiffness in the elasticity relations; c∗ = E∗ /(ρ∗ ν¯ ∗ ) is the characteristic speed of sound in the shell material; F∗ = R∗ h∗ /¯ν∗ , S∗ = R∗ h2∗ /¯ν∗ J∗ = R∗ h3∗ /¯ν∗ are the values for normalization of the cross-section parameters of edges (areas and moments of inertia). We also introduce a dimensionless frequency parameter, related to the circular frequency ω = 2πf, where f is the frequency in hertz, by the formula: = ωR∗ /c∗ . The formulae of transition to dimensionless quantities have the form [3]:

(34.16)

In Formulae (34.16), dimensionless quantities are grouped by braces with the index “L” in the left parts of the equations. Their dimensional (normalized) analogs are implied in brackets with the index “D” in the right parts of the formulae. As a test design, we consider a circular cylindrical shell supported by the edges of the longitudinal and circumferential directions. The construction was analyzed in [2] by Kirchhoff-Love theory, so a comparison of mathematical models can be made. The main surface of the shell has a radius R. We assume R* = R, then A1 = 1, A2 = 1, k2 = 1. We apply the method of complex amplitudes to the equations for the cylindrical shell and separate the n-th circumferential mode. After the transition to dimensionless quantities, kinematic relations are reduced to the form: E11 n = u n , E22 n = nvn + wn , E12n = vn − nun , K11 n = ε∗ ϕ1 n , K22 n = ε∗ nϕ2n , K12n = ε∗ (ϕ2n − nϕ1n ), E13n = ϕ1n − ϑ1n , E23n = ϕ2n − ϑ2n , ϑ1n = −wn , ϑ2n = vn + nwn ;

(34.17)

The simplest analytical solution is constructed for the free support: v = 0, M11 = 0, T11 = 0, w = 0, Q11 = 0, ϕ2 = 0. These conditions and homogeneous (q3n = 0) Eqs. (34.1)–(34.3) satisfy the following forms of natural oscillations: un (x) = unk cos(mx), vn (x) = vnk sin(mx), wn (x) = wnk sin(mx),

422

A. S. Yudin

ϕ1n (x) = ϕ1nk cos(mx), ϕ2n (x) = ϕ2nk sin(mx),

(34.18)

where m = kπ/L, k is a number of longitudinal half-waves, x = α1 is the longitudinal coordinate. We will also denote the circumferential coordinate as θ = α2 . The problems of forced oscillations can be solved by decomposition of the displacement amplitudes in the eigenforms of oscillations (34.17), i.e. in the Fourier series and along the longitudinal coordinate. This provides a separation of equations to determine the coefficients by mode numbers. In the circumferential coordinate θ, cosine and sine series expansions are performed in rows in the interval (0, 2π) due to the symmetry of the load in the diametrical plane (DP), which is assumed. In the longitudinal direction, the solutions on the interval (0, L) are also represented by rows of sines and cosines. Restrictions on the load coordinates along the length of the shell are not imposed. Here we perform the decomposition of even and odd functions on the interval (−L, L), which are formally considered as a continuation of the solution to the interval (−L, 0) in an even or odd way. We are only interested in the part on the interval (0, L) of the shell. Therefore, the number n is the number of waves in the circumferential direction, and k is the number of half-waves on the generator of the shell. The series solution for displacement and rotation angles as functions of coordinates and frequency is M

M

N

u(x, θ, ) = u 0k () cos[(kπ/L)x] + u nk () cos[(kπ/L)x] cos(nθ), k=1 M N

k=1 n=1

v(x, θ, ) = vnk () sin[(kπ/L)x] sin(nθ),

k=1 n=1 M M N w(x, θ, ) = w0k () sin[(kπ/L)x] + wnk () sin[(kπ/L)x] cos(nθ), k=1 k=1 n=1 M M N ϕ1 (x, θ, ) = ϕ10k () cos[(kπ/L)x] + ϕ1nk () cos[(kπ/L)x] cos(nθ), k=1 k=1 n=1 M N ϕ2 (x, θ, ) = ϕ2nk () sin[(kπ/L)x] sin(nθ). k=1 n=1

(34.19) Using expansions of this type in all relations and equations, we obtain for the coefficients of trigonometric series: E 11nk = −mu nk , E 22nk = nvnk + wnk , , E 12nk = mvnk − nu nk , K 11nk = −ε∗ mϕ1nk , K 12nk = ε∗ nϕ2nk , K 12n = ε∗ (mϕ2nk − nϕ1nk ), E 13nk = ϕ1nk + ϑ1nk , E 23nk = ϕ2nk + ϑ2nk , ϑ1nk = −mwnk , ϑ2nk = vnk + nwnk , ϑ2n = vn + nwn ; (34.20) T11nk = B11 E11nk + B12 E22nk + A11 K11nk + A12 K22nk , T22nk = B12 E11nk + B22 E22nk + A12 K11nk + A22 K22nk , M11nk = A11 E11nk + A12 E22nk + D11 K11nk + D12 K22nk ,

34 Shell with Auxetic Properties in the Model Taking into Account …

423

M22nk = A12 E11nk + A22 E22nk + D12 K11nk + D22 K22nk , Snk = B33 E12nk + 2A33 K12nk , Hnk = A33 E12nk + 2D33 K12nk , Q11nk = G13 E13nk , Q22nk = G23 E23nk ;

(34.21)

mT11nk + nSnk + 2 (bunk +ε∗ cϕ1nk ) = 0, - mSnk - nT22nk + Q22nk + 2 (bvnk + ε∗ cϕ2nk ) = 0, - mQ11nk + nQ22nk - T22nk + 2 bwnk + q3nk = 0, mM11nk + nHnk - Q11nk /ε∗ + 2 (cunk + ε∗ dϕ1nk ) = 0, - mHnk - nM22nk - Q22nk /ε∗ + 2 (cvnk + ε∗ dϕ2nk ) = 0.

(34.22)

We consider the load acting on the normal to the shell and equivalent to the concentrated force Q3 . Let l is the length of the platform along the longitudinal coordinate, δ1 is the length of a segment of its midline (like a trapezoid); 2δ is the angle of coverage along the circumferential coordinate; x1 , θ1 are the longitudinal and angular coordinates of the center of the site, S = lδ1 is the area of application of the load. Let us move on to dimensionless quantities by formulae: {l, δ1 }L = {l, δ1 }D /R∗ , {Q3 }L = {Q3 }D (1 − ν2∗ )/E∗ h2∗ , {q3 }L = {q3 }D (1 − ν2∗ )R2∗ /E∗ h2∗ .

(34.23)

Further (in a dimensionless form), the concentrated force is “smeared” across the site into the normal intensity load q3a = Q3 /(lδ1 ) distributed over the surface within the platform. In the domain of curvilinear coordinates {x∈(0, L); θ∈(0, 2π)}, corresponding to the shell under consideration, the distributed load can be specified using Heviside step function h(x), which is 0 at x < 0 and 1 at x ≥ 0. Then in the field of definition q3 (x, θ) = q3a 1 (x) 2 (θ), where

1 (x) = [H(x − (x1 − l/2)) − H(x − (x1 + l/2))],

2 (θ) = [H(θ − (θ1 − δ)) − H(θ − (θ1 + δ))].

(34.24)

424

A. S. Yudin

The decomposition of the even function 2 (θ) into cosines has the form: N

2 (θ) = δ/π + [2/(nπ)] sin(nδ) cos(nθ1 ) cos(nθ).

(34.25)

n=1

Let us continue 1 (x) on the interval (-L, 0) in an odd way. The corresponding expansion in the interval (-L, L) by sine has the form:

1 (x) =

M

[4 (kπ)] sin[(kπ/L)l 2)] sin[(kπ/L)x1 ] sin[(kπ/L)x)].

(34.26)

k=1

Thus, the normal load q3 (x, θ) is approximated by a double row: q(x, θ) =

M N M aθ 0 axk sin[(kπ/L)x] + aθn axk sin[(kπ/L)x] cos(nθ), 2 k=1 n=1 k=1

(34.27) where aθ 0 = q3a 2l L, aθn = q3a [2 (nπ)] sin(nδ) cos(nθ1 ), axk = q3a [4 (kπ )] sin[(kπ/L)l 2] sin(mx1 ).

(34.28)

or q(x, θ) =

N M

qnk sin[(kπ/L)x] cos(nθ), qk0 = aθ 0 axk 2, qkn = aθ n axk .

n=0 k=1

(34.29) Let us substitute (34.20) into (34.21) and then into (34.22). Collecting the coefficients at unk , vnk , wnk , ϕ1nk , ϕ2nk , we obtain algebraic system of equations of the fifth order to determine the coefficients of the series (34.19) when n > 0: KX = B.

Here K = Kλμ , λ, μ = 1, . . . , 5 is the matrix of the system; X is the column with unknown elements: X1 = unk , X2 = vnk , X3 = wnk , X4 = ϕ1nk , X5 = ϕ2nk ; B is the right part, dependent on the load ratios: ⎡

K11 K12 K13 K14 K15

⎢ ⎢ K21 K22 K23 K24 K25 ⎢ ⎢ K = ⎢ K31 K32 K33 K34 K35 ⎢ ⎢ ⎣ K41 K42 K43 K44 K45 K51 K52 K53 K54 K55

⎤

⎡ X1 ⎥ ⎢X ⎥ ⎢ 2 ⎥ ⎢ ⎥ ⎥, X = ⎢ X3 ⎢ ⎥ ⎥ ⎣ X4 ⎦ X5

⎤

⎡

⎤ 0 ⎢ 0 ⎥ ⎥ ⎢ ⎥ ⎥ ⎢ ⎥ ⎥ ⎥, B = ⎢ qnk ⎥. ⎢ ⎥ ⎥ ⎣ 0 ⎦ ⎦ 0

(34.30)

34 Shell with Auxetic Properties in the Model Taking into Account …

425

The elements of the matrix K are defined by formulae: K 11 = b2 − B11 m 2 − B33 n 2 , K 12 = mn(B12 + B33 ), K 13 = B12 m, K 14 = ε∗ (c2 − A11 m 2 − 2 A33 n 2 ), K 15 = ε∗ m(A12 m + 2 A33 n); K 21 = mn(B12 + B33 ), K 22 = b2 − B33 m 2 − B22 n 2 − G 23 , K 23 = −n(B22 + G 23 ); K 24 = ε∗ mn(A12 + 2 A33 ), K 25 = ε∗ (c2 − 2 A33 m 2 − A22 n 2 ) + G 23 ; K 31 = B12 m, K 32 = −n(B22 + G 23 ), K 33 = b2 − G 13 m 2 − G 23 n 2 − B22 , K 34 = ε∗ (A12 m + A22 n) − G 13 m, K 35 = n(G 23 − ε∗ A22 ); K 41 = −(A11 m 2 + A33 n 2 ) , K 42 = mn(A12 + A33 ), K 43 = m(A12 − G 13 /ε∗ ), K 44 = ε∗ (d2 − D11 m 2 − 2D33 n 2 ) − G 13 /ε∗ , K 45 = ε∗ mn(D12 + 2D33 ); K 51 = mn(A12 + A33 ), K 52 = c2 − A22 n 2 − A33 m 2 + G 23 /ε∗ , K 53 = n(G 23 /ε∗ − A22 ), K 54 = ε∗ mn(D12 + 2D33 ), K 55 = ε∗ (d2 − 2D33 m 2 − D22 n 2 ) − G 23 /ε∗ .

(34.31)

The equations for determining the coefficients of the zero circumferential mode are processed separately. The problem is reduced to a system of three algebraic equations: PY = C with respect to Y1 = u0k , Y2 = w0k , Y3 = ϕ10k , where ⎡

⎤ ⎤ ⎡ ⎤ ⎡ P11 P12 P13 Y1 0 P = ⎣ P21 P22 P23 ⎦, Y = ⎣ Y2 ⎦, C = ⎣ q0k ⎦, P31 P32 P33 Y3 0

(34.32)

P11 = b2 − B11 m2 , P12 = B12 m, P13 = ε∗ (c2 − A11 m2 ) ; P21 = B12 m, P22 = b2 − G13 m2 − B22 , P23 = ε∗ mA12 − G13 m; P31 = c2 − A11 m2 , P32 = m(A12 − G13 /ε∗ ), P33 = ε∗ (d2 − D11 m2 ) − G23 /ε∗ . (34.33)

34.4 Calculations and Analysis The shell was considered as the initial one, the rigidity of the constructive anisotropy of which is similar to that considered in [2]. Loss factor η = 0.03, dimensionless length L = π. The driving harmonic force is applied in the middle of the length. Let us consider the comparison of models for orthogonal (theory of Kirchhoff— Love—K) and slope normal (the theory of Timoshenko type—T), first. Model K corresponds to the dashed curves, model T—to the continuous ones. The results for the second model have lower vibration amplitudes and strongly depend on the values of the transverse shear modules G13 and G23 . It was assumed in the calculations G13 = G23 . It is possible both to coincide with the main resonance (mode n = 3, Fig. 34.1), and to leave this resonance to other frequencies (Fig. 34.2). At the same time, close

426

A. S. Yudin

Fig. 34.1 ν = 0.3, G13 = 0.000087B33

Fig. 34.2 ν = 0.3, G13 = 0.005B33

in frequency resonance modes n = 2 and n = 4 can be cut off. The resonance of the n = 5 mode can also be shifted. Let us try to explain the difference between the theories of K and T. We turn to the equations of oscillations (34.9), (34.10). It is necessary to remove the terms associated with the inertia of turns in variant K in the fourth and fifth equations. There are no elasticity relations for shear forces here, since transverse deformations are considered to be zero. The transverse forces are determined from the last two equations through bending and torques and are substituted into the second and third equations.

34 Shell with Auxetic Properties in the Model Taking into Account …

427

Fig. 34.3 ν = −0.5, G13 = 0.0001B33

Accordingly, these values are affected by the flexural and torsional stiffness of the shell. In theory of T, the shearing forces become independent stress state components affecting four of the five equations. Therefore, the transverse shear strains and transverse shear modules become decisive here, by varying which it is possible to more flexibly control the amplitude-frequency characteristics. Let us consider the influence of the Poisson’s ratio ν on the amplitude-frequency characteristics in the model of T. The coefficient ν was set equal to −0.5 and −0.3 in the auxetic version. In general, the influence of the negative Poisson’s ratio has a positive effect on vibration damping. Here, both the suppression of the resonances n = 2 and n = 4 (Fig. 34.3), and their preservation (Fig. 34.4) are also observed. Model variation of material parameters was performed here. It is necessary to set the properties of the material based on the analysis of its structure and mechanical test data to calculate specific products.

428

A. S. Yudin

Fig. 34.4 ν = −0.3, G13 = 0.0036B33

Acknowledgements Research was financially supported by Southern Federal University, 2020 (Ministry of Science and Higher Education of the Russian Federation).

References 1. D.A. Konjok, K.W. Wojciechowski, Y.M. Pleskachevsky, S.V. Shilko, Mechanics of Composite Materials and Structures (Moscow), vol. 10, no. 1 (2004), pp. 35–69 2. A.S. Yudin, S.A. Yudin. in Proceedings of the 2015 International Conference on Physics and Mechanics of New Materials and Their Applications, devoted to 100th Anniversary of the Southern Federal University, ed. by I.A. Parinov, S.-H. Chang, V.Y. Topolov (Nova Science Publishers, New York, 2016), pp. 447–452 3. A.S. Yudin, Stability and Oscillations of Structurally Anisotropic and Articulated Shells of Rotation (Southern Federal University Press, Rostov-on-Don, 2011), 362 p. (In Russian)

Chapter 35

Coupled Problem of Thermoviscoelasticity for Composite Polymer Shell of Revolution V. G. Safronenko

Abstract The problem of connectedness of mechanical and thermal fields has acquired great practical importance in the mechanics of shells made of polymer composite materials. A number of specific properties of polymers, such as low thermal conductivity, high sensitivity to temperature change, large hysteresis losses, lead to harmonic loading under the effect of heat generation in the body of the shell, namely dissipative heating. To solve the problem of forced vibrations of polymer composite shells, taking into account thermomechanical connectivity, along with effective thermal-viscoelastic characteristics, it is necessary to specify effective thermal characteristics (thermal conductivity, thermal expansion, and specific heat). A complete system of relations is presented, including the equations of forced oscillations of polymer-based composite shells of revolution, heat conduction equations taking into account the effect of heat generation, the constitutive equations of thermoviscoelasticity with the corresponding boundary conditions. As an example, we consider forced axisymmetric vibrations of a fibrous-layered cylindrical shell. In the following, it is assumed that the hard fitting condition is satisfied at the ends of the shell and the temperature is kept constant.

35.1 Introduction At the first stage, the solution of the heat generation problem is considered without taking into account the temperature dependences of the properties of the polymer (the so-called weakly coupled problem). Numerical calculations are made for three variants of reinforcement. The amplitude-frequency and temperature-frequency characteristics in the frequency range, including the first eigenfrequencies, are obtained. Further, the related problem of thermoviscoelasticity is considered for the case of axisymmetric forced vibrations. The problem is essentially non-linear in nature due

V. G. Safronenko (B) I. I. Vorovich Mathematics, Mechanics and Computer Sciences Institute, Southern Federal University, Rostov-on-Don, Russia e-mail: [email protected]; [email protected] © Springer Nature Switzerland AG 2020 I. A. Parinov et al. (eds.), Advanced Materials, Springer Proceedings in Materials 6, https://doi.org/10.1007/978-3-030-45120-2_35

429

430

V. G. Safronenko

to the dependence of polymer properties on temperature and the presence of a dissipative function in the heat equation. Therefore, in solving a system of differential equations, in addition to the orthogonal sweep method, an iterative method was implemented with a given accuracy. The calculations indicate a significant discrepancy between the amplitudes and heat generation temperature in the vicinity of the resonant frequencies. In this case, the solution of the problem, which does not take into account the effect of temperature on the properties of the polymer, yields substantially underestimated values both in the calculation of the amplitude-frequency and temperature-frequency characteristics. Outside the resonance regions, the solutions of both problems are fairly close.

35.2 Methods The complete system of equations describing the related problem of thermoviscoelasticity for the shell of revolution has the following form in common notations: 1 dy1∗ A1 dα1 1 dy2∗ A1 dα1 1 dy3∗ A1 dα1 1 dy4∗ A1 dα1 1 dy5∗ A1 dα1 1 dy6∗ A1 dα1 1 dy7 A1 dα1 1 dy8 A1 dα1

= ψ(T22 − y1 ) − k1 y3 − ρ11 2 y4 − q1 , 1 = ψ M22) − y2 + y3 − ε1 ρ12 2 y5 , ε1 = −ψ y3 + k1 y1 + k2 T22 − ρ11 2 y6 − q3 , = E 11 − k1 y6 , = K 11 , = k1 y4 − θ1 , = − C1 (y8 − Tcp ) − ψ y7 , = −C2 μ11 y7

(35.1)

In the case of axisymmetric loading the resolving functions are [1]: y1∗ = T11 ; y5∗ = ϕ1 ; yi∗

=

yiR

y2∗ = M11 ; y6∗ = w;

+

i yiI

y3∗ = Q 11 ;

y7 = q1 ;

y4∗ = u;

y8 = T. (35.2)

35 Coupled Problem of Thermoviscoelasticity for Composite Polymer …

431

To solve the problem of forced oscillations of polymer composite shells taking into account thermomechanical coupling, along with effective viscoelastic characteristics, it is necessary to set effective thermal characteristics (coefficients of thermal conductivity, thermal expansion and specific heat capacity). For a polydisperse medium with cylindrical inclusions corresponding to a fibrous composite, the effective thermal conductivity coefficients are given in [2]. Due to the transversal isotropy of the medium, only two components of the tensor of the effective thermal conductivity coefficients are independent, and Fourier’s law is written as ⎤ ⎡ ⎤⎡ ⎤ 0 −λ11 0 ∇1 T q1 ⎣ q2 ⎦ = ⎣ 0 −λ22 0 ⎦⎣ ∇2 T ⎦ q3 ∇3 T 0 0 −λ22 ⎡

(35.3)

In the coordinate axes (α 1 , α 2 , z) entered on the median surface of the shell of revolution, respectively: ∇1 T =

1 ∂T 1 ∂T ∂T ; ∇2 T = ; ∇1 T = A1 ∂α1 A2 ∂α2 ∂z

(35.4)

In this case, the effective coefficient in the axial direction (along the fiber) is determined by the rule of mixtures. For a two-phase medium, we obtain: λ11 = Vf λf + Vm λm .

(35.5)

where λm , λf are thermal conductivity coefficients of isotropic matrix and fiber materials. The effective coefficient λ22 can be found by the formula: λ22 = λm 1 +

Vf λm λf −λm

+

1−Vf 2

(35.6)

We assume that the temperature gradient over the thickness of the thin shell is zero. In this case, the matrix of effective thermal conductivity coefficients in the axes of symmetry has the form:

Λ=

−λ11 0 0 −λ22

(35.7)

Consider the case, where a new coordinate system (α1 , α2 , z) is derived from the system (α1 , α2 , z) by rotating by some angle β. We introduce a transition matrix B, which has the form:

cos β − sin β B= (35.8) sin β cos β

432

V. G. Safronenko

The thermal conductivity matrix in the new coordinate system will look like this: Λ = B −1 ΛB Λ =

−(λ11 cos2 β + λ22 sin2 β) sin β cos β(λ11 − λ22 ) sin β cos β(λ11 − λ22 ) −(λ11 sin2 β + λ22 cos2 β)

(35.9)

The matrix of thermal resistance, inverse Λ has the form:

M= =

−μ11 −μ12 −μ21 −μ22

= (Λ )−1

22 cos − (λ11 sin λβ+λ 11 λ22 2

2

β)

11 −λ22 ) − sin β cosλ11β(λ λ22

11 −λ22 ) 22 sin − sin β cosλ11β(λ − (λ11 cos λβ+λ λ22 11 λ22 2

2

β)

(35.10)

In the case of an axisymmetric problem for an arbitrary shell, the Fourier equation can be written as dT = −μ11 q1 . A1 dα1

(35.11)

The energy equation, composed taking into account the convective heat transfer on the front surface of the shell, will be written as 2α dq1 1 T − Tcp , + ψq1 = − A1 dα1 h h

(35.12)

where λ is the effective coefficient of thermal conductivity; α is the coefficient of heat transfer from the shell surface. The boundary conditions for the energy equation under conditions of preservation at the ends of the shell of a constant temperature T 0 , and the absence of heat flow, have the form: T |α1 =0 = T0 T |α1 =L = T0 . (35.13) q1 |α1 =0 = 0 q1 |α1 =L = 0 Taking into account the expression of the dissipative function, we give the equation of thermal conductivity to the dimensionless form. ω 2

E ∗ h 2∗ ∧ R h ∗ ∧ I E ∗ h 2∗ ∧ I h ∗ ∧ R T11 E 11 − T E + ··· R∗ R∗ R∗ 11 R∗ 11 E ∗ h 3∗ ∧ I h ∗ ∧ R E ∗ h 3∗ ∧ R h ∗ ∧ I M11 2 K 11 − M11 2 K 11 + · · · + R∗ R∗ R∗ R∗

=

35 Coupled Problem of Thermoviscoelasticity for Composite Polymer …

433

E ∗ h 2∗ ˜ R h ∗ ∧ I E ∗ h 2∗ ∧ I h ∗ ∧ R + Q 23 E Q 23 E 23 − R∗ R∗ R∗ R∗ 23 ∧ ∧ E ∗ E ∗ h 3∗ ∧ R ∧ I R I = (T E + · · · + ε M K + ··· 1 11 11 11 11 2 R∗2 ρ∗ R∗2 ∧

∧

+ Q 23R E 23I ).

(35.14)

We obtain the following dimensionless quantities: ∧

=

∧

dq1 = ∧ R∗ A1 dα1

ρ∗ R∗3 T h ∧ ∧ , T = , h = 3 E∗ E∗ h∗ T∗ h∗

(35.15)

E ∗ E ∗ h 3∗ ∧ 1 2α 1 ∧ ∧ ∧ ∧ − Tcp )T∗ − ψ q1 , ∧ − ∧ (T 3 ρ∗ R∗ h∗h h∗h R∗

∧

T∗ dT ∧ = −K μ11 q1 ∧ R∗ A1 dα1

(35.16)

Write down finally (35.12) as ∧

dq1 ∧ 1 ∧ ∧ ∧ ∧ = ∧ − C1 (T − Tcp ) − ψ q1 , ∧ A1 dα1 h ∧

where C1 =

2αT∗ ∧ 1 dT ∧ = −C2 μ11 q1 ,q = q1 , ∧ h∗ K 1 R∗ K A1 dα1

(35.17)

R2 K E h2 where C2 = T∗∗ , K = Eρ∗∗ R∗ 3 ∗ . ∗ In the future, it is assumed that at the ends of the shell, the condition of anchorage is fulfilled and a constant temperature is maintained: y4∗ = 0, y5∗ = 0, y6∗ = 0, y7 = 0, y8 = Tcp at a1 = 0, L

(35.18)

35.3 Numerical Experiment Let us consider the forced axisymmetric oscillations of the fibrous-layered cylindrical shell, taking into account the thermomechanical coupling. The physical and mechanical characteristics of the polymer matrix correspond to the dependencies [3]. Let the multilayer cylindrical shell be exposed to an external load with an intensity of p3 = 5 kPa. The load is distributed over a ring of width R. The shell consists of five layers, while the physical and mechanical characteristics of the reinforcing

434

V. G. Safronenko

fibers correspond to carbon fiber with mechanical properties: E f = 186 GPA; ν f = 0.3; ρ f = 1730 kg/m3 ; λf = 20 W/(m deg). Characteristics of the polymer matrix: ρ m = 1214 kg/m3 ; λm = 0.15 W/(m deg). Medium temperature T 0 = 293 K. Let us consider at the first stage the solution of the problem of heat formation without taking into account the dependence of the properties of the polymer on temperature (the so-called loosely coupled problem). Numerical calculations are made for three variants of reinforcement. The specific content of fibers in the composite V f = 0.7. Figure 35.1 presents the amplitudefrequency characteristics of the shell in the frequency range, including the first resonances and Table 35.1 shows values of the first three resonant frequencies and their oscillation amplitudes. Figure 35.2 presents the temperature-frequency dependences for these three reinforcement options and Table 35.2 shows values of the self-heating temperature at first three resonant frequencies. Next, we consider the related thermoviscoelasticity problem for the case of axisymmetric forced oscillations. The problem is essentially nonlinear due to the dependence of the polymer properties on temperature and the presence of a dissipative function in the energy equation. Therefore, by solving the system of differential

Fig. 35.1 Amplitude-frequency characteristics for the three variants of reinforcement

Table 35.1 Values of the first three resonant frequencies and their oscillation amplitudes 1

|W 1 |

2

|W 2 |

3

|W 3 |

β = 0°

0.477

0.01

0.549

0.005

–

–

β = 45°

0.507

0.008

0.574

0.005

0.631

0.0084

35 Coupled Problem of Thermoviscoelasticity for Composite Polymer …

435

Fig. 35.2 Self-heating temperature

Table 35.2 Values of the self-heating temperature at first three resonant frequencies

T1

T2

T3

β = 0°

1.62

1.15

–

β = 45°

1.46

1.21

1.37

equations, in addition to the orthogonal run method, an iterative method with a given accuracy was implemented. The results of amplitude-frequency characteristics calculations corresponding to the coupled and weakly coupled formulation of the problem are present in Fig. 35.3a and b, respectively. The coupled problem is understood here as a problem in which the physical and mechanical properties of the polymer depend only on the initial temperature of the shell equal to T 0 . The corresponding temperature-frequency characteristics are shown in Fig. 35.4a and b. The frequency ranges including the first resonances are considered, where there is a gap in the solution of the related problem at the intervals 1 = [0.415–0.485] and 2 = [0.623–0.634]. In this frequency range, the convergence of the solution is violated, and the accumulation of the critical error is achieved at the first iterations. By solving a weakly coupled problem, stationary vibrational and temperature regimes exist for all taken values of the frequency parameter. The calculations indicate a significant discrepancy between the amplitudes and temperature of heat formation in the vicinity of resonance frequencies. In this case, the solution of the problem, which does not take into account the influence of temperature on the properties of the polymer, gives significantly underestimated values both in the calculation of amplitude-frequency and temperature-frequency characteristics. Outside the resonant regions, the solutions of both problems are quite close. Figure 35.5a and b present typical distributions of transverse deflection and temperature along the length of the shell in the vicinity of the first resonance at a frequency = 0.4.

436

V. G. Safronenko

(a)

(b) coupled task

weak ly coupled

Fig. 35.3 Amplitude–frequency characteristics

35.4 Conclusion The forced oscillations of the composite polymer shell of revolution are considered taking into account the thermomechanical coupling. The related problem of thermoviscoelasticity for a fibrous-layered cylindrical shell is investigated numerically in an axisymmetric formulation. The problem of heat formation with and without taking into account the dependence of the properties of the polymer matrix on temperature is considered.

35 Coupled Problem of Thermoviscoelasticity for Composite Polymer …

(a)

(b) weakly coupled problem Fig. 35.4 Temperature–frequency characteristics

coupled problem

437

438

V. G. Safronenko

Fig. 35.5 Distributions of transverse deflection and temperature along shell length

References 1. E.I. Grigolyuk, G.M. Kulikov, Multilayer Reinforced Shell (Mashinostroenie, Moscow, 1988), 288 p. (in Russian) 2. R.M. Cristensen, Mechanics of Composite Materials (Mir, Moscow, 1982), 336 p. (in Russian) 3. Y.P. Stepanenko, K.V. Isaev, A.D. Azarov, In: Proceedings of II International Conference “Modern Problems of Continuum Mechanics, Rostov-on-Don, vol. 1, 118 (1996) (in Russian)

Chapter 36

The Study of Stratification of Multilayer Structures Based on Finite Element Modeling and Neural Network Technologies A. V. Cherpakov, P. V. Vasiliev, A. N. Soloviev, I. A. Parinov and B. V. Sobol Abstract An approach to solving the problem of identifying the thickness of the layers of a multilayer structure using the combination of the finite element method and artificial neural networks (ANNs) is presented. The simulation of a multilayer structure in the ANSYS finite element software is presented. The construction model consists of 4 layers, each of which has certain properties. The model is an imitation of the soil foundation of the road surface. Simulation in the form of a simplified, plane statement of the problem is considered. The analysis of surface waves, excited during the simulation of impact loading. The wave field of displacements in a given section of the structure is analyzed. Based on a numerical experiment, an approach is constructed to estimate the thickness of one of the layers of the structure. The application of ANN to restore information about the thickness of one of the layers is considered. As a result of the study, a method for identifying the thickness of the layers of a multilayer structure was developed, based on a combination of the finite element method and ANN.

36.1 Introduction The reconstruction of properties and defects, the restoration of the homogeneity of the structure of materials in layered structures, for example, such as pavements and various soil bases, is an important technical problem. Solving the reconstruction problem will allow us to evaluate the current state of the structure of the studied A. V. Cherpakov (B) · A. N. Soloviev Department of Theoretical and Applied Mechanics, Don State Technical University, 1, Gagarin Square, Rostov-on-Don, Russia 344010 e-mail: [email protected] A. V. Cherpakov · A. N. Soloviev · I. A. Parinov Institute of Mathematics, Mechanics and Computer Sciences, Southern Federal University, 8a, Milchakov Str., Rostov-on-Don, Russia 344000 P. V. Vasiliev · B. V. Sobol Department of Information Technologies, Don State Technical University, 1, Gagarin Square, Rostov-on-Don, Russia 344010 © Springer Nature Switzerland AG 2020 I. A. Parinov et al. (eds.), Advanced Materials, Springer Proceedings in Materials 6, https://doi.org/10.1007/978-3-030-45120-2_36

439

440

A. V. Cherpakov et al.

layered structure. The task of restoring information about stratification of layered structures is especially relevant for monitoring and comparative analysis of structural changes from mechanical action on layers in a certain area of the structure. Such identification can be carried out using instruments (laser displacement sensors, cycle meters, accelerometers, etc.), which are located along the investigated surface of the structure and monitor it [1]. A more attractive detection method is the use of acoustic sensors and receivers mounted on the external surface and detecting various zones of structural heterogeneity (defects, inclusions, voids, etc.) based on the reflected signals from the defects. Such a system should be equipped with software, allowing the analysis of the reflected signal to identify a defective area of the structure. Corresponding software can be developed based on the use of an artificial neural network (ANN) [2]. The use of ANN in reconstruction of the damaged state of structural elements is described in [3–12]. The use of various architectures and algorithms of ANN is described in [3–7]. Defining defects in anisotropic plates using ANN is the subject of [8]. In [9], the authors pointed out the advantages of identification methods that do not require the preliminary construction of a mathematical model of the object of study. In this chapter, we develop a method for reconstructing the depth of one of the layers of a layered structure using pavement as an example. Mathematically, the problem is reduced to the inverse geometric problem of the theory of elasticity [13]. The structure is loaded in the form of a pulsed impact effect at a certain distance from the studied zone; a series of sensors recording vibrations is located in a certain sequence in the linear direction of the study zone. The transverse and longitudinal vibrations are measured during the time when the waves reflected from the ends of the simulated section of the structure have not time to reach the sensor. In this way, real conditions for studying the layered structure of the soil base are simulated. Analysis of the measured amplitude-time characteristics (ATCs) shows the possibility of their use in inverse problems of defect recovery. An ANN is used as a tool for solving the inverse problem of reconstruction of defect parameters. The popularity of using ANNs is due to the fact that they were originally designed to solve just such problems, to find nonlinear dependencies in multidimensional data arrays. ANN, unlike other algorithmic constructions, are not programmed, but trained on a multitude of data for various studied design parameters. Training samples are built by solving direct problems in the finite element (FE) software ANSYS. The trained network, having received new, previously unknown analysis results, is able to correctly recognize the defect parameters. The use of FE modeling is rather effectively shown in [14–20]. We study the parameters of the natural modes of vibration, as well as their angular values of the forms of the vibration curves, showing fairly good correlation data with the magnitude of the defect in the structural element. The aim of the work is to build a FE model in the ANSYS software and develop principles for solving the problem of identifying layer parameters, using the example of restoring information about the second layer for given parameters of the structure properties, in a multilayer structure with pulsed excitation based on a combination of numerical experimental analysis and the use of neural network technologies.

36 The Study of Stratification of Multilayer Structures …

441

36.2 Statement of the Problem The problem is solved in a plane formulation using the finite element method (FEM). In this work, linear equations of the theory of elasticity are used taking into account the energy dissipation adopted in the ANSYS package [21, 22]. For an elastic medium, we have: ρ u¨ i + αρ u˙ i − σi j, j = f i ; σi j = ci jkl (εkl + β ε˙ kl ); εkl = u k,l + u l,k /2; where ρ is the density of material; u i are the components of the vector function of displacements; σi, j are the components of the tensor of mechanical stresses; fi are the components of the vector of the density of mass forces; εkl components of the strain tensor; ci jkl components of the fourth-rank tensor of elastic moduli; α non-negative damping coefficients (in ANSYS). Let us consider in more detail the mechanical boundary conditions. When determining the mechanical boundary conditions, the body boundary is represented as a union of disjoint regions S = Su St Sut on which the following conditions are specified: (i) is the condition for fixing the border or given movements

u i | Su = u i0 (ii) is the condition of the force action under which the components of the vector of mechanical stresses are specified ti = σi j n j St = pi (iii) is the condition for smooth contact with an absolutely rigid body—equality to zero of normal displacements and tangential stresses: u n = u i n i | Sut = 0, ti(k) = σi j n j τi(k)

Sut

=0

442

A. V. Cherpakov et al.

36.3 FE Modeling We consider the problem in a flat setting. As a simulated structure, an element of a multilayer structure, including 4 layers, was selected. Figure 36.1 shows an example of the physical structure of the “base” system “road construction—soil”. The numbers in the figure indicate the numbers of layers of the structure, the physical and geometric characteristics of which are given in Table 36.1. All layers are rigidly coupled with each other and with the underlying half-space (Fig. 36.1). As input parameters, the surface displacement field is considered as a result of short-term pulsed exposure. Parameters of layer properties are known. The thickness of the second layer d2 is considered as the investigated variable parameter. The magnitude of the variation of the 2nd layer lies in the range of d 2 = 0–1.1 m. It is assumed that under dynamic loading of the structure, the dependences of the thickness variations of the second layer d2 on the magnitude of the vibration responses measured at certain points of the structure will be found. An impulse in the form of a force Pt of a conditional unit amplitude is applied at point 1 (Fig. 36.2b). Pulse loading has a linear character with respect to the time of application of the load in the form of force (Fig. 36.2a). The load application time is τ = 0.003 s, which corresponds to the parameters of real impact loading. The displacement of wave field is analyzed in the area adjacent to the point of influence on the surface of layer 1. The characteristics of the waves propagating in the layered structure are studied based on the implementation of the FEM using the ANSYS complex. In the result of impulse loading, transverse and longitudinal waves of displacements of points arise both on the surface of the structure and throughout its volume. Fig. 36.1 Notation for layered soil structure with horizontal interfaces

Table 36.1 Parameters of the layers Layer No.

Elements

Thickness (m)

E (GPa)

ρ (kg/m3 )

ν

Damping factor

1

Asphalt-concrete

0.1

4

2000

0.33

0.001

2

Disconnected layers

0–1.1

0.1

2000

0.33

0.001

3

Underlying layer

0.1

2

2000

0.33

0.001

4

Underlying half-space

5

0.1

2000

0.33

0.001

36 The Study of Stratification of Multilayer Structures …

443

Fig. 36.2 a Diagram of the impulse load from the force Pt , applied at point 1 of the structure; an example of the result of transverse vibrations at a certain point at time t = 0.02 s, by modeling structural vibrations

An example of the implementation of the calculation results is a graph of the shape of transverse vibrations at time t = 0.02 s, when modeling structural vibrations (Fig. 36.2b). Control points are located on the surface at a distance of 0.1 m from each other. The first point is located at a distance of 0.1 m from the place of impact. Data is collected at 60 points. Figure 36.3 shows the results of numerical calculations of transverse displacements at various points on the surface. In the process of solving

Fig. 36.3 Amplitudes of the displacements of the traveling shear wave at the studied points on the surface at different points in time

444

A. V. Cherpakov et al.

Fig. 36.4 a Plots of the maximum amplitudes of transverse vibrations; b bending angles of curves of maximum amplitudes at the corresponding points Npt on the surface of the structure

the problem, the transverse displacements are calculated at the control points of the structure in the time range of t = 0−1 s. Of particular interest is the displacement field of the points of the surface layer in the time range of t = 0−0.12 s. This range is characterized by the fact that the primary form of deflections of the layered structure is formed and there are no vibration responses from the excitation of the outer layers of the structure. The oscillation amplitudes have maximum values of deflections at the corresponding points. The maximum oscillation amplitudes in a given time interval are measured. The curves of transverse deflections are constructed and the bending angles of these curves are calculated depending on the time of registration and the number of the studied point for each value from the varied parameters of thickness d2 of the second layer. Figure 36.4a shows the peak values of the oscillations for a thickness of the second layer d2 = 0.1 m, 0.5 m, 1 m; graphs of the bending angles of the curves at the corresponding measurement points are also presented (Fig. 36.4b). The initial analysis shows that the oscillation amplitudes have a non-linear logarithmic trend of change depending on the registration point. Nonlinearity of the trend is shown by the angles of the deflection of the curve of maximum amplitudes for various values of the depth of layer 2, which has certain pronounced inflection points. Data are collected on the deflection curves of non-stationary oscillations for all variations of the d2 layer.

36 The Study of Stratification of Multilayer Structures …

445

36.4 Application of Neural Network Technologies in the Task of Identifying the Thickness of Hidden Layer of Structure Artificial neural networks are computer systems that take the basics in biological neural networks that make up the brain of animals. Such systems are “learned” to perform tasks based on prepared examples. This is a nonlinear modeling tool. They are typically used to model complex relationships between inputs and outputs to find patterns in large amounts of data. In the framework of this task, it is necessary to establish a relationship between the amplitudes of oscillations propagating in the multilayer structure, as well as the angles of the deflection of the curve of maximum amplitudes with a layer thickness d2 (Fig. 36.2b). Based on the data obtained, at the stage of FE modeling, it is possible to form a training set and conduct training on the constructed neural network model. In the result of the numerical solution of direct problems by using the FE software package ANSYS, data were obtained at 60 points, located on the surface of the multilayer structure. For each set of 60 values, a specific layer height d2 was set. Training vectors have been prepared that contain the amplitudes of oscillations and the angles of deflection of the maxima of the amplitudes as input values, and the thickness of the layer under study as output values. A total of 100 numerical experiments were conducted. Thus, the training and test samples consist of 50 vectors. All data used in training the neural network are normalized and are on the interval [0, 1]. In order to solve the problem of identifying a parameter-value of the layer thickness, it is most rational, in this case, to apply a fully-connected multilayer ANN model. The proposed neural network model consists of 60 input neurons. The first hidden layer contains 32 neurons. The second hidden layer contains 8 neurons. As an activation function, the Rectified Linear Unit (ReLU) was selected. Sigmoid is set as the output activation function. For training, the Adam optimization method (Method for Stochastic Optimization) [23] is used. The root mean square error (MSE) was chosen as the loss function. It has been established that 4000 epochs of training are sufficient to achieve the required level of quality of ANN work, if amplitude values are used in the training set. In Fig. 36.5, the process of training a neural network model based on various data obtained during FE modeling is shown. The analysis shows that when reaching more than 1000 epochs, the mean-square error changes insignificantly.

36.5 Conclusion The problem of unsteady oscillations under pulsed loading of a layered structure is considered. The results of transverse displacements at the control points of the structure during the propagation of the wave from pulse excitation at a certain point are presented. During the simulation, the time interval in which the effects of the

446

A. V. Cherpakov et al.

Fig. 36.5 Change in the error value (MSE) of the neural network during its training based on the values of amplitudes (a), based on the values of the deflection angles of the curve of maximum amplitudes (b)

backward passage of the wave are not taken into account is considered as the analyzed one. Using optimization in the ANSYS complex allowed us to accelerate the process of solving the problem. In the result of the study, an approach was developed to identify the thickness of layers of a multilayer structure, based on a combination of the finite element method and ANN. The most successful configuration of the neural network architecture was established, namely: 60 input neurons, 32 neurons on the first hidden layer, 8 neurons on the second hidden layer and 1 output neuron. The study showed that the prepared volume of the data set is sufficient for the successful training of the constructed model and identification of the thickness of the hidden layer of the structure. In this case, the relative accuracy of determining the layer thickness in the case of applying the values of the amplitudes of the oscillations is 97%, and in the case of applying the values of the inflection angles of the curves of maximum amplitudes 91%. Based on the foregoing, we conclude that ANN algorithms can be successfully used to evaluate the stratification of multilayer structures using acoustic sounding from the far zone. Acknowledgements Research was financially supported by Southern Federal University, 2020 grant number VnGr/2020-04-IM (Ministry of Science and Higher Education of the Russian Federation).

36 The Study of Stratification of Multilayer Structures …

447

References 1. C.B. Park, R.D. Miller, J. Environ. Eng. Geophys. 13(1) (2008) 2. S. Haykin, Neural Networks—A Comprehensive Foundation (Prentice Hall, 1998), 842 p 3. A.A. Krasnoshchekov, B.V. Sobol, A.N. Solov’ev, A.V. Cherpakov, Russian J. Nondestruct. Test. 47(6) (2011) 4. Z. Waszczyszyn, L. Ziemianski, Comput. Struct. 22(79) (2001) 5. A.N. Solov’ev, P.S. Kurbatova, N.I. Saprunov, S.N. Shevcov, in Proceedings of 10-th International Conference “Modern Problems of Continuum Mechanics”, Rostov-on-Don (2006) (in Russian) 6. S.W. Liu, J.H. Huang, J.C. Sung, C.C. Lee, Comput. Methods Appl. Mech. Eng. 191 (2002) 7. V. Khandetsky, I. Antonyuk, NDT&E Int. 7(35) (2002) 8. Y.G. Xu, G.R. Liu, Z.P. Wu, X.M. Huang, Int. J. Solids Struct. 38 (2001) 9. X. Fang, H. Luo, J. Tang, Comput. Struct. 85 (2005) 10. A.N. Solov’ev, B.V. Sobol’, P.V. Vasil’ev, Russian J. Nondestruct. Test. 52(3) (2016) 11. A. Soloviev, B. Sobol, P. Vasiliev, in Advanced Materials—Proceedings of the International Conference on “Physics and Mechanics of New Materials and Their Applications”, PHENMA 2018, ed. by I.A. Parinov, S.-H. Chang, Y.-H. Kim, Springer Proceedings in Physics, vol. 224 (Springer Nature, Cham, Switzerland, 2019), 615–626 12. D.A. Pozharskii, B.V. Sobol, P.V Vasiliev, Mech. Adv. Mater. Struct. (18 May 2018) 13. A.O. Vatul’jan, Inverse Problems in Solid Mechanics (Moscow, Fizmatlit, 2007), 224 p (in Russian) 14. A.V. Cherpakov, A.N. Soloviev, V.V. Gricenko, O.U. Goncharov, Def. Sci. J. 66(1) (2016) 15. V.A. Akopyan, A.N. Solov’ev, A.V. Cherpakov, S.N. Shevtsov, Russian J. Nondestruct. Test. 49(10) (2013) 16. A.V. Cherpakov, O.V. Shilyaeva, M.N. Grigoryan, T.V. Polyakova, IOP Conf. Ser.Mater. Sci. Eng. 698, 066021 (2019) 17. A.V. Cherpakov, E.A. Shlyakhova, I.O. Egorochkina, Y.A. Kokareva, Mater. Sci. Forum 931 (2018) 18. A.N. Soloviev, I.A. Parinov, A.V. Cherpakov, Y.A. Chaika, E.V. Rozhkov, Mater. Phys. Mech. 37(2) (2018) 19. A. Cherpakov, I. Egorochkina, E. Shlyakhova, A. Kharitonov, A. Zarovny, S. Dobrohodskaya, in MATEC Web of Conferences, vol. 106, 04009. (2017) 20. S.N. Shevtsov, A.N. Soloviev, I.A. Parinov, A.V. Cherpakov, V.A. Chebanenko, Piezoelectric Actuators and Generators for Energy Harvesting—Research and Development (Springer Cham, Switzerland, 2018), 182 p 21. A.V. Nasedkin, DrSc Thesis (Phys.-Math. Sciences). Rostov State University, Rostov-on-Don, 271 p. (2001) (in Russian) 22. V.A. Krasil’nikov, V.V. Krylov, Introduction to Physical Acoustics (Moscow, Nauka, 1984), 400 p (in Russian) 23. D. Kingma, J. Ba, in International Conference on Learning Representations. arXiv:1412.6980 (2014)

Chapter 37

The Structural Correlation and Mechanical Properties in Amorphous Hafnium Oxide Under Pressure Nguyen-Hoang Thoan, Nguyen-Trung Do, Nguyen-Ngoc Trung, and Le-Van Vinh Abstract In this chapter, the classical molecular dynamics technique was used to investigate the atomistic structure of amorphous hafnium oxide (HfO2 ) under pressure. The local atomic structure and the liquid-solid transition of HfO2 were analyzed the pair radical distribution functions, bond angle distributions, coordination number and the void distribution. The simulation reveals that although the fractions of structural units HfOx and OHfy strongly change with the density, the partial bond angle distributions of these structural units are identical for all constructed models. This result has enabled us to establish a relationship between the bond angle distributions and the fractions of structural units. From deformation of samples, elastic moduli and Poisson ratio were determined. The Young’s modulus and yield stress increase with the increasing density. The strain hardening becomes more pronounced as the density increases.

37.1 Introduction Hafnium oxide, HfO2 , has been extensively studied for use as silicon dioxide replacements in the gate oxide insulating layer in complementary metal oxide semiconductor (CMOS) devices and resistive RAM devices [1–4]. This oxide has high electric constant (high-κ) of about 25–30 depending on fabrication process conditions. In addition, it has a wide band gap, relatively high refractive index, high thermal and chemical stability, high melting point, excellent compression performance and low thermal expansion coefficient. Solid HfO2 can be formed at different phases including amorphous, monoclinic, tetragonal and cubic. However, HfO2 often deposits as an amorphous phase by CVD or ALD fabrication processes. Many comprehensive studies of the structure and thermodynamics of the HfO2 crystal and amorphous phases N.-H. Thoan · N.-T. Do · N.-N. Trung (B) School of Engineering Physics, Hanoi University of Science and Technology, Hanoi, Vietnam e-mail: [email protected] L.-V. Vinh Phenikaa University, Hanoi, Vietnam © Springer Nature Switzerland AG 2020 I. A. Parinov et al. (eds.), Advanced Materials, Springer Proceedings in Materials 6, https://doi.org/10.1007/978-3-030-45120-2_37

449

450

N.-H. Thoan et al.

have been investigated intensively by both experiments and simulations in recent years [5–9]. Recently, we investigated MD simulation results on liquid-amorphous transition of HfO2 undercooling process [10]. Tapily et al. demonstrated that the initial low temperature ALD deposited HfO2 in its amorphous state is harder and stiffer than the polycrystalline form of HfO2 [11]. Therefore, this has motivated us to carry out this study. Therefore, in this study, we report on the results of density and the structural evolution of a-HfO2 under compression, and discuss the unit structure HfOx and mechanical behavior of these systems.

37.2 Computational Procedures The MD simulation has been performed using an initial configuration containing 6000 atoms (2000 hafnium and 4000 oxygen ones) in a cube under periodic boundary conditions. We apply the Morse-KBS combined potential: ϕi j =

Ci j qi q j e 2 + Di j 1 − exp −ai j ri j − r0 − 1 + 12 ri j ri j

(37.1)

where, r ij is the distance between an ion of type i and an ion of type j (i, j = Hf, O), e is the elementary charge, and qHf = 2.4 and qO = −1.2 are partial charges of hafnium and oxygen respectively; Dij , aij and r 0 are Morse potential parameters (listed in [12]); and C/r 12 is the repulsive contribution. The cation-cation interactions are assumed to be purely coulombic. The long-range Coulomb interactions were calculated with the Ewald summation technique, which is applied to three-dimensional periodic boundary conditions [13]. The Verlet algorithm with a time step of 1.5 fs is adopted and the simulation was executed at a constant pressure (the ensemble NPT). Classical MD simulation and the Verlet algorithm can be seen in detail elsewhere [14, 15]. The scaling method was adopted during the simulation to control the system temperature. The pressure is defined in terms of the virial expression [16]. The initial configuration was randomly generated all atoms in the simulation box corresponding to the density of 10.2 g cm−3 with condition that no two atoms be closer than 1.0 Å. The initial configuration was then equilibrated for 50,000 static relaxation (SR) steps. In the SR method the system is at absolute zero due to no kinetic energy, and the atoms are displaced in the direction in which the resultant force acts. The displacement step (SR step) is proportional to the resultant force. In the next step, this configuration had been equilibrated by MD method at temperature of 5000 K for over 50,000 time steps. Then, the samples were cooled down to 300 K within 470,000 time steps (with the cooling rate of 66.67 K/ps) without and with applying an pressure during cooling process (P = 0–100 GPa). After reaching 300 K, samples are relaxed for 50,000 time steps to get a stable state. To determine the coordination numb